FUNDAMENTALS OF MICROMECHANICS OF SOLIDS
Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui ©...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

FUNDAMENTALS OF MICROMECHANICS OF SOLIDS

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

FUNDAMENTALS OF MICROMECHANICS OF SOLIDS Jianmin Qu Mohammed Cherkaoui

John Wiley & Sons, Inc.

This book is printed on acid-free paper. 嘷 ⬁ Copyright 䉷 2006 by John Wiley & Sons, Inc. All rights reserved Published by John Wiley & Sons, Inc., Hoboken, New Jersey Published simultaneously in Canada No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning, or otherwise, except as permitted under Section 107 or 108 of the 1976 United States Copyright Act, without either the prior written permission of the Publisher, or authorization through payment of the appropriate per-copy fee to the Copyright Clearance Center, 222 Rosewood Drive, Danvers, MA 01923, (978) 750-8400, fax (978) 750-4470, or on the web at www.copyright.com. Requests to the Publisher for permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street, Hoboken, NJ 07030, (201) 748-6011, fax (201) 748-6008, e-mail: [email protected] Limit of Liability / Disclaimer of Warranty: While the publisher and author have used their best efforts in preparing this book, they make no representations or warranties with respect to the accuracy or completeness of the contents of this book and speciﬁcally disclaim any implied warranties of merchantability or ﬁtness for a particular purpose. No warranty may be created or extended by sales representatives or written sales materials. The advice and strategies contained herein may not be suitable for your situation. You should consult with a professional where appropriate. Neither the publisher nor author shall be liable for any loss of proﬁt or any other commercial damages, including but not limited to special, incidental, consequential, or other damages. For general information on our other products and services or for technical support, please contact our Customer Care Department within the United States at (800) 762-2974, outside the United States at (317) 572-3993 or fax (317) 572-4002. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. For more information about Wiley products, visit our web site at www.wiley.com. Library of Congress Cataloging-in-Publication Data: Qu, Jianmin. Fundamentals of micromechanics of solids / Jianmin Qu, Mohammed Cherkaoui. p. cm. Includes bibliographical references. ISBN-13: 978-0-471-46451-8 (cloth) ISBN-10: 0-471-46451-1 (cloth) 1. Nanostructured materials—Mechanical properties—Textbooks. 2. Micromechanics—Textbooks. 3. Microelectromechanical systems—Materials—Textbooks. I. Cherkaoui, Mohammed. II. Title. TA418.9.N35Q22 2006 620.1⬘05—dc22 2005030781 Printed in the United States of America 10

9

8

7

6

5

4

3

2

1

To Qianqian, Bouchra, Lisa, Jalal, Rayan and Hajja-Fetouma.

CONTENTS Preface 1

Introduction

1.1 1.2 1.3 1.4

2

xiii 1

Background and Motivation / 3 Objectives / 4 Organization of Book / 4 Notation Conventions / 5 References / 9

Basic Equations of Continuum Mechanics

11

2.1 2.2 2.3 2.4 2.5

Displacement and Deformation / 11 Stresses and Equilibrium / 15 Energy, Work, and Thermodynamic Potentials / 18 Constitutive Laws / 22 Boundary Value Problems for Small-Strain Linear Elasticity / 34 2.6 Integral Representations of Elasticity Solutions / 35 Problems / 43 Appendix 2.A / 44 Appendix 2.B / 44 Appendix 2.C / 46 References / 47 Suggested Readings / 48 3

Eigenstrains

3.1 3.2 3.3

49

Deﬁnition of Eigenstrains / 49 Some Examples of Eigenstrains / 52 General Solutions of Eigenstrain Problems / 53 vii

viii

CONTENTS

3.4

4

Examples / 56 Problems / 66 Appendix 3.A / 67 Appendix 3.B / 70 References / 70 Suggested Readings / 70

Inclusions and Inhomogeneities

71

4.1 4.2 4.3

Deﬁnitions of Inclusions and Inhomogeneities / 71 Interface Conditions / 73 Ellipsoidal Inclusion with Uniform Eigenstrains (Eshelby Solution) / 77 4.4 Ellipsoidal Inhomogeneities / 84 4.5 Inhomogeneous Inhomogeneities / 88 Problems / 91 Appendix 4.A / 92 Appendix 4.B / 93 Suggested Readings / 98 5

Deﬁnitions of Effective Moduli of Heterogeneous Materials

99

5.1 5.2 5.3 5.4 5.5 5.6

Heterogeneity and Length Scales / 99 Representative Volume Element / 102 Random Media / 102 Macroscopic Averages / 108 Hill’s Lemma / 111 Deﬁnitions of Effective Modulus of Heterogeneous Media / 113 5.7 Concentration Tensors and Effective Properties / 116 Problems / 119 Suggested Readings / 119 6

Bounds for Effective Moduli

6.1

Classical Variational Theorems in Linear Elasticity / 120 6.2 Voigt Upper Bound and Reuss Lower Bound / 123

120

ix

CONTENTS

6.3 6.4

7

Determination of Effective Moduli

7.1 7.2 7.3 7.4 7.5 7.6 7.7

8

196

Composite-Sphere Model / 196 Three-Phase Model / 200 Four-Phase Model / 203 Multicoated Inclusion Problem / 204 Problems / 206 Appendix 8.A / 207 Appendix 8.B / 208 Appendix 8.C / 210 References / 211 Suggested Readings / 212

Effective Properties of Fiber-Reinforced Composite Laminates

9.1

154

Basic Ideas of Micromechanics for Effective Properties / 154 Eshelby Method / 158 Mori–Tanaka Method / 163 Self-Consistent Methods for Composite Materials / 169 Self-Consistent Methods for Polycrystalline Materials / 173 Differential Schemes / 179 Comparison of Different Methods / 183 Problems / 193 Suggested Readings / 195

Determination of the Effective Moduli—Multiinclusion Approaches

8.1 8.2 8.3 8.4

9

Extensions of Classical Variational Principles / 126 Hashin–Shtrikman Bounds / 136 Problems / 145 Appendix 6.A / 147 References / 152 Suggested Readings / 153

Unidirectional Fiber-Reinforced Composites / 214

214

x

CONTENTS

9.2 9.3 9.4

10

Brittle Damage and Failure of Engineering Composites

10.1 10.2 10.3

11

280

Eshelby’s Solution and Kro¨ner’s Model / 283 Applications / 299 Time-Dependent Behavior of Polycrystalline Materials: Secant Approach / 312 Problems / 316 References / 316

Nonlinear Properties of Composites Materials: Thermodynamic Approaches

12.1 12.2 12.3

245

Imperfect Interfaces / 245 Fiber Bridging / 259 Transverse Matrix Cracks / 266 Problems / 277 Appendix 10.A / 277 References / 278 Suggested Readings / 279

Mean Field Theory for Nonlinear Behavior

11.1 11.2 11.3

12

Effective Properties of Multilayer Composites / 226 Effective Properties of a Lamina / 234 Effective Properties of a Laminated Composite Plate / 238 Problems / 240 Appendix 9.A / 240 References / 243 Suggested Readings / 244

Nonlinear Behavior of Constituents / 321 Effective Potentials / 328 The Secant Approach / 331 Problems / 342 Suggested Readings / 345

319

xi

CONTENTS

13

Micromechanics of Martensitic Transformation in Solids

13.1

347

Phase Transformation Mechanisms at Different Scales / 350 13.2 Application: Thermodynamic Forces and Constitutive Equations for Single Crystals / 367 13.3 Overall Behavior of Polycrystalline Materials with Phase Transformation / 373 Problems / 377 References / 379 Suggested Readings / 379 Index / 381

PREFACE For many years, we have taught courses on micromechanics at our respective institutions (JQ at the Georgia Institute of Technology and MC at the University of Metz). We both felt the need for a textbook that (1) provides an integrated approach to the various topics of micromechanics, (2) covers the basic ideas of homogenization, (3) is written pedagogically for graduate and upper-level undergraduate students, (4) contains exercises problems, and (5) can be taught in a semester course. It was such a need that motivated us to start this project. We hope the book in front of you fulﬁlls these objectives. Micromechanics had ﬂourished over the past half-century. The literature is rich and diverse. Holding the book to a reasonable length prevented us from including many of the elegant results published over the years. Although we used our best judgment to cite and compile a list of references that we believe are most relevant to the text, listing such a limited number of references does not do justice to the breadth and depth of the ﬁeld. We sincerely apologize to those authors whose works were not given proper credit or were not cited. The book was developed primarily from our notes for the micromechanics courses that we have taught over the years. Our students, through their questions and comments, provided valuable input to the book. We are very grateful for their contributions. We would like to thank our colleagues at Georgia Tech for their encouragement and collaboration. It has been a great pleasure to be among such an intellectually stimulating group of people. The book was written mainly during evenings and on weekends. At times, we had to neglect our duties as husbands and fathers. We want to acknowledge that without the support of our wives and families, this project would not have been completed. Their understanding and sacriﬁces are greatly appreciated. This book is dedicated to them. JIANMIN QU Atlanta, Georgia

MOHAMMED CHERKAOUI Metz, France xiii

1 INTRODUCTION Mechanics studies the theory of forces and their interactions. It is the pillar of modern sciences. Many of the great scientists in history have been mechanicians including, for example, Aristotle, Archimedes, Leonardo da Vinci, Kepler, and Newton. Continuum mechanics is a relatively young branch of mechanics. It studies the deformation of bodies (solid or ﬂuid) under forces or stresses. Although the basic foundation of continuum mechanics was laid by Galileo, it was during the late eighteenth and the early nineteenth centuries that modern theories of continuum mechanics were gradually developed by Laplace, Fourier, Coriolis, Lagrange, Hamilton, Navier, and Cauchy, among others. It was during this period and up until the early 1900s that continuum mechanics enjoyed its most rapid development into maturity. By the mid-1900s, theories of continuum mechanics had been established upon vigorous mathematics. One of the most successful stories of continuum mechanics is the development and application of fracture mechanics. In 1913, C.E. Inglis looked at a thin plate of glass with an elliptical hole in the middle in a new and different way (Fig. 1.1). The plate was pulled at both ends perpendicular to the ellipse. He found that the stress at point A is given by

冉

A ⫽ 1 ⫹

冊

2a . b

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

1

2

INTRODUCTION

y

σ A

2b

x

2a

(a)

(b)

Figure 1.1 (a) Inglis’ work on stress concentration near an elliptical hole. (b) Grifﬁth’s work on stress concentration near a sharp crack tip.

In other words, the stress at the tip of the elliptical hole can be much larger than the stress applied. In the 1920s, A.A. Grifﬁth extended Inglis’ work. He found that the stress at the ends of the crack approaches inﬁnity: ⫽

K . 兹2x

Grifﬁth also introduced the notion of energy. He said that for a crack to grow, it was necessary for there to be enough potential energy in the system to create the new surface area of the crack. Although he did not know that it takes more than this for a crack to grow, Grifﬁth’s idea of fracture criterion laid the foundation for a brand new theory called fracture mechanics, which is one of the most celebrated branches of continuum mechanics in modern history. More importantly, fracture mechanics brought continuum mechanics and material science together and opened up new opportunities for studying not only deformation of solid bodies but also the failure behavior of solid materials under load. Thus a new ﬁeld called mechanics of materials emerged. In mechanics of material, we use the vigorous continuum mechanics theories to investigate and study how materials with certain microstructures deform and eventually fail under given loads or stresses. Micromechanics is a branch of mechanics of materials. It is the most recent development in applying continuum mechanics theories to real

1.1

BACKGROUND AND MOTIVATION

3

materials. The beginning of micromechanics may be traced back to Eshelby’s seminal study (Eshelby, 1957). But, the theory of micromechanics was not fully developed into a subject area of its own until the early 1980s. Even though it is still an actively researched area now, the theory of micromechanics has matured enough that several books have been published. Among them, the books by Mura (1986), NematNasser and Hori (1993), and Krajcinovic (1996) are probably the most comprehensive and inﬂuential ones. The theory of micromechanics of solids describes the scientiﬁc concepts, principles, and methodologies for the study of thermomechanical behavior of heterogeneous materials. Although the fundamental equations of micromechanics are based on mechanics of continuum, its applications cover a broad range of thermomechanical behavior of materials including plasticity, fracture, and fatigue, constitutive equations of composites, and polycrystalline materials. For example, it applies the theories of elasticity and plasticity to study imperfections in crystals, inclusions, and inhomogeneities in alloys and composite materials. The objective is to study the macroscopic mechanical behavior of materials from an understanding of their microstructure. This involves the application of continuum mechanics to identiﬁable small-scale structures and the use of analytical and numerical methods to compute the macroscopic responses. This science-based approach enables us to predict the behavior of new materials without the need for physical experimentation. It provides a powerful tool for engineering design, fabrication, and analysis of a wide range of materials including polycrystalline, composite, geotechnical, biological, and electronic materials. Optimum microstructures can be forecasted rather than found by trial and error. Fracture and fatigue of solids and structures, martensitic transformations, interphases in composites, and dispersion hardening of alloys are examples of the phenomena that are being elucidated and qualiﬁed by micromechanics.

1.1 BACKGROUND AND MOTIVATION

As the theory of micromechanics matures, many universities around the world are offering courses on this subject. For the past 15 years, the authors have taught micromechanics classes in their respective institutions. We have always been frustrated by not being able to ﬁnd an appropriate textbook for the course. Most existing books on this subject are research monographs, primarily for experts and researchers. They

4

INTRODUCTION

can be excellent research tools but not convenient to use as textbooks. Because the theory of micromechanics is still in its infancy, results were obtained by individual researchers using, sometime, very different approaches/methodologies. In order for the students (or ﬁrst-time learners) to understand the intrinsic connections among different concepts and approaches, a uniﬁed approach (including the use of notations) is needed to develop the micromechanics theory. This will allow both the instructor and the students to fully grasp the essence of the theory. Furthermore, instead of collecting and compiling existing results from the literature, we should identify a set of topics that convey the fundamental ideas of micromechanics and focus on these topics. Related topics not covered in the text should be referenced for those who wish to learn more. Exercise problems should be provided for the convenience of the instructor, as well as for those who wish to study the subject on their own. These are the major considerations that motivated us to write this textbook.

1.2

OBJECTIVES

The intent of this book is not to provide a comprehensive collection of results of micromechanics in the literature, nor is it to be a research reference book for relevant publications. Instead, it is intended to be a textbook for graduate and possibly upper-level undergraduate students. It is to provide a teaching tool for an instructor to teach and a learning aid for a beginner to learn (what we believe) the most fundamental ideas and approaches, the basic concepts, principles, and methodologies of micromechanics. To this end, a uniﬁed mathematical framework is introduced early on in the book. The rest of the theories will be developed based on this framework in a logical and easily understandable approach. In addition to some new results from the authors’ own research, many of the available results in the literature will be derived or re-derived based on this uniﬁed mathematical framework. This approach enables the students to follow the various developments of the micromechanics theories. It also helps the students to quickly comprehend and appreciate the wide range of applications of micromechanics.

1.3 ORGANIZATION OF BOOK

The book is organized into 13 chapters. References and/or Suggested Readings are included at the end of each chapter. Some of these ref-

1.4

NOTATION CONVENTIONS

5

erences contain certain results not derived but used in the text. Others are listed because they present either alternative approaches for the same problem or provide additional topics related to those discussed in the chapter. We have made great effort to make the book somewhat self-contained. The goal was that a reader with the basic knowledge of continuum mechanics should be able to follow this book without consulting other publications. Each chapter also contains a set of problems. The students, as well as the instructor, may ﬁnd these exercises useful. The level of difﬁculty varies signiﬁcantly among the problems. The students should not feel discouraged if they cannot solve some of the problems on their ﬁrst attempt. The reminder of this chapter presents the most frequently used notations and notation conventions used in this book. In the next chapter, a brief summary of the basic theories of continuum mechanics is presented. The rest of the chapters are grouped into linear theories (Chapters 3–10) and nonlinear theories (Chapter 11–13). 1.4 NOTATION CONVENTIONS

One of the difﬁculties many people encounter in studying micromechanics is the different kinds of notations used in the literature. For consistency, we will use the following conventions throughout this book, unless otherwise noted. Index notation for vectors and tensors will be used extensively. Whenever possible, the base letter for a vector (ﬁrst-order tensor) will be a lowercase italic letter, for a second-order tensor it will be a lowercase Greek letter, and for a fourth-order tensor it will be an uppercase italic letter. For example, ui represents a vector, ij represents a second-order tensor, and Lijkl represents a fourth-order tensor. Exceptions to these rules are certain letters conventionally used for speciﬁc physical entities. For example, Gij is for the Green function, which is a second-order tensor. The summary convention will be used:

冘冘L 3

Lijklkl ⬅

3

.

ijkl kl

(1.4.1)

l⫽1 k⫽1

Alternately, when it is convenient, the direct (or matrix) notation of vectors and tensors will be used as well. Boldface letters will be used for this purpose. For example, u represents a vector, represents a

6

INTRODUCTION

second-order tensor, and L represents a fourth-order tensor. To distinguish tensors with the same base letter a subscript will be used. For example, L1 and L2 are used to denote two different fourth-order tensors. Note that these subscripts are entirely different from the subscripts used to represent the components of a tensor. Subscripts on matrix notations do not follow the summation convention, therefore, when a tensor in the matrix notation with a subscript is written in index forms, we will change the subscript to superscript with parenthesis, for example, (2) L1 ⇔ L(1) and L2 ⇔ Lijkl . ijkl

Throughout the book, index and matrix notations will be used interchangeably based on whichever is convenient. To avoid confusion, we use the following notations to represent the tensor algebraic operations. Dot product: Double-dot product: Dyad:

ijnj ⇔ n Lijklkl ⇔ L⬊, minj ⇔ m n,

LijklTklmn ⇔ L⬊T nimj ⇔ n m

Since dot and double-dot operations will be used extensively, we will, when there is no ambiguity, neglect the dot(s) and simply write, for example, L⬊ ⇔ L and n ⇔ n. A fourth-order tensor, A, is nonsingular if and only there exists a fourth-order tensor, for example, B, such that AB ⫽ BA ⫽ I.

(1.4.2)

In this case, B is the inverse of A, or A is the inverse of B, that is, B ⫽ A⫺1

or A ⫽ B⫺1.

(1.4.3)

An equivalent deﬁnition can be given as follows: A is singular if and only if there exists a second-order tensor ⫽ 0, such that A ⫽ 0. A fourth-order isotropic tensor can be written as Aijkl ⫽ a␦ij␦kl ⫹ b(␦ik␦jl ⫹ ␦il␦jk ⫺ –32 ␦ij␦kl).

(1.4.4)

For convenience, we introduce the following two fourth order tensors:

1.4

I hijkl ⫽ –13 ␦ij␦kl,

NOTATION CONVENTIONS

d I ijkl ⫽ –12 (␦ik␦jl ⫹ ␦il␦jk ⫺ –32 ␦ij␦kl),

7

(1.4.5)

so that the fourth-order isotropic tensor given in (1.4.4) can be written as A ⫽ 3aIh ⫹ 2bId.

(1.4.6)

It can be easily shown that, if is a second-order tensor, then A ⫽ 3aI ⫹ 2b⬘,

(1.4.7)

where ⫽ kk is the spherical part of , and ⬘ij ⫽ ij ⫺ –31 kk␦ij

(1.4.8)

is the deviatoric part of . Furthermore, the following statements can be easily proven: 1. A ⫽ 3aIh ⫹ 2bId is positive deﬁnite if and only if a ⬎ 0, b ⬎ 0. 1 h 1 d I ⫹ I. 2. A⫺1 ⫽ 3a 2b 3. I ⫽ Ih ⫹ Id is the identity tensor, that is, I ⫽ AA⫺1 ⫽ A⫺1A. 4. If B ⫽ 3cIh ⫹ 2dId, then A ⫹ B ⫽ 3(a ⫹ c)Ih ⫹ 2(b ⫹ d)Id. 5. AB ⫽ BA ⫽ 9acIh ⫹ 4bdId. Additionally, we introduce another symbolic notation for fourthorder isotropic tensors: A ⫽ (3a, 2b).

(1.4.9)

The following statements can be easily proven: 1. A ⫽ (3a, 2b) is positive deﬁnite if and only if a ⬎ 0, b ⬎ 0. 1 1 , . 2. A⫺1 ⫽ 3a 2b 3. I ⫽ (1,1) is the identity tensor, that is, I ⫽ AA⫺1 ⫽ A⫺1A ⫽ (1,1). 4. If B ⫽ (3c, 2d), then A ⫹ B ⫽ (3a ⫹ 3c, 2b ⫹ 2d). 5. AB ⫽ BA ⫽ (9ac, 4bd).

冉 冊

8

INTRODUCTION

For tensor calculus, the most often used operations are the gradient and divergence. The gradient of a scalar function results in a ﬁrst-order tensor: b ⫽ ⵜƒ ⇔ bj ⫽

⭸ƒ ⬅ ƒ, j. ⭸xj

(1.4.10)

The divergence of a vector is a scalar: a ⫽ div[b] ⫽

⭸b1 ⭸b ⭸b ⫹ 2 ⫹ 3 ⇔ a ⫽ bj, j. ⭸x1 ⭸x2 ⭸x3

(1.4.11)

In the above, the notation (•), j indicates the derivative with respect to the independent variable of the function. If the function has more than one independent variable, ambiguity may arise. In this case, instead of using, for example, ƒ, j(x, y), we will use the standard notation to explicitly indicate partial derivatives, for example, ⭸ƒ(x, y) . ⭸x

(1.4.12)

The divergence of a second-order tensor becomes a vector: p ⫽ ⵜ ⇔ pi ⫽

⭸ij ⫽ ij, j. ⭸xj

(1.4.13)

For integrals, a single integral sign will be used. For line (onedimensional) integrals, the integration variable will be used for the inﬁnitesimal line element, for example, y⫽

冕 ƒ(x) dx, L

where L is the line of integration. For surface (two-dimensional) integrals, we will typically use dS for the inﬁnitesimal area element, for example, y⫽

冕 ƒ(x) dS, S

REFERENCES

9

where S is the area of integration. Here, it is implied that x is the integration variable since the integrand depends on x only. If the integrand depends on more than one independent variable, we will explicitly indicate which variable is being integrated, for example, y(z) ⫽

冕 ƒ(x, z) dS(x). S

Similarly, for volume (three-dimensional) integrals, we will use either one of the following two forms: y⫽

冕 ƒ(x) dV,

y(z) ⫽

V

冕 ƒ(x, z) dV(x). V

Finally, we introduce some special tensors. The Kronecker delta ␦ij is deﬁned by ␦ij ⫽

再

1 for i ⫽ j . 0 for i ⫽ j

(1.4.14)

And the permutation tensor ijk is deﬁned by ijk ⫽

冦

1

⫺1

0

when i, j, k are an even permutation of 1, 2, 3 when i, j, k are an odd permutation of 1, 2, 3 . when any two indices are equal (1.4.15)

For example, 123 ⫽ 231 ⫽ 312 ⫽1, 213 ⫽ 132 ⫽ 321 ⫽ ⫺1, and others are zero. The permutation tensor and the Kronecker delta ␦ij are related through the ⫺ ␦ relationship: ijkmnk ⫽ ␦im␦jn ⫺ ␦in␦jm.

(1.4.16)

REFERENCES Eshelby, J. D. (1957). The Determination of Elastic Field of an Ellipsoidal Inclusion, and Related Problems, Proc. Roy. Soc. London, Vol. A241, pp. 376–396.

10

INTRODUCTION

Krajcinovic, D. (1996). Damage Mechanics, North-Holland, New York. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff Pub., Boston. Nemat-Nasser, S. and M. Hori (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York.

2 BASIC EQUATIONS OF CONTINUUM MECHANICS In this chapter, we will introduce some basic equations of continuum mechanics. It is assumed that the readers already have had some prior knowledge of the subject. Therefore, lengthly derivations are omitted. Only equations that are needed later for deriving the micromechanics theories are outlined. For more detailed and in-depth knowledge of continuum mechanics, we refer to the References and Suggested Readings at the end of this chapter. The fundamental equations governing the deformation of continuum can be roughly classiﬁed into four categories: (1) kinematic equations that deal with the description of motion and deformation, (2) kinetic equations that deal with forces, stresses, and their equilibrium, (3) constitutive equations that describe the material’s response under load, and (4) boundary and initial conditions that are necessary to uniquely deﬁne the boundary/initial value problems. We will discuss these classes of equations separately.

2.1 DISPLACEMENT AND DEFORMATION

At any given instant of time t, a continuum having a volume V and bounding surface S will occupy a certain region R of the physical space; see Figure 2.1. When the continuum undergoes deformation, the particles (material points) within the continuum may be displaced from one spatial position to another along various paths. The displacement of a particle can be written as Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

11

12

BASIC EQUATIONS OF CONTINUUM MECHANICS

S0 X3

S

u X

x

V V0 X2 Reference X1 Configuration

x1

x3 x2

Current Configuration

Figure 2.1 Reference and current conﬁgurations.

u ⫽ x ⫺ X,

(2.1.1)

where x is the position occupied at current time t by the particle that occupied position X in the initial conﬁguration (t ⫽ 0). In some literature, x is referred to as the spatial (Eulerian) coordinate, and X is referred to as the material coordinate. This is because X can be viewed as a label attached to a material particle while x indicates where the particle is located at a give time. The current position x of a particle originally located at X in the initial conﬁguration can be expressed by xi ⫽ xi(X, t).

(2.1.2)

Clearly, the above equation provides a way to ﬁnd the new location of each particle after the deformation. This way of describing the deformation is called the Lagrangian description. On the other hand, the Eulerian description uses the following equation: XI ⫽ XI (x, t)

(2.1.3)

to keep track of which particle happens to be at the location xi at the current time t. For clarity, capital letters are used for the subscript of a tensor component associated with the Lagrangian coordinate system (the initial conﬁguration), and the lowercase letters are used for the subscript of a tensor component associated with the Eulerian coordinate system (the current or deformed conﬁguration). Such a distinction is unnecessary if both the Lagrangian and Eulerian conﬁgurations use the same coordinate system. Equations (2.1.2)–(2.1.3) may be interpreted as a mapping between the initial conﬁguration and the current conﬁguration. The continuum

2.1

DISPLACEMENT AND DEFORMATION

13

mechanics theory assumes that such mapping is sufﬁciently smooth (differentiable) and one to one, that is, the Jacobian J ⫽ 兩⭸xi / ⭸XJ兩 should not become zero at any time. Partial differentiation of (2.1.2) with respect to XJ and (2.1.3) with respect to xj yield, respectively, dxi ⫽ FiJ dXJ,

dXI ⫽ F Ij⫺1 dxj,

(2.1.4)

where FiJ ⫽

⭸xi ⭸XJ

and F⫺1 Ij ⫽

⭸XI ⭸xj

(2.1.5)

are called the material deformation gradient tensor and the spatial deformation gradient tensor, respectively. Through the polar decomposition (Malvern, 1969), the material deformation gradient tensor can be written as FiJ ⫽ RiKUKJ ⫽ Vik RkJ

(2.1.6)

where Rij is the (orthogonal) rotation tensor, and Uij and Vij are symmetric, positive deﬁnite tensors known as the right- and left-stretch tensors, respectively. Based on their deﬁnitions, a length segment dXI connecting two neighboring particles in the undeformed conﬁguration becomes a length segment dxi connecting the same two particles now in the deformed conﬁguration. The difference between the lengths (square) of these two segments, dxi dxi ⫺ dXI dXI, can be used as a measure of deformation occurring in the neighborhood of these particles when the continuum is deformed from the initial conﬁguration to the current conﬁguration, that is, dxi dxi ⫺ dXI dXI ⫽ 2EIJ dXI dXJ ⫽ 2E*ij dxi dxj,

(2.1.7)

where

冉 冉

冊 冉 冊 冉

冊 冊

EIJ ⫽

⭸uj 1 ⭸ui ⭸u ⭸u 1 ⭸xk ⭸xk ⫺ ␦IJ ⫽ ⫹ ⫹ k k 2 ⭸XI ⭸XJ 2 ⭸XJ ⭸XI ⭸XI ⭸XJ

(2.1.8)

E*ij ⫽

1 ⭸X ⭸X 1 ⭸uI ⭸uJ ⭸uK ⭸uK ␦ij ⫺ K K ⫽ ⫹ ⫺ 2 ⭸xi ⭸xj 2 ⭸xj ⭸xi ⭸xi ⭸xj

(2.1.9)

14

BASIC EQUATIONS OF CONTINUUM MECHANICS

are called the Lagrangian (Green) ﬁnite strain tensor and the Eulerian (or Cauchy) ﬁnite strain tensor, respectively. When the same coordinate system is used for both the initial reference conﬁguration and the current conﬁgurations, the strain tensors can be further written as Eij ⫽

冉

冊

⭸uj ⭸u ⭸u 1 ⭸ui ⫹ ⫹ k k , 2 ⭸Xi ⭸Xi ⭸Xi ⭸Xj

冉

冊

1 ⭸ui ⭸uj ⭸uk ⭸uk ⫹ ⫺ . 2 ⭸xi ⭸xi ⭸xi ⭸xj

E* ij ⫽

(2.1.10) When the displacement gradients are small, that is, 兩⭸ui / ⭸Xj兩 ⬍⬍ 1 and 兩⭸ui / ⭸xj兩 ⬍⬍ 1, neglecting the higher order terms leads to ⭸ui ⭸u ⭸Xk ⭸u ⫽ i ⫽ i ⭸xj ⭸Xk ⭸xj ⭸Xk

冉

␦kj ⫺

冊

⭸Xk ⭸xj

⫽

⭸ui . ⭸Xj

(2.1.11)

冊

(2.1.12)

Thus one has, from (2.1.8) and (2.1.9), that Eij ⫽

冉

冊

冉

⭸uj 1 ⭸ui ⭸uj 1 ⭸ui ⫹ ⫽ E* ⫹ ⫽ ij, ij ⫽ 2 ⭸Xi ⭸Xi 2 ⭸xi ⭸xi

where ij is called the inﬁnitesimal strain tensor. Other kinematic tensors often used in viscoelastic and plastic theories are the rate of deformation tensor and the spin tensor: Dij ⫽

冉

冊

1 ⭸vi ⭸vj ⫹ , 2 ⭸xj ⭸xi

Wij ⫽

冉

冊

1 ⭸vi ⭸vj ⫺ , 2 ⭸xj ⭸xi

(2.1.13)

where vi(x1, x2, x3, t) is the velocity ﬁeld vi ⫽

dui dxi ⫽ dt dt

expressed in terms of the Eulerian (spatial) coordinates xi. For small strain deformation,

(2.1.14)

2.2

冋 冉 冊册 冋 冉 冊

dij d 1 ⭸ui ⭸uj ⫽ ⫹ dt dt 2 ⭸xj ⭸xi ⫽

STRESSES AND EQUILIBRIUM

⫽

15

册

1 ⭸(dui /dt) ⭸(duj /dt) ⫹ 2 ⭸xi ⭸xi

1 ⭸vi ⭸vj ⫹ , 2 ⭸xj ⭸xi

that is, dij ⫽ Dij. dt

(2.1.15)

This is no longer true for ﬁnite deformation. Instead, we have (Malvern, 1969) dEIJ ⫽ FmI DmnFnJ. dt

(2.1.16)

2.2 STRESSES AND EQUILIBRIUM

The state of stress at a point in a continuum can be represented by the Cauchy stress tensor ij in the current (or deformed) conﬁguration. Note that the components of the Cauchy stress tensor are deﬁned as force per unit area in the deformed conﬁguration. Balance of the moment of momentum (Cauchy’s second law of motion) dictates the symmetry of the Cauchy stress tensor, that is, ij ⫽ ji. Furthermore, in the deformed conﬁguration, Cauchy’s ﬁrst law of motion yields the equilibrium equation ⭸ji ⫹ ƒi ⫽ 0 ⭸xj

or ⵜ ⫹ f ⫽ 0,

(2.2.1)

where ƒi is the body force per unit volume in the deformed conﬁguration. Equation (2.2.1) is valid for any material point within a continuum body. For a material point on the surface (boundary) of the a continuum (see Fig. 2.2), the following Cauchy formula applies:

16

BASIC EQUATIONS OF CONTINUUM MECHANICS

S

n p

x

x3

V x1

x2

Figure 2.2 Cauchy formula on the deformed (current) surface.

ij nj兩S ⫽ pi

or n兩S ⫽ p,

(2.2.2)

where, as shown in Figure 2.2, ni is the unit outward normal vector of the surface S and pi is the traction vector applied on S. Note that pi is measured as force per unit deformed area. Note that (2.2.1) describes the equilibrium of an inﬁnitesimal material element in the deformed conﬁguration. The Cauchy stress tensor is typically written as a function of the Eulerian spatial coordinates xi. To describe the equilibrium in the initial (undeformed) conﬁguration, the Piola–Kirchhoff stress tensors may be introduced. The ﬁrst Piola–Kirchhoff stress tensor, 0Ij, is deﬁned as the actual force in the deformed conﬁguration per unit undeformed area in the undeformed conﬁguration, while the second Piola–Kirchhoff stress tensor, ˜ IJ, is deﬁned as a ﬁctitious force in the undeformed conﬁguration per unit undeformed area in the undeformed conﬁguration. The ﬁctitious force here is obtained by transforming the actual force in the deformed conﬁguration back to the undeformed conﬁguration, which is equivalent to premultiplying the actual force in the deformed conﬁguration by the spatial deformation gradient tensor, F⫺1 Ij . Hence, the two Piola–Kirchhoff stresses are related by the deformation gradient tensors: ⫺1 0 ˜ IJ ⫽ FJk Ik

or Ij0 ⫽ ˜ IKFjK.

(2.2.3)

The Piola–Kirchhoff stresses are typically written as functions of the Lagrangian material coordinates Xi. They can be related to the Cauchy stress tensor by ⫺1 0Ij ⫽ JFIk kj,

or

⫺1 ⫺1 ˜ IJ ⫽ JFIk FJm km

(2.2.4)

2.2

ij ⫽

STRESSES AND EQUILIBRIUM

1 1 FiKFjM ⫽ ˜ KM ⫽ FiK 0Kj, J J

17

(2.2.5)

where J is the Jacobian given by J ⫽ 兩⭸xi / ⭸Xj兩 ⫽ 0 / , and 0 and are the mass density measured in the initial reference state and the current deformed state, respectively. It is seen from (2.2.4) that ˜ IJ is symmetric while 0Ij is generally nonsymmetric. It is important to keep in mind that the Piola–Kirchhoff stress tensors are not actual stresses, that is, they do not exist in the continuum under consideration. They are introduced to simplify the equilibrium equation in the initial conﬁguration, namely, ⭸ 0Ji ⫹ ƒ0 ⫽ 0 ⭸XJ

or

⭸(˜ JKFiK) ⫹ ƒ0 ⫽ 0, ⭸XJ

(2.2.6)

where ƒ0 is the body force per unit volume in the initial conﬁguration. The Cauchy formula given by (2.2.2) can also be expressed in the initial conﬁguration, 0Ji NJ ⫽ FiJ p˜ J,

˜ JI Nj ⫽ FIj⫺1 pj0,

(2.2.7)

where p0j ⫽

dS p, dS0 j

p˜ J ⫽

dS ⫺1 F p, dS0 Jk k

(2.2.8)

and dS0 is an area element in the initial conﬁguration, and dS is the same area element in the deformed conﬁguration. Note that pj is the force acting on the deformed surface per unit deformed area. Therefore, p0j is the force acting on the deformed surface per unit undeformed area, while p˜ J is a ﬁctitious force acting on the deformed surface per unit undeformed area. This ﬁctitious force is the actual force acting on 0 the deformed surface transformed by F⫺1 ˜ J is a real Jk . Neither of pj and p traction vector. They are called pseudotraction vectors introduced to accommodate the pseudostress tensors. For small deformation, that is, 兩⭸ui / ⭸XJ兩 ⬍⬍ 1 and 兩⭸ui / ⭸xj兩 ⬍⬍ 1, one can show from (2.1.5) that when the same coordinate system is used for both the Lagrangian and Eulerian conﬁgurations,

18

BASIC EQUATIONS OF CONTINUUM MECHANICS

Fij ⬇ ␦ij ⫹

⭸ui ⭸Xj

and J ⫽

冏 冏

⭸xi ⭸u ⬇ 1 ⫹ i. ⭸Xj ⭸Xj

(2.2.9)

Thus, it follows from (2.2.4) that Piola–Kirchhoff stresses reduce to the Cauchy stress, ij ⫽ ˜ ij ⫽ ij0

(2.2.10)

for small deformation. Furthermore, the distinction between ni and Ni and between dS and dS0 can also be neglected. Thus, the pseudotraction vectors reduce to the Cauchy traction vector as well.

2.3 ENERGY, WORK, AND THERMODYNAMIC POTENTIALS

We ﬁrst review some of the integral identities from mathematical physics. Consider region D bounded by the surface S. The outward unit normal vector of S is denoted by ni; see Figure 2.3. Let ƒ(x1, x2, x3) be a continuously differentiable scalar function deﬁned in D. The Green’s theorem states that

冕 ⭸⭸xƒ dV ⫽ 冕 ƒn dS. D

S

i

(2.3.1)

i

Let ui(x1, x2, x3) be a continuously differentiable vector function deﬁned in D. The divergence theorem states that

冕 ⭸⭸ux dV ⫽ 冕 u n dS i

D

i

S

i

i

or

冕 ⵜu dV ⫽ 冕 u • n dS D

(2.3.2)

S

Next consider a simple, closed, and smooth curve L. Let S be any smooth surface spanned across the closed curve. The tangential direction of the curve and the normal direction of the surface are denoted S

n

D

Figure 2.3 Region D bounded by the surface S.

2.3

ENERGY, WORK, AND THERMODYNAMIC POTENTIALS

19

by ti and ni, respectively. To get the positive orientation of L think of yourself as walking along the curve. While you are walking along the curve if your head is pointing in the same direction as the unit normal vectors of the surface while the surface is on the left, then you are walking in the positive direction on L; see Figure 2.4. Now, let ui(x1, x2, x3) be a continuously differentiable scalar function deﬁned on the surface S. The Stokes’ theorem states that

冕 u S

ijk k, j

ni dS ⫽

冕 u t dL L

i i

or

冕 (ⵜ ⫻ u) • n dS ⫽ 冕 u • t dL, S

L

(2.3.3) where ijk is the permutation symbol. Note that (2.3.1)–(2.3.3) are mathematical identities. They are true regardless of the physical interpretation of the functions involved. Nevertheless, when properly interpreted, these integral identiﬁes may be used to state the conservation of certain physical entities. Now, let us consider the energy of a continuum. Generally speaking, the total energy of a continuum is comprised of two parts, the kinetic energy and the internal energy. The kinetic energy is associated with the macroscopically observable motion of the continuum. Usually, the kinetic energy of the random thermal agitation of the atoms is considered part of the internal energy associated with the temperature of the continuum. The other part of the internal energy may include stored strain energy and possibly other forms of energy, such as chemical, electrical, and optical energies. Let be the mass density and be the internal energy per unit mass or speciﬁc internal energy for a continuum in the current (deformed) conﬁguration. The ﬁrst law of thermodynamics in conjunction with the divergence theorem leads to the following energy equation (Malvern, 1969):

n

S t

L

Figure 2.4 Stokes’ theorem.

20

BASIC EQUATIONS OF CONTINUUM MECHANICS

d ⭸q ⫽ ij Dij ⫹ r ⫺ i, dt ⭸xi

(2.3.4)

where ij is the Cauchy stress tensor, Dij is the rate of deformation tensor, r is the distributed internal heat source per unit mass, and qi is the (outward) heat ﬂux vector. The ﬁrst term on the right-hand side of (2.3.4) is called stress power. It represents the power input per unit deformed volume provided by the stress ﬁeld. The last two terms of the right-hand side represent the total heat input from internal heat source and external heat ﬂux. Together, the right-hand side of (2.3.4) gives the total energy input, while the left-hand side shows the time rate of change of internal energy. Therefore, (2.3.4) is a mathematical statement of conservation of energy. The quantity of particular interest to us is the stress power, ij Dij. In a volume V of the deformed conﬁguration, the stress power is given by

冕D V

ij

ij

dV.

(2.3.5)

This can be converted to the initial reference conﬁguration in terms of the Piola–Kirchhoff stress tensors:

冕D V

ij

ij

dV ⫽

冕

V0

0Ij

dFjI dV0 ⫽ dt

冕

V0

˜ IJ

dEIJ dV0. dt

(2.3.6)

For this reason, we call (ij, Dij) a conjugate pair in the current deformed conﬁguration, and ( 0Ij, dFjI /dt) and (˜ IJ, dEIJ /dt) conjugate pairs in the initial reference conﬁguration. In computing the energy, we must use variables that form a conjugate pair in the same conﬁguration. We are now ready to introduce the thermodynamic potentials. The fundamental assumption here is that the internal energy per unit mass of a continuum can be uniquely determined by the speciﬁc entropy s, and some state variables i, that is, ⫽ (s, 1, 2, . . . , n).

(2.3.7)

This is called the caloric equation of state, and is, therefore, a thermodynamic potential. From here, one can deﬁne the thermodynamic temperature and thermodynamic forces, respectively:

2.3

T⫽

ENERGY, WORK, AND THERMODYNAMIC POTENTIALS

冉冊 ⭸ ⭸s

冉冊

21

⭸ . ⭸i s

(2.3.8)

ds ⫽ i di ⫹ T ds.

(2.3.9)

and i ⫽

i

These yield d ⫽

冉冊 ⭸ ⭸i

di ⫹

s

冉冊 ⭸ ⭸s

i

For adiabatic (r ⫺ qi,i ⫽ 0) and isentropic (ds ⫽ 0) deformation, and for isothermal (dT ⫽ 0) deformation with reversible heat transfer (r ⫺ qi,i ⫽ T ds/dt), the work of the thermodynamic forces is recoverable, and the rate of work of the thermodynamic forces equals the stress power: i

di ⫽ ij Dij. dt

(2.3.10)

Thus, in these cases, the rate of change of the internal energy is given by

d ds ⫽ ij Dij ⫹ T . dt dt

(2.3.11)

In the reference conﬁguration, this takes the form d 1 dEIJ ds ⫽ ˜ ⫹T . dt 0 IJ dt dt

(2.3.12)

Other thermodynamic potentials used often in continuum mechanics are: Enthalpy: Helmholtz free energy: Gibbs free energy:

⫽ ⫺ ii.

h ⫽ ⫺ sT. g ⫽ ⫺ sT ⫺ ii.

(2.3.13) (2.3.14) (2.3.15)

22

BASIC EQUATIONS OF CONTINUUM MECHANICS

2.4

CONSTITUTIVE LAWS

Constitutive laws are used to describe material behavior when subjected to applied thermomechanical loads. One of the major areas of micromechanics is to develop constitutive laws for heterogeneous materials under various thermomechanical loading conditions. For real materials, their thermomechanical behavior can be rather complex. It is usually not feasible to write down one or a set of equations to describe the entire range of material behavior. Instead, we formulate separately constitutive equations describing various kinds of idealized material response, each of which is a mathematical formulation designed to approximate physical observations of a real material’s response over a suitably restricted range. Speciﬁcally, constitutive laws for ideal materials are prescribed by equations that establish the relationship between deformation and the internal stresses in the material. For example, G(ij, Dij) ⫽ 0

(2.4.1)

describes a relationship between the Cauchy stress tensor and the rate of deformation tensor. In what follows, we will describe some commonly used constitutive laws governing certain idealized material behavior. Elasticity

If there exists a potential function W of strain for a given material such that the stress in the material is related to the strain by ˜ IJ ⫽

⭸W , ⭸EIJ

(2.4.2)

then the material is called an elastic (or hyperelastic) material, and such material behavior is called elasticity. Equation (2.4.2) is the constitutive equation for elastic materials. For elastic material under isothermal and isentropic conditions, the Helmholtz free energy can be taken as the elastic potential W ⫽ 0h, that is, ˜ IJ ⫽

⭸W ⭸h ⭸ ⫽ 0 ⫽ 0 . ⭸EIJ ⭸EIJ ⭸EIJ

Thus, ˜ IJ / 0 is the thermodynamic force conjugate to EIJ.

(2.4.3)

2.4

CONSTITUTIVE LAWS

23

Another consequence of the elastic potential is that the state of deformation is uniquely determined by the state variables. In the isothermal case, the state variables are the strain components. The stress ﬁeld corresponding to a strain ﬁeld is unique regardless how that state of strain is arrived. In other words, the deformation is history independent. Consequently, upon unloading, an elastic material recovers its original state or shape and size. Since W is assumed to be a function of strain only, it can also be interpreted as the strain energy per unit undeformed volume. In the initial reference conﬁguration, the Taylor expansion of W can be written as W ⫽ W0 ⫹ cIJ EIJ ⫹ –21 LIJKLEIJ EKL ⫹ –61 cIJKLMNEIJ EKLEMN ⫹ , (2.4.4) where, traditionally, LIJKL are called the second-order elastic constants and cIJKLMN are called the third-order elastic constants. The constants W0 and cIJ are typically zero unless, for example, when residual stress exists in the initial reference conﬁguration. A material is said to behave linear elastically if the higher order terms in (2.4.4) can be neglected and the stresses are linearly related to the strains. In the undeformed conﬁguration, the constitutive equation for linear elastic materials can be written in terms of the second Piola–Kirchhoff stress tensor and the Lagrangian ﬁnite strain tensor, ˜ IJ ⫽ LIJKLEKL

or EIJ ⫽ MIJKL˜ KL,

(2.4.5)

where the fourth-order tensor LIJKL is called the elasticity (or stiffness) tensor, and MIJKL is the compliance tensor, which is the inverse of the stiffness tensor, that is, MIJMNLMNKL ⫽ IIJKL ⬅ –21 (␦IK␦JL ⫹ ␦IL␦JK),

(2.4.6)

where ␦IJ is the Kronecker delta: ␦IJ ⫽

再

1 for I ⫽ J . 0 for I ⫽ J

(2.4.7)

Most engineering materials show linear elastic behavior only when the deformation is very small. In this case, the small-strain constitutive

24

BASIC EQUATIONS OF CONTINUUM MECHANICS

law for linear elastic materials can be written in terms of the Cauchy stress tensor and the inﬁnitesimal strain tensor: ij ⫽ Lijklkl

or ij ⫽ Mijklkl.

(2.4.8)

The above equation is often referred to as the generalized Hooke law. For linear elastic materials, it is sometime convenient to write the Hooke law in terms of the Voigt elastic constants: ⫽ C,

(2.4.9)

where

⫽

冤冥 冤冥 11 22 33 , 23 31 12

⫽

11 22 33 , 223 231 212

(2.4.10)

and the elements of the 6 ⫻ 6 stiffness matrix C are called the (Voigt) elastic constants. They are related to the components of stiffness tensor L through the relationship shown in Table 2.1. Both the stiffness and compliance tensors are fourth-order tensors. They obey the tensor transformation law, Lˆ ijkl ⫽ ␣im␣jn␣kp␣lqLmnpq,

ˆ ijkl ⫽ ␣im␣jn␣kp␣lqMmnpq, M

(2.4.11)

ˆ ijkl are the components of the stiffness and compliance where Lˆ ijkl and M tensors, respectively, in the xˆ i coordinate system, which is related to the original xi coordinate system by the rotation tensor ␣ij through Table 2.1

Relationship between Lijkl and Cij

Lijkl

kl

ij

11

22

33

23

31

12

11 22 33 23 31 12

C11 C21 C31 C41 C51 C61

C12 C22 C32 C42 C52 C62

C13 C23 C33 C43 C53 C63

C14 C24 C34 C44 C54 C64

C15 C25 C35 C45 C55 C65

C16 C26 C36 C46 C56 C66

2.4

CONSTITUTIVE LAWS

xˆ i ⫽ ␣ij xj.

25

(2.4.12)

For the Voigt elasticity matrix, if the coordinate transformation is a rotation about the x3 axis by an angle , one can show that (Ting, 1996), ˆ ⫽ ⍀C⍀T, Sˆ ⫽ (⍀⫺1)T S⍀⫺1, C

(2.4.13)

where

冤

m2 n2 0 ⍀⫽ 0 0 ⫺mn

n2 m2 0 0 0 mn

0 0 0 0 0 0 1 0 0 0 m ⫺n 0 n m 0 0 0

2mn

⫺2mn

0 0 0

m2 ⫺ n2

冥

(2.4.14)

in which m ⫽ cos , n ⫽ sin . The stiffness tensor of a linear elastic material is positive deﬁnite and possesses the following symmetries: Lijkl ⫽ Lklij ⫽ Ljikl.

(2.4.15)

Because of these symmetries, there are 81 independent components called elastic constants in the most general case. The number of independent components of the stiffness tensor is much less when the material possesses certain symmetries. For example, for materials with cubic symmetry, such as face-center-cubic (FCC) and body-centercubic (BCC) crystals, the stiffness tensor has only three independent components: Lijkl ⫽ ␦ij␦kl ⫹ (␦ik␦jl ⫹ ␦il␦jk) ⫹ dijkl,

(2.4.16)

where , , and are related to the Voigt constants by ⫽ C12,

⫽ C44,

⫽ C11 ⫺ C12 ⫺ 2C44.

(2.4.17)

The symbol dijkl is deﬁned by the following: d1111 ⫽ d2222 ⫽ d3333 ⫽ 1,

others ⫽ zero.

(2.4.18)

For isotropic materials, there are only two independent components in the stiffness tensor, that is,

26

BASIC EQUATIONS OF CONTINUUM MECHANICS

Lijkl ⫽ ␦ij␦kl ⫹ (␦ik␦jl ⫹ ␦il␦jk),

(2.4.19)

where the Lame constants and are related to the Voigt constants by ⫽ C12,

⫽ C44.

(2.4.20)

In some cases, it is more convenient to rewrite (2.4.19) as Lijkl ⫽ K␦ij␦kl ⫹ (␦ik␦jl ⫹ ␦il␦jk ⫺ –23 ␦ij␦kl),

(2.4.21)

where K and are the bulk and shear moduli, respectively. The corresponding compliance tensor is given by Mijkl ⫽

1 1 ␦ij␦kl ⫹ (␦ ␦ ⫹ ␦il␦jk ⫺ –23 ␦ij␦kl). 9K 4 ik jl

(2.4.22)

Using the symbolic notation (1.4.2), the isotropic stiffness tensor and compliance tensor can be written as L ⫽ (3K, 2),

M⫽

冉

冊

1 1 , . 3K 2

(2.4.23)

Other elastic constants such as Young’s modulus, Poisson’s ratio, the shear modulus, and so forth, are also commonly used for isotropic materials. The relationships among the various elastic constants for isotropic materials are given in Appendix 2.A. The Voigt elastic constants for materials with other types of symmetries are listed in Appendix 2.B. Thermoelasticity

In addition to mechanical stresses, temperature change may also cause deformation in a continuum. Vice versa, deformation of a continuum may cause the temperature in the continuum to change. Such temperature effects in elastic materials are described by thermoelastic constitutive laws. Some commonly used thermoelastic constitutive laws are presented here. We assume that, at the temperature T0, the continuum is stress free in the initial reference state. In the deformed (current) state, let the temperature be T. The Helmholtz free energy is given by (2.3.14)

2.4

CONSTITUTIVE LAWS

27

h(EIJ, T) ⫽ (EIJ, T) ⫺ Ts(EIJ, T),

(2.4.24)

dh ⭸h dEIJ ⭸h dT d dT ds ⫽ ⫹ ⫽ ⫺s ⫺T . ⭸EIJ dt ⭸T dt dt dt dt dt

(2.4.25)

or

Making use of (2.3.12) and (2.3.11) in the above, we have

冉

s⫹

冊

⭸h ⭸T

冉

冊

dT 1 ⭸h dEIJ ⫺ ˜ IJ ⫺ ⫽ 0. dt 0 ⭸EIJ dt

(2.4.26)

Since EIJ and T are independent state variables, satisfaction of the above equation means ⭸h , ⭸T

s⫽⫺

˜ IJ ⫽ 0

⭸h . ⭸EIJ

(2.4.27)

The difference between the second of (2.4.27) and (2.4.3) is that the Helmholtz free energy in (2.4.27) is a function of both strain and temperature. The Taylor expansion of the Helmholtz free energy in terms of strains and temperature can be written as 0h ⫽ h0 ⫹ cIJ EIJ ⫹ –21 LIJKLEIJ EKL ⫹ ␣ ⌬T ⫹ –21  ⌬T 2 ⫺ ␣KLLIJKLEIJ ⌬T .

(2.4.28)

For convenience, we have used ⌬T ⫽ T ⫺ T0.

(2.4.29)

It thus follows that ⭸h 1 ⫽ ⫺ (␣ ⫹  ⌬T ⫹ ␣IJ EIJ ), ⭸T 0

s⫽⫺ ˜ IJ ⫽ 0

⭸h ⫽ cIJ ⫹ LIJKLEKL ⫺ LIJKL␣KL ⌬T . ⭸EIJ

(2.4.30)

(2.4.31)

28

BASIC EQUATIONS OF CONTINUUM MECHANICS

Equation (2.4.31) is the stress–strain relationship in thermoelasticity. The constant term cIJ is usually zero unless initial stresses are present. The fourth-order tensor LIJKL is the second-order elasticity tensor introduced in (2.4.4). The second-order tensor ␣IJ is called the linear coefﬁcient of thermal expansion. The quantity E*KL ⫽ ␣KL ⌬T

(2.4.32)

corresponds to the deformation due to temperature change. We will call it thermal strain. Note that although (2.4.31) provides the stress–strain relationship, it is not a complete description of the constitutive law for thermoelasticity. In thermoelasticity, in addition to stresses and strains, temperature is also an unknown ﬁeld quantity that needs to be solved simultaneously with the deformation. Therefore, the complete constitutive law of thermoelasticity should also include (2.4.30), which will provide the constitutive relation for heat conduction in the continuum. Such coupled deformation and temperature problems are rather difﬁcult to solve. Fortunately, in most engineering applications, the effect of deformation on the temperature ﬁeld is negligible. Therefore, one can solve for the temperature ﬁeld ﬁrst by solving the heat conduction problem independent of the deformation. Once the temperature ﬁeld is known, the only constitutive relation needed for solving the deformation problem in thermoelastic materials is (2.4.31). Such approach that decouples the heat conduction and thermoelasticity into two separate problems is often used in engineering applications. In case of small strain deformation, the linear thermoelastic stress– strain relationship can be written as ij ⫽ Lijkl(kl ⫺ *), kl

(2.4.33)

where the thermal strain *kl is given by * kl ⫽ ␣kl⌬T.

(2.4.34)

If the material is isotropic (both elastically and thermally), the elastic stiffness tensor Lijkl is given by (2.4.21), and the coefﬁcient of thermal expansion is given by ␣ij ⫽ ␣␦ij,

(2.4.35)

2.4

CONSTITUTIVE LAWS

29

where ␣ is the isotropic coefﬁcient of thermal expansion. Thus, the small-strain constitutive law for isotropic thermoelastic material can be written as ij ⫽ (K ⫺ –23 )(kk ⫺ 3␣ ⌬T)␦ij ⫹ 2ij.

(2.4.36)

Viscoelasticity

Viscoelastic constitutive laws are used to describe the time-dependent characteristics of material deformation. In this section, we will limit ourselves to small-strain deformation and linear viscoelasticity theories. In this case, a commonly used stress–strain relationship is given by

冕G t

ij(t) ⫽ Gijkl(t)kl(0) ⫹

(t ⫺ s)

ijkl

0

dkl(s) ds, ds

(2.4.37)

where ij(t) is the time-dependent strain tensor and Gijkl(t) is called the relaxation function. It has been assumed that for t ⬍ 0, both ij(t) and Gijkl(t) are zero, that is, ij(t) ⫽ 0 and Gijkl(t) ⫽ 0 for t ⬍ 0. Further, the symmetry of the stress and strain tensors implies Gijkl(t) ⫽ Gjikl(t) ⫽ Gijlk(t).

(2.4.38)

Under constant strain kj(t) ⫽ kj(0), we have dkl(t)/dt ⫽ 0. Thus, (2.4.37) reduces to ij(t) ⫽ Gijkl(t)kj(0).

(2.4.39)

This is the reason that Gijkl(t) is termed a relaxation function, for it represents the stress relaxation under constant strain. Alternative to (2.4.37), the viscoelastic stress–strain law can also be written as

冕J t

ij(t) ⫽ Jijkl(t)kl(0) ⫹

0

(t ⫺ s)

ijkl

dkl(s) ds, ds

(2.4.40)

where it has been assumed that for t ⬍ 0, both ij(t) and Jijkl(t) are zero, that is, ij(t) ⫽ 0 and Jijkl(t) ⫽ 0 for t ⬍ 0. The fourth-order tensor function Jijkl(t) is called the creep function because under constant stress kj(t) ⫽ kj(0), we have dkl(t)/dt ⫽ 0. Thus, it follows from (2.4.40) that

30

BASIC EQUATIONS OF CONTINUUM MECHANICS

ij(t) ⫽ Jijkl(t)kj(0).

(2.4.41)

Now, consider the Laplace transform ៣

ƒ(s) ⫽

冕

⬁

ƒ(t)e⫺st dt.

(2.4.42)

0

Note that

冕 冋冕 ƒ(t ⫺ s)g(s) ds册e ⬁

t

0

0

⫺st

冕

⬁

0

៣

៣

dt ⫽ ƒ(s)g(s),

dg(s) ⫺st ៣ e dt ⫽ sg(s) ⫺ g(0). ds

(2.4.43)

(2.4.44)

Applying the Laplace transform to both sides of (2.4.37)–(2.4.40) and making use of the above equations, we obtain ៣ ៣ ៣ ij(t) ⫽ sGijkl(s) kl(s)

៣ ៣ ៣ ij(t) ⫽ sJ ijkl(s)kl(s).

and

(2.4.45)

It thus follows that ៣

៣

sGijkl(s) ⫽ [sJ ijkl(s)]⫺1.

(2.4.46)

We see that, in the Laplace transform space, (2.4.45) is very similar to the linear elastic constitutive law (Hooke’s law). The function ៣ sGijkl(s) can be viewed as the ‘‘stiffness tensor’’ of the viscoelastic ៣ material in the Laplace transform space, while sJ ijkl(s) is the ‘‘compliance tensor.’’ Note that it is generally not true that Gijkl(t) ⫽ [Jijkl(t)]⫺1, although one can show that (Christensen, 1982) lim Gijkl(t) ⫽ lim [Jijkl(t)]⫺1 t→0

t→0

and

lim Gijkl(t) ⫽ lim [Jijkl(t)]⫺1. t→⬁

t→⬁

(2.4.47) When the material is isotropic, the relaxation and creep functions can be written as

2.4

CONSTITUTIVE LAWS

31

Gijkl(t) ⫽ –13 [Gb(t) ⫺ Gs(t)] ⫹ –12 Gs(t)(␦ik␦jl ⫹ ␦il␦jk),

(2.4.48)

Jijkl(t) ⫽ –31 [Jb(t) ⫺ Js(t)] ⫹ –21 Js(t)(␦ik␦jl ⫹ ␦il␦jk),

(2.4.49)

where Gs(t) and Gb(t) are, respectively, the shear and bulk relaxation functions, while Js(t) and Jb(t) are the shear and bulk creep functions, respectively. Making use of the above in (2.4.37) and (2.4.40), respectively, leads to ⬘ij(t) ⫽ Gs(t)⬘ij(0) ⫹

冕 G (t ⫺ s) d⬘ds(s) ds,

(2.4.50)

kk(t) ⫽ Gb(t)kk(0) ⫹

冕 G (t ⫺ s) dds(s) ds,

(2.4.51)

⬘ij(t) ⫽ Js(t)ij(0) ⫹

冕 J (t ⫺ s) dds⬘(s) ds,

(2.4.52)

kk(t) ⫽ Jb(t)kk(0) ⫹

冕 J (t ⫺ s) dds(s) ds.

(2.4.53)

t

ij

s

0

t

kk

b

0

and t

0

ij

s

t

kk

0

b

In the Laplace transform space, these stress–strain relationships can be written as ៣ ៣ ៣ ⬘ij(s) ⫽ sGs(s) ⬘kl(s),

៣ ៣ ៣ kk(s) ⫽ sGb(s) kk(s)

(2.4.54)

៣ ៣ ៣ ⬘ij(s) ⫽ sJ s(s)⬘ij(s),

៣ ៣ ៣ ⬘kk(s) ⫽ sJ b(s)⬘kk(s),

(2.4.55)

and

៣

៣

where ⬘ij(s) and ij⬘ (s) are the deviatoric strain and deviatoric stress tensors in the Laplace transform space, respectively, Plasticity

For many engineering materials, particularly, metallic materials, deformation becomes permanent once the strain goes beyond the elastic

32

BASIC EQUATIONS OF CONTINUUM MECHANICS

limit. Although the mechanisms causing such permanent deformation are rather complex, the macroscopic behavior can be approximately represented by certain functions called elastic-plastic constitutive laws. More detailed and in-depth discussions of elastic-plastic constitutive laws will be given in Chapters 11–13. Here, we will only outline the basic ideas of some commonly used constitutive laws for idealized elastic-plastic materials. For a material to be plastically deformed, certain combinations of the stress components, called the effective stress, must be larger than a threshold value, which is typically called the yield strength of the material. When the effective stress is below the yield strength, the material behaves linear elastically, and the linear elastic constitutive law can be used. When the effective stress is above the yield strength, the material behaves plastically, and elastic-plastic constitutive laws are needed to describe the postyield behavior. Thus, elastic-plastic constitutive laws typically consist of a yield criterion and a function to describe the postyield stress–strain relationship. The latter is called the ﬂow rule; for plastic deformation it is called historically plastic ﬂow. It is assumed that, for a given state of a material, there exists a function ƒ(ij) called the yield function such that the material behaves elastically if ƒ(ij) ⬍ 0,

or

ƒ(ij) ⫽ 0

and

⭸ƒ dij ⬍ 0, ⭸ij dt

(2.4.56)

and the material behaves plastically if ƒ(ij) ⫽ 0

and

⭸ƒ dij ⱖ 0. ⭸ij dt

(2.4.57)

The above yield criterion can be understood as follows. The equation ƒ(ij) ⫽ 0 deﬁnes a yield surface in the stress space. It is one of the basic assumptions in plasticity that the yield surface is a closed concave surface enclosing the origin of the stress space. Therefore, we can speak of its inside and outside. For a stress state inside the yield surface, we have ƒ(ij) ⬍ 0. The stress is not high enough to yield the material yet, and the deformation is elastic. When the stress state reaches the yield surface, that is, ƒ(ij) ⫽ 0, the situation is not unique. It depends on whether, at the next moment, the stress state is moving out of or moving back inside the yield surface. Note that ⭸ƒ/ ⭸ij is an outward (not

2.4

CONSTITUTIVE LAWS

33

necessarily unit) vector of the yield surface, and dij /dt is the direction of stress increment. Therefore, (⭸ƒ/ ⭸ij)(dij /dt) ⱖ 0 means that the direction of stress increment at the next moment is moving out of the yield surface, thus plastic yielding occurs. On the other hand, (⭸ƒ/ ⭸ij)(dij /dt) ⬍ 0 means that the stress state is moving back inside the yield surface; thus the deformation is elastic. The most commonly used yield functions are the von Mises yield function ƒ(ij) ⫽ J2 ⫺ k2,

(2.4.58)

and the Tresca yield function ƒ(ij) ⫽ 4J 23 ⫺ 27J 32 ⫺ 36J 22 ⫹ 96k4J2 ⫺ 64k6,

(2.4.59)

where k is a material constant (yield strength in pure shear), and J2 ⫽ –21 ⬘ijij⬘ ,

J3 ⫽ –31 ⬘ij⬘jk⬘ki,

(2.4.60)

are called, respectively, the second and third invariants of the deviatoric stress tensor ⬘ij ⫽ ij ⫺ –31 kk␦ij.

(2.4.61)

For other types of yield functions, the readers are referred to the References and Suggested Reading at the end of this chapter. Among the many ﬂow rules for postyield behavior, the simplest one is the Levy–Mises perfectly plastic constitutive law. It assumes that postyield deformation is incompressible and fully characterized by the rate of deformation tensor, which is related to the deviatoric Cauchy stress tensor through ⬘ij ⫽

k兹2 兹DmnDmn

Dij,

Dkk ⫽ 0.

(2.4.62)

Together, the yield conditions (2.4.56) and (2.4.57) and the postyield stress–strain relationship (2.4.62) form a constitutive law to describe mechanical behavior of an elastic–perfectly plastic material. Note that such simple constitutive law is rather limited in its application to real engineering materials because (1) it assumes that plastic deformation

34

BASIC EQUATIONS OF CONTINUUM MECHANICS

does not produce any volume change (incompressibility), and (2) it assumes no work hardening. More realistic constitutive laws for elasticplastic materials will be discussed in Chapters 10–13.

2.5 BOUNDARY VALUE PROBLEMS FOR SMALL-STRAIN LINEAR ELASTICITY

For the remaining part of this chapter, we will focus on linear elastic material under small-strain deformation. As discussed in previous sections, the distinction between the reference and current conﬁgurations can be neglected when the deformation is small. Therefore, for such small deformation, we will not distinguish the different types of stress and strain measures, nor do we need to distinguish the spatial coordinate from the material coordinate. Instead, for convenience, we will simply use ij for stress and ij for strain, and xi for coordinates. Now, consider a continuum of volume V and surface S (see Fig. 2.5). The total surface S may be divided into S ⫽ Su ⫹ S , where it is assumed that the displacements are prescribed on Su and the traction is prescribed on S , that is, ui兩Su ⫽ u (0) i

(2.5.1)

ij nj兩S ⫽ p(0) i ,

(2.5.2)

where u (0) and p i(0) are given values of displacement and traction on Su i and S , respectively. Within the domain V, the stress must satisfy the equilibrium equation (2.2.1),

Sσ

n V

Su

Figure 2.5 An elastic body V in the undeformed conﬁguration.

2.6

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

ji, j ⫹ ƒi ⫽ 0

in V

35

(2.5.3)

where ƒi is the body force per unit volume. Combining (2.5.1), (2.5.2), and (2.5.3) in conjunction with Hooke’s law, we arrive at the following boundary value problem: ji, j ⫹ ƒi ⫽ 0

in V,

(2.5.4)

ij ⫽ Lijkluk,l

in V,

(2.5.5)

ui兩Su ⫽ u i(0),

(2.5.6)

ij nj兩S ⫽ p(0) i .

(2.5.7)

This is a well-posed boundary value problem with nine unknowns (six stress components plus three displacement components) and nine equations. Theoretically speaking, for a given set of functions u (0) and p i(0) i on S, and a given function ƒi in V, the stresses and displacements in V can be uniquely determined by solving the above boundary value problem. In most cases, numerical methods by computers are needed to obtain the solutions. Making use of Hooke’s law, the stress tensor can be eliminated from the above boundary value problem. Thus we have alternatively, Lijkluk,lj ⫹ ƒi ⫽ 0

in V,

(2.5.8)

ui兩Su ⫽ u i(0),

(2.5.9)

Lijkluk,lnj兩S ⫽ p(0) i .

(2.5.10)

2.6 INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

Let us ﬁrst consider a boundary value problem in an unbounded domain V comprised of a homogeneous linear elastic material with elasticity tensor Lijkl. We assume that the body force ƒi is localized, that is, ƒi → 0

as x 21 ⫹ x 22 ⫹ x 23 → ⬁.

and the entire boundary (at inﬁnity) is traction free, that is,

(2.6.1)

36

BASIC EQUATIONS OF CONTINUUM MECHANICS

Lijkluk,lnj兩S ⫽ pi(0) → 0

as x 21 ⫹ x 22 ⫹ x 23 → ⬁.

(2.6.2)

Under these conditions, the displacement ui should satisfy the following boundary value problem: Lijkluk,lj ⫹ ƒi ⫽ 0 ui → 0

in V,

as x 12 ⫹ x 22 ⫹ x 32 → ⬁.

(2.6.3) (2.6.4)

Several approaches can be used to solve this problem. We will use the Fourier transform method. The one-dimensional Fourier transform is deﬁned by the following integrals: gˆ () ⫽

1 2

g(x) ⫽

冕

⬁

⫺⬁

冕

⬁

g(x)e⫺ix dx,

gˆ ()eix d,

⫺⬁

(2.6.5)

(2.6.6)

where i ⫽ 兹⫺1 and gˆ () is used to denote the Fourier transform of g(x). In three-dimensional space, the Fourier transform may be deﬁned by the following pair of integrals: gˆ () ⫽

冕

⬁

1 (2)3

g(x) ⫽

⫺⬁

冕

⬁

⫺⬁

g(x)e⫺ix dx

gˆ ()eix d

(2.67)

(2.6.8)

where x ⫽ (x1, x2, x3),

⫽ (1, 2, 3),

(2.6.9)

and the integrals in (2.6.7) and (2.6.8) are over the entire threedimensional space, while dx and d are volume elements in the x space and the space, respectively. If g(x) → 0 as 兩x兩 → ⬁, then by integration by parts, we have

2.6

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

1 (2)3

冕

⬁

⫺⬁

⭸g(x) ⫺ix e dx ⫽ ijgˆ (). ⭸xj

37

(2.6.10)

Next, multiply both sides of (2.5.8) by e⫺ix /(2)3 and integrate: Lijkl

再

1 (2)3

冕

⬁

⫺⬁

冎

uk,lj(x)e⫺ix dx ⫹

1 (2)3

冕

⬁

⫺⬁

ƒi(x)e⫺ix dx ⫽ 0. (2.6.11)

Since ui vanishes at inﬁnity, (2.6.10) can be used in (2.6.11) to yield Lijkl(il)(ij)ˆuk() ⫹ ƒˆ i() ⫽ 0,

(2.6.12)

where uˆ k and ƒˆ i are the Fourier transforms of and uk and ƒi, respectively. Equation (2.6.12) can also be written as Kikuˆ k ⫽ ƒˆ i,

(2.6.13)

where the dependence of uˆ k and ƒˆ i on is implied without writing it out explicitly as an argument, and Kik ⫽ Kik() ⫽ Lijkllj.

(2.6.14)

It then follows from (2.6.13) that uˆ i ⫽ ƒˆ j Nij()/D(),

(2.6.15)

Nij() ⫽ –21 ikljmnKkm()Kln(),

(2.6.16)

D() ⫽ mnlKm1()Kn2()Kl3(),

(2.6.17)

where

and ijk is the permutation tensor introduced in (1.4.15). Note that Nij is the cofactor of Kij and D is the determinant of Kij. Therefore, Nij /D is the inverse of Kij. Expressions of Nij and D for isotropic, cubic, and transversely isotropic materials are given in Appendix 2.C. Equation (2.6.15) means that uˆ i is known explicitly as a function of once the stiffness tensor L and the body force f are known. The

38

BASIC EQUATIONS OF CONTINUUM MECHANICS

displacement in the physical space (the x space) can be obtained by taking the inverse transform of (2.6.15),

冕

⬁

ui(x) ⫽

⫺⬁

ƒˆ i() ⫽

ƒˆ j()Nij()D⫺1()eix d,

冕

⬁

1 (2)3

⫺⬁

ƒi(x)e⫺ix dx.

(2.6.18)

(2.6.19)

The corresponding stresses can then be obtained by substituting (2.6.18) into (2.4.8): ij(x) ⫽ i

冕

⬁

⫺⬁

ƒˆ m()LijklNkm()lD⫺1()eix d.

(2.6.20)

Equations (2.6.18) and (2.6.20) are integral representations of the displacements and stresses on V. An alternative form of (2.6.18) can be obtained by substituting (2.6.19) into (2.6.18): ui(x) ⫽

冕

⬁

ƒj(y)G⬁ij (x, y) dy,

⫺⬁

(2.6.21)

where G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij()D⫺1()ei(x⫺y) d.

(2.6.22)

The second-order tensor function G ⬁ij given in (2.6.22) is called the Green’s function in an unbounded elastic domain. One can easily show that G ⬁ij is a solution to the following problem: Lijkl

⭸2G⬁km(x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl⭸xj

G⬁ij (x, y) → 0

as 兩x兩 → ⬁,

(2.6.23) (2.6.24)

where ␦(x) is the three-dimensional Dirac delta function. Physically, the Green’s function is the displacement ﬁeld generated by a unit force. Since the domain is homogeneous and unbounded, only the difference between the x point (where the displacement is measured) and the y

2.6

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

39

point (where the unit force is applied) determines the Green function, that is, G⬁ij (x, y) ⫽ Gij⬁(x ⫺ y).

(2.6.25)

Additionally, by using the reciprocal theorem, it can be easily shown that G⬁ij (x, y) ⫽ Gij⬁(x ⫺ y) ⫽ Gji⬁(y ⫺ x) ⫽ Gji⬁(y, x).

(2.6.26)

It then follows that ⭸G⬁ij (x, y) ⭸Gij⬁(x, y) ⫽⫺ . ⭸xi ⭸yi

(2.6.27)

Recall that Nij() and D⫺1() are homogeneous polynomials of degree 4 and 6, respectively, with respect to , we have Nij(⫺)D⫺1(⫺) ⫽ Nij()D⫺1(). Therefore, by changing to ⫺, we can write (2.6.22) in a slightly different form: G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij()D⫺1()e⫺i(x⫺y) d.

(2.6.28)

Furthermore, the volume element in the space can be written as ˆ ˆ ), d ⫽ d1 d2 d3 ⫽ 2 d dS(

(2.6.29)

where ⫽ 兩兩 ⫽ 兹 21 ⫹ 22 ⫹ 23,

ˆ ⫽ , 兩兩

(2.6.30)

ˆ ˆ ) is a surface element on the unit sphere in the space. Thus, and dS( the integral in (2.6.22) can be converted to

G⬁ij (x, y) ⫽

1 (2)3

冕 冋冕 N ()D ⬁

2

0

Sˆ

ij

⫺1

册

ˆ ˆ ) d. ()ei(x⫺y) dS(

(2.6.31)

The homogeneity of degree zero of 2Nij()D⫺1() with respect to leads to

40

BASIC EQUATIONS OF CONTINUUM MECHANICS

2Nij(ˆ )D⫺1(ˆ ) ⫽ Nij(ˆ )D⫺1(ˆ ).

(2.6.32)

It thus follows from (2.6.31) that Gij⬁(x, y) ⫽

1 (2)3

冕 冋冕 N (ˆ )D ⬁

Sˆ

0

⫺1

ij

册

ˆ ˆ ˆ ) d. (ˆ )ei(x⫺y) dS(

(2.6.33)

Following the same procedure, we can rewrite (2.6.28) into Gij⬁(x, y) ⫽

1 (2)3

冕 冋冕 N (ˆ )D 0

⫺⬁

Sˆ

⫺1

ij

册

ˆ ˆ ˆ ) d. (ˆ )ei(x⫺y) dS(

(2.6.34)

Adding these two expressions together gives

冕 冋冕 N (ˆ )D (ˆ )e dS(ˆ ˆ )册 d 1 冕 冋冕 e d册 N (ˆ )D (ˆ ) dS(ˆ ˆ ). ⫽ 2(2)

G⬁ij (x, y) ⫽

⬁

1 2(2)3

⫺⬁

Sˆ

⬁

3

⫺⬁

Sˆ

ij

⫺1

ˆ i(x⫺y)

ˆ i(x⫺y)

ij

⫺1

(2.6.35)

Making use of the following identity in the above expression,

冕

⬁

⫺⬁

ˆ ei(x⫺y) d ⫽ 2␦[ˆ (x ⫺ y)],

(2.6.36)

we have G⬁ij (x, y) ⫽

1 8 2

冕 ␦[ˆ (x ⫺ y)]N (ˆ )D Sˆ

ij

⫺1

ˆ ˆ ). (ˆ ) dS(

(2.6.37)

The integral representations (2.6.18) and (2.6.37) will be used in the following chapters to derive the Eshelby solution. For isotropic materials, D() ⫽ 2( ⫹ 2) 6,

(2.6.38)

Nij() ⫽ 2{( ⫹ 2)␦ij 2 ⫺ ( ⫹ )ij}.

(2.6.39)

The integral in (2.6.37) can be evaluated to yield the Green’s function for isotropic material:

2.6

G⬁ij (x, y) ⫽ ⫽

41

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

再

冎

␦ij 1 1 ⭸2兩x ⫺ y兩 ⫺ 4 兩x ⫺ y兩 4(1 ⫺ v) ⭸xi⭸xj

1 16(1 ⫺ v)兩x ⫺ y兩

再

(3 ⫺ 4v)␦ij ⫹

冎

(xi ⫺ yi)(xj ⫺ yj) . 兩x ⫺ y兩2 (2.6.40)

The integral representations discussed above are the general solutions to problems deﬁned in an unbounded domain. When the problem domain is ﬁnite, the integral representations will need to include the boundary contributions. In this case, the Green’s function approach is often used. Let us consider the boundary value problem stated by (2.5.8)–(2.5.10). To account for the boundary conditions, we deﬁne the Green’s function by the following equations: Lijkl

⭸2Gkm(x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl ⭸xj

Lijkl

in V.

(2.6.41)

Gij(x, y)兩x僆Su ⫽ 0,

(2.6.42)

⭸Gkm(x, y) nj兩x僆S ⫽ 0. ⭸xl

(2.6.43)

Again, by using the reciprocal theorem, it can be easily shown that Gij(x, y) ⫽ Gji(y, x).

(2.6.44)

Multiplying (2.6.41) by ui(x) and integrating the results over the volume V lead to

冕 u (x)L V

i

ijkl

⭸2Gkm(x, y) dV(x) ⫹ um(y) ⫽ 0. ⭸xl⭸xj

(2.6.45)

By using the divergence theorem, we can write the volume integral in (2.6.45) as

42

BASIC EQUATIONS OF CONTINUUM MECHANICS

冕 u (x)L ⭸ G⭸x ⭸(x,x y) dV(x) ⭸G (x, y) ⫽ 冕 u (x)L n dS(x) ⫺ 冕 u (x)L ⭸x 2

km

i

V

ijkl

l

j

km

i

S

ijkl

j

V

l

i, j

ijkl

⭸Gkm(x, y) dV(x). ⭸xl

(2.6.46) Analogously, multiplying (2.5.8) by Gim(x, y) and integrating the result over the volume V lead to

冕 G (x, y)L im

V

u (x) dV(x) ⫹

ijkl k,lj

冕 G (x, y)ƒ (x) dV(x) ⫽ 0. V

im

i

(2.6.47)

Following the procedures that led to (2.6.46), the ﬁrst volume integral in the above equation can be written as

冕 G (x, y)L u (x) dV(x) ⭸G (x, y) ⫽ 冕 G (x, y)L u (x)n dS(x) ⫺ 冕 L ⭸x V

im

ijkl k,lj

im

S

im

ijkl k,l

j

u (x) dV(x).

ijkl k,l

V

j

(2.6.48) Note that the last volume integral on the right-hand side of (2.6.46) is the same as that of (2.6.48). Therefore, by subtracting (2.6.45) from (2.6.47), we arrive at um(y) ⫽

冕 G (x, y)L u (x)n dS(x) ⫹ 冕 G (x, y)ƒ (x) dV(x) ⭸G (x, y) ⫺ 冕 u (x)L n dS(x). (2.6.49) ⭸x S

im

ijkl k,l

j

V

im

i

km

S

i

ijkl

j

l

Enforcing the boundary conditions (2.6.42) and (2.6.43) and (2.5.9) and (2.5.10) in the above, we ﬁnally arrive at the solution to the boundary value problem (2.5.8)–(2.5.10) in terms of the Green’s function Gij(x, y),

PROBLEMS

um(y) ⫽

43

冕 G (x, y)ƒ (x) dV(x) ⫹ 冕 G (x, y)p (x) dS(x) ⭸G (x, y) ⫺ 冕 u (x)L n dS(x). (2.6.50) ⭸x im

V

Su

i

S

0 i

im

km

0 i

ijkl

j

l

By making use of (2.6.44), the above can be written equivalently as ui(x) ⫽

冕 G (x, y)ƒ (y) dV(y) ⫹ 冕 G (x, y)p (y) dS(y) ⭸G (x, y) ⫺ 冕 u (y)L n dS(y). ⭸y im

V

Su

m

0 m

S

0 m

im

ik

mjkl

j

(2.6.51)

l

PROBLEMS

2.1 If for any function ƒ(x) that is continuous at x ⫽ 0

冕

⬁

⫺⬁

ƒ(x)␦(x) dx ⫽ ƒ(0),

then ␦(x) is called the Dirac delta function. Prove the following properties: x␦(x) ⫽ 0,

␦(ax) ⫽

1 ␦(x), a

␦(⫺x) ⫽ ␦(x).

2.2 Show that the Green’s function G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij()D⫺1()ei(x⫺y) d

satisﬁes the following boundary value problem: ⬁ LijklGlm,ik (x, y) ⫹ ␦jm␦(x ⫺ y) ⫽ 0,

G⬁ij (x, y) → 0

as 兩x兩 → ⬁,

44

BASIC EQUATIONS OF CONTINUUM MECHANICS

where ␦(x) is the three-dimensional Dirac delta function deﬁned by

冕

Vr

␦(x) dV ⫽ 1,

where Vr is any spherical volume x 21 ⫹ x 22 ⫹ x 23 ⫽ r 2. 2.3 Show (2.6.26) and (2.6.27). APPENDIX 2.A RELATIONSHIP AMONG ELASTIC CONSTANTS OF ISOTROPIC MATERIALS

E, v

E, G

K, v

K, G

,

E

E

E

3(1 ⫺ 2 v)K

v

v

⫺1 ⫹

9K 1 ⫹ 3K / G 1 ⫺ 2G / 3K 2 ⫹ 2G / 3K

(3 ⫹ 2 / ) 1 ⫹ / 1 2(1 ⫹ / )

3(1 ⫺ 2 v)K 2(1 ⫹ v)

G

K

K

⫹

G K

E 2(1 ⫹ v) E 3(1 ⫺ 2 v) Ev (1 ⫹ v)(1 ⫺ 2v) E 2(1 ⫹ v)

E 2G

G E 9 ⫺ 3E / G E(1 ⫺ 2G / E) 3 ⫺ E/G G

v

3Kv 1⫹v 3(1 ⫺ 2v)K 2(1 ⫹ v)

K⫺

2G 3

2 3

G

APPENDIX 2.B VOIGT ELASTIC CONSTANTS FOR MATERIALS WITH VARIOUS SYMMETRIES Orthotropic Materials (nine indepenent constants)

冤

C11 C12 C13 C⫽ 0 0 0

C12 C22 C23 0 0 0

C13 0 C23 0 C33 0 0 C44 0 0 0 0

0 0 0 0 C55 0

冥

0 0 0 0 0 C66

APPENDIX 2.B

VOIGT ELASTIC CONSTANTS

45

Transversely Isotropic Materials (ﬁve independent constants)

冤

C11 C12 C13 C⫽ 0 0 0

C12 C11 C13 0 0 0

C13 0 C13 0 C33 0 0 C44 0 0 0 0

0 0 0 0 C44 0

冥

0 0 0 0 0

0.5(C11 ⫺ C12)

for axis of symmetry in the x3 direction, and

冤

C11 C12 C12 C⫽ 0 0 0

C12 C22 C23 0 0 0

C12 0 0 C23 0 0 C22 0 0 0 0.5(C22 ⫺ C23) 0 0 0 C44 0 0 0

冥

0 0 0 0 0 C44

for axis of symmetry in the x1 direction. Cubic Materials (three independent constants)

冤

C11 C12 C12 C⫽ 0 0 0

C12 C11 C12 0 0 0

C12 0 C12 0 C11 0 0 C44 0 0 0 0

0 0 0 0 C44 0

冥

0 0 0 0 0 C44

Isotropic Materials (two independent constants)

C⫽

冤

C11 C12 C12 0 0 0

C12 C11 C12 0 0 0

冥

C12 0 0 0 C12 0 0 0 C11 0 0 0 0 0.5(C11 ⫺ C12) 0 0 0 0 0.5(C11 ⫺ C12) 0 0 0 0 0.5(C11 ⫺ C12)

46

BASIC EQUATIONS OF CONTINUUM MECHANICS

APPENDIX 2.C

EXPRESSIONS OF Nij() AND D()

Transversly Isotropic Materials

D() ⫽ (␣⬘2 ⫹ ␥ 32){␣␥4 ⫹ (␣ ⫹ ␥2 ⫺ ␥⬘2)2 32 ⫹ ␥ 34} ⫽ (␣⬘2 ⫹ ␥ 23){(␥2 ⫹  23)(␣2 ⫹ ␥ 23) ⫺ ␥⬘22 32},

N11() ⫽ (␣⬘ 21 ⫹ ␣ 22 ⫹ ␥ 23)(␥2 ⫹  32) ⫺ ␥⬘2 22 32, N12() ⫽ ␥⬘212 32 ⫺ (␣ ⫺ ␣⬘)12(␥2 ⫹  32), N13() ⫽ (␣ ⫺ ␣⬘)␥⬘1 223 ⫺ ␥⬘13(␣⬘ 12 ⫹ ␣ 22 ⫹ ␥ 32), N22() ⫽ (␣ 12 ⫹ ␣⬘ 22 ⫹ ␥ 32)(␥2 ⫹  32) ⫺ ␥⬘2 12 32, N23() ⫽ (␣ ⫺ ␣⬘)␥⬘ 2123 ⫺ ␥⬘23(␣ 21 ⫹ ␣⬘ 22 ⫹ ␥ 23), N33() ⫽ (␣ 12 ⫹ ␣⬘ 22 ⫹ ␥ 32)(␣⬘ 12 ⫹ ␣ 22 ⫹ ␥ 32) ⫺ (␣ ⫺ ␣⬘)2 12 22, where ␣ ⫽ C11 ⫽ C22,  ⫽ C33,

␣⬘ ⫽ C66 ⫽ –12 (C11 ⫺ C12), ␥⬘ ⫺ ␥ ⫽ C13 ⫽ C23,

␥ ⫽ C44 ⫽ C55,

2 ⫽ 12 ⫹ 22.

Cubic Materials

D() ⫽ 2( ⫹ 2 ⫹ ⬘) 6 ⫹ ⬘(2 ⫹ 2 ⫹ ⬘) 2( 21 22 ⫹ 22 23 ⫹ 23 21) ⫹ ⬘2(3 ⫹ 3 ⫹ ⬘) 12 22 32,

N11() ⫽ 2 4 ⫹  2( 22 ⫹ 32) ⫹ ␥ 22 32, N12() ⫽ ⫺( ⫹ )12( 2 ⫹ ⬘ 23),

REFERENCES

47

and the other components are obtained by the cyclic permutation of 1, 2, 3, where 2 ⫽ ii,  ⫽ ( ⫹ ⫹ ⬘), ␥ ⫽ ⬘(2 ⫹ 2 ⫹ ⬘), ⫽ C12, ⫽ C44, ⬘ ⫽ C11 ⫺ C12 ⫺ 2C44. Isotropic Materials

D() ⫽ 2( ⫹ 2) 6, Nij() ⫽ 2{( ⫹ 2)␦ij 2 ⫺ ( ⫹ )ij}, where 2 ⫽ kk. Also LjlmnlNij()D⫺1() ⫽ ( ⫹ 2)⫺1⫺4{␦mni 2 ⫹ ( ⫹ 2)␦imn 2 ⫹ ( ⫹ 2)␦inm 2 ⫺ 2( ⫹ )mni}, ⫺1 LijklLpqmnqlNkp()D () ⫽ ( ⫹ 2)⫺1⫺4{2␦ij␦mn 4 ⫹ 2␦mnij 2 ⫹ 2␦ijmn 2 ⫹ ( ⫹ 2)(␦imjn ⫹ ␦jmin ⫹ ␦injm ⫹ ␦jnim) 2 ⫺ 4( ⫹ )ijmn}.

REFERENCES Christensen, R. M. (1982). Theory of Viscoelasticity—An Introduction, 2nd ed., Academic Press, New York. Malvern, L. E. (1969). Introduction to the Mechanics of Continuous Medium, Prentice-Hall, Englewood Cliffs, NJ. Ting, T. C. T. (1996). Anisotropic Elasticity—Theory and Applications, Oxford University Press, New York.

48

BASIC EQUATIONS OF CONTINUUM MECHANICS

SUGGESTED READINGS Fung, Y. C. (1965). Foundations of Solid Mechanics, Prentice-Hall, Englewood Cliffs, NJ. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Dordrecht.

3 EIGENSTRAINS In this chapter, we will ﬁrst deﬁne what eigenstrain is and give some examples of it. Then, we will derive the general solutions to the displacements, stresses, and strains when an eigenstrain ﬁeld is present in a linear elastic solid.

3.1

DEFINITION OF EIGENSTRAINS

Eigenstrain is a generic name introduced in micromechanics to represent inelastic strains such as thermal strains, phase transformation strains, initial strains, plastic strains, misﬁt strains, and the like. In the literature, other names have been used for eigenstrains by various authors, such as stress-free transformation strains by Eshelby and elastic polarization strains by Kro¨ner. In this book, we will use the term eigenstrain to represent any inelastic strains. For small-strain deformation, we will use the following notation convention: ij ⫽ total strain,

eij ⫽ elastic strain, ij* ⫽ eigenstrain (inelastic).

When both elastic strain and eigenstrain coexist in a continuum, the total strain is given by the sum Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

49

50

EIGENSTRAINS

ij ⫽ eij ⫹ ij*.

(3.1.1)

The above equation implies that both the elastic strain and eigenstrain act together to cause a material point in the continuum to displace from its initial location to its ﬁnal location in the deformed conﬁguration. The ﬁnal position of the material particle after the deformation determines the total strain, that is, the total strain is related to the displacement through [see (2.1.12)] ij ⫽ –21 (ui, j ⫹ uj,i),

(3.1.2)

where ui is the total displacement ﬁeld cause by both the elastic strain and the eigenstrain. Although the total strain can be separated into elastic and inelastic parts, it is not always possible to separate the displacement into elastic and inelastic parts. So, we will not introduce the concepts of elastic displacement and eigen displacement. Therefore, it is unnecessary to use ‘‘total’’ for the displacement. It will be understood that displacement ui is always the total displacement caused by both strains. For sufﬁciently smooth displacement ﬁelds, the total strain tensor satisﬁes Saint Venant’s compatibility conditions: Rij ⫽ ikpjlqpq,kl ⫽ 0,

(3.1.3)

where ijk is the permutation symbol deﬁned by (1.4.15). Note that it is only the total strain, or the sum of the elastic strain and eigenstrain, that must be compatible, that is, satisfying the compatibility condition (3.1.3). The elastic strain and the eigenstrain by themselves alone do not have to be compatible. In fact, we will see in later examples that they often are not compatible by themselves. Another way of saying, for example, that the eigenstrain ﬁeld is not compatible is that there is no differentiable function u* i such that 1 * ij ⫽ – 2 (u* i, j ⫹ u*). j,i

(3.1.4)

Or, equivalently, one can say that R*ij ⫽ ikpjlq*pq,kl ⫽ 0. Let us now consider Hooke’s law when eigenstrains are present. As discussed in Chapter 2, Hoooke’s law describes the stress–strain relationship for linear elastic materials. In other words, it relates the stress to the elastic strain in a linear elastic material. When eigenstrain is

3.1

DEFINITION OF EIGENSTRAINS

51

present in a linear elastic material, the total strain is given by (3.1.1). Thus the elastic strain is the difference between the total strain and eigenstrain: eij ⫽ ij ⫺ ij*. Consequently, Hooke’s law should be written as ij ⫽ Lijklekl ⫽ Lijkl(kl ⫺ *), kl

(3.1.5)

eij ⫽ ij ⫺ *ij ⫽ Mijklkl.

(3.1.6)

or

The interpretation of (3.1.5) is that the stress in a linear elastic material is caused only by elastic strain. If there is no elastic strain, there would be no stress. For this reason, we do not introduce the concept of eigenstress in this book. As a simple example to understand (3.1.5), let us consider the uniaxial tension of a metal bar. A typical uniaxial stress–strain curve is shown in Figure 3.1. The eigenstrain in this case is the plastic strain p while the elastic strain is e. Clearly, we have the total strain ⫽ p ⫹ e. It is clearly seen from this ﬁgure that ⫽ Ee ⫽ E( ⫺ p). In other words, the stress is the elastic constant (Young’s modulus) times the elastic strain, which is the difference between the total strain and the eigenstrain.

σ

E

εp

E

εe

ε

Figure 3.1 Uniaxial stress–strain curve.

52

EIGENSTRAINS

3.2 SOME EXAMPLES OF EIGENSTRAINS

First, consider an aluminum ball of radius a at temperature T0. When the temperature is raised to T, the ball expands. It follows from (2.4.34) that the thermal strain is given by * ij ⫽ ␣A ⌬T ␦ij,

(3.2.1)

where ␣A is the coefﬁcient of thermal expansion for aluminum, ␦ij is the Kronecker delta, and ⌬T ⫽ T ⫺ T0 is the temperature change. Since there is no constraint to the ball, no stress is induced by the temperature rise. Thus, it follows from (3.1.6) that the elastic strain is zero, that is, eij ⫽ ij ⫺ *ij ⫽ Mijklkl ⫽ 0.

(3.2.2)

Consequently, the eigenstrain in this case is equal to the total strain: ij ⫽ eij ⫹ * * ⫽ ␣A ⌬T ␦ij. ij ⫽ ij

(3.2.3)

We see that thermal strain is an eigenstrain. Next, let the aluminum ball be embedded in a rigid matrix at temperature T0. Then, raise the temperature to T. In this case, the total strain of the aluminum ball is zero because of the rigid constraint. This means that ij ⫽ eij ⫹ * ij ⫽ eij ⫹ ␣A ⌬T ␦ij ⫽ 0,

(3.2.4)

eij ⫽ ⫺ij* ⫽ ⫺aA ⌬T ␦ij.

(3.2.5)

or

It is seen that the elastic strain is no longer zero due to the constraint. Because of the nonzero elastic strain, the stress in the aluminum ball is also nonzero. It is given by Hooke’s law: ij ⫽ Lijklekl ⫽ ⫺␣ALnnij ⌬T.

(3.2.6)

This stress could be very large. For example, for polycrystalline aluminum (isotropic), (3.2.6) can be simpliﬁed to

3.3

GENERAL SOLUTIONS OF EIGENSTRAIN PROBLEMS

E␣A ij ⫽ ⫺ ⌬T ␦ij, 1 ⫺ 2

53

(3.2.7)

where for aluminum E ⫽ 71 ⫻ 109 Pa,

␣A ⫽ 24 ⫻ 10⫺6 / ⬚C,

v ⫽ 0.3.

Therefore, the thermally induced stress is ij ⬇ 4.3 MPa

⌬T ␦. ⬚C ij

(3.2.8)

So, a temperature change of 10⬚ Celsius would cause 43 MPa stress! Finally, let us assume that the aluminum ball is embedded in a copper matrix at temperature T0. Again, let the temperature be raised to T. In this case, the total strain is given by ij ⫽

再

eAij ⫹ ␣A ⌬T ␦ij eCij ⫹ ␣C ⌬T ␦ij

in the Al ball in the Cu matrix

(3.2.9)

where ␣C is the coefﬁcient of thermal expansion of copper. Since the shell is deformable, the total strain is not zero in the aluminum ball, nor is it zero in the copper matrix. The thermally induced stresses cannot be obtained easily in this case; see Problem 3.2. Nevertheless, we know that stresses are induced due to the mismatch between the thermal expansion coefﬁcients. The above examples show that thermal strain is a type of eigenstrain. Other types of eigenstrains include plastic strain, phase transformation strain, and the like. 3.3 GENERAL SOLUTIONS OF EIGENSTRAIN PROBLEMS

Consider an unbounded elastic body, V, on which an eigenstrain ﬁeld * ij is prescribed. Without the body force, the equations of equilibrium is given by ij, j ⫽ 0

in V

(3.3.1)

Because of the eigenstrains, Hooke’s law takes the form of (3.1.5), that is,

54

EIGENSTRAINS

ij ⫽ Lijklekl ⫽ Lijkl(kl ⫺ *), kl

(3.3.2)

where ij is the total strain. Since the total strain must be compatible, we have ij ⫽ –21 (ui, j ⫹ uj,i),

(3.3.3)

where ui is the total displacement. Next, making use of (3.3.3) in (3.3.2) and the symmetry of the stiffness tensor, we obtain ij ⫽ Lijkluk,l ⫺ Lijkl*. kl

(3.3.4)

Substitution of (3.3.4) into (3.3.1) yields Lijkluk,lj ⫺ Lijkl*kl, j ⫽ 0

in V.

(3.3.5)

This is the governing equation for the total displacement ﬁeld in V. We further assume that the radiation condition is also satisﬁed, that is, ui → 0

as 兩x兩 → ⬁.

(3.3.6)

This condition implies that the nonzero eigenstrain can only be distributed over a ﬁnite domain within V. Comparing (3.3.5) and (3.3.6) to (2.6.3) and (2.6.4), we conclude that the solution to the eigenstrain problem can be obtained from the elasticity solution if the body force ƒi in the elasticity solution is replaced by ⫺Lijklkl, * j. To this end, consider the boundary value problem stated by (2.6.3) and (2.6.4). Assuming that the body force is given by the eigenstrain ƒi ⫽ ⫺Lijkl*kl, j,

(3.3.7)

then, through integration by parts, the Fourier transform of ƒi can be written as ƒˆ i() ⫽

⫺1 (2)3

冕

⬁

⫺⬁

Lijkl*kl, j(x)e⫺i䡠x dx ⫽ ⫺ijLijklˆ *, kl

where ˆ kl* is the Fourier transform of the eigenstrain *(x): kl

(3.3.8)

3.3

GENERAL SOLUTIONS OF EIGENSTRAIN PROBLEMS

ˆ *( kl ) ⫽

1 (2)3

冕

⬁

⫺⬁

⫺i䡠x *(x)e dx. kl

55

(3.3.9)

Substituting (3.3.8) into (2.6.18), we obtain the solution to the boundary value problem stated by (3.3.5) and (3.3.6): ui(x) ⫽ ⫺i

冕

⬁

⫺⬁

Ljlmnˆ *mn()l Nij()D⫺1()ei䡠x d.

(3.3.10)

The corresponding strain tensor is ij(x) ⫽

1 2

冕

⬁

⫺⬁

Lklmnˆ *mn()l[l Nik() ⫹ iNjk()]D⫺1()ei䡠x d.

(3.3.11)

The stress tensor thus follows from (3.3.4):

再冕

ij(x) ⫽ Lijkl

⬁

⫺⬁

冎

Lpqmnˆ mn * ()lqNkp()D⫺1()ei䡠x d ⫺ ij*(x) . (3.3.12)

An alternative approach is to use Green’s function. By substituting (3.3.7) into (2.6.21), we obtain

冕

⬁

ui(x) ⫽ ⫺

⫺⬁

⬁ Lmjkl*kl, j(y)Gmi (x, y) dy,

(3.3.13)

where G⬁mi(x, y) is the inﬁnite domain Green’s function given in (2.6.22). Applying divergence theorem to (3.3.13) yields ui(x) ⫽

冕

⬁

⫺⬁

Lmjkl*(y) kl

⭸G⬁mi(x, y) dy. ⭸yj

The corresponding strain and stress ﬁelds are

(3.3.14)

56

EIGENSTRAINS

ij(x) ⫽

再冕

⬁

ij(x) ⫽ Lijkl

⫺⬁

冕

⬁

⫺⬁

Lklmn⌫⬁ijkl(x ⫺ y)*mn(y) dy,

(3.3.15)

冎

⬁ Lpqmnmn * (y)⌫klpq (x ⫺ y) dV(y) ⫺ kl*(x) ,

(3.3.16)

where the fourth-order tensor ⌫⬁ijkl(x, y) is given by ⌫⬁ijkl(x, y) ⫽

冋

册

1 ⭸2Gki⬁ (x, y) ⭸2G⬁kj(x, y) ⭸2Gli⬁(x, y) ⭸2Glj⬁(x, y) ⫹ ⫹ ⫹ . 4 ⭸xj ⭸yl ⭸xi ⭸yl ⭸xj ⭸yk ⭸xi ⭸yk (3.3.17)

For future reference, we deﬁne PVijkl(x) ⫽

冕⌫ V

⬁ ijkl

(x, y) dV(y),

(3.3.18)

where the superscript V indicates that the integral is over the volume V. 3.4 EXAMPLES Straight-Screw Dislocation

Consider the straight-screw dislocation in a cubic crystal shown in Figure 3.2. The eigenstrain corresponding to this screw dislocation is given by

x3 x2

x1

Figure 3.2 Straight-screw dislocation.

3.4

EXAMPLES

1 * 23 ⫽ – 2 b␦(x2)H(⫺x1),

57

(3.4.1)

where b is the Burgers vector of the dislocation. The Fourier transform of *23 is easily calculated from (3.3.9):

冕 12 b␦(x )H(⫺x )e dx b ⫽ 冕 H(⫺x )e dx 冕 e 2(2) ⬁

1 (2)3

* 23() ⫽

2

⫺⬁

⬁

3

1

⫺⬁

1

⫺i1x1

⫺i䡠x

⬁

1

⫺i3x3

⫺⬁

dx3.

(3.4.2)

Note that

冕

⬁

⫺⬁

冕

H(⫺x1)e⫺i1x1 dx1 ⫽

⬁

⫺⬁

⫺1 , i1

e⫺i3x3 dx3 ⫽ 2␦(3).

(3.4.3)

(3.4.4)

We have b ␦(3) . 2(2)2 i1

ˆ * 23() ⫽ ⫺

(3.4.5)

Substitution of (3.4.5) into (3.3.10) and use of the properties of delta function yield

冕 L b ⫽ 冕 冕 (2)

ui(x) ⫽

b (2)2

2

⬁

⫺⬁

jl23

⬁

⬁

⫺⬁

⫺⬁

␦(3) N ()D⫺1()ei䡠x d 1 l ij ⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 d1 d2. 1 l Nij()D ()e

(3.4.6)

For materials with cubic symmetry, the integrand in (3.4.6) is simpliﬁed to ⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 0, 1 l N1j()D ()e

(3.4.7)

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 0, 1 l N2j()D ()e

(3.4.8)

58

EIGENSTRAINS

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 1 l N3j()D ()e

2 ei(1x1⫹2x2). 1( ⫹ 22) 2 1

(3.4.9)

Therefore, we have u1(x) ⫽ u2(x) ⫽ 0,

(3.4.10)

and u3(x) ⫽

b (2)2

冕

⬁

⫺⬁

冉冊

2 b x ei(1x1⫹2x2) d1 d2 ⫽ tan⫺1 2 . 2 1( ⫹ 2) 2 x1 2 1

(3.4.11) The only nonzero strain component is the shear strain: 23 ⫽

1 ⭸u3 b x1 ⫽ . 2 2 ⭸x2 4 x 1 ⫹ x 32

(3.4.12)

It follows from Hooke’s law for cubic materials (2.4.12) that the only nonzero stress component is the shear stress: 23 ⫽ 2C4423 ⫽

C44b x1 . 2 2 x 1 ⫹ x 23

(3.4.13)

These results are identical to those obtained by Burgers in 1939 for isotropic materials. Straight-Edge Dislocation

Consider a straight-edge dislocation in a cubic material as shown in Figure 3.3. The eigenstrain corresponding to this dislocation is given by 1 * 12 ⫽ – 2 b␦(x2)H(⫺x1),

(3.4.14)

where again, b is the Burgers vector of the dislocation. We are to ﬁnd the corresponding displacements and stresses. Following the procedures used in deriving (3.4.5), the Fourier transform of 12 * is easily calculated from (3.3.9):

3.4

x2

EXAMPLES

59

x1

x3

Figure 3.3 Straight-edge dislocation.

12 * () ⫽

1 (2)3

冕

⬁

1 b ␦(3) b␦(x2)H(⫺x1)ei䡠x dx ⫽ ⫺ . 2 2(2)2 i1

⫺⬁

(3.4.15)

Substitution of (3.4.15) into (3.3.10) and use of the properties of the delta function yield

冕 L b ⫽ 冕 冕 (2)

ui(x) ⫽

b (2)2

2

⬁

⫺⬁

jl12

⬁

⬁

⫺⬁

⫺⬁

␦(3) N ()D⫺1()ei䡠x d 1 l ij ⫺1 i䡠x (Ljl12⫺1 )兩3⫽0 d1 d2. 1 l Nij()D ()e

(3.4.16)

For materials with cubic symmetry, the integrand in (3.4.16) is simpliﬁed to ⫺1 i䡠x (Ljl12⫺1 )兩3⫽0 ⫽ 1 l N1j()D ()e

ei(1x1⫹2x2)2( 12 ⫹ 22 ⫺ ␣ 12) , 1[( 12 ⫹ 22)2 ⫹  12 22] (3.4.17)

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 1 l N2j()D ()e

ei(1x1⫹2x2)( 21 ⫹ 22 ⫺ ␣ 22) , ( 21 ⫹ 22)2 ⫹  21 22

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 0, 1 l N3j()D ()e

where

(3.4.18) (3.4.19)

60

EIGENSTRAINS

2 ⫹ 2 ⫹ , ⫹ 2 ⫹

␣⫽

⫽

␣ .

(3.4.20)

Therefore, we have u3(x) ⫽ 0

(3.4.21)

and u1(x) ⫽

b (2)2

u2(x) ⫽

冕 冕

b (2)2

⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2( 21 ⫹ 22 ⫺ ␣ 21) d1 d2, 1[( 12 ⫹ 22)2 ⫹  12 22]

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)( 12 ⫹ 22 ⫺ ␣ 22) d1 d2. ( 12 ⫹ 22)2 ⫹  12 22

(3.4.22)

(3.4.23)

The nonzero strain components are 11 ⫽

⭸u1 ib ⫽ ⭸x1 (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2( 12 ⫹ 22 ⫺ ␣ 12) d1 d2, [( 12 ⫹ 22)2 ⫹  12 22] (3.4.24)

22 ⫽

⭸u2 ib ⫽ ⭸x2 (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2( 12 ⫹ 22 ⫺ ␣ 22) d1 d2, ( 12 ⫹ 22)2 ⫹  12 22] (3.4.25)

12 ⫽ ⫽

冉

冊

1 ⭸u1 ⭸u2 ⫹ 2 ⭸x2 ⭸x1 ib 2(2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)[( 21 ⫹ 22)2 ⫺ 2␣ 12 22]) d1 d2. 1[( 21 ⫹ 22)2 ⫹  21 22] (3.4.26)

In terms of the integrals deﬁned in Appendix 3.A, these strains can be written as

3.4

61

ib [(1 ⫺ ␣)I1 ⫹ I2], (2)2

(3.4.27)

ib ⫽ [I1 ⫹ (1 ⫺ ␣)I2], (2)2

(3.4.28)

ib ⫽ [I3 ⫺ (2␣ ⫹ )I1], 2(2)2

(3.4.29)

11 ⫽

22 ⫽

12 ⫽

EXAMPLES

where I1, I2, and I3 are given in Appendix 3.A. For isotropic materials, ⫽ 0, ⫽ 2v /(1 ⫺ 2v). Thus, ␣⫽

1

 ⫽ 0.

, 1⫺v

(3.4.30)

The nonzero displacement components in this case are simpliﬁed to u1(x) ⫽

b (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)

冋

册

2 ␣ ⫺ 2 2 12 2 d1 d2, 2 1( ⫹ 2) ( 1 ⫹ 2) 2 1

(3.4.31) u2(x) ⫽

b (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)

冋

1

12 ⫹ 22

⫺

册

␣ 22 d1 d2. ( 21 ⫹ 22)2

(3.4.32) Making use of the integrals given in Appendix 3.B, we arrive at the displacement components for isotropic materials: u1(x) ⫽

u2(x) ⫽

冋 冋

冉冊

册

b x 1 x1x2 2 tan⫺1 2 ⫹ , 4 x1 1 ⫺ v x 21 ⫹ x 22

册

b x 22 1 ⫺ 2v ⫺ log(x 21 ⫹ x 22) . 2 4 (1 ⫺ v) x 1 ⫹ x 22 2

(3.4.33)

(3.4.34)

The corresponding strain components are obtained by taking the derivatives of the displacements:

62

EIGENSTRAINS

11 ⫽

⭸u1 ⫺bx2[x 12(3 ⫺ 2v) ⫹ x 22(1 ⫺ 2v)] ⫽ , ⭸x1 4 (1 ⫺ v)(x 12 ⫹ x 22)2

(3.4.35)

22 ⫽

⭸u2 ⫺bx2[x 12(1 ⫹ 2v) ⫺ x 22(1 ⫺ 2v)] ⫽ , ⭸x2 4 (1 ⫺ v)(x 12 ⫹ x 22)2

(3.4.36)

12 ⫽

1 ⭸u1 ⭸u2 bx1(x 12 ⫺ x 22) ⫹ ⫽ . 2 ⭸x2 ⭸x1 4 (1 ⫺ v)(x 12 ⫹ x 22)2

冉

冊

(3.4.37)

The corresponding stresses are obtained by using Hooke’s law for isotropic materials: 11 ⫽

⫺b x2(3x 12 ⫹ x 22) , 2 (1 ⫺ v)(x 21 ⫹ x 22)2

(3.4.38)

22 ⫽

b x2(x 21 ⫺ x 22) , 2 (1 ⫺ v)(x 21 ⫹ x 22)2

(3.4.39)

12 ⫽

b x1(x 21 ⫺ x 22) . 2 (1 ⫺ v)(x 21 ⫺ x 22)2

(3.4.40)

These are the classic solutions for a straight-edge dislocation. Dislocation of General Nature

Consider a dislocation loop L inside a crystalline material as shown in Figure 3.4. Let the area of the slip plane be denoted by S. To describe the slip caused by the dislocation, one side of the slip plane is labeled S⫹ and the other side is labeled S⫺. The slip is a result of S⫹ moving relative to S⫺ by a Burgers vector b. The unit normal vector of S⫹

S+

S−

b n L

Figure 3.4 Dislocation of general nature.

3.4

EXAMPLES

63

pointing to S⫺ is denoted by n. The eigenstrain corresponding to such a dislocation loop can then be written as *(x) ⫽ ⫺–12 (binj ⫹ bjni)␦(S ⫺ x), ij

(3.4.41)

where ␦(S ⫺ x) is called the surface Dirac delta function deﬁned by ␦(S ⫺ x) ⫽

冕 ␦(x ⫺ z) dS(z).

(3.4.42)

S

It can be easily shown that for any continuous function deﬁned in the volume V that contains the surface S, the surface Dirac delta function satisﬁes the following:

冕 ƒ(x)␦(S ⫺ x) dV(x) ⫽ 冕 ƒ(x) dS(x). V

(3.4.43)

S

Substituting (3.4.41) into (3.3.14) and making use of (3.4.43), we obtain the displacement ﬁeld due to the dislocation loop L, 1 ui(x) ⫽ ⫺ 2

冕

⬁

⫺⬁

Lmjkl(bk nl ⫹ bl nk)␦(S ⫺ y)

冕L

⫽⫺

S

mjkl bk nl

⭸G⬁mi(x, y) dy ⭸yj

⭸G⬁mi(x, y) dS(y). ⭸yj

(3.4.44)

Upon using the properties of Green’s function (2.6.27), the above equation can be written as ui(x) ⫽

冕L S

mjkl bk nl

⭸G⬁mi(x, y) dS(y). ⭸xj

(3.4.45)

This is the well-known Volterra formula. The displacement gradient thus follows from the Volterra formula: ui, j(x) ⫽

冕L S

mnkl

bk nl

⭸G⬁mi(x, y) dS(y). ⭸xn ⭸xj

The stress caused by the dislocation loop L is thus given by

(3.4.46)

64

EIGENSTRAINS

ij ⫽ Lijkl(kl ⫺ *) kl ⫽ Lijkluk,l ⫺ Lijkl*. kl

(3.4.47)

Note that Lijkl*kl ⫽ ⫺–12 Lijkl(bk nl ⫹ bl nk)␦(S ⫺ x) ⫽ ⫺Lijkl bk nl␦(S ⫺ x).

(3.4.48)

Introducing (3.4.48) into (3.4.47) yields ij ⫽ Lijkl[uk,l ⫹ bk nl␦(S ⫺ x)] ⫽ Lijklkl,

(3.4.49)

冕L

(3.4.50)

where ij ⫽

S

mnkl

bk nl

⭸2G⬁mi(x, y) dS(y) ⫹ binj␦(S ⫺ x) ⭸xn ⭸xj

is called the elastic distortion. We next show that the surface integral in (3.4.50) can be converted to a line integral along the dislocation loop. To this end, consider the following line integral along the dislocation loop:

冕

L

jnh pqmn

L

⭸G⬁ip(x, y) bmth dL(y), ⭸xq

(3.4.51)

where th is the tangential unit vector along the dislocation loop. Making use of the Stokes’ theorem (2.3.3),

冕 L

⭸G⬁ip(x, y) bmth dL(y) ⭸xq

L

jnh pqmn

冕

⫽⫺

S

klhjnhLpqmn

⭸G⬁ip(x, y) bmnk dS(y), ⭸xq ⭸xl

(3.4.52)

where the negative sign is due to the properties of Green’s function (2.6.27). Using the ⫺ ␦ relationship (1.4.16), the right-hand side of (3.4.52) can be written as

3.4

冕

⫺

S

⭸G⬁ip(x, y) bmnk dS(y) ⭸xq ⭸xl

klhjnhLpqmn

冕 冉L

⫽⫺

⭸G⬁ip(x, y) ⭸G⬁ip(x, y) bmnj ⫺ Lpqmn bmnn ⭸xq ⭸xn ⭸xq ⭸xj

pqmn

S

EXAMPLES

冊

65

dS(y). (3.4.53)

Since

Lpqmn

⭸G⬁ip(x, y) ⫹ ␦mi␦(x ⫺ y) ⫽ 0, ⭸xq ⭸xn

(3.4.54)

we can simplify (3.4.53) to

冕

⫺

L

klh jnh pqmn

S

⭸G⬁ip(x, y) bmnk dS(y) ⭸xq ⭸xl

⫽ binj␦(S ⫺ x) ⫹

冕L S

pqmn

⭸G⬁ip(x, y) bmnn dS(y). ⭸xq ⭸xj

(3.4.55)

Comparison of (3.4.55) and (3.4.50) leads to

冕

ij ⫽ ⫺

S

klhjnhLpqmn

⭸G⬁ip(x, y) bmnk dS(y). ⭸xq ⭸xl

(3.4.56)

It then follows from (3.4.52) that

冕L ⫽冕

ij ⫽

S

L

mnkl bk nl

L

jnh pqmn

⭸2G⬁mi(x, y) dS(y) ⫹ binj␦(S ⫺ x) ⭸xn ⭸xj ⭸G⬁ip(x, y) bmth dL(y). ⭸xq

(3.4.57)

This is known as the Mura formula (Mura, 1987). The stress ﬁeld thus follows from (3.4.49):

66

EIGENSTRAINS

ij ⫽ Lijkl

冕 L

lnhLpqmn

⭸G⬁kp(x, y) bmth dL(y). ⭸xq

(3.4.58)

The fact that the stress ﬁeld is represented as a line integral along the dislocation loop indicates that the stress depends only on the loop, not the slip plane area S.

PROBLEMS

3.1 Consider a composite bar (one dimensional) whose ends are ﬁxed on rigid walls as shown in Figure 3.5. When the temperature is T0, the interface between Al and Cu is at the middle x ⫽ L/2. Please ﬁnd the position of the interface when the temperature is raised to T ⬎ T0. Assume the Young’s moduli and the thermal expansion coefﬁcients of Al and Cu are, respectively, Ea, Ec, ␣a, and ␣c. 3.2 Consider a spherical aluminum ball embedded in a copper matrix of inﬁnite extent at temperature T. When the temperature rises by ⌬T, ﬁnd the stress ﬁelds in both the ball and the matrix. 3.3 Consider a Cu water pipe in your house. Assuming the pipe has an outer diameter of 2.54 cm with wall thickness of 1 mm. Is it safe to expose this pipe to ⫺20⬚C with water in it? If the required factor of safety is 3, what is the lowest temperature this water pipe can stand? The properties of Cu and ice are given below.

Cu Ice

Young’s Modulus

Poisson’s Ratio

CTE

Tensile Strength

125 GPa 9.5 GPa

0.33 0.33

17 ⫻ 10⫺6 / ⬚C ⫺50 ⫻ 10⫺6 / ⬚C

70 MPa N/A

L /2

L /2

Al

Cu

x

Figure 3.5

APPENDIX 3.A

67

APPENDIX 3.A

We introduce the following integrals:

冕 冕 ⫽冕 冕

I1 ⫽

⬁

⬁

⫺⬁

⫺⬁

⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2 12 d d [( ⫹ 22)2 ⫹  12 22] 1 2 2 1

ei(1x1⫹2x2)1 22 d d , [( 12 ⫹ 22)2 ⫹  12 22] 1 2

冕 冕 ⫽冕 冕

I2 ⫽

⬁

⬁

⫺⬁

⫺⬁

⬁

⬁

⫺⬁

⫺⬁

I3 ⫽

(3.A.1)

ei(1x1⫹2x2) 32 d d ( 12 ⫹ 22)2 ⫹  12 22 1 2 ei(1x1⫹2x2) 31 d d , ( 12 ⫹ 22)2 ⫹  12 22 1 2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2) d1 d2. 1

(3.A.2)

(3.A.3)

Let us consider (3.A.3) ﬁrst. Making use of the well-known integrals,

冕

⬁

⫺⬁

冕

⬁

ei2x2 d2 ⫽ 2␦(x2),

ei1x1 d1 ⫽ i sgn(x1), 1

(3.A.4)

ei1x1 d1 ⫽ 2i2␦(x2)sgn(x1). 1

(3.A.5)

⫺⬁

we can reduce (3.A.3) to I3 ⫽

冕

⬁

⫺⬁

ei2x2 d2

冕

⬁

⫺⬁

To evaluate the other integrals, we introduce the polar coordinate systems x1 ⫽ r cos ,

x2 ⫽ r sin ,

1 ⫽ cos ,

The above integrals can then be written as

2 ⫽ sin .

68

EIGENSTRAINS

冕 冕

I1 ⫽

2

⬁

0

0

I2 ⫽

eircos(⫺) sin cos2 d d, [1 ⫹  cos2 sin2 ]

冕 冕 2

⬁

0

0

(3.A.6)

eircos(⫺) sin3 d d. [1 ⫹  cos2 sin2 ]

(3.A.7)

冕

(3.A.8)

Next, consider the integral I⫽

⬁

0

eircos(⫺) d.

Making use of the expansion

冘 i J (r)cos[k( ⫺ )],

(3.A.9)

冘 i J (r)cos[k( ⫺ )]冊 d.

(3.A.10)

eircos(⫺) ⫽ J0(r) ⫹ 2

⬁

k

k

k⫽1

we have I⫽

冕

⬁

0

冉

J0(r) ⫹ 2

⬁

k

k

k⫽1

where Jk(●) is the Bessel function of order k. Since

冕

⬁

0

1 Jk(r) d ⫽ , r

for any k ⱖ 0 and r ⬎ 0,

(3.A.11)

we obtain

冉 冘 i cos[k( ⫺ )]冊 1 ⫽ 冉1 ⫹ 2 冘 i [cos(k)cos(k) ⫹ sin(k)sin(k)]冊. r

I⫽

1 1⫹2 r

⬁

k

k⫽1 ⬁

k

k⫽1

Substituting (3.A.12) into (3.A.6)–(3.A.7) yields

(3.A.12)

APPENDIX 3.A

I1 ⫽ I2 ⫽

69

2 r

冘 i [a

cos(k) ⫹ b1k sin(k)],

(3.A.13)

k⫽0

2 r

冘 i [a

cos(k) ⫹ b2k sin(k)],

(3.A.14)

⬁

k

1k

⬁

k

2k

k⫽0

where a10 ⫽

1 2

冕

2

0

sin cos2 d , [1 ⫹  cos2 sin2 ]

(3.A.15)

a1k ⫽

冕

(3.A.16)

0

cos(k)sin cos2 d, [1 ⫹  cos2 sin2 ]

b1k ⫽

冕

sin(k)sin cos2 d, [1 ⫹  cos2 sin2 ]

(3.A.17)

a20 ⫽

2

2

0

1 2

冕

2

0

sin3 d , [1 ⫹  cos2 sin2 ]

(3.A.18)

a2k ⫽

冕

(3.A.19)

0

cos(k)sin3 d , [1 ⫹  cos2 sin2 ]

b2k ⫽

冕

sin(k)sin3 d . [1 ⫹  cos2 sin2 ]

(3.A.20)

2

2

0

For isotropic materials,  ⫽ 0. The nonzero coefﬁcients from (3.A.15) to (3.A.20) are b11 ⫽ b13 ⫽ , 4

b21 ⫽

3 , 4

b23 ⫽ ⫺ . 4

Thus, I1 ⫽ I2 ⫽

i i [sin ⫺ sin(3)] ⫽ [2 sin3 ⫺ sin ], 2r r

i i [3 sin ⫹ sin(3)] ⫽ [3 sin ⫺ 2 sin3 ]. 2r r

70

EIGENSTRAINS

APPENDIX 3.B

The following integrals are given in Mura (1987, pp. 17):

冉冊

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

2ei(1x1⫹2x2) x d1 d2 ⫽ 2 tan⫺1 2 , 2 2 1( 1 ⫹ 2) x1

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

冕 冕 冕 冕 ⬁

⬁

⫺⬁

⫺⬁

⬁

⬁

⫺⬁

⫺⬁

(3.B.1)

21ei(1x1⫹2x2) ⫺ x x d1 d2 ⫽ 2 1 22, 2 2 2 ( 1 ⫹ 2) x1 ⫹ x2

(3.B.2)

ei(1x1⫹2x2) d1 d2 ⫽ ⫺ log(x 21 ⫹ x 22), 21 ⫹ 22

(3.B.3)

22ei(1x1⫹2x2) x 22 2 2 d d ⫽ ⫺ log(x ⫹ x ) ⫺ . 1 2 1 2 ( 12 ⫹ 22)2 2 x 12 ⫹ x 22

(3.B.4)

REFERENCES Burgers, J. M. (1939). ‘‘Some considerations on the ﬁelds of stress connected with dislocations in a regular crystal lattice, I, II,’’ Proc. Kon. Nederl. Akad. Wetensch., Vo. 42, pp. 293–324 and pp. 378–399. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston, MA, Chapter 1.

SUGGESTED READING Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York.

4 INCLUSIONS AND INHOMOGENEITIES In this chapter, we ﬁrst introduce the concepts of inclusions and inhomogeneities. We will then derive the stress and displacement ﬁelds due to the presence of inclusions and inhomogeneities. Finally, we will derive explicitly solutions to ellipsoidal inclusions and inhomogeneities.

4.1 DEFINITIONS OF INCLUSIONS AND INHOMOGENEITIES

Although the terms inclusion and inhomogeneity are used interchangeably in the literature, we will use them differently throughout this book. The readers are advised that the distinction between these two terms made in this book is mainly for the convenience of discussion. An inclusion is deﬁned as a subdomain ⍀ in a domain D, where eigenstrain *(x) is given in ⍀ and is zero in D ⫺ ⍀. The material ij properties in ⍀ and in D ⫺ ⍀ are the same. The domain outside ⍀, that is, D ⫺ ⍀, is called the matrix; see Figure 4.1. For linear elastic material, this can be stated as ⍀ is an inclusion ⇔ *(x) ⫽0 ij

for x 僆 ⍀ 僆 D

ij*(x) ⫽ 0

for x 僆 D ⫺ ⍀

Lijkl is uniform throughout D Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

71

72

INCLUSIONS AND INHOMOGENEITIES

ε ij* (x) = 0 ε ij* (x) ≠ 0 Ω

L(0) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.1 Inclusion.

An inhomogeneity is deﬁned as a subdomain ⍀ in domain D, where the material properties in ⍀ and in D ⫺ ⍀ are different. The domain outside ⍀, that is, D ⫺ ⍀, is called the matrix; see Figure 4.2. For linear elastic material, this can be stated as ⍀ is an inhomogeneity ⇔ Lijkl (x) ⫽

再

L(1) in ⍀ 僆 D ijkl (0) Lijkl in D ⫺ ⍀ no eigenstrain throughout D

From the above deﬁnition, we see that inclusion is nothing but a distribution of eigenstrains in an otherwise homogeneous material. The presence of eigenstrain may cause stresses in the material. On the other hand, inhomogeneity is a foreign material embedded in an otherwise homogeneous matrix material. If the inhomogeneity ﬁts into the sur-

ε ij* (x) = 0 ε ij* (x) = 0 Ω

L(1) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.2 Inhomogeneity.

4.2

INTERFACE CONDITIONS

73

rounding matrix perfectly, there will not be stress produced either in the matrix or in the inhomogeneity.

4.2 INTERFACE CONDITIONS

Consider an inclusion ⍀ in an elastic domain D of elastic stiffness tensor Lijkl. The interface between ⍀ and its surrounding material will be denoted by S. We wish to investigate the continuity of ﬁeld quantities (displacements, strain, stress) across this interface. If the material across the interface S is continuous (e.g., no gap and slip), we call it a perfect interface. For perfect interface, the displacement and the interfacial traction across the interface must be continuous, that is, ⌬ui ⬅ ui(S⫹) ⫺ ui(S⫺) ⫽ 0,

(4.2.1)

⌬ijnj ⬅ [ij(S⫹) ⫺ ij(S⫺)]nj ⫽ 0.

(4.2.2)

where nj is the outward unit normal to the interface S, and ui(S⫹) and ij(S⫹) are the values of ui(x) and ij(x) evaluated at the positive side of S, while ui(S⫺) and ij(S⫺) are the values of ui(x) and ij(x) evaluated at the negative side of S. The positive side of S is the side to which nj points; see Figure 4.3. It then follows from (4.2.1) that the displacement gradient may have a jump across the interface given by ⌬ui, j ⬅ ui, j(S⫹) ⫺ ui, j(S⫺) ⫽ inj,

(4.2.3)

where i is the magnitude of the jump that will be determined shortly. Note that the right-hand side of (4.2.3) is orthogonal to the tangent vector of S. Thus, Eq. (4.2.3) simply says that, due to the constraint of (4.2.1), the tangential derivatives of the displacements along S must be continuous.

S

S−

n S+

Figure 4.3 Interface with positive and negative sides.

74

INCLUSIONS AND INHOMOGENEITIES

Next, making use of Hooke’s law (3.1.5) in (4.2.2) and the fact that the stiffness tensor is the same inside and outside the inclusion yields Lijkl (⌬uk,l ⫺ ⌬*)n kl j ⫽ 0,

(4.2.4)

⌬* *(S⫹) ⫺ kl*(S⫺) ⫽ ⫺kl*(S⫺). kl ⬅ kl

(4.2.5)

⫹ *(S ) ⫽ 0, kl

(4.2.6)

where

Since

substitution of (4.2.3) into (4.2.4) gives ⫺ Lijkl nl njk ⫽ ⫺Lijkl*(S )nj. kl

(4.2.7)

This is a system of algebraic equations for k. Comparing it with (2.6.13), one can easily write out the solution ⫺ i ⫽ ⫺Ljkmn* mn(S )nk Nij(n)/D(n),

(4.2.8)

Nij(n) ⫽ –21 ikljmnKkm(n)Kln(n),

(4.2.9)

D(n) ⫽ mnlKm1(n)Kn2(n)Kl3(n),

(4.2.10)

Kik(n) ⫽ Lijkl ninj,

(4.2.11)

where

ijk ⫽ permutation tensor.

Notice that Nij is the cofactor of Kij and D is the determinant of Kij. Therefore, Nij /D is the inverse of Kij. Expressions of Nij and D for isotropic, cubic, and transversely isotropic materials are given in Appendix 4.A. Substituting (4.2.8) into (4.2.3) we arrived at ⫺ ⌬ui, j ⫽ ⫺Llkmn* mn(S )nknj Nil (n)/D(n).

It thus follows that

(4.2.12)

4.2

INTERFACE CONDITIONS

⫺ ⌬ij ⫽ ⫺–12 Llkmn* mn(S )nk{nj Nil (n) ⫹ ni Njl (n)}/D(n),

75

(4.2.13)

⌬ij ⬅ ij(S⫹) ⫺ ij(S⫺) ⫽ Lijkl (⌬uk,l ⫺ ⌬kl *) ⫺ ⫺1 ⫽ Lijkl{⫺Llkmn* )}. mn(S )nknj Nil (n)/D(n) ⫹ *(S kl

(4.2.14)

Note that for a given inclusion the right-hand sides of (4.2.13) and (4.2.14) involve only known quantities. Therefore, if the strain and stress are known within the inclusion, the corresponding strain and stress just outside the inclusion can be computed from these equations. This proves the following uniqueness theorem. Uniqueness Theorem for Inclusion–Matrix Interface If the stress or strain tensor is known locally at one side of the interface between an inclusion and the surrounding matrix, then their jumps and consequent values at the other side of the interface are explicitly determinable in terms of the matrix moduli, the eigenstrain in the inclusion, and the interface normal. Let us now consider the continuity conditions at the interface between an inhomogeneity and its surrounding matrix. Let the stiffness tensor of inhomogeneity be L(1) ijkl and that of the matrix be Lijkl. Further, we assume that the interface is a perfect one, that is, the continuity conditions (4.2.1) and (4.2.2) are satisﬁed. Consequently, Eq. (4.2.3) also holds. Making use of Hooke’s law, we have ij(S⫹) ⫽ Lijkluk,l (S⫹),

⫺ ij(S⫺) ⫽ L(1) ijkluk,l (S ).

(4.2.15)

Substituting the above into (4.2.2) yields ⫺ Lijkluk,l (S⫹)nj ⫽ L(1) ijkluk,l (S )nj.

(4.2.16)

Eliminating uk,l(S⫹) in the above equation by using (4.2.3), we arrive at the following equation for i: Lijklknl nj ⫽ ⌬Lijkluk,l (S⫺)nj, where

(4.2.17)

76

INCLUSIONS AND INHOMOGENEITIES

⌬Lijkl ⫽ L(1) ijkl ⫺ Lijkl.

(4.2.18)

Similar to (4.2.7), Eq. (4.2.17) can be solved to yield i ⫽ ⌬Ljkmnum,n(S⫺)nk Nij(n)/D(n) ⫽ ⌬Ljkmnmn(S⫺)nk Nij(n)/D(n).

(4.2.19) Making use of the above in (4.2.3) yields ⌬ui, j ⫽ ⌬Llkmnmn(S⫺)nl nj Nik(n)/D(n).

(4.2.20)

Thus, we have ⌬ij ⫽ –12 ⌬Llkmnmn(S⫺1)nl{nj Nik(n) ⫹ ni Njk(n)}/D(n).

(4.2.21)

Further, combination of (4.2.20) and the ﬁrst of (4.2.15) gives ij(S⫹) ⫽ Lijkl{kl (S⫺) ⫹ ⌬Lpqmnmn(S⫺)nl nqNkp(n)/D(n)}

or ⌬ij ⫽ ⌬Lpqmnmn(S⫺)[Lijkl nl nqNkp(n)/D(n) ⫺ ␦pq].

(4.2.22)

Again, we notice from (4.2.21) and (4.2.22) that for a given inhomogeneity, if the strain or the stress ﬁeld on one inside the interface is known, the corresponding strain and stress immediately on the other side of interface can be computed. Therefore, similar to the inclusion case, we can state a uniqueness theorem for the inhomogeneity. Uniqueness Theorem for Inhomogeneity–Matrix Interface If the stress or strain tensor is known locally at one side of the interface between an inhomogeneity and its surrounding matrix, then their jumps and consequent values at the other side of the interface are explicitly determinable in terms of the moduli of the inhomogeneity and the matrix and the interface normal.

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

77

4.3 ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

Consider an inﬁnite domain D containing an ellipsoidal inclusion ⍀ with uniform eigenstrain *. ij Let the stiffness tensor of the material be Lijkl, and the ellipsoidal inclusion (Figure 4.4) be described by ⍀ ⫽ {x1, x2, x3; (x1 /a1)2 ⫹ (x2 /a2)2 ⫹ (x3 /a3)2 ⱕ 1},

(4.3.1)

where a1, a2, and a3 are the semiaxes of the ellipsoid. Since ij*(x) ⫽

再

* ij

for x 傺 ⍀ for x 傺 ⍀,

0

(4.3.2)

it then follows from Green’s function formulation of the general solution to eigenstrain problems (3.3.14), (3.3.15), and (3.3.16) that ui(x) ⫽ Lmjklkl*

冕 ⭸G (x⭸y ⫺ y) dV(y), ⬁ mi

⍀

(4.3.3)

j

⍀ ij(x) ⫽ Lklmn* mnPijkl (x),

(4.3.4)

⍀ ij(x) ⫽ Lijkl (Lpqmnmn * Pklpq (x) ⫺ kl*),

(4.3.5)

where ⌫⬁ijkl (x, y) ⫽

冋

册

1 ⭸2Gki⬁ (x, y) ⭸2G⬁kj(x, y) ⭸2Gli⬁(x, y) ⭸2Glj⬁(x, y) ⫹ ⫹ ⫹ 4 ⭸xj ⭸yl ⭸xi ⭸yl ⭸xj ⭸yk ⭸xi ⭸yk

(4.3.6) was introduced by (3.3.17), and x3 x2

ε ij* Ω

x1

Figure 4.4 Ellipsoidal inclusion ⍀.

78

INCLUSIONS AND INHOMOGENEITIES

P⍀ijkl (x) ⫽

冕⌫ ⍀

⬁ ijkl

(x, y) dV(y).

(4.3.7)

For convenience, we introduce ⍀ Sijkl (x) ⫽ LmnklPijmn (x).

(4.3.8)

Then (4.3.4) and (4.3.5) can be rewritten as ij(x) ⫽ Sijkl (x)*, kl

ij(x) ⫽ Lijkl{Sklmn(x)* mn ⫺ *} kl ⫽ Lijkl{Sklmn(x) ⫺ Iklmn}* mn,

(4.3.9) (4.3.10)

where Iijkl is the fourth-order identity tensor given by Iijkl ⬅ –12 (␦ik␦jl ⫹ ␦il␦jk).

(4.3.11)

It is noted that (4.3.3)–(4.3.10) are valid for both x inside and outside the inclusion ⍀. We now show that P⍀ijkl (x) is a constant fourth-order tensor for x inside ⍀, that is, P⍀ijkl (x) ⫽ Pijkl ⫽

a1a2a3 4

冕H Sˆ

ijkl

ˆ ), x 傺 ⍀ ()a⫺3D⫺1() dS(

(4.3.12)

where Pijkl is referred to as the Hill polarization tensor, and Hijkl () ⫽ Nik()jl ⫹ Njk()il ⫹ Nil ()jk ⫹ Njl ()ik, a ⫽ 兹(a1ˆ 1)2 ⫹ (a2ˆ 2)2 ⫹ (a3ˆ 3)2.

(4.3.13) (4.3.14)

In (4.3.12), the integration is over the surface of the unit sphere Sˆ as shown in Figure 4.5. To this end, let us consider the integral ξ3 1

ξ1

ξ2 Sˆ

ˆ Figure 4.5 Unit sphere S.

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

Gijkl (x) ⫽

冕 ⭸ G⭸x (x,⭸ ) d ⫽ ⫺⭸x⭸ ⭸x 冕 G (x, ) d. ⬁ ki

2

⍀

79

2

j

l

j

l

(4.3.15)

ik

⍀

Replacing Green’s function in the above integral by its expression (2.6.37), we have 1 ⭸2 Gijkl (x) ⫽ ⫺ 2 8 ⭸xj ⭸xl

冕 再冕 ␦[ˆ 䡠 (x ⫺ )]N (ˆ )D ⍀

⫺1

ik

Sˆ

冎

ˆ ˆ ) d. (ˆ ) dS(

(4.3.16) Exchanging the order of integration, 1 ⭸2 Gijkl (x) ⫽ ⫺ 2 8 ⭸xj ⭸xl

冕 再冕 ␦[ˆ 䡠 (x ⫺ )] d冎 N (ˆ )D

ˆ ˆ ). (ˆ ) dS(

⫺1

ik

⍀

Sˆ

(4.3.17) Making use of the result in Appendix 4.A, we have aaa ⭸2 Gijkl (x) ⫽ ⫺ 1 2 3 8 ⭸xj ⭸xl ⫽

a1a2a3 4

冕 ˆ ˆ a Sˆ

j l

冕 a1 [a ⫺ (ˆ 䡠 x) ]N (ˆ )D 2

Sˆ

2

ik

3

ˆ ˆ ) (ˆ ) dS(

⫺1

ˆ ˆ ). Nik(ˆ )D⫺1(ˆ ) dS(

⫺3

(4.3.18)

Substituting (4.3.18) into (4.3.7) yields (4.3.12). Consequently, it follows from (4.3.8) that for x inside the inclusion ⍀, Sijkl ⫽ LmnklPijmn ⫽ lmnkl

a1a2a3 4

冕H Sˆ

ijmn

ˆ ). ()a⫺3D⫺1() dS(

(4.3.19)

This proves (4.3.12). Consequently, it follows from (4.3.9) that the total strain (and the stress as well) is uniform inside the ellipsoidal inclusion when the eigenstrain is uniform, that is, ij(x) ⫽ Sijkl* kl

for x 傺 ⍀

(4.3.20)

where the fourth-order tensor Sijkl is commonly referred to as the Eshelby inclusion tensor, and (4.3.20) is called the Eshelby ellipsoidal inclusion solution. It can be seen from (4.3.12) that

80

INCLUSIONS AND INHOMOGENEITIES

Sijkl ⫽ Sjikl ⫽ Sijlk.

(4.3.21)

However, the Eshelby tensor does not possess the diagonal symmetry, that is, in general, Sijkl ⫽ Sklij. Having obtained the total strain within the inclusion, the stress ﬁeld within the inclusion can be computed from Hooke’s law (3.1.5): ij ⫽ Lijkl (kl ⫺ *) *, kl ⫽ Lijklkl ⫹ ij

(4.3.22)

* ij ⫽ ⫺Lijkl* kl

(4.3.23)

where

is called the stress polarization. It is the stress in the inclusion caused by the eigenstrain *ij when the inclusion is not allowed to deform at all (i.e., the total strain is zero, kl ⫽ 0). This can be easily understood if we recalled the example in Chapter 3, where an aluminum ball is heated while the ball is constrained so the total strain is zero. The corresponding stress generated in the ball, according to (3.2.6), is ij ⫽ ij* ⫽ ⫺␣ALnnij ⌬T

because the eigenstrain in this case is ␣A ⌬T. It then follows from (4.3.19) that the Eshelby solution (4.3.20) can be written as ij ⫽ Sijkl* kl ⫽ PijmnLmnkl* kl ⫽ ⫺Pijmn * mn,

(4.3.24)

where Pijmn ⫽ Sijkl Mklmn is called the stress polarization. Note that this is not the stress on the inclusion. The stress on the inclusion (4.3.22) is given by ij ⫽ Lijkl (Sklmn* mn ⫺ *) kl ⫽ ⫺Qijkl*, kl

where the fourth-order tensor Qijkl ⫽ Lijmn(Imnkl ⫺ Smnkl)

(4.3.25)

can be viewed as the dual of the stress polarization tensor Pijkl.

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

81

One can also show that L(I ⫺ S) ⫽ (I ⫺ ST)L

(4.3.26)

is positive deﬁnite. To this end, consider the total strain energy of the ellipsoidal inclusion problem:

冕 ( ⫺ *) dv ⫽ 21 冕 u dv ⫺ 21 冕 * dv 1 1 ⫽ 冕 [( u ) ⫺ u ] dv ⫺ 冕 L ( ⫺ *)* dv 2 2 1 1 1 ⫽ 冕 u n ds ⫺ 冕 u dv ⫺ 冕 L ( ⫺ *)* dv, 2 2 2

U⫽

1 2

ij

D

ij

ij

D

ij i , j

D

ij, j i

ij i j

S⬁

ij i, j

D

⍀

ij, j i

ij ij

⍀

ijkl

kl

⍀

kl

ijkl

kl

ij

kl

ij

(4.3.27) where S⬁ is the boundary of D. Since D is an inﬁnite domain and the stress vanishes at inﬁnity, the surface integral must be zero. By virtue of the equilibrium equation, the second term on the right-hand side of (4.3.27) is also zero. Therefore, we have

冕 (* ⫺ )L* dv ⫽ 21 冕 (* ⫺ S*)L* dv 1 1 ⫽ 冕 *(I ⫺ S )L* dv ⫽ 冕 *L(I ⫺ S)* dv. 2 2

U⫽

1 2

⍀

⍀

T

⍀

⍀

(4.3.28)

Since the strain energy must be positive and becomes zero only if the eigenstrain is zero, we must have

冕 *(I ⫺ S )L* dv ⫽ 冕 *L(I ⫺ S)* dv ⱖ 0. T

⍀

⍀

(4.3.29)

Note that S is independent of the size of ⍀ and (4.3.29) should hold for any size of ⍀, we can conclude from (4.3.29) that *(I ⫺ ST)L* ⫽ *L(I ⫺ S)* ⱖ 0,

(4.3.30)

and the equal sign is realized only when * ⫽ 0. This proves that L(I ⫺ S) ⫽ (I ⫺ ST)L is positive deﬁnite. Two corollaries of (4.3.30) are

82

INCLUSIONS AND INHOMOGENEITIES

LS ⫽ STL,

(4.3.31)

and (I ⫺ S) is nonsingular. Next, we show that S is also nonsingular. We begin by computing the strain energy stored in the region outside the inclusion:

冕 1 ⫽ 冕 2

Um ⫽

1 2

D⫺⍀

D⫺⍀

ijij dv ⫽

1 2

冕

D⫺⍀

ijui, j dv

[(ijui), j ⫺ ij, jui] dv.

(4.3.32)

Again, the second term on the right hand of (4.3.32) vanishes because of equilibrium. The ﬁrst term can be converted to a surface integral by using the divergence theorem: Um ⫽

1 2

冕

S⬁

ijuinj ds ⫺

1 2

冕 u n ds, S

(4.3.33)

ij i j

where the negative sign of the second term comes about because nj is the outward normal vector of ⍀. The ﬁrst term vanishes because the stresses go to zero at inﬁnity. Thus, we have 1 Um ⫽ ⫺ 2

冕 u n ds ⫽ ⫺12 冕 u S

ij i j

⍀

ij i, j

1 dv ⫽ ⫺ 2

冕 ⍀

ij ij

dv.

(4.3.34)

If S is singular, there must exist an eigenstrain ﬁeld ˆ * kl ⫽ 0

(4.3.35)

such that ij ⫽ Sijklˆ * kl ⫽ 0

on ⍀.

(4.3.36)

In what follows, we will show that (4.3.36) contradicts (4.3.35), that is, if (4.3.36) is satisﬁed, then (4.3.35) cannot be true, thus proving that S cannot be singular. To this end, ﬁrst compute the corresponding stress on ⍀ when (4.3.36) holds:

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

ij ⫽ Lijkl (kl ⫺ ˆ *) ˆ *. kl ⫽ ⫺Lijkl kl

83

(4.3.37)

Substitution of (4.3.36) into (4.3.34) leads to Um ⫽ 0. It then follows from (4.3.32) that ij ⫽ ij ⫽ 0 in the region outside the inclusion, or ij(S⫹) ⫽ 0. On the other hand, the traction continuity condition on the inclusion/ matrix interface yields 0 ⫽ ij(S⫹)nj ⫽ ij(S⫺)nj ⫽ ⫺Lijklˆ *n kl j,

(4.3.38)

where (4.3.37) has been used in deriving the last equation of (4.3.38). Note that Lijkl ˆ * kl is a constant second-order tensor while nj varies along the boundary. For (4.3.38) to hold for the entire boundary, we must have Lijklˆ * ˆ kl* ⫽ 0. kl ⫽ 0. Since Lijkl is nonsingular, we end up with This contradicts (4.3.35). Therefore, S cannot be singular. We also note that Sijkl is independent of the eigenstrain. But, it does depend on the matrix material. For general anisotropic materials, numerical methods are typically required to carry out the integral in Sijkl. For isotropic materials, the integral can be written in terms of elliptical integrals and explicit expression in terms of elemental functions can be obtained for certain special cases. For example, the Eshelby tensor Sijkl for a spherical inclusion in an isotropic material is a fourth-order isotropic tensor: Sijkl ⫽ ␥␦ij␦kl ⫹ ␦(␦ik␦jl ⫹ il␦jk ⫺ –23 ␦ij␦kl),

(4.3.39)

where ␥⫽

K 3K ⫹ 4

⫽

1⫹v , 9(1 ⫺ v)

␦⫽

3(K ⫹ 2) 4 ⫺ 5v ⫽ . 5(3K ⫹ 4) 15(1 ⫺ v) (4.3.40)

Using the symbolic notation introduced in (1.3.3), we can simply write S ⫽ (3␥, 2␦).

(4.3.41)

The expressions of Sijkl for inclusions of special shapes are given in Appendix 4.B. Before closing this section, we mention that (4.3.20) is no longer valid for a material point outside the inclusion ⍀. To obtain the strain

84

INCLUSIONS AND INHOMOGENEITIES

and stress ﬁelds outside the inclusion, one needs to evaluate the integral in (4.3.7) for x outside the ellipsoid. An alternative approach is to use the continuity conditions at the interface between an inclusion and its surrounding matrix. Since the stresses and strains are known inside the inclusion, the stresses and strains, based on the uniqueness theorem, can be obtained just outside the inclusion. This allows us to compute the strain and stress ﬁeld anywhere outside the inclusion. The stresses and strains outside the inclusion will not be needed in this book. So, we will not present them. However, we do note that for x outside of ⍀r, Sr(x) decades as 㛳x㛳⫺3 as 㛳x㛳 → ⬁. Readers are referred to the Suggested Readings at end of this chapter for further details.

4.4 ELLIPSOIDAL INHOMOGENEITIES

Consider an elastic body D with elastic modulus L0 containing an ellipsoidal inhomogeneity ⍀ with elastic modulus tensor L1. Let D be subjected to surface traction p0 ⫽ 0 䡠 n on the boundary of D, as shown in Figure 4.6. We are to ﬁnd the stress ﬁelds in D. Obviously, when L1 ⫽ L0, the material is homogeneous. Consequently, the total stress ﬁeld becomes uniform throughout D (see Figure 4.7), and is given by t ⫽ 0

(4.4.1)

It is therefore conceivable that, through the principle of linear superposition, when L1 is different from L0, the total stress ﬁeld in D can be written as

ε ij* (x) = 0 ε ij* (x) = 0 Ω

L(1) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.6 Ellipsoidal inhomogeneity.

4.4

ELLIPSOIDAL INHOMOGENEITIES

85

ε ij* (x) = 0 ε ij* (x) = 0

(0) L(1) ijkl ( x ) = Lijkl ( x )

Ω L(0) ijkl ( x)

D

Figure 4.7 Uniform stress ﬁeld in homogeneous body.

t ⫽ 0 ⫹ ,

(4.4.2)

where is the stress perturbation due to the presence of the inhomogeneity ⍀. Obviously, the perturbed stress ﬁeld should satisfy the equilibrium equations and the homogeneous boundary condition 䡠n⫽0

on S.

(4.4.3)

If 0 is used to denote the strain ﬁeld corresponding to 0, that is, 0 ⫽ L00,

(4.4.4)

then the total strain on the inclusion can be written as t ⫽ 0 ⫹ ,

(4.4.5)

where is the perturbed strain ﬁeld due to the presence of the inhomogeneity. Application of Hooke’s law in D and D ⫺ ⍀ yields, respectively, t ⫽ 0 ⫹ ⫽ L1(0 ⫹ ) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

(4.4.6)

in D ⫺ ⍀,

(4.4.7)

Our task is to solve for and by the so-called equivalent inclusion method. To this end, let us consider a homogeneous body D with elastic modulus tensor L0 everywhere, containing an inclusion ⍀ with eigen-

86

INCLUSIONS AND INHOMOGENEITIES

strain * (the value of which is to be determined); see Figure 4.8. The eigenstrain * is introduced here to simulate the inhomogeneity. In other words, we are trying to create an inclusion problem which, by properly adjusting the value of *, has the same stress ﬁeld as that of the inhomogeneity problem. For the inclusion problem shown in Figure 4.8, Hooke’s law gives t ⫽ 0 ⫹ ⫽ L0(0 ⫹ ⫺ *) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

(4.4.8)

in D ⫺ ⍀,

(4.4.9)

where 0 and 0 are the ﬁelds in D due to the applied traction p0 ⫽ 0 䡠 n when the inclusion is absent, and and are the ﬁelds due to eigenstrain * in the inclusion ⍀. From the Eshelby solution (4.3.20), ⫽ S*,

(4.4.10)

we can rewrite (4.4.8) as t ⫽ 0 ⫹ ⫽ L0(0 ⫹ S* ⫺ *)

in ⍀.

(4.4.11)

Now, recall that we created this inclusion problem to simulate the inhomogeneity problem. We want to adjust the eigenstrain * so that the stress ﬁeld in the inclusion ⍀ given by (4.4.11) is the same as the stress ﬁeld in the inhomogeneity ⍀ given by (4.4.6), namely,

ε ij* (x) = 0 ε ij* (x) ≠ 0 Ω

L(0) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.8 Ellipsoidal inclusion.

4.4

ELLIPSOIDAL INHOMOGENEITIES

L0(0 ⫹ S* ⫺ *) ⫽ L1(0 ⫹ )

in ⍀.

87

(4.4.12)

Making use of the Eshelby solution (4.3.20) again yields L0(0 ⫹ S* ⫺ *) ⫽ L1(0 ⫹ S*)

in ⍀.

(4.4.13)

This is called the equivalent inclusion equation. From this equation, the eigenstrain needed to simulate the inhomogeneity can be solved: * ⫽ ⫺[(L1 ⫺ L0)S ⫹ L0]⫺1(L1 ⫺ L0)0 ⫽ ⫺((L1 ⫺ L0)⫺1[(L1 ⫺ L0)S ⫹ L0])⫺10 ⫽ ⫺[S ⫹ (L1 ⫺ L0)⫺1L0)]⫺10.

(4.4.14)

The total strain on the inclusion thus follows from (4.4.5): t ⫽ 0 ⫹ ⫽ 0 ⫹ S* ⫽ T0,

(4.4.15)

where T ⫽ I ⫺ S[S ⫹ (L1 ⫺ L0)⫺1L0]⫺1 ⫽ [S ⫹ (L1 ⫺ L0)⫺1L0) ⫺ S][S ⫹ (L1 ⫺ L0)⫺1L0]⫺1 ⫽ (L1 ⫺ L0)⫺1L0[S ⫹ (L1 ⫺ L0)⫺1L0]⫺1 ⫽ ([S ⫹ (L1 ⫺ L0)⫺1L0]L0⫺1(L1 ⫺ L0))⫺1 ⫺1 ⫽ [SL⫺1 0 (L1 ⫺ L0) ⫹ I]

(4.4.16)

or ⫺1 T ⫽ [I ⫹ SL⫺1 0 (L1 ⫺ L0)] .

(4.4.17)

Since the stresses in the inclusion are the same as those in the inhomogeneity, the total stress in the inhomogeneity is, therefore, given by t ⫽ 0 ⫹ ⫽ L0(0 ⫹ S* ⫺ *),

(4.4.18)

where * is given by (4.4.14). This completes the solution of the inhomogeneity problem.

88

INCLUSIONS AND INHOMOGENEITIES

To close this section, we need to mention that when the eigenstrain is given by (4.4.14), the stresses for the inclusion problem and the inhomogeneity problem are identical not only inside ⍀ but also in D ⫺ ⍀. This can be shown by using the uniqueness theorem for inclusions and inhomogeneities.

4.5 INHOMOGENEOUS INHOMOGENEITIES

Sometimes an inhomogeneity may possesses its own eigenstrains. Such inhomogeneities are called inhomogeneous inhomogeneities. In other words, a subdomain occupied by foreign material may involve a distribution of eigenstrains as well. Examples of such inhomogeneous inhomogeneities include the formation of martensite blades in quenched carbon steels and precipitations in alloys. To solve for the inhomogeneous inhomogeneity problem, let us consider the inhomogeneity shown in Figure 4.1. Let D be subjected to surface traction p0 ⫽ 0 䡠 n on the boundary. Furthermore, we assume that a uniform eigenstrain p is prescribed on the inhomogeneities ⍀. We are to ﬁnd the stress ﬁeld in D. If 0 is used to denote the strain ﬁeld corresponding to 0, that is, 0 ⫽ L00,

(4.5.1)

then application of Hooke’s law in D and D ⫺ ⍀ yields, respectively, t ⫽ 0 ⫹ ⫽ L1(0 ⫹ ⫺ p) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

(4.5.2)

in D ⫺ ⍀,

(4.5.3)

where and are the perturbed stress and strain ﬁelds, respectively, caused by the sum of two factors, the inhomogeneity and the eigenstrain p in the inhomogeneity. Our task is to solve for and . Imagine that the inhomogeneous inhomogeneity is being simulated by an inclusion in a homogeneous matrix with elastic stiffness tensor L, where the total eigenstrain on the inclusion is p ⫹ *. Then, (4.5.2) and (4.5.3) can be rewritten as

4.5

INHOMOGENEOUS INHOMOGENEITIES

t ⫽ 0 ⫹ ⫽ L0(0 ⫹ ⫺ p ⫺ *) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

in D ⫺ ⍀.

89

(4.5.4) (4.5.5)

Consequently, the equivalent inclusion equation becomes L0(0 ⫹ ⫺ p ⫺ *) ⫽ L1(0 ⫹ ⫺ p)

in ⍀.

(4.5.6)

The Eshelby solution (4.3.20) in this case takes the form of ⫽ S** ⫽ S(p ⫹ *),

(4.5.7)

** ⫽ p ⫹ *.

(4.5.8)

where

Introducing (4.5.7) into (4.5.6) yields L0(0 ⫹ S** ⫺ **) ⫽ L1(0 ⫹ S** ⫺ p)

in ⍀.

(4.5.9)

This can be solved to obtain ** ⫽ [L0(S ⫺ I) ⫺ L1S]⫺1(⌬L M00 ⫺ L1p),

(4.5.10)

⌬L ⫽ L1 ⫺ L0.

(4.5.11)

where

Note that S[L0(S ⫺ I) ⫺ L1S]⫺1 ⫽ S[L0(S ⫺ I) ⫺ L1S]⫺1 ⫽ ⫺(L0S⫺1 ⫺ L0 ⫹ L1)⫺1 ⫽ ⫺(H ⫹ L1)⫺1,

(4.5.12) where

90

INCLUSIONS AND INHOMOGENEITIES

H ⫽ L0S⫺1 ⫺ L0 ⫽ L0(S⫺1 ⫺ I) ⫽ P⫺1 ⫺ L0

(4.5.13)

is known as Hill’s constraint tensor. Therefore, (4.5.10) can be written alternatively, ** ⫽ ⫺S⫺1(H ⫹ L1)⫺1(⌬L M00 ⫺ L1p).

(4.5.14)

Once the eigenstrain ** is known, the total strain on the inhomogeneous inhomogeneity can be computed as t ⫽ 0 ⫹ ⫽ 0 ⫹ S**.

(4.5.15)

Therefore, substituting (4.5.14) into (4.5.15), we can write the total strain in the inhomogeneous inhomogeneity as t ⫽ 0 ⫹ ⫽ 0 ⫺ (H ⫹ L1)⫺1(⌬L M00 ⫹ p),

(4.5.16)

where the stress polarization is deﬁned by p ⫽ ⫺L1p.

(4.5.17)

Similarly, the total stress on the inhomogeneous inhomogeneity is given by (4.5.4) t ⫽ L0(0 ⫹ S** ⫺ **) ⫽ 0 ⫺ L0(I ⫺ S⫺1)(H ⫹ L1)⫺1(⌬L M00 ⫹ p)

in ⍀

⫽ 0 ⫹ H(H ⫹ L1)⫺1(⌬L M00 ⫹ p).

(4.5.18)

Making use of (4.5.16) in (4.5.18) gives an alternative form: t ⫽ 0 ⫺ H(t ⫺ 0)

in ⍀.

(4.5.19)

In the absence of the applied loading, (4.5.16) and (4.5.18) become, respectively, t ⫽ ⫺(H ⫹ L1)⫺1 p, t ⫽ H(H ⫹ L1)⫺1 p ⫽ ⫺Ht

(4.5.20) in ⍀.

(4.5.21)

PROBLEMS

91

PROBLEMS

4.1 A spherical cavity of radius a is present in an otherwise uniform, isotropic, linearly elastic solid of inﬁnite extent with Poisson’s ratio . A uniaxial tension 0ij ⫽ 0␦i3␦j3 is applied at inﬁnity. (See Fig. 4.9.) 1. Use the equivalent inclusion method to ﬁnd the stress components ij(x1, x2, x3) at points (0, 0, a) and (0, a, 0). 2. Deﬁne the stress concentration factors by t ⫽

33(0, a, 0) , 0

c ⫽

11(0, 0, a) 0

and plot the stress concentration factors versus the Poisson’s ratio . 4.2 Prove that the stress polarization tensor Pijkl symmetric and positive-deﬁnite. Further, *M ij ijkl * kl ⱖ *P ij ijkl * kl ⱖ 0

for any arbitrary second-order tensor *. ij 4.3 Prove the identity ⫺(L1 ⫺ L0)⫺1L0 ⫽ M1(M1 ⫺ M0)⫺1.

σ0 x3 x2 x1

σ0

Figure 4.9

92

INCLUSIONS AND INHOMOGENEITIES

APPENDIX 4A

Consider the integral I⫽

冕 ␦[ˆ 䡠 (x ⫺ )] d,

(4.A.1)

⍀

where the integration doman ⍀ is an ellipsoid deﬁned by (4.3.1). To carry out this integral, we introduce the following substitutions: ⫽

冤 冥

冤 冥

1 /a1 2 /a2 , 3 /a3

x1 /a1 x ⫽ x2 /a2 , x3 /a3

a ˆ 1 1ˆ1 ⫽ a , a 2ˆ2 a33

冤 冥

(4.A.2)

where a ⫽ 兹(a1ˆ 1)2 ⫹ (a2ˆ 2)2 ⫹ (a3ˆ 3)2.

(4.A.3)

Then, the volume integral over the ellipsoid can be converted to a volume integral overa unit sphere: I⫽

冕 ␦[ˆ 䡠 (x ⫺ )] d ⫽ 冕 ⍀

iiⱕ1

␦[a( 䡠 x ⫺ 䡠 )]a1a2a3 d.

(4.A.4) In the case 䡠 x ⬍ 1, the above integral can be written as

冕 再冕 冋冕 ␦( 䡠 x ⫺ z) dr册 dz冎 d aaa ⫽ 冕 再冕 (1 ⫺ z )␦( 䡠 x ⫺ z) dz冎 d 2a aaa ⫽ 冕 [1 ⫺ ( 䡠 x) ] d 2a

I⫽

a1a2a3 a 1 2 3

1 2 3

2

1

兹1⫺z2

0

⫺1

0

2

1

0

⫺1

2

2

2

0

⫽

a1a2a3 [1 ⫺ ( 䡠 x)2]. a

See Figure 4.10. Returning to the original variables, we have

(4.A.5)

APPENDIX 4B

ESHELBY TENSOR FOR ISOTROPIC MATERIALS

93

η

r x

ϕ

z

ξ

Figure 4.10 Domain of integration.

I⫽

a1a2a3 a a a [1 ⫺ ( 䡠 x)2] ⫽ 1 32 3 [a2 ⫺ (ˆ 䡠 x)2]. a a

(4.A.6)

For a point x inside the ellipsoid, the corresponding x is inside a unit sphere, that is, 㛳x㛳 ⬍ 1. Since is a unit vector, we have 䡠 x ⬍ 1 for any point x inside the ellipsoid ⍀. Therefore, the above result is valid for any point x inside the ellipsoid ⍀. APPENDIX 4B ESHELBY TENSOR FOR ISOTROPIC MATERIALS WITH POISSON’S RATIO Ellipsoid (a1 ⬎ a2 ⬎ a3)

S1111 ⫽

3 1 ⫺ 2v a2I ⫹ I, 8 (1 ⫺ v) 1 11 8 (1 ⫺ v) 1

S1122 ⫽

1 1 ⫺ 2v a22I12 ⫺ I, 8 (1 ⫺ v) 8 (1 ⫺ v) 1

S1133 ⫽

1 1 ⫺ 2v a23I13 ⫺ I, 8 (1 ⫺ v) 8 (1 ⫺ v) 1

S1212 ⫽

a21 ⫹ a22 1 ⫺ 2v I12 ⫹ (I ⫹ I2). 16 (1 ⫺ v) 16 (1 ⫺ v) 1

All other nonzero components are obtained by the cyclic permutation of the above equations. The components that cannot be obtained by the cyclic permutation are zero; for instance, S1112 ⫽ S1223 ⫽ S1232 ⫽ 0.

94

INCLUSIONS AND INHOMOGENEITIES

In the above equations, the constants I1, I2, I11, I12, and I13 are given by the following: I1 ⫽ I3 ⫽

4a1a2a3 {F(, k) ⫺ E(, k)}, (a ⫺ a22)(a12 ⫺ a32)1 / 2 2 1

再

冎

4a1a2a3 a2(a21 ⫺ a23)1 / 2 ⫺ E(, k) , (a22 ⫺ a32)(a12 ⫺ a32)1 / 2 a1a3

where the elliptical integrals are deﬁned by F(, k) ⫽ E(, k) ⫽

冕 (1 ⫺ k dwsin w)

2

0

2

,

1/2

冕 (1 ⫺ k sin w)

2

2

1/2

dw,

0

⫽ sin⫺1(1 ⫺ a32 /a12)1 / 2,

k ⫽ {(a12 ⫺ a22)/(a12 ⫺ a32)}1 / 2.

Furthermore I1 ⫹ I2 ⫹ I3 ⫽ 4, 3I11 ⫹ I12 ⫹ I13 ⫽ 4 /a12, 3a21I11 ⫹ a22I12 ⫹ a32I13 ⫽ 3I1, I12 ⫽ (I2 ⫺ I1)/(a21 ⫺ a22). These equations and their cyclic counterparts give sufﬁcient relations to express Ii and Iij in terms of I1 and I3. Sphere (a1 ⫽ a2 ⫽ a3 ⫽ a)

I1 ⫽ I2 ⫽ I3 ⫽ 4 /3, I11 ⫽ I22 ⫽ I33 ⫽ I12 ⫽ I23 ⫽ I31 ⫽ 4 /5a2, S1111 ⫽ S2222 ⫽ S3333 ⫽

7 ⫺ 5v , 15(1 ⫺ v)

APPENDIX 4B

ESHELBY TENSOR FOR ISOTROPIC MATERIALS

S1122 ⫽ S2233 ⫽ S3311 ⫽ S1133 ⫽ S2211 ⫽ S3322 ⫽ S1212 ⫽ S2323 ⫽ S3131 ⫽

95

5v ⫺ 1 , 15(1 ⫺ v)

4 ⫺ 5v . 15(1 ⫺ v)

Elliptic Cylinder (a3 → ⬁)

I1 ⫽ 4a2 /(a1 ⫹ a2),

I2 ⫽ 4a1 /(a1 ⫹ a2), I3 ⫽ 0

I12 ⫽ 4 /(a1 ⫹ a2)2,

3I11 ⫽ 4 /a21 ⫺ I12,

3I22 ⫽ 4 /a22 ⫺ I12,

I13 ⫽ I23 ⫽ I33 ⫽ 0,

a32I13 ⫽ I1, S1111 ⫽ S2222 ⫽

a32I23 ⫽ I2,

a32I33 ⫽ 0.

再

冎

a22 ⫹ 2a1a2 a2 ⫹ (1 ⫺ 2v) , 2 2(1 ⫺ v) (a1 ⫹ a2) a1 ⫹ a2 1

再

冎

a21 ⫹ 2a1a2 a1 ⫹ (1 ⫺ 2v) , 2 2(1 ⫺ v) (a1 ⫹ a2) a1 ⫹ a 2 1

S1122 ⫽

1

再

a22

2(1 ⫺ v) (a1 ⫹ a2)

S2233 ⫽

2

1

2va1 , 2(1 ⫺ v) a1 ⫹ a2 S1133 ⫽

S2211 ⫽

1

再

S2323 ⫽

S1212 ⫽ a1

a2 a1 ⫹ a 2

冎

,

冎

,

S3311 ⫽ 0,

1

2va2 , 2(1 ⫺ v) a1 ⫹ a2 a12

2(1 ⫺ v) (a1 ⫹ a2)

S3322 ⫽ 0,

⫺ (1 ⫺ 2v)

S3333 ⫽ 0,

2

⫺ (1 ⫺ 2v)

a1 a1 ⫹ a 2

再

冎

a12 ⫹ a22 1 ⫺ 2v ⫹ , 2(1 ⫺ v) 2(a1 ⫹ a2)2 2 1

, 2(a1 ⫹ a2)

S3131 ⫽

a2

. 2(a1 ⫹ a2)

96

INCLUSIONS AND INHOMOGENEITIES

Penny Shape (a1 ⫽ a2 ⬎⬎ a3)

I1 ⫽ I2 ⫽ 2a3 /a1,

I3 ⫽ 4 ⫺ 2 2a3 /a1,

I12 ⫽ I21 ⫽ 3 2a3 /4a31, I13 ⫽ I23 ⫽ I31 ⫽ I32 ⫽ 3(–34 ⫺ 2a3 /a1)/a12, I11 ⫽ I22 ⫽ 3 2a3 /4a31, S1111 ⫽ S2222 ⫽

13 ⫺ 8v a 3, 32(1 ⫺ v) a1

S1122 ⫽ S2211 ⫽

7 ⫺ 8v a 3, 32(1 ⫺ v) a1

Skk11 ⫽ Skk22 ⫽

S3333 ⫽ 1 ⫺

8v ⫺ 1 a 3, 32(1 ⫺ v) a1

S3311 ⫽ S3322 ⫽ S1212 ⫽

I33 ⫽ –34 /a32;

v 1⫺v

S2233 ⫽

冉

1⫺

2v ⫺ 1 a 3, 8(1 ⫺ v) a1

冊

4v ⫹ 1 a3 , 8v a1

S1313 ⫽ S2323 ⫽

1 ⫺ 2v a3 v ⫹ , 1 ⫺ v 4 a1 1 ⫺ v

1 ⫺ 2v a3 , 1 ⫺ v 4 a1

冉

冊

1 v ⫺ 2 a3 1⫹ , 2 1 ⫺ v 4 a1

Skk33 ⫽ 1 ⫺

1 ⫺ 2v a3 . 1 ⫺ v 2 a1

When a3 ⫽ 0, I1 ⫽ I2 ⫽ 0, I3 ⫽ 4, I12 ⫽ 0,

I23 ⫽ 4 /a22,

I11 ⫽ I22 ⫽ 0,

I31 ⫽ 4 /a12,

a23I33 ⫽ 4 /3,

S2323 ⫽ S3131 ⫽ –12 , S3311 ⫽ S3322 ⫽ v /(1 ⫺ v), S3333 ⫽ 1,

and all other Sijkl ⫽ 0.

APPENDIX 4B

ESHELBY TENSOR FOR ISOTROPIC MATERIALS

97

Flat Ellipsoid (a1 ⬎ a2 ⬎⬎ a3)

I1 ⫽ 4a2a3{F(k) ⫺ E(k)}/(a21 ⫺ a22), I2 ⫽ 4a3E(k)/a2 ⫺ 4a2a3{F(k) ⫺ E(k)}/(a21 ⫺ a22), I3 ⫽ 4 ⫺ 4a3E(k)/a2, I12 ⫽ [4a3E(k)/a2 ⫺ 8a2a3{F(k) ⫺ E(k)}/(a12 ⫺ a22)]/(a12 ⫺ a22), I23 ⫽ [4 ⫺ 8a3E(k)/a2 ⫹ 4a2a3{F(k) ⫺ E(k)}/(a21 ⫺ a22)]/a22, I31 ⫽ [4 ⫺ 4a2a3{F(k) ⫺ E(k)}/(a12 ⫺ a22) ⫺ 4a3E(k)/a2]/a21, I33 ⫽ 4 /3a23, where F(k) and E(k) are the complete elliptic integrals of the ﬁrst and the second kind, respectively, E(k) ⫽

冕

(1 ⫺ k2 sin2 )1/ 2 d,

F(k) ⫽

冕

(1 ⫺ k2 sin2 )⫺1 / 2 d,

/2

0

/2

0

k2 ⫽ (a12 ⫺ a22)/a12. Oblate Spheroid (a1 ⫽ a2 ⬎ a3)

再

冉 冊冎

2a2a a a a2 I1 ⫽ I2 ⫽ 2 1 233 / 2 cos⫺1 3 ⫺ 3 1 ⫺ 23 (a1 ⫺ a3) a1 a1 a1

1/2

,

I3 ⫽ 4 ⫺ 2I1, I11 ⫽ I22 ⫽ I12, I12 ⫽ /a12 ⫺ –41 I13 ⫽ /a21 ⫺ I13 ⫽ I23 ⫽ (I1 ⫺ I3)/(a32 ⫺ a12),

I1 ⫺ I3 , 4(a23 ⫺ a21)

3I33 ⫽ 4 /a32 ⫺ 2I13.

98

INCLUSIONS AND INHOMOGENEITIES

Prolate Spheroid (a1 ⬎ a2 ⫽ a3)

I2 ⫽ I3 ⫽

再 冉 冊

2a1a32 a1 a12 ⫺1 (a12 ⫺ a32)3 / 2 a3 a32

I1 ⫽ 4 ⫺ 2I2,

1/2

⫺ cosh⫺1

冎

a1 , a3

I12 ⫽ (I2 ⫺ I1)/(a21 ⫺ a22),

3I11 ⫽ 4 /a21 ⫺ 2I12, I22 ⫽ I33 ⫽ I23,

3I22 ⫽ 4 /a22 ⫺ I23 ⫺ (I2 ⫺ I1)/(a12 ⫺ a22),

I23 ⫽ /a22 ⫺ (I2 ⫺ I1)/4(a12 ⫺ a22). SUGGESTED READING Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston, Chapters 3–4. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York, Chapter 7.

5 DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS Most engineering materials are heterogeneous in nature. They generally consist of different constituents or phases, which are distinguishable at speciﬁc scales. Each constituent may show different physical properties (e.g., elastic moduli, thermal expansion, yield strength, electrical conductivity, thermal conductivity, etc.) and/or material orientations. However, in many engineering applications, a structure component may contain numerous such constituents such that it is impractical or even impossible to account for each and every one of them for engineering design and analysis. What is really relevant is the overall or effective property of the material from which the component is made. In this chapter, we will lay out the basic deﬁnitions of overall or effective properties of engineering materials that are heterogeneous at the length scale of interest. Generally speaking, heterogeneous materials can be classiﬁed into two categories, periodic and nonperiodic. In this text, we will focus primarily on heterogeneous materials with nonperiodic microstructures. So, unless indicated otherwise, the term heterogeneous material refers to heterogeneous materials with nonperiodic microstructures. Examples of such materials may include most of the ﬁber or particulate reinforced composites and polycrystalline materials. 5.1 HETEROGENEITY AND LENGTH SCALES

Generally speaking, engineering materials are heterogeneous, that is, they have microstructure and they contain heterogeneities. However, Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

99

100

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

what constitutes a heterogeneity depends on the length scales used in the observation. Certain constituents or phases in a given material are identiﬁable only at or below a speciﬁc length scale. At such a length scale, each constituent may be homogeneous, but when observed at a smaller length scale, the constituent itself may become heterogeneous. A polycrystal copper, for example, may seem to be homogeneous with the naked eye (⬃10 m). But, under optical microscope (⬃1 m), the polycrystal copper is composed of many grains—small single copper crystals with different orientations. At this length scale, although each grain can be treated as a homogeneous material, the polycrystal copper as an assembly of grains cannot be treated as a homogeneous material any more because the microstructure attributes, such as grain size, orientation, and grain boundaries, dictate how the material behaves at this length. When we go down further along the length scales, we know that each grain also has its own microstructure. The behavior and properties of materials at each length scale are controlled by the observable microstructure at the corresponding length scale. Therefore, whether a material is heterogeneous or not depends on the length scale used in the observation. In other words, when studying the properties of a real material, which is always heterogeneous, we need to deﬁne the length scale at which the properties of interest are directly relevant. Microstructure features not observable at this length can be neglected. In fact, for practical purposes, it is only certain averaged effects of the microstructure that are of interest. So, in the study of heterogeneous materials, we often speak of overall properties. By that we mean the properties averaged over a certain volume of the heterogeneous material. For such overall properties to be meaningful, the average taken over any arbitrary volume element comparable with the relevant length scale must be the same with the heterogeneous material sample under consideration. Heterogeneous materials that meet this requirement are said to be macroscopically homogeneous. We will give a more quantitative deﬁnition of macroscopic homogeneity later in this chapter. For now, let us consider, for example, a ﬁber-reinforced composite laminate. It is certainly impractical and unnecessary to deal with each individual ﬁber when the overall bending rigidity of the laminate is of primary interest. On the other hand, the bending rigidity of the laminate is very closely related to the lay up of the various layers within the laminate. To derive the overall rigidity of the composite, the laminate must be treated as a stack of plies each being different in composition and/or orientation, albeit each ply can be treated as a homogeneous layer.

5.1

HETEROGENEITY AND LENGTH SCALES

101

In the examples given above, we have implicitly implied that there is a separation of length scales D and d on which the macroscopic properties (e.g., bending rigidity of the composite laminate) and microscopic properties (elasticity of the plies) are deﬁned, respectively. The microscale length d corresponds to the smallest constituent whose physical properties, orientation, and shape are judged to have direct ﬁrst-order effects on the macroscopic overall physical properties of the heterogeneous material at the length scale D. The choice of d is generally adapted to the problem under consideration. An appropriate choice should be guided by systematic ‘‘multiscale’’ experimental observations. Generally speaking, an optimum choice would be the one that includes a good balance between the deﬁnitions of the microscale that have a ﬁrst-order effect on the overall properties, and the simplicity of the resulting model. The macroscale length D should be large enough so that the microscale ﬂuctuations (perturbations) of the stress and strain ﬁelds due to the local variation of microstructure at the scale d inﬂuence the overall effective property only through their averages. In fact, in the framework of micromechanics, the stress and strain ﬁelds are split into contributions corresponding to different length scales. It is assumed that these length scales are sufﬁciently different in terms of their order of magnitude, so that for each pair of them, the ﬂuctuations of stress and strain ﬁelds (micro or local quantities) at the smaller length scale inﬂuence the overall (or macroscopic) behavior at the larger length scale only through their averages, and, conversely, ﬂuctuations of stress and strain ﬁelds as well as the compositional gradients (macro or global quantities) are not signiﬁcant at the smaller length scale. Therefore, at this scale, these macroﬁelds are locally uniform and can be described as uniformly applied stresses and strains. To meet these conditions, the typical dimension of the microscale constituents should be orders of magnitude smaller than the macroscale element so that, d/D ⬍⬍ 1. In the composite laminate example mentioned above, if the thickness of each single ply is on the order of d ⬃ 0.1 mm, the thickness of the laminate should be at least on the order of D ⬃ 1 mm so that the macroscopic effective bending rigidity can be deﬁned meaningfully. Note that the identiﬁcation of d and D is dependent of the length scale of interest. In the above example, since our interest is in the overall bending rigidity of the laminate, we have taken the overall thickness of the laminate to be our macroscopic length parameter and the thickness of each ply to be our microscopic parameter. This way, it implies that each ply is a homogeneous material with no micro-

102

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

structure. However, if we are interested in the behavior of each individual ply, that is, our interest is in the length scale of the ply thickness, we must then identify the ply thickness as our macroscopic length parameter. In this case, the microscopic length parameter d would be the diameter of the individual ﬁbers within the ply. Each ply as a whole can no longer be viewed as a homogeneous material. Instead, it becomes a composite consisting of polymer resin and the ﬁbers. Each constituent can be considered a homogeneous material.

5.2 REPRESENTATIVE VOLUME ELEMENT

In light of the above discussions, we introduce the concept of microhomogeneity. The microstructure of heterogeneous materials is, at any given length scale, very complex, and, to a certain extent, random. To describe the precise topographic features of the microstructure variation is usually impractical and very often impossible. In fact, for practical purposes, it is only certain averaged effects of the microstructure that are of interest. So, in the study of heterogeneous materials, we often speak of overall properties. By that we mean the properties averaged over a certain volume of the heterogeneous material. For such overall properties to be meaningful, the average taken over any arbitrary volume element comparable with the relevant length scale must be the same with the heterogeneous material sample under consideration. Heterogeneous materials that meet this requirement are said to be macroscopically heterogeneous. In light of the discussions in the preceding paragraph, if in a heterogeneous material the microscopic length parameter d and the macroscopic length parameter D can be identiﬁed for a length scale of interest such that d/D ⬍⬍ 1, then the heterogeneous material is microscopically homogeneous at the length scale D. A volume element with characteristic dimension of D is called a representative volume element (RVE) because the overall properties on any RVE would be the same. In other words, the overall properties of each RVE represent the overall properties of the heterogeneous material.

5.3 RANDOM MEDIA

The foregoing discussions assumed that the microstructure of the heterogeneous material is known. In reality, the microstructures of engi-

5.3

RANDOM MEDIA

103

neering materials are very complex and very often random in nature. It is impractical and even impossible to have knowledge on every detail of the microstructure conﬁguration at any given length scale, except in cases such as those displaying periodicity. Typically, only certain ‘‘average’’ features of the microstructure will be known, and such information is likely to be statistical in character. In this section, we will discuss how such statistical information can be incorporated in the deﬁnition of RVE. Consider a batch of particulate-reinforced composite blocks made under the same processing conditions. Let R denote the batch and N be the total number of blocks in R. Assume that all the blocks are the same size D, which is much larger than the particle diameter d, and the particle content (e.g., volume fraction) c is the same for all blocks. However, due to manufacture variability, the distribution of the particles in each block is inevitably different one from the other. Consequently, if we choose a small volume at the same location x on each block, the particle content c(x, ␣) in this small volume may not be the same among all the blocks, and thus, the average 具c(x)典 ⫽

1 N

冘 c(x, ␣), N

␣⫽1

(5.3.1)

may depend on N. However, it is conceivable that if N is very large, the average value computed from (5.3.1) would become relatively independent of N. In the limit of N → ⬁, the summation can be replaced by an integral over the sample space R, and the average becomes independent of N: 具c(x)典 ⫽ lim N→⬁

1 N

冘 c(x, ␣) ⫽ 冕 c(x, ␣) d␣. N

␣⫽1

(5.3.2)

R

Such an averaging scheme is called the ensemble average. Now, let us consider a different average by picking out a block randomly from the batch; call it the ␣th block. First we divide this block into M subdomains of volume Vi, where 兺M i⫽1 Vi ⫽ V with V being the total volume of the block. Then, we calculate the particle volume fraction c(x, ␣) on each of the subdomains, where xi is the coordinate of a representative point, for example, the centroid of Vi. Again, due to manufacture variability, the particle volume fraction on each of the subdomains may not be the same among all the subdomains, and, thus, the average

104

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

c(␣) ⫽

1 V

冘 c(x )V M

i

(5.3.3)

i

i⫽1

may depend on M. However, it is conceivable that if M is very large, the average value computed from (5.3.3) would become relatively independent of M. In the limit of M → ⬁, the summation can be replaced by an integral over the entire volume V and the average becomes independent of M: c(␣) ⫽ lim M→⬁

1 V

冘 c(x )V ⫽ V1 冕 c(x) dv. M

i

i

i⫽1

(5.3.4)

V

We will call this average scheme the volume (or spatial) average. Note that the ensemble average is carried out over a group of blocks made under the same process, while the volume average is performed over an individual block out of the group. The nature of manufacture variability is such that the local particle volume fraction c(x, ␣) at x can be viewed as a random function of the sample ␣, as well as a random function of the position x; each represents a different random process. The ensemble average gives the mean value among all the samples in the sample space, while the volume average tells us the mean value over a particular sample. Imagine that the particle distribution in each and every block were exactly the same; it is plausible that the two average schemes should give the same value, that is, 具c(x)典 ⫽ c(␣),

(5.3.5)

冕 c(x, ␣) d␣ ⫽ V1 冕 c(x, ␣) dV(x).

(5.3.6)

or

R

V

This statement, that is, ensemble average equals volume average, is known as the ergodic hypothesis, a concept used frequently in stochastic analysis, where time average is used in lieu of the volume average deﬁned in (5.3.4). Let us now generalize the ergodic hypothesis to the description of microstructure features in heterogeneous materials. Consider, generally, a group of heterogeneous materials. Let us name the group R and each member of the group will be characterized by the label ␣. The value of ␣ is taken as deﬁning the member (one of the materials in the group)

5.3

RANDOM MEDIA

105

completely. Further, assume that, associated with ␣, there is a probability distribution function p(␣) deﬁned over R, which satisﬁes

冕 p(␣) d␣ ⫽ 1.

(5.3.7)

R

Next, assume that each member of the group has a total volume V and consists of N different types of inhomogeneities or phases. The r th phase in sample ␣ is assumed to occupy the volume Vr(␣), r ⫽1, 2, 3, . . . , N. To describe the material’s microstructure or the spatial distribution of inhomogeneities, it is convenient to introduce the characteristic function that takes the value of 1 if x lies within the volume Vr(␣) and zero otherwise, that is, ƒr(x, ␣) ⫽

再

1 0

x 僆 Vr(␣) . x ⰻ Vr(␣)

(5.3.8)

Clearly, the characteristic function ƒr(x, ␣) satisﬁes the following consistency condition:

冘 ƒ (x, ␣) ⫽ 1. N

(5.3.9)

r

r⫽1

Thus, the ensemble average of ƒr(x, ␣) deﬁnes the probability Pr(x) of ﬁnding phase r at location x: Pr(x) ⫽ 具ƒr(x, ␣)典 ⬅

冕 ƒ (x, ␣)p(␣) d␣. r

(5.3.10)

R

The function Pr(x) is also referred to as the one-point correlation function for the characteristic function ƒr(x, ␣). Likewise, the probability Prs(x, x⬘) of ﬁnding simultaneously phase r at x and phase s at x⬘ is Prs(x, x⬘) ⫽ 具ƒr(x, ␣)ƒs(x⬘, ␣)典 ⬅

冕 ƒ (x, ␣)ƒ (x⬘, ␣)p(␣) d␣. V

r

s

(5.3.11)

The function Prs(x, x⬘) is also referred to as the two-point correlation function for the characteristic function ƒr(x, ␣). Following this approach, probabilities involving, for example, k points, or k-point correlation function, can be deﬁned similarly.

106

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

Let us now develop an understanding of the geometrical interpretations of the correlation functions. Consider an epoxy matrix containing spherical silica particles, a two-phase composite used commonly in the electronics industry. If we take a large group of the material samples, each has the same particle content and a volume V large enough to contain many particles, we can, in principle, compute the one-point correlations Pr(x) (r ⫽ 1, 2) by knowing the distribution density p(␣) and the characteristic function ƒr(x, ␣). Let r ⫽ 1 be the matrix phase and r ⫽ 2 be the particle phase. If we found that P2(x) is a constant (i.e., independent of x), then we can say that the particles are uniformly distributed through each sample. This is because P2(x) ⫽ const. means that the chance of ﬁnding a particle is the same everywhere in V. Note that this does not necessarily mean that the particles are everywhere in V. It just gives us a sense of how ‘‘uniformly’’ the particles are distributed. Next, we take x to be the center of a particle and x⬘ to be the center of another particle, and compute P22(x, x⬘). Let us assume that it satisﬁes P22(x, x⬘) ⫽ P22(x ⫺ x⬘), that is, the two-point correlation function P22(x, x⬘) depends only on the distance between the two points, regardless where these two points are located. What that means is that if one takes a measuring stick shorter than the smallest dimension of V, and places the stick inside V, the chance that there is a particle at each end of the stick is the same regardless of where the stick is placed. The other two-point correlation functions P11(x, x⬘), P12(x, x⬘), and P21(x, x⬘) can be interpreted similarly. Clearly the twopoint correlation functions give us another measure of the ‘‘uniformity’’ of the heterogeneous materials. Said differently, if a material is statistically uniform, then its correlation functions Pr(x), Prs(x, x⬘), and so forth are insensitive to translation, that is, Pr(x) reduces to a constant, Prs(x, x⬘) becomes a function of (x ⫺ x⬘) only, and so on. More generally, in micromechanics, a heterogeneous medium is called statistically homogeneous (or uniform) of grade k if the correlation functions up to the k point are all translation invariant. Since it is very unlikely that enough information is available to computer the k-point correlation function for k greater than 2, in this book we will typically call a statistically homogenous of grade 2 simply statistically homogeneous. In what follows, we show that if the characteristic function of a heterogeneous material satisﬁes the ergodic hypothesis, the material is statistically homogeneous. To this end, consider the volume average of the characteristic function ƒr(x, ␣) for sample ␣:

5.3

ƒr(x, ␣) ⫽

1 V

RANDOM MEDIA

冕 ƒ (x, ␣) dV(x) ⫽ VV ⬅ c , r

V

r

r

107

(5.3.12)

where cr is the volume fraction of the rth phase in the heterogeneous material. The ergodic hypothesis thus means Pr(x) ⫽ 具ƒr(x, ␣)典 ⬅ ƒr(x, ␣) ⫽ cr .

(5.3.13)

Next, consider the volume average of the two-point correlation: ƒr(x, ␣)ƒs(x⬘, ␣) ⫽

1 V

冕 ƒ (x, ␣)ƒ (x⬘, ␣) dV(x). r

V

s

(5.3.14)

Let xⴖ ⫽ x ⫺ x⬘.

(5.3.15)

Then, we have 1 V

冕 ƒ (x, ␣)ƒ (x⬘, ␣) dV(x) ⫽ V1 冕 V

r

s

Vr

ƒs(x ⫺ xⴖ, ␣) dV(x) ⫽ grs(xⴖ), (5.3.16)

or ƒr(x, ␣)ƒs(x⬘, ␣) ⫽ grs(xⴖ) ⫽ grs(x ⫺ x⬘).

(5.3.17)

Therefore, according to the ergodic hypothesis, Prs(x, x⬘) ⫽ 具ƒr(x, ␣)ƒs(x⬘, ␣)典 ⫽ ƒr(x, ␣)ƒs(x⬘, ␣) ⫽ grs(x ⫺ x⬘). This completes the proof. We can summarize the foregoing discussions as follows: 1. The microstructure or the distribution of heterogeneities in a heterogeneous material can be characterized quantitatively by the correlation functions Pr(x), Prs(x, x⬘), and so forth, which are the ensemble average of the characteristic function ƒr(x, ␣).

108

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

2. The heterogeneous material is considered statistically homogeneous if the correlation functions are translation invariant, that is, Pr(x) ⫽ cr, Prs(x, x⬘) ⫽ grs(x ⫺ x⬘), and so forth. 3. If the correlation functions are ergodic, that is, the ensemble average equals the volume average, then they are translation invariant. Therefore, if the correlation functions of a heterogeneous material are ergodic, the material is considered statistically homogeneous. Having considered the random media and introduced the concepts of ergodicity and statistical homogeneity, we can now give the representative volume element (RVE) a more precise deﬁnition. To deﬁne the length scale corresponding to the properties of interest, we need to select an RVE of the heterogeneous material in question. The size of the RVE must be such that it includes a very large number of inhomogeneities and in the meanwhile be statistically homogeneous and representative of the local continuum properties, so that appropriate averaging schemes over these domains give rise to the same mechanical properties, corresponding to the overall or effective mechanical properties. Finally, to close this section, we mention that in the rest of this book, we will be mainly concerned with the statistically homogeneous media. Therefore, it will be assumed implicitly, unless indicted otherwise, that the ensemble average and the volume average are the same, that is, 具h(x)典 ⫽

冕 h(x, ␣) d␣ ⫽ V1 冕 h(x, ␣) dV(x) ⫽ h(␣),

(5.3.18)

V

R

where h(x, ␣) can be either a scalar or a tensor function. 5.4 MACROSCOPIC AVERAGES

In this section, attention is focused on developing averaging theorems devoted to heterogeneous materials with arbitrary constituents independent of their thermomechanical behavior. The average stresses over a domain D is deﬁned as ij ⫽

1 D

冕 D

ij

dV,

or ⫽

1 D

冕 dV. D

Similarly, the average strain over in a domain D is deﬁned as

(5.4.1)

5.4

ij ⫽

1 D

冕 D

ij

dV,

109

MACROSCOPIC AVERAGES

or ⫽

冕 dV.

1 D

(5.4.2)

D

In these deﬁnitions, the domain D does not need to be homogeneous, nor does it need to be a single domain. Note that, as mentioned earlier, the volume average and ensemble average are the same for statistically homogeneous materials. Average-Stress Theorem Let 0ij be a given constant stress tensor and S be the entire boundary of a domain D with outward normal nj. If ij nj兩S ⫽ pj0 ⫽ ij0 nj

(5.4.3)

is prescribed on S, then the average stress on D is given by ij ⫽ ij0 .

(5.4.4)

To prove this theorem, consider the deﬁnition of average stress: ij ⫽

冕

1 D

ij

D

dV ⫽

1 D

冕 ␦

dV.

ik jk

D

(5.4.5)

Note that xj,k ⫽ ␦jk, so ij ⫽

1 D

冕x

dV ⫽

ik j,k

D

1 D

冕 [( x )

ik j ,k

D

⫺ ik,k] dV.

(5.4.6)

When there is no body force as assumed here, the second term in the above integral vanishes. Making use of the divergence theorem and then the traction boundary condition (5.4.3), we have ij ⫽

1 D

冕 x n dS ⫽ D1 冕 x n dS. S

ik j

k

0 ik

S

j

k

(5.4.7)

Making use of the divergence theorem again leads to ij ⫽ ik0

1 D

冕x D

j,k

dV ⫽ ik0

1 D

冕␦ D

jk

dV ⫽ ij0.

This completes the proof of the average stress theorem.

(5.4.8)

110

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

What the average stress theorem tells us is that when a body is subjected to the traction boundary condition (5.4.3) with 0ij being a constant stress tensor, the stress averaged over the entire body is the same as 0ij, regardless the complexity of the stress ﬁeld within the domain. Therefore, in the rest of this book, traction boundary conditions will be written as ij nj兩S ⫽ ij nj,

(5.4.9)

with the understanding that ij is the average stress tensor in the body enclosed by S when (5.4.9) is applied. Average-Strain Theorem Let 0ij be a given constant strain tensor and S be the entire boundary of a domain D with outward normal nj. If ui兩S ⫽ ij0 xj

(5.4.10)

is given on S, then the average strain on D is given by ij ⫽ ij0 .

(5.4.11)

To prove this theorem, consider the deﬁnition of average strain:

冕 dV ⫽ 2D1 冕 (u ⫹ u ) dV 1 ⫽ 冕 u dV ⫹ 2D1 冕 u dV. 2D

ij ⫽

1 D

ij

D

D

i, j

D

i, j

D

j,i

j,i

(5.4.12)

Making use of the divergence theorem yields ij ⫽

1 2D

冕 u n dS ⫹ 2D1 冕 u n dS. S

i j

S

j

i

(5.4.13)

Substitute the boundary condition (5.4.10) into the above integrals:

5.5

ij ⫽

1 2D

111

HILL’S LEMMA

冕 x n dS ⫹ 2D1 冕 x n dS. S

0 ik k j

S

0 jk k i

Making use of the divergence theorem again, ij ⫽

1 2D

冕x D

0 ik k, j

dV ⫹

1 2D

冕x

0 jk k,i

D

dV ⫽

1 0 ( ⫹ ji0) ⫽ ij0. 2 ij (5.4.14)

This completes the proof of the average strain theorem. According to average strain theorem, if the displacements along the entire boundary of a given body is prescribed by (5.4.10) with 0ij being a constant strain tensor, then the strain ﬁeld averaged over the entire body is 0ij, regardless the complexity of strain ﬁeld within the body. Thus, in the rest of this book, displacement boundary conditions will be written as ui兩S ⫽ ij xj,

(5.4.15)

with the understanding that ij is the average strain tensor in the body enclosed by S when (5.4.15) is applied. 5.5

HILL’S LEMMA

Again, consider an RVE with volume V and boundary S. For any stress and strain ﬁelds ij and ij at a given point in the RVE under prescribed boundary traction or boundary displacement condition, one has the following result: ijij ⫺ ijij ⫽

1 D

冕 (u ⫺ x )( n ⫺ n ) dS, S

i

j ij

ik k

ik k

(5.5.1)

where the overbar stands for the volume average; for example, ijij ⫽

1 V

冕 V

ij ij

dv.

(5.5.2)

To prove Hill’s lemma, let us ﬁrst expand the integrand of the surface integral on the right-hand side of (5.5.1):

112

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

冕 (u ⫺ x )( n ⫺ n ) dS ⫽ 冕 (u n ⫺ u n ⫺ n x i

S

j ij

i

S

ik k

ik k

ik k

i k

ik

ik k j ij

⫹ xj nkijik) dS.

(5.5.3)

The following surface integrals can be easily evaluated:

冕 u n dS ⫽ 冕 u S

i

ik k

V

冕 un i k

S

ik

i, j

ij

冕

dV ⫽

dS ⫽ ik

V

冕u

i,k

V

ik k j

ik ik

V

冕 x n dS ⫽ 冕 ␦ S

j

k

V

jk

ij

dV ⫽ Dijij,

dV ⫽ Dikik,

冕 n x dS ⫽ 冕 ␦ S

ij

dV ⫽ Dij,

dV ⫽ D␦jk.

Substituting the above into (5.5.3) yields 1 D

冕 (u ⫺ x )( n ⫺ n ) dS ⫽ S

i

j ij

ik k

ik k

ij ij

⫺ ikik ⫺ ijij ⫹ ikik

⫽ ijij ⫺ ijij.

(5.5.4)

This proves Hill’s lemma (5.5.1). A corollary of Hill’s lemma can be stated as follows: ijij ⫽ ijij,

(5.5.5)

if ijnj兩S ⫽ ij nj, or ui兩S ⫽ ij xj. In other words, for statically admissible stress ﬁelds (ijnj兩S ⫽ ij nj), or kinematically admissible displacement ﬁelds (ui兩S ⫽ ij xj), the volume average of the product ijij is the same as the product of the volume averages ij and ij. Equation (5.5.5) is also known as Hill’s macrohomogeneity condition or Mandel–Hill condition. Note that ijij is twice the value of strain energy density, (5.5.5) implies that the volume-averaged strain energy density of a heterogeneous material can be obtained from the volume averages of the stresses and strains. Accordingly, homogenization can be interpreted as ﬁnding a homogeneous comparison material that is energetically equiv-

5.6

DEFINITIONS OF EFFECTIVE MODULUS OF HETEROGENEOUS MEDIA

113

alent to a given microstructured material. This idea will be used to deﬁne the effective properties of heterogeneous media next. 5.6 DEFINITIONS OF EFFECTIVE MODULUS OF HETEROGENEOUS MEDIA

In this section, we introduce the concept of effective modulus of a statistically homogeneous heterogeneous medium. It is assumed that such a medium can be represented by an RVE consisting of N distinct phases dispersed throughout the RVE as inhomogeneities (or heterogeneities) of dimension much less than the size of the RVE. For the moment, perfect bonding will be assumed across the interfaces between the different phases. Nonperfect interfaces will be considered in Chapter 10. Some common engineering materials are special cases of the heterogeneous material described in the preceding paragraph. For example, a polycrystalline material can be viewed as a heterogeneous material with inﬁnite (N ⫽ ⬁) number of distinct phases. Fiber- (particulate-) reinforced composites contain two distinct phases (N ⫽ 2), namely ﬁbers (particles) and the matrix. Heterogeneous materials with a distinct matrix phase are called composite materials. For convenience, body force is not considered in the remaining part of the book unless indicated otherwise. Consider a heterogeneous material D bounded by surface S. Assume that the heterogeneous material consists of randomly oriented and shaped inhomogeneities embedded in a matrix with stiffness tensor L0. Let the stiffness tenors of the inhomogeneities be L1, L2, L3, . . . , LN, as shown in Figure 5.1.

L( N ) L(2) L( r ) L(1)

L(0) Figure 5.1 Multiphase heterogeneous material.

114

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

A straightforward deﬁnition of the effective modulus (stiffness) tensor of the heterogeneous material is given by the following relationship: ⫽ L,

(5.6.1)

where and are, respectively, the average stress and strain tensors, and the fourth tensor L deﬁned by (5.6.1) is call the effective modulus or effective stiffness tensor of the heterogeneous material. Similarly, the effective compliance tensor of the heterogeneous material is deﬁned by ⫽ M,

(5.6.2)

where the fourth-order tensor M is called the effective compliance tensor of the heterogeneous material. Obviously, it follows from the definitions that LM ⫽ ML ⫽ I,

or L⫺1 ⫽ M.

(5.6.3)

Although such deﬁnitions stated above are straightforward, they are not very convenient to use. An alternative deﬁnition of the effective modulus tensor can be given based on the strain energy concept. To this end, let us consider two materials of the same geometry. One is a heterogeneous material, the other is a homogeneous one with stiffness tensor L, as shown in Figure 5.2. First, assume displacements are prescribed on the boundary of both materials, namely

L( N ) L(2) L

L( r )

L(1) L(0) (a)

(b)

Figure 5.2 (a) Heterogeneous material and (b) its comparison material.

5.6

DEFINITIONS OF EFFECTIVE MODULUS OF HETEROGENEOUS MEDIA

ui兩S ⫽ ij xj,

115

(5.6.4)

where ij, as discussed in the previous section, would be the average strain in both materials. The stiffness tensor L of the homogeneous material is said to be the effective stiffness tensor of the heterogeneous material shown in Figure 5.2(a) if and only if Uc ⫽ Uh,

(5.6.5)

where Uc and Uh are the strain energy stored in the heterogeneous material and in the homogeneous material, respectively. It can be easily shown that the two deﬁnitions of the stiffness tenor given above are equivalent. To this end, we calculate ﬁrst the strain energy stored in the composite: Uc ⫽

1 2

冕 D

ij ij

dv ⫽ Dijij.

(5.6.6)

Making use of (5.6.4) in conjunction with Hill’s lemma (5.5.5), we arrive at Uc ⫽

D . 2 ij ij

(5.6.7)

Uc ⫽

D . 2

(5.6.8)

In matrix notation, we have

For the homogeneous material, it is obvious the strain and stress ﬁelds are uniform when (5.6.4) is applied. They are ij ⫽ ij and ij ⫽ Lijklkl. So, the total strain energy of the homogeneous material is given by Uh ⫽ or in matrix notation

D D ⫽ ij Lijklkl, 2 ij ij 2

(5.6.9)

116

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

Uh ⫽

D L. 2

(5.6.10)

Comparing (5.6.8) with (5.6.10), we conclude that Uc ⫽ Uh for any arbitrary , if and only if ⫽ L. Consequently, we have proved that the two foregoing deﬁnitions of stiffness tenors for heterogeneous materials are equivalent. An alternative deﬁnition of the effective compliance tensor also can be given based on the strain energy concept. For example, consider the two materials shown in Figure 5.2. Assume that the homogeneous material has a compliance tensor M. This time let the traction ijnj兩S ⫽ ij nj be prescribed on the entire boundary of both materials. Then, the compliance tensor M is said to be the effective compliance tensor of the composite shown in Figure 5.2(a) if and only if Uc ⫽ Uh,

(5.6.11)

where again Uc and Uh are the strain energy stored in the composite and in the homogeneous material, respectively. Proof of the equivalency between this deﬁnition and the one given by (5.6.2) is straightforward; see Problem 5.1. Although the deﬁnition based on strain energy does not seem as straightforwards as the direct deﬁnition, it is nevertheless convenient for the determination of the effective properties, as will be seen in later chapters.

5.7 CONCENTRATION TENSORS AND EFFECTIVE PROPERTIES

Consider the composite material shown in Figure 5.2(a). Let the displacement boundary condition be given by ui兩S ⫽ ij xj.

(5.7.1)

Then, it follows from (5.4.11) that

冘 c , N

⫽

r r

r⫽0

(5.7.2)

5.7

CONCENTRATION TENSORS AND EFFECTIVE PROPERTIES

117

where r is the average strain on the rth inhomogeneity and cr is the volume fraction of the rth inhomogeneity. The case of r ⫽ 0 is for the matrix. Note that is the average strain of the entire composite material and r is the average strain of the rth inhomogeneity. Thus, a ‘‘strain concentration tensor’’ Ar (r ⬎ 0) can be deﬁned for the rth inhomogeneity through r ⫽ Ar.

(5.7.3)

Clearly, the ‘‘magnitude’’ of Ar represents the strain concentration on the inhomogeneity. Substituting (5.7.3) into (5.7.2) yields

冘 N

c00 ⫽ ⫺

冘 c A . N

crr ⫽ ⫺

r

r

(5.7.4)

r⫽1

r⫽1

Next, consider the average stress in the composite

冘 c ⫽ c L ⫹ 冘 c L , N

⫽

N

r

r

0

0 0

r

r

r

(5.7.5)

r⫽1

r⫽0

where r is the average stress tensor in the rth inhomogeneity, and Hooke’s law r ⫽ Lrr for each inhomogeneity has been used. Making use of (5.7.4) in (5.7.5) gives the following: ⫽

冤

L0 ⫹

冘 c (L ⫺ L )A 册. N

r

r

0

r

(5.7.6)

r⫽1

Comparing (5.7.6) with (5.6.1) leads to

冘 c (L ⫺ L )A . N

L ⫽ L0 ⫹

r

r

0

r

(5.7.7)

r⫽1

In other words, the effective stiffness tensor of a composite material can be expressed in terms of the stiffness tensors of the constituent materials, their corresponding volume fraction and the strain concentration tensors. Among these, the strain concentration tensor is the only unknown in typical engineering applications. Much of the effort in micromechanics has been devoted to ﬁnd ways to compute the con-

118

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

centration tensor. Several of the most commonly used methods to approximate the concentration tensors are discussed in Chapters 7 and 8. Along a parallel path, it can be shown (Problem 5.2) that under the traction boundary condition ijnj兩S ⫽ ij nj, the effective compliance tensor of a composite is given by

冘 c (M ⫺ M )B , N

M ⫽ M0 ⫹

r

r

0

(5.7.8)

r

r⫽1

where Br is the stress concentration tensor for the rth inhomogeneity, that is, r ⫽ Br,

(5.7.9)

where r is the average stress in the rth inhomogeneity and is the average stress over the entire composite. The concentration tensors introduced above represent the stress– strain concentration of the rth inhomogeneity with respect to the average strain over the entire sample. It can be regarded as the global concentration tensors. Since the composite has a distinctive matrix phase in which all the other inhomogeneities are embedded, one can also introduce the local concentration tensors through r ⫽ Gr0

and r ⫽ Hr0

(5.7.10)

where 0 and 0 are, respectively, the average strain and average stress tensor in the matrix phase. Clearly, Gr and Hr are, respectively, the strain and stress concentration tensors of the rth inhomogeneity with respect to the average strain and stress in the matrix immediately surrounding itself. To ﬁnd the relationship between the local and global concentration tensors, consider the average strain:

冘 c ⫽ c ⫹ 冘 c ⫽ c ⫹ 冘 cG ⫽ 冋c I ⫹ 冘 c G 册 . N

N

⫽

r r

0 0

N

r r

r⫽1

r⫽0

0 0

r

r 0

r⫽1

N

0

r

r⫽1

This yields

r

0

(5.7.11)

SUGGESTED READING

0 ⫽

冋

册

冘

⫺1

N

c0I ⫹

119

.

cnGn

n⫽1

(5.7.12)

Substitution of the above equation into (5.7.10) results in

冋

冘cG册

⫺1

N

r ⫽ Gr c0I ⫹

n

.

n

(5.7.13)

n⫽1

Comparing this to the deﬁnition of global concentration tensor (5.7.3) leads to

冋

r⫽1

冋

冘cH册

Ar ⫽ Gr c0I ⫹

冘 cG册

⫺1

N

r

.

r

(5.7.14)

Similarly, one can show that Br ⫽ Hr c0I ⫹

⫺1

N

n

n

.

(5.7.15)

n⫽1

Because of these relationships, the knowledge of the local concentration tensors is sufﬁcient to determine the effective stiffness (compliant) tensor of the composite. PROBLEMS

5.1 Prove the equivalency between the two deﬁnitions of the effective compliance tensor. 5.2 Assume that a composite is subjected to the traction boundary condition ijnj兩S ⫽ ijnj. Show Eq. (5.7.8). 5.3 Derive (5.7.15). SUGGESTED READING Krajinovic, D. (1996). Damage Mechanics, Elsevier, New York, Chapter 1. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston. Nemat-Nasser, S. and Hori, M. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York, Chapter 1. Torquato, S. (2001). Random Heterogeneous Materials: Microstructure and Macroscopic Properties, Springer, New York.

6 BOUNDS FOR EFFECTIVE MODULI Obtaining the effective modulus tensor of a heterogeneous material is often a very difﬁcult task. In most cases, only approximate solutions can be found. Several of these approximate estimates will be discussed in Chapters 7–9. Although exact solutions to the effective moduli may not be found easily, for all practical purposes, knowing the bounds for these moduli is enough. In this chapter, some of these bounds are derived based on variation principles.

6.1 CLASSICAL VARIATIONAL THEOREMS IN LINEAR ELASTICITY

To prepare for the study of bounds of the effective properties of composite materials, we state here, without proof, two of the classical variational theorems in linear elasticity. Minimum Potential Energy Theorem Among all the kinematically admissible displacement ﬁelds, the true solution makes the following potential energy minimum: ⌸[ui] ⫽

1 2

冕L D

u u d ⫺

ijkl k,l i, j

冕

S

p0i ui ds,

(6.1.1)

where D is the total volume, and S is the portion of the boundary of D where traction p0i is prescribed. 120

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

6.1

CLASSICAL VARIATIONAL THEOREMS IN LINEAR ELASTICITY

121

Minimum Complementary Energy Theorem Among all the statically admissible stress ﬁelds, the true solution makes the following complementary energy minimum: ⌸c[ij] ⫽

1 2

冕M D

冕

klij d ⫺

ijkl

Su

ui0ij nj ds,

(6.1.2)

where D is the total volume, and Su is the portion of the boundary of D where displacement u0i is prescribed. It should be mentioned that the stiffness tensor L, and the compliance tensor M in the above theorems need not be uniform throughout D, meaning that both theorems are applicable to heterogeneous materials. In what follows, we will derive, based on the above theorems, some variational principles that are convenient to use for obtaining the bounds of effective properties. To begin, consider the heterogeneous material considered in Section 5.6. Let the displacement be prescribed on the boundary S: ui兩S ⫽ ij xj,

(6.1.3)

where ij is a constant strain tensor, which, according to the average strain theorem (5.4.11), is also the average in the composite under such boundary condition: ij ⫽

1 D

冕 D

ij

d.

(6.1.4)

Therefore, the overbar on the strain tensor causes no confusion between the given strain tensor on the boundary and the average strain tensor in D since they are the same. Under the displacement boundary condition (6.1.3), the potential energy of the composite, following (6.1.1), can be written as ⌸[ui] ⫽

1 2

冕L D

u u d ⫽

ijkl k,l i, j

1 2

冕L D

d,

ijkl kl ij

(6.1.5)

since no traction is prescribed. To facilitate the following discussions, we will denote the actual displacement ﬁeld by ui and any kinematically admissible displacement ﬁeld by uˆ i. Clearly, under the displacement

122

BOUNDS FOR EFFECTIVE MODULI

boundary condition, all kinematically admissible displacement (the actual displacement included) ﬁelds must satisfy (6.1.3). Let U be the average strain energy density in the heterogeneous material when it is subjected to (6.1.3): U⫽

1 2D

冕L

d ⫽

ijkl kl ij

D

1 L , 2 ij ijkl kl

(6.1.6)

where Lijkl is the effective stiffness tensor of the heterogeneous material and the last equality follows from (5.6.6). Then, according to the minimum potential energy theorem, the following inequality holds for any kinematically admissible displacement ﬁeld uˆ i: Uⱕ

冕L

1 2D

uˆ uˆ d.

(6.1.7)

ijkl k,l i, j

D

Now, consider the complimentary energy. Again, under the displacement boundary condition (6.1.3), the complimentary energy becomes ⌸c[ij] ⫽

1 2

冕M

klij d ⫺

ijkl

D

冕 x n ds. S

ik k

ij

j

(6.1.8)

Upon the use of the divergence theorem on the second term, ⌸c[ij] ⫽

1 2

冕M

klij d ⫺

ijkl

D

冕 ( x ) ds. D

ik k

ij j

(6.1.9)

For any statically admissible stress ﬁeld, that is, ij, j ⫽ 0, the above reduces to ⌸c[ij] ⫽

1 2

冕M D

klij d ⫺ ij

ijkl

冕 D

ij

d,

(6.1.10)

where ij is the average stress in D, ij ⫽

1 D

冕 D

ij

d.

(6.1.11)

Let ij be the actual stress ﬁeld and ˆ ij be any kinematically admissible stress ﬁeld. Then, by making use of Hooke’s law, ij ⫽ Mijklkl, we can show, following the steps described in (5.6.6) and (5.6.7), that

6.2

⌸c[ij] ⫽

1 2

VOIGT UPPER BOUND AND REUSS LOWER BOUND

冕M D

klij d ⫺ ij

ijkl

冕

d ⫽ ⫺DU,

ij

D

123

(6.1.12)

where U is the average strain energy density as introduced in (6.1.7). Thus, according to the minimum complimentary energy theorem, the following inequality holds for any statically admissible stress ˆ ij: U ⱖ ij

1 D

冕 ˆ D

ij

d ⫺

1 2D

冕M D

ˆ klˆ ij d.

ijkl

(6.1.13)

Combining (6.1.7) and (6.1.13), we arrive at the following inequalities, in matrix notations:

冕 ˆ d ⫺ 冕 ˆ Mˆ d ⱕ 2DU ⱕ 冕 ˆ Lˆ d, D

D

(6.1.14)

D

where ˆ ij can be any stress ﬁeld that satisﬁes ˆ ij, j ⫽ 0

in D,

(6.1.15)

and ˆ ij ⫽ (ˆui, j ⫹ uˆ j,i) /2 with uˆ i being any displacement ﬁeld that satisﬁes uˆ i ⫽ ij xj on S.

(6.1.16)

6.2 VOIGT UPPER BOUND AND REUSS LOWER BOUND

Again, consider the heterogeneous material discussed in Section 5.6. Let the heterogeneous material be subjected to the displacement boundary condition, ui ⫽ ij xj on S,

(6.2.1)

where ij is a given constant strain tensor. According to the average strain theorem stated in Section 5.4, the average strain in D is also ij. Next, we deﬁne uˆ i ⫽ ij xj everywhere in D.

(6.2.2)

Obviously, the uˆ i so deﬁned is a kinematically admissible displacement ﬁeld, that is,

124

BOUNDS FOR EFFECTIVE MODULI

uˆ i ⫽ ij xj on S.

(6.2.3)

The kinematical admissible strain ﬁeld corresponding to uˆ i is simply ij. Further, for the boundary condition (6.2.1), any constant stress tensor ˆ ij would be a statically admissible stress ﬁeld. Thus, by substituting (6.2.2) and a constant tensor ˆ ij into (6.1.14) yields 2 ˆ ⫺ ˆ MR ˆ ⱕ 2U ⱕ L⬘,

(6.2.4)

where LV ⫽

1 D

冕 L d,

MR ⫽

D

1 D

冕 M d.

(6.2.5)

D

Since ˆ can be any constant stress tensor, we should try to select one that maximizes the far left-hand side of (6.2.4) to obtain the optimal lower bound. It turns out that ˆ ⫽ LR ⫽ (MR)⫺1

(6.2.6)

would be the choice. Substituting (6.2.6) and (6.1.6) into (6.2.4), we obtain the following: LR ⱕ L ⱕ LV ,

(6.2.7)

where R ⫺1

L ⫽ (M ) R

冋

1 ⫽ D

冕 M d册

⫺1

;

(6.2.8)

D

These inequalities must hold true for any constant strain tensor . Therefore, we conclude LR ⱕ L ⱕ LV,

(6.2.9)

where LV deﬁned by the ﬁrst of (6.2.5) is called the Voigt upper bound, and LR deﬁned by (6.2.8) is called the Reuss lower bound. If the stiffness tensor of the rth phase of volume ⍀r is uniform and given by Lr , where r ⫽ 0, 1, . . . , N (r ⫽ 0 corresponds to the matrix), then the ﬁrst of (6.2.5) can be simpliﬁed to

6.2

VOIGT UPPER BOUND AND REUSS LOWER BOUND

冘cL,

125

N

LV ⫽

r

(6.2.10)

r ⫽ 1, 2, . . . , N

(6.2.11)

r

r⫽0

where cr ⫽

⍀r

D

,

are the volume fraction of the inhomogeneities with stiffness tensor Lr. Obviously, we have the relationship

冘 c ⫽ 1. N

(6.2.12)

r

r⫽0

Equation (6.2.10) gives the Voigt upper bound for the effective stiffness tensor of a composite with N distinct phases. Similarly, (6.2.8) can be written as

冋冘 册

⫺1

N

L ⫽ R

cr Mr

,

(6.2.13)

r⫽0

where Mr is the compliance tensor for the rth phase. It is noted that the bounds are derived in terms of the volume faction of each phase only. Therefore, they are independent of the geometry of the phases and their distribution. Example 6.1 Consider an isotropic matrix of stiffness tensor L0 ⫽ (3K0, 20) reinforced by particles of stiffness tensor L1 ⫽ (3K1, 21). We are to ﬁnd the bounds of the effective elastic constants. To solve this problem, let us ﬁrst consider the compliance tensors. Following the rules discussed in Section 1.4: M0 ⫽ Thus,

冉

冊

1 1 , , 3K0 20

M1 ⫽

冉

冊

1 1 , . 3K1 21

(6.2.14)

126

BOUNDS FOR EFFECTIVE MODULI

⫺1

[c0M0 ⫹ c1M1]

冉 冉

c0 c c c ⫽ ⫹ 1, 0 ⫹ 1 3K0 3K1 20 21 ⫽

冊

⫺1

冊

3K0K1 201 , . c0K1 ⫹ c1K0 c01 ⫹ c10

(6.2.15)

According to (6.2.9), the effective stiffness tensor of the composite satisﬁes the inequality [c0M0 ⫹ c1M1]⫺1 ⱕ L ⫽ (3K, 2) ⱕ c0L0 ⫹ c1L1,

(6.2.16)

where K and are the effective bulk and shear moduli of the composite, respectively, and c1 is the volume fraction of the particles. Making use of (6.2.15) in (6.2.16), we have K0K1 ⱕ K ⱕ K0 ⫹ c1(K1 ⫺ K0), K1 ⫺ c1(K1 ⫺ K0)

(6.2.17)

01 ⱕ ( ⱕ 0 ⫹ c1(1 ⫺ 0). 1 ⫺ c1(1 ⫺ 0)

(6.2.18)

These give the upper and lower bounds for the effective bulk and shear moduli of the composite.

6.3 EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

It is noted that the Voigt upper and the Reuss lower bounds were obtained by specifying a kinematically admissible displacement ﬁeld in the potential energy and by specifying a statically admissible stress ﬁeld in the complimentary energy. In other words, the key to ﬁnd bounds is to ﬁnd suitable admissible ﬁelds. In fact, this approach is rather general. Tighter bounds can be derived by specifying kinematically and statically admissible ﬁelds that make some explicit allowance for the microstructure of the composite. To this end, let us ﬁrst try to develop an alternative form of the classical variational principles that are better suited for developing bounds of the effective properties of heterogeneous materials. For the heterogeneous material considered in Section 5.6, we assume that the following displacement boundary condition is prescribed:

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

ui ⫽ ij xj on S.

127

(6.3.1)

Our objective is to ﬁnd a kinematically admissible displacement ﬁeld (rather than a constant tensor as in the Voigt upper bound) and a statically admissible stress tensor (rather than a constant tensor as in the Reuss lower bound) for this heterogeneous material under the boundary condition (6.3.1). To this end, let us write the elastic stiffness tensor of the heterogeneous material in the following form: L(x) ⫽ Lh ⫹ L p(x),

(6.3.2)

where it is understood that L(x) is a function of position vector x, Lh is a constant fourth-order tensor representing a homogeneous material, and L p(x), being the difference between L(x) and Lh, is also a function of position vector x, representing the perturbation from the homogeneous material. The constant stiffness tensor Lh is introduced to represent a homogeneous ‘‘comparison’’ material. The corresponding actual stress ﬁeld in the heterogeneous material is then given by (x) ⫽ Lh(x) ⫹ (x),

(6.3.3)

where ij (x) ⫽

冉

冊

1 ⭸ui(x) ⭸uj(x) ⫹ 2 ⭸xj ⭸xi

(6.3.4)

is the actual strain tensor in D and (x) ⫽ L p(x)(x)

(6.3.5)

is called the stress polarization in some of the literature. Clearly, (x) is symmetric, that is, ij(x) ⫽ ji(x), because of the symmetry of L p(x). In light of (6.3.3), the equations of equilibrium in terms of the displacement can be written as Lhijkluk,lj (x) ⫹ ij, j (x) ⫽ 0

in D.

(6.3.6)

If we treat the second term on the left-hand side as a body force, the solution to the boundary value problem (6.3.1) and (6.3.6) can be attained in terms of Green’s function; see (2.6.51):

128

BOUNDS FOR EFFECTIVE MODULI

冕L

ui(x) ⫽

h pjkl

S

⭸Gki(x, y) pq yq nj dS(y) ⫹ ⭸xl

冕 G (x, y) ⭸⭸y(y) dV(y), mn

mi

D

n

(6.3.7) where Gmi(x, y) is Green’s function in the homogeneous comparison material satisfying h Lijkl

⭸2Gkm,lj (x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl ⭸xj

in V,

Gij (x, y)兩x僆S ⫽ 0.

(6.3.8) (6.3.9)

By using the divergence theorem and (6.3.8), the surface integral in (6.3.7) can be simpliﬁed to

冕L S

⭸Gki(x, y) pq yq nj dS(y) ⭸xi

h pjkl

冕L

⫽⫺ ⫽

h pjkl

D

⭸2Gki(x, y) y dV(y) ⫹ ⭸xl ⫹ ⭸yj pq q

冕 ␦ ␦(x, y) D

pi

y dV(y) ⫹

pq q

冕L

冕L

h pjkl

D

⭸Gki(x, y) pj dV(y) ⭸xl

Gki(x, y)pj nj dS(y)

h pjkl

S

⫽ iq xq.

(6.3.10)

Substituting (6.3.10) into (6.3.7) and applying the divergence theorem to the volume integral in conjunction with (6.3.9), we have

冕 G (x, y) ⭸⭸y(y) dV(y) ⭸G (x, y) ⫽ x ⫺冕 (y) dV(y). y

ui(x) ⫽ iq xq ⫹

mn

D

mi

n

mi

iq q

mn

D

(6.3.11)

n

The displacement gradient is thus given by ui, j (x) ⫽ ij ⫺

冕 ⭸ G⭸x(x⭸y⫺ y) 2

mi

D

(y) dV(y).

mn

j

n

The strain tensor follows (6.3.12) readily,

(6.3.12)

6.3

ij (x) ⫽ ij ⫺

1 2

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

冕 冉⭸ G⭸x(x⭸y⫺ y) ⫹ ⭸ G⭸x(x⭸y⫺ y)冊 2

2

mj

mi

D

129

j

n

i

mn

(y) dV(y),

n

(6.3.13) Using the symmetry properties of mn(y), we can rewrite the above into (x) ⫽ ⫺

冕 ⌫(x, y)(y) dV(y),

(6.3.14)

D

where ⌫ijkl(x, y) 1 ⭸2Gki(x ⫺ y) ⭸2Gkj (x ⫺ y) ⭸2Gli(x ⫺ y) ⭸2Glj (x ⫺ y) ⫽ ⫹ ⫹ ⫹ . 4 ⭸xj ⭸yl ⭸xi ⭸yl ⭸xj ⭸yk ⭸xi ⭸yk

冋

册

(6.3.15) Since the integral operator in (6.3.14) will be used many times, we will, for convenience, use the following symbolic notation to indicate the integration operation:

冕 ⌫(x, y)(y) dV(y) ⬅ ⌫(x, y) * (y).

(6.3.16)

D

Using this notation, (6.3.14) can be awritten as (x) ⫽ ⫺ ⌫(x, y) * (y).

(6.3.17)

Before proceeding forward, we note that the integral operator is selfadjoint, that is, (x) * [⌫(x, y) * (y)] ⫽ (x) * [⌫(x, y) * (y)].

(6.3.18)

This can be readily proven by noting that ⌫(x, y) ⫽ ⌫(y, x).

Further, we have

(6.3.19)

130

BOUNDS FOR EFFECTIVE MODULI

冕 ⌫(x, y) dV(y) ⫽ 0,

⌫(z, x) * Lh⌫(x, y) ⫽ ⌫(z, y).

D

(6.3.20)

The ﬁrst of (6.3.20) can be veriﬁed by noting, for example,

冕 ⭸ G⭸x (x,⭸y y) dV(y) ⫽ ⭸⭸x 冕 ⭸G ⭸(x,y y) dV(y) ⭸ ⫽ 冕 G (x, y)n dS(y) ⫽ 0. ⭸x 2

ki

D

ki

j

l

j

D

j

S

l

ki

l

(6.3.21)

The second of (6.3.20) can be veriﬁed by noting, for example,

冕 ⭸ G⭸x (z,⭸z x) L ⭸ G⭸x (x,⭸y y) dV(x) ⭸G (x, y) ⭸ ⭸G (z, x) ⫽ 冕 L dV(x) ⭸z ⭸y ⭸x ⭸x ⭸G (x, y) ⭸ ⭸ ⫽ 冕 G (z, x)L 再 冋 册 ⭸z ⭸y ⭸x ⭸x 2

2

ki

D

pm

h klmn

l

j

n

q

2

ki

j

q

D

pm

h klmn

l

n

2

j

D

q

l

⫺ Gki(z, x)Lhklmn ⭸2 ⫽⫺ ⭸zj ⭸yq ⫽

⭸2 ⭸zj ⭸yq

h klmn

ki

冕 G (z, x)L

h klmn

ki

D

冎

⭸Gpm(x, y) ⭸xn ⭸xl

pm

n

dV(x)

⭸Gpm(x, y) dV(x) ⭸xn ⭸xl

冕 G (z, x)␦ ␦(x ⫺ y) dV(x) ki

D

kp

⭸2Gpi(z, y) ⫽ . ⭸zj ⭸yq

(6.3.22)

Let us now consider (6.3.11). Because of (6.3.9), we have ui(x)兩x僆S ⫽ iq xq兩x僆S ⫹

冕 G (x, y)兩 D

mi

x僆S

⭸mn(y) dV(y) ⫽ iq xq兩x僆S, ⭸yn

regardless of the choice of (y). In other words, for any given ˆ (y), the displacement derived from (6.3.11), therefore, the corresponding strain derived from (6.3.17),

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

ˆ (x) ⫽ ⫺ ⌫(x, y) * ˆ (y)

131

(6.3.23)

are kinematically admissible displacement and strain ﬁelds, respectively. Therefore, the minimum potential energy theorem (6.1.7) leads us to the following inequality: 2DU ⱕ

冕 ˆ Lˆ d ⫽ 冕 ˆ L ˆ d ⫹ 冕 ˆ L ˆ d. h

D

p

D

(6.3.24)

D

Substitute (6.3.23) into (6.3.24) and make use of properties of the integral operator ⌫(x, y), and (6.3.19) and (6.3.20), we arrive at the following inequality: 2D(U ⫺ Uh) ⱕ

冕 ˆ ⌫(x, y) * ˆ(y) d ⫹ 冕 L d ⫺ 2 冕 L ⌫(x, y) * ˆ (y) d ⫹ 冕 ⌫(x, y) * ˆ (y)L ⌫(x, y) * ˆ (y) d, p

D

D

p

D

p

D

(6.3.25)

where Uh ⫽

1 2D

冕 L d. h

(6.3.26)

D

Through a straightforward simpliﬁcation, one can show that the last term in (6.3.25) can be rewritten as

冕 ⌫(x, y) * ˆ(y)L ⌫(x, y) * ˆ(y) d ⫽ 冕 [ˆ]L [ˆ] d ⫺ 冕 ˆ (L ) ˆ d ⫺ 2 冕 ˆ ⌫(x, y) * ˆ (y) d ⫺ 冕 L d ⫹ 2 冕 {ˆ ⫹ L ⌫(x, y) * ˆ (y)} d, p

D

p ⫺1

p

D

D

p

D

D

p

D

(6.3.27)

where [ˆ] ⫽ (L p)⫺1ˆ ⫹ ⌫(x, y) * ˆ (y) ⫺ .

(6.3.28)

132

BOUNDS FOR EFFECTIVE MODULI

Substituting (6.3.27) into (6.3.25), we obtain, for any stress tensor ˆ , the desired inequality, 2D(U ⫺ Uh) ⱕ ⫺H[ˆ] ⫹

冕 [ˆ]L [ˆ] d, p

(6.3.29)

D

where H[ˆ] ⫽

冕 ˆ [ˆ] d ⫺ 冕 ˆ d. D

(6.3.30)

D

Next, we want to know what happens if the ˆ in (6.3.29) is indeed the actual stress polarization tensor of the problem, that is, ˆ ⫽ . In this case, we have, from (6.3.5) and (6.3.17), that [] ⫽ (L p)⫺1 ⫹ ⌫(x, y) * (y) ⫺ ⫽ 0,

(6.3.31)

therefore, the second term on the right-hand side of (6.3.29) would vanish. Further

冕 d ⫽ ⫺冕 (L ⫺ L ) d ⫽ ⫺2D(U ⫺ U ).

H[] ⫽ ⫺

h

D

D

h

(6.3.32)

In other words, the right-hand side of (6.3.29) is minimized if ˆ ⫽ is used, and the minimum value is equal to the left-hand side, 2D(U ⫺ Uh). We can now summarize the above derivations. First, once Lh is selected, the perturbed part of the stiffness tensor L p and Green’s function ⌫(x, y) can be computed from (6.3.2) and (6.3.8) and (6.3.9). Second, displacement ui generated from (6.3.11) is a kinematically admissible displacement ﬁeld, which leads the minimum potential energy theorem to the inequality (6.3.29). Third, the inequality is valid for any stress tensor ˆ . Finally, the equal sign is realized when ˆ is replaced by the actual solution to the stress polarization tensor of the problem. Therefore, we have just proved the following theorem. Theorem 6.1 Among all the symmetric second-order tensors, the true solution to the stress polarization tensor ˆ renders the following functional minimum:

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

I[ˆ] ⫽ Uh ⫺

1 1 H[ˆ] ⫹ 2D 2D

冕 [ˆ]L [ˆ] d, p

133

(6.3.33)

D

and the minimum value of I[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{I[ˆ]} ⫽ –12 L.

(6.3.34)

The inequality (6.3.29) can be further simpliﬁed if one assumes that L is negative semideﬁnite, that is, for any , p

冕 [ˆ]L [ˆ] d ⱕ 0. p

(6.3.35)

D

In this case, (6.3.29) reduces to 2D(U ⫺ Uh) ⱕ ⫺H[ˆ].

(6.3.36)

Therefore, we have the following theorem. Theorem 6.1a (Hashin–Shtrikman Variational Principle) When L p is negative semideﬁnite, among all the symmetric second-order tensors, the true solution to the stress polarization tensor ˆ renders the following functional minimum: Ih[ˆ] ⫽ Uh ⫺

1 H[ˆ], 2D

(6.3.37)

and the minimum value of Ih[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Ih[ˆ]} ⫽ –21 L.

(6.3.38)

Let us now turn to the complimentary energy principle. Introducing (6.3.17) to (6.3.3) yields

134

BOUNDS FOR EFFECTIVE MODULI

(x) ⫽ Lh ⫺ Lh

冕 ⌫(x, y)(y) dV(y) ⫹ (x).

(6.3.39)

D

Thus, it follows from, for example,

冕 冉⭸⭸x L ⭸ G⭸x (x,⭸y y)冊 (y) dV(y) ⭸ ⭸ G (x, y) ⫽冕 L (y)冊 dV(y) 冉 ⭸y ⭸x ⭸x ⭸ G (x, y) ⫺冕 L (y) dV(y) ⭸x ⭸x ⭸ G (x, y) ⭸ G (x, y) ⫽冕 L n dS(y) ⫺ 冕 L (y) dV(y) ⭸x ⭸x ⭸x ⭸x ⭸ G (x, y) ⫽ ⫺冕 ␦ ␦(x ⫺ y)n dS(y) ⫺ 冕 L (y) dV(y) ⭸x ⭸x ⭸ G (x, y) ⫽ ⫺冕 L (y) dV(y) ⭸x ⭸x 2

D

km

h ijmn

kl

j

n

l

2

km

h ijmn

D

kl

l

n

j

2

km

h ijmn

D

kl,l

n

j

2

h ijmn

S

2

km

l

n

D

j

km

h ijmn

kl,l

n

j

2

S

ik

l

D

h ijmn

km

kl,l

n

j

2

D

h ijmn

km

kl,l

n

j

that div((x)) ⫽ Lh

冕 ⌫(x, y)div((y)) dV(y) ⫹ div((x)).

(6.3.40)

D

One may then conclude that for any statically admissible stress tensor ˆ (x), that is, div((x)) ⫽ 0, the stress tensor ˆ (x) generated from (6.3.3) ˆ (x) ⫽ Lh(x) ⫹ ˆ (x),

(6.3.41)

is also a statically admissible stress ﬁeld, that is, div( ˆ (x)) ⫽ div(Lh(x) ⫹ ˆ (x)) ⫽ div(Lh(x)) ⫽ 0.

(6.3.42)

Having established that ˆ (x) is statically admissible, whenever ˆ (x) is, we can now consider (6.1.13) for a statically admissible ˆ (x),

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

冕 ˆ d ⫺ 冕 ˆ Mˆ d ⫽冕 ˆ d ⫺ 冕 ˆ (M ⫹ M ) ˆ d,

2DU ⱖ

D

D

D

D

h

p

135

(6.3.43)

where, analogous to (6.3.2), the compliance tensor is written as M(x) ⫽ Mh ⫹ Mp(x),

(6.3.44)

and the superscripts on the compliance tensors carry the same meaning as those for the stiffness tensors. Substituting (6.3.41) into (6.3.43), following similar steps in deriving (6.3.29) and making use of the identity, LhMp ⫹ L p(Mh ⫹ Mp) ⫽ 0,

(6.3.45)

we conclude that 2D(U ⫺ Uh) ⱖ ⫺H[ˆ] ⫺

冕 L [ˆ]M L [ˆ] d, h

p

h

(6.3.46)

D

for any statically admissible stress tensor ˆ (x). As shown earlier, if ˆ (x) happens to be the true stress polarization to the deformation problem considered here, the equal sign in (6.3.46) holds. We have just proved the following variational theorem. Theorem 6.2 Among all the statically admissible stress ﬁelds, the true solution renders the following functional maximum, Ic[ˆ] ⫽ Uh ⫺

1 1 H[ˆ] ⫺ 2D 2D

冕 L [ˆ]M L [ˆ] d, h

p

h

(6.3.47)

D

and the maximum value of Ic[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Ic[ˆ]} ⫽ –12 L.

(6.3.48)

If Mp is negative semideﬁnite (or, equivalently, L p is positive semideﬁnite), that is,

136

BOUNDS FOR EFFECTIVE MODULI

冕 L [ˆ]M L [ˆ] d ⱕ 0, h

p

h

D

then (6.3.46) implies 2D(U ⫺ Uh) ⱖ ⫺H[ˆ].

(6.3.49)

This leads to another form of the Hashin–Shtrikman variational principle. Theorem 6.2a (Hashin–Shtrikman Variational Principle) Among all the statically admissible stress ﬁelds, the true solution renders the following functional maximum: Ich[ˆ] ⫽ 2DUh ⫺ H[ˆ],

(6.3.50)

and the maximum value of Ich[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Ich[ˆ]} ⫽ –12 L.

(6.3.51)

6.4 HASHIN–SHTRIKMAN BOUNDS

As can be seen from (6.3.36) and (6.3.49), the key to developing the bounds is to ﬁnd an appropriate statically admissible stress tensor ˆ . This is what we will do next. Remembering that the Reuss and Voigt bounds were obtained by assuming uniform admissible ﬁelds throughout the composite, let us try a piecewise uniform ﬁeld for ˆ , ˆ (x)兩x僆⍀r ⫽ ˆ r ,

r ⫽ 0, 1, 2, . . . , N.

(6.4.1)

In other words, we assume that the stress polarization tensor is a constant tensor on each inhomogeneity including the matrix. Introducing (6.4.1) into (6.3.28) yields

6.4

冘 ⍀c 冕

137

HASHIN–SHTRIKMAN BOUNDS

N

[ˆ] ⫽ (L p)⫺1ˆ ⫹ D

r

s⫽0

s

⍀s

⌫(x, y) dV(y)s ⫺ .

(6.4.2)

It thus follows from (6.3.30) that

冘 冕 冋(L ) ⫹ D 冘 ⍀c 冕 ⌫(x, y) dV(y) ⫺ 册 d ⫺ 冘 冕 d ⫽ D 冘 c (L ) ⫹ D 冘 冘 c c P ⫺ 2D 冘 c , N

N

H[ˆ] ⫽

r

⍀r

r⫽0

p ⫺1

r

s⫽0

s

N

N

s

⍀s

N

r⫽0

⍀r

r

N

r r

p ⫺1 r r

N

2

r s r

rs s

r⫽0 s⫽0

r⫽0

r r

r⫽0

(6.4.3) where cr is the volume fraction of the rth inhomogeneity and (L pr )⫺1 ⫽ Prs ⫽

1 ⍀r⍀s

1 ⍀r

冕冕 ⍀r

⍀s

冕

⍀r

(L p)⫺1 d,

⌫(x, y) dV(y) dV(x).

(6.4.4)

(6.4.5)

The validity of (6.4.4) is based on the fact that the stiffness tensor is uniform on each inhomogeneity. Clearly, H[ˆ] is now a quadratic function of the constant tensor r. The speciﬁc r that gives the extreme value of H[ˆ] can be determined from ⭸H[ˆ] / ⭸r ⫽ 0,

冘 c P ⫽ , N

p ⫺1 r r

(L ) ⫹ D

s

rs s

r ⫽ 0, 1, . . . , N.

(6.4.6)

s⫽0

This is a system of linear algebraic equations for r . The solution can be written formally as r ⫽ Rr.

This leads to the following extreme value of H[ˆ]:

(6.4.7)

138

BOUNDS FOR EFFECTIVE MODULI

冘 c R ⫽ D(L ⫺ L)˜ , N

H[ˆ]兩r⫽Rr ⫽ ⫺D

h

r

r

(6.4.8)

r⫽0

where

冘 c R. N

L˜ ⫽ Lh ⫹

r

(6.4.9)

r

r⫽0

For L p being negative semideﬁnite, substituting (6.4.8) into (6.3.36) yields 2U ⫽ L ⱕ L˜ ,

(6.4.10)

or

冘cR, N

L ⱕ L˜ ⫽ Lh ⫹

r

r

(6.4.11)

r⫽0

with L˜ being given by (6.4.9). Dually, for L p being positive semideﬁnite, substituting (6.4.8) into (6.3.49) yields

冘 c R. N

L ⱖ L˜ ⫽ Lh ⫹

r

r

(6.4.12)

r⫽0

The inequalities (6.4.11) and (6.4.12) are the Hashin–Shtrikman bounds for the effective stiffness tensor of a heterogeneous material containing N-phase inhomogeneities. In general, the Hashin–Shtrikman bounds are more restrictive than Voigt and Reuss bounds. It is noted that, in order to evaluate the Hashin–Shtrikman bounds, the double integral in (6.4.5) needs to be evaluated. Although, theoretically speaking, the integral can be carried out for a given heterogeneous material, the large number of inhomogeneities and the statistical nature of their distributions in a heterogeneous material render the integration impractical. We need to ﬁnd a practical way to evaluate it, albeit, approximately. Recall from (6.3.15) that the integrand consists of the second derivatives of Green’s function Gij(x, y) in the domain D, which satisﬁes zero displacement boundary condition; see (6.3.8) and (6.3.9). One of the proposals of simplifying (6.4.5) (see Willis, 1982) is to replace

6.4

HASHIN–SHTRIKMAN BOUNDS

139

Green’s function Gij(x, y) in the ﬁnite domain D by its counterpart in the inﬁnite domain, Prs ⬇

1 ⍀r⍀s

冕冕 ⍀r

⌫⬁(x, y) dV(y) dV(x),

⍀s

(6.4.13)

where ⌫⬁(x, y) is given by (3.3.18), which is related to Green’s function in an unbounded domain, G⬁ij (x, y) derived in Section 2.6: G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij ()D⫺1()ei䡠(x⫺y) d.

(6.4.14)

For statistically homogeneous and isotropic distribution of inhomogeneities, the integral in (6.4.13) can be evaluated; see Appendix 6.A: Prs ⬇

冕冕 ⍀⍀ 1

r

s

⍀r

⍀s

⌫⬁(x, y) dV(y) dV(x) ⫽

1 ⍀s

(␦rs ⫺ cs)P,

(6.4.15)

where P(x) ⫽

冕

⌫⬁(x, y) dV(y)

Sˆ 2

for x 僆 Sˆ 2,

(6.4.16)

and the integral is over a unit sphere Sˆ 2. It follows from (4.3.19) that the tensor P is related to the Eshelby tensor S through P ⫽ S(Lh)⫺1.

(6.4.17)

Substituting (6.4.15) into (6.4.6) yields

冘 c ⫽ , N

(L pr )⫺1r ⫹ Pr ⫺ P

s s

r ⫽ 0, 1, . . . , N,

(6.4.18)

s⫽0

which can be rewritten as

冉

r ⫽ [(L pr )⫺1 ⫹ P]⫺1 ⫹ P

Further,

冘 c 冊, N

s s

s⫽0

r ⫽ 0, 1, . . . , N. (6.4.19)

140

BOUNDS FOR EFFECTIVE MODULI

冘

冉

冘 ⫽ 冘 c [(L )

N

N

r⫽0

r⫽0

s s

s⫽0

N

r

冘 c冊 N

cr [(L pr )⫺1 ⫹ P]⫺1 ⫹ P

crr ⫽

冘 [(L ) N

p ⫺1 r

⫹ P]⫺1 ⫹

⫹ P]⫺1 P

r⫽0

r⫽0

冘 c. N

p ⫺1 r

s s

s⫽0

(6.4.20) Finally, making use of (6.4.7), we have

冘 c R ⫽ 再I ⫺ 冘 c [(L ) ⫽ 冋 冘 c (I ⫹ L P) N

冎

⫺1

N

s

s

r

p ⫺1 r

r⫽0

s⫽0

N

p r

r

r⫽0

⫹ P]⫺1P

册

⫺1

⫺1

冘 c [(L ) N

p ⫺1 r

r

⫹ P]⫺1

r⫽0

冘 c (I ⫹ L P) N

p r

r

⫺1

L pr .

(6.4.21)

r⫽0

Thus, it follows from (6.4.9) that

冋冘 c (I ⫹ L P) N

L˜ ⫽ Lh ⫹

r

p r

r⫽0

册

⫺1

⫺1

冘 c (I ⫹ L P) N

r

p r

⫺1

L pr .

(6.4.22)

r⫽0

Example 6.2 Let a composite material be made of a matrix with elastic stiffness tensor L0 containing uniformly distributed identical spherical inhomogeneities with elastic stiffness tensor L1. Assume that both L0 and L1 are isotropic and given by L0 ⫽ (3K0, 20),

L1 ⫽ (3K1, 21),

(6.4.23)

where K1 ⬎ K0, 1 ⬎ 0. If the volume fraction of the inhomogeneities is c1, ﬁnd the bounds of its effective stiffness tensor. To ﬁnd the bounds for the effective stiffness tensor of the composites, we need to know the tensor L˜ as given by (6.4.22). To this end, let us compute the relevant tensors one at a time. First, we choose (it will be seen later that the choice is arbitrary) Lh ⫽ L0. Consequently,

(6.4.24)

6.4

L p(x) ⫽

HASHIN–SHTRIKMAN BOUNDS

再

L1 ⫺ L0 x 僆 ⍀1 . 0 x 僆 ⍀0

141

(6.4.25)

So, L p0 ⫽

冕 ⍀ 1

0

⍀0

L p d ⫽ 0,

L 1p ⫽

1 ⍀1

冕

⍀1

L p d ⫽ L1 ⫺ L0. (6.4.26)

Introducing the above to (6.4.22) leads to

冋冘

冋冘

cr(I ⫹ L rpP)⫺1

r⫽0

册

⫺1

1

⫽

⫺1

cr(I ⫹ L P) p r

r⫽0

册

⫺1

1

L˜ ⫽ L0 ⫹

冘 c (I ⫹ L P) 1

p r

r

⫺1

(Lr ⫺ L0)

r⫽0

冘 c (I ⫹ L P) 1

p r

r

⫺1

Lr

r⫽0

⫽ {c0I ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1}⫺1 ⫻ {c0L0 ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1L1}.

(6.4.27)

For spherical inhomogeneities, the Eshelby tensor is given by (see Appendix 4.B) S ⫽ (3␥0, 2␦0),

(6.4.28)

where ␥0 ⫽

K0 3K0 ⫹ 40

⫽

1 ⫹ 0 , 9(1 ⫺ 0)

␦0 ⫽

3(K0 ⫹ 20) 4 ⫺ 5 0 ⫽ . 5(3K0 ⫹ 40) 15(1 ⫺ 0) (6.4.29)

Therefore, making use of (6.4.17), we have I ⫹ (L1 ⫺ L0)P

冉 冊

⫽ (1,1) ⫹ (3K1 ⫺ 3K0, 21 ⫺ 20)(3␥0, 2␦0) ⫽

冉

Thus,

K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␥0(1 ⫺ 0) , . K0 0

冊

1 1 , 3K0 20

(6.4.30)

142

BOUNDS FOR EFFECTIVE MODULI

[I ⫹ (L1 ⫺ L0)P]⫺1 ⫽

冉

冊

K0 0 , . K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␥0(1 ⫺ 0) (6.4.31)

This leads to L˜ ⫽ {c0I ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1}⫺1{c0L0 ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1L1} ˘ 2 ⫽ (3K, ˘ ),

where ˘ ⫽ K

˘ ⫽

K0{(1 ⫺ c1)[K0 ⫹ 3␥0(K1 ⫺ K0)] ⫹ c1K1} , K0 ⫹ 3␥0(1 ⫺ c1)(K1 ⫺ K0)

(6.4.32)

0{(1 ⫺ c1)[0 ⫹ 2␦0(1 ⫺ 0)] ⫹ c11} . 0 ⫹ 2␦0(1 ⫺ c1)(1 ⫺ 0)

Introducing (6.4.29) into the above expressions, ˘ ⫽ K

K0(3K1 ⫹ 40) ⫹ 4c10(K1 ⫺ K0) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

˘ ⫽

601(K0 ⫹ 20) ⫹ 0(9K0 ⫹ 80)[c11 ⫹ (1 ⫺ c1)0] . 0(9K0 ⫹ 80) ⫹ 6(K0 ⫹ 20)[c10 ⫹ (1 ⫺ c1)1] (6.4.33)

Since K1 ⬎ K0, 1 ⬎ 0, one can see that the tensor L p(x) deﬁned by (6.4.25) is positive semideﬁnite. It thus follows from (6.4.12) that ˘ 2 L ⫽ (3K, 2) ⱖ L˜ ⫽ (3K, ˘ ),

or equivalently, Kⱖ ⱖ

K0(3K1 ⫹ 40) ⫹ 4c10(K1 ⫺ K0) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(6.4.34)

601(K0 ⫹ 20) ⫹ 0(9K0 ⫹ 80)[c11 ⫹ (1 ⫺ c1)0] . 0(9K0 ⫹ 80) ⫹ 6(K0 ⫹ 20)[c10 ⫹ (1 ⫺ c1)1] (6.4.35)

6.4

HASHIN–SHTRIKMAN BOUNDS

143

These are the Hashin–Shtrikman lower bounds. To ﬁnd the Hashin–Shtrikman upper bounds, we choose Lh ⫽ L1. Consequently, L p(x) ⫽

(6.4.36)

再

L0 ⫺ L1 x 僆 ⍀0 . 0 x 僆 ⍀1

(6.4.37)

So, L p0 ⫽

1 ⍀0

冕

⍀0

L p d ⫽ L0 ⫺ L1,

1

L 1p ⫽

⍀1

冕

L p d ⫽ 0.

⍀1

(6.4.38) Thus, we have

冋冘 c (I ⫹ L P) 1

L˜ ⫽ L1 ⫹

冋冘

p r

r

r⫽0

册

⫺1

1

⫽

⫺1

cr(I ⫹ L P) p r

r⫽0

册

⫺1

⫺1

冘 c (I ⫹ L P) 1

p r

r

⫺1

(Lr ⫺ L1)

r⫽0

冘 c (I ⫹ L P) 1

r

p r

⫺1

Lr

r⫽0

⫽ {c0[I ⫹ (L0 ⫺ L1)P]⫺1 ⫹ c1I}⫺1 ⫻ {c0[I ⫹ (L0 ⫺ L1)P]⫺1L0 ⫹ c1L1}.

(6.4.39)

Since I ⫹ (L0 ⫺ L1)P

冉 冊

⫽ (1,1) ⫹ (3K0 ⫺ 3K1, 20 ⫺ 21)(3␥0, 2␦0) ⫽

冉

K0 ⫹ 3␥0(K0 ⫺ K1) 0 ⫹ 2␥0(0 ⫺ 1) , . K0 0

冊

1 1 , 3K0 20

(6.4.40)

Thus, [I ⫹ (L0 ⫺ L1)P]⫺1 ⫽

冉

冊

0 K0 , . K0 ⫹ 3␥0(K0 ⫺ K1) 0 ⫹ 2␥0(0 ⫺ 1)

(6.4.41)

144

BOUNDS FOR EFFECTIVE MODULI

This leads to L˜ ⫽ {c0[I ⫹ (L0 ⫺ L1)P]⫺1 ⫹ c1I}⫺1 ៣ ៣ ⫻ {c0[I ⫹ (L0 ⫺ L1)P]⫺1L0 ⫹ c1L1} ⫽ (3K, 2),

(6.4.42)

where ៣

K⫽

K20 ⫺ c1(K1 ⫺ K0)(3␥0K1 ⫺ K0) , K0 ⫺ 3␥0c1(K1 ⫺ K0)

2 ⫺ c1(1 ⫺ 0)(2␦01 ⫺ 0) ៣ ⫽ 0 . 0 ⫺ 2␦0c1(1 ⫺ 0)

(6.4.43)

Introducing (6.4.29) into the above expressions, ៣

K⫽

K0(3K0 ⫹ 40) ⫹ c1(K1 ⫺ K0)[40 ⫺ 3(K1 ⫺ K0)] , 3K0 ⫹ 40 ⫺ 3c1(K1 ⫺ K0)

520(3K0 ⫹ 40) ⫹ c1(1 ⫺ 0)[50(3K0 ⫹ 40) ⫺ 61(K0 ⫹ 20)] ៣ ⫽ . 50(3K0 ⫹ 40) ⫺ 6c1(K0 ⫹ 20)(1 ⫺ 0) (6.4.44) Since K1 ⬎ K0, 1 ⬎ 0, one can see that the tensor L p(x) deﬁned by (6.4.37) is negative semideﬁnite. It thus follows from (6.4.11) that ៣

៣

L ⫽ (3K, 2) ⱕ L˜ ⫽ (3K, 2), or equivalently, Kⱕ

K0(3K0 ⫹ 40) ⫹ c1(K1 ⫺ K0)[40 ⫺ 3(K1 ⫺ K0)] , 3K0 ⫹ 40 ⫺ 3c1(K1 ⫺ K0) 520(3K0 ⫹ 40) ⫹ c1(1 ⫺ 0) [50(3K0 ⫹ 40) ⫺ 61(K0 ⫹ 20)] ⱕ . 50(3K0 ⫹ 40) ⫺ 6c1(K0 ⫹ 20)(1 ⫺ 0)

These are the Hashin–Shtrikman upper bounds.

(6.4.45)

(6.4.46)

PROBLEMS

145

PROBLEMS

6.1 Show that 2 ˆ ⫺ ˆ MR ˆ ⱕ (MR)⫺1 for any constant tensor ˆ ij. 6.2 Show that the integral operator

冕 ⌫(x, y)(y) dV(y) ⬅ ⌫(x, y) * (y) D

is self-adjoint, that is, (x) * (⌫(x, y) * (y)) ⫽ (x) * (⌫(x, y) * (y)).

6.3 Show the identity LhMp ⫹ L p(Mh ⫹ Mp) ⫽ 0. 6.4 Show that, for a composite comprising isotropic matrix and Nphase isotropic, spherical inhomogeneities, the Hashin–Shtrikman bounds are given by

冉冘 K ⫹c K*冊

⫺1

N

r⫽0

冉冘 N

r⫽0

r

冊

r ⫹ S*

⫺1

r

r⫽0

S

cr

冉冘 K ⫹c K*冊 N

⫺ K* S ⱕ K ⱕ

r

⫺1

冉冘 N

⫺ S* ⱕ ⱕ

r⫽0

r

⫺ K*, L

L

cr

冊

r ⫹ * L

⫺1

⫺ L*,

where K* L ⫽

4L , 3

L* ⫽

3 , 2[1/ L ⫹ 10/(9KL ⫹ 8L)]

K* S ⫽

4S , 3

* S ⫽

3 , 2[1/ S ⫹ 10/(9KS ⫹ 8S)]

L ⫽ max{0, 1, . . . , N},

S ⫽ min{0, 1, . . . , N},

KL ⫽ max{K0, K1, . . . , KN},

KS ⫽ min{K0, K1, . . . , KN}.

146

BOUNDS FOR EFFECTIVE MODULI

6.5 Assume that the traction boundary condition n兩x僆S ⫽ n is prescribed on the entire boundary, where is a constant stress tensor (the average stress). Use the minimum potential energy theorem to prove that for any continuously differentiable displacement ﬁeld uˆ i,

冕 ˆ Lˆ d ⫹ 2 冕 ˆ d,

2DU ⱖ ⫺

D

D

where U⫽

1 2D

冕 L d ⫽ 12 L, D

ˆ ij ⫽ –12 (ˆui,j ⫹ uˆ j,i).

(Hint: Since there is no displacement boundary, any continuously differentiable displacement ﬁeld would be kinematically admissible.) 6.6 Show that under the traction boundary condition n兩x僆S ⫽ n,

冕L

⫺

D

uˆ uˆ d ⫹ 2ij

ijkl i, j k,l

冕 uˆ D

i, j

d ⱕ 2DU ⱕ

冕 ˆ M D

ij

ˆ kl d,

ijkl

where uˆ i is any continuously differentiable displacement ﬁeld and ˆ ij is any statically admissible stress ﬁelds, that is, ˆ ij,i ⫽ 0 in D and ijnj兩x僆S ⫽ ij nj on S. 6.7 Following the notations introduced in Appendix 6.A, please show that the following inequality holds for any eigenstrain ˆ : ˜ ) ⫺ 2D(U ⫺ Uhc ) ⱖ ⫺H(ˆ

冕 ␥(x)L (x)␥(x) dV(x). p

D

6.8 Prove Theorems 6.4 and 6.4a in Appendix 6A. 6.9 Prove Lpqij 兰S

˜ mi(x, y) ⭸G msns dS(y) ⫽ pq. ⭸xj

APPENDIX 6.A

147

APPENDIX 6.A

In Sections 6.3 and 6.4, the variational theorems have been established for heterogeneous material under the displacement boundary conditions. Let us now consider the traction boundary condition, (x)n兩x僆S ⫽ n,

(6.A.1)

where is a constant stress tensor. Analogous to (6.3.5), we introduce a strain polarization * (or eigenstrain) through ⫽ Mh ⫹ *

or ⫽ (Mh)⫺1( ⫺ *),

(6.A.2)

where Mh is deﬁned in (6.3.44), and is the actual total strain in the heterogeneous material D, which is related to the displacements through (6.3.4). Using Hooke’s law ⫽ M in the ﬁrst of (6.A.2) gives * ⫽ Mp.

(6.A.3)

Substituting the second of (6.A.2) into the equations of equilibrium, Lhijkluk,lj (x) ⫺ Lhijkl*kl, j (x) ⫽ 0

in D,

(6.A.4)

where Lhijkl is to denote the inverse of Mhijkl. To solve (6.A.4) under the traction boundary condition (6.A.1), let us consider the following Green’s function: h Lijkl

˜ km(x, y) ⭸2G ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl ⭸xj h Lijkl

in V,

˜ km(x, y) ⭸G nj兩x僆S ⫽ 0. ⭸xl

(6.A.5)

(6.A.6)

It then follows from (2.6.51) that ui(x) ⫽

冕 G˜ (x, y) S

mi

msns dS(y) ⫺

冕 G˜ (x, y) ⭸L ⭸y*(y) dV(y). h mnkl kl

V

mi

n

(6.A.7) The corresponding displacement gradient tensor follows immediately:

148

BOUNDS FOR EFFECTIVE MODULI

ui, j (x) ⫽

冕 ⭸G˜ ⭸(x,x y)

ms ns dS(y) ⫺

mi

S

j

冕 ⭸G˜ x(x, y) ⭸L ⭸y*(y) dV(y). h mnkl kl

mi

V

j

n

(6.A.8) The use of Hooke’s law leads us to the corresponding stress tensor:

冕 ⭸G˜ ⭸(x,x y) n dS(y) ˜ (x, y) ⭸L *(y) ⭸G ⫺L 冕 dV(y). ⭸x ⭸y

pq(x) ⫽ Lpqij

mi

ms s

S

j

h mnkl kl

mi

pqij

D

j

(6.A.9)

n

It is easy to show that Lpqij

冕 ⭸G˜ ⭸(x,x y)

n dS(y) ⫽ pq.

mi

ms s

S

(6.A.10)

j

Thus, the stress tensor is simpliﬁed to pq(x) ⫽ pq ⫺ Lpqij

冕 ⭸G˜ ⭸(x,x y) ⭸L ⭸y*(y) dV(y). h mnkl kl

mi

D

j

(6.A.11)

n

Note that pq is a constant stress tensor (the average stress in the composite). Therefore, by making use of the properties of Green’s function, one can show that

冕 ⭸G˜⭸x (x,⭸x y) ⭸L ⭸y*(y) dV(y)

pq,q(x) ⫽ ⫺Lpqij ⫽ ⫽

and

冕␦ D

h mnkl kl

mi

D

j

␦(x ⫺ y)

mp

q

n

h ⭸Lmnkl kl *(y) dV(y) ⭸yn

h ⭸Lpnkl kl *(x) ⫽ Lhpnklkl,n * (x) ⭸xn

(6.A.12)

149

APPENDIX 6.A

pq(x)nq兩x僆S ⫽ ⫺Lpqij ⫽ ⫺Lpqij

冕 ⭸G˜ ⭸(x,x y) n ⭸L ⭸y*(y) dV(y) ⫹ 冕 ⭸G˜ ⭸(x,x y) n ⭸L ⭸y*(y) dV(y) ⫹ h mnkl kl

mi

q

D

j

nq

pq

nq

h mnkl kl

mi

q

D

pq

n

j

n

⫽ pq nq.

(6.A.13)

In other words, regardless of the choice of *(y), the stress tensor kl generated from (6.A.11) is always a statically admissible stress ﬁeld, that is, it satisﬁes (6.A.4) and (6.A.1). For convenience, we deﬁne the following operator to represent the volume integral in (6.A.11): Lpqij

冕 ⭸G˜ ⭸(x,x y) ⭸L ⭸y*(y) dV(y) ⬅ 冕 ⌫˜ h mjkl kl

mi

D

j

j

D

(x, y)kl*(y) dV(y).

pqkl

(6.A.14) Analogues to (6.3.16), the operator can also be written symbolically,

冕 ⌫˜ (x, y)*(y) dV(y) ⬅ ⌫˜ (x, y) * *(y).

(6.A.15)

D

Thus, the stress tensor can be written formally as ˜ (x, y) * *(y). (x) ⫽ ⫺ ⌫

(6.A.16)

It then follows from (6.A.3) that (Mp)⫺1*(x) ⫹ ⌫˜ (x, y) * * ⫽ .

(6.A.17)

Let ˆ (y) be any strain polarization, and ˆ (x) ⫽ ⫺ ⌫˜ (x, y) * *(y)

(6.A.18)

the corresponding statically admissible stress ﬁeld. The minimum complementary energy theorem takes the following form:

150

BOUNDS FOR EFFECTIVE MODULI

2DUc ⱕ

冕 ˆ (x)M(x)ˆ (x) dV(x),

(6.A.19)

D

where 1 2D

Uc ⫽

冕M

klij d ⫽

ijkl

D

1 M. 2

(6.A.20)

Substituting (6.A.18) into (6.A.19), after some simpliﬁcations, yields ˜ ) ⫹ 2D(U ⫺ Uhc ) ⱕ ⫺H(ˆ

冕 ␥(x)M (x)␥(x) dV(x). p

(6.A.21)

D

where the compliance tensor has been decomposed as in (6.3.44) and Uh ⫽ –12 Mh,

(6.A.22)

Lh␥(x) ⫽ ⌫˜ (x, y) * ˆ (y) ⫹ (Mh)⫺1ˆ (x) ⫺ ,

冕 ˆ (x)L ␥(x) dV(x) ⫹ 冕 ˆ (x) d.

˜ ) ⫽ ⫺ H(ˆ

h

D

(6.A.23)

D

If ˆ happens to be the actual strain polarization * for the problem at hand, then the use of (6.A.17) leads to ␥(x) ⫽ 0, ˜ *) ⫽ H(

冕 *(x) d ⫽ 冕 (M(x) ⫺ M ) d ⫽ 2D(U ⫺ U ). h

D

D

c

h c

In other words, the equal sign in (6.A.21) is attained when the actual strain polarization * for the problem at hand is used. Therefore, we can state the following variational principle. Theorem 6.3 Among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional minimum:

APPENDIX 6.A

Jc[ˆ] ⫽

1 1 ˜ 1 Mh ⫺ H(ˆ) ⫹ 2 2D 2D

151

冕 ␥(x)M (x)␥(x) dV(x), p

D

(6.A.24) and the minimum value of Jc[ˆ] is the strain energy of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Jc[ˆ]} ⫽ –12 M.

(6.A.25)

The inequality (6.A.21) can be further simpliﬁed if one assumes that Mp(x) is negative semideﬁnite, that is, for any ˆ ,

冕 ␥(x)M (x)␥(x) d ⱕ 0. p

(6.A.26)

D

In this case, (6.A.21) reduces to 2D(U ⫺ Uh) ⱕ ⫺H[ˆ].

(6.A.27)

Therefore, we have the following theorem. Theorem 6.3a When Mp(x) is negative semideﬁnite, among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional minimum: Jch[ˆ] ⫽

1 1 ˜ Mh ⫺ H(ˆ), 2 2D

(6.A.28)

and the minimum value of Jch[ˆ] is the strain energy of the composite under the displacement boundary condition (6.3.1), that is, min{Jch[ˆ]} ⫽

1 M. 2D

(6.A.29)

This is another form of the Hashin–Shtrikman variational principle. The duals of the above theorems can be easily proven by using the minimum potential energy theorem; see Problem 6.7.

152

BOUNDS FOR EFFECTIVE MODULI

Theorem 6.4 Among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional maximum: J[ˆ] ⫽

1 1 ˜ 1 Mh ⫺ H(ˆ) ⫺ 2 2D 2D

冕 ␥(x)L (x)␥(x) dV(x), p

(6.A.30)

D

and the maximum value of J[ˆ] is the strain energy of the composite under the displacement boundary condition (6.3.1), that is, min{J[ˆ]} ⫽ –12 M.

(6.A.31)

The inequality (6.A.21) can be further simpliﬁed if one assumes that Mp(x) is negative semideﬁnite, that is, for any ˆ ,

冕 ␥(x)L (x)␥(x) d ⱕ 0. p

(6.A.32)

D

In this case, we have the following theorem. Theorem 6.4a When Mp(x) is negative semideﬁnite, among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional maximum: Jh[ˆ] ⫽

1 1 ˜ Mh ⫺ H(ˆ), 2 2D

(6.A.33)

and the maximum value of Jh[ˆ] is the strain energy of the composite under the displacement boundary condition (6.3.1), that is, min{Jh[ˆ]} ⫽ –12 M.

(6.A.34)

This is another form of the Hashin–Shtrikman variational principle.

REFERENCE Willis, J. R. (1982). Elasticity Theory of Composites, in Mechanics of Solids—The Rodney Hill 60th Anniversary Volume, H. G. Hopkins and M. J. Sewell, eds., Pergamon Press, Oxford. pp. 635–686.

SUGGESTED READING

153

SUGGESTED READING Hashin, Z. and S. Shtrikman. (1961). Note on a Variational Approach to the Theory of Composite Elastic Materials, J. Franklin Inst., Vol. 271, pp. 336– 341. Hashin, Z. and S. Shtrikman. (1963). A Variational Approach to the Theory of the Elastic Behavior of Multiphase Materials, J. Mech. Phys. Solids, Vol. 11, pp. 127–140. Mura, T. and T. Koya. (1992). Variational Methods in Mechanics, Oxford University Press, New York, Chapter 21. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York, Chapter 3, Section 9. Willis, J. R. (1977). Bounds and Self-Consistent Estimates for the Overall Properties of Anisotropic Composites, J. Mech. Phys. Solids, Vol. 25, pp. 185–202. Willis, J. R. (1981). Variational and Related Methods for the Overall Properties of Composites, Adv. Appl. Mech., Vol. 21, pp. 1–78.

7 DETERMINATION OF EFFECTIVE MODULI In this chapter, we develop several methods to evaluate approximately the effective properties of heterogeneous materials. All the approaches presented are based on the Eshelby single-inclusion solution. In the next chapter, we will present other methods of evaluating the effective properties that are based on multiple-inclusion approaches.

7.1 BASIC IDEAS OF MICROMECHANICS FOR EFFECTIVE PROPERTIES

Consider a heterogeneous material D consisting of a matrix phase ⍀0 and ellipsoidal inhomogeneities, ⍀1, ⍀2, . . . , ⍀N, as shown in Figure 7.1. The volume fraction of ⍀r is cr ⫽ ⍀r / ⍀. Clearly, one has

冘 c ⫽ 1. N

r

r⫽0

Let the stiffness tenor of ⍀r be Lr (r ⫽ 0, 1, . . . , N). Our objective is to determine the effective elastic modulus of the composite materials in terms of the stiffness tensors of the matrix and the inhomogeneities and their respective volume fractions. We learned from Section 5.7 that the effective elastic stiffness tensor can be easily computed once the local or the global concentration tensors are known. However, the exact expressions of the concentration tensors are rather difﬁcult to obtain. So, the various methods discussed in this chapter are aimed at obtaining approximate solutions to these concentration tensors. The multiphase composite shown in Figure 7.1 is a very general case. Most engineering composites are two-phase materials, namely, 154

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

7.1

BASIC IDEAS OF MICROMECHANICS FOR EFFECTIVE PROPERTIES

155

Ω3

Ω2 Ωr ΩN

Ω1 Ω0

Figure 7.1 Multiphase composite.

matrix phase and the reinforcement phase. The most common types of reinforcement phases are either particles (particulate-reinforced composites) or ﬁbers (ﬁber-reinforced composites). The results derived below for the multiphase composite can be easily speciﬁed to the case of two-phase composite by assuming that all the inhomogeneities are the same. The basic idea of micromechanics is to develop solutions of either the global or local concentration tensors. Once such concentration tensors are known, the effective properties can be easily obtained per the discussions in Section 5.7. One common approach of developing the concentration tensors is to use the Eshelby solution in conjunction with the equivalent inclusion method. To this end, we assume that the composite is subjected to either the displacement boundary condition u兩S ⫽ 0x

(7.1.1)

or the traction boundary condition • n兩S ⫽ 0n,

(7.1.2)

where 0 and 0 are constant second-order tensors and are related by 0 ⫽ L00.

If all the inhomogeneities are absent and the entire volume D is ﬁlled with the matrix material L0, or equivalently, L0 ⫽ L1 ⫽ L2 ⫽ ⫽

156

DETERMINATION OF EFFECTIVE MODULI

LN, it is obvious that the strain and stress ﬁeld would be 0 and 0, respectively, throughout the volume D; see Figure 7.2. In the actual composite, the inhomogeneities have distinctive properties from the matrix material. The strain and stress in the matrix will no longer be 0 and 0. For example, consider a typical inhomogeneity called the rth inhomogeneity; see Figure 7.3a. It is surrounded by the matrix material with elastic stiffness tensor L0. The strain in the matrix around the rth inhomogeneity is conceivably different from 0 for two reasons. First, the rth inhomogeneity itself perturbs the uniform distribution of strains in the matrix. Second, the other inhomogeneities, especially those near by, also contribute to the strain perturbation. Thus, as far as the rth inhomogeneity is concerned, it might be viewed as an isolated inhomogeneity placed in a uniform matrix that possessed certain strain before the inhomogeneity is embedded. For convenience, we will denote this strain by ˆ 0. Furthermore, it is also plausible that the inﬂuence of other inhomogeneities can be accounted for by assuming that the rth inhomogeneity is embedded in a matrix material that is somewhat different from the actual matrix. We will use Lˆ0 to denote the stiffness tensor of this ﬁctitious matrix material; see Figure 7.3b. Now the companion problem can be restated as follows. An ellipsoidal inhomogeneity ⍀r with stiffness tensor Lr is placed within a uniform matrix of stiffness tensor Lˆ0, which had been subjected to the uniform strain ˆ 0 before the inhomogeneity was embedded; see Figure 7.3b. Our objective is to ﬁnd proper values for ˆ 0 and Lˆ0 so that the stress (and strain) on ⍀r is the same as that occurring on the rth inhomogeneity the actual composite. To ﬁnd such ˆ 0 and Lˆ0, let us pretend at the moment that they are known. We will ﬁrst establish how the stresses and strains of the companion problem are related to ˆ 0 and Lˆ0. This can be done by solving the Eshelby inclusion problem. The stress and strain on the inhomogeneity can be obtained by the equivalent inclusion method discussed in Section 4.4. The equivalent inclusion equation in this case is

L0 0

0

Figure 7.2 Homogeneous material.

7.1

157

BASIC IDEAS OF MICROMECHANICS FOR EFFECTIVE PROPERTIES

V3

V2 Vr

Vr VN

= ˆ0

V1

Lˆ 0

V0

(a)

(b)

Figure 7.3 (a) The rth inhomogeneity in the composite; (b) The rth inhomogeneity in a uniform matrix of stiffness Lˆ 0, which had been subjected to the uniform strain ˆ 0 before the inhomogeneity was embedded.

ˆ 0 ⫹ pt Lr (ˆ0 ⫹ pt r ) ⫽ L0 (ˆ r ⫺ *), r

(7.1.3)

where, according to the Eshelby solution given in Section 4.3, ˆ pt r ⫽ Srr*,

(7.1.4)

where Sˆr is the Eshelby tensor computed using the elastic constants of Lˆ0 and the geometry of the rth inhomogeneity ⍀r. Substitution of the Eshelby solution into the equivalent inclusion equation yields the eigenstrain ˆ ˆ ˆ ⫺1 * 0. r ⫽ [(Lr ⫺ L0)Sr ⫹ L0] (Lr ⫺ L0)ˆ

(7.1.5)

The total strain in the rth inhomogeneity can then be written as r ⫽ ˆ 0 ⫹ pt ˆ 0 ⫹ Sˆ r* ⫽ Tˆ rˆ 0, r ⫽

(7.1.6)

Tˆ r ⫽ [I ⫹ Sˆ rLˆ 0⫺1(Lr ⫺ Lˆ 0)]⫺1.

(7.1.7)

where

The derivation of the last equality in (7.1.6) is similar to that of (4.4.15). The corresponding stress on the rth inhomogeneity is

158

DETERMINATION OF EFFECTIVE MODULI

ˆ rˆ 0. r ⫽ Lrr ⫽ LrT

(7.1.8)

We now have related the strain and stress ﬁelds in the rth inhomogeneity to an unknown strain ﬁeld ˆ 0 and a ﬁctitious matrix material with L ˆ 0. It will be seen later that the micromechanics schemes discussed below use various approximations to identify and compute ˆ 0 and Lˆ0. Once ˆ 0 and Lˆ0 are known, the concentration tensors can be obtained and so can the effective properties of the composite.

7.2 ESHELBY METHOD

If the inhomogeneities in the composite shown in Figure 7.1 are far apart from each other, their interactions may be neglected. In other words, each inhomogeneity can be treated as if it exists in a homogeneous matrix without the interference by other inhomogeneities. Therefore, a typical inhomogeneity, for example, the rth inhomogeneity, can be treated as an ellipsoidal inhomogeneity in an otherwise uniform matrix of stiffness L0, which was subjected to a uniform strain 0 before the inhomogeneity was imbedded. Therefore, we choose in (7.1.3), Lˆ 0 ⫽ L0 and ˆ 0 ⫽ 0

(7.2.1)

and consequently,

V3

V2 Vr

Vr

VN

=

V1 V0

(a)

0

L0

(b)

Figure 7.4 (a) The rth inhomogeneity in the composite. (b) The rth inhomogeneity in the original matrix of stiffness L0, which had been subjected to the uniform strain 0 before the inhomogeneity was embedded.

7.2

ESHELBY METHOD

Sˆ r ⫽ Sr,

159

(7.2.2)

where Sr is the Eshelby tensor computed using the matrix material property L0 and the geometry of the rth inhomogeneity ⍀r. These equations simply imply that other inhomogeneities have no inﬂuence on the rth inhomogeneity at all. So, the interactions between inhomogeneities are completely ignored. In this case, the strain in the rth inhomogeneity follows directly from (7.1.6): r ⫽ 0 ⫹ rpt ⫽ 0 ⫹ Sr* ⫽ Tr0,

(7.2.3)

Tr ⫽ [I ⫹ Sr L0⫺1(Lr ⫺ L0)]⫺1.

(7.2.4)

where

For future reference, we want to mention that although Tr is deﬁned for r ⬎ 0, it is nevertheless true that T0 ⫽ I as seen from (7.2.4). We now assume that the composite is subjected to the displacement boundary condition u兩S ⫽ 0 • x.

(7.2.5)

It follows from the average strain theorem discussed in Section 5.4 that the average strain tensor of the composite is equal to 0, that is, ⫽

1 V

冕 dV ⫽ . 0

(7.2.6)

V

Therefore, Eq. (7.2.3) can be rewritten as r ⫽ Tr.

(7.2.7)

By comparing (5.7.3) and (7.2.7), it is clear that the global strain concentration tensor for the rth inhomogeneity is Ar ⫽ Tr.

(7.2.8)

Thus, it follows from (5.7.7) that the effective stiffness tensor of the composite is given by

160

DETERMINATION OF EFFECTIVE MODULI

冘c (L ⫺ L )T ⫽ L ⫹ 冘 c (L ⫺ L )[I ⫹ S (M L ⫺ I)] N

L ⫽ L0 ⫹

r

r

0

r

r⫽1 N

0

r

r

0

r

0

r

⫺1

.

(7.2.9)

r⫽1

This is the Eshelby estimate of the effective stiffness tensor. Recall that this effective stiffness tensor was derived based on the assumption made earlier that the inhomogeneities in the composite are so far apart that they do not interfere with each other. Thus, the Eshelby estimate is valid only for very low volume fraction of inhomogeneities, or the dilute case. Instead of the displacement boundary conditions, a traction boundary condition • n兩S ⫽ 0n

(7.2.10)

can be prescribed. In this case, the average strain of the composite is no longer equal to 0, that is, ⫽

1 V

冕 dV ⫽ , 0

(7.2.11)

V

where 0 ⫽ M00.

(7.2.12)

Instead, we have, according to the average stress theorem discussed in Section 5.4, ⫽

1 V

冕 dV ⫽ . 0

(7.2.13)

V

Substituting (7.2.12) and (7.2.13) into (7.2.3) and making use of r ⫽ Lrr yield r ⫽ LrTr M0.

(7.2.14)

The global stress concentration tensor is thus given by Br ⫽ LrTr M0 ⫽ [Mr ⫺ Sr (Mr ⫺ M0)]⫺1 M0.

(7.2.15)

7.2

161

ESHELBY METHOD

It then follows from (5.7.8) that the effective compliant tensor of the composite is given by

冘 c (M ⫺ M )B ⫽ M ⫹ 冘 c (M ⫺ M )L T M . N

M ⫽ M0 ⫹

N

r

r

0

r

0

r

r

0

r

r

0

r⫽1

r⫽1

(7.2.16) It can be further simpliﬁed to

冘c [(L ⫺ L )S ⫹ L ] N

M ⫽ M0 ⫺

r

r

0

r

0

⫺1

(Lr ⫺ L0)M0.

(7.2.17)

r⫽1

This is the Eshelby estimate of the effective compliance of the composite in consideration. Finally, let us check the consistency of the Eshelby estimates by considering

冋

冘 册冋 冘c (L ⫺ L )T 册 ⫽ I ⫺ 冋 冘 c (I ⫺ M L )T 册冋 冘 c (I ⫺ M L )T 册 N

ML ⫽ M0 ⫹

N

cr (Mr ⫺ M0)LrTr M0

L0 ⫹

r

r

0

r

r⫽1

r⫽1

N

N

r

r⫽1

⫽ I ⫹ O(c2r ).

0

r

r

r

0

r

r

r⫽1

(7.2.18)

It is seen that ML ⫽ I only when the terms with order of c2r are neglected. In other words, the Eshelby estimates are consistent only up to the ﬁrst order of the volume fraction of the inhomogeneities. To close this section, we note that both the volume fraction and the geometry of the inhomogeneities are taken into consideration in the Eshelby estimate. However, the distribution of the inhomogeneities is neglected. More importantly, the interaction between the inhomogeneities is not taken into consideration because the eigenstrain in each inclusion is calculated by assuming that the other inclusions are not present. Therefore, this method is limited to low (dilute) concentration of inhomogeneities. The method is also called by some authors the dilute concentration method. Example 7.1 Consider a particulate-reinforced composite material. Assume that all particles are spherical and randomly dispersed throughout the matrix. Further, assume that both the particle and the matrix

162

DETERMINATION OF EFFECTIVE MODULI

are made of isotropic elastic materials. Their elastic stiffness tensors are L0 ⫽ (3K0, 20)

for the matrix,

(7.2.19)

for the particles,

(7.2.20)

and L1 ⫽ (3K1, 21)

where the matrix symbolic notation for the fourth-order tensors introduced in Section 1.4 has been used for the stiffness tensors. The isotropic elastic constants Kr and r are the bulk and shear moduli, respectively, for the matrix (r ⫽ 0) and the particles (r ⫽ 1). Finally, we assume that the volume fraction of the particles in the composite is c1. To ﬁnd the effective stiffness tensor of the composites, we can use (7.2.9) directly by specifying N ⫽ 1. To this end, let us compute the relevant tensors one at a time. First, the Eshelby tensor for an isotropic material with L0 ⫽ (3K0, 20) can be written as (see Appendix 4.B) S1 ⫽ (3␥0, 2␦0),

(7.2.21)

where ␥0 ⫽

K0 3K0 ⫹ 40

⫽

1 ⫹ v0 , 9(1 ⫺ v0)

␦0 ⫽

3(K0 ⫹ 20) 4 ⫺ 5v0 ⫽ . 5(3K0 ⫹ 40) 15(1 ⫺ v0) (7.2.22)

Next, let us compute the fourth-order tensor T1: ⫺1 T1 ⫽ [I ⫹ S1L⫺1 0 (L1 ⫺ L0)]

⫽ {(1,1) ⫹ (3␥0, 2␦0)[(3K0, 20)⫺1(3K1, 21) ⫺ (1,1)]}⫺1 ⫽

冋 冋 冋

冉

(1, 1) ⫹ (3␥0, 2␦0)

K1 ⫺ K0 1 ⫺ 0 , K0 0

冊册 册 册

K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␦0(1 ⫺ 0) ⫽ , K0 0 ⫽

⫺1

⫺1

K0 0 , . K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␦0(1 ⫺ 0)

(7.2.23)

7.3

163

MORI–TANAKA METHOD

Finally, L ⫽ L0 ⫹ c1 (L1 ⫺ L0)T1 ⫽ (3K0, 20) ⫹

冋

册

3c1K0 (K1 ⫺ K0) 2c10(1 ⫺ 0) , . K0 ⫹ 3␥0 (K1 ⫺ K0) 0 ⫹ 2␦0(1 ⫺ 0) (7.2.24)

Thus, we have K ⫽ K0 ⫹

c1K0 (K1 ⫺ K0) , K0 ⫹ 3␥0 (K1 ⫺ K0)

⫽ 0 ⫹

c10 (1 ⫺ 0) . 0 ⫹ 2␦0(1 ⫺ 0)

(7.2.25)

Making use of (7.2.22) in (7.2.25) yields alternative expressions c (K ⫺ K0)(3K0 ⫹ 40) K ⫽ K0 ⫹ 1 1 , 3K1 ⫹ 40 ⫽ 0 ⫹

(7.2.26)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 3K0(30 ⫹ 21) ⫹ 40 (20 ⫹ 31)

(7.2.27)

This completes the solution. Note that in the above derivations, we have used the symbolic notations of fourth-order isotropic tensors and followed the rules of operation on using such symbolic notations, as introduced in Section 1.4. The advantages of such operation are clearly seen.

7.3 MORI–TANAKA METHOD

Before presenting the Mori–Tanaka method, let us recall the average strain and average stress of a composite as deﬁned in Section 5.4: ⫽

where

1 D

冕 dV ⫽ 冘 , N

D

r

r⫽0

⫽

1 D

冕 dV ⫽ 冘 , N

D

r

r⫽0

(7.3.1)

164

DETERMINATION OF EFFECTIVE MODULI

r ⫽

冕 ⍀ 1

r

⍀r

dV

and r ⫽

1 ⍀r

冕

⍀r

dV

(7.3.2)

are the strain and stress tensors, respectively, averaged over the rth inhomogeneity. For example, 1 is the average strain in the inhomogeneity with stiffness tensor L1, and 0 is the average strain in the matrix phase, see Fig. 7.5. Furthermore, r ⫽ Lrr.

Now consider the composite material shown in Figure 7.1. For a typical inhomogeneity Lr (r ⬎ 0) in the composite, the effects (or the existence) of other inhomogeneities are communicated to it through the strain and stress ﬁelds in its surrounding matrix material. Although the strain and stress ﬁelds are different from one location to another in the matrix, the averages (0 and 0) represent good approximations of the actual ﬁelds in the matrix surrounding each inhomogeneity, when a large number of inhomogeneities exit and are randomly distributed in the matrix (which is the case for most engineering composites). Also, it would be reasonable to assume that taking only one inhomogeneity out will not affect the overall elastic behavior of the composite. In other words, when the rth inhomogeneity is removed and replaced by the matrix material (or equivalently, let Lr ⫽ L0), the averages (0 and 0) will remain the same. Therefore, as far as the rth inhomogeneity is concerned, it can be viewed as an ellipsoidal inhomogeneity with stiffness tensor Lr placed within a uniform matrix of stiffness tensor

0

V0

Figure 7.5 Average strain in matrix.

7.3

165

MORI–TANAKA METHOD

L0, which had been subjected to the uniform strain 0 before the inhomogeneity was embedded, see Fig. 7.6. Thus, we choose in (7.1.3), Lˆ 0 ⫽ L0 and ˆ 0 ⫽ 0

(7.3.3)

Sˆ r ⫽ Sr.

(7.3.4)

and consequently

Comparing these with (7.2.1) and (7.2.2), it is seen that the only difference between the Eshelby and the Mori–Tanaka methods is the use of ˆ 0. Note that ˆ 0 represents how the effects of other inhomogeneities are accounted for. Because the Eshelby method assumes no interaction between the inhomogeneities, it takes ˆ 0 ⫽ 0, which is the strain in the matrix when none of the inhomogeneities is present. The Mori–Tanaka method also assumes the absence of all inhomogeneities, but it includes certain effects of the inhomogeneity by taking ˆ 0 ⫽ 0, because 0 is the average strain in the matrix phase when all inhomogeneities are present. For this reason, the Mori–Tanaka method provides better estimate of the effective modulus than the Eshelby method does for composite with nondilute reinforcement phases.

Vr

Vr

=

0

0

V0

(a)

L0

(b)

Figure 7.6 (a) The rth inhomogeneity in the composite. (b) The rth inhomogeneity in the original matrix of stiffness L0, which had been subjected to the uniform strain 0 before the inhomogeneity was embedded.

166

DETERMINATION OF EFFECTIVE MODULI

The use of (7.3.3) and (7.3.4) in (7.1.6) yields the strain in the rth inhomogeneity r ⫽ 0 ⫹ rpt ⫽ 0 ⫹ Sr* r ⫽ Tr0,

(7.3.5)

where Tr is the same as that of (7.2.4). Although (7.2.7) and (7.3.5) have similar appearance, they are very different equations in that (7.2.7) relates the total strain on the inhomogeneity to the average strain over the entire composite, while (7.3.5) relates the total strain on the inhomogeneity to the average strain on the matrix surrounding the inhomogeneity. Therefore, the tensor Tr in (7.2.7) represents the global strain concentration, while the tensor Tr in (7.3.5) represents local strain concentration tensor introduced in (5.7.9), that is, Gr ⫽ Tr.

(7.3.6)

Thus, it follows from (5.7.14) that the global strain concentration tensor is

冋

冘cG册

Ar ⫽ Gr c0I ⫹

冋冘 册

⫺1

N

n

⫺1

N

⫽ Tr

n

cnTn

,

(7.3.7)

n⫽0

n⫽1

where the fact that T0 ⫽ I has been used. Consequently, the effective stiffness tensor of the composite follows directly from (5.7.7):

冘 c (L ⫺ L )A ⫽ L ⫹ 冘 c (L ⫺ L )T 冋 冘 c T 册 ⫽ L ⫹ 冘 c L T 冋冘 c T 册 ⫺ L 冘 c T 冋冘 c T 册 ⫽ 冘 c L T 冋冘 c T 册 (7.3.8) N

L ⫽ L0 ⫹

r

r

0

r

r⫽1 N

0

r

r

0

r

n

N

r

r

r

n

N

n

N

r

r⫽0

r

n

n

n⫽0

⫺1

N

r

⫺1

N

0

n⫽0

r⫽0

r

⫺1

N

0

r

n

n⫽0

r⫽0

r⫽0

⫺1

N

n

n

n⫽0

or

冘 c L T 冋冘 c T 册 N

L⫽

r

r⫽0

⫺1

N

r

r

n

n

.

(7.3.9)

n⫽0

This is the Mori–Tanaka estimate of the effective stiffness tensor.

7.3

MORI–TANAKA METHOD

167

To obtain the Mori–Tanaka estimate of the effective complaint tensor, we substitute 0 ⫽ M00,

r ⫽ Lrr

(7.3.10)

into (7.3.5), which yields r ⫽ LrTr M00.

(7.3.11)

The local stress concentration tensor is thus given by Hr ⫽ LrTr M0.

(7.3.12)

It then follows from (5.7.15) that the global stress concentration tensor is given by

冋

冘cH册

⫺1

N

Br ⫽ Hr c0I ⫹

n

n

n⫽1

冋冘 c L T M 册

⫺1

N

⫽ LrTr M0

n

n

n

,

0

(7.3.13)

n⫽0

where the fact that H0 ⫽ L0T0M0 ⫽ I has been used. The Mori–Tanaka effective compliant tensor thus follows from (5.7.8):

冘 c (M ⫺ M )B ⫽ M ⫹ 冘 c (M ⫺ M )L T M 冋 冘 c L T M 册 ⫽ M ⫹ 冘 c T M 冋冘 c L T M 册 ⫺ M 冘 c L T M 冋冘 c L T M 册 ⫽ 冘 c T M 冋冘 c L T M 册 ⫽ 冘 c T 冋冘 c L T 册 N

M ⫽ M0 ⫹

r

r

0

r

r⫽1 N

0

r

r

0

r

r

0

n

N

r

r

0

n

N

n

n

0

⫺1

N

0

r

r

r

0

n

n

n

0

n⫽0

r⫽0

N

⫺1

N

0

n

n

n

0

n⫽0

r⫽0 N

⫺1

N

r

or

0

n⫽0

r⫽0

r⫽0

n

⫺1

N

0

r

n

n⫽0

r⫽0

r

⫺1

N

r

n

n⫽0

n

n

(7.3.14)

168

DETERMINATION OF EFFECTIVE MODULI

冘 N

M⫽

r⫽0

冋冘

册

⫺1

N

crTr

cnLnTn

n⫽0

.

(7.3.15)

This is the Mori–Tanaka estimate of the effective compliance tensor of the composite in consideration. It is easy to see from (7.3.9) and (7.3.15) that, unlike in the Eshelby method, the Mori–Tanaka method yields ML ⫽ LM ⫽ I for any cr. Example 7.2 Let us use the Mori–Tanaka method to estimate the effective elastic tensor and the effective compliant tensor for the composite considered in Example 7.1. First, consider (7.3.9) for r ⫽ 1, L ⫽ (c0L0T0 ⫹ c1L1T1)(c0T0 ⫹ c1T1)⫺1 ⫽ (c0L0 ⫹ c1L1T1)(c0I ⫹ c1T1)⫺1,

(7.3.16)

T1 ⫽ [I ⫹ S1 (M0L1 ⫺ I)]⫺1.

(7.3.17)

where

By substituting (7.3.17) into (7.3.16) and making use of (7.2.19)– (7.2.22), we obtain using the symbolic notation, L ⫽ (3K, 2),

(7.3.18)

where K ⫽ K0 ⫹

c1K0(K1 ⫺ K0) , K0 ⫹ 3␥0(1 ⫺ c1)(K1 ⫺ K0)

(7.3.19)

⫽ 0 ⫹

c10(1 ⫺ 0) . 0 ⫹ 2␦0(1 ⫺ c1)(1 ⫺ 0)

(7.3.20)

Eliminating ␥0 and ␦0 by using (7.2.22), we can rewrite (7.3.20) as K ⫽ K0 ⫹ ⫽ 0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(7.3.21)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 50(3K0 ⫹ 40) ⫹ 6(1 ⫺ c1)(1 ⫺ 0)(K0 ⫹ 20) (7.3.22)

7.4

SELF-CONSISTENT METHODS FOR COMPOSITE MATERIALS

169

These are the Mori–Tanaka estimates of the effective elastic constants for a composite with spherical particles.

7.4 SELF-CONSISTENT METHODS FOR COMPOSITE MATERIALS

Again, consider the composite material stated in Section 7.1. Let us pretend at this point that we already knew the effective stiffness tensor L and its inverse M. Since there are numerous inhomogeneities in the composite, we know that the effective properties (L and M) will not be affected if one inhomogeneity is removed from the composite. Now, focus our attention to a typical inhomogeneity, for example, the rth inhomogeneity. When the composite is subjected to either the displacement boundary condition or the traction boundary condition, one may envision that the effects of the applied loads (through the boundary condition) and the interaction with other inhomogeneity can be accounted for by assuming that the rth inhomogeneity is placed within a homogeneous matrix of stiffness L that had been subjected to the strain tensor before the inhomogeneity is embedded; see Figure 7.7. With this understanding, we can choose in (7.1.3),

V3

V2 Vr

Vr

VN

=

V1

L

V0

(a)

(b)

Figure 7.7 (a) The rth inhomogeneity in the actual composite. (b) The rth inhomogeneity in a homogeneous matrix with (as-yet-unknown) effective stiffness L that has been subjected to the uniform strain before the inhomogeneity was embedded.

170

DETERMINATION OF EFFECTIVE MODULI

Lˆ 0 ⫽ L and ˆ 0 ⫽ ,

(7.4.1)

Sˆ r ⫽ Sr,

(7.4.2)

and consequently,

where the overbar on the Eshelby tensor indicates that its elements should be computed based on the effective elastic constants of the composite. Substituting (7.4.1) and (7.4.2) into (7.1.6) yields the total strain in the rth inhomogeneity: r ⫽ ⫹ pt r ⫽ ⫹ S* r ⫽ Tr,

(7.4.3)

Tr ⫽ [I ⫽ SrL⫺1(Lr ⫺ L)]⫺1.

(7.4.4)

where

The corresponding stress on the rth inhomogeneity is r ⫽ Lrr ⫽ LrTr ⫽ LrTr M.

(7.4.5)

It is seen that the global strain and stress concentration tensors for the rth inhomogeneity are, respectively, Ar ⫽ Tr and Br ⫽ LrTr M.

(7.4.6)

Thus, it follows from (5.7.7) and (5.7.8) that the effective stiffness and compliant tensors of the composite are given, respectively, by

冘 c (L ⫺ L )T ,

(7.4.7)

冘 c (M ⫺ M )L T M,

(7.4.8)

N

L ⫽ L0 ⫹

r

r

0

r

r⫽1 N

M ⫽ M0 ⫹

r

r

0

r

r

r⫽1

where Tr is given in (7.4.4). These are the self-consistent estimates of the effective stiffness and compliant tensors of the composite. Unlike the Eshelby and Mori–Tanaka methods, the self-consistent method

7.4

SELF-CONSISTENT METHODS FOR COMPOSITE MATERIALS

171

yields implicit equations for the effective properties. Solutions to these implicit equations typically require numerical iterations using computers. To prove the consistency of the self-consistent estimates, let us consider (7.4.7). Premultiplying by M0 and postmultiplying by L⫺1, we arrive at

冘 c M (L ⫺ L )T L ⫹ 冘 c (M ⫺ M )L T L N

M0 ⫽ L⫺1 ⫹

r

0

r

0

r

⫺1

r⫽1 N

⫺1

⫽L

r

0

r

r

r

⫺1

.

(7.4.9)

r⫽1

By rearranging the terms, we obtain

冘 c (M ⫺ M )L T L N

⫺1

L

⫽ M0 ⫹

r

r

0

r

r

⫺1

.

(7.4.10)

r⫽1

Comparing (7.4.10) with (7.4.8), we observe that M ⫽ L⫺1.

(7.4.11)

L ⫽ M⫺1.

(7.4.12)

Similarly, one can show that

Thus, we have ML ⫽ LM ⫽ I, that is, the self-consistent estimates are indeed consistent. Example 7.3 Consider again the composite described in Example 7.1. To ﬁnd the effective stiffness tensor of the composites using the selfconsistent method, we can use (7.4.7) directly by specifying N ⫽ 1. To this end, let us compute the relevant tensors one at a time. First, the Eshelby tensor for an isotropic material with L ⫽ (3K,2) can be written as (see Appendix 4.B) S ⫽ (3␥, 2␦), where

(7.4.13)

172

␥⫽

DETERMINATION OF EFFECTIVE MODULI

K 3K ⫹ 4

⫽

1⫹ 3K ⫹ 6 4 ⫺ 5 , ␦⫽ ⫽ . 9(1 ⫺ ) 15K ⫹ 20 15(1 ⫺ )

(7.4.14)

Next, let us compute the fourth-order tensor T1, T1 ⫽ [I ⫹ S(L⫺1L1 ⫺ I)]⫺1 ⫽ {(1,1) ⫹ (3␥, 2␦)[(3K, 2)⫺1(3K1, 21) ⫺ (1,1)]}⫺1

冋 冋 冋

冉

冊册 册 册

⫺1

K ⫺ K 1 ⫺ ⫽ (1,1) ⫹ (3␥, 2␦) 1 , K

K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ ) ⫽ , K ⫽

⫺1

K , . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ )

(7.4.15)

Finally L ⫽ L0 ⫹ c1 (L1 ⫺ L0)T1 ⫽ (3K0, 20) ⫹ c1 ⫽

冋

3K0 ⫹

冋

册

3K(K1 ⫺ K0) 2(1 ⫺ 0) , K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ )

册

3c1K(K1 ⫺ K0) 2c1(1 ⫺ 0) , 20 ⫹ . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ ) (7.4.16)

Thus, we have K ⫽ K0 ⫹

c1K(K1 ⫺ K0) c (1 ⫺ 0) , ⫽ 0 ⫹ 1 . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ )

(7.4.17)

This is a pair of nonlinear algebraic equations. The roots of these equations are the effective elastic constants of the composite. Because of the uniqueness of the problem, selections must be made judiciously based on physical ground if there are multiple roots. A common method to ﬁnd the roots is iteration. Making use of (7.4.14) in (7.4.17) yields a pair of alternative expressions:

7.5

SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

c1(K1 ⫺ K0)(3K ⫹ 4) , 3K1 ⫹ 4

(7.4.18)

5c1(1 ⫺ 0)(3K ⫹ 4) . 3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)

(7.4.19)

K ⫽ K0 ⫹ ⫽ 0 ⫹

173

7.5 SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

The derivations used to develop the methods of determining the effective properties described in previous sections including the selfconsistent method rely on the fact that the composite has a distinct matrix in which other inhomogeneities are embedded. For certain heterogeneous materials, such as polycrystalline materials, there is no distinct matrix phase. In a polycrystal, each grain can be viewed as an inhomogeneity embedded in the remaining grains, and, hence, all grains have the same signiﬁcance. Clearly, there is a complete symmetry in treating each grain as an inhomogeneity. The concept of a matrix with embedded inhomogeneities is thus no longer meaningful. In this section, we will describe other self-consistent methods that treat all inhomogeneities (one may consider the matrix as one of the inhomogeneities) on an equal footing. To begin, let us consider a polycrystalline material comprising N randomly distributed grains. The different grains can be either different materials (in the case of alloys) or grains with different crystallographic orientations (in the case of single-element polycrystals). We assume that the rth grain has volume fraction of cr, r ⫽ 1, 2, 3, . . . , N. It then follows from (5.4.1) that the average strain and average stress in the polycrystal is given by

冘 c, N

⫽

r r

r⫽1

冘 c, N

⫽

r

r

(7.5.1)

r⫽1

where r and r are the average strain and stress tensors, respectively, on the rth grain. Note that is the average strain of the entire polycrystal and r is the average strain of the rth grain. The global strain concentration tensor Ar is deﬁned for the rth grain through (5.7.3):

174

DETERMINATION OF EFFECTIVE MODULI

r ⫽ Ar.

(7.5.2)

Similarly, the global stress concentration tensor is deﬁned for the rth grain through (5.7.9): r ⫽ Br.

(7.5.3)

It then follows from (7.5.2) and (7.5.3) and the use of Hooke’s law that

冘

冘 c L A ,

(7.5.4)

冘 c ⫽ 冘 c M ⫽ 冘 c M B .

(7.5.5)

N

⫽

N

cr Lrr ⫽

r⫽1

r⫽1

N

⫽

冘 N

crr ⫽

N

r r

r

r

N

r

r

r

r⫽1

r⫽1

r

r⫽1

r

r

r

r⫽1

These lead to

冘 N

L⫽

r⫽1

冘 c MB. N

cr LrAr,

M⫽

r

r

r

(7.5.6)

r⫽1

Clearly, once the strain concentration tensor Ar is known as a function of the effective stiffness tensor L for the polycrystal, the ﬁrst of (7.5.6) can be used to obtain the effective stiffness tensor L. Similarly, if the stress concentration tensor Br is known as a function of the effective compliance tensor M, the second of (7.5.6) can be used to obtain the effective compliance tensor M. Generally speaking, the effective compliance and stiffness tensor obtained from these two equations may not be consistent, unless the exact expressions of Ar and Br are used. One way to obtain an approximate solution to Ar is to view each grain as an ellipsoidal inhomogeneity embedded in a homogeneous matrix (consisting of all the other grains) of elastic stiffness tensor L. Under this assumption, when the polycrystal is subjected to displacement boundary condition u兩x僆S ⫽ x, the strain concentration tensor Ar is given by (7.2.4) and (7.2.7) with M0 and L0 replaced by M and L, respectively, because in this case the rth inhomogeneity is embedded in a homogeneous matrix with L, instead of L0, Ar ⫽ [I ⫹ Sr M(Lr ⫺ L]⫺1,

(7.5.7)

7.5

SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

175

where Sr is the Eshelby tensor computed based on L. Substituting (7.5.7) into the ﬁrst of (7.5.6) results in a self-consistent scheme for L:

冘 c L [I ⫹ S L N

L⫽

r

r

⫺1

r

(Lr ⫺ L)]⫺1.

(7.5.8)

r⫽1

To obtain an approximate solution to Br, let us consider the traction boundary condition (7.2.10). In this case, it follows from (7.2.15) that Br ⫽ [Mr ⫺ Sr(Mr ⫺ M)]⫺1 M.

(7.5.9)

Substituting (7.5.9) into the second of (7.5.6) yields a self-consistent scheme for M,

冘 c M [M ⫺ S (M ⫺ M)] N

I⫽

r

r

r

r

r

⫺1

.

(7.5.10)

r⫽1

It can be shown (see Problem 7.8) that the concentration tensors can be written in alternative forms: Ar ⫽ (Lr ⫹ Hr)⫺1(L ⫹ Hr),

⫺1 ⫺1 Br ⫽ (Mr ⫹ H⫺1 r ) (M ⫹ Hr ),

(7.5.11) where Hr ⫽ L(S⫺1 ⫺ I) r

(7.5.12)

is the Hill’s constraint tensor (4.5.13). Thus, the self-consistent schemes can be recast into more symmetric forms:

冘 c L (L ⫹ H ) N

L⫽

r

r

r

r

⫺1

(L ⫹ Hr),

(7.5.13)

r⫽1

冘 c M (M ⫹ H N

M⫽

r

r⫽1

r

r

⫺1 ⫺1 r

) (M ⫹ Hr⫺1).

(7.5.14)

176

DETERMINATION OF EFFECTIVE MODULI

These are implicit algebraic equations for the effective stiffness tensor L. Solutions to these algebraic equations are the effective properties of the polycrystal. Making use of the relationships (see Problem 7.9) LrAr ⫽ BrL,

MrBr ⫽ Ar M,

one can easily show that the stiffness and compliance tensors predicted from (7.5.13) and (7.5.14), respectively, are indeed consistent, that is, LM ⫽ ML ⫽ I. Let us now consider a single-phase polycrystalline material. Singlephase polycrystal is an assembly of grains, all of which are comprised of the same material. Although all the grains are of the same material, their physical orientations are different. By physical orientation we mean rotations of the grain with respect to a ﬁxed reference frame, or equivalently, the rotation of the stiffness tensor with respect to a ﬁxed coordinate system. For example, let L be the elastic stiffness tensor of a single crystal in a ﬁxed coordinate system (x1, x2, x3). Then, the stiffness tensor of the same crystal in a different orientation can be represented by a rotation of L, that is, L(r) ijkl ⫽ ␣ip␣jq␣kr␣lsLpqrs,

(7.5.15)

where the rotation matrix can be expressed, for example, in terms of the Euler angles , , and : ␣11 ⫽ cos cos cos ⫺ sin sin , ␣12 ⫽ ⫺cos cos sin ⫺ sin cos , ␣13 ⫽ sin cos , ␣21 ⫽ cos sin cos ⫹ cos sin , ␣22 ⫽ ⫺cos sin sin ⫹ cos cos , ␣13 ⫽ sin sin , ␣31 ⫽ ⫺sin cos , ␣32 ⫽ sin sin , ␣32 ⫽ cos ,

where

(7.5.16)

7.5

SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

0 ⱕ ⱕ 2,

0 ⱕ ⱕ ,

0 ⱕ ⱕ 2.

177

(7.5.17)

Since all the grains are comprised of the same material, only with different orientations, we can write, symbolically, that, ˜ Lr ⫽ L(L, , , ),

˜ Mr ⫽ M(M, , , ).

(7.5.18)

To characterize the physical orientation of the grains in a given single-phase polycrystal, we use a distribution function ƒ(, , ), that is, 1 8 2

冕

2

0

d

冕

0

sin d

冕

2

0

ƒ(, , ) d ⫽ 1.

(7.5.19)

The value ƒ(0, 0, 0) represents the percent of grains that are all oriented in the direction (0, 0, 0). Clearly, ƒ(, , ) ⫽ ␦( ⫺ 0)␦( ⫺ 0)␦( ⫺ 0) would mean all the grains are orientated in the (0, 0, 0) direction. In addition to physical orientation, each grain (ellipsoidal inhomogeneity) in the polycrystal has its own size, shape, and orientation, all of which may not be the same for all grains. Since these geometric attributes come into the self-consistent equations through only the Eshelby tensor, which is independent of the size of the inhomogeneity, one may conclude that the effective stiffness tensor predicted by the selfconsistent methods (7.5.13) and (7.5.14) is invariant to the grain size. Because of the large number of grains involved, distribution functions are typically used to characterize the geometric shapes and orientations of grains. For example, we can use the Euler angles to indicate the geometric orientation of a grain, so that S(r) ijkl ⫽ ␣ip␣jq␣kr␣lsSpqrs,

(7.5.20)

where Spqrs is the Eshelby tensor for an ellipsoidal inclusion written in the same ﬁxed coordinate system (x1, x2, x3). For convenience, one may choose the ellipsoidal inclusion in such a way that its major axes coincide with the axes of the rectangular coordinate system. Therefore, if all grains have similar shape, the Eshelby tensor for each grain can be written as

178

DETERMINATION OF EFFECTIVE MODULI

˜ Sr ⫽ S(L, , , ),

(7.5.21)

where (, , ) follows a distribution function g(, , ). Replacing the summation by integration and the volume fraction by the distribution function, we can change the self-consistent equations (7.5.13) and (7.5.14) to their integral counterparts that are more suited for polycrystalline materials: ˜ ⫺1 ˜ ˜ ⫹ SL 具g具ƒL[I (L ⫺ L)]⫺1典典 ⫽ L,

(7.5.22)

˜ ˜ ˜ ˜ ⫺ S(M ⫺ M)]⫺1典典 ⫽ I, 具g具ƒM[M

(7.5.23)

where the symbol 具 典 ⫽ is deﬁned as 具典⬅

冕

2

0

d

冕

0

sin d

冕

2

0

d.

(7.5.24)

Let us, for brevity, use only (7.5.22) to consider some special cases: 1. Both geometric and physical orientations are random. In this case, ƒ(, , ) ⫽ g(, , ) ⫽ 1. Thus, (7.5.22) reduces to ˜ ⫺1 ˜ ˜ [I ⫹ SL 具具L (L ⫺ L)]⫺1典典 ⫽ L.

(7.5.25)

2. Both geometric and physical orientations are aligned. In this case, ƒ(, , ) ⫽ g(, , ) ⫽ ␦()␦()␦(). Thus, (7.5.22) reduces to ˜ L(L, 0, 0, 0)[I ˜ ˜ ⫹ S(L, 0, 0, 0)M(L(L, 0, 0, 0) ⫺ L)]⫺1 ⫽ L. (7.5.26)

It can be easily seen from (7.5.20) and (7.5.15) that ˜ S(L, 0, 0, 0) ⫽ S,

˜ L(L, 0, 0, 0) ⫽ L.

(7.5.27)

Thus, we have L[I ⫹ SM(L ⫺ L)]⫺1 ⫽ L. Equivalently, this leads to

(7.5.28)

7.6

L ⫽ L,

DIFFERENTIAL SCHEMES

179

(7.5.29)

that is, the effective stiffness tensor is the stiffness tensor of the single crystal. This is certainly expected since all the grains are aligned both geometrically and physically. In other words, the polycrystal in this case is actually a single crystal!

7.6 DIFFERENTIAL SCHEMES

The differential scheme in determining the effective modulus of a composite takes a somewhat different approach from the methods introduced in previous sections. The differential approach was motivated by the fact that the effective properties of a dilute composite can be calculated with relatively high accuracy. Therefore, one may imagine that a composite with a ﬁnite concentration of inhomogeneities can be constructed through the following process. First, start with the homogeneous matrix material with elastic stiffness tensor L0. Then, add a small amount (volume fraction ⌬c) inhomogeneities with elastic stiffness tensor L1. We now have a composite with dilute concentration. The effective elastic stiffness tensor L(1)(⌬c, L0) can be obtained accurately, where the fact that the effective stiffness tensor depends on the volume fraction of the inhomogeneities and the matrix material is explicitly indicated. In the next step, we will start with a homogenous matrix of elastic stiffness tensor L(1)(⌬c, L0). Then add a small amount (volume fraction ⌬c) of inhomogeneities of stiffness tensor L1. Again, we have created a new composite. As far as this composite is concerned, it still has a dilute concentration of L1. Therefore, the effective stiffness tensor of this new composite can be obtained accurately using the same method used for the previous step. The only difference here is that the matrix material in the current step is L(1)(⌬c, L0). Therefore, one can symbolically write the effective stiffness tensor at the current step as L(2)(⌬c, L(1)). This process can continue. Each time, the newly obtained composite will be viewed as a homogeneous matrix, and a small amount of inhomogeneities of L1 is added to obtain the next composite, until the desired volume fraction is achieved. Such a repetitive process leads to differential equations for the effective properties as functions of the concentrations (or volume fractions of the inhomogeneities). This is the basic idea of all the differential schemes. To illustrate how such thought process can be translated into differential equations, let us consider a two-phase composite (N ⫽ 1). Ac-

180

DETERMINATION OF EFFECTIVE MODULI

cording to (5.7.7), the effective stiffness tensor of a two-phase composite can be written as L(c1) ⫽ L0 ⫹ c1 (L1 ⫺ L0)⬊A1(L0),

(7.6.1)

where the dependence of L on the volume fraction c1 and A1 on L0 is explicitly indicated, and the strain concentration tensor A1 is deﬁned by 1 ⫽ A1 (L0)⬊.

(7.6.2)

In the above, the symbol ⬊ has been used to indicate the tensor product. This is to make it clear that A1 (L0) means A1 is a function of L0. Let us assume that the effective stiffness tensor L(c1) is known at a volume fraction c1 ⫽

⍀1 , ⍀0 ⫹ ⍀1

(7.6.3)

where ⍀0 and ⍀1 are, respectively, the volumes of the matrix and inhomogeneities. If the composite with stiffness tensor L(c1) is viewed as a homogeneous ‘‘matrix,’’ a new composite can be made by adding ⌬⍀1 amount of new inhomogeneities to the ‘‘matrix.’’ The volume fraction of the newly added inhomogeneities is ⌬⍀1 . ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1

(7.6.4)

For such small-volume fractions, the effective elastic stiffness tensor can be obtained from (7.6.1) by replacing L0 by the new matrix property L(c1), that is, L(c1 ⫹ ⌬c1) ⫽ L(c1) ⫹

⌬⍀1 (L ⫺ L(c1))⬊A1(L(c1)), ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1 1

(7.6.5) where ⌬c is the increment of the volume fraction of L1 in the composite due to the addition of ⌬⍀1 amount of L1. Clearly, the total volume fraction of L1 in this newly constructed composite is

7.6

c1 ⫹ ⌬c1 ⫽

181

DIFFERENTIAL SCHEMES

⍀1 ⫹ ⌬⍀1 . ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1

(7.6.6)

Subtracting (7.6.3) from (7.6.6) yields ⌬c1 ⫽

⍀0⌬⍀1 (⍀0 ⫹ ⍀1)(⍀0 ⫹ ⍀1 ⫹ ⌬⍀1)

⫽

(⍀0 ⫹ ⍀1 ⫺ ⍀1)⌬⍀1 (⍀0 ⫹ ⍀1)(⍀0 ⫹ ⍀1 ⫹ ⌬⍀1)

⫽

(1 ⫺ c1)⌬⍀1 ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1

(7.6.7)

or ⌬⍀1 ⌬c1 ⫽ . ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1 (1 ⫺ c1)

(7.6.8)

Substitution of (7.6.8) into (7.6.5) yield L(c1 ⫹ ⌬c1) ⫺ L(c1) 1 ⫽ (L ⫺ L(c1))⬊A1(L(c1)). ⌬c1 1 ⫺ c1 1

(7.6.9)

In the limit of ⌬c1 → 0, a ﬁrst-order differential equation is derived: dL(c1) 1 ⫽ (L ⫺ L(c1))⬊A1(L(c1)). dc1 (1 ⫺ c1) 1

(7.6.10)

The initial condition to compliment the differential equation is obviously L(c1)兩c1⫽0 ⫽ L0.

(7.6.11)

It is straightforward to derive the dual of (7.6.10) and (7.6.11), dM(c1) 1 ⫽ (M1 ⫺ M(c1))⬊B1(M(c1)), dc1 (1 ⫺ c1)

(7.6.12)

M(c1)兩c1⫽0 ⫽ M0,

(7.6.13)

182

DETERMINATION OF EFFECTIVE MODULI

where B1 is the stress concentration tensor deﬁned by (5.7.8). These initial value problems are the starting point for the various differential schemes, depending on how the strain concentration tensors A1 and B1 are computed. Let us consider ﬁrst the Eshelby approach discussed in Section 7.2. It follows from (7.2.8) and (7.2.4) that A1(L(c1)) ⫽ T1兩L0⫽L(c1) ⫽ [I ⫹ S1(L⫺1L1 ⫺ I)]⫺1,

(7.6.14)

where L⫺1 ⫽ S1 ⫽ (3␥, 2␦) ⫽

冉

冉

冊

1 1 , , 3K 2

(7.6.15)

冊

3(K ⫹ 2) , . 3K ⫹ 4 5(3K ⫹ 4) K

(7.6.16)

Note that it goes without saying that all the quantities with an overbar are functions of the volume fraction c. Substituting the above into (7.6.10) and (7.6.11) yields dL 1 ⫽ (L ⫺ L)[I ⫹ S1(L⫺1L1 ⫺ I)]⫺1, dc1 1 ⫺ c1 1

(7.6.17)

L(0) ⫽ L0.

(7.6.18)

For the composite described in Example 7.2, we have T1兩L0⫽L(c) ⫽ [I ⫹ S1(L⫺1L1 ⫺ I)]⫺1 K ⫽ , . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺

冉

冊

(7.6.19)

Making use of the above in (7.6.17), we have dK (K ⫺ K1)(3K ⫹ 4) ⫹ ⫽ 0, dc (1 ⫺ c)(3K1 ⫹ 4) d 5( ⫺ 1)(3K ⫹ 4) ⫹ ⫽ 0. dc (1 ⫺ c)[3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)] The solution must satisfy the initial conditions

(7.6.20)

(7.6.21)

7.7

COMPARISON OF DIFFERENT METHODS

K(0) ⫽ K0 and (0) ⫽ 0.

183

(7.6.22)

Clearly, this is a set of highly nonlinear ordinary differential equations. Numerical procedures are typically required to obtain the solution. Another version of the differential scheme is attained by following the Mori–Tanaka approach in obtaining the strain concentration tensor. It follows from (7.3.7) that A1(L(c1)) ⫽ T1[(1 ⫺ c1)I ⫹ c1T1]⫺1兩L0⫽L(c1). The differential equation now becomes dL 1 ⫽ (L ⫺ L)T1[(1 ⫺ c1)I ⫹ c1T1]⫺1兩L0⫽L(c1). dc1 1 ⫺ c1 1

(7.6.23)

7.7 COMPARISON OF DIFFERENT METHODS

In the previous sections, we have introduced several methods of estimating the effective stiffness (compliance) tensors for a given composite, namely, the Eshelby method (or the dilute concentration method), the Mori–Tanaka method, the self-consistent method, and the differential method. In this section, we will use these methods to obtain the effective moduli of several idealized composite materials where explicit analytical solutions can be obtained. We will compare the results to assess the validity and accuracy of these methods. We ﬁrst state that, based on the assumptions made in deriving them, all these methods ignore the spatial distribution of the inhomogeneities, that is, they all assume uniform distribution. However, the shapes and orientations of the ellipsoidal inhomogeneities are taken into account through the Eshelby tensor Sr. Note that the Eshelby tensor is shape dependent but not size dependent. Thus, the effective modulus tensor predicted by these methods will not depend on the size of the inhomogeneities. Interactions among the inhomogeneities are taken into consideration differently by different methods. In general, the Eshelby method works only for very dilute concentration, and the other methods are applicable to somewhat higher concentration. We will see some numerical examples later in this section. Now consider the composite material described in Example 7.1. For convenience, we list below the equations for the effective moduli of this composite obtained by all these methods and consider a few special cases.

184

DETERMINATION OF EFFECTIVE MODULI

The Eshelby method: c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K1 ⫹ 40

(7.7.1)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 3K0(30 ⫹ 21) ⫹ 4 0(20 ⫹ 31)

(7.7.2)

K ⫽ K0 ⫹

⫽ 0 ⫹

The Mori–Tanaka method: K ⫽ K0 ⫹

⫽ 0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(7.7.3)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 50(3K0 ⫹ 40) ⫹ 6(1 ⫺ c1)(1 ⫺ 0)(K0 ⫹ 20) (7.7.4)

The self-consistent method: c1(K1 ⫺ K0)(3K ⫹ 4) , 3K1 ⫹ 4

(7.7.5)

5c1(1 ⫺ 0)(3K ⫹ 4) . 3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)

(7.7.6)

K ⫽ K0 ⫹

⫽ 0 ⫹

The differential method: dK (K ⫺ K1)(3K ⫹ 4) ⫹ ⫽ 0, dc1 (1 ⫺ c1)(3K1 ⫹ 4) d 5( ⫺ 1)(3K ⫹ 4) ⫹ ⫽ 0, dc1 (1 ⫺ c1)[3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)] K兩c1⫽0 ⫽ K0 and 兩c1⫽0 ⫽ 0.

(7.7.7)

(7.7.8) (7.7.9)

7.7

COMPARISON OF DIFFERENT METHODS

185

Dilute Concentration

For dilute concentration of inhomogeneities, we can assume c1 ⬍⬍ 1. Therefore, by expanding (7.7.3) and (7.7.4) into power series of c1 and neglecting high-order terms, we have c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K1 ⫹ 40

(7.7.10)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 3K0(30 ⫹ 21) ⫹ 40(20 ⫹ 31)

(7.7.11)

K ⫽ K0 ⫹

⫽ 0 ⫹

Comparing the above with the Eshelby estimate, it is seen that at the dilute concentration, the Mori–Tanaka estimate reduces to the Eshelby results. As for the self-consistent estimate, we can ﬁrst expand K and into power series of c1, that is, K ⫽ K0 ⫹ c1K0(1) ⫹ c12K0(1) . . . ,

(7.7.12)

⫽ 0 ⫹ c10(1) ⫹ c120(1) . . . .

(7.7.13)

Substituting these expansions into (7.7.5) and (7.7.6) yields immediately that the self-consistent estimate, in the dilute case, also reduces to the Eshelby estimate. Following similar steps, one can show that the differential method predicts the same results as well (as expected, since the differential method was based on the solution to the dilute case). In other words, all four methods yield the same results when the volume fraction of the inhomogeneity is very low. In the limit of c1 → 0, the effective modulus of the composite as predicted by all these methods reduce to the modulus of the matrix, as it should. High-Concentration Asymptotes

For this case, we are interested in the limit c1 → 1, meaning the entire ‘‘composite’’ consists of particles only. Certainly, this would require multiple size particles; see Problem 7.6. Since the composite contains particles only, it is expected that the effective modulus of the composite

186

DETERMINATION OF EFFECTIVE MODULI

should be the modulus of the particles. Taking the limit c1 → 1 in (7.7.1)–(7.7.6), we ﬁnd that the Eshelby method predicts K0(2K1 ⫺ K0) ⫹ 40K1 , 3K1 ⫹ 40

(7.7.14)

0[3K0(71 ⫺ 20) ⫹ 40(81 ⫺ 30)] . 3K0(30 ⫹ 21) ⫹ 40(20 ⫹ 31)

(7.7.15)

K⫽

⫽

It is not surprising that the Eshelby method does not predict the correct values because the Eshelby method is valid only for dilute concentrations. It is very easy to see by setting c1 ⫽ 1 in (7.7.3) and (7.7.4) that the Mori–Tanaka method does predict the proper limiting values for the effective moduli: K ⫽ K1,

⫽ 1.

(7.7.16)

It can also be easily veriﬁed that (7.7.16) represent a set of solutions to the self-consistent equations (7.7.5) and (7.7.6). In other words, the self-consistent method also predicts the property high-concentration limit. Rigid Particles

To mimic rigid particles, one may consider the limiting case of 0 → 0, 1

K0 → 0. K1

(7.7.17)

Also, on physical grounds, we assume that → 0, 1

K →0 K1

for any 0 ⱕ c1 ⬍ 1. Making use of the above in (7.7.1)–(7.7.4), we obtain

(7.7.18)

7.7

K ⫽ K0 ⫹

COMPARISON OF DIFFERENT METHODS

c1(3K0 ⫹ 40) , 3

⫽ 0 ⫹

187

5c10(3K0 ⫹ 40) , 6(K0 ⫹ 20) (7.7.19)

from the Eshelby method, and K ⫽ K0 ⫹

c1(3K0 ⫹ 40) , 3(1 ⫺ c1)

⫽ 0 ⫹

5c10(3K0 ⫹ 40) 6(K0 ⫹ 20)(1 ⫺ c1) (7.7.20)

from the Mori–Tanaka method. Again, it is seen that both methods predict correctly that K ⫽ K0 and ⫽ 0 at the low-concentration limit c1 → 0. At the high-concentration limit, c1 → 1, the Mori–Tanaka method predicts that the effective modulus increases without bound (as it should because the composite is full of rigid particles), while the Eshelby method yields a ﬁnite value. This is expected, for we know that the Eshelby method is applicable only for the dilute case. Making use of (7.7.17) and (7.7.18) in the self-consistent estimate, we obtain K ⫽ K0 ⫹

c1(3K ⫹ ) , 3

⫽ 0 ⫹

5c1(3K ⫹ 4) . 6(K ⫹ 2)

(7.7.21)

The effective bulk modulus K can be solved from (7.7.21) to yield K⫽

3K0 ⫹ 4c1 . 3(1 ⫺ c1)

(7.7.22)

Substituting (7.7.22) into the second of (7.7.21) yields

冉冊 冋

12(1 ⫺ 2c1)

0

2

⫹

3(2 ⫺ 5c1)

册

K0 6K0 ⫺ 4(3 ⫺ c1) ⫺ ⫽ 0. 0 0 0 (7.7.23)

When c1 ⫽ 0.5, the above equation reduces to

188

DETERMINATION OF EFFECTIVE MODULI

12K00 ⫽⫺ ⬍ 0. 3K0 ⫹ 200

(7.7.24)

This is not a physically possible solution because the effective shear modulus should be positive. For c1 ⫽ 0.5, the quadratic equation (7.7.23) yields two roots. Numerical analysis shows that both roots are real. One of them is always negative and other is given by  ⫽␣⫹ ⫹ 0 1 ⫺ 2c1

冪冉

␣⫹

冊

 1 ⫺ 2c1

2

⫹

1 ⫹ 0 , 3(1 ⫺ 20)(1 ⫺ 2c1) (7.7.25)

where 0 is the Poisson ratio of the matrix material, and 3(1 ⫹ 30) ␣⫽⫺ , 24(1 ⫺ 20)

⫽

11 ⫺ 190 . 24(1 ⫺ 20)

(7.7.26)

In deriving (7.7.25), we have used the relationship 0 3(1 ⫺ 20) ⫽ . K0 2(1 ⫹ 0)

(7.7.27)

Since 0 ⱕ 0 ⱕ 0.5, it can be shown that the right hand of (7.7.25) is positive only for 0 ⱕ c1 ⬍ 0.5. In other words, for spherical rigid particles dispersed in a matrix material, the self-consistent method yields a physically meaningful solution to the effective shear modulus only if the particle volume fraction is less than 50%. Now, consider the differential method. Making use of (7.7.18) in (7.7.7) and (7.7.8) yields dK (3K ⫹ 4) ⫺ ⫽ 0, dc1 3(1 ⫺ c1)

(7.7.28)

d 5(3K ⫹ 4) ⫺ ⫽ 0. dc1 6(1 ⫺ c1)(K ⫹ 2)

(7.7.29)

Solutions to this system of nonlinear differential equations are still fairly complicated. To exam the high-concentration asymptotic behavior of the differential scheme predictions, let us expand the solution near c1 ⫽ 1:

7.7

K⫽

冘 (1 ⫺Ac ) ⬁

n

n⫽0

, m–n

COMPARISON OF DIFFERENT METHODS

⫽

冘 (1 ⫺Bc ) ⬁

n

n⫽0

1

189

,

m–n

(7.7.30)

1

where the asymptotic behavior is dictated by the constant m, which is to be determined from the solution procedure. Substituting (7.7.30) into (7.7.28) and (7.7.29) and keeping the leading order terms only, we obtain the following eigenvalue problem:

冋

3(m ⫺ 1) 3(2m ⫺ 5)

册冋 册 冋 册

⫺4 4(2m ⫺ 5)

A0 0 ⫽ . B0 0

(7.7.31)

The corresponding eigenvalues are m ⫽ 0 and m ⫽ 2. The eigenvalue m ⫽ 2 should be chosen on physical ground. Therefore, the asymptotic behavior of the differential scheme for c1 → 1 is K⬇

A0 , (1 ⫺ c1)2

⬇

B0 . (1 ⫺ c1)2

(7.7.32)

In summary, for the case of rigid particles, the Eshelby method yields ﬁnite values of the effective moduli in the high-concentration limit c1 → 1, while the self-consistent method yields no solution for c1 ⬎ 1 in this case. Both the Mori–Tanaka and the differential methods predict unbounded effective moduli, but their asymptotic behavior is different. The Mori–Tanaka solution behaves as 1/(1 ⫺ c1) while the differential solution behaves as 1/(1 ⫺ c1)2. Other interesting features of the differential scheme can also be explored. For example, in the case of the incompressible matrix, that is, /K → 0, (7.7.28) and (7.7.29) reduce to dK K ⫺ ⫽ 0, dc 1 ⫺ c1

(7.7.33)

d 5 ⫺ ⫽ 0. dc 2(1 ⫺ c1)

(7.7.34)

The solutions that satisfy the initial conditions (7.7.9) are K⫽

K0

, 1⫺c

⫽

0 . (1 ⫺ c1)5 / 2

We see that the differential scheme does predict correctly

(7.7.35)

190

DETERMINATION OF EFFECTIVE MODULI

K ⫽ K0,

⫽ 0

(7.7.36)

in the low-concentration limit c → 0. It also predicts that in the highconcentration limit c → 1, shear modulus approaches to inﬁnity with the order of 1/(1 ⫺ c1)5 / 2. Note that the solutions (7.7.32) and (7.7.35) are different in that the former is valid c1 ⫽ 1, while the later is for the incompressible matrix, and is valid for all ranges of c1 between 0 and 1. Voids

Consider a matrix containing spherical voids. When the void content is zero (c1 ⫽ 0), we should expect that the effective modulus is the same as that of the matrix. For high concentration of voids (c1 → 1), we should expect the effective modulus approaches to zero. Let us see how the various methods predict these limiting cases. For voids, we can consider the limiting case of 1 → 0, 0

K1 → 0. 0

(7.7.37)

The Eshelby estimate reduces to K ⫽ K0 ⫺

c1K0(3K0 ⫹ 40) , 40

(7.7.38)

⫽ 0 ⫺

5c10(3K0 ⫹ 40) . 9K0 ⫹ 80

(7.7.39)

They correctly predict the low-concentration limiting value for c1 → 0. For c1 → 1, the Eshelby method yields 3K 3 K ⫽ ⫺ 0, 40

6 (K ⫹ 20) ⫽⫺ 0 0 . 9K0 ⫹ 80

(7.7.40)

These obviously are not physically admissible solutions. The Mori–Tanaka method gives K ⫽ K0 ⫺

c1K0(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫺ 3(1 ⫺ c1)K0

(7.7.41)

7.7

⫽ 0 ⫺

COMPARISON OF DIFFERENT METHODS

5c10(3K0 ⫹ 40) . 5(3K0 ⫹ 40) ⫺ 6(1 ⫺ c1)(K0 ⫹ 20)

191

(7.7.42)

For low concentration, c1K0(3K0 ⫹ 40) , 40

K ⬇ K0 ⫺

⬇ 0 ⫺

5c10(3K0 ⫹ 40) . 9K0 ⫹ 80 (7.7.43)

For high concentration K⬇

40K0 (1 ⫺ c1), 3K0 ⫹ 40

⬇

0(9K0 ⫹ 80) (1 ⫺ c1). 5(3K0 ⫹ 40)

(7.7.44) We see that the Mori–Tanaka method predicts both low- and highconcentration limits correctly, while the Eshelby method is only good for low concentration. Similarly, the self-consistent estimate reduces K ⫽ K0 ⫺

c1K0(3K ⫹ 4) , 4

⫽ 0 ⫺

5c10(3K ⫹ 4) . 9K ⫹ 8

(7.7.45)

Solving the ﬁrst of (7.7.45) for K yields K⫽

4(1 ⫺ c1)K0 . 3c1K0 ⫹ 4

(7.7.46)

Making use of this in the second of (7.7.45) gives us the following quadratic equation for the effective shear modulus:

冉冊 冋

8 0

2

⫹

3(3 ⫺ c1)

册

K0 K ⫺ 4(2 ⫺ 5c1) ⫺ 9(1 ⫺ 2c1) 0 ⫽ 0. 0 0 0 (7.7.47)

When c1 ⫽ 0.5, the two roots of this quadratic equation are, respectively, zero and

192

DETERMINATION OF EFFECTIVE MODULI

冉

⫽⫺

冊

15K0 0 ⫹ ⬍ 0. 16 4

Neither of them is physically meaningful. For c1 ⫽ 0.5, the two roots are all real. Numerical analysis shows that one of these roots is always negative and the other root is given by ⫽ ␣(1 ⫺ 2c1) ⫺  ⫹ 0

冪[␣(1 ⫺ 2c ) ⫺ ] ⫹ 3(1 ⫹4(1 ⫺)(12⫺) 2c ), 0

2

1

1

0

(7.7.48) where 3(3 ⫺ 70) , 16(1 ⫺ 20)

␣⫽

⫽

7 ⫹ 0 . 16(1 ⫺ 20)

(7.7.49)

Since 0 ⱕ 0 ⱕ 0.5, it can be shown that the right hand of (7.7.48) is positive only for 0 ⱕ c1 ⬍ 0.5. In other words, for spherical voids dispersed in an elastic matrix material, the self-consistent method yields a physically meaningful solution to the effective shear modulus only if the void volume fraction is less than 50%. It is seen from the above cases that the self-consistent method has trouble when the particles are rigid or voids. In fact, it is generally true that the self-consistent method does not work well when the contrast between the inhomogeneities and matrix is too large. Now, consider the differential scheme. Use of (7.7.37) leads to dK K(3K ⫹ 4) ⫹ ⫽ 0, dc1 4(1 ⫺ c1)

(7.7.50)

d 5(3K ⫹ 4) ⫹ ⫽ 0. dc1 (1 ⫺ c1)[9K ⫹ 8]

(7.7.51)

Again, we ﬁrst consider the asymptotic behavior near c1 ⫽ 1: K⫽

冘 A (1 ⫺ c ) ⬁

m⫹n

n

n⫽0

1

,

⫽

冘 B (1 ⫺ c ) ⬁

m⫹n

n

1

.

(7.7.52)

n⫽0

By substituting (7.7.52) into (7.7.50) and (7.7.51) and keeping the leading order terms only, we obtain the following eigenvalue problem:

PROBLEMS

冋

3 3(3m ⫺ 5)

册冋 册 冋 册

4(1 ⫺ m) 4(2m ⫺ 5)

A0 0 ⫽ . B0 0

193

(7.7.53)

The corresponding eigenvalues are m ⫽ 0 and m ⫽ 2. The eigenvalue m ⫽ 2 should be chosen on physical ground. Therefore, the asymptotic behavior of the differential scheme for c1 → 1 is ⬇ B0(1 ⫺ c1)2.

K ⬇ A0(1 ⫺ c1)2,

(7.7.54)

Next, let us further assume that the matrix is incompressible, that is, /K → 0. In this case, Eq. (7.7.51) reduces to d 5 ⫹ ⫽ 0. dc1 3(1 ⫺ c1)

(7.7.55)

The solution that satisﬁes the initial condition (7.7.9) is ⫽ 0(1 ⫺ c1)3 / 5.

In summary, for the case of voids, the Eshelby method yields ﬁnite values of the effective moduli in the high-concentration limit c1 → 1, while the self-consistent method yields no physical solution for c1 ⬎ 0.5 in this case. Both the Mori–Tanaka and the differential physical solution for methods yield vanishing effective moduli, but their asymptotic behavior is different. The Mori–Tanaka solution behaves as 1 ⫺ c1, while the differential solution behaves as (1 ⫺ c1)2. PROBLEMS

7.1 Derive (7.2.17) from (7.2.16). 7.2 Show that the Eshelby estimate of the elastic constants for an isotropic spherical particulate-reinforced composite can also be written as

再 冘 ⫹c (2␦ (⫺ ⫺) )冎 c (K ⫺ K ) K ⫽ K 再1 ⫺ 冘 K ⫹ 3␥ (K ⫺ K )冎

⫺1

N

⫽ 0 1 ⫺

r

r⫽1

0

r

0

0

r

⫺1

N

r

r

0

0

r⫽1

where

,

0

0

0

r

0

,

194

DETERMINATION OF EFFECTIVE MODULI

␥0 ⫽ ␦0 ⫽

K0 3K0 ⫹ 40

⫽

1 ⫹ v0 , 9(1 ⫺ v0)

3K0 ⫹ 60 4 ⫺ 5v0 ⫽ . 15K0 ⫹ 200 15(1 ⫺ v0)

7.3 Show, when all the inclusions are similar in shape, that alternative forms of the Mori–Tanaka effective stiffness and compliance tensors are, respectively, given by

再冘 c (L* ⫹ L ) 冎 ⫺ L*, M ⫽ 再 冘 c (M ⫹ M*) 冎 ⫺ M*, ⫺1

N

L⫽

r

0

r

⫺1

0

r⫽0

⫺1

N

r

r

0

⫺1

0

r⫽0

where ⫺1 L* 0 ⫽ L0(S0 ⫺ I),

⫺1 M* ⫺ I]M(0). 0 ⫽ [(I ⫺ S0)

7.4 Prove (7.4.12). 7.5 Show that all three (Eshelby, Mori–Tanake, and self-consistent) estimates are the same for very low volume fractions of inhomogeneities (dilute concentration). 7.6 Assume spherical particles of equal size are dispersed in a matrix material. What is the highest possible volume fraction of the particles? 7.7 Assume circular cross-section ﬁbers of equal radius are placed in a matrix. If all the ﬁbers are aligned in the same direction, what is the highest possible ﬁber volume fraction? 7.8 Show that [I ⫹ Sr M(Lr ⫺ L)]⫺1 ⫽ (Lr ⫹ Hr)⫺1(L ⫹ Hr), ⫺1 ⫺1 [Mr ⫺ Sr(Mr ⫺ M)]⫺1 M ⫽ (Mr ⫹ H⫺1 r ) (M ⫹ Hr ),

where Hr ⫽ L(Sr⫺1 ⫺ I) is the Hill constraint tensor (4.5.14). 7.9 Prove

SUGGESTED READINGS

195

Lr[I ⫹ Sr M(Lr ⫺ L)]⫺1 ⫽ [Mr ⫺ Sr(Mr ⫺ M)]⫺1, Mr[Mr ⫺ Sr(Mr ⫺ M)]⫺1 ⫽ [I ⫹ Sr M(Lr ⫺ L)]⫺1.

SUGGESTED READINGS Benveniste, Y. (1987). A New Approach to the Application of Mori–Tanaka’s Theory in Composite Materials, Mech. Mat., Vol. 6, pp. 147–157. Christensen, R. M. (1990). A Critical Evaluation for a Class of Micromechanics Models, J. Mech. Phys. Solids, Vol. 38, pp. 379–404. Christensen, R. M. (1991). Mechanics of Composite Materials, Krieger, Malabar, FL. Hashin, Z. (1988). The Differential Scheme and Its Applications to Cracked Materials, J. Mech. Phys. Solids, Vol. 36, pp. 719–734. Hill, R. (1963). Elastic Properties of Reinforced Solids: Some Theatrical Principles, J. Mech. Phys. of Solids, Vol. 11, pp. 357–372. Hill, R. (1965). A Self-Consistent Mechanics of Composite Materials. J. Mech. Phys. Solids, Vol. 13, pp. 213–222. McLaughlin, R. (1977). A Study of the Differential Scheme for Composite Materials, Int. J. Engng. Sci., Vol. 15, pp. 237–244. Mori, T. and K. Tanaka. (1973). Average Stress in Matrix and Average Elastic Energy of Materials with Misﬁtting Inclusions, Acta Metall., Vol. 21, pp. 571–574. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston, Chapter 7, Section 45. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York. Norris, A. N. (1985). A Differential Scheme for the Effective Modulus of Composites, Mech. Mat., Vol. 4, pp. 1–16. Walpole, L. J. (1969). On the Overall Elastic Moduli of Composite Materials, J. Mech. Phys. Solids, Vol. 17, pp. 235–251. Walpole, L. J. (1981). Elastic Behavior of Composite Materials: Theoretical Foundations, Advances in Applied Mechanics, Vol. 21, pp. 169–242.

8 DETERMINATION OF EFFECTIVE MODULI— MULTIINCLUSION APPROACHES The methods discussed in the previous chapter are all based on a singleinclusion idea. In this chapter, we will introduce methods of determining the effective properties based on multiple inclusions. This includes coated inclusions.

8.1 COMPOSITE-SPHERE MODEL

The composite-sphere model was ﬁrst introduced by Hashin (1962). It mainly applies to particulate-reinforced composites. This model postulates that a composite is made of an assembly of composite spheres of various sizes. Each composite sphere has a core of radius a comprised of the particle material with stiffness tensor L1 and a shell of thickness b ⫺ a comprised of the matrix material with stiffness tensor L0. Regardless the size of the composite sphere, the ratio of a/b for all spheres in composite is such that the volume fraction of the particle in each composite sphere is that of the particle volume fraction c1 of the entire composite, that is, c1 ⫽ (a/b)3. The size distribution of the composite spheres must be such that the entire space of the composite is fully occupied by the composite spheres. This requires the presence of composite spheres of inﬁnitely small sizes; see Figure 8.1. Clearly, such a model may not be appropriate for a composite with uniform size particles. However, the microstructure so constructed enables us to ﬁnd an exact solution for the effective bulk modulus.

196

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

8.1

COMPOSITE-SPHERE MODEL

197

a b

a

a

b

b Homoteneous Sphere

Composite Sphere

Figure 8.1 Composite-sphere model.

Let us consider ﬁrst the effective bulk modulus of a typical sphere, for example, the rth composite sphere. This can be easily obtained by solving a spherically symmetric deformation problem; see Problem 8.1: Kr ⫽ K0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(8.1.1)

where c1 ⫽ (a/b)3 is the volume fraction of the particle material. It is interesting to note that this happens to be the Mori–Tanaka estimate of the effective bulk modulus of a particulate-reinforced composite; see Example 7.2. Although (8.1.1) is for the rth composite sphere, it also applies to the entire representative volume element of the composite. To prove this, let the entire representative volume element be subjected to a hydrostatic pressure p, that is, the stress everywhere in the representative volume element of the composite is given by ij ⫽ p␦ij.

(8.1.2)

The corresponding complimentary energy density can then be written as ⌸c[ij] ⫽

1 p p2 ijij ⫽ ii ⫽ . 2 2 2K

where K effective bulk modulus of the composite.

(8.1.3)

198

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

On the other hand, we also know that (8.1.2) is also a statically admissible stress ﬁeld. Therefore, it follows from the minimum complimentary energy theorem (see Section 6.1) that p2 p2 ⫽ ⌸c[ij] ⱕ ⌸c[ˆ ij] ⫽ , 2K 2Kr

(8.1.4)

1 1 ⱕ . K Kr

(8.1.5)

that is,

Similarly, if we assume that the representative volume element of the composite is subjected to displacement boundary conditions so that the strain everywhere in the representative volume element is given by ij ⫽ 0␦ij, then the use of the minimum potential energy theorem leads to K ⱕ Kr.

(8.1.6)

Combining (8.1.5) and (8.1.6) yields the desired relationship: K ⫽ Kr ⫽ K0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) . 3K0 ⫹ 40 ⫹ (1 ⫺ c1)(K1 ⫺ K0)

(8.1.7)

This equality can also be understood as follows. If the composite sphere is in a state of pure radial compression (dilatation), it can be substituted with a sphere of equivalent homogeneous material without perturbing the state of stress in its surroundings. Since the substitution can be performed on all composite spheres in the composite, and each sphere has the same c1 ⫽ (a/b)3, the effective bulk modulus of the entire composite should also be given by that of each individual composite sphere. Unlike the effective bulk modulus, the effective shear modulus is rather difﬁcult to estimate for the composite sphere model. This is due to the fact that a composite sphere subjected to shear deformation does not behave as a homogeneous sphere. Hence, the substitution scheme is not valid. The composite sphere model was extended by Hashin and Rosen (1964) to the case of inﬁnitely long cylinders imbedded in an isotropic matrix. Later, Hill (1964) and Hashin (1966) used the composite-sphere model to determine the effective modulus of ﬁber-reinforced composite

8.1

199

COMPOSITE-SPHERE MODEL

materials; see Figure 8.2. They were able to ﬁnd the exact solutions to four of the ﬁve elastic moduli (Christensen and Lo, 1979): Longitudinal Young’s modulus EL: EL ⫽ cƒEƒ ⫹ cmEm ⫹

4cƒcm(vƒ ⫺ vm)2 m , (8.1.8) 1 ⫹ 3cƒ m /(3Km ⫹ m) ⫹ 3cm m /(3Kƒ ⫹ ƒ)

Transverse bulk modulus KT: KT ⫽ Km ⫹ ⫹

m 3

cƒ , 3/(3Kƒ ⫹ ƒ ⫺ 3Km ⫺ m) ⫹ 3cƒ /(3Km ⫹ 4m) (8.1.9)

Longitudinal shear modulus L: L ⫽

(cƒƒ ⫹ cmm ⫹ ƒ)m , cmƒ ⫹ cƒm ⫹ m

(8.1.10)

Longitudinal Poisson’s ratio vLT: vLT ⫽ cƒvƒ ⫹ cmvm ⫹

3cƒcm(vƒ ⫺ vm)m[cƒ m /(3Km ⫹ m) ⫹ cmm /(3Kƒ ⫹ ƒ)] , 1 ⫹ 3cƒ m /(3Km ⫹ m) ⫹ 3cm m /(3Kƒ ⫹ƒ) (8.1.11)

Figure 8.2 Two-phase composite-cylinder model.

200

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

where Kƒ, ƒ, and Km, m are the bulk and shear moduli of the ﬁber and the matrix, respectively. The remaining modulus, the transverse shear modulus, cannot be obtained exactly using the two-phase composite-sphere model. It will be obtained in the next section using the three-phase model.

8.2 THREE-PHASE MODEL

The three-phase model or generalized self-consistent model (Christensen and Lo, 1979) is an extension of the composite-sphere model. As in the composite-sphere model, the three-phase model assumes that each particle of radius a is surrounded by a shell of matrix material with thickness b ⫺ a, so that the particle volume fraction is given by c1 ⫽ (a/b)3. Next, instead of using such composite spheres to ﬁll in the entire representative volume element of the composite as in the composite-sphere model, the three-phase model assumes that the composite sphere is imbedded in an effective medium whose properties are yet to be determined; see Figure 8.3. This is very similar to the selfconsistent method discussed in Sections 7.4 and 7.5; thus the name generalized self-consistent method. The reason it is called generalized is that in the three-phase model, each particle is in contact with or surrounded by the actual matrix material, while in the conventional self-consistent methods discussed in Sections 7.4 and 7.5, the particles are in indirect contact with the effective medium instead of the actual matrix.

Effective Medium

a b Matrix Particle

Figure 8.3 Three-phase model.

8.2

201

THREE-PHASE MODEL

It turns out that the effective bulk modulus of a three-phase composite sphere is also given by (8.1.1); see Problem 8.2. Following the similar argument used to arrive at (8.1.7), one can also show that the effective bulk modulus of the representative volume element of a composite coincides with the effective bulk modulus of the three-phase composite sphere, that is, K ⫽ Kr ⫽ K0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) . 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(8.2.1)

Figure 8.4 shows the comparison of effective bulk modulus obtained experimentally, and predicted by the three-phase model and the selfconsistent model, for a polymer matrix with voids. The data are normalized by the matrix bulk modulus. The Poisson ratio of the matrix is 0.193. The experimental data are from Walsh et al. (1965). It is seen that the conventional self-consistent method underestimates the experimental results. As discussed in Section 7.7, the self-consistent method yields no physically admissible solution for void volume fraction above 0.5. The three-phase model, on the other hand, provides solutions for the entire range of void volume fraction and the results are in fairly good agreement with the experimental data, even when the volume fraction of voids is large. Unlike the effective bulk modulus, obtaining the effective shear modulus is rather complicated. It involves solving the shear deformation of

1.0 Experimental Data: Walsh et al. (1965) Christensen and Lo (1979)

0.8

Self-Consistent Scheme 0.6

K K0

0.4 0.2 0.0 0.0

0.2

0.6 0.4 Volume Fraction

0.8

1.0

Figure 8.4 Normalized effective bulk modulus (void / glass) with vM ⫽ 0.193.

202

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

a three-phase composite sphere. Detailed description of the solution procedure is given in Appendix 8.A. The solution can be written formally as ⫺B Ⳳ 兹B2 ⫺ AC ⫽ , 0 A

(8.2.2)

where the constants A, B, and C are given in Appendix 8.A. Presented in Figure 8.5 are the effective modulus estimated by the three-phase model and the Hashin–Shtrikman bounds (Hashin and Shtrikman, 1963, Hashin, 1966; Walpole, 1966). The material parameters used in this comparison are 1 / 0 ⫽ 135.14, v1 ⫽ 0.20, and v0 ⫽ 0.35. It is seen from Figure 8.5 that the effective shear modulus from the three-phase model is bounded by the Hashin–Shtrikman lower and upper bounds. The three-phase model has also been applied to ﬁber-reinforced composite materials (Christensen and Lo, 1979) for obtaining the effective transverse shear modulus. Again, the solution procedure is rather complicated. The solution can be written formally as ⫺B Ⳳ 兹B2 ⫺ AC T ⫽ , m A

(8.2.3)

where the constants A, B, and C are given in Appendix 8.B. 21

Upper Bound: Hashin (1962) Christensen and Lo (1979)

µ µ0

Lower Bound: Hashin–Strikman (1963) and Walpole (1966)

16

11

6.0

0.0 0.0

0.2

0.6 0.4 Volume Fraction

0.8

1.0

Figure 8.5 Normalized effective shear modulus for spherical model with 1 / 0 ⫽ 135.14, v1 ⫽ 0.20, and v0 ⫽ 0.35 (boron / epoxy composite).

8.3

FOUR-PHASE MODEL

203

8.3 FOUR-PHASE MODEL

The four-phase model was developed in order to take into account more complex heterogeneities found in advanced composite materials. In the four-phase model, an interphase is introduced between the inhomogeneity and the surrounding matrix. This enables the modeling of composites with coated ﬁbers or particles. This model is very commonly used in civil engineering applications (e.g., Li et al., 1999; Hashin and Monteiro 2003; Heukamp et al., 2004). Bardella et al. (2002) have also used the four-phase model to estimate the effective behavior of synthetic foam, which are materials composed of a polymer matrix reinforced with hollow glass inclusions and isolated porosities. The four-phase model can be applied in different ways. Some treat the four phases in a single formulation, while others split them into a threephase model and a composite-sphere model. This later approach was taken by Li et al. (1999) to evaluate the effective elastic properties of an isotropic elastic medium. Their model was divided into two parts; one part corresponds to the three-phase model of Christensen and Lo (1979); the other part corresponds to the two-phase composite-sphere model of Hashin (1962); see Figure 8.6. Note that the problem shown in Figure 8.6(b) is equivalent to the three-phase model. Therefore, the corresponding effective bulk modulus is given by (8.2.1): K ⫽ K0 ⫹

(Ke ⫺ K0)(3K0 ⫹ 40)(b3 /c3) , 3K0 ⫹ 40 ⫹ 3(Ke ⫺ K0)(1 ⫺ b3 /c3)

Effective Medium

Particle Coating Matrix (a)

(8.3.1)

Effective Medium

Homogenized Particle and Coating (b)

Matrix

Particle

Coating (c)

Figure 8.6 Decomposition of four-phase model: (a) four, (b) three, and (c) two phases.

204

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

where K0 and 0 are, respectively, the bulk and shear moduli of the matrix, and Ke is the effective bulk modulus of the coated inhomogeneity, which can be obtained by solving the problem depicted in Figure 8.6(a): Ke ⫽ Kc ⫹

(K1 ⫺ Kc)(3Kc ⫹ 4c)(a3 /b3) , 3Kc ⫹ 4c ⫹ 3(K1 ⫺ Kc)(1 ⫺ a3 /b3)

(8.3.2)

where Kc and c are the bulk and shear moduli of the coating layer, respectively, and K1 is the bulk modulus of the inhomogeneity. Substitution of (8.3.2) into (8.3.1) yields the effective bulk modulus of the representative volume element of the composite. It is interesting to note that the effective bulk modulus depends not only on the elastic properties of the inhomogeneity and the matrix but also on the dimensions of the inhomogeneity and its coating material.

8.4 MULTICOATED INCLUSION PROBLEM

The ideas of the two-phase and three-phase models can be extended to develop the multiphase model. In the multiphase model, it is assumed that a spherical inhomogeneity comprised of isotropic material is coated with N layers of different isotropic materials. The interfaces between the inhomogeneity and the coating and between the coatings are all assumed perfect. To obtain the effective bulk modulus, we subject the multicoated composite to pure dilatational deformation. It follows from the derivation in the previous sections that the effective modulus can be written as Herve and Zaoui (1993):

Rn

K1

K2

Kn

R1 R2

Figure 8.7 Multicoated inclusion schematic.

8.4

Kn ⫽ Kn ⫹

MULTICOATED INCLUSION PROBLEM

(R3n⫺1 /R3n)(Kn⫺1 ⫺ Kn)(3Kn ⫹ 4n) , 3Kn ⫹ 4n ⫹ 3(1 ⫺ R3n⫺1 /R3n)(Kn⫺1 ⫺ Kn)

205

n ⱖ 2, (8.4.1)

where Rn and Rn⫺1 are, respectively, the radii of phase n and (n ⫺ 1), Kn and n are, respectively, the bulk and shear moduli of phase n, and Kn⫺1 is the effective bulk modulus of the (n ⫺ 1)-coated inclusion. If we deﬁne K1 ⫽ K1 and KN ⫽ K, (8.4.1) provides a recursive relationship to compute the effective bulk modulus. For n ⫽ 2, the effective bulk modulus reduces to that of the twophase composite sphere model: K ⫽ K2 ⫹

c2(K1 ⫺ K2)(3K2 ⫹ 42) , 3K2 ⫹ 42 ⫹ 3(1 ⫺ c2)(K1 ⫺ K2)

(8.4.2)

where c ⫽ R31 / R32 gives the volume fraction of the inhomogeneity, and the subscripts 1 and 2 refer to the inhomogeneity and the coating, respectively. For n ⫽ 3, the effective bulk modulus can be expressed as K ⫽ K3 ⫹

(R32 /R33)(K2 ⫺ K3)(3K3 ⫹ 43) , 3K3 ⫹ 43 ⫹ 3(1 ⫺ R32 /R33)(K2 ⫺ K3)

(8.4.3)

K2 ⫽ K2 ⫹

(R31 /R32)(K1 ⫺ K2)(3K2 ⫹ 42) . 3K2 ⫹ 42 ⫹ 3(1 ⫺ R31 /R32)(K1 ⫺ K2)

(8.4.4)

where

Shown in Figure 8.8 are the prediction of the effective bulk modulus by the multicoated inclusion method. The data are normalized by the matrix’s bulk modulus, K3. The parameter  ⫽ K2 /K3 is the ratio of the bulk moduli of the coating and the matrix. The Poisson ratios of the particle, matrix, and coating are all set to be 0.3 (v1 ⫽ v2 ⫽ v3 ⫽ 0.3). The ratio of the bulk modulus of particle and of matrix is set to 6 (K1 /K3 ⫽ 6), and the volume fraction of the particle with coating is c1 ⫹ c2 ⫽ 0.2. It is seen that when  ⬎ 1 the interface is more rigid than the matrix. The case  ⫽ 6 corresponds to a simply coated inclusion (Christensen and Lo, 1979). The same remark stands for all values of  when the volume fraction of coating is in the neighborhood 0.2.

206

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

1.0

β = 1000

K K3

β = 10

β = 100

0.8

β =6

0.6

β =1

0.4

β = 0.1 β = 0.01

0.2 0.0 0.0

0.05

0.1

0.15

0.2

Volume Fraction of Coating

Figure 8.8 Normalized effective bulk modulus K / KN⫺1 (Herve´ and Zaoui, 1993) of a composite material, made of coated particle (phase 2), for different values  ⫽ 1 / M (1 denotes the inclusion) with v1 ⫽ v2 ⫽ v3 ⫽ 0.3, 1 / M ⫽ 6, c1 ⫹ c2 ⫽ 0.2.

The effective shear modulus predicted by the multiphase model is given by ⫺B Ⳳ 兹B2 ⫺ 4AC ⫽ , N 2A

(8.4.5)

where the constants A, B, and C are given in Appendix 8.C. PROBLEMS

8.1 Consider a composite-sphere consists of a core of radius a and a shell of thickness b ⫺ a surrounding the core; see Figure 8.9. Let both the core and shell be made of isotropic elastic material with

b a K1, µ1 K0, µ0

Figure 8.9

207

APPENDIX 8.A

moduli K0, 0 and K1, 1, respectively. Please ﬁnd the effective bulk modulus of the composite sphere. 8.2 Consider a three-phase concentric sphere as shown in Figure 8.10. Please ﬁnd the effective bulk modulus of the composite sphere.

APPENDIX 8.A

To derive (8.2.2), the elasticity problem depicted in Figure 8.3 needs to be solved under simple shear deformation. This can be carried out by writing the displacement ﬁelds in a spherical coordinate system in each of the three regions: the inhomogeneity (r ⱕ a), the matrix (a ⱕ r ⱕ b), and the effective medium (b ⱕ r). The following equation can then be derived after making use of the equilibrium equations and the continuity conditions at the interfaces between the different regions:

冉冊

A 0

2

冉冊

⫹ 2B

⫹ C ⫽ 0, 0

(8.A.1)

where

冉

A⫽8

冊

冋冉 冊 冉 冊

册

1 ⫺ 1 (4 ⫺ 5v0)1c10 / 3 ⫺ 2 63 1 ⫺ 1 2 ⫹ 213 c7 / 3 0 0

⫹ 252

冉

冊

1 ⫺ 1 2c5 / 3 ⫺ 50 1 ⫺ 1 (7 ⫺ 12v0 ⫹ 8v02)2c 0 0

⫹ 4(7 ⫺ 10v0)23,

b a K1, µ0 K0, µ0

K, µ

Figure 8.10

208

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

冉 冊 冋冉 冊 冉 冊 冉 冊 冉 冊

B ⫽ ⫺2

1 ⫺ 1 (4 ⫺ 5v0)1c10 / 3 0

⫹ 2 63 ⫹ 75

C⫽4

册

冉

冊

1 ⫺ 1 2 ⫹ 213 c7 / 3 ⫺ 252 1 ⫺ 1 2c5 / 3 0 0

1 ⫺ 1 (3 ⫺ v0)v02c ⫹ 3(15v0 ⫺ 7)23, 0

冋冉 冊 冉 冊

册

1 ⫺ 1 (5v0 ⫺ 7)1c10 / 3 ⫺ 2 63 1 ⫺ 1 2 ⫹ 213 c7 / 3 0 0

⫹ 252

1 ⫺ 1 2c5 / 3 ⫹ 25 1 ⫺ 1 (v02 ⫺ 7)2c 0 0

⫺ (7 ⫹ 5v0)23,

with 1 ⫽

冉

冊

冉冊 冊 冉

1 ⫺ 1 (49 ⫺ 50v1v0) ⫹ 35 1 (v1 ⫺ 2v0) ⫹ 35(2v1 ⫺ v0), 0 0

冉 冉冊

2 ⫽ 5v1

3 ⫽

冊

1 ⫺8 ⫹7 1⫹4 , 0 0

1 (8 ⫺ 10v0) ⫹ (7 ⫺ 5v0), 0

where c is the volume fraction of the particles, that is, c ⫽ (a/b)3.

APPENDIX 8.B

Detailed derivation of the three-phase composite cylinder model can be found in Christensen and Lo (1979). The results are list below for the effective transverse shear modulus.

APPENDIX 8.B

冉冊

冉冊

2

A T m

⫹ 2B

T ⫹ C ⫽ 0, m

209

(8.B.1)

where A ⫽ 3c(1 ⫺ c)2 ⫹ ⫻

冋 冋 冉 冉

冋

冊冉 冊 冉 冊册 冊 冉 冊册 冊冉 冊 冉 冊册 冊 冉 冊册 冊冋 冉 冊册

ƒ ⫺1 m

ƒ ⫹ ƒ m

ƒ ƒ m ⫹ ƒm ⫺ ⫺ ƒ c3 m m m

cm

ƒ ƒ ⫺1 ⫺ ⫹1 m m m

ƒ ⫺1 m

B ⫽ ⫺3c(1 ⫺ c)2 ⫹

冉

,

(8.B.2)

ƒ ⫹ ƒ m

ƒ 1 ƒ m ⫹ 1 ⫹ ⫺1 c 2 m m

⫻

冋

冉 冉

⫹

ƒ c (m ⫺ 1) ⫺1 2 m

(m ⫺ 1)

ƒ ƒ ⫹ ƒ ⫺ 2 ⫺ ƒ c3 m m m

ƒ ƒ m ⫹ ƒ ⫹ ⫺ 1 c3 , m m

(8.B.3)

冉

C ⫽ 3c(1 ⫺ c)2 ⫹ ⫻

and

冋 冋

ƒ ⫺1 m

冉

冊冉

冊 冊册 冊册

ƒ ⫹ ƒ m

ƒ ƒ ⫹ ƒ ⫺ ⫺ ƒ c3 m m m

冉

ƒ ƒ m ⫹ 1 ⫹ ⫺1 c , m m

(8.B.4)

210

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

冉冊

3

a c⫽ , b

m ⫽ 3 ⫺ 4vm,

ƒ ⫽ 3 ⫺ 4vƒ.

(8.B.5)

APPENDIX 8.C

The constants in (8.4.5) are given by 7 2 A ⫽ 4R10 n (1 ⫺ 2vn)(7 ⫺ 10vn)Z12 ⫹ 20Rn(7 ⫺ 12vn ⫹ 8vn)Z42 ⫹ 12Rn5(1 ⫺ 2vn)(Z14 ⫺ 7Z23) ⫹ 20Rn3(1 ⫺ 2vn)2Z13 ⫹ 16(4 ⫺ 5vn)(1 ⫺ 2vn)Z43,

B ⫽ 4Rn10(1 ⫺ 2vn)(15vn ⫺ 7)Z12 ⫹ 60Rn7(vn ⫺ 3)vnZ42 ⫺ 24R5n(1 ⫺ 2vn)(Z14 ⫺ 7Z23) ⫺ 40R3n(1 ⫺ 2vn)2Z13 ⫺ 8(1 ⫺ 5vn)(1 ⫺ 2vn)Z43, 7 2 C ⫽ ⫺R10 n (1 ⫺ 2vn)(7 ⫹ 5vn)Z12 ⫹ 10Rn(7 ⫺ vn)Z42 ⫹ 12Rn5(1 ⫺ 2vn)(Z14 ⫺ 7Z23) ⫹ 20Rn3(1 ⫺ 2vn)2Z13 ⫺ 8(1 ⫺ 5vn)(1 ⫺ 2vn)Z43,

where Z␣ ⫽ P␣(n⫺1) P(n⫺1) ⫺ P(n⫺1) P(n⫺1) 1 2 1 ␣2 P(n) ⫽

with ␣ 僆 [1,4] and  僆 [1,4],

写M n

( j)

.

j⫽1

ck 3 M

(k)

⫽

0

1

R5k ␣k 2

5(1 ⫺ vk⫹1) ⫺5

6

(1 ⫺ 2vk⫹1)␣kRk3

Rk2(3bk ⫺ 7ck) 5(1 ⫺ 2vk) (1 ⫺ 2vk⫹1)bk 7(1 ⫺ 2vk) 7 ⫺Rk (2␣k ⫺ 147␣k) 70(1 ⫺ 2vk) 7(1 ⫺ 2vk⫹1)␣kRk5 2(1 ⫺ 2vk)

REFERENCES

⫺12␣k 5 k

R

⫺20(1 ⫺ 2vk⫹1)␣k

7R7k dk 7

211

4(ƒk ⫺ 27␣k) 15(1 ⫺ 2vk)Rk3 ⫺12␣k(1 ⫺ 2vk⫹1) 7(1 ⫺ 2v)R ... , 2 Rk (105(1 ⫺ vk⫹1) ⫹ 12␣k(7 ⫺ 10vk) ⫺ 7ek) 35(1 ⫺ 2vk) ek(1 ⫺ 2vk) 3(1 ⫺ 2vk)

with ␣k ⫽

冉 冊

k (7 ⫹ 5vk)(7 ⫺ 10vk⫹1) ⫺ (7 ⫺ 10vk)(7 ⫹ 5vk⫹1), k⫹1

冉 冉 冉 冉 冉

冊 冊 冊 冊 冊

bk ⫽ 4(7 ⫺ 10vk) ⫹

k (7 ⫹ 5vk), k⫹1

ck ⫽ (7 ⫺ 5vk⫹1) ⫹ 2

k (4 ⫺ 5vk⫹1), k⫹1

dk ⫽ (7 ⫹ 5vk⫹1) ⫹ 4

k (7 ⫺ 10vk⫹1), k⫹1

ek ⫽ 2(4 ⫺ 5vk) ⫹ ƒk ⫽ (4 ⫺ 5vk)(7 ⫺ 5vk⫹1) ⫺ ␣k ⫽

k (7 ⫺ 5vk), k⫹1

k (4 ⫺ 5vk⫹1)(7 ⫺ 5vk), k⫹1

k ⫺ 1. k⫹1

REFERENCES Christensen, R. M. and K. H. Lo. (1979). Solutions for Effective Shear Properties in Three Phase Sphere and Cylinder Models, J. Mech. Phys. Solids, Vol. 27, pp. 315–330.

212

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

Hashin, Z. (1962). The Elastic Moduli of Heterogeneous Materials, J. Appl. Mech., Vol. 29, pp. 143–150. Hashin, Z. (1966). Viscoelastic Fiber Reinforced Materials, AIAA J., Vol. 4, pp. 1411–1417. Hashin, Z. and B. W. Rosen. (1964). The Elastic Moduli of ReinforcedReinforced Materials, J. Appl. Mech., Vol. 31, pp. 223–228. Hashin, Z. and S. Shtrikman. (1963). A Variational Approach to the Theory of the Elastic Behavior of Multiphase Materials, J. Mech. Phys. Solids, Vol. 11, pp. 127–140. Herve´, E. and A. Zaoui. (1993). N-Layered Inclusion-Based Micromechanical Modeling, Int. J. Eng. Sci., Vol. 31, pp. 1–10. Hill, R. (1964). Theory of Mechanical Properties of Fibre-Strengthened Materials—I: Elastic Behavior,’’ J. Mech. Phys. Solids, Vol. 12, pp. 199–212. Li, G., Y. Zhao, and S. S. Pang. (1999). Four-Phase Sphere Modeling of Effective Bulk Modulus of Concrete, Cement and Concrete Research, Vol. 29, pp. 839–845. Walpole, L. J. (1966). On the Bounds for Overall Elastic Moduli of Inhomogeneous Systems—I, J. Mech. Phys. Solids, Vol. 14, pp. 151–162. Walpole, L. J. (1969). On the Overall Elastic Moduli of Composite Materials, J. Mech. Phys. Solids, Vol. 17, pp. 235–251. Walsh, J. B., W. F. Brace, and A. W. England. (1965). The Effect of Porosity on Compressibility of Glass, J. Am. Ceram. Soc., Vol. 48, pp. 605–608.

SUGGESTED READINGS Bardella, L. and F. Genna. (2001). On the Elastic Behavior of Syntactic Foams, Int. J. Solids Structures, Vol. 38, pp. 7235–7260. Benveniste, Y. (1987). A New Approach to the Application of Mori–Tanaka’s Theory in Composite Materials, Mech. Mater., Vol. 6, pp. 147–157. Benveniste, Y., G. J. Dvorak, and T. Chen. (1989). Stress Field in Composite with Coated Inclusions, Mech. Mater., Vol. 7, pp. 305–317. Budiansky, B. and T. Wu. (1962). Theoretical Prediction of Plastic Strains in Polycrystals, In Proc. 4th U.S. Nat. Cong. Theo. Appl. Mech., pp. 1175– 1183. Cherkaoui, M., H. Sabar, and M. Berveiller. (1994). Micromechanical Approach of the Coated Inclusion Problem and Applications to Composite Materials, J. Eng. Mater. Tech., Vol. 116, pp. 274–278. Cherkaoui, M., H. Sabar, and M. Berveiller. (1995). Elastic Composites with Coated Reinforcements: A Micromechanical Approach for Nonhomothetic Topology, Int. J. Eng. Sci., Vol. 33, pp. 829–843. Christensen, R. M. (1991). Mechanics of Composite Materials, Krieger, Malabar, FL.

SUGGESTED READINGS

213

El Mouden, M., M. Cherkaoui, A. Molinari, and M. Berveiller. (1998). The Overall Elastic Response of Materials Containing Coated Inclusions in a Periodic Array, Int. J. Engng. Sci., Vol. 36, pp. 813–829. Hashin, Z. and P. J. M. Monteiro. (2003). An Inverse Method to Determine the Elastic Properties of the Interphase between the Aggregate and the Cement Paste, Cem. Conc. Res., Vol. 32, pp. 1291–1300. Heukamp, F. H., E. Lemarchand, and F. J. Ulm. (2005). The Effect of Interfacial Properties on the Cohesion of Highly Filled Composite Materials, Int. J, Solids Structures, Vol. 42, 287–305. Hill, R. (1963). Elastic Properties of Reinforced Solids: Some Theoretical Principles, J. Mech. Phys. of Solids, Vol. 11, pp. 357–372. Hill, R. (1995). A Self-Consistent Mechanics of Composite Materials, J. Mech. Phys. Solids, Vol. 13, pp. 213–222. Hori, M. and S. Nemat-Nasser. (1993). Double-Inclusion Model and Overall Moduli of Multi-Phase Composites, Mech. Mater., Vol. 14, pp. 189–206. Jasiuk, I. and M. W. Kouider. (1993). The Effect of an Inhomogeneous Interphase on the Elastic Constants of Transversely Isotropic Composites, Mech. Mater., Vol. 15, pp. 53–63. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York. Norris, A. N. (1985). A Differential Scheme for the Effective Modulus of Composites, Mech. Mater., Vol. 4, pp. 1–16. Qiu, Y. P. and G. J. Weng. (1991). Elastic Moduli of Thickly Coated Particle and Fiber-Reinforced Composites, J. Appl. Mech., Vol. 58, pp. 388–398.

9 EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES A ﬁber-reinforced composite laminate is a special kind of heterogeneous material. It typically consists of multiple layers of plies, each ply is thin sheet of matrix material reinforced by unidirectional ﬁbers. Glass ﬁber- and graphite ﬁber-reinforced epoxy matrix composites are the most commonly used composite laminates. In this chapter, we will apply some of the theories developed in previous chapters to determine the effective properties for ﬁber-reinforced composite laminates.

9.1 UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

Consider a matrix material reinforced by circular cross-section ﬁbers all aligned in the x1 direction, as schematically shown in Figure 9.1. Let the volume fraction of the ﬁber be cƒ and volume fraction of the matrix be cm. Obviously, we have cm ⫹ cƒ ⫽ 1.

(9.1.1)

We further assume that both the ﬁber and the matrix are isotropic, and their elastic properties are deﬁned by the Young’s modulus Eƒ, Em and Poisson’s ratio ƒ, m, respectively. Because of the cylindrical nature of the composite, the effective elastic properties are transversely isotropic. In the Voigt notation, this can be written as 214

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

215

x3 x2

x1

Figure 9.1 Unidirectional ﬁber-reinforced composite.

冤冥冤 11 22 33 23 13 12

⫽

C11

C12

C12

0

0

0

C12

C22

C23

0

0

0

C12

C23

C22

0

0

0

0

0

0

0

0

0

0

0

0

C22 ⫺ C23 0 2 0 C66 0

0

0 0 C66

冥冤 冥 11 22 33 223 213 212

(9.1.2)

where Cij are the effective Voigt elastic constants of the unidirectional ﬁber-reinforced composite. For convenience and without causing any confusion, we have omitted the overbar for the effective Voigt elastic constants, which are related to the effective elasticity tensor Lijkl through the relationship described by Table 2.1. Equation (9.1.2) is written in a coordinate system where the x1 axis is in the direction of the ﬁbers. In the coordinate system xˆ i shown in Figure 9.2, where the xˆ 1 axis forms an angle from the ﬁber direction, the expressions for the components Cˆ ij of the Voigt elastic matrix are different. They are related to Cij through a coordinate rotation; see (2.4.13): x1 xˆ2

xˆ1 θ

x1

Figure 9.2 Fibers not aligned with coordinate axis.

216

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

Cˆ 11 ⫽ Q11m4 ⫹ 2(C12 ⫹ 2C66)m2n2 ⫹ C22n4, Cˆ 22 ⫽ C11n4 ⫹ 2(C12 ⫹ 2C66)m2n2 ⫹ C22m4, Cˆ 33 ⫽ C33, Cˆ 12 ⫽ (C11 ⫹ C22 ⫺ 4C66)m2n2 ⫹ C12(m4 ⫹ n4), Cˆ 13 ⫽ C13m3 ⫹ C23n2, Cˆ 23 ⫽ C13n3 ⫹ C23m2, Cˆ 36 ⫽ (C23 ⫺ C13)mn,

(9.1.3)

Cˆ 44 ⫽ C44m3 ⫹ C55n2, Cˆ 55 ⫽ C55m3 ⫹ C44n2, Cˆ 66 ⫽ (C11 ⫹ C22 ⫺ 2C12)m2n2 ⫹ 2C22mn(m2 ⫺ n2) ⫹ C66(m2 ⫺ n2)2, Cˆ 45 ⫽ (C44 ⫺ C55)mn, Cˆ 16 ⫽ (C22 ⫺ C12 ⫺ 2C66)mn3 ⫺ (C11 ⫺ C12 ⫺ 2C66)m3n, Cˆ 26 ⫽ (C22 ⫺ C12 ⫺ 2C66)m3n ⫺ (C11 ⫺ C12 ⫺ 2C66)mn3, in which m ⫽ cos , n ⫽ sin . Therefore, in a coordinate system not aligned with the ﬁber, the Voigt elasticity matrix has the following form:

冤

Cˆ 11 Cˆ 12 ˆ ˆ ⫽ C13 C 0 0 ˆ C16

Cˆ 12 Cˆ 22 Cˆ 23 0 0 ˆ C26

Cˆ 13 Cˆ 23 Cˆ 33 0 0 ˆ C36

0 0 0 Cˆ 44 Cˆ 45 0

0 0 0 Cˆ 45 Cˆ 55 0

冥

Cˆ 16 Cˆ 26 Cˆ 36 . 0 0 ˆ C66

(9.1.4)

Now, let us go back to (9.1.2). Taking the inverse of the elasticity tensor yields

冤冥冤 11 22 33 223 213 212

S11 S12 S12 ⫽ 0 0 0

S12 S22 S23 0 0 0

S12 S23 S22 0 0 0

0 0 0 0 0 0 0 0 0 S44 0 0 0 S66 0 0 0 S66

冥冤 冥

11 22 33 , 23 13 12

(9.1.5)

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

217

where S11 ⫽

⫺2C

C22 ⫹ C23 , ⫹ C11(C22 ⫹ C23)

(9.1.6)

C12 , 2C 212 ⫺ C11(C22 ⫹ C23)

(9.1.7)

2 C 12 ⫺ C11C22 , 2 (C22 ⫺ C23)[2C 12 ⫺ C11(C22 ⫹ C23)]

(9.1.8)

C 212 ⫺ C11C23 , 2 (C22 ⫺ C23)[⫺2C 12 ⫹ C11(C22 ⫹ C23)]

(9.1.9)

S12 ⫽

S22 ⫽

S23 ⫽

2 12

S44 ⫽ 2(S22 ⫺ S23) ⫽

2 C22 ⫺ C23

,

S66 ⫽

1 C66

(9.1.10)

are the ﬁve elastic compliance constants. They can be related to the engineering constants easily as follows. Under a uniaxial loading in the x1 direction, we have 11 ⫽ S1111,

22 ⫽ 33 ⫽ S1211.

(9.1.11)

The ﬁrst of (9.1.11) deﬁnes the longitudinal Young modulus in the ﬁber direction: EL ⫽

11 1 2C 212 ⫽ ⫽ C11 ⫺ . 11 S11 C22 ⫹ C23

(9.1.12)

The contraction in the transverse direction that accompanies the uniaxial stress in the ﬁber direction deﬁnes the corresponding Poisson ratio through S C12 LT ⫽ ⫺ 22 ⫽ ⫺ 33 ⫽ ⫺ 12 ⫽ . 11 11 S11 C22 ⫹ C23

(9.1.13)

Similarly, when the uniaxial stress is in the x2 direction (transverse to the ﬁber), we have

218

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

11 ⫽ S1222,

22 ⫽ S2222,

33 ⫽ S2322.

(9.1.14)

The second of (9.1.14) deﬁnes the Young modulus in the transverse direction: ET ⫽

2 22 1 C 2 (C ⫺ 2C23) ⫹ C11C 23 ⫽ ⫽ C22 ⫺ 12 22 . 22 S22 C11C22 ⫺ C 212

(9.1.15)

In this case, the contraction in the ﬁber direction that accompanies the uniaxial stress in the transverse direction deﬁnes the corresponding Poisson ratio through S C (C ⫺ C23) TL ⫽ ⫺ 11 ⫽ ⫺ 12 ⫽ 12 22 . 2 22 S22 C11C22 ⫺ C 12

(9.1.16)

Analogously, the contraction in the other transverse direction that accompanies the uniaxial stress in one transverse direction deﬁnes another Poisson ratio, S C C ⫺ C 212 TT ⫽ ⫺ 33 ⫽ ⫺ 23 ⫽ 11 23 . 22 S22 C11C22 ⫺ C 212

(9.1.17)

As a convention in labeling the Poisson ratios in this text, the ﬁrst subscript indicates the direction of the uniaxial stress, and the second subscript indicates the direction normal to the loading direction in which the contraction takes place. It is clear from the above or simply from the material asymmetry that TL ⫽ LT. However, it can be easily veriﬁed by direction substitution of their deﬁnitions that LT TL ⫽ . EL ET

(9.1.18)

If a simple shear 12 ⫽ 21 is applied, we will have 212 ⫽ S6612. Thus the longitudinal shear modulus is deﬁned as L ⫽

12 1 ⫽ ⫽ C66. 212 S66

(9.1.19)

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

219

Similarly, when the material is subjected to the simple shear 23, the corresponding shear strain is 223 ⫽ S4423. Thus, the corresponding shear modulus is deﬁned by T ⫽

23 1 1 ⫽ ⫽ (C22 ⫺ C23). 223 S44 2

(9.1.20)

It is clear from the above deﬁnitions that L is the shear modulus when the ﬁbers are shifted relative to each other in the longitudinal direction, while T is the shear modulus when the ﬁbers are shifted relative to each other in the transverse directions. Finally, a plane strain bulk modulus can be introduced by applying biaxial stresses 22 ⫽ 33 ⫽ . Since the elastic properties are isotropic in the x2x3 plane, the corresponding strain ﬁeld is given by 22 ⫽ 33 ⫽ . We thus have ⫽ 2KT ,

(9.1.21)

where KT is the plane strain bulk modulus within the isotropic plane given by KT ⫽ –21 (C22 ⫹ C23).

(9.1.22)

So far, we have introduced two Young moduli, two shear moduli, one bulk modulus, and three Poisson ratios. Not all the eight engineering constants are independent. Since they are deﬁned based on the ﬁve stiffness constants Cij as shown in (9.1.2), it can be easily concluded that there are only ﬁve independent engineering constants. In addition to (9.1.18), the following relationships among these engineering constants can also be veriﬁed by direct substitution: ET ⫽

4TKT , 2 KT ⫹ T ⫹ 4 LT TKT /EL

(9.1.23)

TT ⫽

KT ⫺ T ⫺ 4 2LTTKT /EL , 2 KT ⫹ T ⫹ 4 LT TKT /EL

(9.1.24)

冉

2LT ⫽ ⫺TT ⫺

冊

1 ET 1 ET EL ⫹ . 4 KT 4 T ET

(9.1.25)

220

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

Making use of the deﬁnitions of the engineering elastic constants, the Voigt elasticity matrix for transversely isotropic solids with the x1 direction being the axis of symmetry can be rewritten as

冤

冥

2 EL ⫹ 4 LT KT 2LTKT 2LTKT 0 0 0 2LTKT KT ⫹ T KT ⫺ T 0 0 0 2LTKT KT ⫹ T KT ⫹ T 0 0 0 C⫽ . T 0 0 0 0 0 0 0 0 0 L 0 0 0 0 0 0 L

(9.1.26)

It is interesting to investigate the bounds on the various Poisson ratios. For example, If a material has a very large transverse shear modulus, that is, T → ⬁, then it follows from (9.1.24) that TT → ⫺1. On the other hand, if a material has very large plane strain bulk modulus and very large longitudinal Young’s modulus, that is, KT → ⬁ and EL → ⬁, then it follows from (9.1.24) that TT → 1. Therefore, we can conclude that ⫺1 ⬍ TT ⬍ 1.

(9.1.27)

Next, consider (9.1.23). Solving for 2LT gives 2LT ⫽

冉

冊

EL EL 1 2 ⫺ ⫹ . ET 4 KT T

(9.1.28)

Since the second term on the right-hand side of (9.1.28) is positive, we arrive at 兩LT兩 ⱕ

冪EE .

(9.1.29)

冪EE .

(9.1.30)

L T

Making use of (9.1.18) also yields 兩TL兩 ⱕ

T L

Let us now consider how the effective properties Cij are related to the elastic properties of the ﬁber and the matrix. Several methods can be used for this purpose. We ﬁrst consider a very simple approach.

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

221

Recall that in Chapter 6, we discussed the Reuss lower and Voigt upper bounds for the effective modulus of heterogeneous materials. In what follows, we will apply these bounds to unidirectional ﬁberreinforced composite materials. Assume that both the ﬁbers and the matrix are isotropic and linearly elastic materials. It then follows from (6.2.10) that the Voigt upper bound of the elasticity tensor is given by LV ⫽ cmLm ⫹ cƒLƒ,

(9.1.31)

where Lƒ and Lm are the elasticity tensors of the ﬁber and the matrix, respectively. In terms of the Voigt notation, (9.1.31) implies that the nonzero components of the elasticity tensor can be written as C V11 ⫽ C V22 ⫽ C V33 ⫽

cƒEƒ(1 ⫺ ƒ) cmEm(1 ⫺ m) ⫹ , (1 ⫹ ƒ)(1 ⫺ 2ƒ) (1 ⫹ m)(1 ⫺ 2m) (9.1.32)

V V V V V V C 12 ⫽ C 21 ⫽ C 13 ⫽ C 31 ⫽ C 23 ⫽ C 32 ⫽

⫹

cƒEƒƒ (1 ⫹ ƒ)(1 ⫺ 2ƒ)

cmEmm , (1 ⫹ m)(1 ⫺ 2m) C V44 ⫽ C V55 ⫽ C V66 ⫽

(9.1.33) cƒEƒ cmEm ⫹ , 2(1 ⫹ ƒ) 2(1 ⫹m)

(9.1.34)

where Eƒ, ƒ and Em, m are the Young moldulus and the Poisson ratio of the ﬁber and matrix, respectively. The corresponding upper bound for the effective Young’s modulus is thus given by 2C V12C V12 ⫽ cƒEƒ ⫹ cmEm V V C 22 ⫹ C 12 2cƒcmEƒEm(ƒ ⫺ m)2 ⫹ . cƒEƒ(1 ⫹ m)(1 ⫺ 2m) ⫹ cmEm(1 ⫹ ƒ)(1 ⫺ 2ƒ)

E V ⫽ C V11 ⫺

(9.1.35) The corresponding upper bound for the effective Poisson’s ratio is

222

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

V ⫽ ⫽

V V C V12(C 11 ⫺ C 12 ) V V V V C 11C 11 ⫺ C 12C 12

cƒƒEƒ(1 ⫹ m)(1 ⫺ 2m) ⫹ cmmEm(1 ⫹ ƒ)(1 ⫺ 2ƒ) . cƒEƒ(1 ⫹ m)(1 ⫺ 2m) ⫹ cmEm(1 ⫹ ƒ)(1 ⫺ 2ƒ)

(9.1.36)

If the Poisson ratios of the ﬁber and the matrix are the same, that is, ƒ ⫽ m ⫽ , we have E V ⫽ cƒEƒ ⫹ cmEm,

V ⫽ .

(9.1.37)

On the other hand, the Reuss lower bound (6.2.13) gives L R ⫽ [cƒMƒ ⫹ cmMm]⫺1.

(9.1.38)

In terms the Voigt notation, this means R R C 11 ⫽ C R22 ⫽ C 33 ⫽

EƒEm[(cƒEm(1 ⫺ ƒ) ⫹ cmEƒ(1 ⫺ m)] , D

R R R R C R12 ⫽ C R21 ⫽ C 13 ⫽ C 31 ⫽ C 23 ⫽ C 32 ⫽

(9.1.39)

EƒEm[(cƒEmƒ ⫹ cmEƒm) , D (9.1.40)

C R44 ⫽ C R55 ⫽ C R66 ⫽

EƒEm[(cƒEm(1 ⫺ 2ƒ) ⫹ cmEƒ(1 ⫺ 2m)] , (9.1.41) 2D

where D ⫽ [(cƒEm(1 ⫺ ƒ) ⫹ cmEƒ(1 ⫹ m)] ⫻ [(cƒEm(1 ⫺ 2ƒ) ⫹ cmEƒ(1 ⫺ 2m)].

(9.1.42)

Following the procedures similar to (9.1.35) and (9.1.36), we obtain the lower bounds for the effective Young modulus and the effective Poisson ratio corresponding to (9.1.38),

9.1

ER ⫽

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

EƒEm , cƒEm ⫹ cmEƒ

R ⫽

cƒƒEm ⫹ cmmEƒ . cmEƒ ⫹ cƒEm

223

(9.1.43)

Again, if the Poisson ratios of the ﬁber and the matrix are the same, that is, ƒ ⫽ m ⫽ , we have ER ⫽

EƒEm , cƒEm ⫹ cmEƒ

R ⫽ .

(9.1.44)

It can be shown (see Problem 9.1) that the Voigt upper bound gives a better approximation in the ﬁber direction, while the Reuss lower bound gives a better approximation in the direction perpendicular (transverse) to the ﬁber. Therefore, by neglecting the difference in Poisson’s ratio, one may take the Young modulus in the ﬁber direction to be EL ⫽ E V ⫽ cƒEƒ ⫹ cmEm,

(9.1.45)

and the Young modulus in the transverse direction to be ET ⫽

EƒEm . cƒEm ⫹ cmEƒ

(9.1.46)

Equations (9.1.45) and (9.1.46) are the well-known rule of mixture formulas used commonly in engineering practice. Based on the derivations above, it is clear that these are actually the upper and lower bounds when the Poisson ratios are the same for the matrix and the ﬁbers. More accurate estimate of the unidirectional ﬁber-reinforced composite can be obtained by using the techniques developed in Chapters 7 and 8. To this end, we ﬁrst evaluate the Eshelby tensor for an inﬁnitely long cylindrical inclusion of circular cross section. It follows from Appendix 4.B that in the limit of a2 ⫽ a3 ⫽ a and a1 → ⬁, we obtain the nonzero components of the Eshelby tensor: S2222 ⫽ S3333 ⫽

5 ⫺ 4 , 8(1 ⫺ )

S2233 ⫽ S3322 ⫽

S2211 ⫽ S3311 ⫽

, 2(1 ⫺ )

4 ⫺ 1 , 8(1 ⫺ )

(9.1.47)

(9.1.48)

224

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

S2323 ⫽ S3223 ⫽ S2332 ⫽ S3232 ⫽

3 ⫺ 4 , 8(1 ⫺ )

(9.1.49)

S3131 ⫽ S1331 ⫽ S3113 ⫽ S1313 ⫽ S1212 ⫽ S2112 ⫽ S1221 ⫽ S2121 ⫽ –41 . (9.1.50) Making use of the Eshelby tensor in, for example, the Mori–Tanaka estimate (7.3.8), we have the effective elasticity tensor of the unidirectional ﬁber-reinforced composite given by L ⫽ (cmLm ⫹ cƒLƒTƒ)[cmI ⫹ cƒTƒ]⫺1,

(9.1.51)

Tƒ ⫽ [I ⫹ S(MmLƒ ⫺ I)]⫺1

(9.1.52)

where

is the strain concentration tensor (7.2.4). In conjunction with the deﬁnitions of the engineering constants, (9.1.51) leads to EL ⫽ [c ⫹ (1 ⫺ c)]Em ⫹

2c(1 ⫺ c)(ƒ ⫺ m)2Em , (1 ⫺ c)(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)[1 ⫹ c(1 ⫺ 2m)] (9.1.53)

KT ⫽

{(1 ⫺ c)(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)[1 ⫹ c(1 ⫺ 2m)]}Em , 2(1 ⫹m)[(1 ⫹ ƒ)(1 ⫺ 2ƒ)(c ⫹ 1 ⫺ 2m) ⫹ (1 ⫺ c)(1 ⫹ m)(1 ⫺ 2m)] (9.1.54)

T ⫽

[(1 ⫺ c)(1 ⫹ ƒ) ⫹ (1 ⫹ m)[c ⫹ (3 ⫺ 4m)]Em , 2(1 ⫹ m){(1 ⫺ c)(1 ⫹ m)(3 ⫺ 4m) ⫹ (1 ⫹ ƒ)[1 ⫹ c(3 ⫺ 4m)]} (9.1.55)

L ⫽

[(1 ⫹ c)(1 ⫹ m) ⫹ (1 ⫺ c)(1 ⫹ ƒ)]Em , 2(1 ⫹ m)[(1 ⫺ c)(1 ⫹ m) ⫹ (1 ⫹ c)(1 ⫹ ƒ)]

(9.1.56)

9.1

LT ⫽

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

225

2c(1 ⫺ 2m)ƒ ⫹ (1 ⫺ c)[(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)]m , 2c(1 ⫺ m2 ) ⫹ (1 ⫺ c)[(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)] (9.1.57)

where c ⫽ cƒ is the ﬁber volume fraction, and ⫽

Eƒ . Em

The other engineering constants can be obtained through their relationships discussed earlier. For example, the transverse Young modulus ET can be obtained from (9.1.23) based on the above equations. Unfortunately, the expression for ET is extremely complex. We will not reproduce it here. By neglecting the difference in Poisson’s ratio between the ﬁber and the matrix, that is, m ⫽ ƒ ⫽ , we have EL ⫽ [c ⫹ (1 ⫺ c)]Em, KT ⫽

(9.1.58)

[1 ⫹ ⫺ 2 ⫺ c(1 ⫺ 2)(1 ⫺ )]Em , 2(1 ⫹ )(1 ⫺ 2)[1 ⫺ c( ⫺ 1) ⫹ ⫺ 2]

(9.1.59)

[1 ⫺ c(1 ⫺ ) ⫹ (3 ⫺ 4)]Em , 2(1 ⫹ )[1 ⫹ (3 ⫺ 4)(c ⫹ (1 ⫺ c))]

(9.1.60)

Em[(1 ⫺ c) ⫹ (1 ⫹ c)] , 2(1 ⫹ )[(1 ⫹ c) ⫹ (1 ⫺ c)]

(9.1.61)

T ⫽

L ⫽

LT ⫽ .

(9.1.62)

Even in this case, the expression for ET is still too long to be recorded here. However, the following expression seems to give a pretty good approximation for most of the materials of practical interest: ET ⬇

2(1 ⫺ c) ⫹ (1 ⫹ 2c) E . (1 ⫺ c) ⫹ (2 ⫹ c) m

(9.1.63)

For the dilute case (c ⬍⬍ 1), the following expression for ET can be derived:

226

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

ET ⫽

Em c ⫹ (1 ⫺ c) c(1 ⫺ )2[1 ⫺ 2 ⫹ 2 2(3 ⫺ 4) ⫹ 2(1 ⫺ 3 ⫹ 5 2 ⫺ 23]Em ⫹ , (1 ⫹ ⫺ 2)(1 ⫹ 3 ⫺ 4)

(9.1.64)

Generally speaking, the solutions from upper and lower bounds, as well as the ones from the Mori–Tanaka methods are approximate. Using the composite cylinder model, see Section 8.1, the exact relationships between the effective engineering constants and the moduli of the ﬁbers and the matrix can be obtained (Christensen, 1979); see (8.1.8)–(8.1.11). Note that the composite cylinder model does not yield the exact solution for the transverse shear modulus T . In the event that m ⫽ ƒ ⫽ , (8.1.8)–(8.1.11) reduce to (9.1.58)– (9.1.62). In other words, the Mori–Tanaka estimate gives the exact solution when m ⫽ ƒ ⫽ .

9.2 EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

In this section, we consider a ﬁber-reinforced composite material consisting of multiple layers. Each layer is assumed to be a unidirectional ﬁber-reinforced composite. The bonding between the layers is assumed perfect, that is, the displacement and tractions across the interfaces are continuous. We further assume that the thickness of the layers is much greater than the ﬁber diameter. As discussed in Chapter 5, the effective properties of the layered composite can be obtained through a hierarchical approach. First, the effective properties of each layer are evaluated based on the method discussed in the previous section. Once this is done, the effective properties of the layered composite will be estimated by assuming that each layer is a homogeneous, transversely isotropic solid. In other words, the individual ﬁbers are not explicitly accounted for in the second level of homogenization. Instead, only the collective effect of all the ﬁbers in each layer is explicitly included in the effective properties of the laminate. Therefore, when we consider the effective properties of a multilayered composite, we may assume that each later is homogeneous. To facilitate the discussions below, let us ﬁrst deﬁne the following:

9.2

n ⫽

冤 冥

33 23 , 13

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

t ⫽

冤 冥

11 22 , 12

n ⫽

冤 冥 33

223 , 213

t ⫽

227

冤 冥

11 22 . 212

(9.2.1) For the rest of this section, the summation convention is temporarily suspended. Sums will be explicitly indicated by the summation sign. This way, we can rewrite Hooke’s law using the Voigt notation as n ⫽ Cnnn ⫹ Cntt,

t ⫽ Ctnn ⫹ Cttt,

(9.2.2)

where

冤

C34 C44 C45

C35 C45 , C55

冥

C13 Cnt ⫽ C14 C15

冤

C14 C24 C46

C15 C25 , C56

冥

C11 Ctt ⫽ C12 C16

C33 Cnn ⫽ C34 C35 C13 Ctn ⫽ C23 C36

冤

C23 C24 C25

C36 C46 , C56

冥

(9.2.3)

冤

C12 C22 C26

C16 C26 . C66

冥

(9.2.4)

Obviously, Cnn ⫽ (Cnn)T,

Ctt ⫽ (Ctt)T, Ctn ⫽ (Cnt)T.

(9.2.5)

Also, because of the positive deﬁniteness of the Voigt elasticity matrix, we know that Cnn and Ctt are positive deﬁnite matrices. Now, consider a multilayer composite consisting of N layers of homogeneous materials as shown in Figure 9.3. We assume that each layer is homogeneous with its Voigt elastic matrix given by C(k), k ⫽ 1, 2, . . . , N. Therefore, for the kth layer, it follows from (9.2.2) that (k) (k) (k) (k) (k) n ⫽ C nn n ⫹ C nt t ,

(k) (k) (k) (k) ⫽ C (k) t tn n ⫹ C tt t ,

(9.2.6)

where the superscript (k) indicates that the base letter is associated with the kth layer. It is assumed that the representative volume element being considered is under a uniform state of deformation, even though the actual composite may be subjected to arbitrary loading. We further assume that the layers are perfectly bonded together, meaning that the

228

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

x3 hN hk

x1

h

h1

Figure 9.3 Multilayer composite.

traction and displacements are continuous across the layer interfaces. This immediately leads to (k) n ⫽ n,

t(k) ⫽ t,

for k ⫽ 1, 2, . . . , N

(9.2.7)

Making use of (9.2.7) in the ﬁrst of (9.2.6) yields (k) ⫺1 (k) (k) n ⫽ (C nn ) (n ⫺ C nt t).

(9.2.8)

Taking the average of (k) n over the representative volume element leads to

冘 c ⫽ 冘 c (C N

n ⫽

N

(k) k n

k⫽1

k

冘 c (C N

(k) ⫺1 nn

)

n ⫺

k⫽1

k

(k) ⫺1 nn

(k) ) C nt t,

(9.2.9)

k⫽1

where ck ⫽ hk /h is the volume fraction of the kth layer. By rearranging the terms in (9.2.9), we have n ⫽ Cnnn ⫹ Cntt,

(9.2.10)

where

冋冘

Cnn ⫽

k⫽1

册

⫺1

N

(k) ⫺1 nn

ck(C )

,

(9.2.11)

9.2

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

冋冘

册

N

⫺1 (k) ck(C (k) . nn ) C n

Cnt ⫽ Cnn

k⫽1

229

(9.2.12)

We next substitute (9.2.8) into the second of (9.2.6). This gives us (k) (k) ⫺1 (k) (k) ⫽ C tn (C nn ) (n ⫺ C (k) t nt t) ⫹ C tt t (k) (k) ⫺1 (k) ⫺1 (k) ⫽ C tn (C nn ) n ⫹ [C tt(k) ⫺ C (k) tn (C nn ) C2 nt ]t.

(9.2.13)

Taking the average of (k) t over the representative volume element leads to

冘 c ⫽ 冘 c C (C ) ⫹ 冘 c [C ⫺ C (C ) C ] . N

t ⫽

N

k

(k) t

(k) ⫺1 nn

(k) tn

k

n

k⫽1

k⫽1

N

(k) tt

k

(k) tn

(k) ⫺1 nn

(k) nt

t

(9.2.14)

k⫽1

Substitution of (9.2.10) into the above yields t ⫽ Ctnn ⫹ Cttt,

(9.2.15)

where

冋冘 c C

册

N

Ctn ⫽

k

(k) ⫺1 (C nn ) Cnn,

(k) tn

k⫽1

冘 N

Ctt ⫽

冘 cC

(9.2.16)

N

ckC tt(k) ⫹

k⫽1

k

(k) ⫺1 (k) (C nn ) (Cnt ⫺ C nt ).

(k) tn

(9.2.17)

k⫽1

Clearly, Cnn, Cnt, Ctn, and Ctt provide the complete effective Voigt elastic matrix of the layered composite. Taking advantage of the symmetry properties (9.2.5), it can be shown that Cnn ⫽ (Cnn)T,

Ctt ⫽ (Ctt)T,

Ctn ⫽ (Cnt)T.

Next, we assume that each layer is a monoclinic material with its plane of symmetry in the x1x2 plane. In this case, the Voigt elastic matrix has the following form:

230

C

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

(k) nn

冤

冥

C (k) 0 0 33 (k) ⫽ 0 C 44 C (k) 45 , (k) 0 C (k) C 45 55

C

(k) tn

C

⫽ (C ) , (k) T nt

C

冤

冥

(k) (k) (k) C 13 C 23 C 36 ⫽ 0 0 0 , 0 0 0

(k) nt

冤

冥

C (k) C (k) C (k) 11 12 16 (k) (k) (k) ⫽ C 12 C 22 C 26 . (k) (k) (k) C 16 C 26 C 66

(k) tt

(9.2.18)

(9.2.19)

Substituting these into (9.2.11) and (9.2.12) yields

冘 Cc

冤 冉 冤

k (k) 33

k⫽1

Cnn ⫽

⫽

0

0

⫺

(k)

k

k⫽1 N

(k) k 45 (k)

k⫽1

冘 Cc 冊

冘 c⌬C 冘 c⌬C N

(k) ckC 55

k⫽1 N

0

0

冘⌬ cC ⫺冘 ⌬ N

k

k⫽1

(k) 45 (k)

(k) 44 (k)

N

k (k) 33

k⫽1

冥

⫺1

N

0 1 D 1 D

0 0

0

冘⌬ 冘 c⌬C N

(k) ckC 44 (k)

k⫽1 N

k

k⫽1

1 D 1 D

(k) 45 (k)

冘 c⌬C 冘 c⌬C N

冥

k

(k) 45 (k)

k

(k) 55 (k)

k⫽1 N k⫽1

,

(9.2.20)

where

冘 N

D⫽

ckC (k) 55 ⌬(k)

k⫽1

冘 N

k⫽1

(k) ckC 44

⌬(k)

冋冘 册 N

⫺

k⫽1

(k) ckC 45

⌬(k)

2

,

(k) (k) (k) 2 ⌬(k) ⫽ C 44 C 55 ⫺ (C 45 ) ⬎ 0.

(9.2.21) (9.2.22)

Next, making use of (9.2.20) in (9.2.16) yields

冉冘 冊 N

Ctn ⫽

k⫽1

Finally, (9.2.17) leads to

ck C (k) 33

⫺1

冘 N

k⫽1

冤

(k) 0 13 ck C (k) C 0 23 (k) C 33 (k) C 36 0

冥

0 0 . 0

(9.2.23)

9.2

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

冤

冘

k⫽1

冘 N

⫺

k⫽1

冤

冥

(k) (k) (k) (k) (k) (k) C 23 C 13 C 36 C 13 13 C 13 ck C (k) (k) (k) (k) (k) (k) C C C C C 13 23 23 23 36 C 23 C (k) (k) (k) (k) (k) (k) 33 C (k) C C C C 13 36 23 36 36 C 36

冉冘 冊 N

⫹

冥

(k) (k) (k) C 11 C 12 C 16 (k) (k) (k) ck C 12 C 22 C 26 (k) (k) (k) C 16 C 26 C 66

N

Ctt ⫽

231

r⫽1

cr (r) C 33

⫺1

冘 冘 C c cC N

N

m k (m) (k) 33 33

k⫽1 m⫽1

冤

冥

(k) (k) (k) C (m) C (m) C (m) 13 C 13 23 C 13 36 C 13 (m) (k) (m) (k) (m) (k) ⫻ C 13 C 23 C 23 C 23 C 36 C 23 . (k) (k) (k) C (m) C (m) C (m) 13 C 36 23 C 36 36 C 36

(9.2.24)

If we let Cij be the elements of the 6 ⫻ 6 Voigt effective elastic matrix C, results from (9.2.20), (9.2.23), and (9.2.24) can be summarized as follows:

冘 c 冋C N

Cij ⫽

k

(k) ij

⫺

k⫽1

(k) C (k) C (k) i3 C j3 i3 ⫹ (k) C (k) C 33 33

冉冘 Cc 冊 冋 冘 cCC ⫺1

N

r⫽1

N

m

r (r) 33

m⫽1

册册

(m) 3j (m) 33

(9.2.25) for i, j ⫽ 1, 2, 3, 6: Cij ⫽

1 D

⫽0

冘 c⌬C N

k

k⫽1

(k) ij (k)

for i, j ⫽ 4, 5,

for i ⫽ 1, 2, 3, 6;

(9.2.26)

j ⫽ 4, 5.

(9.2.27)

Similarly, the compliance matrix can be partitioned as

冤

冥

S13 S23 S36 Snt ⫽ S14 S24 S46 , S15 S25 S56

冤

冥

S11 S12 S16 Stt ⫽ S12 S22 S26 , S16 S26 S66

S33 S34 S35 Snn ⫽ S34 S44 S45 , S35 S45 S55 S13 S14 S15 Stn ⫽ S23 S24 S25 , S36 S46 S56

冤

冥

(9.2.28)

冤

冥

(9.2.29)

232

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

Following the same procedure, elements of the effective compliance matrix are given by (see Appendix 9.A)

冥 冋冘

冤

S11 S12 S16 Stt ⫽ S12 S22 S26 ⫽ S16 S26 S66

⫺1 ck(S (k) tt )

k⫽1

冥 冋冘 冥 冋冘

冤

S13 S14 S15 Stn ⫽ S23 S24 S25 ⫽ Stt S36 S46 S56

冤

S13 S23 S36 Snt ⫽ S14 S24 S46 ⫽ S15 S25 S56

冤

冥

S33 S34 S35 Snn ⫽ S34 S44 S45 ⫽ S35 S45 S55

冘

册

⫺1

N

,

(9.2.30)

册

N

⫺1 (k) ck(S (k) tt ) S tn ,

k⫽1

册

N

(k) ck S nt (S tt(k))⫺1 Stt,

k⫽1

N

冘cS

(9.2.31)

(9.2.32)

N

(k) ck S nn ⫹

k⫽1

k

(k) (S tt(k))⫺1(Stn ⫺ S tn ).

(k) nt

k⫽1

(9.2.33) Example 9.1 Consider a layered material consisting of two alternating layers. The layers are identical, except that the ﬁber directions are perpendicular to each other between adjacent layers. We are to ﬁnd the effective elastic constants for this layered composite. To this end, let us denote the Voigt elasticity matrix for the layer whose ﬁber direction is in the x1 direction by

C (1) ⫽

冤

C11

C12 C12

0

0

0

C12

C22

C23

0

0

0

C12

C23

C22

0

0

0

0

0

0

0

0

0

0

0

0

C22 ⫺ C23 0 2 0 C66 0

0

冥

.

0 0

(9.2.34)

C66

A 90⬚ rotation about the x3 axis yields the Voigt elasticity matrix for the adjacent layer:

9.2

C (2) ⫽

冤

233

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

C22

C12

C23

0

0

0

C12

C11

C12

0

0

0

C23

C23

C22

0

0

0

0

0

0

C66

0

0

0

0

0

0

0

0

0

0

冥

.

C22 ⫺ C23 2 0

0

(9.2.35)

C66

Making use of these in (9.2.25)–(9.2.27) with N ⫽ 2, c1 ⫽ c2 ⫽ –12 , we arrive at (k) (k) ⌬(k) ⫽ C 44 C 55 ⫽

(C22 ⫺ C23)C66 , 2

D⫽

冉

冊

2

1 2 1 ⫹ . 4 C22 ⫺ C23 C66 (9.2.36)

Thus, the nonzero components of the effective Voigt elasticity matrix of the layered composite are C11 ⫽ C22 ⫽

C33 ⫽ C22, C13 ⫽ C23 ⫽

C44 ⫽ C55 ⫽

冋

册

1 (C ⫺ C23)2 C11 ⫹ C22 ⫺ 12 , 2 2C22 C12 ⫽ C12 ⫺

(9.2.37)

(C12 ⫺ C23)2 , 4C22

C12 ⫹ C23 , 2

(9.2.38)

2C66(C22 ⫺ C23) , 2C66 ⫹ (C22 ⫺ C23)

C66 ⫽ C66.

(9.2.39)

Making use of (9.2.30), the in-plane Young modulus and shear modulus can be written in terms of the engineering constants of the individual layer: E0 ⫽

(EL ⫹ ET)2 ⫺ 4E 2L 2TL , 2(EL ⫹ ET)(1 ⫺ LTTL)

0 ⫽

2EL . EL ⫹ ET TL

(9.2.40)

234

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

9.3 EFFECTIVE PROPERTIES OF A LAMINA

In the composite material literature, a lamina is a thin layer of unidirectional ﬁber-reinforced composite material; see Figure 9.4. Because the thickness is much smaller relative to the in-plane dimensions, the deformation of a lamina can be approximated by a state of plane stress. This means 13 ⬇ 23 ⬇ 33 ⬇ 0.

(9.3.1)

It thus follows from Hooke’s law that L13klkl ⫽ L23klkl ⫽ L33klkl ⫽ 0.

(9.3.2)

For a lamina, the effective elasticity tensor is transversely isotropic with the axis of symmetry being the x1 axis, as shown in Figure 9.3, the above equation yields 13 ⫽ 23 ⫽ 0

L l and 33 ⫽ ⫺ 1311 11 ⫺ 1322 22. L3333 L3333

(9.3.3)

Substituting the above into Hooke’s law again, we arrive at

冉 冉

冊 冉 冊 冉

冊 冊

11 ⫽ L1111 ⫺

L1311 L 11 ⫹ L1122 ⫺ 1322 22, L3333 L3333

(9.3.4)

22 ⫽ L2211 ⫺

L1311 L 11 ⫹ L2222 ⫺ 1322 22. L3333 L3333

(9.3.5)

Therefore, in the reduced form of the Voigt notation, the stress–strain relationship for a thin lamina can be written as x3 x2 x1

Figure 9.4 Thin lamina.

9.3

EFFECTIVE PROPERTIES OF A LAMINA

冤冥 冤 1 2 6

冥冤 冥

Q11 Q12 0 Q12 Q22 0 0 0 Q66

⫽

1 2 , 6

235

(9.3.6)

where

冤冥 冤 冥 冤冥 冤 冥 1 2 6

⫽

11 22 , 12

1 2 6

11 22 , 212

(9.3.7)

i, j ⫽ 1, 2, 6

(9.3.8)

⫽

and Qij ⫽ Cij ⫺

Ci3Cj3 , C33

with Cij being the Voigt elastic constants of the lamina. Note that Cij is transversely isotropic so that C63 ⫽ 0. Thus, Q66 ⫽ C66. The matrix Q in (9.3.6) is called the reduced stiffness matrix of the lamina. The reduced compliance matrix S (not to be confused with the Eshelby tensor) for the lamina is obtained by inverting (9.3.6),

冤冥 冤 1 2 6

⫽

S11 S12 0 S12 S22 0 0 0 S66

冥冤 冥

1 2 , 6

(9.3.9)

where S11 ⫽

Q22 , 2 Q11Q22 ⫺ Q12

S22 ⫽

Q12 S12 ⫽ ⫺ , 2 Q11Q22 ⫺ Q12

Q11 , 2 Q11Q22 ⫺ Q12 S66 ⫽

1 . Q66

(9.3.10)

(9.3.11)

The Young moduli in the ﬁber and transverse to the ﬁber directions can thus be deﬁned, respectively, as EL ⫽

2 1 Q Q ⫺ Q12 ⫽ 11 22 , S11 Q22

ET ⫽

1 Q Q ⫺ Q212 ⫽ 11 22 . S22 Q11

The shear modulus in the plane of the lamina is

(9.3.12)

236

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

L ⫽ Q66.

(9.3.13)

The corresponding Poisson ratios are S Q LT ⫽ ⫺ 12 ⫽ 12, S11 Q22

S Q TL ⫽ ⫺ 12 ⫽ 12. S22 Q11

(9.3.14)

Note that LT represents the contraction in the transverse direction when the lamina is stretched in the ﬁber direction, while TL represents the contraction in the ﬁber direction when the lamina is stretched in the transverse direction. These are exactly the same engineering elastic constants as introduced in Section 9.1. As discussed in Section 9.1, only four of these engineering elastic constants are independent because 2 Q12(Q11Q22 ⫺ Q12 ) ⫽ TLEL. Q11Q22

LT ET ⫽

(9.3.15)

Therefore, (9.3.12)–(9.3.14) can be inverted to obtain Q11 ⫽

EL , 1 ⫺ LTTL

Q22 ⫽

Q12 ⫽

ET , 1 ⫺ LTTL

Q66 ⫽ L,

LTET TLEL ⫽ . 1 ⫺ LTTL 1 ⫺ LTTL

(9.3.16)

(9.3.17)

The corresponding components of the reduced compliance tensor are S11 ⫽

1 , EL

S22 ⫽

1 , ET

S66 ⫽

S12 ⫽ ⫺ LT ⫽ ⫺ TL. EL ET

1 , L

(9.3.18)

(9.3.19)

Equations (9.3.6) and (9.3.9) are written in a coordinate system where the x1 axis is in the direction of the ﬁbers. In the coordinate system xˆ i shown in Figure 9.2, where the xˆ 1 axis forms an angle from the ﬁber direction, the stress–strain relationship becomes

9.3

冤冥 冤 x y xy

ˆ 11 Q ˆ 12 ⫽ Q ˆ 13 Q

EFFECTIVE PROPERTIES OF A LAMINA

ˆ 12 Q ˆ 22 Q ˆ 23 Q

ˆ 13 Q ˆ 23 Q ˆ 66 Q

冥冤 冥

x y , ␥xy

237

(9.3.20)

where ˆ 11 ⫽ Q11m4 ⫹ 2(Q12 ⫹ 2Q66)m2n2 ⫹ Q22n4, Q

(9.3.21)

ˆ 22 ⫽ Q11n4 ⫹ 2(Q12 ⫹ 2Q66)m2n2 ⫹ Q22m4, Q

(9.3.22)

ˆ 12 ⫽ (Q11 ⫹ Q22 ⫺ 4Q66)m2n2 ⫹ Q12(m4 ⫹ n4), Q

(9.2.23)

ˆ 16 ⫽ (Q11 ⫺ Q12 ⫺ 2Q66)m3n ⫹ (Q12 ⫺ Q22 ⫹ 2Q66)mn3, Q

(9.3.24)

ˆ 26 ⫽ (Q11 ⫺ Q12 ⫺ 2Q66)mn3 ⫹ (Q12 ⫺ Q22 ⫹ 2Q66)m3n, Q

(9.3.25)

ˆ 66 ⫽ (Q11 ⫹ Q22 ⫺ 2Q12 ⫺ 2Q66)m2n2 ⫹ Q66(m4 ⫹ n4), Q

(9.3.26)

in which m ⫽ cos , n ⫽ sin . Since the lamina is very thin, its deformation can be represented by the deformation of its midplane using the Kirchhoff assumption, that is, a cross-section plane perpendicular to the midplane prior to the deformation remains perpendicular to the midplane after deformation. Mathematically, this means x ⫽

⭸u0 ⭸2w0 ⫺z , ⭸x ⭸x 2

␥xy ⫽ 2xy ⫽

y ⫽

⭸0 ⭸2w0 ⫺z , ⭸y ⭸y 2

⭸u0 ⭸ ⭸2w0 ⫹ 0 ⫺ 2z , ⭸y ⭸x ⭸x⭸y

(9.3.27)

(9.3.28)

where u0 and 0 are the in-plane displacement of the midplane and w0 is the out-of-plane displacement (deﬂection) of the midplane of the lamina. The coordinate z indicates the location relative to the middle plane. Substitution of (9.3.27) and (9.3.28) into (9.3.20) yields

238

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

冤冥 冤 x y xy

ˆ 11 Q ˆ 12 ⫽ Q ˆ 13 Q

冥冤 冥 冤

ˆ 12 Q ˆ 22 Q ˆ 23 Q

ˆ 13 Q ˆ 23 Q ˆ 66 Q

x0 y0 0 ␥ xy

ˆ 11 Q ˆ 12 Q ˆ 12 Q ˆ 22 ⫹z Q ˆ 13 Q ˆ 23 Q

冥冤 冥

ˆ 13 Q ˆ 23 Q ˆ 66 Q

kx ky , kxy (9.3.29)

where

0x y0 ␥ 0xy

冤 冥

冤 冥

(9.3.30)

冤冥

(9.3.31)

⭸u0 ⭸x

⫽

⭸0 ⭸y

⭸u0 ⭸ ⫹ 0 ⭸y ⭸x

is the midplane strain and

冤冥

kx ky ⫽ ⫺ kxy

⭸2w0 ⭸y 2 ⭸2w0 ⭸y 2

2

⭸2w0 ⭸x⭸y

is the midplane curvature.

9.4 EFFECTIVE PROPERTIES OF A LAMINATED COMPOSITE PLATE

Composite laminates in engineering applications typically consist of multiple unidirectional ﬁber-reinforced laminas (or plies) stacked up together. The stacking sequence of a laminate can be designated by a standard notation. For example, [02 /902 / ⫺453 /453]s is used to designate a laminate that starting from the bottom, that is, at z ⫽ ⫺h/2 (h is the total thickness of the laminate), there are two plies at 0⬚ orientation ( ⫽ 0⬚), two plies at 90⬚ orientation, followed by three plies at ⫺45⬚, and last three plies at ⫹45⬚ orientation. The subscript s indicates that the laminate is symmetrical with respect to the midplane (z ⫽ 0), that is, the top half of the laminate is a mirror image of the bottom

9.4

239

EFFECTIVE PROPERTIES OF A LAMINATED COMPOSITE PLATE

half. For nonsymmetrical laminates, the total stacking sequence needs to be explicitly indicated. In this case, a subscript T will be used. For most engineering laminates of practical interest, the thickness of each ply is in the order of millimeters. The diameter of the ﬁber is typically in the order of micrometers. To bridge these two length scales, we will take a hierarchical approach in order to estimate the effective properties of the laminate. First, the effective properties of the unidirectional ply are evaluated based on the method discussed in the previous chapter. Once this is done, the effective properties of the laminate will be estimated by assuming each ply as a homogeneous, transversely isotropic layer. Now consider a generic laminate shown in Figure 9.3. We assume that the bonding between the plies is perfect, that is, displacements and tractions are continuous across the ply interfaces. Since the stresses in a laminate vary from layer to layer, it is convenient to introduce the resultant forces and moments:

冤 冥

Nx Ny ⫽ Nxy

冕

h/2

⫺h / 2

冤冥 x y xy

冤 冥

Mx My ⫽ Mxy

dz,

冕

h/2

⫺h / 2

冤冥

x y z dz. xy

(9.4.1)

In terms of the resultants, (9.3.29) can be rewritten as

冤 冥 冤

Nx A11 Ny ⫽ A12 Nxy A13

A12 A22 A23

A13 A23 A66

冥冤 冥 冤 x0 0y 0 ␥ xy

B11 B12 B13 B22 B23 B13 B23 B66

⫹ z B12

冥冤 冥

kx ky , kxy (9.4.2)

冤 冥 冤

Mx B11 My ⫽ B12 Mxy B13

B12 B22 B23

冥冤 冥 冤 x0 0y 0 ␥ xy

B13 B23 B66

D11 ⫹ z D12 D13

D12 D22 D23

D13 D23 D66

冥冤 冥

kx ky , kxy (9.4.3)

where

冘 (Qˆ ) (h ⫺ h n

Aij ⫽

ij k

k

),

(9.4.4)

2 k⫺1

(9.4.5)

k⫺1

k⫽1

1 Bij ⫽ 2

冘 (Qˆ ) (h ⫺ h n

ij k

k⫽1

2 k

),

240

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

x3 x2 x1

Figure 9.5

Dij ⫽

1 3

冘 (Qˆ ) (h ⫺ h n

ij k

3 k

3 k⫺1

)

(9.4.6)

k⫽1

are called the extensional stiffness matrix, coupling stiffness matrix, and bending stiffness matrix of the laminate, respectively. PROBLEMS

9.1 Consider a unidirectional ﬁber-reinforced composite plate as shown in Figure 9.5 (ﬁbers are in the x1 direction). Find the lower and upper bounds for the effective Young modulus E11 and E22 by using the minimum potential and minimum complementary energy theorems, respectively. Compare your results with the rule of mixture predictions. (Hint: Use 0ij ⫽ 0␦i1␦j1 and 0ij ⫽ 0␦i1␦j1 for E11. Use ij0 ⫽ 0␦i2␦j2 and 0ij ⫽ 0␦i2␦j2 for E22.) 9.2 Derive the extensional stiffness matrix, the coupling stiffness matrix, and the bending stiffness matrix of a generic laminate. 9.3 Prove (9.2.29)–(9.2.32). 9.4 Consider a ﬁber-reinforced cross-ply laminate as shown in Figure 9.4. Further, assume that all the layers have the same thickness and their elastic constants are given by EL, ET, L, LT, and TL. They are related to the elastic properties of the ﬁber, the matrix, and the ﬁber volume fraction through the micromechanics schemes discussed in Section 9.1. Find the matrices A, B, and D as deﬁned in (9.4.6)–(9.4.8).

APPENDIX 9.A

To facilitate the discussions below, let us ﬁrst deﬁne the following:

APPENDIX 9.A

n ⫽

冤 冥

33 23 , 13

t ⫽

冤 冥

11 22 , 12

n ⫽

冤 冥 33

223 , 213

t ⫽

241

冤 冥

11 22 . 212

(9.A.1) Thus, we have n ⫽ Sntt ⫹ Snnn,

t ⫽ Sttt ⫹ Stnn,

(9.A.2)

where

冤

冥

S13 S23 S36 Snt ⫽ S14 S24 S46 , S15 S25 S56

冤

冥

S11 S12 S16 Stt ⫽ S12 S22 S26 . S16 S26 S66

S33 S34 S35 Snn ⫽ S34 S44 S45 , S35 S45 S55 S13 S14 S15 Stn ⫽ S23 S24 S25 , S36 S46 S56

冤

冥

(9.A.3)

冤

冥

(9.A.4)

Obviously, Snn ⫽ (Snn)T,

Stt ⫽ (Stt)T, Stn ⫽ (Snt)T.

(9.A.5)

Also, because of the positive deﬁniteness of the Voigt compliance matrix, we know that Snn and Stt are positive deﬁnite matrices. Now, consider a multilayered composite consisting of N layers of homogeneous materials as shown in Figure 9.3. We assume that each layer is homogeneous with its Voigt elastic matrix given by S(k), k ⫽ 1, 2, . . . , N. Therefore, for the kth layer, it follows from (9.A.2) that (k) (k) (k) (k) (k) n ⫽ S nn n ⫹ S nt t ,

(k) (k) t(k) ⫽ S tn n ⫹ S tt(k) t(k),

(9.A.6)

where the superscript (k) indicates the quantity associated with the kth layer. It is assumed that the representative element being considered is under a uniform state of deformation, even though the actual composite may be subjected to arbitrary loading. We further assume that the layers are perfectly bonded together, meaning that the traction and displacements are continuous across the layer interfaces. This immediately leads to

242

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

(k) n ⫽ n,

t(k) ⫽ t,

for k ⫽ 1, 2, . . . , N.

(9.A.7)

Making use of the above in the second of (9.A.6) yields ⫺1 (k) (k) ⫽ (S (k) t tt ) (n ⫺ S tn n).

(9.A.8)

Taking the average of (k) t over the representative volume element leads to

冘 c N

n ⫽

k

冘 c (S N

(k) t

⫽

k

)

t ⫺

k⫽1

k⫽1

冘 c (S N

(k) ⫺1 tt

k

(k) ⫺1 tt

(k) ) S tn n,

(9.A.9)

k⫽1

where ck ⫽ hk /h is the volume fraction of the kth layer. By rearranging the terms in (9.A.9), we have t ⫽ Sttt ⫹ Stnn,

(9.A.10)

where

冤

冥

S11 S12 S16 Stt ⫽ S12 S22 S26 ⫽ S16 S26 S66

冋冘 c (S k

冥 冋冘

冤

(k) ⫺1 tt

)

k⫽1

S13 S14 S15 Stn ⫽ S23 S24 S25 ⫽ Stt S36 S46 S56

册

⫺1

N

,

(9.A.11)

册

N

⫺1 (k) ck(S (k) tt ) S tn .

k⫽1

(9.A.12)

We next substitute (9.A.8) into the ﬁrst of (9.A.6). This gives us (k) (k) (k) ⫺1 (k) (k) (k) ⫺1 (k) n ⫽ [S nn ⫺ S nt (S tt ) S tn ]n ⫹ S nt (S tt ) t.

(9.A.13)

Taking the average of (k) t over the representative volume element leads to

冘 c ⫽ 冘 c [S N

n ⫽

N

(k) k n

k⫽1

k

冘cS N

(k) nn

(k) ⫺1 tt

⫺ S (S ) S ]n ⫹ (k) nt

(k) tn

k⫽1

Substitution of (9.A.10) into the above yields

k

k⫽1

⫺1 (S (k) tt ) t.

(k) nt

REFERENCE

n ⫽ Snnn ⫹ Sntt,

243

(9.A.14)

where

冥 冋冘

冤

S13 S23 S36 Snt ⫽ S14 S24 S46 ⫽ S15 S25 S56

冤

冥

S33 S34 S35 Snn ⫽ S34 S44 S45 ⫽ S35 S45 S55

冘cS

(k) ck S nt (S tt(k))⫺1 Stt,

k⫽1

N

k

册

N

冘cS

(9.A.15)

N

(k) nn

⫹

k⫽1

k

(k) (S tt(k))⫺1(Stn ⫺ S tn ).

(k) nt

k⫽1

(9.A.16) Clearly, Snn, Snt, Stn, and Stt provide the complete effective Voigt compliant matrix of the layered composite. Taking advantage of the symmetry properties (9.A.5), it can be shown that Snn ⫽ (Snn)T,

Stt ⫽ (Stt)T,

Stn ⫽ (Snt)T.

Next, we assume that each layer is a monoclinic material with its plane of symmetry in the x1x2 plane. In this case, the Voigt elastic matrix has the following forms:

(k) S nn

冤

冥

S (k) 0 0 33 (k) (k) ⫽ 0 S 44 S 45 , (k) (k) 0 S 45 S 55

S

(k) tn

⫽ (S ) , (k) T nt

(k) S nt

S

(k) tt

冤

冥

(k) (k) (k) S 13 S 23 S 36 ⫽ 0 0 0 , 0 0 0

(9.A.17)

冤

(9.A.18)

冥

(k) (k) (k) S 11 S 12 S 16 (k) (k) (k) ⫽ S 12 S 22 S 26 . (k) (k) (k) S 16 S 26 S 66

REFERENCE Christensen, R. M. (1979). Mechanics of Composite Materials, Krieger, Malabar, FL.

244

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

SUGGESTED READINGS Agarwal, B. D. and L. J. Broutman. (1990). Analysis and Performance of Fiber Composites, Wiley, New York. Chawla, K. K. (1987). Composite Materials—Science and Engineering, Springer, New York. Hyer, M. W. (1998). Stress Analysis of Fiber-Reinforced Composite Materials, McGraw-Hill, Boston.

10 BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES Micromechanics has been used extensively in the study of damage and failure of engineering materials. There is a large body of literature in this area. It is certainly not possible, nor the intent of this chapter, to provide an extensive summary of existing results. The objective here is to take a few examples that are illustrative of how the micromechanics methods and techniques are being used to understand and model certain commonly seen damage and failure modes in engineering composite materials. We will discuss one example in each of the three areas; interfaces, ﬁber, and matrix.

10.1 IMPERFECT INTERFACES

Let the interface between two media be denoted by S. As discussed in Section 4.2, we call an interface S a perfect interface if the two media are mechanically coherent, that is, the displacement and traction ﬁelds are continuous across this interface. The continuity of displacement and traction across a perfect interface can be written as ⌬ui ⬅ ui(S⫹) ⫺ ui(S⫺) ⫽ 0,

(10.1.1)

⌬ij nj ⬅ [ij(S⫹) ⫺ ij(S⫺)]nj ⫽ 0,

(10.1.2)

where nj is the unit normal vector of the interface S, and ui(S⫹) and ij(S⫹) are the values of ui(x) and ij(x) evaluated at the positive side Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

245

246

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

of S, while ui(S⫺) and ij(S⫺) are the values of ui(x) and ij(x) evaluated at the negative side of S. It is assumed that nj points to the positive side of S; see Figure 4.3. In many engineering applications, the interfaces in a composite material may not be perfect. In this section, we will discuss one of the simplest models used to model the imperfect interfaces. For quasi-static problems, the imperfection of interfaces is reﬂected mainly by the discontinuity of displacement ﬁeld across the interface. The interfacial spring model therefore postulates that the traction is continuous across the interface ⌬ij nj ⬅ [ij(S⫹) ⫺ ij(S⫺)]nj ⫽ 0,

(10.1.3)

but the displacement ﬁeld is discontinuous. The jump in the displacement ﬁeld across the interface is proportional to the traction vector on the interface, that is, ⌬ui ⬅ ui(S⫹) ⫺ ui(S⫺) ⫽ ijik nk,

(10.1.4)

where the second-order tensor ij represents the compliance of the interface. For simplicity, we assume that ij is symmetric and positive deﬁnite. It is clear from (10.1.4) that ij ⫽ 0 corresponds to a perfect interface, while ij → ⬁ represents complete debond (ik nk ⫽ 0). From this point of view, a slight deviation from the perfect interface case can be modeled by the limit of ij → 0. A special form of ij that has some physical signiﬁcance is given by ij ⫽ ␣␦ij ⫹ ( ⫺ ␣)ninj.

(10.1.5)

It can be easily shown that ␣ and  represent the compliance in the tangential and normal directions of the interfaces, respectively, that is, ⌬ui(␦ik ⫺ ni nk) ⫽ ␣ij nj(␦ik ⫺ ni nk),

(10.1.6)

⌬ui ni ⫽ ij nj ni.

(10.1.7)

When  ⫽ 0, such constitutive characterization of the interfaces allows for relative sliding between the two surfaces, but not separation. Furthermore, the free-sliding case studied by Mura (1987) can be achieved by setting ␣ → ⬁ with  ⫽ 0. Therefore, solutions to the case of small ␣ with  ⫽ 0 provide the approximations in contrast to the sliding interface. It also should be mentioned that material interpenetration

10.1

IMPERFECT INTERFACES

247

may take place when  ⫽ 0, which is a violation of the compatibility requirement. Further discussions on this may be found in Achenbach and Zhu (1989). For the remainder of this section, we focus on the effective elastic properties of composite materials with imperfect interfaces. First, we will solve the Eshelby inclusion problem with imperfect interface. Then, we will use the Mori–Tanaka approach to estimate the effective elastic properties. Finally, the bounds of the effective properties for such composite will be developed based on the classical variational principles. Consider an elastic solid of inﬁnite extent containing an ellipsoidal inclusion ⍀ with eigenstrain distribution ij*. Assume that the interface between the inclusion and the surrounding medium is imperfect and the displacement jump across the interface is governed by (10.1.6) and (10.1.7). We will call this eigenstrain problem the modiﬁed Eshelby inclusion problem. In what follows, we would like to develop a solution to this modiﬁed Eshelby inclusion problem. It follows from (3.3.5) that the displacement ﬁeld should satisfy the following equations of equilibrium: Lijkl uk,lj(x) ⫺ Lijkl *kl, j(x) ⫽ 0 ui(x) → 0

in ⍀.

as 兩x兩 → ⬁.

(10.1.8) (10.1.9)

Furthermore, it follows from (2.6.23) and (2.6.24) that the Green function G⬁ij (x, y) satisﬁes Lijkl

⭸2G⬁km(x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0, ⭸xl ⭸xj

(10.1.10)

G⬁ij (x, y) → 0

(10.1.11)

as 兩x兩 → ⬁,

where ␦(x) is the three-dimensional Dirac delta function. Now, let us multiply (10.1.10) by ui(x) and integrate the resulting equation over a volume V. This leads to

冕 u (x)L V

i

ijkl

⭸2G⬁km(x, y) dV(x) ⫽ ⭸xl ⭸xj

再

⫺um(y)

0

y僆V . yⰻV

(10.1.12)

By using the divergence theorem, we can rewrite the volume integral in (10.1.12) as

248

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冕 u (x)L ⭸ G⭸x (x,⭸x y) dV(x) ⭸G (x, y) ⫽ 冕 u (x)L n dS(x) ⫺ 冕 u (x)L ⭸x 2

km

i

V

ijkl

l

j

km

i

S

ijkl

j

V

l

i, j

ijkl

⭸Gkm(x, y) dV(x), ⭸xl

(10.1.13) where S is the surface of V, and ni is the unit outward normal of S. Next, multiplying (10.1.8) by Gim(x, y) and integrating the result over the volume V lead to

冕 G (x, y)L V

⬁ im

ijkl

uk,lj(x) dV(x) ⫺

冕 G (x, y)L V

⬁ im

* (x) dV(x) ⫽ 0.

ijkl kl, j

(10.1.14) Following the procedures that led to (10.1.13), the ﬁrst volume integral in the above equation can be written as

冕 G (x, y)L u (x) dV(x) ⭸G (x, y) ⫽ 冕 G (x, y)L u (x)n dS(x) ⫺ 冕 L ⭸x ⬁ im

V

ijkl

⬁ im

⬁ im

S

k,lj

ijkl

k,l

j

ijkl

V

uk,l(x) dV(x).

j

(10.1.15) Note that the last volume integral on the right-hand side of (10.1.13) is the same as that of (10.1.15). Therefore, by subtracting (10.1.12) from (10.1.14), we arrive at

冕L S

冋

⬁ Gim (x, y)uk,l(x) ⫺ ui(x)

ijkl

⫺

冕 G (x, y)L V

⬁ im

* (x) dV(x) ⫽

ijkl kl, j

册

⭸G⬁im(x, y) nj dS(x) ⭸xl

再

um(y) 0

y僆V . yⰻV

(10.1.16)

Finally, making use of the divergence theorem on the volume integral, we arrive at

10.1

再

冕L

⬁ Gim (x, y)[uk,l(x) ⫺ *(x)] ⫺ ui(x) kl

ijkl

S

⫹

冕 ⭸G ⭸(x,x y) L ⬁ im

*(x) dV(x) ⫽

ijkl kl

V

l

再

IMPERFECT INTERFACES

冎

⭸G⬁im(x, y) ⭸xl

nj dS(x)

y僆V . yⰻV

um(y) 0

249

(10.1.17)

Now, taking the region V to be the inclusion ⍀, and letting y 僆 ⍀ where the eigenstrain is given, the above integral representation yields um(y) ⫽

冕

S⫺

⫹

再

⬁ Lijkl Gim (x, y)[uk,l(x) ⫺ *(x)] ⫺ ui(x) kl

冕 ⭸G ⭸(x,x y) L ⬁ im

冎

⭸G⬁im(x, y) ⭸xl

*(x) dV(x).

(10.1.18)

ijkl kl

V

nj dS(x)

l

Note that for y 僆 S⫺, Hooke’s law (3.3.2) yields Lijkl[uk,l(x) ⫺ *(x)] ⫽ ij(x). kl

(10.1.19)

Therefore, (10.1.18) can be rewritten as um(y) ⫽

冕

S⫺

⫹

冋

G⬁im(x, y)kl(x) ⫺ ui(x)Lijkl

冕 ⭸G ⭸(x,x y) L ⬁ im

V

册

⭸G⬁im(x, y) ⭸xl

nj dS(x)

*(x) dV(x).

(10.1.20)

ijkl kl

l

Next, take V to be the region exterior to ⍀. Then, for y inside ⍀, or equivalently, for y outside V where the eigenstrain is zero, (10.1.17) yields

冕

S⫹

冋

⬁ Lijkl Gim (x, y)uk,l(x) ⫺ ui(x)

or, make use of Hooke’s law,

册

⭸G⬁im(x, y) ⭸xl

nj dS(x) ⫽ 0,

(10.1.21)

250

冕

S⫹

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冋

G⬁im(x, y)kl(x) ⫺ ui(x)Lijkl

册

⭸G⬁im(x, y) ⭸xl

nj dS(x) ⫽ 0.

(10.1.22)

Note that both (10.1.20) and (10.1.22) are valid for y inside ⍀. Thus, it follows from subtracting (10.1.21) from (10.1.18) that

冕 ⭸G ⭸(x,y y) L *(y) dV(y) ⭸G (x, y) ⫹ 冕 ⌬u (y)L n dS(y), ⭸y ⬁ im

um(x) ⫽

ijkl kl

V

l

⬁ im

i

S

ijkl

j

(10.1.23)

l

where we have used the traction continuity condition (10.1.3). For convenience, we have also switched the variables x and y and made use of the symmetry properties of the inﬁnite domain Green’s function (2.6.26). The above equation is an integral representation of the displacement ﬁeld within the inclusion. An integral equation can be derived by letting the point x approach the boundary S. Solving such integral equations typically requires numerical methods. In what follows, we will discuss some special cases of (10.1.23) and develop approximate and asymptotic solutions. First, we assume that the eigenstrain is uniform on ⍀. Then, (10.1.23) leads to um,n(x) ⫽

冕 ⭸G⭸y (x,⭸x y) L * dV(y) ⭸G (x, y) ⫹ 冕 ⌬u (y)L n dS(y), ⭸y ⭸x ⬁ im

ijkl kl

V

l

n

⬁ im

i

S

ijkl

j

l

(10.1.24)

n

or ij(x) ⫽ Lklmn* kl ⫹

冕L

冕⌫

klmn

S

⬁ ijmn

⍀

(y, x) dV(y)

⌬uk(y)⌫⬁ijmn(y, x)nl dS(y),

(10.1.25)

where ⌫⬁ijmn(y, x) is deﬁned by (4.3.6). It then follows from (4.3.8) that ij(x) ⫽ *S kl ijkl ⫹

冕L S

klmn

⌬uk(y)⌫⬁ijmn(y, x) nl dS(y),

(10.1.26)

10.1

IMPERFECT INTERFACES

251

where Sijkl is the Eshelby inclusion tensor. Making use of (10.1.4) in (10.1.26) gives ij(x) ⫽ Sijkl* kl ⫹

冕L S

⬁ kppq(y)⌫ijmn (y, x)nqnl dS(y).

klmn

(10.1.27)

Clearly, the ﬁrst term in (10.1.27) is identical to the original Eshelby solution. The effect of imperfect interface comes through the surface integral involving the displacement jump at the interface. Since perfect interface corresponds to ij ⫽ 0, a weakly imperfect interface may be modeled by a very small ij. Thus, (10.1.27) provides a convenient basis for constructing asymptotic solutions for the imperfect interface problem. To this end, we make use of Hooke’s law (3.3.2) in (10.1.27) to obtain ij(x) ⫽ *S kl ijkl ⫺ ⫹

冕L S

冕L S

L

⬁ kpst*⌫ijmn (y, x)nqni dS(y)

L

klmn pqst

klmn pqst

⬁ kpst(y)⌫ijmn (y, x)nqnl dS(y).

(10.1.28)

An iteration procedure can now be formulated, (n) ij (x) ⫽ *S kl ijkl ⫺ ⫹

冕L S

冕L S

L

⬁ kpst*⌫ijmn (y, x)nqnl dS(y)

klmn pqst

⬁ kpst(n⫺1)(y)⌫ijmn (y, x)nqnl dS(y)

L

klmn pqst

for n ⫽ 1, 2, . . . . The initial value can be set to (0) *. ij ⫽ Sijklij

(10.1.29)

The leading order solution for small ij can now be obtained as ij(x) ⬇ (1) ij (x) ⫽ Sijkl* kl ⫹ Zijst(x)(Istkl ⫺ Sstkl)*, kl

(10.1.30)

冕⌫

(10.1.31)

where Zijst(x) ⫽ LklmnLstpq

S

⬁ kp ijmn

(y, x)nqnl dS(y).

252

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

Alternatively, (10.1.30) can also be written as ij(x) ⫽ S M ijkl(x)*, kl

(10.1.32)

SM ijkl(x) ⫽ Sijkl ⫹ Zijst(x)(Istkl ⫺ Sstkl)

(10.1.33)

where

can be viewed as the modiﬁed Eshelby inclusion tensor for an ellipsoidal inclusion with weakly imperfect interface. One signiﬁcant difference of the modiﬁed Eshelby inclusion problem is that the strain within the ellipsoidal inclusion is no longer uniform even though the eigenstrain is. A quantity that will be needed later is the average of the modiﬁed Eshelby tensor SM ijkl(x) ⫽

1 ⍀

冕S ⍀

M ijkl

(x) dV.

(10.1.34)

To carry out the integral, consider

冕Z ⍀

(x) dV ⫽ LklmnLstpq

ijst

⫽ LklmnLstpq ⫽ SijmnLstpq

冕 冋冕 ⌫ (y, x) dV(x)]n n dS(y) 冕 P n n dS(y) 冕 n n dS(y), (10.1.35) S

S

S

kp

kp

⍀

⬁ ijmn

q l

⬁ ijmn q l

mp q n

where (4.3.7) has been used. Making use of the above, the integral in (10.1.34) can be carried out to yield SM ijkl ⫽ Sijkl ⫹ SijmnRmnpqLpqst(Istkl ⫺ Sstkl),

(10.1.36)

where Rmnpq ⫽

1 4⍀

冕 ( S

n n ⫹ mqnpnn ⫹ npnqnm ⫹ nqnpnm) dS(y).

mp q n

(10.1.37) Clearly, we have Rmnpq ⫽ Rnmpq ⫽ Rnmqp ⫽ Rmnqp. Note that Rmnpq depends on the interface properties through ij and the geometry of the

10.1

IMPERFECT INTERFACES

253

inclusion. Expressions of Rmnpq for ellipsoids, cylinders, and spheres are given in Appendix 10.A. Now, we are ready to consider a composite material consisting of randomly oriented and shaped inhomogeneities embedded in a matrix with stiffness tensor L0. Let the stiffness tenors of the inhomogeneities be L1, L2, L3, . . . , LN, as shown in Figure 7.1. We further assume that interfaces between the inhomogeneities and the matrix are not perfect. The interfacial jump condition is given by (10.1.4). We ﬁrst consider the average stress and average strain ﬁelds in the composite. It follows from (5.4.1) and (5.4.2) that the average stress over the entire representative volume element of the composite is ⫽

1 D

冕 dV ⫽ 冘 c , N

r

D

r

(10.1.38)

r⫽0

where r ⫽

1 ⍀r

冕

⍀r

dV

is the average stress on the rth inhomogeneity, while the average strain over the entire representative volume element of the composite is given by ⫽

1 D

冕 dV ⫽ 冘 c ⫹ 2D1 冘 冕 N

N

r r

D

r⫽0

r⫽1

Sr

(⌬u 嘸 n ⫹ n 嘸 ⌬u) dS, (10.1.39)

where Sr is the surface of ⍀r, r is the average stain in the rth inhomogeneity r ⫽

1 ⍀r

冕

⍀r

dV,

(10.1.40)

and the symbol 嘸 indicates a dyad, see Section 1.4. By using the displacement jump condition (10.1.4), the surface integral in (10.1.39) can be written as

冕

Sr

(⌬u 嘸 n ⫹ n 嘸 ⌬u) dS ⫽

冕

Sr

[( 䡠 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 䡠 n)] dS.

(10.1.41)

254

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

The integral is rather difﬁcult to evaluate. So, we will make an ad hoc approximation (Qu, 1993a),

冕

Sr

[( 䡠 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 䡠 n)] dS ⬇

冕

Sr

[( 䡠 r 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 r 䡠 n)] dS,

(10.1.42)

that is, replacing the stress distribution along Sr by the average stress on ⍀r. Clearly, (10.1.42) would be exact if the stress is uniform on ⍀r. The right-hand side of (10.1.42) can be further written as

冕

Sr

[( 䡠 r 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 r 䡠 n)] dS ⫽ 2⍀r Rrr,

(10.1.43)

where the fourth-order tensor Rr is deﬁned by (10.1.37). Finally, we can write the average strain on the composite as

冘 c ⫹ 冘 cR. N

⫽

N

r r

r

r

r

(10.1.44)

r⫽1

r⫽0

Let us now consider the effective elastic properties of the composite. To this end, let the representative volume element of the composite be subjected to the following traction boundary condition: 䡠 n兩S ⫽ 䡠 n,

(10.1.45)

where is the average stress over the representative volume element of the composite, according to the average stress theorem introduced in Section 5.4 (It can be easily shown that the average stress theorem is still valid in this case). The Mori–Tanaka method assumes that the average strain in the rth inhomogeneity can be written as [see (7.3.5)] r ⫽ 0 ⫹ pt r ,

r ⫽ 1, 2, . . . , N,

(10.1.46)

pt where pt r is the average r perturbance of the strain ﬁeld in the rth inhomogeneity. The corresponding average stress is

r ⫽ Lrr ⫽ Lr(0 ⫹ pt r ),

r ⫽ 1, 2, . . . , N.

(10.1.47)

10.1

IMPERFECT INTERFACES

255

The Mori–Tanaka method further assumes that each inhomogeneity ⍀r (r ⬎ 0) is embedded, in the absence of other inhomogeneities, in a uniform material of stiffness L0, which was prestressed by 0. When the inhomogeneity is simulated by an inclusion with eigenstrain *, r the equivalent inclusion equation becomes (see Section 4.4) r ⫽ Lr(0 ⫹ rpt) ⫽ L0(0 ⫹ rpt ⫺ r*).

(10.1.48)

It is further assumed that M pt r ⫽ S r *, r

(10.1.49)

where S M r is the modiﬁed Eshelby tensor averaged over ⍀r as given by (10.1.36). Substituting (10.1.49) into (10.1.48) yields an equation for r*, which can be solved to obtain M ⫺1 * r ⫽ [(Lr ⫺ L0)S r ⫹ L0] (Lr ⫺ L0)0.

(10.1.50)

The total strain in the rth inhomogeneity can then be written as r ⫽ 0 ⫹ rpt ⫽ 0 ⫹ S rMr* ⫽ TrM 0,

(10.1.51)

M ⫺1 ⫺1 TM r ⫽ [I ⫹ S r L0 (Lr ⫺ L0)] .

(10.1.52)

where

The above derivation is very similar to the steps leading to (7.1.6). The average stress on the rth inhomogeneity then follows from substituting (10.1.51) into (10.1.47), r ⫽ LrTrM 0 ⫽ HrM 0,

(10.1.53)

where M HM r ⫽ LrTr M0

is the local stress concentration tensor; see (7.3.11). Note that, although (10.1.53) was derived for r ⬎ 0, it can be easily see that it is also valid for r ⫽ 0. Making use of (10.1.53) in the average stress leads to

256

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冘 c ⫽ 冘 cH . N

⫽

N

r

r

M r

r

(10.1.54)

0

r⫽0

r⫽0

Consequently,

冉冘 冊

⫺1

N

0 ⫽

.

crHM r

(10.1.55)

r⫽0

Introducing (10.1.55) back to (10.1.53) yields r ⫽ BM r ,

(10.1.56)

where

冉冘 冊

⫺1

N

B ⫽H M r

M r

M r

crH

(10.1.57)

r⫽0

is the global stress concentration tensor; see (7.3.12). It then follows from (10.1.56) that the average strain in the rth inhomogeneity is r ⫽ Mr BrM .

(10.1.58)

Making use of (10.1.56) and (10.1.58) in (10.1.44) yields

冘 c M B ⫹ 冘 c R B . N

⫽

N

r

M r

r

r

M r

r

r⫽1

r⫽0

This immediately leads to

冘 cM B ⫹ 冘 cR B ⫽ c M B ⫹ 冘 c (M ⫹ R )B ⫽ 冋c M ⫹ 冘 c (M ⫹ R )L T M 册冉 冘 c L T M 冊 ⫽ 冋c I ⫹ 冘 c (M ⫹ R )L T 册冉 冘 c L T 冊 . N

N

M⫽

r

M r

r

r

r

M r

r⫽1

r⫽0

N

0

M 0

0

r

r

M r

r

r⫽1

N

0

0

r

r

r

r

0

r

N

0

⫺1

N

r

r⫽1

r

M r

r⫽0

r⫽1

0

⫺1

N

M r

r

r

r

M r

r

r⫽0

r

M r

(10.1.59)

10.1

IMPERFECT INTERFACES

257

This gives the Mori–Tanaka estimate of the effective compliance of the composite material with imperfect interfaces:

冋

冘

册冉冘

N

M ⫽ c0I ⫹

crLrTM r

r⫽0

r⫽1

冊

⫺1

N

cr(Mr ⫹ Rr)LrTM r

.

(10.1.60)

By specifying displacement boundary conditions, one can obtain the effective stiffness tensor; see Problem 10.1:

冉冘 N

L⫽

冊冋

crLrTrM

r⫽0

c0I ⫹

冘

册

⫺1

N

cr(Mr ⫹ Rr)LrTrM

r⫽1

.

(10.1.61)

Obviously, we have LM ⫽ ML ⫽ I.

(10.1.62)

Furthermore, it can be easily veriﬁed that when → 0, we have Rr → 0 and T M r → Tr. Therefore, the effective elastic properties (10.1.59) and (10.1.61) reduce to those of the perfect interface cases (7.3.14) and (7.3.8), respectively. Example 10.1 Consider a composite consisting of an isotropic matrix with L0 and isotropic, spherical particles of L1. The interface between the particles and the matrix is described by the displacement jump condition (10.1.4) where ij ⫽ ␣(␦ij ⫺ ni nj).

(10.1.63)

We are to ﬁnd the effective elastic properties of the composite. Since the materials are isotropic, we may represent them as L0 ⫽ (3K0, 20),

L1 ⫽ (3K1, 21).

(10.1.64)

The composite should also be isotropic, that is, L ⫽ (3K, 2). It follows from Appendix 10.A that R1 ⫽

2␣ (0, 3), 5d

(10.1.65)

where d is the diameter of the particles. The modiﬁed Eshelby tensor is thus given by

258

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

M M SM 1 ⫽ S1 ⫹ S1R1L0(I ⫺ S1) ⫽ (3␥ 0 , 2␦ 0 ),

(10.1.66)

where

冉

冊

(10.1.67)

冊

(10.1.68)

L ⫽ (c0L0 ⫹ c1L1T1M)(c0I ⫹ c1(M1 ⫹ R1)L1T1M)⫺1.

(10.1.69)

M (3␥ M 3␥0, 2␦0 ⫹ 0 , 2␦ 0 ) ⫽

24␣0␦0 (1 ⫺ 2␦0) . 5d

Thus, M ⫺1 ⫺1 TM 1 ⫽ [I ⫹ S 1 L0 (L1 ⫺ L0)]

⫽

冉

K0 0 , . M K0 ⫹ 3␥ M (K ⫺ K ) ⫹ 2 ␦ 0 1 0 0 0 (1 ⫺ 0)

The effective stiffness tensor is obtained from

Carrying out the matrix algebra, we ﬁnally arrive at K ⫽ K0 ⫹ ⫽ 0 ⫹

c1K0(K1 ⫺ K0) , K0 ⫹ 3␥0(1 ⫺ c1)(K1 ⫺ K0)

c10[5d(1 ⫺ 0) ⫺ 12␣01] . 5d0 ⫹ 10d␦ 0M(1 ⫺ c1)(1 ⫺ 0) ⫹ 12c1␣01

(10.1.70)

(10.1.71)

It is seen that the effective bulk modulus is the same as that of the perfect interface case. Only the effective shear modulus is affected by the imperfect interface. It is also noticed that the effective shear modulus depends not only on the volume fraction of the particles but also on the particle size. This is very different from the perfect interface case where only the volume fraction of the particles matters. To close this section, we state two variation principles for composites with imperfect interfaces (Qu, 1993b). The proof of them is straightforward; see Problem 10.2. Principle of Minimum Potential Energy Among all kinematically admissible displacement ﬁelds, the true one makes the following functional minimum:

10.2

⌸(u) ⫽

1 2

冕 :L: dV ⫺ 冕 D

S

u 䡠 䡠 n dS ⫹

1 2

FIBER BRIDGING

冕 ⌬u 䡠

⫺1

⌫

259

䡠 ⌬u dS,

(10.1.72) where S is the portion of the external boundary where traction is prescribed, and ⌫ is the union of all internal interfaces. Principle of Minimum Complimentary Energy Among all statically admissible stress ﬁelds, the true one makes the following functional minimum: ⌸c() ⫽

冕 :M: dV ⫺ 冕 u 䡠 䡠 n dS 1 ⫹ 冕 n 䡠 䡠 䡠 䡠 n dS, 2 1 2

D

Su

⌫

(10.1.73)

where Su is the portion of the external boundary where displacement is prescribed, and ⌫ is the union of all internal interfaces.

10.2

FIBER BRIDGING

Fibers in engineering composites typically have higher elastic modulus than the matrix. Because of this, the effective elastic modulus of the composite is higher than that of the matrix material. In addition to the enhancement of elastic stiffness, ﬁbers can also enhance the fracture toughness of the matrix material. In this section, we will consider a very simple example to illustrate how the ﬁbers in a composite affect the composite’s fracture behavior. Let us consider a unidirectional ﬁber-reinforced composite material. Assume that the matrix has a crack perpendicular to the ﬁber direction, as shown in Figure 10.1. When the composite is subjected to a uniform tensile load ⬁ in the ﬁber direction at inﬁnity, a mode I stress intensity is created at the crack tips, which is characterized by the stress intensity factor KI. According to linear elastic fracture mechanics, the crack may start growing leading to the fracture of the material if the stress intensity factor KI becomes greater than the fracture toughness of the matrix material KIc, that is,

260

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

σ∞

2a

σ∞ Figure 10.1 Unidirectional ﬁber-reinforced composite with Grifﬁth crack.

KI ⱖ KIc.

(10.2.1)

If, under the same given load, KI can be reduced, it effectively improves the fracture toughness of the material. We will see from the following analysis that ﬁbers that bridge the crack surfaces can effectively reduce KI, thus improving the fracture strength of the composite. For simplicity, we will limit ourselves to plane strain deformation, so the crack can be considered as a two-dimensional slit, which is referred to as the Grifﬁth crack in fracture mechanics literature. We further assume that the size of the existing crack in the composite is much greater than the ﬁber diameter. This assumption is valid for most engineering applications where the ﬁber diameter is in the order of micrometers, while the ﬂaw size is typically several hundred micrometers, or millimeters. Under this assumption, the unidirectional ﬁberreinforced composite can be viewed as a homogeneous, transversely isotropic solid as discussed in Section 9.1. To proceed, we ﬁrst transfer the externally applied load ⬁ to the crack surface. A simple linear superposition argument would show that loading on the crack surfaces is equivalent to loading at inﬁnity in that they produce the same stress intensity factors. So, in what follows, we will consider ⬁ being applied on the cracks surface instead of at inﬁnity. If there were no ﬁbers bridging the crack faces, the stress intensity factor of a Grifﬁth crack of length 2a in a homogeneous, transversely

10.2

FIBER BRIDGING

261

isotropic elastic solid subject to normal loading ⬁ on the crack surfaces is given by (see Tada et al., 1985; Qu and Bassani, 1993) dx 冕 冪 兹a ⫺ x .

KI ⫽ 2

a

a

⬁ 2

0

2

(10.2.2)

However, the bridging ﬁbers limit the opening of the crack faces, so the actual (or effective) stress intensity factor at the crack tip is rather different from (10.2.2). In other words, not all the applied stress ⬁ is working to open the crack surfaces. Instead, a portion of the applied stress ⬁ has to stretch the bridging ﬁbers. Or, one may view this in a different way. The bridging ﬁbers exert a stress p(x) on the crack surfaces, which works against the applied stress ⬁ by trying to close the crack. Thus, effectively, the problem at hand is equivalent to a crack without bridging ﬁbers, but the externally applied load is ⬁ ⫺ p(x). Therefore, the actual stress intensity factor should be, following (10.2.2), KI ⫽ 2

dx . 冪 冕 [兹⫺a p(x)] ⫺x a

a

0

⬁

2

2

(10.2.3)

What we need to do next is to ﬁnd p(x). Since the total load is shared between the ﬁbers and the matrix, we have ⬁ ⫽ cƒƒ⬁ ⫹ cm⬁m,

(10.2.4)

where, as deﬁned before, cƒ and cm are the volume fractions of the ﬁber and the matrix, respectively. Away from the crack, the axial stresses in the ﬁber and in the matrix are denoted by ⬁ƒ and m⬁ , respectively. Since the axial strain is the same for both ﬁber and matrix (no gross ﬁber pull-out), one must have ⬁ƒ ⬁ ⫽ m ⫽ ⬁, Eƒ Em EL

(10.2.5)

where, again, Eƒ and Em are the Young moduli of the ﬁber and matrix, respectively, while EL is the effective Young modulus of the unidirectional ﬁber-reinforced composite in the ﬁber direction. Combining (10.2.4) and (10.2.5) yields the stress in the ﬁber

262

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

⬁ƒ ⫽

⬁Eƒ , cmEm(1 ⫹ )

(10.2.6)

Eƒcƒ . Emcm

(10.2.7)

where ⫽

This is the axial stress in the ﬁber far away from the crack (or when the crack is absent). We now consider the axial stress in the ﬁber near the crack faces. Shown in Figure 10.2 is a representative element near the crack faces containing one ﬁber. The center of the ﬁber is x distance away from the center of the crack. Due to geometric singularities, the stresses near the intersection of the ﬁber and crack surfaces are very high. It is perceivable that certain portions of the ﬁber–matrix interface had failed and sliding between the ﬁber and matrix had occurred. We assume that the length of the sliding region is l and the shear stress on the interface due to friction is denoted by (assume it is a constant). Outside the sliding area, the axial stress in the ﬁber is given by (10.2.6). Within the sliding area, the axial stress in the ﬁber can be obtained by balancing the axial stress in the ﬁber and the shear stress on the ﬁber surface due to friction, ƒ(z) ⫽ ƒ⬁ ⫹

2b 2 z ⫽ ƒ⬁ ⫹ z, 2 b b

(10.2.8)

where b is the ﬁber radius. According to Hooke’s law, the strain in the ﬁber follows from (10.2.8),

l(x)

z

x

2v(x)

Fiber

2b

Matrix

Figure 10.2 Representative element of crack surfaces r distance from crack center.

10.2

ƒ(z) ⫽

FIBER BRIDGING

⬁ƒ 2 ⫹ z. Eƒ bEƒ

263

(10.2.9)

Integration of (10.2.9) with respect to z leads to the total elongation of the ﬁber within the sliding area

冕

冉

l(x)

2⌬ƒ(x) ⫽ 2

0

ƒ(z) dz ⫽ 2

冊

⬁ƒ l(x) ⫹ l(x). Eƒ bEƒ

(10.2.10)

The factor 2 in the above equation comes from the fact that the sliding area is symmetric with respect to the crack plane. We now consider the matrix surrounding the ﬁber. Analogous to (10.2.8), we assume that the stress in the matrix within the sliding area is also a linear function of z. Further, the axial stress in the matrix must be zero on the crack surfaces. Thus, we write

冋

m(z) ⫽ 1 ⫺

册

z ⬁ . l(x) m

(10.2.11)

The corresponding strain thus follows:

冋

册

⬁m z 1⫺ . Em l(x)

m(z) ⫽

(10.2.12)

Consequently, integration of (10.2.12) gives the axial elongation of the matrix within the sliding area

冕

l(x)

2⌬m(x) ⫽ 2

m(z) dz ⫽

0

⬁ml(x) . Em

(10.2.13)

Comparing (10.2.10) and (10.2.13), we have the total crack opening displacement

冋

2v(x) ⫽ 2⌬ƒ(x) ⫺ 2⌬m(x) ⫽ 2

册

⬁ƒ l(x) ⬁ l(x) ⫹ l(x) ⫺ m . Eƒ bEƒ Em

(10.2.14)

Substituting (10.2.6) into (10.2.14) yields the following crack opening displacement:

264

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

v(x) ⫽

冋

册

l(x) ⬁ ⫹ l(x). bEƒ 2(Eƒcƒ ⫹ Emcm)

(10.2.15)

This can also be solved to obtain the length of the sliding zone, l(x) ⫽

⬁b 4(1 ⫹ )cƒ

冋冪

1⫹

册

16(1 ⫹ )2Eƒc2ƒv(x) ⫺1 . 2 ⬁2 b

(10.2.16)

Clearly, for the ﬁber at the crack tip, the crack opening displacement is zero, that is, v(a) ⫽ 0. It thus follows from (10.2.16) that l(a) ⫽ 0. That means that the ﬁbers outside the cracked area do no show any pull-out, which is consistent with our intuition. If we now substitute (10.2.16) back to (10.2.8), we can calculate the stress exerted on the crack surface by the bridging ﬁbers: p(x) ⫽ cƒƒ(l) ⫽

⬁ 2(1 ⫹ )

冋冪

1⫹

册

16(1 ⫹ )2Eƒc2ƒv(x) ⫹1 . 2 ⬁2 b (10.2.17)

Note that p(x) is positive. It represents the stress carried by the bridging ﬁbers over the cracked area. One may also view p(x) as the stress acting on the crack surface trying to close the crack opening by working against the externally applied load ⬁. Equation (10.2.17) is a relationship between p(x) and v(x). For convenience, let us recast (10.2.17) into a nondimensional form: p(x) ⫽ ⬁ 2(1 ⫹ )

冋冪

1⫹

册

4(1 ⫹ )(x) ⫹1 , 20

(10.2.18)

where 0 ⫽

2⬁b . 4(1 ⫹ )Eƒc2ƒ

(10.2.19)

Since p(x) ⱕ ⬁, it can be easily shown from (10.2.18) that (x) ⱕ 0. Shown in Figure 10.3 is the relationship between the bridging force p(x) and the parameter ⫽ Eƒcƒ /Emcm for various crack opening displacement values. It is seen that as increases (either higher ﬁber

10.2

265

FIBER BRIDGING

1.0 0.8

p( x) 0.6 σ∞

v( x) v0 = 0.2 v( x) v0 = 0.4 v( x) v0 = 0.6

0.4 0.2 0.0 0.0

0.5

1.0

1.5

η

2.0

2.5

3.0

Figure 10.3 Relationship between bridging force and ⫽ Eƒcƒ / Emcm.

modulus, or more ﬁbers, or both), the bridge forces increase as well. Higher crack opening displacement also causes higher bridging forces. For a given crack, the crack opening displacement is typically highest near the center of the crack. Therefore, that is where the bridging force is the highest. Higher bridging means higher stress in the bridging ﬁber. So, conceivably, some of the ﬁbers near the center of the crack may break. Such a situation has been studied by a number of investigators (e.g., Cui, 1992; Xia et al., 1994; Budiansky and Cui, 1995). As discussed earlier, the problem at hand is equivalent to a crack in a homogeneous, transversely isotropic solid subject to normal pressure ⬁ ⫺ p(x). The crack opening displacement in this case is given by (see, e.g., Qu and Bassani, 1993)

(r) ⫽

2D

冕 [

冏

a

0

⬁

⫺ p(t)]log

2D ⫽ 2D⬁兹a ⫺ x ⫺ 2

2

兹a2 ⫺ x2 ⫹ 兹a2 ⫺ t2 兹a2 ⫺ x2 ⫺ 兹a2 ⫺ t2

冏

dt

冕 p(t)log冏兹a ⫺ x ⫺ 兹a ⫺ t 冏 dt, a

0

兹a2 ⫺ x2 ⫹ 兹a2 ⫺ t2 2

2

2

2

(10.2.20) where

266

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

D⫽

冪冉A 2A 冊冉2A 2A 11

22

12

⫹ A66

⫹

11

A11 ⫽

1 ⫺ 2 , ET

22

(10.2.21)

11

A22 ⫽

(1 ⫹ ) A12 ⫽ ⫺ TT , EL

冪AA 冊,

EL ⫺ 2ET , E 2L

A66 ⫽

1 . L

(10.2.22)

In deriving the above expressions, it has been assumed that ƒ ⫽ m ⫽ . The other engineering constants EL, ET, and L, and TT are deﬁned in Section 9.1. They are related to the elastic properties of the ﬁber and matrix through the formulas discussed in the same section. Substituting (10.2.17) into (10.2.20) yields an integral equation for the crack opening displacement. Numerical methods are needed to obtain the solution to the integral equation. Once the crack opening displacement (x) is solved, the pressure p(x) can be evaluated from (10.2.17). Once p(x) is known, linear elastic fracture mechanics dictates that fracture may occur when KI ⫽ 2

dx ⫽K . 冪 冕 [兹⫺a p(x)] ⫺x a

a

0

⬁

2

2

Ic

(10.2.23)

Since p(x) is positive, the stress intensity factor calculated from (10.2.23) is lower than the case without ﬁber bridging. Therefore, the bridge ﬁber effectively increases the fracture toughness of the composite.

10.3

TRANSVERSE MATRIX CRACKS

Transverse matrix cracking is one of the most common damage mode in cross-ply laminates. It has been observed in both ceramic matrix and polymer matrix composites that the evolution of transverse matrix cracking shows two distinct stages. When tensile stress is applied in the ﬁber direction of the 0⬚ ply, cracks are formed in the 90⬚ ply at a load level much lower than the ultimate strength of the laminate. These transverse matrix cracks are tunneling cracks in that they almost instantaneously run through the entire specimen width and the thickness

10.3

TRANSVERSE MATRIX CRACKS

267

of the 90⬚ ply but arrest at the 0⬚ /90⬚ ply interfaces. As the load further increases, more transverse cracks are initiated. At some critical load, the number of cracks ceases to increase; instead, the existing cracks may penetrate into the adjacent 0⬚ layers and eventually fracture the 0⬚ ﬁbers (for ceramic matrix composite CMCs), or divert into the 0⬚ /90⬚ ply interfaces (for polymer matrix composite PMCs). Catastrophic failure becomes imminent when the 0⬚ ﬁbers are broken. In what follows, we will develop a micromechanics model for the onset and subsequent multiplication of transverse cracks in the 90⬚ layers at the ﬁrst stage of damage evolution based on the Grifﬁth fracture criterion. The cross section of a typical ﬁber-reinforced cross-ply laminate is schematically shown in Figure 10.4. For convenience, the following convention is adopted here. The layers with vertical ﬁbers in the y direction are called 0⬚ layers (or plies) and the layers with ﬁbers perpendicular to the page (in the z direction) are called 90⬚ layers (or plies). It is assumed that the cross-ply laminates have equal distribution of 0⬚ and 90⬚ plies. The effective modulus of the ﬁber-reinforced cross-ply laminate shown in Figure 10.4 has been studied in Section 9.2. What we will need here is the plane-strain Young modulus in the y direction of the uncracked cross-ply laminate; see (9.2.40): E0 ⫽

(EL ⫹ ET)2 ⫺ 4E 2L 2TL , 2(EL ⫹ ET)(1 ⫺ LTTL)

0 ⫽

2EL , EL ⫹ ET TL

y

x 2

1

z

Figure 10.4 Cross section of cross-ply laminate.

(10.3.1)

268

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

where TL LT, EL, and ET are the effective engineering elastic constants of the unidirectional ﬁber-reinforced composite. These engineering elastic constants can be related to the Young moduli of the ﬁber and the matrix materials as discussed in Chapter 9. If we assume further that the Poisson ratios for the ﬁber and the matrix are the same, that is, m ⫽ ƒ ⫽ , the above equations reduce to E0 ⫽

(EL /ET ⫹ 1)2 ⫺ 4 2(EL /ET)2 ET, 2(EL /ET ⫹ 1)(1 ⫺ 2)

0 ⫽ .

(10.3.2)

It is obvious from (9.1.58) to (9.1.64) that the ratio EL /ET depends only on the ﬁber volume fraction c and the ratio ⫽ Eƒ /Em. Therefore, one can conclude that, besides a common factor Em, for a cross-ply laminate with equal number of 0⬚ and 90⬚ plies of equal thickness, the effective elastic properties depend only on , , and c. As the matrix cracks multiply, the effective stiffness of the composite decreases. We will use a differential scheme to estimate the effective modulus as a function of the crack density. The idea is based on the notion of incremental construction of the strain energy by introducing one crack at a time in the 90⬚ layer. Suppose that at a given crack density ƒ in the 90⬚ layer, the composite is homogenized with effective Young’s modulus Ec(ƒ), where the dependence of Ec on the crack density is explicitly indicated. The fundamental assumption of the differential method is that when an additional crack is introduced in the 90⬚ layer, the change of strain energy due to this addition is the energy released from the formation of the new crack. To this end, consider a pair of 0⬚ and 90⬚ layers in the cross-ply laminate as shown in Figure 10.5. Assume that there are N cracks in the 90⬚ layer (material 1) within the height L. Let the representative element be subjected to an applied strain in the y direction. Then, at this given crack density, the total strain energy in this pair of layers can be written as U(ƒ) ⫽ –12 Ec(ƒ) 2(4t)L,

(10.3.3)

where h⫽

L . 2N

(10.3.4)

When an additional crack is introduced, the crack density becomes

10.3

2t

2t

2

1

TRANSVERSE MATRIX CRACKS

269

σ

2h

L

σ

Figure 10.5 Transverse matrix cracks in cross-ply laminate under uniaxial loading.

ƒ1 ⫽

t , h1

h1 ⫽

L

. 2(N ⫹ 1)

(10.3.5)

The total strain energy at this crack density becomes U(ƒ1) ⫽ –12 Ec(ƒ1) 2(4t)L.

(10.3.6)

Based on the differential scheme, the difference between (10.3.3) and (10.3.6) is the energy released due to one transverse crack given by

再冕

1 U(ƒ1) ⫺ U(ƒ) ⫽ ⫺ 2 2

t

⫺t

冎

(x)␦(x) dx ,

(10.3.7)

where ␦(x) is the crack opening displacement deﬁned by ⌬(x) ⫽ uy(x, 0⫹) ⫺ uy(x, 0⫺)

for ⫺t ⱕ x ⱕ t.

(10.3.8)

Note that the right-hand side of (10.3.7) is the energy released when a crack is formed in the laminate with effective Young’s modulus Ec(ƒ). Therefore, the stress (x) in the 90⬚ layer (prior to the formation of this crack) should be uniform and given by

270

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冋

(x) ⫽ 2Ec(ƒ) ⫺

册

EL , 1 ⫺ 2ET /EL

(10.3.9)

where EL is the longitudinal (ﬁber direction) modulus of the individual layers. Substituting (10.3.9) into the right-hand side of (10.3.7) yields

冋

U(ƒ1) ⫺ U(ƒ) ⫽ ⫺ 2Ec(ƒ) ⫺

册

EL 2t⌬, 1 ⫺ 2ET /EL

(10.3.10)

where ⌬ is the average crack opening displacement deﬁned by ⌬⫽

1 2t

冕

t

⫺t

⌬0(x) dx,

(10.3.11)

and ⌬0(x) is the crack opening displacement due to a unit applied strain ﬁeld, that is, ⌬0(x) ⫽

⌬(x) .

(10.3.12)

Since ⌬(x) can be calculated by the ﬁnite-element method for given , ⌬0(x) can then be obtained through linear superposition from (10.3.12). Next, consider the left-hand side of (10.3.10). It follows from (10.3.3) and (10.3.6) that U(ƒ1) ⫺ U(ƒ) ⫽ 2 2 Lt[Ec(ƒ1) ⫺ Ec(ƒ)].

(10.3.13)

On the other hand, making use of (10.3.4) and (10.3.5) yields L⫽

2t

. ƒ1 ⫺ ƒ

(10.3.14)

Substitution of (10.3.14) into (10.3.13) gives U(ƒ1) ⫺ U(ƒ) ⫽ 4 2t2

[Ec(ƒ1) ⫺ Ec(ƒ)] . ƒ1 ⫺ ƒ

(10.3.15)

Obviously, in the limiting of ƒ1 → ƒ, (10.3.15) can be written as a differential equation:

10.3

TRANSVERSE MATRIX CRACKS

U(ƒ1) ⫺ U(ƒ) ⫽ 4 2t2

dEc(ƒ) . dƒ

271

(10.3.16)

Combining (10.3.10)–(10.3.16) yields

冋

册

dEc ⌬ EL ⫽⫺ 2Ec(ƒ) ⫺ . dƒ 4t 1 ⫺ 2ET /EL

(10.3.17)

In addition to (10.3.17), Ec(ƒ) should also satisfy the initial condition that when there is no crack (ƒ ⫽ 0), Ec(0) ⫽ E0.

(10.3.18)

Equations (10.3.17) and (10.3.18) form an initial value problem for the effective Young modulus of the composite. The solution to the initial value problem (10.3.17) and (10.3.18) is given by (Qu and Hoiseth, 1998)

再 冉 冊

冋

冉 冊册冎

ƒ⌬ EL ƒ⌬ Ec(ƒ) ⫽ E0 exp ⫺ ⫹ 1 ⫺ exp ⫺ 2t EL ⫹ ET 2t

.

(10.3.19)

It is seen that this solution approaches the theoretical limit Ec(ƒ) EL → , E0 ET ⫹ EL

(10.3.20)

as ƒ → ⬁ in which only the 0⬚ layers carry the load. It is seen from (10.3.19) that once ⌬, the crack opening displacement of a single crack in an inﬁnitely long (h/t → ⬁) specimen, is known, the effective elastic modulus of the laminate with any crack density can be predicted. Shown in Figure 10.6 is the predicted Young modulus Ec as a function of crack density ƒ for c ⫽ 0.55 and various values of . The solid lines are the analytical solution from (10.3.19), and the symbols are the exact solutions from the ﬁnite-element method (Qu and Hoiseth, 1998). It is found that for the wide range of materials considered, the maximum difference between the ﬁnite element and the analytical solutions is less than 5 percent. The effective Young modulus given by (10.3.19) can only give the stiffness as a function of crack density. To predict the effective (overall) stress–strain behavior, damage (cracking) evolution must be modeled.

272

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

1.0

0.9 Ef /Em = 30 0.8

Ec /E0

Ef /Em = 20 0.7 Ef /Em = 10 0.6

ν = 0.3, c = 0.55

0.0 0.0

Ef /Em = 5

0.5 1.0 1.5 2.0 Transverse Crack Density, f

2.5

Figure 10.6 Effective Young’s modulus. Lines are from the analytical solution and symbols are from the ﬁnite-element solutions.

To this end, a fracture criterion is required. Once a fracture criterion is established, solutions of crack density can be obtained as a function of the applied strain . As the cross-ply laminate is loaded in the y direction, transverse cracks develop in the 90⬚ layers. Assume the transverse cracks initiate as tunneling cracks, namely, they span the entire 90⬚ ply and propagate in the width direction of the laminate (the z direction). Then, based on linear elastic fracture mechanics, the energy released due to the formation of a new tunneling crack can be written as (Hutchinson and Suo, 1991), Gss(ƒ) ⫽

1 4t

冕

t

⫺t

(x)⌬(x) dx,

(10.3.21)

where ⌬(x) is the crack opening displacement given in (10.3.11) and (x) ⫽ y(x, 0), that is, the normal stress on the crack line prior to cracking. Note that both ⌬(x) and (x) depend on the crack density ƒ. Therefore, Gss is a function of ƒ. Through simple dimensional analysis, the energy release rate can be written as

10.3

TRANSVERSE MATRIX CRACKS

Gss(ƒ) ⫽ 2tE0g(, , c, ƒ),

273

(10.3.22)

where is the applied strain, E0 is the overall plane strain Young modulus for the uncracked composite deﬁned in (10.3.2), and g(, , c, ƒ) is the nondimensional energy release rate. The energy release rate Gss(ƒ) can also be related to the effective stiffness through the principle of conservation of energy. To develop such a relationship, consider a specimen containing N cracks in the 90⬚ layer. It follows from the conservation of strain energy that (Qu and Hoiseth, 1998) 1 1 Nt Ec(ƒ) 2(2hNt) ⫽ E0 2(2hNt) ⫺ G (ƒ), 2 2 2 ss

(10.3.23)

where 2hN is the height of the specimen (thickness is unit). Substituting (10.3.22) into (10.3.23) yields

冋

g(, , c, ƒ) ⫽ 1 ⫺

册

Ec(ƒ) 2 , E0 ƒ

(10.3.24)

where Ec is the effective Young modulus determined in the previous section. Making use of (10.3.24) gives the steady-state energy release rate for tunneling cracks

冋

冉 冊册

Gss(ƒ) 2ET ␦ƒ ⫽ g(, , c, ƒ) ⫽ 1 ⫺ exp ⫺ 2 tE0 (EL ⫹ ET)ƒ 2t

.

(10.3.25)

An interesting limit of (10.3.25) as ƒ → 0 is Gss(0) ⫽

ET 2␦ E0. ET ⫹ EL

(10.3.26)

This can also be obtained directly from (10.3.21) by using (10.3.9) and (10.3.11). Next, consider a 90⬚ layer with an existing set of transverse matrix cracks of density ƒ. Assume that a new set of cracks bisecting the existing set is in the process of tunneling across the layer; see Figure 10.7. The energy released by the cracks in the process of tunneling is (Hutchinson and Suo, 1991)

274

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

2h

New Cracks 2t

Figure 10.7 Multiplication of transverse matrix cracking in cross-ply laminate.

2Gss(2ƒ) ⫺ Gss(ƒ).

(10.3.27)

Then, based on the Grifﬁth energy criterion in linear elastic fracture mechanics, a new set of cracks will be initiated if the following equation is satisﬁed: G (2) c ⫽ 2Gss(2ƒ) ⫺ Gss(ƒ),

(10.3.28)

where G (2) is the plane strain mode I toughness of the 90⬚ layer c (material 2). Substituting (10.3.26) into (10.3.28) yields G c(2) ⫽

冋 冉 冊

冉 冊册

2 2tE0ET ␦ƒ ␦ƒ exp ⫺ ⫺ exp ⫺ (EL ⫹ ET)ƒ 2t t

.

(10.3.29)

Equation (10.3.29) is the desired evolution equation for the crack density ƒ as a function of the applied strain . For ⫽ 0.3, c ⫽ 0.55, the crack density ƒ as a function of 兹tE0 /G (2) c is plotted in Figure 10.8 for ⫽ 1, 5, 10, 20, 30. Figure 10.9 presents a comparison between the theoretical predictions and the experimental data for crack density versus applied load. The experimental data is from Varna and Berglund (1991). The tested material is an AS/3501-06 carbon ﬁber–epoxy [02 /902]s laminate. In the numerical calculations, no adjustment parameters are used. All material constants are taken directly from Varna and Berglund (1991). It is seen that the predicted crack density versus load curve (dotted line) has the same trend as the experimental one but is slightly shifted to the right. This may be attributed to many factors. Chief among them

10.3

TRANSVERSE MATRIX CRACKS

275

1.0

Transverse Crack Density, f

0.8

0.6

0.4

Ef /Em = 1 Ef /Em = 5 Ef /Em = 10 Ef /Em = 20 Ef /Em = 30

0.2

0.0 0

1

2

3

4

5

ε E0t Gc( 2 )

Figure 10.8 Crack density vs. applied strain.

AS/3501-60 [02/902]s 2.0 (2)

2

Theoretical Prediction (Gc = 104 J/m ) (2) 2 Theoretical Prediction (Gc = 130 J/m ) Experimental Data

Crack Density f

1.5

1.0

0.5

0.0 0.0

0.5

1.0

1.5

2.0

Applied Stress s 0 (GPa)

Figure 10.9 Comparison between experimental and analytical results for crack density vs. applied load.

276

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

is the fact that the model is based on the assumption that the laminate contains an inﬁnite number of layers, while the experimental data were obtained for a [02 /902]s laminate. Since the model predicts the trend correctly, a simple parameter adjustment can be done in practical applications to correlate the prediction with the measurement. For example, in the case considered here, by reducing the toughness of the 2 90⬚ layer in the direction of the ﬁber from G(2) c ⫽ 130 J/m as reported (2) 2 in Varna and Berglund (1991) to Gc ⫽ 104 J/m , the model predicts excellent agreement with the experiments as shown by the solid line in Figure 10.10. Note that, in the limit of ƒ → 0, Eq. (10.3.29) becomes G (2) c ⫽

2␦ E0ET . ET ⫹ EL

(10.3.30)

Thus, the threshold strain at which transverse matrix cracking starts to occur is th ⫽

冪

G (2) c (ET ⫹ EL) . ␦ E0ET

(10.3.31)

4

E f /E m = 1 E f /E m = 5

3

E f /E m = 1 0

σ

E f /E m = 2 0

E 0 G c( 2 ) t

E f /E m = 3 0 2

1

0 0

1

2

ε E 0t G

3 (2) c

Figure 10.10 Effective stress–strain curves.

4

277

APPENDIX 10.A

Now, consider the effect of matrix cracking on the overall stress–strain behavior. To begin the calculation, the threshold strain th is obtained from (10.3.31) for the given composite system. Then, the strain is increased gradually. For each value of ⬎ th, the corresponding crack density ƒ is computed from (10.3.29). Substituting this value of ƒ into (10.3.19) yields the corresponding effective Young modulus at this given strain. Finally, the stress (ƒ) corresponding to this strain is evaluated from (ƒ) ⫽ Ec(ƒ)(ƒ).

(10.3.32)

For ⫽ 0.3, c ⫽ 0.55, the overall stress–strain curves for various values of are presented in Figure 10.10. Note that these curves are invariant to G(2) c because of the normalization. PROBLEMS

10.1 Consider a composite material consisting of randomly oriented and shaped inhomogeneities embedded in a matrix with stiffness tensor L0. Let the stiffness tenors of the inhomogeneities be L1, L2, L3, . . . , LN, as shown in Figure 7.1. We further assume that interfaces between the inhomogeneities and the matrix are not perfect. The interfacial jump condition is given by (10.1.4). Find the effective stiffness tensor of this composite. 10.2 Prove the two variational principles stated in Section 10.1. APPENDIX 10.A

By substituting (10.1.5) into (10.1.36), we obtain the following: Rijkl ⫽ ␣Pijkl ⫹ ( ⫺ ␣)Qijkl

(10.A.1)

with Pijkl ⫽

冕 冋冕

册

2 3 d (␦iknˆ j nˆ l ⫹ ␦jknˆ i nˆ l ⫹ ␦ilnˆ j nˆ k ⫹ ␦jlnˆ i nˆ k) 0 16 0 n ⫻ sin d, (10.A.2)

Qijkl ⫽

3 4

冕 冋冕

2

0

0

册

nˆ i nˆ j nˆ k nˆ l d sin d, n

(10.A.3)

278

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

where n ⫽ 兹nˆ i nˆ i, nˆ ⫽

冉

(10.A.4)

冊

sin cos sin sin cos , , . a1 a2 a3

(10.A.5)

For spheres (a1 ⫽ a2 ⫽ a3 ⫽ a), we have n ⫽ 1/a. Thus, Pijkl ⫽

1 I , a ijkl

Qijkl ⫽

1 (2I ⫹ ␦ij␦kl). 5a ijkl

(10.A.6)

For cylinders (a1 ⫽ a2 ⫽ a, a3 → ⬁), the non-zero components are P1111 ⫽ P2222 ⫽ 4P2323 ⫽ 4P1313 ⫽ 2P1212 ⫽

3 , 8a

(10.A.7)

Q1111 ⫽ Q2222 ⫽ 3Q2323 ⫽ 3Q1313 ⫽ 3Q1212 ⫽

9 . 32a

(10.A.8)

REFERENCES Achenbach, J. D. and H. Zhu. (1989). Effects of Interfacial Zone on Mechanical Behavior and Failure of Fiber-Reinforced Composites, J. Mech. Phys. Solids, Vol. 37, pp. 381–393. Budiansky, B. and Y. Cui. (1995). Toughening of Ceramics by Short Aligned Fibers, Mech. Mater., Vol. 21, pp. 139–146. Cui, Y. (1992). Interaction of Fiber and Transformation Toughening, J. Mech. Phys. Solids, Vol. 40, pp. 1837–1850. Hutchinson, J. W. and Z. Suo. (1991). Mixed Mode Cracking in Layered Materials, Adv. Appl. Mech., Vol. 29, pp. 62–191. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston. Qu, J. (1993a). Eshelby Tensor for an Elastic Inclusion with Slightly Weakened Interface, J. Appl. Mech., Vol. 60, pp. 1048–1050. Qu, J. (1993b). Effects of Slightly Weakened Interfaces on the Overall Elastic Properties of Composite Materials, Mech. Mater., Vol. 14, p. 269–281. Qu, J. and J. L. Bassani. (1993). Interfacial Fracture Mechanics for Anisotropic Bimaterials, J. Appl. Mech., Vol. 60, pp. 422–431.

SUGGESTED READINGS

279

Qu, J. and K. Hoiseth. (1998). Evolution of Transverse Matrix Cracking in Cross-Ply Laminates, Int. J. Fatigue Fracture Eng. Mater. Structures, Vol. 21, pp. 451–464. Tada, H., P. Paris, and G. R. Irwin. (1985). The Stress Analysis of Cracks Handbook, Del Research, St. Louis. Varna, J., and L. A. Berglund. (1991). Multiple Transverse Cracking and Stiffness Reduction in Cross-Play Laminates, J. Composites Tech. Res., JCTRER, Vol. 27, pp. 99–106. Xia, Z. C., J. W. Hutchinson, A. G. Evans, and B. Budiansky. (1994). On Large Scale Sliding in Fiber-Reinforced Composite, J. Mech. Phys. Solids, Vol. 42, pp. 1139–1158.

SUGGESTED READINGS Budiansky, B. and J. W. Hutchinson. (1986). Matrix Fracture in FiberReinforced Ceramics, J. Mech. Phys. Solids, Vol. 34, pp. 167–189. Christensen, R. M. (1979). Mechanics of Composite Materials, Wiley, New York. Hashin, Z. (1985). Analysis of Cracked Laminates: A Variational Approach, Mech. Mater., Vol. 4, pp. 121–136. Hoiseth, K. and J. Qu. (2003). Cracking Paths at the Ply Interface in a CrossPly Laminate, Composites Part B: Engr., Vol. 34, pp. 437–445. Laws, N. and D. J. Dvorak. (1988). Progressive Transverse Cracking in Composite Laminates, J. Composite Mater., Vol. 22, pp. 900–916. Xia, Z. C., R. R. Carr, and J. W. Hutchinson. (1993). Transverse Cracking in Fiber-Reinforced Brittle Matrix, Cross-Ply Laminates, Acta Metall., Vol. 41, pp. 2365–2376.

11 MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR In previous chapters, we have assumed that all the inhomogeneities in the heterogeneous material behave linear elastically. Therefore, the overall behavior of the heterogeneous material is also linear elastic. For linear elastic behavior, the effective stiffness tensor is usually sufﬁcient to fully characterize the stress–strain relationship, or the material’s response under load. If one or more of the inhomogeneities in a heterogeneous medium behave nonlinearly (nonlinear elastic, viscoelastic, elastoplastic, elastoviscoplastic, etc.), the overall behavior, or the effective properties of the heterogeneous medium, will not be linear elastic. Unlike the effective stiffness and compliance for linear materials, the effective properties of nonlinear heterogeneous materials are much more complex to model and characterize. The main difﬁculty is the typical strong intraphase ﬂuctuations of the stress and strain ﬁelds in nonlinear heterogeneous materials and in the hereditary nature of most inelastic behaviors. At a given length scale, the responses of the inhomogeneities can vary markedly at different load levels. For example, a two-phase elastoplastic composite material effectively behaves as a multiphase material, and phase averages have less predictive capabilities than in the linear elastic case. In this chapter, we will develop a general framework based on the mean ﬁeld theories to describe the nonlinear behavior of heterogeneous media. Historically, the mean ﬁeld theory for inelastic behavior was developed mainly for crystalline materials initially. The early knowledge acquired through physical metallurgical studies of the plastic behavior 280

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

281

of single crystals leads naturally to a certain interest in their extension to polycrystals, where the main challenge is to relate the mechanical response of an aggregate of crystals (known as a polycrystal) to the fundamental mechanisms of single-crystal deformation. Speciﬁcally, the problem of predicting the yield stress of a polycrystal as a function of the yield strength of the constituent single crystals was considered by Sachs (1928) and studied more extensively later by Taylor (1938), whereas Schmid and Boas (1935) originated their fundamental law regarding the crystallographic slip within single crystals. Note that these earlier theoretical frameworks are speciﬁc to crystal plasticity and are formulated within a context closer to physical metallurgy than to mechanics of materials. More rigorous mechanistic analysis was carries out by Bishop and Hill (1951), who generalized the Taylor model to describe the different loading paths and to show their extreme features for the yield stress of polycrystalline materials. Subsequently, the development of metal forming processing and related plastic anisotropy problems resulting from texture evolutions provided the driving force in extending the Taylor model to more accurate approaches. In 1957, Eshelby introduced the concept of eigenstrains. The plastic deformation in each single crystal can be simulated by an eigenstrain distribution. Thus, the same homogenization techniques for linear elasticity can be followed to describe the nonlinear behavior of polycrystalline materials. This way of thinking was ﬁrst adopted by Budiansky and Mangasarian (1960) and developed later by Kro¨ner (1961). Their work constitutes the fundamental basis of the self-consistent mean ﬁeld theories for nonlinear behavior of heterogeneous materials. Unlike the Sachs and Taylor models, the self-consistent framework ensures both the compatibility and equilibrium conditions across the grains interface in polycrystalline aggregate. However, as discussed later, Kro¨ner’s model is limited to spherical inhomogeneities and isotropic matrix with incompressible plasticity. The next breakthrough was made by Hill (1965), who adopted the same concept as Kro¨ner (in the sense of Eshelby) by introducing an original idea of describing the plastic ﬂow by a sequence of linearizations leading to an incremental procedure of homogenization. In Hill’s approach, the overall behavior of the polycrystal, as well as the behavior of each grain, is approximated by a ‘‘pseudo’’-elastic behavior at each loading increment. Therefore, plastic unloading is accounted for. However, the nonlinear material behavior, compounded by the nonuniformity of stress and strain ﬁelds, renders the linearized properties nonuniform in each phase. This constitutes the major difﬁculty in using the Hill model without appropriate approximations.

282

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

The treatment of this difﬁculty was the center of different investigations leading to the emergence of mean ﬁeld theories with different varieties of linearization sequences of the nonlinear behavior. Within these procedures, one can distinguish between the secant, the tangent, and afﬁne approaches. The classical secant formulation was developed by Berveiller and Zaoui (1979) for crystalline materials and adapted later by Tandon and Weng (1988) to the case of two-phase elastoplastic composite materials. The secant formulation, which can be viewed as an intermediate method between the Kro¨ner approach and the incremental method of Hill, reduces signiﬁcantly the complexity of the Hill model by assuming isotropic homogeneous plastic ﬂow in each phase. The ﬁrst tangent mean ﬁeld method was introduced by Hutchinson (1976) to describe steady-state creep behavior of crystalline materials. It turns out that Hutchinson’s use of the power law creep also leads to another variant of the secant method (see below). More recently, Molinari et al. (1987) derived a tangent formulation for viscoplastic power law by adopting a sequence of linearization similar to linear thermoelasticity. All of these self-consistent methods rely on the assumption of piecewise uniform properties so that the Eshelby inclusion solution could be combined with the linearization procedure to obtain the overall nonlinear properties. However, for most nonlinear behavior such as plastic ﬂow, the ﬁelds ﬂuctuate in each phase and their heterogeneity increases (e.g., with the plastic ﬂow) at each loading increment. This makes it difﬁcult to assess the predictive capabilities of these self-consistent methods and to select the accurate one. Such limitation was the main motivation behind the development of the variational principles for nonlinear behaviors in the mid-1990s. Variational approaches for elastic and viscoelastic composites (Willis, 1983; Talbot and Willis, 1985; Castan˜eda, 1991; Suquet, 1993) combined with a linearization procedure enable us to compare some nonlinear mean ﬁeld theories to rigorous bounds of the Hashin– Shtrikman type. It turned out (Gilormini, 1997) that both tangent and secant approaches lead to estimates that are too stiff and can even violate the bounds in some cases. Different ways of thinking have emerged recently to overcome this deﬁciency of the mean ﬁeld theories. Improvements can be made by modifying the secant approach to take into account a better description of stress and strain ﬂuctuations at the microscale level. A ﬁrst attempt in this direction was made for particulate-reinforced composite by Qiu and Weng (1992). It uses the average strain energy in the matrix to

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

283

deﬁne its effective stress. Under this theory, the results are valid only for incompressible materials. A more general theory valid for arbitrary microstructure and compressible matrix has been developed by Suquet (1995). It was based on the second-order moments in each individual phase of the linear comparison solid. The use of second order moments has also been adopted independently by Hu (1996) and Buryachenko (1996). Another variety of the second-order estimates has been proposed by Castan˜eda (1996). It was based on Taylor’s second-order developments of stress, strain, and resulting potentials. An alternative in extending mean ﬁeld theories to secant formulation plasticity has been introduced by Dvorak (1992) using the transformation ﬁeld theory. The methodology models the plastic ﬂow of multiphase materials by a uniform piecewise distribution of eigenstrains. Such approaches are in principle suitable for use as micromechanically based constitutive laws in ﬁnite element codes. They are also very attractive in terms of computational requirements but tend to strongly overestimate the nonlinear overall response of heterogeneous materials because they essentially use elastic accommodation of microstress and strains throughout the loading history. In this chapter, several varieties of self-consistent mean ﬁeld theories will be discussed in details. Illustrative results for face-center-cubic (FCC) elastoplastic polycrystalline materials using an incremental selfconsistent scheme at small strains will be presented.

11.1

¨ NER’S MODEL ESHELBY’S SOLUTION AND KRO

As discussion above, the ﬁrst attempts made in modeling the elastoplastic behavior of polycrystalline materials through a homogenization scheme had their principal inspiration from the Eshelby inclusion solution in linear elasticity. The idea of liking these two problems came from two considerations. First of all, it is possible to describe the plastic strain of each individual grain by a distribution of eigenstrains (or stress-free strain) as introduced by Eshelby. Second, the interactions between a typical grain and its surrounding grains can be simulated by an inclusion problem of a single inhomogeneity undergoing a stressfree plastic strain while being surrounded by an equivalent homogeneous elastoplastic medium with appropriate boundary conditions. To introduce Kro¨ner’s model, let us consider a representative volume element of a polycrystalline material of total volume D comprised of N single crystals. It is assumed that D is much larger than the volume

284

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

of each crystal in the representative volume element of the polycrystal aggregate so that N ⬎⬎ 1. The representative volume element may be subjected to either the traction boundary condition • n兩S ⫽ • n

(11.1.1)

or the rate form of displacement boundary condition u˙ 兩S ⫽ ˙ • x,

(11.1.2)

where S is the surface of D and n is the outward unit normal of S. The overdot indicates the rate, or increment. Note that the rate here is typically not the change with respect to time. Instead, it is the change (or increment) with respect to the load. According to the average stress and average strain theorems introduced in Section 5.4, the volume averages of stress and strain tensors are ⫽

1 D

冕 dV, D

˙ ⫽

1 D

冕 ˙ dV.

(11.1.3)

D

For the sake of simplicity, we will consider in this chapter smallstrain deformation only. Therefore, it is possible to decompose the total strain and total strain rate into elastic and plastic parts, that is, ⫽ e ⫹ p,

˙ ⫽ ˙ e ⫹ ˙ p,

(11.1.4)

where e and p are the elastic and plastic parts of the strain tensor, respectively. The volume averages of strain and strain rate tensors can be decomposed similarly: ⫽ e ⫹ p,

˙ ⫽ ˙ e ⫹ ˙ p.

(11.1.5)

Note that, as discussed in Section 3.1, neither the elastic strain e nor the plastic strain p is compatible by itself, although the sum of these two ﬁelds is compatible. In other words, there is no, for example, such displacement ﬁeld uei such that eij ⫽ (ui,e j ⫹ uej,i)/2.

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

11.1

285

As discussed in Section 3.1, the elastic strain is related to the total stress through Hooke’s law, ⫽ Le ⫽ L( ⫺ p).

(11.1.6)

Single-phase polycrystals can be viewed as an assembly of essentially the same single crystals of different orientations and sizes. Therefore, an ensemble average of a ﬁeld quantity can be deﬁned as the average over all single crystals; see Section 5.3. For example, the ensemble averages of the stress and strain tensors are

冘 c ,

冘 c ,

N

具典 ⫽

r

r

N

具典 ⫽

r r

(11.1.7)

r⫽1

r⫽1

where cr is the volume fraction of the rth crystal in the polycrystal assembly D. As discussed in Section 5.3, we consider only statistically homogeneous media in this book. Therefore, the volume average and ensemble average of a ﬁeld quantity should be the same, for example, ⬅

⬅

1 D

冕 dV ⫽ 具典 ⬅ 冘 c ,

(11.1.8)

1 D

冕 dV ⫽ 具典 ⬅ 冘 c .

(11.1.9)

N

r

D

r

r⫽1 N

D

r r

r⫽1

Similarly, ˙ ⫽ 具典 ˙ ,

˙ ⫽ 具˙ 典.

(11.1.10)

However, due to the interphase incompatibilities of the elastoplastic strain ﬁelds, the elastic and plastic strain tensors by themselves may not be ergodic, that is, e ⫽ 具e典,

p ⫽ 具p典,

˙ e ⫽ 具˙ e典,

˙ p ⫽ 具˙ p典.

(11.1.11)

To illustrate these, let us assume that the representative volume element D is subjected to the traction boundary condition (11.1.1). In the absence of body forces (so assumed for the rest of this chapter), the total stress ﬁeld must satisfy

286

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

ⵜ⫽0

in D

(11.1.12)

n兩S ⫽ n.

(11.1.13)

and

Next, let e be the stress ﬁeld in D induced by the traction boundary condition (11.1.1) when all the single crystals in the polycrystal assembly D are linear elastic, that is, ⵜ e ⫽ 0

in D

(11.1.14)

e n兩S ⫽ n.

(11.1.15)

and

Clearly, the above equations imply that e is a statically admissible stress ﬁeld for the polycrystal assembly D subjected to the traction boundary condition (11.1.1), even when plastic deformation occurs. Further, since (11.1.14) and (11.1.15) describe a pure linear elastic problem, it then follows from (11.1.9) that e ⫽ ⫽ 具典 ⫽ 具 e典.

The strain ﬁeld corresponding to e can be written as ij ⫽ –12 (uei, j ⫹ uei, j) ⫽ Mijklekl,

(11.1.16) (11.1.17) (11.1.18)

where uei is the displacement ﬁeld when all the single crystals in the polycrystal assembly D behave linear elastically. Note that this ij is typically not the elastic part of the total strain ﬁeld eij introduced in (11.1.4), that is, ij ⫽ eij. Conceivably, e and are different because of plastic deformation that occurred in D. So, we introduce the plastic residual stress ﬁeld by p ⫽ ⫺ e

or ⫽ e ⫹ p.

(11.1.19)

It is so named because p represents the stress ﬁeld remained in the plastically deformed polycrystal assembly D after elastic unloading ( e ⫽ 0). Further, it follows from (11.1.16) that

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

p ⫽ 具 p典 ⫽ 0.

287

(11.1.20)

Equations (11.1.12)–(11.1.15) also imply that ⵜ p ⫽ 0

in D

(11.1.21)

and p n兩S ⫽ 0.

(11.1.22)

We call such stress ﬁeld self-equilibrium stress ﬁeld. Note that generally e ⫽ Le,

(11.1.23)

⫽ e ⫽ Le.

(11.1.24)

although

These can be seen from (11.1.6) and (11.1.19). Now, consider again the linear elastic problem. The stress ﬁeld in the rth single-crystal ⍀r can be written as er ⫽ Br

in ⍀r

(11.1.25)

where Br is the local elastic stress concentration tensor introduced in (5.7.9), which can be determined approximately by the homogenization schemes developed in Chapter 7. Note that

冘 c ⫽ 冘 c B ⫽ 冘 c B 具典 ⫽ 冘 c B 具 典. N

具 典 ⫽ e

N

r

r⫽1

e r

N

N

e

r

r

r⫽1

r

r

r

r⫽1

r

r⫽1

(11.1.26)

Thus,

冘 c B ⫽ I. N

具Br典 ⫽

r

r

r⫽1

Substituting (11.1.25) into the second of (11.1.19) yields

(11.1.27)

288

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

r ⫽ Br ⫹ rp

in ⍀r .

(11.1.28)

It then follows from the decomposition (11.1.4) that 具BT典 ⫽ 具BTe典 ⫹ 具BTp典,

(11.1.29)

具BT典 ⫽ 具MB典 ⫹ 具BTp典.

(11.1.30)

or

In deriving (11.1.30), we have substituted the elastic strain by using Hooke’s law in terms of elastic compliance M. The diagonal symmetry of M allows us to replace BT with B. In (11.1.30), we can show easily that the ﬁeld MB is kinematically admissible. Thus, application of the Hill lemma to 具MB典 yields 具MB典 ⫽ 具典具MB典 ⫽ M ⫽ e,

(11.1.31)

where M ⫽ 具MB典 is the effective elastic compliance of the polycrystalline material. On the other hand, since BT is statically admissible, one can write 具BT典 ⫽ 具BT典 ⫽ 具典 ⫽ ,

(11.1.32)

where (11.1.27) has been used. By combining (11.1.29), (11.1.31), and (11.1.32), one can conclude that e ⫽ 具BTe典 ⫽ 具e典,

p ⫽ 具BTp典 ⫽ 具p典.

(11.1.33)

The same statement can be made for the rates, ˙ e ⫽ 具BTe典 ⫽ 具˙ e典,

˙ p ⫽ 具BT˙ p典 ⫽ 具˙ p典.

(11.1.34)

Based on the foregoing discussions, one can derive some interesting and well-known features of crystalline materials.

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

289

Stored Elastic Strain Energy

The total elastic strain energy stored in D is given by U⫽

1 2

冕 dV. e

(11.1.35)

D

Making use of (11.1.6) and (11.1.19), we can rewrite this as

冕 M dV ⫽ 12 冕 ( ⫹ )M( ⫹ ) dV 1 1 ⫽ 冕 M dV ⫹ 冕 M dV ⫹ 冕 M dV. 2 2

U⫽

1 2

e

D

p

e

p

D

e

e

p

D

e

p

D

p

D

(11.1.36) Note that the ﬁrst term on the right-hand side is the strain energy in an elastic body. Thus, it follows from the discussions in Section 5.6 that

冕 M e

D

e

dV ⫽ DeMe ⫽ DM.

(11.1.37)

The second integral is

冕 M p

D

e

dV ⫽

冕 D

p ij

ij dV ⫽

冕 u

p e ij i, j

D

dV ⫽

冕 u n dV ⫽ 0, S

p e ij i j

(11.1.38) where we have used (11.1.18), (11.1.21), and (11.1.22). Thus, the strain energy stored in D when subjected to the traction boundary condition (11.1.13) is given by U⫽

D 1 M ⫹ 2 2

冕 M p

p

dV.

(11.1.39)

D

We see that the stored elastic strain energy contains, in addition to the macroscopic strain energy resulting from the applied load, a contribution from the plastic residual stresses.

290

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

Dissipated Energy

The dissipated energy due to plasticity, or the stress power from plasticity, is deﬁned as [see (2.3.5)] W⫽

1 2

冕 ˙ dV. p

D

Making use of the strain decomposition, this can be rewritten as W⫽

1 2

冕 ˙ dV ⫺ 12 冕 ˙ dV. e

D

(11.1.40)

D

It follows from the Hill lemma (5.5.5) that the ﬁrst term on the righthand side of (11.1.40) can be written as

冕 ˙ dV ⫽ D˙ ⫽ D D

e

⫹ D p .

(11.1.41)

Following the same arguments used in deriving the strain energy, the second term on the right-hand side of (11.1.40) can be written as

冕 ˙ dV ⫽ 冕 M˙ dV ⫽ D˙ ⫹ 冕 M˙ e

D

e

D

p

p

dV.

(11.1.42)

D

Hence D 1 ˙ p ⫽ W ⫹ 2 2

冕 M˙ p

D

p

dV ⫽

1 2

冕 ˙ dV ⫹ 21 冕 M˙ p

D

p

p

dV.

D

(11.1.43) This clearly shows that the macroscopic plastic stress power D˙ p is not completely dissipative. The ﬁrst term on the right-hand side of (11.1.43) is dissipative, while the second term resulting from the plastic residual stress is stored in the material. This contribution may explain the ‘‘interphase’’ work hardening observed in polycrystalline materials (see below).

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

291

Interphase Work Hardening

Following the same procedure used in calculating the dissipation energy, one can easily obtain the following: D 1 ˙ ˙ p ⫽ 2 2

冕 ˙ ˙ dV ⫹ 12冕 ˙ M˙ p

p

D

p

dV.

(11.1.44)

D

If all the single crystals in the polycrystal assembly behave as elastic perfectly plastic materials (without work hardening), then the plastic ﬂow of each crystal can be described using the normality rule as ˙ ˙ p ⫽ ˙ ƒ˙ ⫽ 0

in D,

where ƒ() is the yield surface and ˙ is the well-known plastic parameter. Therefore, we have D 1 ˙ ˙ p ⫽ 2 2

冕 ˙ M˙ p

D

p

dV ⱖ 0

(11.1.45)

because M is positive deﬁnite. Clearly, one can conclude from the inequality (11.1.45) that the macroscopic or homogenized behavior of polycrystal assembly display work hardening during its plastic ﬂow even though all of its single crystals are perfectly plastic. In other words, the inhomogeneity of the material is one of the sources of its work hardening. Such prediction has been conﬁrmed experimentally for polycrystalline materials. For example, for most single crystals, there is very little work hardening during the early stage (easy glide region) of deformation. However, during this stage, the polycrystal experiences a signiﬁcant work hardening due to the intergranular interactions among the single crystals. In general, a nonlinear heterogeneous material can be considered as a standard generalized material (in the sense of thermodynamics) by deﬁning appropriate internal variables, state variables, and associated thermodynamic forces. Such formulation requires an inﬁnite number of internal variables (e.g., the plastic strain ﬁeld), which renders such a procedure not feasible for practical situations. This is why nonlinear heterogeneous materials require suitable approximations to model their overall behavior. The modeling of nonlinear behavior in inhomoge-

292

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

neous materials is still a challenging issue and has not been solved completely yet.

Kro¨ner’s Approach

The modeling of elastoplastic behavior of polycrystalline materials by the concept of Eshelby’s elastic solutions was initiated by Budiansky and Mangasarian (1960). Their original idea was to model the ﬁrst stage of the plastic deformation so that Eshelby’s elastic inclusion solution is applicable without any major modiﬁcations. They argued that the favorably oriented grains that ﬁrst experience a plastic deformation can be simulated by an ellipsoidal inclusion subjected to stress-free plastic strain (eigenstrain) in interaction within an elastic inﬁnite medium representing the other grains that are still at the elastic regime. This approximation is also supported by the fact that the number of grains undergoing plastic deformation is low at the earlier stage of the plastic ﬂow, and hence the homogenization procedure can be performed by the dilute approximation. In other words, the interactions between the plastically deformed grains can be neglected. Subsequently, Kro¨ner, who initiated the self-consistent scheme in elasticity, proposed a similar formulation that enables us to describe the elastoplastic behavior beyond the earlier stages of the plastic ﬂow. Unlike Budiansky’s approach, Kro¨ner considered the inﬁnite medium in the Eshelby scheme as the ‘‘unknown’’ homogeneous medium subjected to an average p at a certain stage of the plastic ﬂow. To solve the interaction or localization problem for a given set of grains subjected to uniform plastic strain p, whereas the polycrystals as a whole is plastically deformed by p, Kro¨ner’s approximation adopts the Eshelby solution by describing the set of grains by an ellipsoidal inclusion subjected to an eigenstrain p and surrounded by an inﬁnite medium, which in turn is subjected to a uniform deformation p. One of the limitations of Kro¨ner’s model is that the framework was developed based on isotropic and spherical grains, and incompressible plasticity. Let us ﬁrst consider a homogeneous elastic matrix of stiffness L and volume D, subjected to a uniform strain . Let ⍀r be an ellipsoidal inclusion embedded within the matrix. It goes without saying that ⍀r ⬍⬍ D. To simulate the plasticity, let pr be an eigenstrain ﬁeld distributed in ⍀r . According to the Eshelby inclusion solution, the total strain on the inclusion is given by

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

r ⫽ ⫹ Srrp

in ⍀r ,

293

(11.1.46)

where Sr is the Eshelby inclusion tensor for ⍀r . This gives pr ⫽ Sr⫺1(r ⫺ )

in ⍀r .

(11.1.47)

The total stress ﬁeld in the inclusion is thus given by [see (4.3.22)] r ⫽ L(r ⫺ pr )

in ⍀r .

(11.1.48)

Substituting (11.1.46) into (11.1.48) gives r ⫽ L ⫹ L(Sr ⫺ I)rp ⫽ ⫹ L(Sr ⫺ I)rp,

(11.1.49)

where ⫽ L is the stress tensor averaged over the entire polycrystal assembly D. Recall that Eshelby’s tensor Sr depends on the elastic stiffness tensor L and the shape and orientation of the inclusion. Therefore, in its general form, (11.1.49) is capable of capturing the plastic anisotropy resulting from morphological aspects related to the irregular shape of grains. As mentioned above, Kro¨ner initially considered the case of spherical inclusions in isotropic matrix. Under such conditions, one has [see (2.4.23)] L ⫽ 3KIh ⫹ 2Id,

Sr ⫽ 3␥Ih ⫹ 2␦Id,

(11.1.50)

where ␥⫽

K 3K ⫹ 4

⫽

1⫹ , 9(1 ⫺ )

␦⫽

3(K ⫹ 2) 4 ⫺ 5 ⫽ , 5(3K ⫹ 4) 15(1 ⫺ ) (11.1.51)

K and are, respectively, the bulk and shear moduli, and is the Poisson ratio of the isotropic matrix material. The symbolic notation introduced in Section 1.4 has been used for isotropic fourth-order tensors. Thus, we have

294

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

L(Sr ⫺ I) ⫽ 3K(3␥ ⫺ 1)Ih ⫹ 2(2␦ ⫺1)Id.

(11.1.52)

The incompressibility of the plastic deformation means Ihpr ⫽ 0.

(11.1.53)

Thus, substituting (11.1.52) into (11.1.49) yields r ⫽ ⫹ 2(2␦ ⫺ 1)Idpr .

(11.1.54)

To describe the plastic ﬂow, (11.1.54) should be written in a rate or incremental form, that is, ˙r ⫽ ˙ ⫹ 2(2␦ ⫺1)Id˙ rp.

(11.1.55)

Substituting the second of (11.1.47) into (11.1.55), we arrive at ˙r ⫽ ˙ ⫹

(2␦ ⫺ 1) d I (˙r ⫺ ˙ ). 2␦

(11.1.56)

Equation (11.1.56) relates local quantities ˙ r and ˙ r to the macroscopic quantities ˙ and ˙ . It constitutes the ﬁrst step for a homogenization scheme crucial for an accurate prediction of the macroscopic behavior. It is clearly seen from (11.1.56) that the interaction between the different quantities is purely elastic. This results from the description of the plastic strain as an eigenstrain leading to a purely heterogeneous elastic problem. In reality, however, during the plastic ﬂow, constraints exerted by the aggregate on a single grain become softer than in the elastic regime and change with the plastic deformation. Since the Kro¨ner model is based on elastic constraints that remain elastic during the plastic ﬂow, it will result in stiffer predictions of the overall behavior. Let us now introduce the instantaneous or tangent modulus of the polycrystal Lt and the tangent modulus of the single-crystal Lt through ˙ ⫽ Lt˙ ,

˙ r ⫽ Lrt ˙ r .

(11.1.57)

Substituting (11.1.57) into (11.1.56) leads to

冋

Ltr ⫺

or

册 冋

册

(2␦ ⫺ 1) d (2␦ ⫺ 1) d I ˙ r ⫽ Lt ⫺ I ˙ 2␦ 2␦

(11.1.58)

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

11.1

˙ r ⫽ Ar˙ ,

295

(11.1.59)

where

冋

Ar ⫽ Lrt ⫺

册 冋

(2␦ ⫺ 1) d I 2␦

⫺1

Lt ⫺

册

(2␦ ⫺ 1) d I 2␦

(11.1.60)

deﬁnes the strain rate concentration tensor. Substitution of (11.1.60) into the second of (11.1.57) leads to

冘 c ˙ ⫽ 冘 L A ˙ . N

˙ ⫽

N

r

t r

r

(11.1.61)

r

r⫽1

r⫽1

One can then conclude that

冘LA N

L ⫽ t

t r

(11.1.62)

r

r⫽1

or

冘L 冋 N

L ⫽ t

t r

r⫽1

册 冋 ⫺1

(2␦ ⫺ 1) d L ⫺ I 2␦ t r

Lt ⫺

册

(2␦ ⫺ 1) d I . 2␦

(11.1.63)

Equation (11.1.63) inherits the implicit character of the selfconsistent scheme as is the case in linear elasticity. Clearly the nonlinearity is captured in (11.1.63) since the local tangent modulus depends on the plastic strain p. If we further assume that the instantaneous tangent modulus tensor is also isotropic, that is, Ltr ⫽ 3KtrIh ⫹ 2trId,

Lt ⫽ 3KtIh ⫹ 2tId,

(11.1.64)

then t r

L

冋

册 冋

(2␦ ⫺ 1) d L ⫺ I 2␦ t r

⫽ 3KtrIh ⫹

⫺1

Lt ⫺

2tr[4␦t ⫺ (2␦ ⫺ 1)] d I. 4␦tr ⫺ (2␦ ⫺ 1)

Making use of this in (11.1.63) gives us

册

(2␦ ⫺ 1) d I 2␦

(11.1.65)

296

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

[4␦ ⫺ (2␦ ⫺ 1)] . 冘 c 4␦ ⫺ (2␦ ⫺ 1) N

t ⫽

r

t r

t

t r

r⫽1

(11.1.66)

To see some insight of the Kro¨ner model prediction, we consider the case tr ⬍⬍ ,

t ⬍⬍ .

(11.1.67)

This is approximately true for later stages of plastic deformation. Under this assumption, (11.1.66) reduces to

冘 c. N

t ⬇

r

t r

(11.1.68)

r⫽1

This last equation is the Taylor–Lin bound, which is equivalent to the Voigt model in linear elasticity. In fact, the Taylor–Lin model (Taylor, 1938; Payne et al. 1958) assumes homogeneous strain in the polycrystalline aggregate so that ⫽ . Therefore, the effective tangent modulus predicted by the Taylor–Lin model simply leads to (11.1.68). Treating the interactions between grains as elastic instead of elastoplastic is one of the major limitations of the Kro¨ner model. Additionally, the consistency attributed to the Kro¨ner approach is not really true since in his procedure the equivalent homogeneous medium is taken to be elastic even though with assigned plastic deformation. These shortcomings are taken into consideration in the Hill selfconsistent model to be discussed next. In closing this section, we mention that although the Kro¨ner model presented here is in terms of a summation over all the single crystals, the results can be easily recast into integral forms (ensemble average), as discussed in Section 7.5. Hill’s Self-Consistent Model

To solve the nonlinear elastoplastic deformation, Hill proposed solving successive linear problems at each loading increment. To accomplish this, Hill introduced the following local and global constitutive laws: ˙ r ⫽ Lrt ˙ r ,

˙ ⫽ Lt˙ ,

(11.1.69)

where Ltr is the tangent modulus of the rth grain, Lt is the effective tangent modulus of the polycrystal assembly, and ˙ r and ˙ r are, re-

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

297

spectively, the stress and strain rates averaged over the rth grain, while ˙ and ˙ are, respectively, the stress and strain rates averaged over the entire polycrystal assembly. The inverse of these equations are ˙ r ⫽ Mrt ˙ r,

˙ ⫽ Mt ˙,

(11.1.70)

where Mtr is the tangent compliance of the rth grain and Mt is the effective tangent compliance tensor of the polycrystal assembly. To solve for Lt, we assume that the rth grain in the polycrystal assembly is simulated by an ellipsoidal inclusion ⍀r embedded in a homogeneous matrix with effective modulus tensor Lt, which is yet to be determined. As in the linear elastic case, such self-consistent approach accounts for, at least partially, the interactions between the grains. Making use of the rate form of (4.5.19), we have ˙r ⫽ ˙ ⫹ Hr(˙ ⫺ ˙ r),

(11.1.71)

where the concentration tensor Hr is given by [see (4.5.13)] Hr ⫽ Lt(S⫺1 ⫺ I). r

(11.1.72)

In the above, Sr is the Eshelby inclusion tensor computed for the inclusion ⍀r embedded in a matrix with elastic stiffness tensor Lt. It depends on the shape of ⍀r and on the overall property Lt. Note that, although (11.1.71) and (11.1.72) are similar to the linear elastic case, the effective property to be determined here is the effective tangent modulus of the heterogeneous material, not the effective elastic modulus. Substituting (11.1.69) into (11.1.71), one obtains (Ltr ⫹ Hr)˙r ⫽ (Lt ⫹ Hr)˙.

(11.1.73)

From this equation, the average strain rate on the rth grain is expressed in terms of the macroscopic strain rate as ˙ r ⫽ Ar˙ ,

(11.1.74)

Ar ⫽ (Lrt ⫹ Hr)⫺1 (Lt ⫹ Hr),

(11.1.75)

where

298

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

is the strain rate concentration tensor in elastoplastic deformation, which depends on the effective tangent modulus and geometrical aspects of the grain in consideration ⍀r . Similarly, making use of (11.1.70) in (11.1.71) gives the average stress rate on the rth grain in terms of the global stress rate, ˙ r ⫽ Br ˙,

(11.1.76)

Br ⫽ (H⫺1 ⫹ Mtr)⫺1 (H⫺1 ⫹ Mt). r r

(11.1.77)

where

It then follows from (11.1.74)–(11.1.76) and (11.1.69) and (11.1.70) that

冘 c ˙ ⫽ 冘 c L ˙ ⫽ 冘 c L A ˙ ,

(11.1.78)

冘 c ˙ ⫽ 冘 c M ˙ ⫽ 冘 c M B ˙ .

(11.1.79)

N

˙ ⫽

N

r

r

r

r⫽1

r⫽1

N

˙ ⫽

N

t r r

N

r r

t r

r

N

r

t r

r

r⫽1

r⫽1

r

r⫽1

r

t r

r

r⫽1

These lead to

冘cLA, N

Lt ⫽

r

r⫽1

t r

r

冘 c MB . N

Mt ⫽

r

t r

r

(11.1.80)

r⫽1

The last two equations are the Hill self-consistent scheme to evaluate the effective tangent modulus and effective tangent compliance tenors of a polycrystal assembly. Note that the second of (11.1.80) requires that the tangent compliance tensor Mt for each grain to exist. When this is the case, one can show that (see Problem 11.6) LtAr ⫽ BrLt and MtBr ⫽ ArMt.

(11.1.81)

This leads to ML ⫽ LM ⫽ I; see Problem 11.6. Therefore, it is sufﬁcient to solve either the ﬁrst or the second of (11.1.80). In practice, the ﬁrst of (11.1.80) is more widely used because Mt is not always well deﬁned for all single crystals for a given polycrystal assembly.

11.2

APPLICATIONS

299

As discussed in Section 7.5, (11.1.80) can be cast into an integral form. We will not repeat the discussion here. Readers are encouraged to formulate (11.1.80) into an integral form on their own. Note that (11.1.80) reduces to the self-consistent estimates (7.5.13) and (7.5.14) if the tangent modulus and tangent compliance tensors are replaced by their corresponding elastic stiffness and compliance tensors. This implies that the linear elastic behavior is a special case of the Hill model for elastoplastic behavior. Generally, (11.1.80) gives more accurate results in comparison with Kro¨ner’s model because Hill’s model captures at least partially the ﬂuctuations of strains between each grain. However, the Hill model is still an approximation because of the use of piecewise uniform mechanical properties on each grain. Therefore, any intraphase ﬂuctuation arising naturally from the elastoplastic behavior is disregarded in this approach. It should also be noted that obtaining Lt from (11.1.80) is not an easy task. This is due to the implicit nature of the equation and the anisotropy of the linearized constitutive laws (11.1.69), which makes the calculation of the Hill constraint tensors a complicated task. In general, the determination of Lt through (11.1.80) requires an iterative procedure. First, for a given state of deformation, an initial guess of Lt is used on the right hand of (11.1.80) to calculate an improved value for Lt. Then, this improved Lt is substituted back into the right-hand side of the equation again to obtain the next improvement. This procedure is repeated sufﬁciently until a convergent value is obtained for Lt. Another major difﬁculty behind the Hill self-consistent model is related to how the effective tangent modulus Lt depends on the prescribed values of strain rate ˙ . Unlike in the single-crystal case where only a ﬁnite number of branches exist, for polycrystals Lt varies continuously as the direction of prescribed strain rate varies in the strain rate space. In other words, Lt is a homogeneous function of degree zero of ˙ (Hutchinson, 1970). In practice, additional assumptions are usually made regarding the anisotropy of the tangent modulus in order to simplify the calculations. Examples of this will be discussed in the next section.

11.2

APPLICATIONS

The main purpose of this section is to explore the feasibility using the Hill self-consistent method to predict stress–strain behavior of poly-

300

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

crystalline materials from the elastoplastic properties of single-crystal constituents. We will focus on FCC metallic materials by presenting brieﬂy the main features of plastic deformation at the continuum level of single crystals under conventional loading conditions of strain rates and temperature. Our attention is not to describe exhaustively the various mechanisms of plastic deformation from a physical metallurgy point of view, for such a purpose the readers are referred to more specialized textbooks and technical papers that are recommended at the end of this chapter. Instead, we will follow a mechanistic procedure to bridge the scales between the single-crystal level and the polycrystalline level. Plastic Deformation of Single Crystals

The physical understanding of single-crystal plasticity was established during the earlier years of the last century, in 1900 to 1938, with the contribution of Ewing and Rosenhain (1900), Bragg and Bragg (1933), Taylor and co-workers (1923, 1925, 1934, 1938), Polanyi (1922), Schmid and Boas (1935), among others. Their experimental measurements established that at room temperature the major source of plastic deformation is the dislocation movements through the crystal lattices. These motions occur on certain crystal planes in certain crystallographic directions, and the crystal structure of metals is not altered by the plastic ﬂow. Mathematical descriptions of these physical phenomena of plastic deformation in single crystals were presented by Taylor (1938), when he investigated the plastic deformation of polycrystalline materials in terms of single-crystal deformation. More rigorous and rational formulations were given by Hill (1965), Hill and Rice (1972), Asaro and Rice (1977), and by Hill and Havner (1982). A comprehensive review of this subject can be found in Azaro (1983). The kinematics of single-crystal deformation and the resulting elastoplastic constitutive laws are based on an idealization of dislocation motion as a collective movement of the atoms leading to slips in certain directions on speciﬁc crystallographic planes. This process occurs when the resolved shear stress on one or more of these slip systems reaches a critical value. As plastic deformation proceeds, the critical yield stresses associated with the slip systems increases. This contributes to the strain hardening of the polycrystalline aggregate. Consider a single crystal with N possible slip systems. Each system g is characterized by the unit normal ng to the slip plane on which the collective movement of dislocations occurs, and by the direction mg of

11.2

APPLICATIONS

301

dislocation gliding, which is colinear with the Burger vector bg of gliding dislocations on the system g, so that bg ⫽ bmg, where b is the magnitude of the Burger vector. The mathematical tool treating the collective movement of dislocations considers each dislocation line as the boundary of a cutting surface Sg with a unit normal ng, across which the discontinuities of the displacement vector are uniform and characterized by the Burger vector bg so that bgi ngi ⫽ 0. This transformation can be described at each material point by a second-order tensor p(r) as pij(r) ⫽ bgi ngj ␦(Sg),

(11.2.1)

where ␦(Sg) is the surface Dirac function given by ␦(Sg) ⫽

冕

Sg

␦(r ⫺ r) dS⬘.

(11.2.2)

If many dislocations with the same Burger vector bg and the same cutting surfaces are present in the single-crystal volume V, one can deﬁne an average transformation p by pij ⫽ bmgi ngj

1 V

冕 ␦(S ) dV. g

(11.2.3)

V

Introducing the average plastic shear ␥ g by ␥g ⫽ b

1 V

冕 ␦(S ) dV g

(11.2.4)

pij ⫽ ␥ gmgi ngj .

(11.2.5)

V

leads to

If we account for all dislocations present at the slip systems, (11.2.5) can be extended to pij ⫽

冘␥mn. g

g g i j

g

The shear rate ␥˙ g is calculated from (11.2.4) as

(11.2.6)

302

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

␥˙ g ⫽ b

⭸ ⭸t

再

1 V

冕 ␦(S ) dV冎. g

(11.2.7)

V

Equation (11.2.7) describing the creation and movement of dislocations at the continuum level corresponds to the Orowan relation. The rate of plastic distortion ˙ p is the sum of the contributions of the shear rates ␥˙ g from all the active slip systems. That is ˙ pij ⫽

冘 ␥˙ m n . g

g g i j

(11.2.8)

g

The symmetric part of the plastic distortion gives the plastic strain rate ˙ pij ⫽

1 ˙p ( ⫹ ˙ pji) ⫽ 2 ij

冘 ␥˙ R , g

g ij

(11.2.9)

g

where Rgij ⫽ –12 (mgi ngj ⫹ mgj ngi ).

(11.2.10)

The antisymmetric part of the plastic distortion deﬁnes the plastic spin, w ˙ pij ⫽

1 ˙p ( ⫺ ˙ jip) ⫽ 2 ij

冘 ␥˙ R˜ , g

g ij

(11.2.11)

g

where R˜ gij ⫽ –12 (mgi ngj ⫺ mgj ngi ).

(11.2.12)

˜ g are also called the orientation The second-order tensors Rg and R tensors because they depend only on the orientation of the single crystal in consideration. Let denote the stress in the single crystal. The so-called resolved shear stress on a slip system g is given by

g ⫽ ij Rgij.

(11.2.13)

Within the framework of time-independent plasticity (any viscous effect is neglected), a slip system g is considered to be active if the resolved shear stress g reaches a critical value gc , which depends on

11.2

APPLICATIONS

303

the previous deformation history of the single crystal, leading to a strain hardening state. It is generally assumed that the deformation history of a given slip system g depends on only the amplitude of shear strain associated with N active systems, so that one can write gc ⫽ F˜ g (␥1, ␥2, . . . , ␥ N).

(11.2.14)

When the amount of shear is small enough, we can use a linear approximation of (11.2.14), gc ⬇ F˜ g (0, 0, . . . , 0) ⫹

冘 ⭸⭸␥F˜ (0, 0, . . . , 0)␥ , g

h

h

h

(11.2.15)

where F˜ g (0, 0, . . . , 0) can be viewed as the initial critical shear stress of the slip system g. It is generally assumed the same for all slip systems. Therefore, (11.2.15) can be expressed as gc ⫽ 0 ⫹

冘H ␥ gh

h

(11.2.16)

h

where 0 ⫽ F˜ g (0, 0, . . . , 0), and Hgh ⫽ ⭸F˜ g / ⭸␥ h (0, 0, . . . , 0) is the strain hardening matrix, which describes the hardening interactions between the different slip systems. Note that the diagonal components of the matrix Hgh deﬁne the self-hardening due to the plastic shear in the same system, while the nondiagonal components correspond to the latent hardening due to shear slip on the other systems. The matrix coefﬁcients can be evaluated by experimental characterization performed on single crystals. At any stage of the deformation process, the rate of changes of critical shear stress is deduced from (11.2.16) as ˙ gc ⫽

冘 H ␥˙ . gh

h

(11.2.17)

h

It follows from the above deﬁnitions that a slip system is potentially active if g ⫽ gc and loading or unloading, respectively, depending on whether ˙ g ⫽ ˙ gc

or

with ␥˙ g ⱖ 0

(11.2.18)

304

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

˙ g ⬍ ˙ gc

with ␥˙ g ⫽ 0.

(11.2.19)

A system is inactive if g ⬍ cg and ␥˙ g ⫽ 0. Relation (11.2.17) is known as the consistency condition whose resolution for each active system g determines the shear rate ␥˙ g on this system. Taking into account (11.2.13) and (11.2.18), the consistency condition writes ˙ ijRijg ⫽

冘 H ␥˙ . gh

h

(11.2.20)

h

From the deﬁnition (11.2.9) of the plastic strain rate, the total strain rate is the sum of the elastic and plastic parts, that is, ˙ ⫽ ˙ e ⫹ ˙ p ⫽ L⫺1 ˙ ⫹

冘 ␥˙ R g

g

(11.2.21)

g

or

冉

˙ ⫽ L ˙ ⫺

冘 ␥˙ R 冊. g

g

(11.2.22)

g

Note that for a given state of stress , ˙ is uniquely related to ˙ if the hardening matrix Hgh, governing the shear rates in different slip systems, is positive semideﬁnite (Hill, 1966), while only for certain hardening laws are the shear rates ␥˙ g always unique. At least one set of shear rates exists that satisﬁes the constitutive relations (11.2.9) and (11.2.17) through (11.2.21) for a prescribed strain rate ˙ (or prescribed stress ˙ ). If there are N nonzero ␥˙ g, they would satisfy N equations resulting from the combination of the consistency condition ˙ g ⫽ ˙ gc and the constitutive relations (11.2.22). In fact, substituting (11.2.22) into (11.2.20) yields the following set of equations:

冘 Q ␥˙ gh

h

⫽ RgL˙,

(11.2.23)

h

where Qgh ⫽ Hgh ⫹ RgLRh.

(11.2.24)

These equations are associated with the loading system together with the constraints ␥˙ h ⱖ 0.

11.2

APPLICATIONS

305

Only for certain hardening laws will the N ⫻ N matrix Qgh be necessarily nonsingular. For perfect plasticity (Hgh ⫽ 0), for example, it is always possible to choose at least one set of linearly independent slip systems among the potentially active ones such that this matrix is nonsingular and the auxiliary equations (11.2.20) are satisﬁed. Thus, for perfect plasticity the dimension of Qgh is never greater than 5 ⫻ 5. If ˜ gh, the N nonzero shear rates for this choice its inverse is denoted by Q of active slip systems are expressed by ៣ ␥˙ g ⫽ ˙ g˙

with

៣g ˙ ⫽

冘Q˜ LR . gh

h

(11.2.25)

h

Recall that the tangent modulus and compliance tensors of a single crystal are given, respectively, by (11.1.69), that is, ˙ ⫽ Lt˙ ,

˙ ⫽ Mt ˙.

(11.2.26)

From the foregoing kinematics of single-crystal plastic deformation, the main feature of the tangent modulus and compliance is that they depend on the set of active slip systems, which in turn depends on the prescribed strain rate ˙ (or stress ˙ ). It is well known in crystal plasticity that the deﬁnitions of tangent modulus and tangent compliance lead to a multibranch description. It also should be noted that, regarding (11.2.26), the inverse of tangent modulus does not exist in all situations. In other words Lt may possess some singularities. Perfect plastic behavior is one of such cases, where the problem of homogenization is typically carried out by using directly the tangent modulus rather than its inverse, since there is no restriction on the strain rate, whereas the stress rate is subjected to certain conditions regarding the regions in stress rate space. Substituting (11.2.25) into (11.2.22) and in comparison to (11.2.26), one obtains the following expression for single-crystal tangent modulus:

冉

Ltijmn ⫽ Lijkl Iklmn ⫺

冘 R ៣˙ g kl

g

冊

g mn

.

(11.2.27)

Using (11.2.25) and (11.2.24), (11.2.27) can be explicitly rewritten as

冉

Ltijkl ⫽ Lijmn Imnkl ⫺

冘 (H

gh

g,h

冊

⫹ RgLRh)⫺1 RgmnLklpqRhpg .

(11.2.28)

306

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

It can be readily shown that the tangent modulus Lt as given by (11.2.28) satisﬁes the symmetries Ltijkl ⫽ Ltklij if Hgh ⫽ Hhg.

(11.2.29)

If the single crystal is assumed to be elastically isotropic, then we have [see (1.4.5)] L ⫽ 3KIh ⫹ 2Id,

(11.2.30)

where Ihijkl ⫽ –13 ␦ij␦kl,

d Iijkl ⫽ –12 (␦ik␦jl ⫹ ␦il␦jk ⫺ –32 ␦ij␦kl).

The tangent modulus thus becomes Ltijkl ⫽ 3KIhijkl ⫹ 2Idijkl ⫺ 42

冘R

g ij

(Hgh ⫹ 2RgpqRhpq)⫺1 Rhkl,

g,h

(11.2.31) where the plastic incompressibility is used. In summary, the single-crystal tangent modulus described by (11.2.28) and (11.2.31) is unique for a given strain rate ˙ even if the strain rates ␥˙ g are not. Referring to (11.2.31), one can remark that even though the elasticity is approximated as isotropic, the tangent moduli are anisotropic in nature. This results from the typical process of the plastic ﬂow activated on discrete slip systems and their interactions governing the strain hardening behavior. Plastic Deformation of Polycrystalline Materials

In the previous section, we presented a possible way to determine the tangent modulus of a single crystal from the theory of homogeneous and continuum slip on well-deﬁned slip systems. Let us now consider a polycrystalline material where the current conﬁguration has undergone certain plastic deformation, and the potentially active slip systems as well as the stress distribution in each grain are known. In this stage the polycrystal is subjected to a loading increment characterized, for example, by a strain rate ˙ . To determine the effective tangent modulus Lt using the Hill self-consistent model, we need to evaluate the instantaneous stress and strain rates, ˙ and ˙ , as well as the tangent moduli t L , for a given prescribed macroscopic stress rate ˙ or strain rate ˙ .

11.2

APPLICATIONS

307

To this end, an iterative procedure is needed. First, a tentative guess is made for Lt so that the Hill constraint tensor given by (11.1.72) can be determined. Then, for each active set of slip systems, necessarily a subset of potentially active systems, the tangent modulus for the grain considered is calculated from (11.2.28) or (11.2.31) in the case of isotropic elasticity. Next, the strain concentration tensor A is computed for this grain using (11.1.75). To ensure that the assumed set of active slip systems do constitute the correct branch of Lt for the prescribed ˙ (or ˙ ), the auxiliary conditions (11.2.20) should be checked by taking into account Eqs. (11.1.75) and (11.2.26). If condition (11.2.20) is fulﬁlled, then Lt is correct for this iteration; if not, a new set of potentially active systems should be chosen until the correct Lt and A are found. This procedure is carried out for each grain orientation. The ﬁnal step in the ﬁrst iteration is to calculate an improved estimate (in comparison to the initial guess) of Lt from (11.1.80). The entire procedure is then repeated until a convergent Lt is reached. In the next two sections, the method is illustrated by simulating a monotonically increasing uniaxial load. In this case, the tangent modulus tensor is transversely isotropic. The corresponding Eshelby inclusion tensor and the Hill constraint tensors are obtained for computing the strain or stress concentration tensors. Hutchinson’s Calculations

Hutchinson (1970) implemented the Hill self-consistent model to study the behavior of a polycrystal consisting of randomly oriented FCC single crystals. In his computational procedure, the grains are considered spherical in shape and their orientations are assumed equally represented so that the average procedure required for the homogenization steps can be performed over all orientations. The elasticity of each single crystal is described by three independent Voigt elastic constants C11, C12, and C44 in the classical way of cubic symmetries. The random distribution of single crystals leads to isotropic overall elastic constant of the polycrystalline aggregate characterized by its bulk modulus K and shear modulus . Using the linear elastic self-consistent method for randomly distributed cubic crystal, the elastic moduli of the polycrystal can be obtained (Problem 11.4): K ⫽ –13 (C11 ⫹ 2C12), 83 ⫹ (5C11 ⫹ 4C12) 2 ⫺ C44 (7C11 ⫺ 4C12) ⫺ C44 (C11 ⫺ C12)(C11 ⫹ 2C12) ⫽ 0.

(11.2.32)

(11.2.33)

308

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

An FCC single crystal has crystallographically similar systems whose unit normals are the four [1,1,1]-type directions, relative to the crystal axes, and whose slip directions are the [1,1,0] types. As for elastic deformation, the self-consistent method can be used to express the initial critical macroscopic stress 0c (the yield stress) in terms of the initial shear stress 0c of a slip system introduced by (11.2.16). That is (see Problem 11.5) 0c ⫽ 0c

冪冉

3

2 ⫹ 32 2 2

冊

,

(11.2.34)

where 2 ⫽

C11 ⫺ C12 , 2(1 ⫺ 2␦) ⫹ 2␦(C11 ⫺ C12)

3 ⫽

C44 , (1 ⫺ 2␦) ⫹ 2␦C44 (11.2.35)

and ␦ is given by (4.3.38). For the case of isotropic elasticity where 2C44 ⫽ C11 ⫺ C12, it can be readily shown that 2 ⫽ 3 ⫽ 1. Hence 0c ⫽ 0c . Note that expression (11.2.33) is equivalent to assuming a Tresca criterion for the overall yield stress. This is only valid if no residual stresses are present in the polycrystalline materials. During a monotonic uniaxial tensile test in the x3 direction, the tangent moduli L display transverse isotropy with respect to the macroscopic coordinate system, so that Hooke’s law can be written in terms of the Voigt elastic constants:

冢冣冢 ˙ 11 ˙ 22 ˙ 33 ˙ 13 ˙ 23 ˙ 12

⫽

Ct11 Ct12 Ct13 Ct11 Ct11 Ct13 Ct11 Ct11 Ct33 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 t C44 0 t 0 C44 0 0

冣冢 冣

0 0 0 0 0 Ct66

˙ 11 ˙ 22 ˙ 33 2˙13 2˙23 2˙12

,

(11.2.36)

where t t Ct66 ⫽ –21 (C11 ⫺ C12 ).

(11.2.37)

11.2

APPLICATIONS

309

Copper is selected for this simulation because its single crystal shows strong elastic anisotropy. The elastic moduli for single-crystal copper used in our calculations are C12 /C11 ⫽ 0.722 and C44 /C11 ⫽ 0.447. The self-consistent predictions using Eqs. (11.2.32)–(11.2.34) give, respectively, the polycrystalline elastic moduli and initial critical shear stress: K ⫽ 0.815C11,

⫽ 0.285C11,

0c ⫽ 1.129 0c

(11.2.38)

or ⫽ 0.343,

E ⫽ 0.722C11,

(11.2.39)

where E is Young’s modulus and Poisson’s ratio. Furthermore, we pay particular attention to the single-crystal strain hardening and its effect on the polycrystalline hardening, by considering both perfect plasticity for each grain, as well as different forms of the hardening matrix Hgh. As shown by Kneer (1965), the transverse isotropy of the overall tangent modulus leads to analytical expressions of the Eshelby tensor. It follows from the Kneer calculations that the Eshelby tensor can be expressed as Sijkl ⫽ TijmnLmnkl, where

冘 K T˜ , 1 z ⫽ 冕 dz, 8 a ⫹az ⫹az ⫹az 3

Tijmn ⫽

(m) (m) ijmn

m⫽0

1

K(m)

0

2m

2

0

1

4

2

6

(m ⫽ 0, 3).

3

The coefﬁcients am and T˜ (m) ijmn are a polynomial functions of the components Cij of the transverse isotropic tangent modulus. Details of this calculation can be found in (Kneer, 1965). We ﬁrst consider the case without strain hardening in single crystals. The results are presented in Figure 11.1 for isotropic elasticity and anisotropic elasticity with the moduli of copper listed in (11.2.38). Clearly, the results show that the elastic anisotropy increases the initial

310

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

2.0 Anisotropic, Nonhardening Single Crystals C12 C11 = 0.722 C44 C11 = 0.447

1.6

σ 2τ c0 1.2 Isotropic, Nonhardening Single Crystals ν = 13 0.8

1

2

Eε 2τ c0

3

4

Figure 11.1 Tensile stress–strain curves for FCC polycrystals with randomly oriented and perfectly plastic single crystals.

yield stress of the polycrystal. This is not expected because the inhomogeneous elasticity arising from single-crystal anisotropy should decrease, rather than increase, the yield strength of the polycrystal yields. This might be explained by the fact that stresses in each grain are estimated by treating them as spherical inclusions. This is one of the limitations of the self-consistent model. As discussed previously, the polycrystalline aggregate displays a strain hardening behavior even if every single crystal in the aggregate behaves as a perfect plastic material. This arises from the intergranular interactions. To show the effect of single-crystal strain hardening, the interaction matrix Hgh should be estimated. In general, this procedure requires an experimental analysis performed on single crystals. Different forms of strain hardening matrix have been proposed in the literature. Taylor’s (1938) isotropic hardening law is the simplest and the most widely used one. This law states that the yield stresses of all slip systems remain equal and increase in proportion to the total shear. So that Hgh ⫽ h for all g and h, we have ˙ gc ⫽ h兺h ␥˙ h. Taylor’s simple hardening law is not able to reproduce the principal features of a single-crystal hardening, nor can it capture the polycrystalline hardening behavior, especially, at later stages of plastic deformation where multiple activations of slip systems render the interactions highly anisotropic. Nevertheless, the Taylor’s hardening law is used in the calculations presented in Figure 11.2 to show at least at the earlier stage of the

11.2

1.6

1.4

h = 0.04 µ

311

h = 0.02 µ

σ 2τ c0

h = 0.0 µ

1.2

1.0

APPLICATIONS

1

3

2

4

Eε p 2τ c0 Figure 11.2 Effect of single-crystal hardening.

plastic ﬂow the effect of single crystals hardening. The computations are performed for different hardening parameters h. Finally, under the same conditions without single-crystal hardening, the stress–strain relationship for polycrystal copper is estimated using the upper bound of the Taylor–Lin model and the Kro¨ner’s selfconsistent model. The comparison is shown in Figure 11.3. As discussed throughout this chapter, the stress–strain curve obtained from Kro¨ner’s model lies above the one obtained by the Hill method. This is expected because in the Kro¨ner inclusion problem, the matrix exerts

Kröner’s model

1.4

σ 2τ c0

Hill’s model 1.2 Lin’s model

1.0

1

2

Eε p

3

4

2τ c0 Figure 11.3 Upper and lower bounds on stress–strain curves.

312

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

an elastic constraint, whereas in the Hill model the matrix provides a much softer constraint because of plastic deformation.

11.3 TIME-DEPENDENT BEHAVIOR OF POLYCRYSTALLINE MATERIALS: SECANT APPROACH

Time-dependent behavior of polycrystalline materials was ﬁrst modeled by Hutchinson (1976) by assuming a power law describing the shear rate on slip systems for a given single crystal. The analysis was performed under small-strain condition leading to an elastoviscoplastic type behavior. Hutchinson (1976) assumed a steady-state creep behavior for single crystals for which the shear rate induced in a slip system g by a given resolved shear stress g is described by a rate-sensitive criterion, which is equivalent to assuming a nonlinear viscous behavior:

冉冊

n

␥˙ ⫽ ␥˙ g

0

g , gc

(11.3.1)

where ␥˙ 0 is a reference rate and n is the inverse of rate sensitivity. When n ⬎⬎ 1, the shear rate increase is negligible unless g is very close to gc . This statement is equivalent to conditions (11.2.19) and (11.2.20) for slip systems activation in time-independent plasticity. The critical shear stress gc , often called reference stress in time-dependent plasticity, is strongly dependent on temperature. The exponent n depends also on temperature, although somewhat less strongly, and usually falls between 3 and 8 for metals. A survey on the temperature ranges where the steady-state creep of polycrystal and single crystal can be approximated by a power law was given by Ashby and Frost (1975). If N is the total number of slip systems, the total strain rate is the sum of the contributions from all these systems:

冘 ␥˙ N

˙ ij ⫽

g⫽1

where

g

s Rijg ⫽ Mijpq pq,

(11.3.2)

11.3

TIME-DEPENDENT BEHAVIOR OF POLYCRYSTALLINE MATERIALS

冘冉 N

s ijpq

M

⫽

g⫽1

␥˙ 0 gc

冊冉 冊 g gc

313

n⫺1

RgijRgpq

(11.3.3)

with Ms being the so-called secant viscoplastic compliance of the single crystal. As reported by Hutchinson (1976), the compliance tensor is homogeneous of degree n ⫺ 1 in stress so that Ms () ⫽ n⫺1Ms ().

(11.3.4)

Let us now deﬁne the stress potential () and strain rate potential (˙ ) such that ˙ ⫽

⭸ ⭸

and ⫽

⭸ . ⭸˙

(11.3.5)

The viscoplastic constitutive law (11.3.2) leads to the following typical relationships between the dissipation ˙ , (), and (˙ ): ˙ ⫽ (n ⫹ 1)() ⫽

n⫹1 (˙) ⫽ n

冘 ␥˙ . n

g

g

(11.3.6)

g⫽1

Substituting (11.3.5) into (11.3.6) and by differentiating (11.3.6) with respect to the stresses, one obtains ⭸ ⭸ ⭸ ⭸2 (kl˙ kl) ⫽ (n ⫹ 1) ⫽ ⫹ kl . ⭸ij ⭸ij ⭸ij ⭸ij ⭸kl

(11.3.7)

This last equation leads to n

⭸ ⭸2 ⫽ kl . ⭸ij ⭸ij ⭸kl

(11.3.8)

Combining (11.3.8) with (11.3.2), we can readily show that Msijkl ⫽ where

1 ⭸2 , n ⭸ij ⭸kl

(11.3.9)

314

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

⭸2 ⭸˙ ⫽ ij ⫽ Mtijkl. ⭸ij ⭸kl ⭸ij

(11.3.10)

In Eq. (11.3.10), Mt is the tangent compliance tensor. On the other hand, a Taylor expansion of (11.3.2) at the vicinity of a point ˜ ⫺ ˙ can be written as ˙ ij ⫽

冏

⭸˙ ij ⭸kl

kl ⫹ ˜˙ ij ⫽ Mtijkl ( ˙ ) kl ⫹ ˜˙ ij,

(11.3.11)

⫽ ˜

where ˜˙ ij is called the back-extrapolated strain rate. From (11.3.9) and (11.3.10), the relation between the grain’s secant and tangent compliances are Mt ⫽ nMs.

(11.3.12)

At the polycrystal level, the macroscopic constitutive law is assumed to be similar to that of single crystals, so that one can write s ˙ ij ⫽ Mijpq pq,

(11.3.13)

where Ms is the macroscopic secant compliance tensor. In the same way as in the single-crystal case, Taylor expansion of (11.3.13) at the vicinity of the macroscopic stress leads to the deﬁnition of a macroscopic tangent modulus Mt as t ˙ ij ⫽ Mijpq () pq ⫹ ˙ ij0,

(11.3.14)

where Mtijkl () ⫽ ⭸˙ ij / ⭸kl兩⫽ and ˙ 0ij is a macroscopic extrapolated strain rate. Hutchinson (1976) has shown that the macroscopic tangent and secant compliance tensors are linked by a relation similar to the one for single crystals, that is, Mt ⫽ nMs. This is derived by deﬁning the macroscopic dissipation ˙ , macroscopic strain rate potential ⌽(˙ ), and stress potential ⌿() such that ˙ ⫽

⭸⌿ ⭸

and ⫽

⭸⌽ . ⭸˙

Note that Eqs. (11.3.11) and (11.3.14) are exact only when they describe the strain rate associated with the stress used as a reference

11.3

TIME-DEPENDENT BEHAVIOR OF POLYCRYSTALLINE MATERIALS

315

for the expansion. Otherwise they are only approximate. This will not present a limitation for the treatment of the grains since the stress and the strain rates are assumed to be uniform within the framework of the self-consistent scheme. As a result, the actual value of stress in the grain considered can be selected to perform the expansion. Starting from the linearized equation (11.3.14), the macroscopic tangent compliance tensor Mt can be estimated by adopting a Hill-type self-consistent method. In other words, one can consider each grain with tangent compliance Mt and prescribed reference strain rate ˜˙ embedded in a homogenized effective medium having the properties of Mt and prescribed reference strain rate ˙ 0. Following the same procedure as for Eqs. (11.1.71) and (11.1.72), the Eshelby solution extended to a tangent formulation gives the interaction relation linking the local to the macroscopic quantities [see (4.5.19)], ˜ ⫺ ), ˙ ⫽ ˙ ⫹ H(

(11.3.15)

˜ is the inverse of the Hill constant tensor, where H ˜ ⫽ (S⫺1 ⫺ I)⫺1 Mt. H

(11.3.16)

Note that Eshelby’s tensor in (11.3.16) depends on the tangent compliance tensor together with the shape of the grain in consideration. As reported by Lebensohn and Tome´ (1993), the relation Mt ⫽ nMs enables us to express the equations in terms of the secant compliance tensor as ˜ ⫽ n(S⫺1 ⫺ I)⫺1 Ms. H

(11.3.17)

Substituting (11.3.2) and (11.3.12) into (11.3.15) yields ⫽ B,

(11.3.18)

where ˜ ⫺1 (Ms ⫹ H). ˜ B ⫽ (Ms ⫹ H)

Finally, the homogenization procedure using ⫽ 具典 and Ms ⫽ 具MsB典 leads to ˜ ⫺1 (Ms ⫹ H) ˜ 典. Ms ⫽ 具Ms ⬊(Ms ⫹ H)

(11.3.19)

316

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

In summary, we have introduced in this section the viscoplastic selfconsistent model initially developed by Hutchinson (1976) for modeling steady-state creep of polycrystalline materials, and have shown how to relate a secant formulation to a tangent formulation. We have also shown how the Eshelby solution required for the self-consistent scheme can be used to combine both the secant and tangent moduli for solving interaction problems. Since Hutchinson’s work (1976), the viscoplastic self-consistent model has been adopted by many authors as an alternative strategy to tackle the problem of large plastic deformations by simply neglecting the elastic deformation. This way of thinking was successively adopted by Molinari et al. (1987) to describe the texture development in cubic polycrystals. For more information regarding the numerical implementation and limitations of the method, the readers are referred to the work of Lebensohn and Tome´ (1993). PROBLEMS

11.1 Prove Eq. (11.1.30). 11.2 Check the consistency L ⫽ (M)⫺1 of the prediction from (11.1.80). 11.3 Show that, for perfect plasticity, the dimension of Qgh is never greater than 5 ⫻ 5. 11.4 For cubic symmetries, if we assume that all single crystals are randomly oriented, show that a self-consistent estimation of the elastic constant of the polycrystal gives isotropic moduli expressed by Eqs. (11.2.32) and (11.2.33). 11.5 For cubic symmetries, if we assume that all single crystals are randomly oriented, show that the overall critical shear stress is given by (11.2.38). 11.6 Show the following relationships: LtAr ⫽ BrL and MtBr ⫽ ArM.

REFERENCES Asaro, R. J. (1983). Crystal Plasticity, J. Appl. Mech., Vol. 50, pp. 921–934. Asaro, R. J. and J. R. Rice (1977). Strain Localization in Ductile Single Crystals, J. Mech. Physics Solids, Vol. 25, pp. 309–338.

REFERENCES

317

Ashby, M. F. and Frost, H. J. (1975). The Kinematics of Inelastic Deformation Above 0 K, in Constitutive Equations in Plasticity, A. S. Argon, ed., MIT Press, Cambridge. pp. 117. Berveiller, M. and A. Zaoui (1979). An Extension of the Self-Consistent Scheme to Plastically-Flowing Polycrystals, J. Mech. Phys. Solids, Vol. 26, pp. 325–344. Bishop, J. F. W. and R. Hill (1951). A Theoretical Derivation of the Plastic Properties of a Polycrystalline Facecentered Metal, Phil. Mag. Vol. 42, pp. 1298–1307. Bragg, W. H. and W. L. Bragg (1933). The Crystalline State, Bell, London. Budiansky, B. and O. L. Mangasarian (1960). Plastic Stress Concentration at Circular Hole in Inﬁnite Sheet Subjected to Equal Biaxial Tension, J. Appl. Mech., Vol. 27, pp. 59–64. Buryachenko, V. (1996). The Overall Elastoplastic Behavior of Multiphase Materials with Isotropic Components, Acta Mech., Vol. 119, pp. 93–117. Castan˜eda, P. (1991). The Effective Mechanical Properties of Nonlinear Isotropic Composites, J. Mech. Phys. Solids, Vol. 39, pp. 45–71. Castan˜eda, P. (1996). Exact Second-Order Estimates for the Effective Mechanical Properties of Nonlinear Composite Materials, J. Mech. Phys. Solids, Vol. 44, pp. 827–862. Dvorak, G. J. (1992). Transformation-Field Analysis of Inelastic Composite Materials, Proc. R. Soc. London, Ser. A, Vol. 431, pp. 89–110. Ewing, J. A. and W. Rosenhain (1900). Experiments In Micro-Metallurgy: Effects of Strain. Preliminary Notice, Philos. Trans. R. Soc. Lond., Vol. A199, pp. 85–90. Eshelby, J. D. (1957). The Determination of the Elastic Field of an Ellipsoidal Inclusion and Related Problems, Proc. Roy. Soc. Lond. Vol. A241, pp. 376– 396. Gilormini, P. (1997). Shortcomings of Several Extensions of the Self Consistent Model for Heterogeneous, Nonlinear Solids, Revue de Metallurgie, Vol. 94, pp. 1081–1087. Hill, R. (1965). Continuum Micro-mechanics of Elastoplastic Polycrystals, J. Mech. Phys. Solids, Vol. 13, pp. 89–101. Hill, R. (1966). Generalized Constitutive Relations for Incremental Deformation of Metals by Multislip, J. Mech. Phys. Solid, Vol. 14, p. 99. Hill, R. and K. S. Havner (1982). Perspectives in the Mechanics of Elastoplastic Crystals, J. Mech. Phys. Solids, Vol. 30, pp. 5–22. Hill, R. and J. R. Rice (1972). Constitutive Analysis of Elasto-Plastic Crystals at Arbitrary Strains, J. Mech. Phys. Solids, Vol. 20, pp. 401–413. Hu, G. (1996). A Method of Plasticity for General Aligned Spheroidal Void of Fiber-Reinforced Composites, Int. J. Plasticity, Vol. 12, pp. 439–449. Hutchinson, J. W. (1970). Elastic-Plastic Behaviour of Polycrystalline Metals and Composites, Proc. R. Soc. Lond., Vol. A319, pp. 247–272.

318

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

Hutchinson, J. W. (1976). Bounds of Self-Consistent Estimates for Creep of Polycrystalline Materials, Proc. R. Soc. Lond., Vol. A348, pp. 101–127. Kro¨ner, E. (1961). Zur plastischen Verformung des Vielkristalls, Acta Metall., Vol. 9, pp. 155–161. Lebensohn, R. and C. N. Tome´ (1993). A Self-Consistent Anisotropic Approach for the Simulation of Plastic Deformation and Texture Development of Polycrystals Applications to Zirconium Alloys, Acta Metall. Mater., Vol. 41, pp. 2611–2624. Masson, R. and A. Zaoui (1999). Self-Consistent Estimates for the RateDependent Elastoplastic Behaviour of Polycrystalline Materials, J. Mech. Phys. Solids, Vol. 47, pp. 1543–1568. Molinari, A., G. R. Canova, and S. Ahzi (1987). A Self-Consistent Approach of the Large Deformation Polycrystal Viscoplasticity, Acta Metall., Vol. 35, pp. 2983–2994. Kneer, G. (1965). Uber die Berechnung der Elastizitatsmoduln vielkristalliner Aggregate mit Textur, Phys. Stat. Sol., Vol. 9, pp. 825–838. Polanyi, von M. (1922). Rontgenographische Bestimmung von Ksistallanordnunge, Naturwissenschaften, Vol. 10, p. 411. Qui, Y. P. and G. J. Weng (1992). A Theory of Plasticity for Porous Materials and Particle-Reinforced Composites, J. Appl. Mech., Vol. 59, pp. 261–268. Schmid, E. and W. Boas (1935). Kristallplastizita¨t, Springer, Berlin, p. 64. Sachs, G. (1928). Zur ableilung einer ﬂeissbedingung (stresses causing ﬂow), VDI Z., Vol. 72, pp. 734–736. Suquet, P. (1993). Overall Potentials and Extremal Surfaces of Power Law or Ideally Plastic Materials, J. Mech. Phys. Solids, Vol. 41, pp. 981–1002. Suquet, P. (1995). Overall Properties of Nonlinear Composites: A Modiﬁed Secant Moduli Theory and Its Link with Ponte Castan˜eda’s Nonlinear Variational Procedure, C.R. Acad. Sci. Paris, Vol. 320 (Se´rie IIb), pp. 563– 571. Talbot, D. and J. Willis (1985). Variational Principles for Inhomogeneous Nonlinear Media,’’ IMA J. Appl. Math., Vol. 35, pp. 39–54. Tandon, G. P. and G. J. Weng (1988). A Theory of Particle-Reinforced Plasticity, J. Appl. Mech., Vol. 55, pp. 126–135. Taylor, G. I. (1934). Plastic Deformation of Crystals, Proc. Roy. Soc., Vol. A145, pp. 362–404. Taylor, G. I. (1938). Plastic Strain in Metals, J. Inst. Metals, Vol. 62, p. 307. Taylor, G. I. and C. F. Elam (1923). The Distortion of an Aluminum Crystal During a Tensile Test, Proc. Roy. Soc., Vol. A102, p. 647. Taylor, G. I. and C. F. Elam (1925). The Plastic Extension and Fracture of Aluminum Crystals, Proc. Roy. Soc., Vol. A108, pp. 28–51. Willis, J. R. (1983). The Overall Response of Composite Materials, J. Appl. Mech., Vol. 50, pp. 1202–1209.

12 NONLINEAR PROPERTIES OF COMPOSITES MATERIALS: THERMODYNAMIC APPROACHES Thermodynamic approaches in micromechanics consist of solving the ﬁeld equations by minimizing a free energy, where the minimum found corresponds to the desired macroscopic potential W(), which represents the mechanical energy stored in the domain V of the representative volume element (RVE) subjected to a macroscopic strain . As mentioned in the linear case through the introduction of variational principles, which leads to different bounds, an exact solution to these ﬁeld equations is rather difﬁcult to obtain and becomes impossible to derive in the nonlinear case. This is mainly due to highly ﬂuctuating ﬁelds resulting from the nonlinear behavior of the constituents. It has been shown that approximated solutions for the local problem can be obtained in the linear case, leading to pertinent estimations of the macroscopic behavior, which are capable of accounting for the inﬂuence of morphological parameters and phase spatial distribution on the global behavior. Unfortunately, due to the nonapplicability of the superposition principle, on which most developments are based in linear cases (e.g., use of elementary solutions such as Eshelby’s one), the philosophy behind these approaches cannot be transported directly to nonlinear behaviors. To take advantage of the knowledge acquired in linear cases, linearization of the local constitutive laws could be one of the interesting approaches. The procedure consists of replacing the nonlinear ﬁeld equations in the RVE by linear equations in the same RVE, whose solution can be evaluated exactly or approximately via the use of the tools developed for linear materials. The linearization is completed with Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

319

320

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

a set of complimentary equations, which characterizes the parameters deﬁning the linear problem (e.g., elasticity moduli). Typically, these equations are nonlinear so that the character of the initial problem is conserved. However, in this case, we will not deal with ﬁeld equations but with equations involving a ﬁnite set of variables which can be solved with the appropriate numerical tools. In most cases, simple algorithms lead to a solution. The methodology presented in the above is referred to as the ‘‘nonlinear extension’’ of a linear model. The local linear problem resulting from the linearization procedure is identical to the homogenization problem for linear composites, referred to as linear comparison composite (LCC). This virtual LCC results solely from the linearization step and has no physical existence. Further, its moduli are distinct from the initial elasticity moduli of the real nonlinear composite. Although it is often the case, the LCC does not necessarily have the same spatial distribution of phases, or the same number of constituents, as the real nonlinear composite. One of the difﬁculties of this method lies in the use of the linear model to obtain the nonlinear macroscopic behavior. Typically, linear models do not provide detailed description of the local ﬁelds in the LCC but only averaged strains or stresses in the phases. This information is sufﬁcient in the case of linear problems since the macroscopic stress can be obtained from averaged strains in the phases via the following equation: ⫽

冘 c ⫽ 冘 c L. r

r

r

r

r r

r

Due to the nonlinear behavior of the constituents, this property does not hold for nonlinear composites where the macroscopic stress is given by ⫽

冘 c ⫽ 冘 c 冓⭸⭸()冔 ⫽ 冘 c ⭸⭸( ) r

r

r

r

r

r

Vr

r

r

r

where () is the local free energy, cr the volume fraction of each phase, and Lr their stiffness. The above general principles will be addressed in this chapter, in the particular case where the LCC is obtained from the secant moduli of the nonlinear constituents. Two approaches, the ‘‘classical’’ approach and the ‘‘modiﬁed’’ approach, will be presented and compared. These

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

321

two approaches are both relatively simple to use and differ only from the set of complimentary equations characterizing the LCC. In the ﬁrst part, the nature of the constitutive laws will be presented and illustrated with examples. Both tangent and secant linearization methods for the constitutive laws will be deﬁned. The variational formulation that deﬁnes the homogenized behavior of heterogeneous materials will be presented in the second part. The general method of ‘‘nonlinear extension’’ of linear models is presented at the end and applied to the case of the classical secant linearization, which shows inconsistencies related to the lack of information regarding the intraphase ﬂuctuations of local ﬁelds. An attempt to estimate these heterogeneities is made through the modiﬁed-secant formulation based on the second-order deformation moments within the phases, correcting the deﬁciencies of the classical extension. The two approaches will be illustrated and compared through the different problems given at the end of this chapter. Recent methodologies to describe the overall behavior of nonlinear composites adopt variational procedures. These approaches are not addressed here. The reader may refer to the Suggested Readings at the end of the chapter.

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

Thermodynamic Potentials

The behavior of the constituents treated in this chapter can be described by two thermodynamic potentials: the free energy and the dissipation potential , which are both expressed as a function of strain and of the appropriate internal variables ␣ (scalar or tensorial): Constitutive laws:

rev ⫽

⭸(, ␣) , ⭸

Complimentary laws: irr ⫽ with

⭸(˙, ␣ ˙) , ⭸˙

⫽ rev ⫹ irr.

⭸(, ␣) , ⭸␣

a⫽⫺

⭸(˙, ␣ ˙) , ⭸␣ ˙

a⫽⫺

(12.1.1)

(12.1.2) (12.1.3)

The convexity of and its nullity at ˙ ⫽ 0 impose a positive dissipation and, consequently, the second law is satisﬁed. The convexity of is associated with the stability of the material. Although many

322

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

approximate formulations have been proposed, there is no homogenization theory giving rigorous solutions to the homogenized behavior of phase mixtures described by (12.1.1)–(12.1.3). However, theories based on rigorous bounds have recently been developed in the simple case where the behavior of the phases can be described with only one potential, the free energy or the dissipation potential, the remaining potential being equal to zero. Behaviors Described by a Single Potential

We assume the behavior of each phase is described with a single convex potential, () or (˙), the remaining potential is equal to zero, such that the stress–strain or stress–strain rate relation can be written as follows: ⫽ rev ⫽

⭸() , ⭸

⫽ 0.

(12.1.4)

⫽ irr ⫽

⭸(˙) , ⭸˙

⫽ 0.

(12.1.5)

Or

Equation (12.1.4) describes a nonlinear elastic behavior under smallstrain deformation, while (12.1.5) corresponds to a purely viscous behavior where deformation can be ﬁnite (the problem is purely Eulerian). For the sake of simplicity of the notations, only the ﬁrst expression will be used (nonlinear elasticity). The results will be directly transferable to the second case by considering as a strain rate. Equation (12.1.4) can be inverted to obtain ⫽

⭸ ˜ () , ⭸

(12.1.6)

where ˜ () is the complimentary energy of the material. Mathematically, the relation between ˜ () and () is obtained via the Legendre transformation: ˜ () ⫽ sup{ : ⫺ ()}.

Let us now consider a few examples.

(12.1.7)

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

323

Isotropic Materials

Most isotropic materials are linear under hydrostatic load and nonlinear under shear; their behavior can be written with the following expressions: m ⫽ 3km,

s ⫽ 2 sec(eq)e,

sec(eq) ⫽

eq , 3eq

(12.1.8)

where m ⫽

kk , 3

m ⫽

kk

3

eq ⫽ (–32 s:s)1 / 2,

,

sij ⫽ ij ⫺ m␦ij, (12.1.9)

eij ⫽ ij ⫺ m␦ij.

eq ⫽ (–23 :)1 / 2,

(12.1.10)

Therefore, the bulk modulus K is constant while the shear modulus sec depends on strain (hence the nonlinearity of the deformation). This behavior is derived from the following free energy: () ⫽ –92 k 2m ⫹ eq(eq),

eq(eq) ⫽

冕

eq

0

eq deq,

(12.1.11)

where eq is the area under the curve in the eq(eq) diagram. The associated complimentary energy ˜ () is written as follows: ˜ () ⫽

1 2 ⫹ ˜ eq(eq). 2K m

(12.1.12)

Here ˜ eq is the dual potential of eq. Hencky’s Model in Plasticity

The elastoplastic behavior is rigorously described with incremental relations that enable us to distinguish plastic and elastic loads. In the case of isotropic hardening (where the hardening variable is ) with the Von Mises criterion, these relations are written as follows:

324

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

e ⫽

⫽ e ⫹ p,

冉 冊

3 s:˙s d y ˙ ⫽ 2 eq d

m 1 I⫹ s, 3K 2

˙ p ⫽

3 ˙ s , 2 eq

⫺1

if eq ⫽ y(),

˙ ⫽ 0

if eq ⬍ y(). (12.1.13)

Hencky’s model, also referred to as the deformation theory of plasticity, neglects the incremental nature of plasticity and replaces the equation describing the evolution of the plastic deformation (12.1.13) by ⫽ e ⫹ p,

e ⫽

m 1 I⫹ s, 3K 2

p ⫽

3 s , 2 eq

⫽ ( y)⫺1(eq).

(12.1.14)

For example, the model proposed by Ramberg and Osgood describes a power law hardening y() ⫽ 0( / 0)1 / n. This model can be written in the three-dimensional case: ⫽ e ⫹ p,

e ⫽

m 1 I⫹ s, 3K 2

p ⫽

冉 冊

30 eq s , 2 0 eq (12.1.15)

which is derived from the following potential:

冉 冊

eq 1 2 1 ˜ () ⫽ m ⫹ (eq)2 ⫹ 0 0 2K 6 n ⫹ 1 0

n⫹1

,

(12.1.16)

where , n ⱖ 1, 0, and 0 are the elastic shear modulus, the hardening exponent, and reference material constants, respectively. In the case of monotonic loading, Hencky’s model is a useful approximation. Unfortunately, it is inapplicable in the case of complex loadings. It can be shown that the incremental method and the deformation theory give the same response under monotonic and radial (the principle stress directions are time independent) loading. The adoption of the deformation theory in the case of heterogeneous materials supposes the stress state to be monotonic and radial at any point of the RVE. This hypothesis is more than likely not satisﬁed. However, in simple cases (e.g., elastoplastic matrix reinforced with simply shaped elastic inclusions), it can be observed that under a monotonic and radial

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

325

macroscopic load, deviations from this hypothesis are small. Therefore, the approximation of the incremental theory by a deformation theory is fairly good. For a more detailed discussion on the relationship between the incremental plasticity and the deformation theory, one can refer to Hutchinson (1976). Creep Behavior

The high-temperature creep of metals can often be treated by neglecting elastic deformation. It is typically expressed by a power law relation between strain rate and Cauchy’s stress: ⫽ mI ⫹ s,

eq ˙ eq ⫽ , 0 ˙ 0

s 2 e˙ ⫽ , eq 3 ˙ eq

˙ m ⫽ 0.

(12.1.17)

The potentials and ˜ describing the dissipation are written as follows:

冉冊

˙ eq ˙ (˙) ⫽ 0 0 m ⫹ 1 ˙ 0

冉 冊

eq ˙ ˜ () ⫽ 0 0 n ⫹ 1 0

m⫹1

,

n⫹1

.

(12.1.18)

Here m ⫽ 1/n, and ˙ 0 and 0 are the strain rate sensitivity exponent and the reference strain rate and stress, respectively. Continuum Description of Single Crystals

The general framework of thermodynamic potentials can also be applied to crystalline materials. The total strain rate, ˙ , in a single crystal is given by a superposition of the elementary shear rates in each slip system

冘 ␥˙ R , N

˙ ⫽

g

g

(12.1.19)

g⫽1

where the shear rate ␥˙ g in the slip system g depends only on the critical shear stress g in this system, such that ␥˙ g ⫽

⭸˜ g g ( ), ⭸ g

(12.1.20)

where the potential ˜ g is convex and typically given by a power law as follows:

326

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

冉 冊

g␥˙ 兩 g兩 ˜ ( ) ⫽ g 0 0 n ⫹ 1 0g g

g

n g⫹1

.

(12.1.21)

In the above, ng ⱖ 1 is the creep exponent, g0 is the critical shear stress for the considered system, and ␥˙ 0 is a reference shear rate. The constitutive law described by Eqs. (12.1.19) and (12.1.20) are derived from a convex potential for the single crystal: ⭸˜ () ˙ ⫽ , ⭸

冘 ˜ ( ) ⫽ 冘 ˜ (R :). N

˜ () ⫽

N

g

g

g⫽1

g

g

(12.1.22)

g⫽1

Secant Moduli Description of the Behavior

In what follows, only one notation of the behavior will be used, based on the elastic potentials, and ˜ . The constitutive law (12.1.8) can be written in a more compact form as follows: ⫽ Lsec():,

(12.1.23)

where Lsec is the secant modulus tensor. In the case of isotropic materials, it is a function of the projection tensors I h and I d: Lsec() ⫽ 3KIh ⫹ 2 sec(eq)Id.

(12.1.24)

Note that Lsec is not uniquely deﬁned. For example, one can add an anisotropic component to the secant tensor without changing the constitutive law: sec d 2 L˜ sec ˜ ije˜ kl), ijkl ⫽ Lijkl ⫹ ␣(I ijkl ⫺ – 3e

e˜ ij ⫽

eij eq

(12.1.25)

such that Lsec(): ⫽ L˜ sec(): for all ␣. And L˜ sec is a secant tensor in the sense described by (12.1.23), but Lsec given by (12.1.24) is the only isotropic tensor verifying this relation. Incremental Formulation and Tangent Moduli

We now discuss homogenization methods based on tangent moduli. It results from an incremental form of the constitutive law given by (12.1.4), obtained with a differentiation with respect to time:

12.1

˙ ⫽ Ltg():˙,

327

NONLINEAR BEHAVIOR OF CONSTITUENTS

Ltg ijkl() ⫽

⭸ij() ⭸2() ⫽ , ⭸ij⭸kl ⭸kl

(12.1.26)

where Ltg() is the tangent modulus tensor, which is typically anisotropic, even when the material is isotropic. Accordingly, in the case of an isotropic material described by Eqs. (12.1.23) and (12.1.24), the tangent tensor is given by h sec d Ltg (eq)I ijkl ⫹ ijkl() ⫽ 3KIijkl ⫹ 2

4 d sec ( ) e˜ e˜ . 3 deq eq eq ij kl

(12.1.27)

For convenience, Ltg can be expressed as h sec Ltg (eq)E 1ijkl ⫹ 2 tg(eq)E 2ijkl, ijkl() ⫽ 3KI ijkl ⫹ 2

(12.1.28)

where E 2ijkl ⫽ –23 e˜ ije˜ kl,

E1 ⫽ I d ⫺ E 2,

tg ⫽ sec ⫹

d sec(eq) 1 deq(eq) eq ⫽ eq. deq 3 deq

(12.1.29)

The tensors E1 and E2 have the following properties: E 2:E 2 ⫽ E 2,

E1:E1 ⫽ E1,

E 2:I h ⫽ 0,

E 2:E1 ⫽ 0,

E1:I h ⫽ 0.

(12.1.30)

The shear modulus tg gives the slope of the curve eq(eq). In the case of isotropic incompressible materials described by a power law, the secant tensor Lsec (12.1.24) and the tangent tensor Ltg (12.1.28) are given by L () ⫽ ⫹⬁I ⫹ 2 (eq)I , sec

h

sec

d

冉冊

1 0 eq (eq) ⫽ 3 0 0 sec

m⫺1

,

(12.1.31) and Ltg() ⫽ ⫹⬁I h ⫹ 2 sec(eq)(E1 ⫹ mE 2),

tg(eq) ⫽ m sec(eq).

(12.1.32)

328

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

To illustrate the nonuniqueness of the secant moduli, it can be easily veriﬁed that the anisotropic tensor (1/m)Ltg is also the secant tensor for isotropic materials described by a power law see Problem 12.1. The tangent modulus tensor is uniquely deﬁned with equation (12.1.26). However, in some cases, it is approximated, to simplify the algebra, by an isotropic tensor, Ltg() ⫽ ⫹⬁I h ⫹ 2 tg(eq)I d.

iso

(12.1.33)

Another isotropic tangent tensor is expressed by Ltg() ⫽ ⫹⬁I h ⫹

iso

1 tg d d 4 ⫹ m sec (L ⬋I )I ⫽ ⫹⬁I h ⫹ 2 (eq)I d. 5 5 (12.1.34)

It should be noted that the above approximation may lead to severe discrepancies in the homogenization schemes adopting a tangent linearization of local constitutive laws.

12.2

EFFECTIVE POTENTIALS

Let us now consider a RVE with volume V and boundary S representing a nonlinear heterogeneous material. The boundary conditions on S are given in terms of combined loading: traction boundary condition p0 on S and displacement boundary condition u0 on Su with S ⫽ S ⫹ Su. We are to ﬁnd the ﬁelds u, , and so that u and fulﬁll the conditions of kinematics:

冦

⫽ –12 (ⵜu ⫹ (ⵜu)T)

u u ⫽ u0

within V is continuous in V. on Su

(12.2.1)

Under the conditions (12.2.1), u and are called kinematically admissible:

再

div ⫹ f ⫽ 0 n ⫽ p0

inside V . on Su

(12.2.2)

Under the conditions (12.2.2), is called statically admissible.

12.2

EFFECTIVE POTENTIALS

329

By introducing the thermodynamics potentials, and are related at each material point r of V by the constitutive laws: (r) ⫽

⭸((r), r) , ⭸

(r) ⫽

⭸ ˜ ( (r), r) . ⭸

(12.2.3)

The solution to the nonlinear problem requires solving one of the following problems: Under displacement boundary conditions related to an applied macroscopic strain , the problem consists of solving the following problem for statistically admissible stress: ∀r僆V

(r) ⫽

⭸((r), r) , ⭸

(12.2.4)

具(r)典V ⫽ .

Under traction boundary conditions related to an applied macroscopic stress , the problem consists of solving the following problem for kinematically admissible strain: ∀r僆V

(r) ⫽

⭸((r), r) , ⭸

(12.2.5)

具 (r)典V ⫽ .

Solutions to (12.1.1) or (12.1.2) lead to the deﬁnition of local stress and strain ﬁelds fulﬁlling the following variational properties, which result from the convexity of the local potentials and ˜ . This can be stated as: The solution of strain ﬁeld for the ﬁrst problem minimizes the free energy , so that 具()典 ⫽ inf具(˜)典,

(12.2.6)

where ˜ is a kinematically admissible strain with 具˜ 典 ⫽ . The solution of stress ﬁeld for the second problem minimizes the complementary free energy ˜ , so that 具 ˜ ()典 ⫽ inf具˜ ( ˜ )典,

˜ is a trial statically admissible stress with 具典 ˜ ⫽ . where

(12.2.7)

330

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

Deﬁnition (12.2.6) corresponds to the macroscopic or effective free energy of the representative volume element, denoted by W (), so that the macroscopic constitutive relation writes ⫽

⭸W() , ⭸

(12.2.8)

with W() ⫽ inf具(˜)典.

(12.2.9)

Equation (12.2.8) can be shown from (12.2.4) and (12.2.6) by using the Hill lemma. Similarly, one can deﬁne a macroscopic complementary energy as ⫽

˜ ) ⭸W( ⭸

˜ ) ⫽ inf具 with W( ˜ ( ˜ )典.

(12.2.10)

˜ are dual convex functions, such that Note that the potentials W and W with the help of the Hill lemma, one has ˜ ) ⫽ 具()典 ⫹ 具 W() ⫹ W( ˜ ()典 ⫽ 具 :典 ⫽ :.

(12.2.11)

The principles of minimum energy (12.2.6) and (12.2.7) may be used ˜ For example, by to set bounds for the effective potentials W and W. choosing the solution of problem (12.1.1) or (12.1.2) corresponding to a uniform stress ⫽ and uniform strain ﬁeld ⫽ , respectively, one obtains the equivalent Voigt and Reuss bounds for the effective potentials. By setting ⫽ in (12.2.9), one has

冘 c ().

(12.2.12)

冘 c ˜ ().

(12.2.13)

n

W() ⱕ 具()典 ⫽

r

r

r⫽1

Similarly n

˜ ) ⱕ 具 W( ˜ ()典 ⫽

r

r

r⫽1

As an application for incompressible power law materials deﬁned by (12.1.18), the Voigt and Reuss bounds read (see Problem 12.2)

12.3

冉冊

0Reuss0 eq m ⫹ 1 0

m⫹1

ⱕ W() ⱕ

THE SECANT APPROACH

冉冊

0Voigt0 eq m ⫹ 1 0

331

m⫹1

,

(12.2.14)

where ⫺m Reuss ⫽ 具⫺n , 0 0 典

12.3

0Voigt ⫽ 具0典.

(12.2.15)

THE SECANT APPROACH

For general purposes, the secant method solves the following ﬁeld equations: ⫽ –12 (ⵜu ⫹ (ⵜu)T),

div ⫽ 0, 具典 ⫽ , (r) ⫽ Lsec(r, (r)):(r),

(12.3.1)

where Lsec is the local secant modulus tensor, which depends on the phase considered. It typically ﬂuctuates within a phase due to the ﬂuctuation of the local strain (r). Therefore, the secant modulus tensor is highly heterogeneous. Its ﬂuctuation results from the nonlinearity of the problem associated with its dependency on the local strain. Indeed, the heterogeneity of secant modulus tensor depends on which type of nonlinear behavior is displayed by the constituents and also on the amount of applied strain. To set up a direct homogenization procedure of such highly heterogeneous materials is very difﬁcult unless systematic approximations are used, which, in general, relies on a linearization procedure with appropriate complementary laws. As a ﬁrst attempt and within a general procedure, the problem could be seen at a given strain state as a linear problem with the following local constitutive law: (r) ⫽ Llin(r):(r),

(12.3.2)

Llin(r) ⫽ Lsec(r, (r)).

(12.3.3)

with

332

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

Deﬁnition (12.3.2) is the linear model required for the linearization procedure of the local behavior, whereas deﬁnition (12.3.3) corresponds to additional or complementary relationships, so that the nonlinear behavior can be captured. When these two steps are accomplished, the problem becomes a classical one. Then an appropriate ‘‘classical’’ linear homogenization scheme can be chosen to obtain the nonlinear macroscopic behavior. However, (12.3.2) and (12.3.3) are still not suitable for analytical calculations due to the inﬁnite number of complementary equations required for deﬁnition (12.3.3). Therefore, approximations are needed, which, clearly, need to render a ﬁnite number of complementary equations with a certain accuracy in describing the heterogeneous nature of the nonlinear behavior. For such a purpose, approximations are introduced both in the step of linearization and complementary equations. The linear model in Eq. (12.3.2) may be assumed piecewise uniform for the stiffness tensor Llin(r), so that, for a given phase r(r ⫽ 1, . . . , n) one has Llin(r) ⫽ Lr. In addition, the complementary equations are reduced to a ﬁnite number corresponding to the identiﬁed number of constituents or phases, which lead to a deﬁnition of stiffness tensors Lr at some effective piecewise uniform strains ˜ r, representing the strain distribution in each phase, and therefore requiring an accurate model to be determined. The n complementary equations read Lr ⫽ Lrsec(˜r),

(12.3.4)

where the nonlinearity of the problem lies in the dependency of each individual effective strain ˜ r on the stiffness Lr of the different phases, so that n nonlinear problems have to be solved, requiring in general simple iterative procedures. Once the tensors Lr are determined, the problem becomes a classical one by taking advantage of the homogenization approaches developed in linear elasticity. The choice of the appropriate linear homogenization scheme to describe the microstructure of the real nonlinear composite material deﬁnes the so-called linear comparison composite, for which the overall effective stiffness L is expressed formally as L ⫽ L(cr, Lr, . . .) ⬅ L(),

(12.3.5)

which depends on the stiffness of each constituent and some morphological aspects related to the microstructure. The overall constitutive law is then nonlinear and formally given by

12.3

THE SECANT APPROACH

⫽ L():.

333

(12.3.6)

In the following, two methods to deﬁne the effective strains ˜ r are discussed and compared. The ﬁrst approach is known as the classical secant method. It simply deﬁnes the effective strains as the average strain in each phase. The second method, called the ‘‘modiﬁed’’ secant method, could be seen as a reﬁnement of the ﬁrst method by introducing the second-order moment of the strain ﬁeld. Classical Method

The classical method has been extensively used to deal with the nonlinear behavior of composite materials. It consists of deﬁning the effective strain ˜ r as the mean value of the local strain ﬁeld over the considered phase. That is ˜ r ⫽ 具(r)典Vr.

(12.3.7)

The main advantage behind assumption (12.3.7) lies in the expression of effective strains ˜ r as a function of the applied strain by means of the global strain concentration Ar: ˜ r ⫽ Ar:, r(r ⫽ 1, . . . , n),

(12.3.8)

which are determined by appropriate explicit or implicit linear mean ﬁeld theories (see Chapter 7), which give the n concentration tensors in terms of the stiffness tensors Lr of each phase for explicit schemes and the overall stiffness L for implicit schemes. That is Ar ⫽ Ar(L, Lr, s ⫽ 1, . . . , n).

(12.3.9)

Finally, since Lr depends on the corresponding effective strain ˜ r through Eq. (12.3.4), Eq. (12.3.8) together with expression (12.3.9) provide n nonlinear equations, whose solutions determine the overall nonlinear property L by means of the constitutive equation (12.3.6). As noticed before, such a scheme requires in general iterative procedure and suitable convergence criteria. Note that through the deﬁnition of a linear comparison composite, upper and lower bounds of the effective properties L can be found using the linear variational principles presented in Chapter 6.

334

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

The classical secant method can be illustrated in case of two-phase materials. In fact, combination of 具(r)典V ⫽ , ˜ 1 ⫽ A1:,

(12.3.10) ˜ 2 ⫽ A2:

leads to c1A1 ⫹ c2 A2 ⫽ I.

(12.3.11)

In addition, from the constitutive law of each constituent, we have 1 ⫽ L1:˜1,

2 ⫽ L2:˜2,

(12.3.12)

and ⫽ c11 ⫹ c22.

(12.3.13)

L ⫽ c1L1:A1 ⫹ c2L2:A2.

(12.3.14)

Equation (12.3.10) gives

Then substituting (12.3.11) in (12.3.14) yields A1 ⫽ A2 ⫽

1 (L ⫺ L2)⫺1(L ⫺ L2), c1 1

(12.3.15)

1 (L ⫺ L1)⫺1(L ⫺ L1). c2 2

Therefore, when the linear homogenization model is identiﬁed to obtain the effective stiffness as L ⫽ L(c1, L1, L2),

(12.3.16)

the solution to the nonlinear problem is given by the following set of equations:

12.3

THE SECANT APPROACH

˜ 1 ⫽

1 (L ⫺ L2)⫺1(L ⫺ L2):, c1 1

˜ 2 ⫽

1 (L ⫺ L1)⫺1(L ⫺ L1):, c2 2

L1 ⫽ L1sec(˜1),

335

(12.3.17)

L2 ⫽ L2sec(˜2)

When the two phases are isotropic, (1) d (2) d L1(˜1) ⫽ 3K1Ih ⫹ 21sec(˜eq )I and L2(2) ⫽ 3K2Ih ⫹ 22sec(˜eq )I ,

(12.3.18) and the linear comparison composite displays an overall isotropy such that L() ⫽ 3KIh ⫹ 2(eq)Id,

(12.3.19)

where the linear homogenization scheme gives K ⫽ K(K1, K2, 1, 2, c1),

⫽ (K1, K2, 1, 2, c1).

(12.3.20)

The set of nonlinear equations (12.3.17) is reduced to (1) ˜ (1) m ⫽ Am m,

(2) (2) ˜ m ⫽ Am m,

(1) (1) ˜ eq ⫽ Aeq eq,

(2) (2) ˜ eq ⫽ Aeq eq,

Am(1) ⫽

1 K ⫺ K2 , c1 K1 ⫺ K2

(1) Aeq ⫽

1 ⫺ 2 , c1 1 ⫺ 2

Am(2) ⫽

1 K ⫺ K1 , c2 K2 ⫺ K1

(2) Aeq ⫽

1 ⫺ 1 , c2 2 ⫺ 1

1 ⫽ sec (1) 1 (˜ eq ),

(12.3.21)

2 ⫽ sec (2) 2 (˜ eq ).

Further, if the materials are incompressible, the linear homogenization model gives ⫽ (1, 2, c1),

and the nonlinear set of equations become

(12.3.22)

336

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

(1) ˜ (1) eq ⫽ Aeq eq,

A(1) eq ⫽

1 ⫺ 2 , c1 1 ⫺ 2

(1) 1 ⫽ 1sec(˜eq ),

(2) (2) ˜ eq ⫽ Aeq eq, (2) Aeq ⫽

1 ⫺ 1 , c2 2 ⫺ 1

(12.3.23)

2 ⫽ sec (2) 2 (˜ eq ).

As discussed above, when the appropriate linear homogenization scheme is chosen, the classical method becomes relatively easy to implement through an iterative algorithm. A few examples are treated as problems at the end of this chapter. Modiﬁed Secant Method

The classical secant method for describing the nonlinear behavior of composite materials assumes basically homogeneous strain ﬁeld within each phase and therefore neglects any intraphase ﬂuctuations of local ﬁelds. This results in few discrepancies and limitations, which was behind the principal motivations in developing the modiﬁed secant approach. Let us ﬁrst recall the basis of the classical secant method, which leads to a certain number of inconsistencies. As shown above, the classical method derives the average stress r over a phase r (r ⫽ 1, . . . , n) as r ⫽ Lr:r ⫽ Lrsec(r):r,

(12.3.24)

which implies the existence of a phase strain energy potential (r)( (r)) determined with respect to the average strain r, such that r ⫽

⭸r(r) . ⭸r

(12.3.25)

In the case of incompressible materials, (12.1.24) reads

(r) eq

where

(r) ⭸(r) eq ( eq ) ⫽ , (r) ⭸ eq

(12.3.26)

(r) eq ⫽

冋

冕

1 Vr

Vr

册

(r) dV

(r) eq ⫽

,

eq

12.3

THE SECANT APPROACH

冋

冕 (r) dV册 .

1 Vr

V

337

(12.3.27)

eq

One can also deﬁne the following equivalent average strain as (r) eq ⫽

1 Vr

冕

Vr

eq(r) dV.

(12.3.28)

The ﬁrst discrepancy of the classical method results from the equalities (12.3.25) and (12.3.26), which are satisﬁed only if the strain ﬁeld is homogeneous in each phase. Or, in general, the nonlinear behavior leads to highly intraphase ﬂuctuations, and as a result one can show that r ⫽

1 Vr

冕

Vr

(r) dV ⫽

1 Vr

冕

Vr

⭸r() ⭸ ( ) dV ⫽ r r , ⭸ ⭸r

(12.3.29)

or in the case of incompressible materials (r) eq ⫽

(r) ⭸(r) eq ( eq ) . ⭸ (r) eq

(12.3.30)

The result (12.3.30) is shown in the following. In fact, one has

冕 (r) dV册 ⫽ 冋V1 冕 ⭸ ( ) ⭸ () 1 ⫽ 冕 dV册 V ⭸ ⭸

(r) eq ⫽

冋

1 Vr

Vr

eq

(r) eq

r

Vr

eq

r

Vr

册

⭸r() dV ⭸

eq

eq

(12.3.31)

eq

eq

which leads to (r) eq ⫽

冋

1 Vr

冕

Vr

册

⭸(r) eq (eq) 2e() dV ⭸eq 3eq

.

(12.3.32)

eq

On the other hand, the convexity of the function e:e leads to the following inequality:

338

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

(r) eq ⫽

冋

1 Vr

冕

Vr

册

⭸(r) eq (eq) 2e() dV ⭸eq 3eq

ⱕ

eq

1 Vr

冕

Vr

⭸(r) eq (eq) dV. ⭸eq

(12.3.33)

Since for most nonlinear composite the function [⭸ (r) eq (eq) / ⭸eq] is concave, one can easily show that 1 Vr

冕

Vr

(r) (r) ⭸(r) ⭸eq ( (r) ⭸eq ( (r) eq (eq) eq ) eq ) dV ⬍ ⫽ , ⭸eq ⭸eq ⭸eq

(12.3.34)

(r) where we further assume that (r) eq ⫽ eq . With (12.3.34), statement (12.3.30) is proved. Another limitation of the classical method results from the fact that the deﬁnition of the macroscopic properties does not necessarily rely on the deﬁnition of a macroscopic W (), so that

⫽

⭸W() . ⭸

(12.3.35)

In fact, it turned out that in some cases of nonlinear composite materials, the following property of the macroscopic potential of isotropic materials ⭸2W(eq, m) ⭸2W(eq, m) ⭸eq ⭸ ⫽ m⫽ ⫽ , ⭸eq ⭸m ⭸eq ⭸m ⭸eq ⭸m

(12.3.36)

is not fulﬁlled by the classical secant approach, see Problem 12.4. The modiﬁed secant method took its inspiration from the above statement. It was developed in accordance to the following. The ﬁrst step is the deﬁnition of the macroscopic potential from the Hill lemma: W() ⫽

1 V

冕 :L(r): dV ⫽ :L:,

(12.3.37)

V

and its derivative with respect to the stiffness Lr of the r phase in the linear comparison composite: ⭸W() ⭸L 1 ⫽ : (r) : ⫽ ⭸L(r) ⭸ L V ijkl ijkl

2 ⭸ 冕 :⭸⭸L(r) : dV ⫹ 冕 :L(r): L V ⭸L V

(r) ijkl

V

(r) ijkl

dV,

(12.3.38) where the local stiffness Lr(r) is assumed to be piecewise uniform:

12.3

THE SECANT APPROACH

冘 L ƒ (r),

339

n

Lr(r) ⫽

(12.3.39)

r r

r⫽1

where ƒr is the characteristic function deﬁned in (5.3.8). With (12.3.39), the ﬁrst term on the right-hand side of (12.3.38) yields 1 V

1 冕 :⭸⭸L(r) : dV ⫽ c 冕 L V V

r

(r) ijkl

r

Vr

ijkl dV ⫽ cr具ijkl典Vr,

(12.3.40)

while the second term writes 1 V

冕 :L(r):⭸⭸L V

(r) ijkl

dV ⫽

再

1 V

冕 (r) dV冎再: V1 冕 ⭸⭸L V

V

(r) ijkl

冎

dV ⫽ 0. (12.3.41)

To establish (12.3.41) we used the Hill lemma in accordance to the fact that the strain ﬁeld ⭸ / ⭸L(r) ijkl is kinematically admissible, so that

冕 ⭸⭸L V

(r) ijkl

dV ⫽ 0.

According to (12.3.40) and (12.3.41), (12.3.38) is reduced to 具ijkl典Vr ⫽

1 ⭸L : (r) :. cr ⭸Lijkl

(12.3.42)

The fourth-order tensor 具ijkl典Vr corresponds to the second-order moment of the strain ﬁeld over the r phase in the linear comparison composite material. It is calculated by (12.3.42) and therefore requires the deﬁnition of the linear homogenization scheme to express the macroscopic properties in terms of the local ones. The diagonal term 具:典Vr of the second-order moment can be adopted in the modiﬁed second method as an alternative way to measure the intraphase ﬂuctuation of the strain ﬁeld better than the classical method. This comes from the convexity of the function :: 具:典Vr ⱖ 具典Vr:具典Vr,

(12.3.43)

where the equal sign holds only if the strain ﬁeld is homogeneous.

340

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

In the case of isotropic materials, the second-order moment uses the equivalent strain such that ⭸L(r) 1 ⭸L 1 ⭸L ijkl d 2 : : ⫽ : (r) : ⫽ 2具ijkl典Vr I ijkl ⫽ 3( (r) eq ) , cr ⭸r cr ⭸Lijkl ⭸r

(12.3.44)

where (r) eq is given by (12.3.28). Finally, by adopting the second-order moment of strain, the modiﬁed secant method involves the following steps: • The identiﬁcation of the appropriate linear homogenization

scheme, which give the overall stiffness L as function of the phase stiffness L(r) ijkl in the linear comparison composite. Then the derivatives in (12.3.44) can be accomplished. • The resolution of the following n nonlinear set of equations (r) (r) L(r) ijkl ⫽ Lijkl( eq ),

(r) eq ⫽

冉

冊

1 ⭸L : : 3cr ⭸r

1/2

,

(12.3.45)

(r) which gives the n unknown secant tensors L(r) ijkl( eq ). As in the case of the classical method, the modiﬁed method requires simple iterative algorithm to derive the overall properties of the nonlinear composite. If the linear comparison composite has overall isotropy, one can easily show from (12.3.45) that

(r) eq

冋冉

1 1 ⭸K 2 ⭸ 2 ⫽ m ⫹ cr 3 ⭸r ⭸r eq

冊册

1/2

,

(12.3.46)

where K and are computed by a linear homogenization approach. Let us illustrate the method in the case of a two-phase isotropic composite material, where phase (1) is softer and dispersed in phase (2). Suppose that Hashin–Shtrikman lower bounds are appropriate to derive the overall properties of the linear composite. One has (see Example 6.2)

12.3

c1

K ⫽ K2 ⫹

1 K1 ⫺ K2

⫽ 2 ⫹

⫹

341

THE SECANT APPROACH

,

c2 K2 ⫹ –43 2

(12.3.47)

c1 , 1 6c2(K2 ⫹ 22)2 ⫹ 1 ⫺ 2 5(3K2 ⫹ 42)

from which one can derive explicit expressions for the second-order moment of strain required to compute the tensor of secant moduli in each phase. The results are (1) eq ⫽

1 ⫺ 2 , c1 1 ⫺ 2 eq

(2) 2 2 1/2 eq ⫽ (N m ⫹ M eq ) ,

(12.3.48)

with

冋

冉

冊

1 1 K ⫺ K2 N⫽ K ⫺ c1K1 3c22 c1 K1 ⫺ K2

2

冉

冊册

1 K ⫺ K1 ⫺ c2K2 c2 K2 ⫺ K1

2

,

(12.3.49) M⫽

冋

冉

冊

2

1 1 ⫺ 2 ⫺ c1 (1) c22 c1 1 ⫺ 2 2 12 1 ⫺ 2 1 ⫺ 2 ⫺ c1c2k2 5 c1 1 ⫺ 2 3K2 ⫹ 42

冉

冊冉

冊册 2

.

(12.3.50)

Concluding Remarks

In the classical and modiﬁed secant nonlinear extensions presented in the above, the phase distribution is the same in the LCC and in the nonlinear composite. As explained in previous sections, this results from the choice of a particular linearization scheme. This option is pertinent and does not lead to any ambiguity in the choice of the linear homogenization model used to describe the morphology of the LCC. However, another richer strategy can be used in which the homogeneous domain for the secant moduli tensors does not correspond to the domain occupied by the constitutive phases. For example, one could deﬁne LCCs with more phases than the nonlinear composite. One can

342

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

easily anticipate that this richer description of the local heterogeneity of the secant moduli will be closer to the real distribution of the moduli in the nonlinear composite. Hence, the prediction will be more suited. However, the evaluation of a large number of internal variables, the critical choice of a linear model, and the difﬁculty related to the larger number of considered phases complicate the use of this approach. There is a conﬁguration where this description can be naturally called upon, at least theoretically; when the phase distribution of the nonlinear composite can be appropriately described with morphological patterns. Let us consider the simple case of Hashin’s composite spheres assembly. In this case, the linear isotropic behavior of the microstructure can be well described with a three-phase self-consistent scheme based on the analytical solution of the problem of a composite inclusion embedded in an inﬁnite medium. PROBLEMS

12.1 Show that (1/m)Ltg is a secant modulus for power law materials deﬁned by constitutive equations (12.1.18), where Ltg is the tensor of tangent moduli given by (12.1.26). 12.2 Show equation (12.2.15). 12.3 Consider a two-phase composite material made of two power law isotropic materials. The two phases obey constitutive relations (12.1.8). They have the same components n and m, the same reference strain 0, but differ by their ﬂow stress denoted by (2) (1) 0 for phase (1) and 0 for phase (2). By combining the nonlinear problem (12.3.23) with a lower bound Hashin–Shtrikman type of estimation of the effective shear modulus , the average strain distribution in each phase does not depend on the volume fractions of the constituents, so that (1) eq ⫽ (2) eq

1 , 2 1 1⫹ ⫺1 5 2

冉

冊

with

冉 冊

(1) 1 0(1) eq ⫽ (2) (2) 2 0 eq

m⫺1

When phase (1) is rigid show from the average condition (2) c1 (1) eq ⫹ c2 eq ⫽ eq

the following results:

.

343

PROBLEMS

(1) lim eq ⫽ 0,

(2) lim eq ⫽

(1) 0→⫹⬁

0(1) →⫹⬁

eq

c2

,

(1) m 5 (2) (2) m lim (1) 0 ( eq ) ⫽ – 2 0 ( eq ) .

(1) 0→⫹⬁

From the deﬁnition of the overall stress deviator s s ⫽ c1s1 ⫹ c2s2 and the constitutive equations of each phase

冉 冊

2 (1) (1) eq s1 ⫽ lim 0 (1) 0 0→⫹⬁ 3

m

e1

冉 冊

(2) 2 (2) eq s2 ⫽ lim 0 0 0(1) →⫹⬁ 3

,

(1) eq

m

e2 (2) eq

show that the overall constitutive equation reads s⫽

冉冊

2 0 eq 3 0 0

m⫺1

e,

with 0 ⫽ 0(2)

(1 ⫹ –23 c1) . (c2)m

12.4 Consider the above problem when the inclusions [phase (1)] are voids. Show that the effective properties of the linear comparison composite are given by K⫽

4 c2 , 3 c1 2

⫽ 2

冉

冊

c2 1 ⫹ –32 c1

and the solution of the nonlinear problem is reduced to (2) eq ⫽

eq . 1 ⫹ –23 c1

Express the overall constitutive laws for the spherical and deviatoric parts and show that the following condition ⭸2W(eq, m) ⭸2W(eq, m) ⭸eq ⭸ ⫽ m⫽ ⫽ ⭸eq ⭸m ⭸eq ⭸m ⭸eq ⭸m

is not satisﬁed.

344

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

12.5 Consider Problem 12.4 when both phases are rigid plastic (m ⫽ 0) and show that the nonlinear problem is reduced to the following relations: (1) 5 eq ⫽ (2) eq 3

冉

(1) eq ⫽0 (2) eq

冊

1⫺

2 (1) 0 5 0(2)

if

(1) 5 0 ⱕ . (2) 0 2

if

0(1) 5 ⱕ , 0(2) 2

If we denote by 0 the ﬂow stress of the rigid plastic composite, show that (2) 0 ⫽ c1 (1) 0 ⫹ c2 0

3 0 ⫽ (2) 0 (1 ⫹ – 2 c1)

if if

(1) 5 0 ⱕ , (2) 0 2 0(1) 5 ⬎ . 0(2) 2

12.6 Consider Problem 12.3 and apply the modiﬁed secant method for what follows. Show Eqs. (12.3.48)–(12.3.50). Show that the linear problem deﬁned by Eq. (12.3.45) is reduced to

(1) eq (2) eq

⫽

⭸ c2 ⭸1 c1 ⭸ ⭸2

冢 冣

1/2

,

with

冉 冊

(1) eq 1 (1) ⫽ 0(2) (2) 2 0 eq

m⫺1

with a lower bound Hashin–Shtrikman estimation of , show that (1) eq ⫽ (2) eq

再冋 冉

2 1 1⫹ ⫺1 5 2

冊册

2

冉

6 ⫹ c1 1 ⫺ 1 25 2

冊冎 2

1/2

.

Show that the ﬂow stress of the composite with rigid inclusions is expressed by 0 ⫽ (2) 0

(1 ⫹ –32 c1)m⫹1 / 2 . (c2)m

SUGGESTED READINGS

345

12.7 Consider Problem 12.4 and show that the nonlinear problem using the modiﬁed method writes

(2) eq

冋

4 2 1 ⫽ m ⫹ ( )2 9c1 1 ⫹ –23 c1 eq

册

1/2

.

Rewrite the overall constitutive laws for the spherical and deviatoric parts and check the following equality: ⭸2W(eq, m) ⭸2W(eq, m) ⭸eq ⭸ ⫽ m⫽ ⫽ ⭸eq ⭸m ⭸eq ⭸m ⭸eq ⭸m

SUGGESTED READINGS Castan˜eda, P. (1991). The Effective Mechanical Properties of Nonlinear Isotropic Composites Materials, J. Mech. Phys. Solids, Vol. 39, pp. 45–71. Castan˜eda, P. (1992). New Variational Principles in Plasticity and Their Applications to Composite Materials, J. Mech. Phys. Solids, Vol. 40, pp. 1757–1788. Castan˜eda, P. (1996). Exact Second-Order Estimates for the Effective Mechanical Properties of Nonlinear Isotropic Composite Materials, J. Mech. Phys. Solids, Vol. 44, pp. 827–862. Castan˜eda, P. and P. Suquet. (1995). On the Effective Mechanical Behavior of Weakly Inhomogenous Nonlinear Materials, Eur. J. Mech. A/Solids, Vol. 14, pp. 205–236. Castan˜eda, P. and J. R. Willis. (1988). On the Overall Properties of Nonlinearly Viscous Composites, Proc. R. Soc. Lond. A, Vol. 416, pp. 217– 244. Castan˜eda, P. and M. Zaidman. (1994). Constitutive Models for Porous Materials with Evolving Microstructure, J. Mech. Phys. Solids, Vol. 42, pp. 1459–1497. Gilormini, P. (1995). A Shortcoming of the Classical Nonlinear Extension of the Self Consistent Model, C. R. Acad. Sci. Paris, Se´rie IIb, Vol. 320, pp. 115–122. Hutchinson, J. W. (1976). Bounds and Self-Consistent Estimates for Creep of Polycrystalline Materials, Proc. R. Soc. Lond., Vol. A 348, pp. 101–127. Michel, J. C. and P. Suquet. (1992). The Constitutive Law of Nonlinear Viscous and Porous Material, J. Mech. Phys. Solids, Vol. 40, pp. 783–812.

346

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

Suquet, P. (1993). Overall Potentials and Extremal Surfaces of Power Law or Ideally Plastic Composites, J. Mech. Phys. Solids Struct., Vol. 41, pp. 981– 1002. Suquet, P. and P. Castan˜eda. (1993). Small-Contrast Perturbation Expansions for the Effective Properties of Nonlinear Composites, C.R. Accad. Sci. Paris, Se´rie II, Vol. 317, pp. 1515–1522. Qiu, Y. P. and G. G. Weng. (1992). A Theory of Plasticity for Porous Materials and Particle-Reinforced Composites, J. Appl. Mech., Vol. 59, pp. 261–268.

13 MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS Martensitic transformation in solids has received considerable attention in recent years because of its broad potential applications. Such phase change can be induced by the application of stress as well as by temperature change. The original interest in martensitic phase transformation came from the special mechanical properties of the transformation product, namely the strength of martensite and the corresponding thermomechanical treatments to produce adequate behavior for engineering applications. Various strain mechanisms enter the behavior of such materials. Most of them are ductile materials, and, therefore, in addition to the plastic ﬂow, a microstructure evolution accompanying the phase change leads to complex strain mechanisms ensuring basically the coexistence of the two phases. These strain mechanisms result from an accommodation process, which enhances ductility at a particular strength level by means of ‘‘transformation induced plasticity,’’ known as the TRIP effect. The classical deﬁnition given to this phenomenon corresponds to the irreversible strain observed even if the specimen is loaded by a stress state less than the yield stress of the softer phase. In such materials, the overall behavior depends strongly on the temperature since the martensitic phase transformation kinetics is related with temperature through the so-called chemical energy. Furthermore, since martensitic phase transformation occurs without diffusion through a cooperative shear movement of atoms, it is recognized that the applied as well as the internal stresses assist the transformation. The role of plastic strain on the progress of martensitic transformation is much Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

347

348

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

Stress

more complicated. Martensitic phase transformation occurs on cooling without applied stress at Ms temperature. Above Ms, the critical stress to undergo martensitic phase transformation increases linearly with temperature up to the Ms temperature deﬁned as the maximum temperature at which martensitic transformation occurs by elastic stress. In this temperature range, martensitic transformation is deﬁned as the stress-assisted transformation. At temperatures above Ms , signiﬁcant plastic ﬂow precedes the transformation, and an additional contribution to transformation arises from the production of new nucleation sites by plastic deformation. In this temperature regime where the transformation critical stress decreases signiﬁcantly, the phase change is deﬁned as the plastic-strain-induced transformation. The temperature dependence of the critical stress for causing martensitic transformation is schematically represented in Figure 13.1 where the Md temperature is introduced to reﬂect the stability of austenitic phase. From a micromechanics point of view, materials with phase transformation can be considered as two-phase composite materials where the ‘‘reinforcement’’ phase evolves. In addition to the usual thermoelastic properties, which may be assumed homogenous for most of these materials, the inelastic behavior of austenite–martensite twophase material appears strongly heterogeneous. According to the diversity of active mechanisms and the evolving microstructure, various coupling have to be described. From a kinematical point of view, a volume element experiences a plastic strain in its austenitic state, followed by the instantaneous transformation strain according to discrete

Strain-Induced Transformation

Stress-Assisted Transformation Ms

M σs

Temperature

Yield Stress of Austenite

Md

Figure 13.1 Schematic representation of critical stress for martensitic transformation as function of temperature.

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

349

values of the possible set of transformation strains and plastic ﬂow in the martensitic state. This phenomenon is also known as dynamic softening. Beside the chemical part of the free energy, the elastic part is due to applied stresses, as well as due to internal stresses generated by the incompatibilities of the total inelastic strain ﬁeld (plastic ⫹ transformation). These couplings render possible a good combination between ductility and strength in materials with phase transformation. In fact any tendency to increase ductility in conventional materials will decrease the strength. For example, a good combination between strength and ductility is a required property to design lightweight structures in automotive bodies and also to improve body safety. To reproduce the various features of materials exhibiting martensitic phase transformation is not a simple task. Since the problem has to be considered from a multiscale point of view taking into account the microstructure evolution accompanying martensitic transformation, only partial solutions have been developed during the last decades. Basically, modeling the behavior of such materials raises, naturally, the following problems: 1. To deﬁne adequate variables describing the microstructure evolution during the phase transformation. For example, the volume fraction ƒ of martensite or a set of volume fractions ƒI (I ⫽ 1, 2, . . .) may constitute an appropriate internal variable. If it is the case, the evolution law of this variable should be speciﬁed. It may be formally written as ƒ˙ ⫽ ( )˙ ⫹ ( )T˙ in terms of control variables, stress and temperature, for example. It should be noticed that any attempt to perform a systematic solution to this problem has to be accomplished through a thermodynamic study to derive energetic criteria for phase transformation. 2. To deﬁne the appropriate scale to describe the transformation strain or TRIP strain, accompanying the phase transformation. As this inelastic strain results from complex accommodation processes, which occur at the microscale, morphological considerations of the transformation product have to be taken into account. At this scale, the deﬁnition of the TRIP strain may leads to a set of transformation strains trI (I ⫽ 1, 2, . . .), which depends on the possible crystallographic orientations of martensite related to the concept of martensitic variants.

350

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

It may be possible to adopt a more macroscopic description by introducing a kind of metallurgical variable tr (,T) to deal with the TRIP strain. However, such a description may lead to a model with limited predictive capabilities. 3. To adopt an appropriate nonlinear homogenization scheme for a well-deﬁned representative volume element (RVE). The choice of an appropriate RVE is also conditioned per the choice of internal and metallurgical variables describing the microstructure evolution and the morphological aspects of the transformation. If the problem is described by the macroscopic variables ƒ and tr (,T), the RVE simply represents a two-phase austenite–martensite composite material. For such a case, simple isotropic secant approach (see Chapter 12) may be sufﬁcient to describe the overall behavior. However, a multivariant description of the transformation product may require the deﬁnition of various RVE. For example, an RVE representing a single crystal with a certain number of martensitic variants (different orientations), surrounded by an austenitic matrix, is required to approximate the stress and strain distribution in each phase. Another RVE can also be deﬁned to account for the polycrystalline structure of these materials. Complete descriptions of the above interrelated problems are still under investigation both experimentally and theoretically. In particular, reﬁned microstructural analyses are needed to understand various mechanisms at different scales. As the problem of multiscale modeling is still challenging for these materials, the reader will ﬁnd in this chapter an introduction to the different microscale mechanisms with certain guidance in terms of micromechanical modeling. We pay particular attention to the problem of coexistence of two phases and resulting discontinuities in terms of stress, strain, and mechanical properties. For such a purpose we describe in details the concept of energy momentum, originally introduced by Eshelby. We show how this framework can be adapted to derive energetic criteria for phase transformation at different scales.

13.1 PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

The elementary mechanism accompanying martensitic transformation lies in a nondiffusion process at the atomic level, which transforms the parent crystallographic lattice (austenite) into a new crystallographic lattice of the transformation product (martensite); see Figure 13.2. This

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

Z⬘

Z

冢

兹2a␣⬘

B ⫽ Y

a␥ 0 0

0 兹2a␣⬘ a␥ 0

351

0 0

冣

c␣⬘ a␥

a␥ ⫽ lattice parameter of austentite a␣⬘, c␣⬘ ⫽ lattice parameters of martensite X⬘

X

Y⬘

Figure 13.2 Bain strain resulting from lattice change during phase transformation.

solid–solid phase transformation results from purely geometrical features in a local lattice distortion called the Bain strain. The Bain strain B describing the geometrical transformation from austenite to martensite is incompatible in nature and therefore requires an accommodation procedure that, in general, affects the transformed regions. This accommodation step depends on the mechanical properties of the parent and product phases and leads to a typical length, shape, and spatial distribution of the product of phase transformation. The concept of the incompatibility accompanying the Bain strain means that the lattice change will generate elastic strain both in parent and product phases and, as a result, internal stresses. These stresses may be sufﬁcient to initiate relaxation mechanisms with certain diversity depending on the mechanical properties of the considered material, which are controlled by the chemical composition, thermomechanical processes, and other parameters. The relaxation mechanisms may be activated as follows: • Inelastic deformations by plastic shear or twinning in parent and

product phases • A typical resulting morphology of the transformed domains, which consists, in general, in a plate and lath shapes • Formation of autoaccommodating groups of martensite Indeed, a complete determination of such an accommodating step relies on a ﬁne description of the typical microstructure of the transformation product. Therefore, it could only be accomplished through

352

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

approximate ways leading to the crystallographic theories of martensitic transformation. One of the well-known theories is the method of Wechsler, Liebermann, and Read (1953), which describes the accommodation step by an inelastic strain preserving the parent phase lattice and leading to the concept of habit plane or interface between austenite and martensite. This theory is based on the concept of inelastic compatibility of a local transformation strain tr (r) assumed to be uniform within an elementary transformed volume VI. In other words, the methodology assumes a given morphology of the transformed region and deals with the compatibility conditions through two different ways: one is based on a concept of energy minimization using the elementary Eshelby’s inclusion, the other deals with the problem of stress and strain discontinuities across the interface SI of the considered domain, where the compatibility conditions rely on the coherency of this interface. Eshelby’s Inclusion Method

Through the basic concept of Eshelby’s inclusion problem, the transformed domain VI is assumed to be ellipsoidal in shape and experiences an eigenstrain corresponding to the lattice distortion described by the Bain strain B. If we denote by L the elastic stiffness tensor of the inﬁnite medium and by V its volume, the free energy density reads W⫽

1 VI B ⬊L⬊(I ⫺ SI)⬊B, 2 V

(13.1.1)

where SI is the Eshelby tensor. If the lattice change do not generate any elastic deformation and therefore any increase of the elastic free energy, the compatibility conditions should fulﬁll the following eigenvalue problem: (I ⫺ SI)⬊B ⫽ 0.

(13.1.2)

In general, with the purely geometric lattice change described by B, Eq. (13.1.2) has no solution. Therefore, an additional inelastic mechanism is required to satisfy the eigenvalue problem raised by (13.1.2). One of the accommodation mechanisms corresponds to a plastic shear or twinning within the transformed domain by preserving its crystallographic lattice; see Figure 13.3. The resulting strain is called ‘‘lattice

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

B

P

353

R

Habit Plane

Figure 13.3 Schematic representation of the accommodation process by twinning or slip in martensite by lattice invariant strain (B, Bain strain; P, plastic deformation or twinning; R, rotation).

invariant strain’’ and denoted here by inv. From this analysis, the transformation strain tr ⫽ B ⫹ inv is compatible so that the conditions (I ⫺ SI)⬊tr ⫽ 0

(13.1.3)

det(tr) ⫽ 0 (determinant).

(13.1.4)

is satisﬁed if

Therefore, a complete determination of tr from (13.1.4) can be performed following the next steps: 1. Plastic shear or twinning is assumed to occur along a slip system of the transformed region with a magnitude ␥ so that the lattice invariant strain reads inv ⫽ ␥R,

(13.1.5)

where R deﬁnes the orientation tensor of the slip or twin system deﬁned by its unit normal n˜ and shear direction m ˜ as Rij ⫽ –12 (m ˜ in˜ j ⫹ m ˜ jn˜ i).

(13.1.6)

2. The second step deﬁnes an interface called the habit plane between the two phases, so that the transformation strain is considered to be predominately shear along this plane. That is trij ⫽ –21 g(minj ⫹ mj ni),

(13.1.7)

354

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

where m is the shear direction and n the unit normal to the habit plane; g is the magnitude of the shear. As stated above, the accommodation process occurs mainly by shear, however, when phase transformation is accompanied by substantial plastic ﬂow, a volumic component is measured, which ranges from 1 to 4%. In other words, the two vectors m and n are not necessarily perpendicular (Fig. 13.4). From Eq. (13.1.7) and for a given B and R, the compatibility equations (13.1.3) and (13.1.4) determine g and the vectors m and n. This ends the second step; see Problem 13.1. Method Using Jump Conditions

For this analysis, the compatibility conditions lie in the deﬁnition of a coherent interface or habit plane SI between the parent and product phases with n being the unit normal of the surface. This hypothesis corresponds to the continuity of displacement ([u] ⫽ 0) and/or velocity ([v] ⫽ 0) ﬁelds as well as the stress vector ([] n ⫽ 0), where [x] ⫽ x⫹ ⫺ x⫺ denotes the jump of x across the interface. In the present case, the ‘‘positive’’ side belongs to the parent phase (austenite), whereas the ‘‘negative’’ one corresponds to the transformed regions (martensite). It is interesting to note that, in the case of shape memory alloys where the transformation occurs mainly without a plastic deformation and under speciﬁc conditions, the analysis can also be adapted to martensite–martensite interfaces. The ﬁeld equations expressed at the interface can be reduced to the following compatibility conditions; see Problem 13.2:

→

gm

Martensite

→

n

→

m Austenite Habit Plane

Figure 13.4 Schematic representation of Eq. (13.1.7).

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

⫺ 1 [ij] ⫽ ⫹ ij ⫺ ij ⫽ – 2 (inj ⫹ j ni),

355

(13.1.8)

where the total strain at each side of the interface ⫹,⫺ ⫽ e⫹,e⫺ ⫹ tr⫹,tr⫺ consists of an elastic part e and a transformation contribution tr resulting from the accommodation process accompanying the phase change; is a vector to be determined. For simplicity, the behavior from each side of the interface is described by linear elastic constitutive law, such that ⫹,⫺ ⫽ L⫹,⫺⬊(⫹,⫺ ⫺ tr⫹,tr⫺).

(13.1.9)

If we further introduce a reference homogeneous elastic medium L such that L⫹,⫺ ⫽ L ⫹ (L⫹,⫺ ⫺ L) ⫽ L ⫹ ⌬ L⫹,⫺, Eq. (13.1.9) is equivalent to [] ⫽ L⬊[] ⫺ L⬊[tr] ⫹ [⌬ L⬊e],

(13.1.10)

or by taking into account the condition [] n ⫽ 0, it results that L⬊[]⬊n ⫽ L⬊[tr]⬊n ⫺ [⌬ L ⬊ e]⬊n.

(13.1.11)

Substituting (13.1.8) into (13.1.11) leads to the following equations whose resolution gives the components of the vector . That is ᑣikk ⫽ ℵi,

(13.1.12)

where ᑣik ⫽ Lijklnj nl and ℵi ⫽ Lijkl [trkl]nj ⫺ [⌬ Lijklkle ]nj. Clearly, Eq. (13.1.11) shows that a compatible phase transformation (e.g., e⫹,e⫺ ⫽ 0) requires heterogeneous transformation strain, for example, [tr] ⫽ 0. Therefore, it results from (13.1.11) that a compatible expression of the transformation strain reads [trij ] ⫽ [ij] ⫽ –21 (inj ⫹ j ni).

(13.1.13)

Direct applications of compatibility conditions (13.1.13) can be generated as follows:

356

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

1. The Bain strain described in Figure 13.2 from purely geometrical considerations does not fulﬁll (13.1.13). In fact, if from the austenitic side we state that tr⫹ ⫽ 0 and from the martensitic side tr⫺ ⫽ B, Eq. (13.1.13) gives [trij ] ⫽ ijB ⫽ –21 (inj ⫹ j ni).

(13.1.14)

2. The accommodation process described in the previous section, which relies on a slip or twinning in the transformed regions [see (13.1.5)], fulﬁlls the compatibility conditions (13.1.13), such that if one assumes that tr⫹ ⫽ 0 and tr ⫽ B ⫹inv, the compatibility conditions writes [trij ] ⫽ ⫺(ijB ⫹ ijinv) ⫽ –21 (inj ⫹ j ni),

(13.1.15)

which is equivalent to Eq. (13.1.7). More recently, mathematical-based approaches have been proposed to predict other compatible morphologies during phase transformation. For details, the reader could refer to the Suggested Readings at the end of this chapter.

Notion of Martensitic Variants

As discussed in previous sections, the accommodation process accompanying the lattice change during phase transformation leads to a typical morphology of the transformation product, which implicitly results in a heterogeneous transformation strain tr (r). In the previous analysis, we adopt an accommodation process through a shear or twinning by deﬁning a habit plane between austenite and martensite leading to expressions (13.1.7) and (13.1.15) of the transformation strain tr. From purely crystallographic considerations and due to high symmetries of the parent phase, 24 couples of n and m are possible to deﬁne a habit plane leading to the notion of martensitic variant. From this concept, each possible martensitic variant is described by its crystallographic orientation, morphology, and transformation strain, which are implicitly interrelated by the accommodation process of the lattice change.

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

357

Kinematics at Single-Crystal Level

The purpose of this section is to discuss the different strain mechanisms during phase transformation at the single-crystal level. This step is required to build micromechanical tools for the ﬁrst scale transition linking the appropriate features of transformed regions to constitutive equations of single crystals. At this level, the concept of martensitic variants is taken into account by assuming that the transformation strain is piecewise uniform within elementary transformed regions corresponding to the different martensitic variants, so that one can write

冘 N

(r) ⫽ tr

trI

I (r),

(13.1.16)

I⫽1

where I (r) are the Heaviside step functions for the different transformed domains or variants I and N their number. The transformation strain trI associated with a martensitic variant I is described by (13.1.7) as trij I ⫽ –12 g (miInjI ⫹ mjI niI) ⫽ gRijI ,

(13.1.17)

where RI is the orientation tensor of the variant I. For a single crystal (taken as an RVE) with volume V subjected at its external boundary ⭸V to a displacement ui ⫽ ij xj, and undergoing an inelastic strain ﬁeld tr (r) ⫹ p (r) within V, the total macroscopic strain is ⫽

1 V

冕 ( (r) ⫹ e

V

tr

(r) ⫹ p (r)] dV ⫽ 具e (r) ⫹ tr (r) ⫹ p (r)典. (13.1.18)

Note that the elastic strain ﬁeld e (r) arises from and the incompatibilities of the ﬁelds tr (r) and p (r), where p (r) denote the plastic strain ﬁeld. In general, it is difﬁcult to distinguish experimentally between the plastic contribution and the transformation one at the macroscopic level. However, in terms of modeling, we will be able to make this distinction if we adopt a crystallographic description of phase transformation.

358

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

For homogeneous elasticity with its elastic stiffness L, one obtains directly the elastic part e of as follows: ⫽ L⫺1⬊ ⫹ tp,

(13.1.19)

where ⫽ 具 (r)典, and tp ⫽ 具tr (r) ⫹ p (r)典 corresponds to the macroscopic inelastic strain arising from the phase transformation and the plastic ﬂow. At this stage, one can distinguish between two cases where the physical aspects of martensitic transformation change signiﬁcantly: 1. In the case of shape memory alloys, the plastic contribution is neglected and the transformation strain becomes

冕

1 tr (r) dV. (13.1.20) V V Due to typical properties of the strain ﬁeld tr (r), one can differenciate between two simpliﬁed forms for tr: • The microstructure of variants as well as the fact that tr (r) is piecewise uniform, this leads to tr ⫽

tr ⫽

1 V

冘冕

VI

I

trI dV ⫽

冘

trI

ƒI,

(13.1.21)

I

where trI are material constants, and ƒI are the internal variables subjected to the following constraints: 0ⱕ

冘 ƒ ⱕ 1,

0 ⱕ ƒI ⱕ 1.

I

(13.1.22)

I

• Since the transformation strain vanishes within the austenitic

phase, thus (13.1.21) can be written as tr ⫽

1 V

冕

VM

tr (r) dV ⫽

再

VM 1 V VM

冕

VM

冎

tr (r) dV

⫽ ƒ˜tr,

(13.1.23) where ƒ ⫽ 兺IƒI is the total volume fraction of martensite, and ˜ tr being the average transformation strain over the total volume VM of martensite, which is an unknown to be determined from solving the deformation problem.

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

359

2. The case of iron base alloys where the phase transformation is accompanied by substantial plastic ﬂow in the parent phase. In this case, it is more critical to distinguish at the macroscopic level between a macroscopic transformation strain [in the sense of Eq. (13.1.23)] and a macroscopic plastic strain. This basically results from the fact that the transformation part contains a plastic contribution resulting from the accommodation process discussed above. An incremental formulation with a multivariant description is more appropriate for this class of materials (see below).

Incremental Formulation: Concept of Moving Boundaries

In most heterogeneous materials, the mechanical properties may be assumed piecewise uniform at appropriate scales. These materials are made up of different phases and/or grains separated by interfaces called grain or phase boundaries. The interfaces are in general stationary with respect to particles and often considered as perfect, at least at low temperatures. This hypothesis corresponds to the continuity of displacement ([u] ⫽ 0) and/or velocity ([v] ⫽ 0) ﬁelds as well as the stress vector ([] n ⫽ 0). The continuity assumptions extended to equivalent forms for the volume lead to the usual localization and homogenization relations, from which the classical scale transition methods are developed. The overall behavior of the RVE is then deduced from the microstructure and the local behavior (basically the purpose of previous chapters). In various situations where inelastic strains result from discrete physical mechanisms such as twinning, martensitic transformation, or recrystallization, the previous hypotheses are no longer valid because of evolving microstructures or moving boundaries whose velocities are different from those of the particles. Consequently, the strain ﬁeld and/ or mechanical properties exhibit discontinuities across moving boundaries and therefore: • Additional terms in localization and homogenization relations have

to be introduced in the framework of local thermodynamics and micromechanics to account for the moving boundaries. • Driving forces, germination, and growing laws describing the evolving microstructure need to be determined. These are discussed next.

360

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

Kinematics of Evolving Microstructure

In materials undergoing martensitic phase transformation, the parent and product phases coexist with the same chemical composition but differ in their lattices, volumes, and shapes. As a result, a complex accommodation process (discussed in the previous section) occurs leading to a typical morphology of the transformation product with multiple interfaces S or boundaries within the transformed region itself, and with the parent phase. During a loading increment (stress or temperature), two scenarios are possible: • The material experiences phase transformation with a complex

movement of interfaces between parent and product phases. • Under particular conditions, reorganization of preexisting trans-

formed regions is possible by a typical movement of interfaces within these regions. For example, it is interesting to link, from kinematics purpose, the macroscopic strain increment ˙ acting on the boundary of an RVE to the velocity ﬁeld. The velocity v of particles belonging to the external boundary of the RVE is assumed as d ij i ⫽ ˙ ij xj ⫽ x. dt j

(13.1.24)

From the deﬁnition of macroscopic strain ij ⫽

1 V

冕 V

ij

(r) dV.

The strain increment is given by ˙ ij ⫽

冉 冊冕

d 1 dt V

V

ij (r) dV ⫹

1 ⭸ V ⭸t

冋冕

V

册

ij (r) dV .

(13.1.25)

By neglecting the change in volume V of the RVE, (13.1.25) is reduced to

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

˙ ij ⫽

1 ⭸ V ⭸t

冋冕

册

ij (r) dV .

V

361

(13.1.26)

The strain ﬁeld is discontinuous along the different moving interfaces, the time derivative in (13.1.26) reads ˙ ij ⫽

1 V

冕 ⭸⭸t(r) dV ⫺ V1 冕 [

˙ ij ⫽

1 V

冕 冋⭸⭸t(r) ⫺ [

ij

V

ij

S

(r)]w␣ n␣ dS,

(13.1.27)

or ij

ij

V

册

(r)] w␣ n␣␦(S) dV,

(13.1.28)

where ␦(S) ⫽ 兰S ␦(r ⫺ r⬘) dS⬘ is the Dirac delta function. [] ⫽ ⫹ ⫺ ⫺ is the jump of the local strain ﬁeld; w is the velocity of the interface at a material point, where the outward unit normal to the interface is denoted by n; and w␣n␣ is a scalar describing the normal velocity of the interface. Applications

For example, the time derivative of (13.1.20) shows different mechanisms associated with martensitic transformation in shape memory alloys, which are not revealed through a simple ‘‘static’’ comparison between the actual conﬁguration and the reference one (austenite). By taking into account the discontinuities [tr (r)] ⫽ tr⫹ ⫺ tr⫺ of the strain ﬁeld tr (r) along the moving boundaries, one has ˙ tr ⫽

1 V

冕 ˙

tr

V

1 V

(r) dV ⫺

冕 [

tr

S

(r)]w␣ n␣ dS,

(13.1.29)

and since the concept of stress-free or eigenstrain is adopted for the transformation strain, so that ˙ tr (r) ⫽ 0. It then follows that ˙ tr ⫽ ⫺

1 V

冕 [

tr

S

(r)]w␣ n␣ dS,

(13.1.30)

362

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

where S represents all of the moving boundaries (austenite–martensite as well as boundaries between the martensitic variants), and ␣ n␣ is the normal velocity of the interface. The ‘‘crystalline’’ description of the martensitic transformation (analogous to crystal plasticity) comes directly from (13.1.30); see Problem 13.3: ˙ tr ⫽

冘

trI

ƒ˙ I,

(13.1.31)

I

where in (13.1.31) the distinction between transformation and exchange between existing variants is not explicitly shown. The different mechanisms are more explicitly described when one expands the time derivative of (13.1.23): ˙ tr ⫹ ƒ˜˙ tr. ˙ tr ⫽ ƒ˜

(13.1.32)

In fact, the analysis of (13.1.32) allows us to distinguish the following phenomena: • Transformation (ƒ˙ ⫽ 0) without deformation (˜ tr ⫽ 0, ˙˜ tr ⫽ 0). • Transformation (ƒ˙ ⫽ 0) with deformation (˜ tr ⫽ 0) but without

reorientation (˙˜ tr ⫽ 0). • Deformation by reorientation (˜˙ tr ⫽ 0) without transformation (ƒ˙ ⫽ 0). • Transformation, deformation, and reorientation ( ƒ˙ ⫽ 0, ˜ tr ⫽ 0, ˜˙ tr ⫽ 0).

In the case of iron-based alloys, the average inelastic strain of the single crystal is given by tp ⫽

1 V

冕 [

tr

V

(r) ⫹ p (r)] dV,

(13.1.33)

where p(r) describes simultaneously the plastic strain of an elementary volume element at austenitic and martensitic states. When the plastic ﬂow becomes signiﬁcant during phase transformation, the reorientation and inverse transformation mechanisms can be disregarded. The pro-

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

363

gression of the transformation can be described by the instantaneous growth of new plates or laths in the austenitic phase. The time derivative of (13.1.33) leads to ˙ tp ⫽

1 V

冕 ˙

tp

V

1 V

(r) dV ⫺

冕 [

tp

S

(r)]w␣ n␣ dS.

(13.1.34)

The volume integral in (13.1.34) describes the plastic ﬂow in residual austenite and preexisting martensitic variants, it could be written as the following form involving the average plastic strain rate ˙ pA in austenite and the average one over a martensitic variant. That is 1 V

冕 ˙

tp

V

(r) dV ⫽ (1 ⫺ ƒ)˙ pA ⫹

冘 ƒ ˙

I MI

.

(13.1.35)

I

The surface integral is much more complicated. It requires the determination of the inelastic strain jump at each point of the moving interface, which can be expressed as [tp (r)] ⫽ p⫹ ⫺ (p⫺ ⫹ trI) ⬇ ⫺trI.

(13.1.36)

Such a jump may be assumed to result only from the accommodation process leading to the deﬁnition of compatible transformation strain trI. However, as can be seen from (13.1.36), a heterogeneous plastic strain p⫹,⫺ ⫽ 0 may occur during the phase transformation. Its determination is not a simple task and may require complex numerical calculations. Since the transformation strain trI contains a plastic contribution corresponding to lattice invariant strain, the contribution of p⫹,⫺ can be neglected. Therefore, the surface integral reads ⫺

1 V

冕 [

tp

S

(r)]w␣ n␣ dS ⫽

冘

trI

ƒ˙ I.

(13.1.37)

I

Substituting (13.1.35) and (13.1.37) into (13.1.34) yields ˙ tp ⫽ (1 ⫺ ƒ)˙ pA ⫹

冘 ƒ ˙ ⫹ 冘 I

I

MI

trI

ƒ˙ I.

I

In (13.1.38) one can distinguish the following contributions:

(13.1.38)

364

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

• The ﬁrst term describes the average plastic ﬂow in the residual

austenitic phase. • The second term corresponds to the plastic ﬂow in the preexisting martensitic phase. • The last term expresses the formation of new plates or laths. At the single-crystal level, the plastic ﬂow of residual austenite may be described through the crystallographic slip by introducing the slip systems of FCC lattices. The plastic strain increment is then expressed by (see Chapter 11) ˙ pA ⫽

冘 P ␥˙ , g

g

(13.1.39)

g

where Pg is the Schmidt tensor and ␥˙ g the shear rate on slip system g. However, it is more difﬁcult to track the crystallographic slip in martensitic variants. This is due to the large number of variables (24 ⫻ 24 variables, 24 possible variants, for each 24 possible slip system). Due to the typical ﬁne microstructure of the transformation product and their typical crystallographic orientation, the plastic deformation of martensite may have no signiﬁcant contribution to the overall ﬂow of the RVE. This statement is also supported by the fact that martensite is a hard phase. Equation (13.1.38) is then reduced to ˙ tp ⫽ (1 ⫺ ƒ)

冘 P ␥˙ ⫹ 冘 g

g

g

trI

ƒ˙ I.

(13.1.40)

I

Equation (13.1.40) contains a classical crystal plasticity problem with internal variables, namely the volume fraction of each possible martensitic variant. To come out with a constitutive law of the RVE representing the single crystal, evolution laws of these internal variables have to be speciﬁed. In general, this step requires additional approximations and can be accomplished through two different ways: 1. To establish a thermodynamic framework to obtain the driving forces for the activation of the internal variables. This method is more appropriate to derive energetic criteria for the phase transformation. 2. To assume evolution laws based on experimental observations without any link with thermodynamics. This method does not require the determination of driving forces; however, its predictive capacities are limited.

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

365

In next sections we present an example displaying the ﬁrst methodology. This is possible by adopting the original work of Eshelby’s momentum tensor. Eshelby’s Energy Momentum Tensor

Eshelby introduced an important concept to deal with the conﬁguration of a solid. It corresponds to the energy momentum tensor, which is another way to combine the ﬁeld equations with energetic considerations. Let us consider a homogeneous material without any incompatibility in which the elastic energy density (r,) only depends on the elastic distortion . Therefore, we can perform the following: ,i (r,) ⫽

⭸ ⭸ ⭸jk ⫽ , ⭸xi ⭸jk ⭸xi

(13.1.41)

where the stress tensor reads jk ⫽

⭸ , ⭸jk

(13.1.42)

and jk ⫽ uj,k, and u is the displacement vector. From the equilibrium equation ik,k ⫽ 0, one can easily show that ,i (r,) ⫽ [jk (r)uj,i (r)],k.

(13.1.43)

Thus, (13.1.43) is equivalent to [(r,)␦ik ⫺ jk (r)uj,i (r)],k ⫽ 0.

(13.1.44)

Eshelby’s energy momentum tensor denoted here by ⍀ is expressed by ⍀ik ⫽ ␦ik ⫺ kjuj,i.

(13.1.45)

Therefore, the energy momentum tensor satisﬁes the following equation resulting from (13.1.44): ⍀ik,k ⫽ 0

13.1.46)

Let us consider now the case of martensitic transformation where the accommodation process leads to a nonhomogeneous transformation

366

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

strain ﬁeld tr (r) undergoing a jump [tr (r)] across an interface between the parent and product phases. Let us deﬁne the following local quantity Fi ⫽ [⍀ik]nk, which can be expressed from (13.1.45) as Fi ⫽ [␦ik ⫺ jkuj,i]nk ⫽ []ni ⫺ [jkuj,i]nk.

(13.1.47)

From the diagonal symmetries of the elastic constant L and the decomposition of the total distortion  into an elastic part e and a transformation contribution tr, one obtains for the jump of elastic energy (see Problem 13.4) [] ⫽ –12 (ij⫹ ⫹ ij⫺)]ije ].

(13.1.48)

On the other hand, the continuity of the traction vector, [] n ⫽ 0, leads to 1 ⫹ ⫺ [jkuj,i]nk ⫽ –21 (jk⫹ ⫹ ⫺ jk )[uj,i]nk ⫽ – 2 (jk ⫹ jk )[ji]nk.

(13.1.49)

Substituting (13.1.48) and (13.1.49) into (13.1.47), one has Fi ⫽ –21 (jk⫹ ⫹ jk⫺){[jke ]ni ⫺ [ji]nk},

(13.1.50)

and by taking into account the compatibility equation (13.1.8), it results [ji]nk ⫽ [uj,i]nk ⫽ j nink ⫽ j nkni ⫽ [jk]ni.

(13.1.51)

Finally with (13.1.51), it follows that Fi ⫽ [⍀ik]nk ⫽ –21 (jk⫹ ⫹ jk⫺)[jktr ]ni.

(13.1.52)

If one follows a complete thermodynamic study—see Cherkaoui et al. (1998)—one can show that the scalar F ⫽ Fiwi

(13.1.53)

is the mechanical driving force if one considers the normal velocity of the interface w␣n␣ as the internal variable describing the microstructure evolution. This variable is, in general, not appropriate to derive constitutive equations of materials with evolving microstructure. It requires time-consuming and complex computational tools. By means of addi-

13.2.

APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS

367

tional hypotheses taking into account the typical morphology of martensite, an alternative description is possible. It could be considered as another scale of description, which adopts the volume fractions of martensite as internal variables. 13.2 APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS FOR SINGLE CRYSTALS Thermodynamic Driving Forces

Recently, Cherkaoui et al. (1998) extended Eshelby’s (1970) pioneering work on the energy momentum tensor to derive the thermodynamic driving force acting on a moving boundary point between the product and the parent phases. That is F ⫽ ⫺–12 (⫹ ⫹ ⫺)⬊[tp] ⫹ [],

(13.2.1)

where [tp] and [] denote the jumps of the inelastic strain and the chemical energy, respectively; ⫹ and ⫺ correspond to the limiting values of the local stress ﬁeld for each side of the moving interface, which can be linked with the help of interface operators Q(L, n), ⫹ ⫽ ⫺ ⫺ Q(L, n) ⬊ [tp],

(13.2.2)

depending on the unit normal to interface and elastic constant of the material. With (13.2.2), (13.2.1) can be rewritten as F ⫽ [–12 Q(L, n) ⫺ ⫺]⬊[tp] ⫹ [].

(13.2.3)

As noticed above, the introduction of (13.2.3) as a thermodynamic driving force assumes that the interface normal velocity is taken as the internal variable characterizing the phase transition. It is also noticed that equation (13.2.3) requires the determination of the local stress and strain ﬁelds in each point of the moving interface. Therefore, the determination of (13.2.3) for any topology of the interface could be obtained only through strong numerical calculations. To go a step further in the scale transition, an alternative relation of (13.2.3) is obtained by introducing the concept of an ellipsoidal growing. The former hypothesis assumes that the moving interface represents an ellipsoidal growing domain. This is in accord with the microstructure developed during

368

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

martensitic transformation corresponding to the formation of microdomains of a typical morphology of plate or lath. Furthermore, as we discussed in the previous kinematic study, the martensitic transformation progresses by the nucleation and instantaneous growth of new domains. This is related to a high interface velocity between the parent and product phases, leading consequently to the following expression for the local jump [tp] of the inelastic strain [tp]I ⫽ p⫹ ⫺ (p⫺ ⫹ trI) ⫽ ⫺trI.

(13.2.4)

In other words, the instantaneous growth of a martensitic domain allows the continuity of the plastic strain over its boundary. In connection with (13.1.40), it implies that the volume fractions ƒI of each possible martensitic variant are the internal variables characterizing the phase transition at the mesoscale, the integration of (13.2.3) along the ellipsoidal domain interface, and thanks to (13.2.4) one obtains the driving force FI for the ‘‘ﬂow’’ ƒ˙ I of a martensitic variant due to the formation of a new domain. That is, S˙ I FI ⫽ ⫺⬊trI ⫺ B(T ⫺ T 0) ⫹ –21 trI⬊L⬊(I ⫺ SI)⬊trI ⫹ –12 trI ⬊L⬊ ˙ I⬊trI ƒI, ƒ (13.2.5) where I is the identity tensor and SI is Eshelby’s tensor depending on the aspect ratio as well as on the orientation of the martensitic microdomain; S˙I corresponds to the variation of SI due to the ellipsoidal growth. For the sake of simplicity, a homothetic growth is assumed giving S˙I ⫽ 0. The term B(T ⫺ T 0) is a linear approximation of the chemical energy jump []. B is a material constant and T 0 the equilibrium temperature. It should be noticed that the derivation of (13.2.5) requires the hypothesis of a uniform stress ﬁeld ⫺ within the growing ellipsoidal domain. Details on the derivation of (13.2.5) as well as on the notion of ellipsoidal growing can be found in Cherkaoui et al. (1998). Equation (13.2.5) gives the thermodynamic driving force for nucleation and growth of martensitic microdomains belonging to different martensitic variants; it requires the knowledge of the stress ﬁeld inside the growing domains. In addition to the overall applied stress, this stress ﬁeld contains several contributions due to different couplings between plasticity and phase transformation at the microscale. In the

13.2.

APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS

369

following, several ways for the determination of internal stresses are discussed from a micromechanics point of view: 1. The simplest way is to neglect any source of internal stresses. In such conditions, Patel and Cohen (1953) have formulated the energy term resulting only from the interaction of applied stress with transformation strains. This corresponds in (13.2.5) to the term ⬊trI ⫺ B(T ⫺ T 0), where ⫺is assumed equal to the applied stress , and all the other contributions are neglected. 2. It is possible to assume an ellipsoidal growth of a martensitic microdomain inside a homogeneous stress ﬁeld corresponding to the average stress over the austenitic phase. At the current conﬁguration of the RVE, if we denote by pA the average plastic strain in the austenitic phase, the interactions between plasticity and martensitic phase transformation are taken into account through the average stress A in the austenitic phase; see Exercise Problem 13.5:

冘 ƒ L ⬊ (I ⫺ S ) ⬊ ( N

A ⫽ ⫺

I

I

pA

⫺ trI),

(13.2.6)

I⫽1

where N is the number of active martensitic variants at the current conﬁguration of the RVE and ƒI their volume fractions. With the instantaneous growth hypothesis, the stress inside a growing microdomain ⫺ belonging to a martensitic variant I is related to A by the following simple form (see Problem 13.6): ⫺ ⫽ A ⫺ L ⬊ (I ⫺ SI) ⬊ trI.

(13.2.7)

With (13.2.7), (13.2.3) leads to FI ⫽ A ⬊ trI ⫺ B(T ⫺ T 0) ⫺ –21 trI ⬊ L ⬊ (I ⫺ SI) ⬊ trI.

(13.2.8)

In the thermodynamic force (13.2.8), one can distinguish two contributions: • A long-range internal stress effect through the term A : trI ⫺ B(T ⫺ T 0). The stress A contains the effects of plastic strain of both

phases, as well as of transformation strains undergone by the pre-

370

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

existing martensitic variants. Depending on the applied and internal stresses, A plays the role of variant selection. • A self-internal stresses effect through the term –12 trI : L : (I ⫺ SI) : trI depending essentially on the morphology of the growing microdomain. The effect of the internal stress ﬁeld (emerging from the plastic ﬂow) on the martensitic phase transformation is known as the strain-induced martensitic phase transformation phenomenon. Classically, the plastic ﬂow at the grain level is described by a homogeneous plastic strain through the plastic slip on crystallographic glide systems. Intragranular stresses arising from this description correspond to the second-order internal stresses. However, for ductile materials undergoing martensitic phase transformation, the role of plastic strain in phase transition is more complicated. In fact, the martensitic plates nucleate at dislocation pile-ups, dislocation dipole, or intersection of slip bands. In such a situation, the description of the strain-induced martensitic transformation is insufﬁcient through a homogeneous plastic strain. In other words, a third-order stress ﬁeld emerging from the heterogeneity of plastic strain has to be taken into account. This can be performed by the decomposition of the local austenitic plastic strain p (r) into: • A uniform part pA corresponding to its average over the whole

volume of the austenitic grain (this part is described by the crystallographic slip). • A ﬂuctuating part ⌬p (r) taking into account the heterogeneity of the plastic strain due to various conﬁgurations of inelastic defects. To take into account the ﬂuctuations of the plastic strain, (13.2.7) giving the stress inside a growing microdomain belonging to a martensitic variant I is extended to ⫺ ⫽ A ⫺ L ⬊ (I ⫺ SI) ⬊ trI ⫹ p (r),

(13.2.9)

where p (r) is a third-order stress ﬁeld resulting from ⌬p (r) p (r) is evaluated using an inclusion problem, where we assume that the martensitic domain nucleates and grows at a plastic defect with volume V p and undergoing a plastic heterogeneity with strength ⌬p. The initial shape of the martensitic nucleus coincides with one of the plastic defects. In such conditions, the thermodynamic force (13.2.8) is extended to the following form [see Cherkaoui et al. (2000)]:

13.2.

APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS

371

FI ⫽ A ⬊ trI ⫺ B(T ⫺ T 0) ⫺ –12 trI ⬊ L ⬊ (I ⫺ SI) ⬊ trI ⫹ gHIn␥ n, (13.2.10) where HIn ⫽ RI ⬊ L ⬊ (SI ⫺ Spn) ⬊ PAn,

(13.2.11)

Spn is Eshelby’s tensor depending on the morphology of the plastic ‘‘defect’’ assumed to have the initial shape of the martensitic nucleus; g and RI are given in Eq. (13.1.17); ␥ n is the plastic slip in the residual austenitic phase; PAn is the corresponding Schmidt tensor; and is a model parameter. For the plastic ﬂow in residual austenitic phase, the associated driving forces are the resolved shear stresses on slip systems given by (see Chapter 11) An ⫽ A ⬊ PAn.

(13.2.12)

As shown by equation (13.2.12), the plastic ﬂow is affected by the phase transformation through the average stress A. This constitutes in addition to the transformation strain the mechanisms of ductility enhancement in these materials. Critical Forces and Constitutive Equations of a Single Crystal

From an energetic point of view, the formation of a martensitic domain is allowed, if the associated driving force FI overcomes a transformation barrier Fc. This critical force stems from the energy necessary to rebuild the crystal lattice at the front of the developed domain. Fc can be considered as a material parameter. Concerning the plasticity of the austenitic phase and since the predominant mechanisms are the plastic slips on the crystallographic glide systems, the usual hardening matrix Hgh A is introduced describing the self and the latent hardening in FCC metals; see Chapter 11. In such conditions, the critical force cg A to achieve for plastic slip on a glide system g is expressed as h cAg ⫽ cA0 ⫹ Hgh A ␥ ,

(13.2.13)

where cA0 is the initial critical shear stress and is identical for all the slip systems.

372

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

When the thermodynamic driving forces reach their critical values, the consistency rule leads to the evolution laws for ƒ˙ I and ␥˙ n. From (13.2.10) and (13.2.12), the consistency rule applied to the transformation type of internal variables gives the following expression: ˙ RI ⫹ gƒ˙ JL⬊(I ⫺ SJ)⬊RI ⬊ RJ ⫺ ƒJL⬊(I ⫺ SJ)⬊RI⬊PAn␥˙ n ⬊ ⫹ HIn␥˙ n ⫺

B ˙ T ⫽ 0. g

(13.2.14)

In the same way, one obtains from (13.2.13) and (13.2.12) the following relation for the plastic type of internal variables: ˙ PAg ⫹ gƒ˙ JL⬊(I ⫺ SJ)⬊PAg ⬊ RJ ⬊ ⫺ ƒJL⬊(I ⫺ SJ)⬊PA ⬊ PA ␥˙ n ⫺ HAgn␥˙ n ⫽ 0. g

n

(13.2.15)

which is added to Eq. (13.2.14) to build a nonlinear system whose solution gives the evolution laws of the internal variables Xi characterizing the martensitic phase transformation and the plastic ﬂow of the parent phase. This could be formally written as ˙ X˙ i ⫽ Akli (,T,X)˙ kl ⫹ Bi (,T,X)T.

(13.2.16)

Equation (13.2.16) can be also expressed formally as function of internal variables Xi as follows: k ˙ ˙ tp ij ⫽ Mij (X)Xk.

(13.2.17)

Combining (13.2.16) and (13.2.17), the inelastic response of an austenitic single crystal is expressed as k k k k ˙ ˙ ˙ tp ij ⫽ Mij (X) Amn (,T,X)mn ⫹ Mij (X)B (,T,X)T.

(13.2.18)

˙ , one obtains the constiBy adding the elastic response ˙ e ⫽ L⫺1 ⬊ tutive equation of an austenitic single crystal undergoing martensitic phase transformation coupled with plasticity. That is

13.3.

OVERALL BEHAVIOR OF POLYCRYSTALLINE MATERIALS

373

k k ˙ ˙ ij ⫽ [L⫺1 ijmn ⫹ Mij (X) Amn (,T,X)]mn

˙ ⫹ Mkij (X) Bk (,T,X)T.

(13.2.19)

Equation (13.2.19) can also be formally written as ˙ ˙ ij ⫽ (L)⫺1˙ mn ⫺ mT,

(13.2.20)

where L and m are the average tangent elastoplastic and thermal moduli of a single crystal, respectively. Equation (13.2.20) is similar to a nonhomogeneous thermoelastic problems where both elastic modulus and thermal expansion coefﬁcients ﬂuctuate in a given composite material. In our case, it corresponds to a polycrystalline aggregate of single crystals with given crystallographic orientations with their constitutive laws described by (13.2.20). Here the thermal contribution arises only from the chemical energy related to phase transformation. Under purely mechanical loading conditions (T˙ ⫽ 0), Eq. (13.2.20) is reduced to the incremental formulation adopted by Hill for his selfconsistent model; see Chapter 11. An extension of Hill’s approach to account for the ‘‘thermal’’ ﬂuctuations of local ﬁelds is not straightforward. In the next section, we recall the ﬁeld equations within a thermomechanical framework. The analysis leads to a thermomechanical integral equation. A self-consistent approximation of this equation reduces to Hill’s model when a purely mechanical loading is applied.

13.3 OVERALL BEHAVIOR OF POLYCRYSTALLINE MATERIALS WITH PHASE TRANSFORMATION

In the previous section, the constitutive equation of an austenitic single crystal has been established within micromechanics and thermodynamics frameworks. This accomplishes the ﬁrst transition method, which takes into account different features of martensitic transformation and its couplings with plastic ﬂow. Interactions between crystals have to be undertaken to describe the thermomechanical behavior of a polycrystalline aggregate, where each constituent is described by the constitutive equation (13.2.20). For such a purpose, let us consider a representative volume element of the polycrystalline aggregate with volume V, subjected on its boundary ⭸V to a velocity ﬁeld v(r) such that

374

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

i(r) ⫽ u˙ i(r) ⫽ ˙ ij xj

if r(xi) 僆 ⭸V,

(13.3.1)

where ˙ is the macroscopic applied strain. The ﬁeld equations ˙ ij,j(r) ⫽ 0,

˙ ij(r) ⫽ –12 [˙ui,j(r) ⫹ u˙ j,i(r)],

˙ ij(r) ⫽ Lijkl(r)˙kl(r) ⫺ mij(r)T˙

(13.3.2)

can be combined to solve the problem through the solution of a thermomechanical integral equation; see Problem 13.7: ˙ mn(r) ⫽ ˙ mn ⫹

冕

V⬘

0 ˙ dV⬘. ⌫mnij (r ⫺ r⬘)[⌬ Lijkl(r⬘)˙kl(r⬘) ⫺ ⌬ mij(r⬘)T]

(13.3.3) To derive (13.3.3), a reference homogeneous medium with properties L0 and M0, and with the same boundary conditions (13.3.1), is introduced such that Lijkl(r) ⫽ L0ijkl ⫹ ⌬ Lijkl(r),

mijkl(r) ⫽ M 0ijkl ⫹ ⌬ mijkl(r),

(13.3.4)

where ⌫0mnij (r ⫺ r⬘) is the modiﬁed Green’s function, expressed by 0 ⌫0mnij(r ⫺ r⬘) ⫽ ⫺–12 [G0ki,kl (r ⫺ r⬘) ⫹ Gkj,li (r ⫺ r⬘)]

(13.3.5)

in terms of Green’s functions G0(r ⫺ r⬘) related to the reference homogeneous medium. Originally, the self-consistent mean ﬁeld theory has its great interest in the properties of the modiﬁed Green tensor ⌫0, which can be divided for any homogeneous medium with tangent moduli L0 into a local part ⌫loc and nonlocal part ⌫nloc such as nloc ⌫0ijkl (r) ⫽ ⌫loc ijkl␦(r) ⫹ ⌫ijkl (r).

(13.3.6)

Substituting (13.3.6) into (13.3.3), and using the properties of the Dirac function ␦(r), the integral equation becomes,

13.3.

OVERALL BEHAVIOR OF POLYCRYSTALLINE MATERIALS

375

loc ˙ ˙ mn(r) ⫽ ˙ mn ⫹ ⌫mnij [⌬ Lijkl (r)˙kl (r) ⫺ ⌬ mij (r)T]

冕⬘ ⌫

⫹

V

(r ⫺ r⬘)

nloc mnij

˙ dV⬘, [⌬ Lijkl(r⬘)˙kl(r⬘) ⫺ ⌬ mij(r⬘)T]

(13.3.7) where the integral form in (13.3.7) is generally difﬁcult to estimate due to high and stochastic ﬂuctuations of the ﬁeld ⌬ L(r⬘)⬊˙ (r⬘) ⫺ ⌬ m(r⬘)T˙. To overcome this difﬁculty, the self-consistent mean ﬁeld theory for elastic materials chooses a reference medium (L0, M0) so that the mean value of the ﬁeld ⌬ L(r⬘)⬊˙ (r⬘) ⫺ ⌬ m(r⬘)T˙ vanishes and therefore the integral in (13.3.7) can be neglected. This condition of vanishing mean value of the ﬂuctuating ﬁeld is also known as the self-consistency condition. In fact, this condition writes

冕

V⬘

˙ dV⬘ ⫽ 0. [⌬ L(r⬘)⬊˙ (r⬘) ⫺ ⌬ m(r⬘)T)

(13.3.8)

On the other hand, one can show in a straightforward manner that Eq. (13.3.8) leads to the following macroscopic behavior (see Problem 13.8): ˙ ij ⫽ L0ijkl˙ kl ⫺ M ij0 ˙T.

(13.3.9)

Expression (13.3.9) shows an interesting property that consists in the typical choice of the reference medium (L0, M0) to fulﬁll the consistency condition stated above. Clearly, it follows from (13.3.9) that the properties of the reference medium should be the effective properties of the considered composite, that is, L0 ⫽ L and M0 ⫽ M. Under the self-consistent approximation, Eq. (13.3.7) is reduced to loc ˙ mn(r) ⫽ ˙ mn ⫹ ⌫mnij [(Lijkl(r) ⫺ Lijkl]˙kl(r)

˙ ⫺ [mij(r) ⫺ Mij]T.

(13.3.10)

Here ⌫loc is calculated with respect to the effective properties L of the polycrystalline material. Equation (13.3.10) may be reorganized as follows:

376

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

˙ ˙ ij(r) ⫽ Aijkl(r)˙ kl ⫺ aij(r)T,

(13.3.11)

where the concentration tensors A and a are expressed by loc Amnkl(r) ⫽ {Imnkl ⫺ ⌫mnij [Lijkl(r) ⫺ Lijkl]}⫺1, loc akl(r) ⫽ Aklmn(r)⌫mnij [mij(r) ⫺ Mij].

(13.2.12)

Note that Eq. (13.3.11) solves the concentration or localization problem, which allows us to determine the effective properties as L ⫽ 具L(r)⬊A(r)典V,

(13.3.13)

M ⫽ 具L(r)⬊a(r) ⫹ m(r)典V,

(13.3.14)

where the following properties have been used: ˙ ⫽ 具 ˙ (r)典V,

˙ ⫽ 具˙ (r)典V,

˙ ⫽ L⬊˙ ⫺ MT. ˙

Note that the mean ﬁeld self-consistent model developed by Hill and extensively discussed in Chapter 11 can be described by the localization problem (13.3.11) in the case of purely mechanical load (T˙ ⫽ 0). In fact, Eshelby’s elementary inclusion problem used by Hill to solve the concentration problem is deduced from (13.3.11) by assuming piecewise uniform tangent modulus, so that ˙ rij ⫽ Arijkl˙ kl

loc r with Arijkl ⫽ [Imnkl ⫺ ⌫mnij (Lijkl ⫺ Lijkl)]⫺1.

(13.3.15)

In Eq. (13.3.15), one can readily show the relationship between ⌫loc and the Hill’s tensor H and as a result the equivalency between Eq. (13.3.13) and (11.1.61) given in Chapter 11; see Problem 13.9. Finally, to adopt the above framework for polycrystalline materials, the representative volume element is assumed to be an aggregate of N single crystals with homogeneous properties (Lg, mg) (g ⫽ 1, . . . , N) and volume fractions ƒg. The integral forms (13.3.13) and (13.3.14) are reduced to the following discrete expressions:

PROBLEMS

冘 ƒ L ⬊A ,

377

N

L ⫽ 具L(r)⬊A(r)典V ⫽

g

g

g

(13.3.16)

g⫽1

冘 ƒ (L ⬊a ⫹ m ), N

M ⫽ 具L(r)⬊a(r) ⫹ m(r)典V ⫽

g

g

g

g

(13.3.17)

g⫽1

where Ag ⫽ [I ⫺ ⌫loc(L)⬊(Lg ⫺ L)]⫺1,

(13.3.18)

ag ⫽ Ag ⬊ ⌫loc (L)⬊(mg ⫺ M).

(13.3.19)

As discussed in Chapter 11, the implementation of Eq. (13.3.16) to (13.3.19) required an iterative numerical scheme. Note that the tangent moduli (Lg, mg) (g ⫽ 1, . . . , N) are deduced from Eq. (13.2.19), which requires the resolution of a nonlinear system involving the various internal variables related to phase transformation and plastic ﬂow in each considered single crystal. Indeed, the present problem dealing with the behavior of polycrystalline materials with phase transformation is much more complicated than a purely plastic problem. Numerical implementation of the present framework and applications to real polycrystalline materials can be found in Cherkaoui et al. (2000). PROBLEMS

13.1 Let us assume that the accommodation process accompanying the Bain strain occurs by plastic deformation p on a slip system with unit normal n˜ and shear direction m ˜ . We denote by ␥, the magnitude of shear. (a) If n˜ is of (1,0,1) type and m ˜ parallel to (1,0,⫺1) direction, provide the expression of p. (b) If the Bain strain is expressed by B ⫽

冢

冣

a 0 0 0 a 0 with a ⫽ 0.132, c ⫽ ⫺0.199 0 0 c

(a and b are lattice parameters) express the compatibility condition and determine ␥.

378

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

(c) Determine n and m in Eq. (13.1.7). 13.2 Prove the compatibility conditions (13.1.8). 13.3 Let us consider a RVE with volume V and that consists of a twophase austenite–martensite composite. We denote by ƒ ⫽ VM /V the volume fraction of martensite. Let us assume that the existing martensite is described by an ellipsoidal domain with boundary or interface S. If the phase transformation occurs by the ellipsoidal growth of this domain: (a) Show that the volume fraction change is expressed by (indications: use the half-axes of an ellipsoid) ƒ˙ ⫽

V˙ M 1 ⫽ V V

冕wn S

␣ ␣

dS.

(b) If the transformation strain is assumed to be piecewise uniform, so that

冘 (r), N

tr(r) ⫽

trI I

l⫽1

prove Eq. (13.1.31). 13.4 Prove Eq. (13.1.48). 13.5 Consider a RVE with an austenitic matrix containing N martensitic variants. Each variant I has experienced an eigen strain trI during the phase transformation. Denote by A the average stress in the matrix and by MI the one in a martensitic variant. By using Kroner’s inclusion problem where the inﬁnite medium represents the austenitic matrix: (a) Show that MI ⫽ A ⫹ L⬊(I ⫺ SI )⬊(PA ⫺ trI). (b) Prove Eq. (13.3.20). 13.6 Consider an inﬁnite medium representing an austenitic matrix with prescribed A and pA. Assume that a martensitic ellipsoidal domain growth instantaneously in this matrix. If we denote by ⫺ the stress within this domain: Show that ⫺ ⫽ A ⫺ L⬊(I ⫺ SI) ⬊ trI.

13.7 Using Green’s functions for inﬁnite medium, prove the integral equation (13.3.21).

SUGGESTED READINGS

379

13.8 Prove Eq. (13.3.22). 13.9 Provide the relation between ⌫loc and Hill’s tensor and prove the equivalency between Eq. (13.3.13) and Eq. (11.1.61) given in Chapter 11.

REFERENCES Cherkaoui, M., M. Berveiller, and X. Lemoine (2000) Couplings Between Plasticity and Martensitic Phase Transformation: Overall Behavior of Polycrystalline TRIP Steels, Int. J. Plasticity, Vol. 16, pp. 1215–1241. Cherkaoui, M., M. Berveiller, and H. Sabar (1998). Micromechanical Modeling of Martensitic Transformation Induced Plasticity (TRIP) in Austenitic Single Crystals, Int. J. Plasticity, Vol. 14, pp. 597–626. Eshelby, J. D. (1970). Energy Relations and the Energy-Momentum Tensor in Continuum Mechanics, In Inelastic Behavior of Solids, M. F. Kanninen, W. F. Alder, A. R. Rosenﬁeld, and R. I. Joffee, eds., McGraw-Hill, New York, pp. 77–115. Patel, J. R. and M. Cohen (1953). Criterion for the Action of Applied Stress in the Martensitic Transformation, Acta Metall., Vol. 1, pp. 531–538. Wechsler, M. S., D. S. Lieberman, and T. A. Read (1953). On the Theory of the Formation of Martensite, AIME Trans. J. Metals, Vol. 197, pp. 1503– 1515.

SUGGESTED READINGS Diani, J. M., and D. M. Parks (1998). Effects of Strain State on the Kinetics of Strain Induced Martensite in Steels, J. Mech. Phys. Solids, Vol. 46, pp. 1613–1635. Fischer, F. D. and S. M. Schlo¨gl (1995). The Inﬂuence of Material Anisotropy on Transformation Induced Plasticity in Steel Subject to Martensitic Transformation, Mech. Mater., Vol. 21, pp. 1–23. Franciosi, P., M. Berveiller, and A. Zaoui (1980). Latent Hardening in Copper and Aluminium Single Crystal, Acta Met., Vol. 28, pp. 273. Gautier, E. and A. Simon (1988). In Phase Transformation, Vol. 87, G. W. Lorimer, ed., Institute of Metals, London, pp. 285–287. Greenwood, G. W. and R. H. Johnson (1965). The Deformation of Metals under Small Stresses During Phase Transformation, Proc. Roy. Soc., Vol. A283, pp. 403.

380

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

Leblond, J. B., J. Devaux, and J. C. Devaux (1989) Mathematical Modelling of Transformation Plasticity in Steels, I: Case of Ideal-Plastic Phases, Int. J. Plasticity, Vol. 5, pp. 551–572. Magee, C. L. (1966). Transformation Kinetics, Microplasticity and Aging of Martensite in Fe-31 Ni, Ph.D. Thesis, Carnegie Institute of Technology, Pittsburgh. Olson, G. B. and M. Cohen (1975). Kinetics of Strain-Induced Martensitic Nucleation, Metall. Trans. A, Vol. 6A, pp. 791. Stringfellow, R. G., D. M. Parks, and G. B. Olson (1992). A Constitutive Model for Transformation Plasticity Accompanying Strain-Induced Martensitic Transformation in Metastable Austenitic Steels, Acta Metall. Mater., Vol. 40, pp. 1703–1716.

INDEX

A adiabatic deformation, 21 austenitic phase, 348, 358, 363– 364, 369, 371 auto-accommodating groups, 351 average strain theorem, 110 average stress theorem, 109 axial stress, 261–263 B Bain strain, 351–352, 354–356, 377 body force, 15, 17, 35, 37, 53–54, 109, 113, 127, 285 bound Hashin-Shtrikman lower, 143, 340 Hashin-Shtrikman upper, 143, 144 Poisson’s ratio, 220 Reuss lower, 123, 138, 330 Voigt upper, 123, 138, 330 boundary value problem, 35–36, 41–43, 54–55, 127 bridging ﬁbers, 261, 264 Burgers vector, 57, 58, 62 C Cauchy formula, 15–17 strain, 14 stress, 15–16, 18, 20, 22, 24, 33 characteristic function, 105–107 coefﬁcient of thermal expansion, 28–29, 52–53 cofactor, 37, 74

compatibility condition, 50, 352, 354–356, 377–378 composite sphere model, 196, 198, 200, 203, 205 concave surface, 32 concentration tensors, 118–119, 154–155, 158, 175, 333 conjugate pair, 20 conservation of energy, 20, 273 consistency condition, 105, 304, 375 constitutive law, 22 continuity of displacement, 245, 354, 359 coordinate rotation, 215 correlation function, 105–108 crack density, 268–269, 271–272, 274, 276, 277 crack opening displacement, 263– 266, 269–272 crack tip, 2, 259, 261, 264 creep behavior, 325 creep function, 29–31 critical shear stress, 303, 309, 312, 316, 325–326, 371 crystal polycrystal, 100, 173–174, 176– 177, 179, 281, 284–286, 291– 294, 296–299, 306–307, 310– 312, 314, 316–318, 373 single, 176, 179, 281, 283, 285– 287, 291, 294, 296, 298–303, 305–314, 316, 325–326, 350, 357, 362, 364, 372–373, 376– 377, 379

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

381

382

INDEX

D debond, 246 deformation tensor, 14, 20, 22–33 deformed conﬁguration, 12–13, 15–17, 20, 50 deformed surface, 17 determinant, 37, 74, 353 Differential Scheme, 179, 195, 213 dilute case, 160, 185, 187, 225 dilute concentration, 185 dislocation dipole, 370 edge, 58 general, 62 loop, 62–64, 66 pile-ups, 370 screw, 56 displacement boundary condition, 111, 116, 121–123, 126, 133, 135–136, 138, 147, 151–152, 155, 159–160, 169, 174, 198, 257, 284, 328–329 distribution function, 177–178 distribution of the inhomogeneities, 161, 183 divergence theorem, 18–19, 41, 55, 82, 109–122, 128, 247, 248 dot product, 6 double dot product, 6 dyad, 6 E effective compliance, 114, 116, 118–119, 161, 168, 174, 232, 257 effective modulus, see also effective stiffness, 113–114, 120, 165, 179, 183, 185, 187, 190, 198, 202, 204, 221, 267– 268, 297 effective stiffness, see also effective modulus, 114–115, 117, 119, 122, 125, 126, 138, 140, 159, 160, 162, 166, 169– 171, 174, 176, 177, 179, 180,

183, 194, 257, 258, 268, 273, 277, 280, 332, 334 elastic distortion, 64, 365 elastic polarization strain, 49 elasticity, 22, 34, 35, 47, 120, 153 elastic-plastic material, 32, 34 elastoviscoplasticity, 312 ellipsoidal inclusion, 71, 77, 79, 81, 86, 177, 247, 252, 292, 297, 317 ellipsoidal inhomogeneity, 84, 156, 158, 164, 174, 177 energy dissipated, 290 elastic, 289 Gibbs free, 21 Helmholtz free, 21 momentum tensor, 365, 367 release rate, 272–273 engineering constants, 217, 219, 224–226, 233, 266 ensemble average, 103–105, 107, 108–109, 285, 296 enthalpy, 21 equivalent inclusion equation, 87, 89, 156, 157, 255 equivalent inclusion method, 85, 91, 155–156 ergodic hypothesis, 104, 106, 107 Eshelby energy momentum tensor, 365, 367 estimate, 160–161, 185, 190, 193 method, 158, 184 modiﬁed, 247, 252 modiﬁed tensor, 252 solution, 40, 80, 86–89, 155, 157, 251, 315, 316 tensor, 79, 80, 83, 139, 141, 157, 159, 162, 170–171, 175, 177, 183, 223–235, 251–252, 255, 257, 293, 297, 307, 309, 352 Euler

INDEX

angles, 176–177 conﬁguration, 12, 17 coordinate, 12 strain, see also Cauchy strain, 14 evolving microstructure, 360 extensional stiffness matrix, 240 external heat ﬂux, 20 F Fiber, 113, 212–214, 217, 243, 244, 259, 278, 279, 317 ﬁber bridging, 259 ﬁber-reinforced composite, 100, 155, 214–215, 221, 223–224, 226, 234, 240, 259–261 ﬂow rule, 32–33 ﬂuctuating ﬁeld, 319, 375 fracture criterion, 2, 267, 272 fracture toughness, 259, 260, 266 G geometric singularity, 262 global strain concentration, 159, 166, 173, 333 grain, 100, 173–174, 176–177, 179, 281, 283, 292–294, 296, 297–299, 306–307, 309–310, 315, 359, 370 Green function, 38, 40–43, 55, 63, 64, 77, 79, 127–128, 132, 138, 139, 147–148 strain, 14 theorem, 18 H habit plane, 352–354, 356 Hashin-Shtrikman variational principle, 133, 136 hereditary nature, 280 hierarchical approach, 226, 239 high concentration, 185 Hill

383

constraint tensor, 90, 175, 194, 299 lemma, 111, 115, 290, 330, 338–339 polarization tensor, 78 homogeneous polynomial, 39 homogenization scheme, 283, 287, 294, 328, 332, 335–336, 339–340, 350 Hooke’s law, 24, 30, 35, 50–53, 58, 62, 74, 75, 80, 85–86, 88, 117, 122, 147–148, 174, 227, 234, 285, 288, 308 Hutchinson’s calculation, 307 hyperelastic material, 22 I incompressibility, 34, 294, 306 incompressible material, 283, 327, 336–337 incremental formulation, 326, 359 indicial notation, 5 inelastic behavior, 280, 348 initial conﬁguration, 12, 13, 17 interface imperfect, 246, 247, 257, 258 inclusion-matrix, 75 inhomogeneity-matrix, 76 perfect, 73, 245–246, 251, 257– 258 sliding, 246 spring model, 246 velocity, 368 internal energy, 19, 20, 21 internal heat source, 20 internal variable, 291, 321, 342, 358, 364, 367–368, 372, 377 interphase incompatibility, 285 intra-phase ﬂuctuation, 280 isentropic deformation, 21, 22 isothermal deformation, 21–23 J jump condition, 354

384

INDEX

K kinematic tensor, 14 kinematically admissible displacement, 112, 120–123, 126–127, 131–132, 258 kinematically admissible strain, 329 kinetic energy, 19 Kirchhoff assumption, 237 Kronecker delta, 9, 23, 52 Kro¨ner approach, 282, 296 Kro¨ner model, 294, 296 L Lagrange description, 12 strain, see also Green strain, 14 lamina, 234 latent hardening, 371 lattice, 70, 350–354, 356, 363, 371, 377 left stretch tensors, 13 linear comparison composite, 320, 332–333, 335, 338–340, 343 M Mandel-Hill condition, 112 martensite-martensite interfaces, 354 martensitic microdomains, 368, 369 martensitic variant, 349–350, 356– 357, 362–364, 368–370, 378 mass density, 17, 19 material asymmetry, 218 coordinates, 16 cubic, 45, 46 isotropic, 25–26, 37, 40, 58, 61– 62, 69, 74, 83, 204, 323, 326, 328, 338, 340, 342 orthotropic, 44 transversely isotropic, 45–46 matrix cracks, 266, 268

minimum complementary energy theorem, 121 minimum potential energy theorem, 120 mocrohomogeneity, 102 modulus bulk, 187, 196–198, 201, 203– 207, 213, 219–220, 258, 307, 323 effective, 261, 268, 269, 271– 273, 277 longitudinal shear, 199 longitudinal Young’s, 199 shear, 26, 126, 162, 188, 190– 192, 198, 200–202, 204–206, 208, 218–220, 226, 233, 235, 258, 293, 307, 323–324, 327, 342 transverse bulk, 199 Young, 51, 214, 221–223, 225, 233, 240 monoclinic material, 229, 243 Mori-Tanaka Method, 163, 184 moving boundary, 359 multicoated inclusion, 204 multilayer composites, 226 Mura formula, 65 N nonlinear behavior, 280–282, 291, 319–320, 331–333, 336–337 non-perfect interface, see also imperfect interface, 113 O one-point correlation, 105–106 orientation tensors, 302 P perfect interface, 73, 245–246, 251, 257–258 perfect plasticity, 305, 309, 316 permutation tensor, 9, 37, 74

INDEX

phase transformation, 49, 53, 347– 351, 354–360, 362–364, 368– 373, 377–379 physical entity, 5, 19 plane strain, 219–220, 238, 260, 273–274 plastic behavior, 280, 305 plastic distortion, 302 plasticity, 31, 316–317, 323, 347, 379 Poisson’s ratio, 199 polar decomposition, 13 potential convex, 322, 326 dissipation, 321, 322 effective, 328 macroscopic, 319, 338 thermodynamics, 18, 20, 21, 321, 325 probability distribution function, 105 Q quadratic equation, 188, 191 quasi-static problems, 246 R reciprocal theorem, 39, 41 recrystallization, 359 reduced stiffness matrix, 235 reference conﬁguration, 14, 20, 21, 23 relaxation function, 29, 31 representative volume element, 102, 108, 197, 198, 200–201, 204, 227, 228, 229, 242, 253– 254, 283, 284, 285, 330, 350, 373, 376 resolved shear stress, 300, 302, 312, 371 right stretch tensor, 13 right stretch tensors, 13 rigid particles, 186 rotation matrix, 176

385

rotation tensor, 13, 24 rule of mixture, 223, 240 RVE, see also representative volume element, 102, 103, 108, 111, 113, 319, 324, 328, 350, 357, 359, 360, 364, 369, 378 S scalar function, 8, 18, 19 secant approach, 312, 331 compliance tensor, 314–315 moduli, 326 viscoplastic compliance, 313 second order elastic constant, 23 self-adjoint operator, 129, 145 self-consistent method, 169, 173, 184 self-equilibrium stress ﬁeld, 287 size distribution, 196 size-dependent propertiy, 183 slip plane, 62, 66, 300 slip system, 300–308, 310, 312, 325, 353, 364, 371, 377 spatial coordinates, 16 spin tensor, 14 statically admissible stress, 112, 121–124, 126–127, 134–136, 146, 149, 198, 259, 286 statistically homogeneous medium, 106, 108, 109, 113, 139, 285 steady-state creep, 282, 312 step function, 357 Stokes’ theorem, 19, 64 strain concentration tensor, 117, 166, 174, 180, 182–183, 224, 307 strain energy, 19, 23, 81–82, 112, 114–116, 122–123, 133, 135– 136, 151–152, 268–269, 273, 282, 289, 290, 336 strain hardening, 300, 303, 306, 309

386

INDEX

strain rate, 284, 295, 297–300, 302, 304–306, 312–315, 322, 325, 363, 374 stress Cauchy, 15–16, 18, 20, 22, 24, 33 deviatoric, 31, 33 ﬁrst Piola-Kirchhoff, 16 power, 20–21, 290 second Piola-Kirchhoff, 16, 23 stress concentration tensor, 118, 160, 167, 170, 174, 182, 255– 256, 287, 307 stress intensity factor, 259–261, 266 stress polarization, 80, 90–91, 127, 132–133, 135–136, 149 stress-free transformation strain, 49 stress-strain relationship, 28, 29, 31–33, 50, 234, 236, 280, 311 summary convention, 5 symbolic notation, 7, 26, 83, 129, 162–163, 168, 293 T tangent compliance tensor, 297– 299, 314–315 tangent modulus, 294–299, 305– 307, 309, 314, 327–328, 376 Taylor expansion, 23, 27, 314 Taylor-Lin model, 296, 311 tensor transformation, 24 texture, 281, 316 thermoelasticity, 26 third order elastic constant, 23 threshold strain, 276, 277 traction boundary condition, 109, 110, 118–119, 146–147, 155, 160, 169, 175, 254, 284–286, 289, 328–329 traction vector, 16, 17, 18, 246, 366 transform Fourier, 36, 37, 54, 57, 58

Laplace, 30–31 Legendre, 322 transverse matrix crack, 266, 269, 273 Tresca yield function, 33 TRIP, 347, 349–350, 379 twinning, 351–354, 356, 359 two-point correlation function, 105–106 U unit outward normal, 16, 248 unit sphere, 39, 78, 92, 93, 139 V variant, 282, 357–358, 362–364, 368, 370, 378 velocity of the interface, 361–362, 366 viscoelasticity, 29, 48 Voids, 190 Voigt elastic constant, 25, 44, 216, 220, 227, 232, 233 Volterra formula, 63 volume average, 104, 106–109, 111, 112, 284, 285 volume fraction, 103–104, 107, 117, 125–126, 137, 140, 154, 160–162, 173, 178–180, 182, 185, 188, 192, 194, 196, 197, 200–201, 205, 208, 214, 225, 228, 240, 242, 258, 261, 268, 285, 320, 342, 349, 358, 364, 367–369, 376, 378 Von Mises criterion, 323 von Mises yield function, 33 W work-hardening, 34 Y yield function, 32–33 yield surface, 32–33, 291

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

FUNDAMENTALS OF MICROMECHANICS OF SOLIDS Jianmin Qu Mohammed Cherkaoui

John Wiley & Sons, Inc.

This book is printed on acid-free paper. 嘷 ⬁ Copyright 䉷 2006 by John Wiley & Sons, Inc. All rights reserved Published by John Wiley & Sons, Inc., Hoboken, New Jersey Published simultaneously in Canada No part of this publication may be reproduced, stored in a retrieval system, or transmitted in any form or by any means, electronic, mechanical, photocopying, recording, scanning, or otherwise, except as permitted under Section 107 or 108 of the 1976 United States Copyright Act, without either the prior written permission of the Publisher, or authorization through payment of the appropriate per-copy fee to the Copyright Clearance Center, 222 Rosewood Drive, Danvers, MA 01923, (978) 750-8400, fax (978) 750-4470, or on the web at www.copyright.com. Requests to the Publisher for permission should be addressed to the Permissions Department, John Wiley & Sons, Inc., 111 River Street, Hoboken, NJ 07030, (201) 748-6011, fax (201) 748-6008, e-mail: [email protected] Limit of Liability / Disclaimer of Warranty: While the publisher and author have used their best efforts in preparing this book, they make no representations or warranties with respect to the accuracy or completeness of the contents of this book and speciﬁcally disclaim any implied warranties of merchantability or ﬁtness for a particular purpose. No warranty may be created or extended by sales representatives or written sales materials. The advice and strategies contained herein may not be suitable for your situation. You should consult with a professional where appropriate. Neither the publisher nor author shall be liable for any loss of proﬁt or any other commercial damages, including but not limited to special, incidental, consequential, or other damages. For general information on our other products and services or for technical support, please contact our Customer Care Department within the United States at (800) 762-2974, outside the United States at (317) 572-3993 or fax (317) 572-4002. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. For more information about Wiley products, visit our web site at www.wiley.com. Library of Congress Cataloging-in-Publication Data: Qu, Jianmin. Fundamentals of micromechanics of solids / Jianmin Qu, Mohammed Cherkaoui. p. cm. Includes bibliographical references. ISBN-13: 978-0-471-46451-8 (cloth) ISBN-10: 0-471-46451-1 (cloth) 1. Nanostructured materials—Mechanical properties—Textbooks. 2. Micromechanics—Textbooks. 3. Microelectromechanical systems—Materials—Textbooks. I. Cherkaoui, Mohammed. II. Title. TA418.9.N35Q22 2006 620.1⬘05—dc22 2005030781 Printed in the United States of America 10

9

8

7

6

5

4

3

2

1

To Qianqian, Bouchra, Lisa, Jalal, Rayan and Hajja-Fetouma.

CONTENTS Preface 1

Introduction

1.1 1.2 1.3 1.4

2

xiii 1

Background and Motivation / 3 Objectives / 4 Organization of Book / 4 Notation Conventions / 5 References / 9

Basic Equations of Continuum Mechanics

11

2.1 2.2 2.3 2.4 2.5

Displacement and Deformation / 11 Stresses and Equilibrium / 15 Energy, Work, and Thermodynamic Potentials / 18 Constitutive Laws / 22 Boundary Value Problems for Small-Strain Linear Elasticity / 34 2.6 Integral Representations of Elasticity Solutions / 35 Problems / 43 Appendix 2.A / 44 Appendix 2.B / 44 Appendix 2.C / 46 References / 47 Suggested Readings / 48 3

Eigenstrains

3.1 3.2 3.3

49

Deﬁnition of Eigenstrains / 49 Some Examples of Eigenstrains / 52 General Solutions of Eigenstrain Problems / 53 vii

viii

CONTENTS

3.4

4

Examples / 56 Problems / 66 Appendix 3.A / 67 Appendix 3.B / 70 References / 70 Suggested Readings / 70

Inclusions and Inhomogeneities

71

4.1 4.2 4.3

Deﬁnitions of Inclusions and Inhomogeneities / 71 Interface Conditions / 73 Ellipsoidal Inclusion with Uniform Eigenstrains (Eshelby Solution) / 77 4.4 Ellipsoidal Inhomogeneities / 84 4.5 Inhomogeneous Inhomogeneities / 88 Problems / 91 Appendix 4.A / 92 Appendix 4.B / 93 Suggested Readings / 98 5

Deﬁnitions of Effective Moduli of Heterogeneous Materials

99

5.1 5.2 5.3 5.4 5.5 5.6

Heterogeneity and Length Scales / 99 Representative Volume Element / 102 Random Media / 102 Macroscopic Averages / 108 Hill’s Lemma / 111 Deﬁnitions of Effective Modulus of Heterogeneous Media / 113 5.7 Concentration Tensors and Effective Properties / 116 Problems / 119 Suggested Readings / 119 6

Bounds for Effective Moduli

6.1

Classical Variational Theorems in Linear Elasticity / 120 6.2 Voigt Upper Bound and Reuss Lower Bound / 123

120

ix

CONTENTS

6.3 6.4

7

Determination of Effective Moduli

7.1 7.2 7.3 7.4 7.5 7.6 7.7

8

196

Composite-Sphere Model / 196 Three-Phase Model / 200 Four-Phase Model / 203 Multicoated Inclusion Problem / 204 Problems / 206 Appendix 8.A / 207 Appendix 8.B / 208 Appendix 8.C / 210 References / 211 Suggested Readings / 212

Effective Properties of Fiber-Reinforced Composite Laminates

9.1

154

Basic Ideas of Micromechanics for Effective Properties / 154 Eshelby Method / 158 Mori–Tanaka Method / 163 Self-Consistent Methods for Composite Materials / 169 Self-Consistent Methods for Polycrystalline Materials / 173 Differential Schemes / 179 Comparison of Different Methods / 183 Problems / 193 Suggested Readings / 195

Determination of the Effective Moduli—Multiinclusion Approaches

8.1 8.2 8.3 8.4

9

Extensions of Classical Variational Principles / 126 Hashin–Shtrikman Bounds / 136 Problems / 145 Appendix 6.A / 147 References / 152 Suggested Readings / 153

Unidirectional Fiber-Reinforced Composites / 214

214

x

CONTENTS

9.2 9.3 9.4

10

Brittle Damage and Failure of Engineering Composites

10.1 10.2 10.3

11

280

Eshelby’s Solution and Kro¨ner’s Model / 283 Applications / 299 Time-Dependent Behavior of Polycrystalline Materials: Secant Approach / 312 Problems / 316 References / 316

Nonlinear Properties of Composites Materials: Thermodynamic Approaches

12.1 12.2 12.3

245

Imperfect Interfaces / 245 Fiber Bridging / 259 Transverse Matrix Cracks / 266 Problems / 277 Appendix 10.A / 277 References / 278 Suggested Readings / 279

Mean Field Theory for Nonlinear Behavior

11.1 11.2 11.3

12

Effective Properties of Multilayer Composites / 226 Effective Properties of a Lamina / 234 Effective Properties of a Laminated Composite Plate / 238 Problems / 240 Appendix 9.A / 240 References / 243 Suggested Readings / 244

Nonlinear Behavior of Constituents / 321 Effective Potentials / 328 The Secant Approach / 331 Problems / 342 Suggested Readings / 345

319

xi

CONTENTS

13

Micromechanics of Martensitic Transformation in Solids

13.1

347

Phase Transformation Mechanisms at Different Scales / 350 13.2 Application: Thermodynamic Forces and Constitutive Equations for Single Crystals / 367 13.3 Overall Behavior of Polycrystalline Materials with Phase Transformation / 373 Problems / 377 References / 379 Suggested Readings / 379 Index / 381

PREFACE For many years, we have taught courses on micromechanics at our respective institutions (JQ at the Georgia Institute of Technology and MC at the University of Metz). We both felt the need for a textbook that (1) provides an integrated approach to the various topics of micromechanics, (2) covers the basic ideas of homogenization, (3) is written pedagogically for graduate and upper-level undergraduate students, (4) contains exercises problems, and (5) can be taught in a semester course. It was such a need that motivated us to start this project. We hope the book in front of you fulﬁlls these objectives. Micromechanics had ﬂourished over the past half-century. The literature is rich and diverse. Holding the book to a reasonable length prevented us from including many of the elegant results published over the years. Although we used our best judgment to cite and compile a list of references that we believe are most relevant to the text, listing such a limited number of references does not do justice to the breadth and depth of the ﬁeld. We sincerely apologize to those authors whose works were not given proper credit or were not cited. The book was developed primarily from our notes for the micromechanics courses that we have taught over the years. Our students, through their questions and comments, provided valuable input to the book. We are very grateful for their contributions. We would like to thank our colleagues at Georgia Tech for their encouragement and collaboration. It has been a great pleasure to be among such an intellectually stimulating group of people. The book was written mainly during evenings and on weekends. At times, we had to neglect our duties as husbands and fathers. We want to acknowledge that without the support of our wives and families, this project would not have been completed. Their understanding and sacriﬁces are greatly appreciated. This book is dedicated to them. JIANMIN QU Atlanta, Georgia

MOHAMMED CHERKAOUI Metz, France xiii

1 INTRODUCTION Mechanics studies the theory of forces and their interactions. It is the pillar of modern sciences. Many of the great scientists in history have been mechanicians including, for example, Aristotle, Archimedes, Leonardo da Vinci, Kepler, and Newton. Continuum mechanics is a relatively young branch of mechanics. It studies the deformation of bodies (solid or ﬂuid) under forces or stresses. Although the basic foundation of continuum mechanics was laid by Galileo, it was during the late eighteenth and the early nineteenth centuries that modern theories of continuum mechanics were gradually developed by Laplace, Fourier, Coriolis, Lagrange, Hamilton, Navier, and Cauchy, among others. It was during this period and up until the early 1900s that continuum mechanics enjoyed its most rapid development into maturity. By the mid-1900s, theories of continuum mechanics had been established upon vigorous mathematics. One of the most successful stories of continuum mechanics is the development and application of fracture mechanics. In 1913, C.E. Inglis looked at a thin plate of glass with an elliptical hole in the middle in a new and different way (Fig. 1.1). The plate was pulled at both ends perpendicular to the ellipse. He found that the stress at point A is given by

冉

A ⫽ 1 ⫹

冊

2a . b

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

1

2

INTRODUCTION

y

σ A

2b

x

2a

(a)

(b)

Figure 1.1 (a) Inglis’ work on stress concentration near an elliptical hole. (b) Grifﬁth’s work on stress concentration near a sharp crack tip.

In other words, the stress at the tip of the elliptical hole can be much larger than the stress applied. In the 1920s, A.A. Grifﬁth extended Inglis’ work. He found that the stress at the ends of the crack approaches inﬁnity: ⫽

K . 兹2x

Grifﬁth also introduced the notion of energy. He said that for a crack to grow, it was necessary for there to be enough potential energy in the system to create the new surface area of the crack. Although he did not know that it takes more than this for a crack to grow, Grifﬁth’s idea of fracture criterion laid the foundation for a brand new theory called fracture mechanics, which is one of the most celebrated branches of continuum mechanics in modern history. More importantly, fracture mechanics brought continuum mechanics and material science together and opened up new opportunities for studying not only deformation of solid bodies but also the failure behavior of solid materials under load. Thus a new ﬁeld called mechanics of materials emerged. In mechanics of material, we use the vigorous continuum mechanics theories to investigate and study how materials with certain microstructures deform and eventually fail under given loads or stresses. Micromechanics is a branch of mechanics of materials. It is the most recent development in applying continuum mechanics theories to real

1.1

BACKGROUND AND MOTIVATION

3

materials. The beginning of micromechanics may be traced back to Eshelby’s seminal study (Eshelby, 1957). But, the theory of micromechanics was not fully developed into a subject area of its own until the early 1980s. Even though it is still an actively researched area now, the theory of micromechanics has matured enough that several books have been published. Among them, the books by Mura (1986), NematNasser and Hori (1993), and Krajcinovic (1996) are probably the most comprehensive and inﬂuential ones. The theory of micromechanics of solids describes the scientiﬁc concepts, principles, and methodologies for the study of thermomechanical behavior of heterogeneous materials. Although the fundamental equations of micromechanics are based on mechanics of continuum, its applications cover a broad range of thermomechanical behavior of materials including plasticity, fracture, and fatigue, constitutive equations of composites, and polycrystalline materials. For example, it applies the theories of elasticity and plasticity to study imperfections in crystals, inclusions, and inhomogeneities in alloys and composite materials. The objective is to study the macroscopic mechanical behavior of materials from an understanding of their microstructure. This involves the application of continuum mechanics to identiﬁable small-scale structures and the use of analytical and numerical methods to compute the macroscopic responses. This science-based approach enables us to predict the behavior of new materials without the need for physical experimentation. It provides a powerful tool for engineering design, fabrication, and analysis of a wide range of materials including polycrystalline, composite, geotechnical, biological, and electronic materials. Optimum microstructures can be forecasted rather than found by trial and error. Fracture and fatigue of solids and structures, martensitic transformations, interphases in composites, and dispersion hardening of alloys are examples of the phenomena that are being elucidated and qualiﬁed by micromechanics.

1.1 BACKGROUND AND MOTIVATION

As the theory of micromechanics matures, many universities around the world are offering courses on this subject. For the past 15 years, the authors have taught micromechanics classes in their respective institutions. We have always been frustrated by not being able to ﬁnd an appropriate textbook for the course. Most existing books on this subject are research monographs, primarily for experts and researchers. They

4

INTRODUCTION

can be excellent research tools but not convenient to use as textbooks. Because the theory of micromechanics is still in its infancy, results were obtained by individual researchers using, sometime, very different approaches/methodologies. In order for the students (or ﬁrst-time learners) to understand the intrinsic connections among different concepts and approaches, a uniﬁed approach (including the use of notations) is needed to develop the micromechanics theory. This will allow both the instructor and the students to fully grasp the essence of the theory. Furthermore, instead of collecting and compiling existing results from the literature, we should identify a set of topics that convey the fundamental ideas of micromechanics and focus on these topics. Related topics not covered in the text should be referenced for those who wish to learn more. Exercise problems should be provided for the convenience of the instructor, as well as for those who wish to study the subject on their own. These are the major considerations that motivated us to write this textbook.

1.2

OBJECTIVES

The intent of this book is not to provide a comprehensive collection of results of micromechanics in the literature, nor is it to be a research reference book for relevant publications. Instead, it is intended to be a textbook for graduate and possibly upper-level undergraduate students. It is to provide a teaching tool for an instructor to teach and a learning aid for a beginner to learn (what we believe) the most fundamental ideas and approaches, the basic concepts, principles, and methodologies of micromechanics. To this end, a uniﬁed mathematical framework is introduced early on in the book. The rest of the theories will be developed based on this framework in a logical and easily understandable approach. In addition to some new results from the authors’ own research, many of the available results in the literature will be derived or re-derived based on this uniﬁed mathematical framework. This approach enables the students to follow the various developments of the micromechanics theories. It also helps the students to quickly comprehend and appreciate the wide range of applications of micromechanics.

1.3 ORGANIZATION OF BOOK

The book is organized into 13 chapters. References and/or Suggested Readings are included at the end of each chapter. Some of these ref-

1.4

NOTATION CONVENTIONS

5

erences contain certain results not derived but used in the text. Others are listed because they present either alternative approaches for the same problem or provide additional topics related to those discussed in the chapter. We have made great effort to make the book somewhat self-contained. The goal was that a reader with the basic knowledge of continuum mechanics should be able to follow this book without consulting other publications. Each chapter also contains a set of problems. The students, as well as the instructor, may ﬁnd these exercises useful. The level of difﬁculty varies signiﬁcantly among the problems. The students should not feel discouraged if they cannot solve some of the problems on their ﬁrst attempt. The reminder of this chapter presents the most frequently used notations and notation conventions used in this book. In the next chapter, a brief summary of the basic theories of continuum mechanics is presented. The rest of the chapters are grouped into linear theories (Chapters 3–10) and nonlinear theories (Chapter 11–13). 1.4 NOTATION CONVENTIONS

One of the difﬁculties many people encounter in studying micromechanics is the different kinds of notations used in the literature. For consistency, we will use the following conventions throughout this book, unless otherwise noted. Index notation for vectors and tensors will be used extensively. Whenever possible, the base letter for a vector (ﬁrst-order tensor) will be a lowercase italic letter, for a second-order tensor it will be a lowercase Greek letter, and for a fourth-order tensor it will be an uppercase italic letter. For example, ui represents a vector, ij represents a second-order tensor, and Lijkl represents a fourth-order tensor. Exceptions to these rules are certain letters conventionally used for speciﬁc physical entities. For example, Gij is for the Green function, which is a second-order tensor. The summary convention will be used:

冘冘L 3

Lijklkl ⬅

3

.

ijkl kl

(1.4.1)

l⫽1 k⫽1

Alternately, when it is convenient, the direct (or matrix) notation of vectors and tensors will be used as well. Boldface letters will be used for this purpose. For example, u represents a vector, represents a

6

INTRODUCTION

second-order tensor, and L represents a fourth-order tensor. To distinguish tensors with the same base letter a subscript will be used. For example, L1 and L2 are used to denote two different fourth-order tensors. Note that these subscripts are entirely different from the subscripts used to represent the components of a tensor. Subscripts on matrix notations do not follow the summation convention, therefore, when a tensor in the matrix notation with a subscript is written in index forms, we will change the subscript to superscript with parenthesis, for example, (2) L1 ⇔ L(1) and L2 ⇔ Lijkl . ijkl

Throughout the book, index and matrix notations will be used interchangeably based on whichever is convenient. To avoid confusion, we use the following notations to represent the tensor algebraic operations. Dot product: Double-dot product: Dyad:

ijnj ⇔ n Lijklkl ⇔ L⬊, minj ⇔ m n,

LijklTklmn ⇔ L⬊T nimj ⇔ n m

Since dot and double-dot operations will be used extensively, we will, when there is no ambiguity, neglect the dot(s) and simply write, for example, L⬊ ⇔ L and n ⇔ n. A fourth-order tensor, A, is nonsingular if and only there exists a fourth-order tensor, for example, B, such that AB ⫽ BA ⫽ I.

(1.4.2)

In this case, B is the inverse of A, or A is the inverse of B, that is, B ⫽ A⫺1

or A ⫽ B⫺1.

(1.4.3)

An equivalent deﬁnition can be given as follows: A is singular if and only if there exists a second-order tensor ⫽ 0, such that A ⫽ 0. A fourth-order isotropic tensor can be written as Aijkl ⫽ a␦ij␦kl ⫹ b(␦ik␦jl ⫹ ␦il␦jk ⫺ –32 ␦ij␦kl).

(1.4.4)

For convenience, we introduce the following two fourth order tensors:

1.4

I hijkl ⫽ –13 ␦ij␦kl,

NOTATION CONVENTIONS

d I ijkl ⫽ –12 (␦ik␦jl ⫹ ␦il␦jk ⫺ –32 ␦ij␦kl),

7

(1.4.5)

so that the fourth-order isotropic tensor given in (1.4.4) can be written as A ⫽ 3aIh ⫹ 2bId.

(1.4.6)

It can be easily shown that, if is a second-order tensor, then A ⫽ 3aI ⫹ 2b⬘,

(1.4.7)

where ⫽ kk is the spherical part of , and ⬘ij ⫽ ij ⫺ –31 kk␦ij

(1.4.8)

is the deviatoric part of . Furthermore, the following statements can be easily proven: 1. A ⫽ 3aIh ⫹ 2bId is positive deﬁnite if and only if a ⬎ 0, b ⬎ 0. 1 h 1 d I ⫹ I. 2. A⫺1 ⫽ 3a 2b 3. I ⫽ Ih ⫹ Id is the identity tensor, that is, I ⫽ AA⫺1 ⫽ A⫺1A. 4. If B ⫽ 3cIh ⫹ 2dId, then A ⫹ B ⫽ 3(a ⫹ c)Ih ⫹ 2(b ⫹ d)Id. 5. AB ⫽ BA ⫽ 9acIh ⫹ 4bdId. Additionally, we introduce another symbolic notation for fourthorder isotropic tensors: A ⫽ (3a, 2b).

(1.4.9)

The following statements can be easily proven: 1. A ⫽ (3a, 2b) is positive deﬁnite if and only if a ⬎ 0, b ⬎ 0. 1 1 , . 2. A⫺1 ⫽ 3a 2b 3. I ⫽ (1,1) is the identity tensor, that is, I ⫽ AA⫺1 ⫽ A⫺1A ⫽ (1,1). 4. If B ⫽ (3c, 2d), then A ⫹ B ⫽ (3a ⫹ 3c, 2b ⫹ 2d). 5. AB ⫽ BA ⫽ (9ac, 4bd).

冉 冊

8

INTRODUCTION

For tensor calculus, the most often used operations are the gradient and divergence. The gradient of a scalar function results in a ﬁrst-order tensor: b ⫽ ⵜƒ ⇔ bj ⫽

⭸ƒ ⬅ ƒ, j. ⭸xj

(1.4.10)

The divergence of a vector is a scalar: a ⫽ div[b] ⫽

⭸b1 ⭸b ⭸b ⫹ 2 ⫹ 3 ⇔ a ⫽ bj, j. ⭸x1 ⭸x2 ⭸x3

(1.4.11)

In the above, the notation (•), j indicates the derivative with respect to the independent variable of the function. If the function has more than one independent variable, ambiguity may arise. In this case, instead of using, for example, ƒ, j(x, y), we will use the standard notation to explicitly indicate partial derivatives, for example, ⭸ƒ(x, y) . ⭸x

(1.4.12)

The divergence of a second-order tensor becomes a vector: p ⫽ ⵜ ⇔ pi ⫽

⭸ij ⫽ ij, j. ⭸xj

(1.4.13)

For integrals, a single integral sign will be used. For line (onedimensional) integrals, the integration variable will be used for the inﬁnitesimal line element, for example, y⫽

冕 ƒ(x) dx, L

where L is the line of integration. For surface (two-dimensional) integrals, we will typically use dS for the inﬁnitesimal area element, for example, y⫽

冕 ƒ(x) dS, S

REFERENCES

9

where S is the area of integration. Here, it is implied that x is the integration variable since the integrand depends on x only. If the integrand depends on more than one independent variable, we will explicitly indicate which variable is being integrated, for example, y(z) ⫽

冕 ƒ(x, z) dS(x). S

Similarly, for volume (three-dimensional) integrals, we will use either one of the following two forms: y⫽

冕 ƒ(x) dV,

y(z) ⫽

V

冕 ƒ(x, z) dV(x). V

Finally, we introduce some special tensors. The Kronecker delta ␦ij is deﬁned by ␦ij ⫽

再

1 for i ⫽ j . 0 for i ⫽ j

(1.4.14)

And the permutation tensor ijk is deﬁned by ijk ⫽

冦

1

⫺1

0

when i, j, k are an even permutation of 1, 2, 3 when i, j, k are an odd permutation of 1, 2, 3 . when any two indices are equal (1.4.15)

For example, 123 ⫽ 231 ⫽ 312 ⫽1, 213 ⫽ 132 ⫽ 321 ⫽ ⫺1, and others are zero. The permutation tensor and the Kronecker delta ␦ij are related through the ⫺ ␦ relationship: ijkmnk ⫽ ␦im␦jn ⫺ ␦in␦jm.

(1.4.16)

REFERENCES Eshelby, J. D. (1957). The Determination of Elastic Field of an Ellipsoidal Inclusion, and Related Problems, Proc. Roy. Soc. London, Vol. A241, pp. 376–396.

10

INTRODUCTION

Krajcinovic, D. (1996). Damage Mechanics, North-Holland, New York. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff Pub., Boston. Nemat-Nasser, S. and M. Hori (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York.

2 BASIC EQUATIONS OF CONTINUUM MECHANICS In this chapter, we will introduce some basic equations of continuum mechanics. It is assumed that the readers already have had some prior knowledge of the subject. Therefore, lengthly derivations are omitted. Only equations that are needed later for deriving the micromechanics theories are outlined. For more detailed and in-depth knowledge of continuum mechanics, we refer to the References and Suggested Readings at the end of this chapter. The fundamental equations governing the deformation of continuum can be roughly classiﬁed into four categories: (1) kinematic equations that deal with the description of motion and deformation, (2) kinetic equations that deal with forces, stresses, and their equilibrium, (3) constitutive equations that describe the material’s response under load, and (4) boundary and initial conditions that are necessary to uniquely deﬁne the boundary/initial value problems. We will discuss these classes of equations separately.

2.1 DISPLACEMENT AND DEFORMATION

At any given instant of time t, a continuum having a volume V and bounding surface S will occupy a certain region R of the physical space; see Figure 2.1. When the continuum undergoes deformation, the particles (material points) within the continuum may be displaced from one spatial position to another along various paths. The displacement of a particle can be written as Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

11

12

BASIC EQUATIONS OF CONTINUUM MECHANICS

S0 X3

S

u X

x

V V0 X2 Reference X1 Configuration

x1

x3 x2

Current Configuration

Figure 2.1 Reference and current conﬁgurations.

u ⫽ x ⫺ X,

(2.1.1)

where x is the position occupied at current time t by the particle that occupied position X in the initial conﬁguration (t ⫽ 0). In some literature, x is referred to as the spatial (Eulerian) coordinate, and X is referred to as the material coordinate. This is because X can be viewed as a label attached to a material particle while x indicates where the particle is located at a give time. The current position x of a particle originally located at X in the initial conﬁguration can be expressed by xi ⫽ xi(X, t).

(2.1.2)

Clearly, the above equation provides a way to ﬁnd the new location of each particle after the deformation. This way of describing the deformation is called the Lagrangian description. On the other hand, the Eulerian description uses the following equation: XI ⫽ XI (x, t)

(2.1.3)

to keep track of which particle happens to be at the location xi at the current time t. For clarity, capital letters are used for the subscript of a tensor component associated with the Lagrangian coordinate system (the initial conﬁguration), and the lowercase letters are used for the subscript of a tensor component associated with the Eulerian coordinate system (the current or deformed conﬁguration). Such a distinction is unnecessary if both the Lagrangian and Eulerian conﬁgurations use the same coordinate system. Equations (2.1.2)–(2.1.3) may be interpreted as a mapping between the initial conﬁguration and the current conﬁguration. The continuum

2.1

DISPLACEMENT AND DEFORMATION

13

mechanics theory assumes that such mapping is sufﬁciently smooth (differentiable) and one to one, that is, the Jacobian J ⫽ 兩⭸xi / ⭸XJ兩 should not become zero at any time. Partial differentiation of (2.1.2) with respect to XJ and (2.1.3) with respect to xj yield, respectively, dxi ⫽ FiJ dXJ,

dXI ⫽ F Ij⫺1 dxj,

(2.1.4)

where FiJ ⫽

⭸xi ⭸XJ

and F⫺1 Ij ⫽

⭸XI ⭸xj

(2.1.5)

are called the material deformation gradient tensor and the spatial deformation gradient tensor, respectively. Through the polar decomposition (Malvern, 1969), the material deformation gradient tensor can be written as FiJ ⫽ RiKUKJ ⫽ Vik RkJ

(2.1.6)

where Rij is the (orthogonal) rotation tensor, and Uij and Vij are symmetric, positive deﬁnite tensors known as the right- and left-stretch tensors, respectively. Based on their deﬁnitions, a length segment dXI connecting two neighboring particles in the undeformed conﬁguration becomes a length segment dxi connecting the same two particles now in the deformed conﬁguration. The difference between the lengths (square) of these two segments, dxi dxi ⫺ dXI dXI, can be used as a measure of deformation occurring in the neighborhood of these particles when the continuum is deformed from the initial conﬁguration to the current conﬁguration, that is, dxi dxi ⫺ dXI dXI ⫽ 2EIJ dXI dXJ ⫽ 2E*ij dxi dxj,

(2.1.7)

where

冉 冉

冊 冉 冊 冉

冊 冊

EIJ ⫽

⭸uj 1 ⭸ui ⭸u ⭸u 1 ⭸xk ⭸xk ⫺ ␦IJ ⫽ ⫹ ⫹ k k 2 ⭸XI ⭸XJ 2 ⭸XJ ⭸XI ⭸XI ⭸XJ

(2.1.8)

E*ij ⫽

1 ⭸X ⭸X 1 ⭸uI ⭸uJ ⭸uK ⭸uK ␦ij ⫺ K K ⫽ ⫹ ⫺ 2 ⭸xi ⭸xj 2 ⭸xj ⭸xi ⭸xi ⭸xj

(2.1.9)

14

BASIC EQUATIONS OF CONTINUUM MECHANICS

are called the Lagrangian (Green) ﬁnite strain tensor and the Eulerian (or Cauchy) ﬁnite strain tensor, respectively. When the same coordinate system is used for both the initial reference conﬁguration and the current conﬁgurations, the strain tensors can be further written as Eij ⫽

冉

冊

⭸uj ⭸u ⭸u 1 ⭸ui ⫹ ⫹ k k , 2 ⭸Xi ⭸Xi ⭸Xi ⭸Xj

冉

冊

1 ⭸ui ⭸uj ⭸uk ⭸uk ⫹ ⫺ . 2 ⭸xi ⭸xi ⭸xi ⭸xj

E* ij ⫽

(2.1.10) When the displacement gradients are small, that is, 兩⭸ui / ⭸Xj兩 ⬍⬍ 1 and 兩⭸ui / ⭸xj兩 ⬍⬍ 1, neglecting the higher order terms leads to ⭸ui ⭸u ⭸Xk ⭸u ⫽ i ⫽ i ⭸xj ⭸Xk ⭸xj ⭸Xk

冉

␦kj ⫺

冊

⭸Xk ⭸xj

⫽

⭸ui . ⭸Xj

(2.1.11)

冊

(2.1.12)

Thus one has, from (2.1.8) and (2.1.9), that Eij ⫽

冉

冊

冉

⭸uj 1 ⭸ui ⭸uj 1 ⭸ui ⫹ ⫽ E* ⫹ ⫽ ij, ij ⫽ 2 ⭸Xi ⭸Xi 2 ⭸xi ⭸xi

where ij is called the inﬁnitesimal strain tensor. Other kinematic tensors often used in viscoelastic and plastic theories are the rate of deformation tensor and the spin tensor: Dij ⫽

冉

冊

1 ⭸vi ⭸vj ⫹ , 2 ⭸xj ⭸xi

Wij ⫽

冉

冊

1 ⭸vi ⭸vj ⫺ , 2 ⭸xj ⭸xi

(2.1.13)

where vi(x1, x2, x3, t) is the velocity ﬁeld vi ⫽

dui dxi ⫽ dt dt

expressed in terms of the Eulerian (spatial) coordinates xi. For small strain deformation,

(2.1.14)

2.2

冋 冉 冊册 冋 冉 冊

dij d 1 ⭸ui ⭸uj ⫽ ⫹ dt dt 2 ⭸xj ⭸xi ⫽

STRESSES AND EQUILIBRIUM

⫽

15

册

1 ⭸(dui /dt) ⭸(duj /dt) ⫹ 2 ⭸xi ⭸xi

1 ⭸vi ⭸vj ⫹ , 2 ⭸xj ⭸xi

that is, dij ⫽ Dij. dt

(2.1.15)

This is no longer true for ﬁnite deformation. Instead, we have (Malvern, 1969) dEIJ ⫽ FmI DmnFnJ. dt

(2.1.16)

2.2 STRESSES AND EQUILIBRIUM

The state of stress at a point in a continuum can be represented by the Cauchy stress tensor ij in the current (or deformed) conﬁguration. Note that the components of the Cauchy stress tensor are deﬁned as force per unit area in the deformed conﬁguration. Balance of the moment of momentum (Cauchy’s second law of motion) dictates the symmetry of the Cauchy stress tensor, that is, ij ⫽ ji. Furthermore, in the deformed conﬁguration, Cauchy’s ﬁrst law of motion yields the equilibrium equation ⭸ji ⫹ ƒi ⫽ 0 ⭸xj

or ⵜ ⫹ f ⫽ 0,

(2.2.1)

where ƒi is the body force per unit volume in the deformed conﬁguration. Equation (2.2.1) is valid for any material point within a continuum body. For a material point on the surface (boundary) of the a continuum (see Fig. 2.2), the following Cauchy formula applies:

16

BASIC EQUATIONS OF CONTINUUM MECHANICS

S

n p

x

x3

V x1

x2

Figure 2.2 Cauchy formula on the deformed (current) surface.

ij nj兩S ⫽ pi

or n兩S ⫽ p,

(2.2.2)

where, as shown in Figure 2.2, ni is the unit outward normal vector of the surface S and pi is the traction vector applied on S. Note that pi is measured as force per unit deformed area. Note that (2.2.1) describes the equilibrium of an inﬁnitesimal material element in the deformed conﬁguration. The Cauchy stress tensor is typically written as a function of the Eulerian spatial coordinates xi. To describe the equilibrium in the initial (undeformed) conﬁguration, the Piola–Kirchhoff stress tensors may be introduced. The ﬁrst Piola–Kirchhoff stress tensor, 0Ij, is deﬁned as the actual force in the deformed conﬁguration per unit undeformed area in the undeformed conﬁguration, while the second Piola–Kirchhoff stress tensor, ˜ IJ, is deﬁned as a ﬁctitious force in the undeformed conﬁguration per unit undeformed area in the undeformed conﬁguration. The ﬁctitious force here is obtained by transforming the actual force in the deformed conﬁguration back to the undeformed conﬁguration, which is equivalent to premultiplying the actual force in the deformed conﬁguration by the spatial deformation gradient tensor, F⫺1 Ij . Hence, the two Piola–Kirchhoff stresses are related by the deformation gradient tensors: ⫺1 0 ˜ IJ ⫽ FJk Ik

or Ij0 ⫽ ˜ IKFjK.

(2.2.3)

The Piola–Kirchhoff stresses are typically written as functions of the Lagrangian material coordinates Xi. They can be related to the Cauchy stress tensor by ⫺1 0Ij ⫽ JFIk kj,

or

⫺1 ⫺1 ˜ IJ ⫽ JFIk FJm km

(2.2.4)

2.2

ij ⫽

STRESSES AND EQUILIBRIUM

1 1 FiKFjM ⫽ ˜ KM ⫽ FiK 0Kj, J J

17

(2.2.5)

where J is the Jacobian given by J ⫽ 兩⭸xi / ⭸Xj兩 ⫽ 0 / , and 0 and are the mass density measured in the initial reference state and the current deformed state, respectively. It is seen from (2.2.4) that ˜ IJ is symmetric while 0Ij is generally nonsymmetric. It is important to keep in mind that the Piola–Kirchhoff stress tensors are not actual stresses, that is, they do not exist in the continuum under consideration. They are introduced to simplify the equilibrium equation in the initial conﬁguration, namely, ⭸ 0Ji ⫹ ƒ0 ⫽ 0 ⭸XJ

or

⭸(˜ JKFiK) ⫹ ƒ0 ⫽ 0, ⭸XJ

(2.2.6)

where ƒ0 is the body force per unit volume in the initial conﬁguration. The Cauchy formula given by (2.2.2) can also be expressed in the initial conﬁguration, 0Ji NJ ⫽ FiJ p˜ J,

˜ JI Nj ⫽ FIj⫺1 pj0,

(2.2.7)

where p0j ⫽

dS p, dS0 j

p˜ J ⫽

dS ⫺1 F p, dS0 Jk k

(2.2.8)

and dS0 is an area element in the initial conﬁguration, and dS is the same area element in the deformed conﬁguration. Note that pj is the force acting on the deformed surface per unit deformed area. Therefore, p0j is the force acting on the deformed surface per unit undeformed area, while p˜ J is a ﬁctitious force acting on the deformed surface per unit undeformed area. This ﬁctitious force is the actual force acting on 0 the deformed surface transformed by F⫺1 ˜ J is a real Jk . Neither of pj and p traction vector. They are called pseudotraction vectors introduced to accommodate the pseudostress tensors. For small deformation, that is, 兩⭸ui / ⭸XJ兩 ⬍⬍ 1 and 兩⭸ui / ⭸xj兩 ⬍⬍ 1, one can show from (2.1.5) that when the same coordinate system is used for both the Lagrangian and Eulerian conﬁgurations,

18

BASIC EQUATIONS OF CONTINUUM MECHANICS

Fij ⬇ ␦ij ⫹

⭸ui ⭸Xj

and J ⫽

冏 冏

⭸xi ⭸u ⬇ 1 ⫹ i. ⭸Xj ⭸Xj

(2.2.9)

Thus, it follows from (2.2.4) that Piola–Kirchhoff stresses reduce to the Cauchy stress, ij ⫽ ˜ ij ⫽ ij0

(2.2.10)

for small deformation. Furthermore, the distinction between ni and Ni and between dS and dS0 can also be neglected. Thus, the pseudotraction vectors reduce to the Cauchy traction vector as well.

2.3 ENERGY, WORK, AND THERMODYNAMIC POTENTIALS

We ﬁrst review some of the integral identities from mathematical physics. Consider region D bounded by the surface S. The outward unit normal vector of S is denoted by ni; see Figure 2.3. Let ƒ(x1, x2, x3) be a continuously differentiable scalar function deﬁned in D. The Green’s theorem states that

冕 ⭸⭸xƒ dV ⫽ 冕 ƒn dS. D

S

i

(2.3.1)

i

Let ui(x1, x2, x3) be a continuously differentiable vector function deﬁned in D. The divergence theorem states that

冕 ⭸⭸ux dV ⫽ 冕 u n dS i

D

i

S

i

i

or

冕 ⵜu dV ⫽ 冕 u • n dS D

(2.3.2)

S

Next consider a simple, closed, and smooth curve L. Let S be any smooth surface spanned across the closed curve. The tangential direction of the curve and the normal direction of the surface are denoted S

n

D

Figure 2.3 Region D bounded by the surface S.

2.3

ENERGY, WORK, AND THERMODYNAMIC POTENTIALS

19

by ti and ni, respectively. To get the positive orientation of L think of yourself as walking along the curve. While you are walking along the curve if your head is pointing in the same direction as the unit normal vectors of the surface while the surface is on the left, then you are walking in the positive direction on L; see Figure 2.4. Now, let ui(x1, x2, x3) be a continuously differentiable scalar function deﬁned on the surface S. The Stokes’ theorem states that

冕 u S

ijk k, j

ni dS ⫽

冕 u t dL L

i i

or

冕 (ⵜ ⫻ u) • n dS ⫽ 冕 u • t dL, S

L

(2.3.3) where ijk is the permutation symbol. Note that (2.3.1)–(2.3.3) are mathematical identities. They are true regardless of the physical interpretation of the functions involved. Nevertheless, when properly interpreted, these integral identiﬁes may be used to state the conservation of certain physical entities. Now, let us consider the energy of a continuum. Generally speaking, the total energy of a continuum is comprised of two parts, the kinetic energy and the internal energy. The kinetic energy is associated with the macroscopically observable motion of the continuum. Usually, the kinetic energy of the random thermal agitation of the atoms is considered part of the internal energy associated with the temperature of the continuum. The other part of the internal energy may include stored strain energy and possibly other forms of energy, such as chemical, electrical, and optical energies. Let be the mass density and be the internal energy per unit mass or speciﬁc internal energy for a continuum in the current (deformed) conﬁguration. The ﬁrst law of thermodynamics in conjunction with the divergence theorem leads to the following energy equation (Malvern, 1969):

n

S t

L

Figure 2.4 Stokes’ theorem.

20

BASIC EQUATIONS OF CONTINUUM MECHANICS

d ⭸q ⫽ ij Dij ⫹ r ⫺ i, dt ⭸xi

(2.3.4)

where ij is the Cauchy stress tensor, Dij is the rate of deformation tensor, r is the distributed internal heat source per unit mass, and qi is the (outward) heat ﬂux vector. The ﬁrst term on the right-hand side of (2.3.4) is called stress power. It represents the power input per unit deformed volume provided by the stress ﬁeld. The last two terms of the right-hand side represent the total heat input from internal heat source and external heat ﬂux. Together, the right-hand side of (2.3.4) gives the total energy input, while the left-hand side shows the time rate of change of internal energy. Therefore, (2.3.4) is a mathematical statement of conservation of energy. The quantity of particular interest to us is the stress power, ij Dij. In a volume V of the deformed conﬁguration, the stress power is given by

冕D V

ij

ij

dV.

(2.3.5)

This can be converted to the initial reference conﬁguration in terms of the Piola–Kirchhoff stress tensors:

冕D V

ij

ij

dV ⫽

冕

V0

0Ij

dFjI dV0 ⫽ dt

冕

V0

˜ IJ

dEIJ dV0. dt

(2.3.6)

For this reason, we call (ij, Dij) a conjugate pair in the current deformed conﬁguration, and ( 0Ij, dFjI /dt) and (˜ IJ, dEIJ /dt) conjugate pairs in the initial reference conﬁguration. In computing the energy, we must use variables that form a conjugate pair in the same conﬁguration. We are now ready to introduce the thermodynamic potentials. The fundamental assumption here is that the internal energy per unit mass of a continuum can be uniquely determined by the speciﬁc entropy s, and some state variables i, that is, ⫽ (s, 1, 2, . . . , n).

(2.3.7)

This is called the caloric equation of state, and is, therefore, a thermodynamic potential. From here, one can deﬁne the thermodynamic temperature and thermodynamic forces, respectively:

2.3

T⫽

ENERGY, WORK, AND THERMODYNAMIC POTENTIALS

冉冊 ⭸ ⭸s

冉冊

21

⭸ . ⭸i s

(2.3.8)

ds ⫽ i di ⫹ T ds.

(2.3.9)

and i ⫽

i

These yield d ⫽

冉冊 ⭸ ⭸i

di ⫹

s

冉冊 ⭸ ⭸s

i

For adiabatic (r ⫺ qi,i ⫽ 0) and isentropic (ds ⫽ 0) deformation, and for isothermal (dT ⫽ 0) deformation with reversible heat transfer (r ⫺ qi,i ⫽ T ds/dt), the work of the thermodynamic forces is recoverable, and the rate of work of the thermodynamic forces equals the stress power: i

di ⫽ ij Dij. dt

(2.3.10)

Thus, in these cases, the rate of change of the internal energy is given by

d ds ⫽ ij Dij ⫹ T . dt dt

(2.3.11)

In the reference conﬁguration, this takes the form d 1 dEIJ ds ⫽ ˜ ⫹T . dt 0 IJ dt dt

(2.3.12)

Other thermodynamic potentials used often in continuum mechanics are: Enthalpy: Helmholtz free energy: Gibbs free energy:

⫽ ⫺ ii.

h ⫽ ⫺ sT. g ⫽ ⫺ sT ⫺ ii.

(2.3.13) (2.3.14) (2.3.15)

22

BASIC EQUATIONS OF CONTINUUM MECHANICS

2.4

CONSTITUTIVE LAWS

Constitutive laws are used to describe material behavior when subjected to applied thermomechanical loads. One of the major areas of micromechanics is to develop constitutive laws for heterogeneous materials under various thermomechanical loading conditions. For real materials, their thermomechanical behavior can be rather complex. It is usually not feasible to write down one or a set of equations to describe the entire range of material behavior. Instead, we formulate separately constitutive equations describing various kinds of idealized material response, each of which is a mathematical formulation designed to approximate physical observations of a real material’s response over a suitably restricted range. Speciﬁcally, constitutive laws for ideal materials are prescribed by equations that establish the relationship between deformation and the internal stresses in the material. For example, G(ij, Dij) ⫽ 0

(2.4.1)

describes a relationship between the Cauchy stress tensor and the rate of deformation tensor. In what follows, we will describe some commonly used constitutive laws governing certain idealized material behavior. Elasticity

If there exists a potential function W of strain for a given material such that the stress in the material is related to the strain by ˜ IJ ⫽

⭸W , ⭸EIJ

(2.4.2)

then the material is called an elastic (or hyperelastic) material, and such material behavior is called elasticity. Equation (2.4.2) is the constitutive equation for elastic materials. For elastic material under isothermal and isentropic conditions, the Helmholtz free energy can be taken as the elastic potential W ⫽ 0h, that is, ˜ IJ ⫽

⭸W ⭸h ⭸ ⫽ 0 ⫽ 0 . ⭸EIJ ⭸EIJ ⭸EIJ

Thus, ˜ IJ / 0 is the thermodynamic force conjugate to EIJ.

(2.4.3)

2.4

CONSTITUTIVE LAWS

23

Another consequence of the elastic potential is that the state of deformation is uniquely determined by the state variables. In the isothermal case, the state variables are the strain components. The stress ﬁeld corresponding to a strain ﬁeld is unique regardless how that state of strain is arrived. In other words, the deformation is history independent. Consequently, upon unloading, an elastic material recovers its original state or shape and size. Since W is assumed to be a function of strain only, it can also be interpreted as the strain energy per unit undeformed volume. In the initial reference conﬁguration, the Taylor expansion of W can be written as W ⫽ W0 ⫹ cIJ EIJ ⫹ –21 LIJKLEIJ EKL ⫹ –61 cIJKLMNEIJ EKLEMN ⫹ , (2.4.4) where, traditionally, LIJKL are called the second-order elastic constants and cIJKLMN are called the third-order elastic constants. The constants W0 and cIJ are typically zero unless, for example, when residual stress exists in the initial reference conﬁguration. A material is said to behave linear elastically if the higher order terms in (2.4.4) can be neglected and the stresses are linearly related to the strains. In the undeformed conﬁguration, the constitutive equation for linear elastic materials can be written in terms of the second Piola–Kirchhoff stress tensor and the Lagrangian ﬁnite strain tensor, ˜ IJ ⫽ LIJKLEKL

or EIJ ⫽ MIJKL˜ KL,

(2.4.5)

where the fourth-order tensor LIJKL is called the elasticity (or stiffness) tensor, and MIJKL is the compliance tensor, which is the inverse of the stiffness tensor, that is, MIJMNLMNKL ⫽ IIJKL ⬅ –21 (␦IK␦JL ⫹ ␦IL␦JK),

(2.4.6)

where ␦IJ is the Kronecker delta: ␦IJ ⫽

再

1 for I ⫽ J . 0 for I ⫽ J

(2.4.7)

Most engineering materials show linear elastic behavior only when the deformation is very small. In this case, the small-strain constitutive

24

BASIC EQUATIONS OF CONTINUUM MECHANICS

law for linear elastic materials can be written in terms of the Cauchy stress tensor and the inﬁnitesimal strain tensor: ij ⫽ Lijklkl

or ij ⫽ Mijklkl.

(2.4.8)

The above equation is often referred to as the generalized Hooke law. For linear elastic materials, it is sometime convenient to write the Hooke law in terms of the Voigt elastic constants: ⫽ C,

(2.4.9)

where

⫽

冤冥 冤冥 11 22 33 , 23 31 12

⫽

11 22 33 , 223 231 212

(2.4.10)

and the elements of the 6 ⫻ 6 stiffness matrix C are called the (Voigt) elastic constants. They are related to the components of stiffness tensor L through the relationship shown in Table 2.1. Both the stiffness and compliance tensors are fourth-order tensors. They obey the tensor transformation law, Lˆ ijkl ⫽ ␣im␣jn␣kp␣lqLmnpq,

ˆ ijkl ⫽ ␣im␣jn␣kp␣lqMmnpq, M

(2.4.11)

ˆ ijkl are the components of the stiffness and compliance where Lˆ ijkl and M tensors, respectively, in the xˆ i coordinate system, which is related to the original xi coordinate system by the rotation tensor ␣ij through Table 2.1

Relationship between Lijkl and Cij

Lijkl

kl

ij

11

22

33

23

31

12

11 22 33 23 31 12

C11 C21 C31 C41 C51 C61

C12 C22 C32 C42 C52 C62

C13 C23 C33 C43 C53 C63

C14 C24 C34 C44 C54 C64

C15 C25 C35 C45 C55 C65

C16 C26 C36 C46 C56 C66

2.4

CONSTITUTIVE LAWS

xˆ i ⫽ ␣ij xj.

25

(2.4.12)

For the Voigt elasticity matrix, if the coordinate transformation is a rotation about the x3 axis by an angle , one can show that (Ting, 1996), ˆ ⫽ ⍀C⍀T, Sˆ ⫽ (⍀⫺1)T S⍀⫺1, C

(2.4.13)

where

冤

m2 n2 0 ⍀⫽ 0 0 ⫺mn

n2 m2 0 0 0 mn

0 0 0 0 0 0 1 0 0 0 m ⫺n 0 n m 0 0 0

2mn

⫺2mn

0 0 0

m2 ⫺ n2

冥

(2.4.14)

in which m ⫽ cos , n ⫽ sin . The stiffness tensor of a linear elastic material is positive deﬁnite and possesses the following symmetries: Lijkl ⫽ Lklij ⫽ Ljikl.

(2.4.15)

Because of these symmetries, there are 81 independent components called elastic constants in the most general case. The number of independent components of the stiffness tensor is much less when the material possesses certain symmetries. For example, for materials with cubic symmetry, such as face-center-cubic (FCC) and body-centercubic (BCC) crystals, the stiffness tensor has only three independent components: Lijkl ⫽ ␦ij␦kl ⫹ (␦ik␦jl ⫹ ␦il␦jk) ⫹ dijkl,

(2.4.16)

where , , and are related to the Voigt constants by ⫽ C12,

⫽ C44,

⫽ C11 ⫺ C12 ⫺ 2C44.

(2.4.17)

The symbol dijkl is deﬁned by the following: d1111 ⫽ d2222 ⫽ d3333 ⫽ 1,

others ⫽ zero.

(2.4.18)

For isotropic materials, there are only two independent components in the stiffness tensor, that is,

26

BASIC EQUATIONS OF CONTINUUM MECHANICS

Lijkl ⫽ ␦ij␦kl ⫹ (␦ik␦jl ⫹ ␦il␦jk),

(2.4.19)

where the Lame constants and are related to the Voigt constants by ⫽ C12,

⫽ C44.

(2.4.20)

In some cases, it is more convenient to rewrite (2.4.19) as Lijkl ⫽ K␦ij␦kl ⫹ (␦ik␦jl ⫹ ␦il␦jk ⫺ –23 ␦ij␦kl),

(2.4.21)

where K and are the bulk and shear moduli, respectively. The corresponding compliance tensor is given by Mijkl ⫽

1 1 ␦ij␦kl ⫹ (␦ ␦ ⫹ ␦il␦jk ⫺ –23 ␦ij␦kl). 9K 4 ik jl

(2.4.22)

Using the symbolic notation (1.4.2), the isotropic stiffness tensor and compliance tensor can be written as L ⫽ (3K, 2),

M⫽

冉

冊

1 1 , . 3K 2

(2.4.23)

Other elastic constants such as Young’s modulus, Poisson’s ratio, the shear modulus, and so forth, are also commonly used for isotropic materials. The relationships among the various elastic constants for isotropic materials are given in Appendix 2.A. The Voigt elastic constants for materials with other types of symmetries are listed in Appendix 2.B. Thermoelasticity

In addition to mechanical stresses, temperature change may also cause deformation in a continuum. Vice versa, deformation of a continuum may cause the temperature in the continuum to change. Such temperature effects in elastic materials are described by thermoelastic constitutive laws. Some commonly used thermoelastic constitutive laws are presented here. We assume that, at the temperature T0, the continuum is stress free in the initial reference state. In the deformed (current) state, let the temperature be T. The Helmholtz free energy is given by (2.3.14)

2.4

CONSTITUTIVE LAWS

27

h(EIJ, T) ⫽ (EIJ, T) ⫺ Ts(EIJ, T),

(2.4.24)

dh ⭸h dEIJ ⭸h dT d dT ds ⫽ ⫹ ⫽ ⫺s ⫺T . ⭸EIJ dt ⭸T dt dt dt dt dt

(2.4.25)

or

Making use of (2.3.12) and (2.3.11) in the above, we have

冉

s⫹

冊

⭸h ⭸T

冉

冊

dT 1 ⭸h dEIJ ⫺ ˜ IJ ⫺ ⫽ 0. dt 0 ⭸EIJ dt

(2.4.26)

Since EIJ and T are independent state variables, satisfaction of the above equation means ⭸h , ⭸T

s⫽⫺

˜ IJ ⫽ 0

⭸h . ⭸EIJ

(2.4.27)

The difference between the second of (2.4.27) and (2.4.3) is that the Helmholtz free energy in (2.4.27) is a function of both strain and temperature. The Taylor expansion of the Helmholtz free energy in terms of strains and temperature can be written as 0h ⫽ h0 ⫹ cIJ EIJ ⫹ –21 LIJKLEIJ EKL ⫹ ␣ ⌬T ⫹ –21  ⌬T 2 ⫺ ␣KLLIJKLEIJ ⌬T .

(2.4.28)

For convenience, we have used ⌬T ⫽ T ⫺ T0.

(2.4.29)

It thus follows that ⭸h 1 ⫽ ⫺ (␣ ⫹  ⌬T ⫹ ␣IJ EIJ ), ⭸T 0

s⫽⫺ ˜ IJ ⫽ 0

⭸h ⫽ cIJ ⫹ LIJKLEKL ⫺ LIJKL␣KL ⌬T . ⭸EIJ

(2.4.30)

(2.4.31)

28

BASIC EQUATIONS OF CONTINUUM MECHANICS

Equation (2.4.31) is the stress–strain relationship in thermoelasticity. The constant term cIJ is usually zero unless initial stresses are present. The fourth-order tensor LIJKL is the second-order elasticity tensor introduced in (2.4.4). The second-order tensor ␣IJ is called the linear coefﬁcient of thermal expansion. The quantity E*KL ⫽ ␣KL ⌬T

(2.4.32)

corresponds to the deformation due to temperature change. We will call it thermal strain. Note that although (2.4.31) provides the stress–strain relationship, it is not a complete description of the constitutive law for thermoelasticity. In thermoelasticity, in addition to stresses and strains, temperature is also an unknown ﬁeld quantity that needs to be solved simultaneously with the deformation. Therefore, the complete constitutive law of thermoelasticity should also include (2.4.30), which will provide the constitutive relation for heat conduction in the continuum. Such coupled deformation and temperature problems are rather difﬁcult to solve. Fortunately, in most engineering applications, the effect of deformation on the temperature ﬁeld is negligible. Therefore, one can solve for the temperature ﬁeld ﬁrst by solving the heat conduction problem independent of the deformation. Once the temperature ﬁeld is known, the only constitutive relation needed for solving the deformation problem in thermoelastic materials is (2.4.31). Such approach that decouples the heat conduction and thermoelasticity into two separate problems is often used in engineering applications. In case of small strain deformation, the linear thermoelastic stress– strain relationship can be written as ij ⫽ Lijkl(kl ⫺ *), kl

(2.4.33)

where the thermal strain *kl is given by * kl ⫽ ␣kl⌬T.

(2.4.34)

If the material is isotropic (both elastically and thermally), the elastic stiffness tensor Lijkl is given by (2.4.21), and the coefﬁcient of thermal expansion is given by ␣ij ⫽ ␣␦ij,

(2.4.35)

2.4

CONSTITUTIVE LAWS

29

where ␣ is the isotropic coefﬁcient of thermal expansion. Thus, the small-strain constitutive law for isotropic thermoelastic material can be written as ij ⫽ (K ⫺ –23 )(kk ⫺ 3␣ ⌬T)␦ij ⫹ 2ij.

(2.4.36)

Viscoelasticity

Viscoelastic constitutive laws are used to describe the time-dependent characteristics of material deformation. In this section, we will limit ourselves to small-strain deformation and linear viscoelasticity theories. In this case, a commonly used stress–strain relationship is given by

冕G t

ij(t) ⫽ Gijkl(t)kl(0) ⫹

(t ⫺ s)

ijkl

0

dkl(s) ds, ds

(2.4.37)

where ij(t) is the time-dependent strain tensor and Gijkl(t) is called the relaxation function. It has been assumed that for t ⬍ 0, both ij(t) and Gijkl(t) are zero, that is, ij(t) ⫽ 0 and Gijkl(t) ⫽ 0 for t ⬍ 0. Further, the symmetry of the stress and strain tensors implies Gijkl(t) ⫽ Gjikl(t) ⫽ Gijlk(t).

(2.4.38)

Under constant strain kj(t) ⫽ kj(0), we have dkl(t)/dt ⫽ 0. Thus, (2.4.37) reduces to ij(t) ⫽ Gijkl(t)kj(0).

(2.4.39)

This is the reason that Gijkl(t) is termed a relaxation function, for it represents the stress relaxation under constant strain. Alternative to (2.4.37), the viscoelastic stress–strain law can also be written as

冕J t

ij(t) ⫽ Jijkl(t)kl(0) ⫹

0

(t ⫺ s)

ijkl

dkl(s) ds, ds

(2.4.40)

where it has been assumed that for t ⬍ 0, both ij(t) and Jijkl(t) are zero, that is, ij(t) ⫽ 0 and Jijkl(t) ⫽ 0 for t ⬍ 0. The fourth-order tensor function Jijkl(t) is called the creep function because under constant stress kj(t) ⫽ kj(0), we have dkl(t)/dt ⫽ 0. Thus, it follows from (2.4.40) that

30

BASIC EQUATIONS OF CONTINUUM MECHANICS

ij(t) ⫽ Jijkl(t)kj(0).

(2.4.41)

Now, consider the Laplace transform ៣

ƒ(s) ⫽

冕

⬁

ƒ(t)e⫺st dt.

(2.4.42)

0

Note that

冕 冋冕 ƒ(t ⫺ s)g(s) ds册e ⬁

t

0

0

⫺st

冕

⬁

0

៣

៣

dt ⫽ ƒ(s)g(s),

dg(s) ⫺st ៣ e dt ⫽ sg(s) ⫺ g(0). ds

(2.4.43)

(2.4.44)

Applying the Laplace transform to both sides of (2.4.37)–(2.4.40) and making use of the above equations, we obtain ៣ ៣ ៣ ij(t) ⫽ sGijkl(s) kl(s)

៣ ៣ ៣ ij(t) ⫽ sJ ijkl(s)kl(s).

and

(2.4.45)

It thus follows that ៣

៣

sGijkl(s) ⫽ [sJ ijkl(s)]⫺1.

(2.4.46)

We see that, in the Laplace transform space, (2.4.45) is very similar to the linear elastic constitutive law (Hooke’s law). The function ៣ sGijkl(s) can be viewed as the ‘‘stiffness tensor’’ of the viscoelastic ៣ material in the Laplace transform space, while sJ ijkl(s) is the ‘‘compliance tensor.’’ Note that it is generally not true that Gijkl(t) ⫽ [Jijkl(t)]⫺1, although one can show that (Christensen, 1982) lim Gijkl(t) ⫽ lim [Jijkl(t)]⫺1 t→0

t→0

and

lim Gijkl(t) ⫽ lim [Jijkl(t)]⫺1. t→⬁

t→⬁

(2.4.47) When the material is isotropic, the relaxation and creep functions can be written as

2.4

CONSTITUTIVE LAWS

31

Gijkl(t) ⫽ –13 [Gb(t) ⫺ Gs(t)] ⫹ –12 Gs(t)(␦ik␦jl ⫹ ␦il␦jk),

(2.4.48)

Jijkl(t) ⫽ –31 [Jb(t) ⫺ Js(t)] ⫹ –21 Js(t)(␦ik␦jl ⫹ ␦il␦jk),

(2.4.49)

where Gs(t) and Gb(t) are, respectively, the shear and bulk relaxation functions, while Js(t) and Jb(t) are the shear and bulk creep functions, respectively. Making use of the above in (2.4.37) and (2.4.40), respectively, leads to ⬘ij(t) ⫽ Gs(t)⬘ij(0) ⫹

冕 G (t ⫺ s) d⬘ds(s) ds,

(2.4.50)

kk(t) ⫽ Gb(t)kk(0) ⫹

冕 G (t ⫺ s) dds(s) ds,

(2.4.51)

⬘ij(t) ⫽ Js(t)ij(0) ⫹

冕 J (t ⫺ s) dds⬘(s) ds,

(2.4.52)

kk(t) ⫽ Jb(t)kk(0) ⫹

冕 J (t ⫺ s) dds(s) ds.

(2.4.53)

t

ij

s

0

t

kk

b

0

and t

0

ij

s

t

kk

0

b

In the Laplace transform space, these stress–strain relationships can be written as ៣ ៣ ៣ ⬘ij(s) ⫽ sGs(s) ⬘kl(s),

៣ ៣ ៣ kk(s) ⫽ sGb(s) kk(s)

(2.4.54)

៣ ៣ ៣ ⬘ij(s) ⫽ sJ s(s)⬘ij(s),

៣ ៣ ៣ ⬘kk(s) ⫽ sJ b(s)⬘kk(s),

(2.4.55)

and

៣

៣

where ⬘ij(s) and ij⬘ (s) are the deviatoric strain and deviatoric stress tensors in the Laplace transform space, respectively, Plasticity

For many engineering materials, particularly, metallic materials, deformation becomes permanent once the strain goes beyond the elastic

32

BASIC EQUATIONS OF CONTINUUM MECHANICS

limit. Although the mechanisms causing such permanent deformation are rather complex, the macroscopic behavior can be approximately represented by certain functions called elastic-plastic constitutive laws. More detailed and in-depth discussions of elastic-plastic constitutive laws will be given in Chapters 11–13. Here, we will only outline the basic ideas of some commonly used constitutive laws for idealized elastic-plastic materials. For a material to be plastically deformed, certain combinations of the stress components, called the effective stress, must be larger than a threshold value, which is typically called the yield strength of the material. When the effective stress is below the yield strength, the material behaves linear elastically, and the linear elastic constitutive law can be used. When the effective stress is above the yield strength, the material behaves plastically, and elastic-plastic constitutive laws are needed to describe the postyield behavior. Thus, elastic-plastic constitutive laws typically consist of a yield criterion and a function to describe the postyield stress–strain relationship. The latter is called the ﬂow rule; for plastic deformation it is called historically plastic ﬂow. It is assumed that, for a given state of a material, there exists a function ƒ(ij) called the yield function such that the material behaves elastically if ƒ(ij) ⬍ 0,

or

ƒ(ij) ⫽ 0

and

⭸ƒ dij ⬍ 0, ⭸ij dt

(2.4.56)

and the material behaves plastically if ƒ(ij) ⫽ 0

and

⭸ƒ dij ⱖ 0. ⭸ij dt

(2.4.57)

The above yield criterion can be understood as follows. The equation ƒ(ij) ⫽ 0 deﬁnes a yield surface in the stress space. It is one of the basic assumptions in plasticity that the yield surface is a closed concave surface enclosing the origin of the stress space. Therefore, we can speak of its inside and outside. For a stress state inside the yield surface, we have ƒ(ij) ⬍ 0. The stress is not high enough to yield the material yet, and the deformation is elastic. When the stress state reaches the yield surface, that is, ƒ(ij) ⫽ 0, the situation is not unique. It depends on whether, at the next moment, the stress state is moving out of or moving back inside the yield surface. Note that ⭸ƒ/ ⭸ij is an outward (not

2.4

CONSTITUTIVE LAWS

33

necessarily unit) vector of the yield surface, and dij /dt is the direction of stress increment. Therefore, (⭸ƒ/ ⭸ij)(dij /dt) ⱖ 0 means that the direction of stress increment at the next moment is moving out of the yield surface, thus plastic yielding occurs. On the other hand, (⭸ƒ/ ⭸ij)(dij /dt) ⬍ 0 means that the stress state is moving back inside the yield surface; thus the deformation is elastic. The most commonly used yield functions are the von Mises yield function ƒ(ij) ⫽ J2 ⫺ k2,

(2.4.58)

and the Tresca yield function ƒ(ij) ⫽ 4J 23 ⫺ 27J 32 ⫺ 36J 22 ⫹ 96k4J2 ⫺ 64k6,

(2.4.59)

where k is a material constant (yield strength in pure shear), and J2 ⫽ –21 ⬘ijij⬘ ,

J3 ⫽ –31 ⬘ij⬘jk⬘ki,

(2.4.60)

are called, respectively, the second and third invariants of the deviatoric stress tensor ⬘ij ⫽ ij ⫺ –31 kk␦ij.

(2.4.61)

For other types of yield functions, the readers are referred to the References and Suggested Reading at the end of this chapter. Among the many ﬂow rules for postyield behavior, the simplest one is the Levy–Mises perfectly plastic constitutive law. It assumes that postyield deformation is incompressible and fully characterized by the rate of deformation tensor, which is related to the deviatoric Cauchy stress tensor through ⬘ij ⫽

k兹2 兹DmnDmn

Dij,

Dkk ⫽ 0.

(2.4.62)

Together, the yield conditions (2.4.56) and (2.4.57) and the postyield stress–strain relationship (2.4.62) form a constitutive law to describe mechanical behavior of an elastic–perfectly plastic material. Note that such simple constitutive law is rather limited in its application to real engineering materials because (1) it assumes that plastic deformation

34

BASIC EQUATIONS OF CONTINUUM MECHANICS

does not produce any volume change (incompressibility), and (2) it assumes no work hardening. More realistic constitutive laws for elasticplastic materials will be discussed in Chapters 10–13.

2.5 BOUNDARY VALUE PROBLEMS FOR SMALL-STRAIN LINEAR ELASTICITY

For the remaining part of this chapter, we will focus on linear elastic material under small-strain deformation. As discussed in previous sections, the distinction between the reference and current conﬁgurations can be neglected when the deformation is small. Therefore, for such small deformation, we will not distinguish the different types of stress and strain measures, nor do we need to distinguish the spatial coordinate from the material coordinate. Instead, for convenience, we will simply use ij for stress and ij for strain, and xi for coordinates. Now, consider a continuum of volume V and surface S (see Fig. 2.5). The total surface S may be divided into S ⫽ Su ⫹ S , where it is assumed that the displacements are prescribed on Su and the traction is prescribed on S , that is, ui兩Su ⫽ u (0) i

(2.5.1)

ij nj兩S ⫽ p(0) i ,

(2.5.2)

where u (0) and p i(0) are given values of displacement and traction on Su i and S , respectively. Within the domain V, the stress must satisfy the equilibrium equation (2.2.1),

Sσ

n V

Su

Figure 2.5 An elastic body V in the undeformed conﬁguration.

2.6

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

ji, j ⫹ ƒi ⫽ 0

in V

35

(2.5.3)

where ƒi is the body force per unit volume. Combining (2.5.1), (2.5.2), and (2.5.3) in conjunction with Hooke’s law, we arrive at the following boundary value problem: ji, j ⫹ ƒi ⫽ 0

in V,

(2.5.4)

ij ⫽ Lijkluk,l

in V,

(2.5.5)

ui兩Su ⫽ u i(0),

(2.5.6)

ij nj兩S ⫽ p(0) i .

(2.5.7)

This is a well-posed boundary value problem with nine unknowns (six stress components plus three displacement components) and nine equations. Theoretically speaking, for a given set of functions u (0) and p i(0) i on S, and a given function ƒi in V, the stresses and displacements in V can be uniquely determined by solving the above boundary value problem. In most cases, numerical methods by computers are needed to obtain the solutions. Making use of Hooke’s law, the stress tensor can be eliminated from the above boundary value problem. Thus we have alternatively, Lijkluk,lj ⫹ ƒi ⫽ 0

in V,

(2.5.8)

ui兩Su ⫽ u i(0),

(2.5.9)

Lijkluk,lnj兩S ⫽ p(0) i .

(2.5.10)

2.6 INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

Let us ﬁrst consider a boundary value problem in an unbounded domain V comprised of a homogeneous linear elastic material with elasticity tensor Lijkl. We assume that the body force ƒi is localized, that is, ƒi → 0

as x 21 ⫹ x 22 ⫹ x 23 → ⬁.

and the entire boundary (at inﬁnity) is traction free, that is,

(2.6.1)

36

BASIC EQUATIONS OF CONTINUUM MECHANICS

Lijkluk,lnj兩S ⫽ pi(0) → 0

as x 21 ⫹ x 22 ⫹ x 23 → ⬁.

(2.6.2)

Under these conditions, the displacement ui should satisfy the following boundary value problem: Lijkluk,lj ⫹ ƒi ⫽ 0 ui → 0

in V,

as x 12 ⫹ x 22 ⫹ x 32 → ⬁.

(2.6.3) (2.6.4)

Several approaches can be used to solve this problem. We will use the Fourier transform method. The one-dimensional Fourier transform is deﬁned by the following integrals: gˆ () ⫽

1 2

g(x) ⫽

冕

⬁

⫺⬁

冕

⬁

g(x)e⫺ix dx,

gˆ ()eix d,

⫺⬁

(2.6.5)

(2.6.6)

where i ⫽ 兹⫺1 and gˆ () is used to denote the Fourier transform of g(x). In three-dimensional space, the Fourier transform may be deﬁned by the following pair of integrals: gˆ () ⫽

冕

⬁

1 (2)3

g(x) ⫽

⫺⬁

冕

⬁

⫺⬁

g(x)e⫺ix dx

gˆ ()eix d

(2.67)

(2.6.8)

where x ⫽ (x1, x2, x3),

⫽ (1, 2, 3),

(2.6.9)

and the integrals in (2.6.7) and (2.6.8) are over the entire threedimensional space, while dx and d are volume elements in the x space and the space, respectively. If g(x) → 0 as 兩x兩 → ⬁, then by integration by parts, we have

2.6

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

1 (2)3

冕

⬁

⫺⬁

⭸g(x) ⫺ix e dx ⫽ ijgˆ (). ⭸xj

37

(2.6.10)

Next, multiply both sides of (2.5.8) by e⫺ix /(2)3 and integrate: Lijkl

再

1 (2)3

冕

⬁

⫺⬁

冎

uk,lj(x)e⫺ix dx ⫹

1 (2)3

冕

⬁

⫺⬁

ƒi(x)e⫺ix dx ⫽ 0. (2.6.11)

Since ui vanishes at inﬁnity, (2.6.10) can be used in (2.6.11) to yield Lijkl(il)(ij)ˆuk() ⫹ ƒˆ i() ⫽ 0,

(2.6.12)

where uˆ k and ƒˆ i are the Fourier transforms of and uk and ƒi, respectively. Equation (2.6.12) can also be written as Kikuˆ k ⫽ ƒˆ i,

(2.6.13)

where the dependence of uˆ k and ƒˆ i on is implied without writing it out explicitly as an argument, and Kik ⫽ Kik() ⫽ Lijkllj.

(2.6.14)

It then follows from (2.6.13) that uˆ i ⫽ ƒˆ j Nij()/D(),

(2.6.15)

Nij() ⫽ –21 ikljmnKkm()Kln(),

(2.6.16)

D() ⫽ mnlKm1()Kn2()Kl3(),

(2.6.17)

where

and ijk is the permutation tensor introduced in (1.4.15). Note that Nij is the cofactor of Kij and D is the determinant of Kij. Therefore, Nij /D is the inverse of Kij. Expressions of Nij and D for isotropic, cubic, and transversely isotropic materials are given in Appendix 2.C. Equation (2.6.15) means that uˆ i is known explicitly as a function of once the stiffness tensor L and the body force f are known. The

38

BASIC EQUATIONS OF CONTINUUM MECHANICS

displacement in the physical space (the x space) can be obtained by taking the inverse transform of (2.6.15),

冕

⬁

ui(x) ⫽

⫺⬁

ƒˆ i() ⫽

ƒˆ j()Nij()D⫺1()eix d,

冕

⬁

1 (2)3

⫺⬁

ƒi(x)e⫺ix dx.

(2.6.18)

(2.6.19)

The corresponding stresses can then be obtained by substituting (2.6.18) into (2.4.8): ij(x) ⫽ i

冕

⬁

⫺⬁

ƒˆ m()LijklNkm()lD⫺1()eix d.

(2.6.20)

Equations (2.6.18) and (2.6.20) are integral representations of the displacements and stresses on V. An alternative form of (2.6.18) can be obtained by substituting (2.6.19) into (2.6.18): ui(x) ⫽

冕

⬁

ƒj(y)G⬁ij (x, y) dy,

⫺⬁

(2.6.21)

where G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij()D⫺1()ei(x⫺y) d.

(2.6.22)

The second-order tensor function G ⬁ij given in (2.6.22) is called the Green’s function in an unbounded elastic domain. One can easily show that G ⬁ij is a solution to the following problem: Lijkl

⭸2G⬁km(x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl⭸xj

G⬁ij (x, y) → 0

as 兩x兩 → ⬁,

(2.6.23) (2.6.24)

where ␦(x) is the three-dimensional Dirac delta function. Physically, the Green’s function is the displacement ﬁeld generated by a unit force. Since the domain is homogeneous and unbounded, only the difference between the x point (where the displacement is measured) and the y

2.6

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

39

point (where the unit force is applied) determines the Green function, that is, G⬁ij (x, y) ⫽ Gij⬁(x ⫺ y).

(2.6.25)

Additionally, by using the reciprocal theorem, it can be easily shown that G⬁ij (x, y) ⫽ Gij⬁(x ⫺ y) ⫽ Gji⬁(y ⫺ x) ⫽ Gji⬁(y, x).

(2.6.26)

It then follows that ⭸G⬁ij (x, y) ⭸Gij⬁(x, y) ⫽⫺ . ⭸xi ⭸yi

(2.6.27)

Recall that Nij() and D⫺1() are homogeneous polynomials of degree 4 and 6, respectively, with respect to , we have Nij(⫺)D⫺1(⫺) ⫽ Nij()D⫺1(). Therefore, by changing to ⫺, we can write (2.6.22) in a slightly different form: G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij()D⫺1()e⫺i(x⫺y) d.

(2.6.28)

Furthermore, the volume element in the space can be written as ˆ ˆ ), d ⫽ d1 d2 d3 ⫽ 2 d dS(

(2.6.29)

where ⫽ 兩兩 ⫽ 兹 21 ⫹ 22 ⫹ 23,

ˆ ⫽ , 兩兩

(2.6.30)

ˆ ˆ ) is a surface element on the unit sphere in the space. Thus, and dS( the integral in (2.6.22) can be converted to

G⬁ij (x, y) ⫽

1 (2)3

冕 冋冕 N ()D ⬁

2

0

Sˆ

ij

⫺1

册

ˆ ˆ ) d. ()ei(x⫺y) dS(

(2.6.31)

The homogeneity of degree zero of 2Nij()D⫺1() with respect to leads to

40

BASIC EQUATIONS OF CONTINUUM MECHANICS

2Nij(ˆ )D⫺1(ˆ ) ⫽ Nij(ˆ )D⫺1(ˆ ).

(2.6.32)

It thus follows from (2.6.31) that Gij⬁(x, y) ⫽

1 (2)3

冕 冋冕 N (ˆ )D ⬁

Sˆ

0

⫺1

ij

册

ˆ ˆ ˆ ) d. (ˆ )ei(x⫺y) dS(

(2.6.33)

Following the same procedure, we can rewrite (2.6.28) into Gij⬁(x, y) ⫽

1 (2)3

冕 冋冕 N (ˆ )D 0

⫺⬁

Sˆ

⫺1

ij

册

ˆ ˆ ˆ ) d. (ˆ )ei(x⫺y) dS(

(2.6.34)

Adding these two expressions together gives

冕 冋冕 N (ˆ )D (ˆ )e dS(ˆ ˆ )册 d 1 冕 冋冕 e d册 N (ˆ )D (ˆ ) dS(ˆ ˆ ). ⫽ 2(2)

G⬁ij (x, y) ⫽

⬁

1 2(2)3

⫺⬁

Sˆ

⬁

3

⫺⬁

Sˆ

ij

⫺1

ˆ i(x⫺y)

ˆ i(x⫺y)

ij

⫺1

(2.6.35)

Making use of the following identity in the above expression,

冕

⬁

⫺⬁

ˆ ei(x⫺y) d ⫽ 2␦[ˆ (x ⫺ y)],

(2.6.36)

we have G⬁ij (x, y) ⫽

1 8 2

冕 ␦[ˆ (x ⫺ y)]N (ˆ )D Sˆ

ij

⫺1

ˆ ˆ ). (ˆ ) dS(

(2.6.37)

The integral representations (2.6.18) and (2.6.37) will be used in the following chapters to derive the Eshelby solution. For isotropic materials, D() ⫽ 2( ⫹ 2) 6,

(2.6.38)

Nij() ⫽ 2{( ⫹ 2)␦ij 2 ⫺ ( ⫹ )ij}.

(2.6.39)

The integral in (2.6.37) can be evaluated to yield the Green’s function for isotropic material:

2.6

G⬁ij (x, y) ⫽ ⫽

41

INTEGRAL REPRESENTATIONS OF ELASTICITY SOLUTIONS

再

冎

␦ij 1 1 ⭸2兩x ⫺ y兩 ⫺ 4 兩x ⫺ y兩 4(1 ⫺ v) ⭸xi⭸xj

1 16(1 ⫺ v)兩x ⫺ y兩

再

(3 ⫺ 4v)␦ij ⫹

冎

(xi ⫺ yi)(xj ⫺ yj) . 兩x ⫺ y兩2 (2.6.40)

The integral representations discussed above are the general solutions to problems deﬁned in an unbounded domain. When the problem domain is ﬁnite, the integral representations will need to include the boundary contributions. In this case, the Green’s function approach is often used. Let us consider the boundary value problem stated by (2.5.8)–(2.5.10). To account for the boundary conditions, we deﬁne the Green’s function by the following equations: Lijkl

⭸2Gkm(x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl ⭸xj

Lijkl

in V.

(2.6.41)

Gij(x, y)兩x僆Su ⫽ 0,

(2.6.42)

⭸Gkm(x, y) nj兩x僆S ⫽ 0. ⭸xl

(2.6.43)

Again, by using the reciprocal theorem, it can be easily shown that Gij(x, y) ⫽ Gji(y, x).

(2.6.44)

Multiplying (2.6.41) by ui(x) and integrating the results over the volume V lead to

冕 u (x)L V

i

ijkl

⭸2Gkm(x, y) dV(x) ⫹ um(y) ⫽ 0. ⭸xl⭸xj

(2.6.45)

By using the divergence theorem, we can write the volume integral in (2.6.45) as

42

BASIC EQUATIONS OF CONTINUUM MECHANICS

冕 u (x)L ⭸ G⭸x ⭸(x,x y) dV(x) ⭸G (x, y) ⫽ 冕 u (x)L n dS(x) ⫺ 冕 u (x)L ⭸x 2

km

i

V

ijkl

l

j

km

i

S

ijkl

j

V

l

i, j

ijkl

⭸Gkm(x, y) dV(x). ⭸xl

(2.6.46) Analogously, multiplying (2.5.8) by Gim(x, y) and integrating the result over the volume V lead to

冕 G (x, y)L im

V

u (x) dV(x) ⫹

ijkl k,lj

冕 G (x, y)ƒ (x) dV(x) ⫽ 0. V

im

i

(2.6.47)

Following the procedures that led to (2.6.46), the ﬁrst volume integral in the above equation can be written as

冕 G (x, y)L u (x) dV(x) ⭸G (x, y) ⫽ 冕 G (x, y)L u (x)n dS(x) ⫺ 冕 L ⭸x V

im

ijkl k,lj

im

S

im

ijkl k,l

j

u (x) dV(x).

ijkl k,l

V

j

(2.6.48) Note that the last volume integral on the right-hand side of (2.6.46) is the same as that of (2.6.48). Therefore, by subtracting (2.6.45) from (2.6.47), we arrive at um(y) ⫽

冕 G (x, y)L u (x)n dS(x) ⫹ 冕 G (x, y)ƒ (x) dV(x) ⭸G (x, y) ⫺ 冕 u (x)L n dS(x). (2.6.49) ⭸x S

im

ijkl k,l

j

V

im

i

km

S

i

ijkl

j

l

Enforcing the boundary conditions (2.6.42) and (2.6.43) and (2.5.9) and (2.5.10) in the above, we ﬁnally arrive at the solution to the boundary value problem (2.5.8)–(2.5.10) in terms of the Green’s function Gij(x, y),

PROBLEMS

um(y) ⫽

43

冕 G (x, y)ƒ (x) dV(x) ⫹ 冕 G (x, y)p (x) dS(x) ⭸G (x, y) ⫺ 冕 u (x)L n dS(x). (2.6.50) ⭸x im

V

Su

i

S

0 i

im

km

0 i

ijkl

j

l

By making use of (2.6.44), the above can be written equivalently as ui(x) ⫽

冕 G (x, y)ƒ (y) dV(y) ⫹ 冕 G (x, y)p (y) dS(y) ⭸G (x, y) ⫺ 冕 u (y)L n dS(y). ⭸y im

V

Su

m

0 m

S

0 m

im

ik

mjkl

j

(2.6.51)

l

PROBLEMS

2.1 If for any function ƒ(x) that is continuous at x ⫽ 0

冕

⬁

⫺⬁

ƒ(x)␦(x) dx ⫽ ƒ(0),

then ␦(x) is called the Dirac delta function. Prove the following properties: x␦(x) ⫽ 0,

␦(ax) ⫽

1 ␦(x), a

␦(⫺x) ⫽ ␦(x).

2.2 Show that the Green’s function G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij()D⫺1()ei(x⫺y) d

satisﬁes the following boundary value problem: ⬁ LijklGlm,ik (x, y) ⫹ ␦jm␦(x ⫺ y) ⫽ 0,

G⬁ij (x, y) → 0

as 兩x兩 → ⬁,

44

BASIC EQUATIONS OF CONTINUUM MECHANICS

where ␦(x) is the three-dimensional Dirac delta function deﬁned by

冕

Vr

␦(x) dV ⫽ 1,

where Vr is any spherical volume x 21 ⫹ x 22 ⫹ x 23 ⫽ r 2. 2.3 Show (2.6.26) and (2.6.27). APPENDIX 2.A RELATIONSHIP AMONG ELASTIC CONSTANTS OF ISOTROPIC MATERIALS

E, v

E, G

K, v

K, G

,

E

E

E

3(1 ⫺ 2 v)K

v

v

⫺1 ⫹

9K 1 ⫹ 3K / G 1 ⫺ 2G / 3K 2 ⫹ 2G / 3K

(3 ⫹ 2 / ) 1 ⫹ / 1 2(1 ⫹ / )

3(1 ⫺ 2 v)K 2(1 ⫹ v)

G

K

K

⫹

G K

E 2(1 ⫹ v) E 3(1 ⫺ 2 v) Ev (1 ⫹ v)(1 ⫺ 2v) E 2(1 ⫹ v)

E 2G

G E 9 ⫺ 3E / G E(1 ⫺ 2G / E) 3 ⫺ E/G G

v

3Kv 1⫹v 3(1 ⫺ 2v)K 2(1 ⫹ v)

K⫺

2G 3

2 3

G

APPENDIX 2.B VOIGT ELASTIC CONSTANTS FOR MATERIALS WITH VARIOUS SYMMETRIES Orthotropic Materials (nine indepenent constants)

冤

C11 C12 C13 C⫽ 0 0 0

C12 C22 C23 0 0 0

C13 0 C23 0 C33 0 0 C44 0 0 0 0

0 0 0 0 C55 0

冥

0 0 0 0 0 C66

APPENDIX 2.B

VOIGT ELASTIC CONSTANTS

45

Transversely Isotropic Materials (ﬁve independent constants)

冤

C11 C12 C13 C⫽ 0 0 0

C12 C11 C13 0 0 0

C13 0 C13 0 C33 0 0 C44 0 0 0 0

0 0 0 0 C44 0

冥

0 0 0 0 0

0.5(C11 ⫺ C12)

for axis of symmetry in the x3 direction, and

冤

C11 C12 C12 C⫽ 0 0 0

C12 C22 C23 0 0 0

C12 0 0 C23 0 0 C22 0 0 0 0.5(C22 ⫺ C23) 0 0 0 C44 0 0 0

冥

0 0 0 0 0 C44

for axis of symmetry in the x1 direction. Cubic Materials (three independent constants)

冤

C11 C12 C12 C⫽ 0 0 0

C12 C11 C12 0 0 0

C12 0 C12 0 C11 0 0 C44 0 0 0 0

0 0 0 0 C44 0

冥

0 0 0 0 0 C44

Isotropic Materials (two independent constants)

C⫽

冤

C11 C12 C12 0 0 0

C12 C11 C12 0 0 0

冥

C12 0 0 0 C12 0 0 0 C11 0 0 0 0 0.5(C11 ⫺ C12) 0 0 0 0 0.5(C11 ⫺ C12) 0 0 0 0 0.5(C11 ⫺ C12)

46

BASIC EQUATIONS OF CONTINUUM MECHANICS

APPENDIX 2.C

EXPRESSIONS OF Nij() AND D()

Transversly Isotropic Materials

D() ⫽ (␣⬘2 ⫹ ␥ 32){␣␥4 ⫹ (␣ ⫹ ␥2 ⫺ ␥⬘2)2 32 ⫹ ␥ 34} ⫽ (␣⬘2 ⫹ ␥ 23){(␥2 ⫹  23)(␣2 ⫹ ␥ 23) ⫺ ␥⬘22 32},

N11() ⫽ (␣⬘ 21 ⫹ ␣ 22 ⫹ ␥ 23)(␥2 ⫹  32) ⫺ ␥⬘2 22 32, N12() ⫽ ␥⬘212 32 ⫺ (␣ ⫺ ␣⬘)12(␥2 ⫹  32), N13() ⫽ (␣ ⫺ ␣⬘)␥⬘1 223 ⫺ ␥⬘13(␣⬘ 12 ⫹ ␣ 22 ⫹ ␥ 32), N22() ⫽ (␣ 12 ⫹ ␣⬘ 22 ⫹ ␥ 32)(␥2 ⫹  32) ⫺ ␥⬘2 12 32, N23() ⫽ (␣ ⫺ ␣⬘)␥⬘ 2123 ⫺ ␥⬘23(␣ 21 ⫹ ␣⬘ 22 ⫹ ␥ 23), N33() ⫽ (␣ 12 ⫹ ␣⬘ 22 ⫹ ␥ 32)(␣⬘ 12 ⫹ ␣ 22 ⫹ ␥ 32) ⫺ (␣ ⫺ ␣⬘)2 12 22, where ␣ ⫽ C11 ⫽ C22,  ⫽ C33,

␣⬘ ⫽ C66 ⫽ –12 (C11 ⫺ C12), ␥⬘ ⫺ ␥ ⫽ C13 ⫽ C23,

␥ ⫽ C44 ⫽ C55,

2 ⫽ 12 ⫹ 22.

Cubic Materials

D() ⫽ 2( ⫹ 2 ⫹ ⬘) 6 ⫹ ⬘(2 ⫹ 2 ⫹ ⬘) 2( 21 22 ⫹ 22 23 ⫹ 23 21) ⫹ ⬘2(3 ⫹ 3 ⫹ ⬘) 12 22 32,

N11() ⫽ 2 4 ⫹  2( 22 ⫹ 32) ⫹ ␥ 22 32, N12() ⫽ ⫺( ⫹ )12( 2 ⫹ ⬘ 23),

REFERENCES

47

and the other components are obtained by the cyclic permutation of 1, 2, 3, where 2 ⫽ ii,  ⫽ ( ⫹ ⫹ ⬘), ␥ ⫽ ⬘(2 ⫹ 2 ⫹ ⬘), ⫽ C12, ⫽ C44, ⬘ ⫽ C11 ⫺ C12 ⫺ 2C44. Isotropic Materials

D() ⫽ 2( ⫹ 2) 6, Nij() ⫽ 2{( ⫹ 2)␦ij 2 ⫺ ( ⫹ )ij}, where 2 ⫽ kk. Also LjlmnlNij()D⫺1() ⫽ ( ⫹ 2)⫺1⫺4{␦mni 2 ⫹ ( ⫹ 2)␦imn 2 ⫹ ( ⫹ 2)␦inm 2 ⫺ 2( ⫹ )mni}, ⫺1 LijklLpqmnqlNkp()D () ⫽ ( ⫹ 2)⫺1⫺4{2␦ij␦mn 4 ⫹ 2␦mnij 2 ⫹ 2␦ijmn 2 ⫹ ( ⫹ 2)(␦imjn ⫹ ␦jmin ⫹ ␦injm ⫹ ␦jnim) 2 ⫺ 4( ⫹ )ijmn}.

REFERENCES Christensen, R. M. (1982). Theory of Viscoelasticity—An Introduction, 2nd ed., Academic Press, New York. Malvern, L. E. (1969). Introduction to the Mechanics of Continuous Medium, Prentice-Hall, Englewood Cliffs, NJ. Ting, T. C. T. (1996). Anisotropic Elasticity—Theory and Applications, Oxford University Press, New York.

48

BASIC EQUATIONS OF CONTINUUM MECHANICS

SUGGESTED READINGS Fung, Y. C. (1965). Foundations of Solid Mechanics, Prentice-Hall, Englewood Cliffs, NJ. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Dordrecht.

3 EIGENSTRAINS In this chapter, we will ﬁrst deﬁne what eigenstrain is and give some examples of it. Then, we will derive the general solutions to the displacements, stresses, and strains when an eigenstrain ﬁeld is present in a linear elastic solid.

3.1

DEFINITION OF EIGENSTRAINS

Eigenstrain is a generic name introduced in micromechanics to represent inelastic strains such as thermal strains, phase transformation strains, initial strains, plastic strains, misﬁt strains, and the like. In the literature, other names have been used for eigenstrains by various authors, such as stress-free transformation strains by Eshelby and elastic polarization strains by Kro¨ner. In this book, we will use the term eigenstrain to represent any inelastic strains. For small-strain deformation, we will use the following notation convention: ij ⫽ total strain,

eij ⫽ elastic strain, ij* ⫽ eigenstrain (inelastic).

When both elastic strain and eigenstrain coexist in a continuum, the total strain is given by the sum Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

49

50

EIGENSTRAINS

ij ⫽ eij ⫹ ij*.

(3.1.1)

The above equation implies that both the elastic strain and eigenstrain act together to cause a material point in the continuum to displace from its initial location to its ﬁnal location in the deformed conﬁguration. The ﬁnal position of the material particle after the deformation determines the total strain, that is, the total strain is related to the displacement through [see (2.1.12)] ij ⫽ –21 (ui, j ⫹ uj,i),

(3.1.2)

where ui is the total displacement ﬁeld cause by both the elastic strain and the eigenstrain. Although the total strain can be separated into elastic and inelastic parts, it is not always possible to separate the displacement into elastic and inelastic parts. So, we will not introduce the concepts of elastic displacement and eigen displacement. Therefore, it is unnecessary to use ‘‘total’’ for the displacement. It will be understood that displacement ui is always the total displacement caused by both strains. For sufﬁciently smooth displacement ﬁelds, the total strain tensor satisﬁes Saint Venant’s compatibility conditions: Rij ⫽ ikpjlqpq,kl ⫽ 0,

(3.1.3)

where ijk is the permutation symbol deﬁned by (1.4.15). Note that it is only the total strain, or the sum of the elastic strain and eigenstrain, that must be compatible, that is, satisfying the compatibility condition (3.1.3). The elastic strain and the eigenstrain by themselves alone do not have to be compatible. In fact, we will see in later examples that they often are not compatible by themselves. Another way of saying, for example, that the eigenstrain ﬁeld is not compatible is that there is no differentiable function u* i such that 1 * ij ⫽ – 2 (u* i, j ⫹ u*). j,i

(3.1.4)

Or, equivalently, one can say that R*ij ⫽ ikpjlq*pq,kl ⫽ 0. Let us now consider Hooke’s law when eigenstrains are present. As discussed in Chapter 2, Hoooke’s law describes the stress–strain relationship for linear elastic materials. In other words, it relates the stress to the elastic strain in a linear elastic material. When eigenstrain is

3.1

DEFINITION OF EIGENSTRAINS

51

present in a linear elastic material, the total strain is given by (3.1.1). Thus the elastic strain is the difference between the total strain and eigenstrain: eij ⫽ ij ⫺ ij*. Consequently, Hooke’s law should be written as ij ⫽ Lijklekl ⫽ Lijkl(kl ⫺ *), kl

(3.1.5)

eij ⫽ ij ⫺ *ij ⫽ Mijklkl.

(3.1.6)

or

The interpretation of (3.1.5) is that the stress in a linear elastic material is caused only by elastic strain. If there is no elastic strain, there would be no stress. For this reason, we do not introduce the concept of eigenstress in this book. As a simple example to understand (3.1.5), let us consider the uniaxial tension of a metal bar. A typical uniaxial stress–strain curve is shown in Figure 3.1. The eigenstrain in this case is the plastic strain p while the elastic strain is e. Clearly, we have the total strain ⫽ p ⫹ e. It is clearly seen from this ﬁgure that ⫽ Ee ⫽ E( ⫺ p). In other words, the stress is the elastic constant (Young’s modulus) times the elastic strain, which is the difference between the total strain and the eigenstrain.

σ

E

εp

E

εe

ε

Figure 3.1 Uniaxial stress–strain curve.

52

EIGENSTRAINS

3.2 SOME EXAMPLES OF EIGENSTRAINS

First, consider an aluminum ball of radius a at temperature T0. When the temperature is raised to T, the ball expands. It follows from (2.4.34) that the thermal strain is given by * ij ⫽ ␣A ⌬T ␦ij,

(3.2.1)

where ␣A is the coefﬁcient of thermal expansion for aluminum, ␦ij is the Kronecker delta, and ⌬T ⫽ T ⫺ T0 is the temperature change. Since there is no constraint to the ball, no stress is induced by the temperature rise. Thus, it follows from (3.1.6) that the elastic strain is zero, that is, eij ⫽ ij ⫺ *ij ⫽ Mijklkl ⫽ 0.

(3.2.2)

Consequently, the eigenstrain in this case is equal to the total strain: ij ⫽ eij ⫹ * * ⫽ ␣A ⌬T ␦ij. ij ⫽ ij

(3.2.3)

We see that thermal strain is an eigenstrain. Next, let the aluminum ball be embedded in a rigid matrix at temperature T0. Then, raise the temperature to T. In this case, the total strain of the aluminum ball is zero because of the rigid constraint. This means that ij ⫽ eij ⫹ * ij ⫽ eij ⫹ ␣A ⌬T ␦ij ⫽ 0,

(3.2.4)

eij ⫽ ⫺ij* ⫽ ⫺aA ⌬T ␦ij.

(3.2.5)

or

It is seen that the elastic strain is no longer zero due to the constraint. Because of the nonzero elastic strain, the stress in the aluminum ball is also nonzero. It is given by Hooke’s law: ij ⫽ Lijklekl ⫽ ⫺␣ALnnij ⌬T.

(3.2.6)

This stress could be very large. For example, for polycrystalline aluminum (isotropic), (3.2.6) can be simpliﬁed to

3.3

GENERAL SOLUTIONS OF EIGENSTRAIN PROBLEMS

E␣A ij ⫽ ⫺ ⌬T ␦ij, 1 ⫺ 2

53

(3.2.7)

where for aluminum E ⫽ 71 ⫻ 109 Pa,

␣A ⫽ 24 ⫻ 10⫺6 / ⬚C,

v ⫽ 0.3.

Therefore, the thermally induced stress is ij ⬇ 4.3 MPa

⌬T ␦. ⬚C ij

(3.2.8)

So, a temperature change of 10⬚ Celsius would cause 43 MPa stress! Finally, let us assume that the aluminum ball is embedded in a copper matrix at temperature T0. Again, let the temperature be raised to T. In this case, the total strain is given by ij ⫽

再

eAij ⫹ ␣A ⌬T ␦ij eCij ⫹ ␣C ⌬T ␦ij

in the Al ball in the Cu matrix

(3.2.9)

where ␣C is the coefﬁcient of thermal expansion of copper. Since the shell is deformable, the total strain is not zero in the aluminum ball, nor is it zero in the copper matrix. The thermally induced stresses cannot be obtained easily in this case; see Problem 3.2. Nevertheless, we know that stresses are induced due to the mismatch between the thermal expansion coefﬁcients. The above examples show that thermal strain is a type of eigenstrain. Other types of eigenstrains include plastic strain, phase transformation strain, and the like. 3.3 GENERAL SOLUTIONS OF EIGENSTRAIN PROBLEMS

Consider an unbounded elastic body, V, on which an eigenstrain ﬁeld * ij is prescribed. Without the body force, the equations of equilibrium is given by ij, j ⫽ 0

in V

(3.3.1)

Because of the eigenstrains, Hooke’s law takes the form of (3.1.5), that is,

54

EIGENSTRAINS

ij ⫽ Lijklekl ⫽ Lijkl(kl ⫺ *), kl

(3.3.2)

where ij is the total strain. Since the total strain must be compatible, we have ij ⫽ –21 (ui, j ⫹ uj,i),

(3.3.3)

where ui is the total displacement. Next, making use of (3.3.3) in (3.3.2) and the symmetry of the stiffness tensor, we obtain ij ⫽ Lijkluk,l ⫺ Lijkl*. kl

(3.3.4)

Substitution of (3.3.4) into (3.3.1) yields Lijkluk,lj ⫺ Lijkl*kl, j ⫽ 0

in V.

(3.3.5)

This is the governing equation for the total displacement ﬁeld in V. We further assume that the radiation condition is also satisﬁed, that is, ui → 0

as 兩x兩 → ⬁.

(3.3.6)

This condition implies that the nonzero eigenstrain can only be distributed over a ﬁnite domain within V. Comparing (3.3.5) and (3.3.6) to (2.6.3) and (2.6.4), we conclude that the solution to the eigenstrain problem can be obtained from the elasticity solution if the body force ƒi in the elasticity solution is replaced by ⫺Lijklkl, * j. To this end, consider the boundary value problem stated by (2.6.3) and (2.6.4). Assuming that the body force is given by the eigenstrain ƒi ⫽ ⫺Lijkl*kl, j,

(3.3.7)

then, through integration by parts, the Fourier transform of ƒi can be written as ƒˆ i() ⫽

⫺1 (2)3

冕

⬁

⫺⬁

Lijkl*kl, j(x)e⫺i䡠x dx ⫽ ⫺ijLijklˆ *, kl

where ˆ kl* is the Fourier transform of the eigenstrain *(x): kl

(3.3.8)

3.3

GENERAL SOLUTIONS OF EIGENSTRAIN PROBLEMS

ˆ *( kl ) ⫽

1 (2)3

冕

⬁

⫺⬁

⫺i䡠x *(x)e dx. kl

55

(3.3.9)

Substituting (3.3.8) into (2.6.18), we obtain the solution to the boundary value problem stated by (3.3.5) and (3.3.6): ui(x) ⫽ ⫺i

冕

⬁

⫺⬁

Ljlmnˆ *mn()l Nij()D⫺1()ei䡠x d.

(3.3.10)

The corresponding strain tensor is ij(x) ⫽

1 2

冕

⬁

⫺⬁

Lklmnˆ *mn()l[l Nik() ⫹ iNjk()]D⫺1()ei䡠x d.

(3.3.11)

The stress tensor thus follows from (3.3.4):

再冕

ij(x) ⫽ Lijkl

⬁

⫺⬁

冎

Lpqmnˆ mn * ()lqNkp()D⫺1()ei䡠x d ⫺ ij*(x) . (3.3.12)

An alternative approach is to use Green’s function. By substituting (3.3.7) into (2.6.21), we obtain

冕

⬁

ui(x) ⫽ ⫺

⫺⬁

⬁ Lmjkl*kl, j(y)Gmi (x, y) dy,

(3.3.13)

where G⬁mi(x, y) is the inﬁnite domain Green’s function given in (2.6.22). Applying divergence theorem to (3.3.13) yields ui(x) ⫽

冕

⬁

⫺⬁

Lmjkl*(y) kl

⭸G⬁mi(x, y) dy. ⭸yj

The corresponding strain and stress ﬁelds are

(3.3.14)

56

EIGENSTRAINS

ij(x) ⫽

再冕

⬁

ij(x) ⫽ Lijkl

⫺⬁

冕

⬁

⫺⬁

Lklmn⌫⬁ijkl(x ⫺ y)*mn(y) dy,

(3.3.15)

冎

⬁ Lpqmnmn * (y)⌫klpq (x ⫺ y) dV(y) ⫺ kl*(x) ,

(3.3.16)

where the fourth-order tensor ⌫⬁ijkl(x, y) is given by ⌫⬁ijkl(x, y) ⫽

冋

册

1 ⭸2Gki⬁ (x, y) ⭸2G⬁kj(x, y) ⭸2Gli⬁(x, y) ⭸2Glj⬁(x, y) ⫹ ⫹ ⫹ . 4 ⭸xj ⭸yl ⭸xi ⭸yl ⭸xj ⭸yk ⭸xi ⭸yk (3.3.17)

For future reference, we deﬁne PVijkl(x) ⫽

冕⌫ V

⬁ ijkl

(x, y) dV(y),

(3.3.18)

where the superscript V indicates that the integral is over the volume V. 3.4 EXAMPLES Straight-Screw Dislocation

Consider the straight-screw dislocation in a cubic crystal shown in Figure 3.2. The eigenstrain corresponding to this screw dislocation is given by

x3 x2

x1

Figure 3.2 Straight-screw dislocation.

3.4

EXAMPLES

1 * 23 ⫽ – 2 b␦(x2)H(⫺x1),

57

(3.4.1)

where b is the Burgers vector of the dislocation. The Fourier transform of *23 is easily calculated from (3.3.9):

冕 12 b␦(x )H(⫺x )e dx b ⫽ 冕 H(⫺x )e dx 冕 e 2(2) ⬁

1 (2)3

* 23() ⫽

2

⫺⬁

⬁

3

1

⫺⬁

1

⫺i1x1

⫺i䡠x

⬁

1

⫺i3x3

⫺⬁

dx3.

(3.4.2)

Note that

冕

⬁

⫺⬁

冕

H(⫺x1)e⫺i1x1 dx1 ⫽

⬁

⫺⬁

⫺1 , i1

e⫺i3x3 dx3 ⫽ 2␦(3).

(3.4.3)

(3.4.4)

We have b ␦(3) . 2(2)2 i1

ˆ * 23() ⫽ ⫺

(3.4.5)

Substitution of (3.4.5) into (3.3.10) and use of the properties of delta function yield

冕 L b ⫽ 冕 冕 (2)

ui(x) ⫽

b (2)2

2

⬁

⫺⬁

jl23

⬁

⬁

⫺⬁

⫺⬁

␦(3) N ()D⫺1()ei䡠x d 1 l ij ⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 d1 d2. 1 l Nij()D ()e

(3.4.6)

For materials with cubic symmetry, the integrand in (3.4.6) is simpliﬁed to ⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 0, 1 l N1j()D ()e

(3.4.7)

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 0, 1 l N2j()D ()e

(3.4.8)

58

EIGENSTRAINS

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 1 l N3j()D ()e

2 ei(1x1⫹2x2). 1( ⫹ 22) 2 1

(3.4.9)

Therefore, we have u1(x) ⫽ u2(x) ⫽ 0,

(3.4.10)

and u3(x) ⫽

b (2)2

冕

⬁

⫺⬁

冉冊

2 b x ei(1x1⫹2x2) d1 d2 ⫽ tan⫺1 2 . 2 1( ⫹ 2) 2 x1 2 1

(3.4.11) The only nonzero strain component is the shear strain: 23 ⫽

1 ⭸u3 b x1 ⫽ . 2 2 ⭸x2 4 x 1 ⫹ x 32

(3.4.12)

It follows from Hooke’s law for cubic materials (2.4.12) that the only nonzero stress component is the shear stress: 23 ⫽ 2C4423 ⫽

C44b x1 . 2 2 x 1 ⫹ x 23

(3.4.13)

These results are identical to those obtained by Burgers in 1939 for isotropic materials. Straight-Edge Dislocation

Consider a straight-edge dislocation in a cubic material as shown in Figure 3.3. The eigenstrain corresponding to this dislocation is given by 1 * 12 ⫽ – 2 b␦(x2)H(⫺x1),

(3.4.14)

where again, b is the Burgers vector of the dislocation. We are to ﬁnd the corresponding displacements and stresses. Following the procedures used in deriving (3.4.5), the Fourier transform of 12 * is easily calculated from (3.3.9):

3.4

x2

EXAMPLES

59

x1

x3

Figure 3.3 Straight-edge dislocation.

12 * () ⫽

1 (2)3

冕

⬁

1 b ␦(3) b␦(x2)H(⫺x1)ei䡠x dx ⫽ ⫺ . 2 2(2)2 i1

⫺⬁

(3.4.15)

Substitution of (3.4.15) into (3.3.10) and use of the properties of the delta function yield

冕 L b ⫽ 冕 冕 (2)

ui(x) ⫽

b (2)2

2

⬁

⫺⬁

jl12

⬁

⬁

⫺⬁

⫺⬁

␦(3) N ()D⫺1()ei䡠x d 1 l ij ⫺1 i䡠x (Ljl12⫺1 )兩3⫽0 d1 d2. 1 l Nij()D ()e

(3.4.16)

For materials with cubic symmetry, the integrand in (3.4.16) is simpliﬁed to ⫺1 i䡠x (Ljl12⫺1 )兩3⫽0 ⫽ 1 l N1j()D ()e

ei(1x1⫹2x2)2( 12 ⫹ 22 ⫺ ␣ 12) , 1[( 12 ⫹ 22)2 ⫹  12 22] (3.4.17)

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 1 l N2j()D ()e

ei(1x1⫹2x2)( 21 ⫹ 22 ⫺ ␣ 22) , ( 21 ⫹ 22)2 ⫹  21 22

⫺1 i䡠x (Ljl23⫺1 )兩3⫽0 ⫽ 0, 1 l N3j()D ()e

where

(3.4.18) (3.4.19)

60

EIGENSTRAINS

2 ⫹ 2 ⫹ , ⫹ 2 ⫹

␣⫽

⫽

␣ .

(3.4.20)

Therefore, we have u3(x) ⫽ 0

(3.4.21)

and u1(x) ⫽

b (2)2

u2(x) ⫽

冕 冕

b (2)2

⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2( 21 ⫹ 22 ⫺ ␣ 21) d1 d2, 1[( 12 ⫹ 22)2 ⫹  12 22]

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)( 12 ⫹ 22 ⫺ ␣ 22) d1 d2. ( 12 ⫹ 22)2 ⫹  12 22

(3.4.22)

(3.4.23)

The nonzero strain components are 11 ⫽

⭸u1 ib ⫽ ⭸x1 (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2( 12 ⫹ 22 ⫺ ␣ 12) d1 d2, [( 12 ⫹ 22)2 ⫹  12 22] (3.4.24)

22 ⫽

⭸u2 ib ⫽ ⭸x2 (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2( 12 ⫹ 22 ⫺ ␣ 22) d1 d2, ( 12 ⫹ 22)2 ⫹  12 22] (3.4.25)

12 ⫽ ⫽

冉

冊

1 ⭸u1 ⭸u2 ⫹ 2 ⭸x2 ⭸x1 ib 2(2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)[( 21 ⫹ 22)2 ⫺ 2␣ 12 22]) d1 d2. 1[( 21 ⫹ 22)2 ⫹  21 22] (3.4.26)

In terms of the integrals deﬁned in Appendix 3.A, these strains can be written as

3.4

61

ib [(1 ⫺ ␣)I1 ⫹ I2], (2)2

(3.4.27)

ib ⫽ [I1 ⫹ (1 ⫺ ␣)I2], (2)2

(3.4.28)

ib ⫽ [I3 ⫺ (2␣ ⫹ )I1], 2(2)2

(3.4.29)

11 ⫽

22 ⫽

12 ⫽

EXAMPLES

where I1, I2, and I3 are given in Appendix 3.A. For isotropic materials, ⫽ 0, ⫽ 2v /(1 ⫺ 2v). Thus, ␣⫽

1

 ⫽ 0.

, 1⫺v

(3.4.30)

The nonzero displacement components in this case are simpliﬁed to u1(x) ⫽

b (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)

冋

册

2 ␣ ⫺ 2 2 12 2 d1 d2, 2 1( ⫹ 2) ( 1 ⫹ 2) 2 1

(3.4.31) u2(x) ⫽

b (2)2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)

冋

1

12 ⫹ 22

⫺

册

␣ 22 d1 d2. ( 21 ⫹ 22)2

(3.4.32) Making use of the integrals given in Appendix 3.B, we arrive at the displacement components for isotropic materials: u1(x) ⫽

u2(x) ⫽

冋 冋

冉冊

册

b x 1 x1x2 2 tan⫺1 2 ⫹ , 4 x1 1 ⫺ v x 21 ⫹ x 22

册

b x 22 1 ⫺ 2v ⫺ log(x 21 ⫹ x 22) . 2 4 (1 ⫺ v) x 1 ⫹ x 22 2

(3.4.33)

(3.4.34)

The corresponding strain components are obtained by taking the derivatives of the displacements:

62

EIGENSTRAINS

11 ⫽

⭸u1 ⫺bx2[x 12(3 ⫺ 2v) ⫹ x 22(1 ⫺ 2v)] ⫽ , ⭸x1 4 (1 ⫺ v)(x 12 ⫹ x 22)2

(3.4.35)

22 ⫽

⭸u2 ⫺bx2[x 12(1 ⫹ 2v) ⫺ x 22(1 ⫺ 2v)] ⫽ , ⭸x2 4 (1 ⫺ v)(x 12 ⫹ x 22)2

(3.4.36)

12 ⫽

1 ⭸u1 ⭸u2 bx1(x 12 ⫺ x 22) ⫹ ⫽ . 2 ⭸x2 ⭸x1 4 (1 ⫺ v)(x 12 ⫹ x 22)2

冉

冊

(3.4.37)

The corresponding stresses are obtained by using Hooke’s law for isotropic materials: 11 ⫽

⫺b x2(3x 12 ⫹ x 22) , 2 (1 ⫺ v)(x 21 ⫹ x 22)2

(3.4.38)

22 ⫽

b x2(x 21 ⫺ x 22) , 2 (1 ⫺ v)(x 21 ⫹ x 22)2

(3.4.39)

12 ⫽

b x1(x 21 ⫺ x 22) . 2 (1 ⫺ v)(x 21 ⫺ x 22)2

(3.4.40)

These are the classic solutions for a straight-edge dislocation. Dislocation of General Nature

Consider a dislocation loop L inside a crystalline material as shown in Figure 3.4. Let the area of the slip plane be denoted by S. To describe the slip caused by the dislocation, one side of the slip plane is labeled S⫹ and the other side is labeled S⫺. The slip is a result of S⫹ moving relative to S⫺ by a Burgers vector b. The unit normal vector of S⫹

S+

S−

b n L

Figure 3.4 Dislocation of general nature.

3.4

EXAMPLES

63

pointing to S⫺ is denoted by n. The eigenstrain corresponding to such a dislocation loop can then be written as *(x) ⫽ ⫺–12 (binj ⫹ bjni)␦(S ⫺ x), ij

(3.4.41)

where ␦(S ⫺ x) is called the surface Dirac delta function deﬁned by ␦(S ⫺ x) ⫽

冕 ␦(x ⫺ z) dS(z).

(3.4.42)

S

It can be easily shown that for any continuous function deﬁned in the volume V that contains the surface S, the surface Dirac delta function satisﬁes the following:

冕 ƒ(x)␦(S ⫺ x) dV(x) ⫽ 冕 ƒ(x) dS(x). V

(3.4.43)

S

Substituting (3.4.41) into (3.3.14) and making use of (3.4.43), we obtain the displacement ﬁeld due to the dislocation loop L, 1 ui(x) ⫽ ⫺ 2

冕

⬁

⫺⬁

Lmjkl(bk nl ⫹ bl nk)␦(S ⫺ y)

冕L

⫽⫺

S

mjkl bk nl

⭸G⬁mi(x, y) dy ⭸yj

⭸G⬁mi(x, y) dS(y). ⭸yj

(3.4.44)

Upon using the properties of Green’s function (2.6.27), the above equation can be written as ui(x) ⫽

冕L S

mjkl bk nl

⭸G⬁mi(x, y) dS(y). ⭸xj

(3.4.45)

This is the well-known Volterra formula. The displacement gradient thus follows from the Volterra formula: ui, j(x) ⫽

冕L S

mnkl

bk nl

⭸G⬁mi(x, y) dS(y). ⭸xn ⭸xj

The stress caused by the dislocation loop L is thus given by

(3.4.46)

64

EIGENSTRAINS

ij ⫽ Lijkl(kl ⫺ *) kl ⫽ Lijkluk,l ⫺ Lijkl*. kl

(3.4.47)

Note that Lijkl*kl ⫽ ⫺–12 Lijkl(bk nl ⫹ bl nk)␦(S ⫺ x) ⫽ ⫺Lijkl bk nl␦(S ⫺ x).

(3.4.48)

Introducing (3.4.48) into (3.4.47) yields ij ⫽ Lijkl[uk,l ⫹ bk nl␦(S ⫺ x)] ⫽ Lijklkl,

(3.4.49)

冕L

(3.4.50)

where ij ⫽

S

mnkl

bk nl

⭸2G⬁mi(x, y) dS(y) ⫹ binj␦(S ⫺ x) ⭸xn ⭸xj

is called the elastic distortion. We next show that the surface integral in (3.4.50) can be converted to a line integral along the dislocation loop. To this end, consider the following line integral along the dislocation loop:

冕

L

jnh pqmn

L

⭸G⬁ip(x, y) bmth dL(y), ⭸xq

(3.4.51)

where th is the tangential unit vector along the dislocation loop. Making use of the Stokes’ theorem (2.3.3),

冕 L

⭸G⬁ip(x, y) bmth dL(y) ⭸xq

L

jnh pqmn

冕

⫽⫺

S

klhjnhLpqmn

⭸G⬁ip(x, y) bmnk dS(y), ⭸xq ⭸xl

(3.4.52)

where the negative sign is due to the properties of Green’s function (2.6.27). Using the ⫺ ␦ relationship (1.4.16), the right-hand side of (3.4.52) can be written as

3.4

冕

⫺

S

⭸G⬁ip(x, y) bmnk dS(y) ⭸xq ⭸xl

klhjnhLpqmn

冕 冉L

⫽⫺

⭸G⬁ip(x, y) ⭸G⬁ip(x, y) bmnj ⫺ Lpqmn bmnn ⭸xq ⭸xn ⭸xq ⭸xj

pqmn

S

EXAMPLES

冊

65

dS(y). (3.4.53)

Since

Lpqmn

⭸G⬁ip(x, y) ⫹ ␦mi␦(x ⫺ y) ⫽ 0, ⭸xq ⭸xn

(3.4.54)

we can simplify (3.4.53) to

冕

⫺

L

klh jnh pqmn

S

⭸G⬁ip(x, y) bmnk dS(y) ⭸xq ⭸xl

⫽ binj␦(S ⫺ x) ⫹

冕L S

pqmn

⭸G⬁ip(x, y) bmnn dS(y). ⭸xq ⭸xj

(3.4.55)

Comparison of (3.4.55) and (3.4.50) leads to

冕

ij ⫽ ⫺

S

klhjnhLpqmn

⭸G⬁ip(x, y) bmnk dS(y). ⭸xq ⭸xl

(3.4.56)

It then follows from (3.4.52) that

冕L ⫽冕

ij ⫽

S

L

mnkl bk nl

L

jnh pqmn

⭸2G⬁mi(x, y) dS(y) ⫹ binj␦(S ⫺ x) ⭸xn ⭸xj ⭸G⬁ip(x, y) bmth dL(y). ⭸xq

(3.4.57)

This is known as the Mura formula (Mura, 1987). The stress ﬁeld thus follows from (3.4.49):

66

EIGENSTRAINS

ij ⫽ Lijkl

冕 L

lnhLpqmn

⭸G⬁kp(x, y) bmth dL(y). ⭸xq

(3.4.58)

The fact that the stress ﬁeld is represented as a line integral along the dislocation loop indicates that the stress depends only on the loop, not the slip plane area S.

PROBLEMS

3.1 Consider a composite bar (one dimensional) whose ends are ﬁxed on rigid walls as shown in Figure 3.5. When the temperature is T0, the interface between Al and Cu is at the middle x ⫽ L/2. Please ﬁnd the position of the interface when the temperature is raised to T ⬎ T0. Assume the Young’s moduli and the thermal expansion coefﬁcients of Al and Cu are, respectively, Ea, Ec, ␣a, and ␣c. 3.2 Consider a spherical aluminum ball embedded in a copper matrix of inﬁnite extent at temperature T. When the temperature rises by ⌬T, ﬁnd the stress ﬁelds in both the ball and the matrix. 3.3 Consider a Cu water pipe in your house. Assuming the pipe has an outer diameter of 2.54 cm with wall thickness of 1 mm. Is it safe to expose this pipe to ⫺20⬚C with water in it? If the required factor of safety is 3, what is the lowest temperature this water pipe can stand? The properties of Cu and ice are given below.

Cu Ice

Young’s Modulus

Poisson’s Ratio

CTE

Tensile Strength

125 GPa 9.5 GPa

0.33 0.33

17 ⫻ 10⫺6 / ⬚C ⫺50 ⫻ 10⫺6 / ⬚C

70 MPa N/A

L /2

L /2

Al

Cu

x

Figure 3.5

APPENDIX 3.A

67

APPENDIX 3.A

We introduce the following integrals:

冕 冕 ⫽冕 冕

I1 ⫽

⬁

⬁

⫺⬁

⫺⬁

⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2)2 12 d d [( ⫹ 22)2 ⫹  12 22] 1 2 2 1

ei(1x1⫹2x2)1 22 d d , [( 12 ⫹ 22)2 ⫹  12 22] 1 2

冕 冕 ⫽冕 冕

I2 ⫽

⬁

⬁

⫺⬁

⫺⬁

⬁

⬁

⫺⬁

⫺⬁

I3 ⫽

(3.A.1)

ei(1x1⫹2x2) 32 d d ( 12 ⫹ 22)2 ⫹  12 22 1 2 ei(1x1⫹2x2) 31 d d , ( 12 ⫹ 22)2 ⫹  12 22 1 2

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

ei(1x1⫹2x2) d1 d2. 1

(3.A.2)

(3.A.3)

Let us consider (3.A.3) ﬁrst. Making use of the well-known integrals,

冕

⬁

⫺⬁

冕

⬁

ei2x2 d2 ⫽ 2␦(x2),

ei1x1 d1 ⫽ i sgn(x1), 1

(3.A.4)

ei1x1 d1 ⫽ 2i2␦(x2)sgn(x1). 1

(3.A.5)

⫺⬁

we can reduce (3.A.3) to I3 ⫽

冕

⬁

⫺⬁

ei2x2 d2

冕

⬁

⫺⬁

To evaluate the other integrals, we introduce the polar coordinate systems x1 ⫽ r cos ,

x2 ⫽ r sin ,

1 ⫽ cos ,

The above integrals can then be written as

2 ⫽ sin .

68

EIGENSTRAINS

冕 冕

I1 ⫽

2

⬁

0

0

I2 ⫽

eircos(⫺) sin cos2 d d, [1 ⫹  cos2 sin2 ]

冕 冕 2

⬁

0

0

(3.A.6)

eircos(⫺) sin3 d d. [1 ⫹  cos2 sin2 ]

(3.A.7)

冕

(3.A.8)

Next, consider the integral I⫽

⬁

0

eircos(⫺) d.

Making use of the expansion

冘 i J (r)cos[k( ⫺ )],

(3.A.9)

冘 i J (r)cos[k( ⫺ )]冊 d.

(3.A.10)

eircos(⫺) ⫽ J0(r) ⫹ 2

⬁

k

k

k⫽1

we have I⫽

冕

⬁

0

冉

J0(r) ⫹ 2

⬁

k

k

k⫽1

where Jk(●) is the Bessel function of order k. Since

冕

⬁

0

1 Jk(r) d ⫽ , r

for any k ⱖ 0 and r ⬎ 0,

(3.A.11)

we obtain

冉 冘 i cos[k( ⫺ )]冊 1 ⫽ 冉1 ⫹ 2 冘 i [cos(k)cos(k) ⫹ sin(k)sin(k)]冊. r

I⫽

1 1⫹2 r

⬁

k

k⫽1 ⬁

k

k⫽1

Substituting (3.A.12) into (3.A.6)–(3.A.7) yields

(3.A.12)

APPENDIX 3.A

I1 ⫽ I2 ⫽

69

2 r

冘 i [a

cos(k) ⫹ b1k sin(k)],

(3.A.13)

k⫽0

2 r

冘 i [a

cos(k) ⫹ b2k sin(k)],

(3.A.14)

⬁

k

1k

⬁

k

2k

k⫽0

where a10 ⫽

1 2

冕

2

0

sin cos2 d , [1 ⫹  cos2 sin2 ]

(3.A.15)

a1k ⫽

冕

(3.A.16)

0

cos(k)sin cos2 d, [1 ⫹  cos2 sin2 ]

b1k ⫽

冕

sin(k)sin cos2 d, [1 ⫹  cos2 sin2 ]

(3.A.17)

a20 ⫽

2

2

0

1 2

冕

2

0

sin3 d , [1 ⫹  cos2 sin2 ]

(3.A.18)

a2k ⫽

冕

(3.A.19)

0

cos(k)sin3 d , [1 ⫹  cos2 sin2 ]

b2k ⫽

冕

sin(k)sin3 d . [1 ⫹  cos2 sin2 ]

(3.A.20)

2

2

0

For isotropic materials,  ⫽ 0. The nonzero coefﬁcients from (3.A.15) to (3.A.20) are b11 ⫽ b13 ⫽ , 4

b21 ⫽

3 , 4

b23 ⫽ ⫺ . 4

Thus, I1 ⫽ I2 ⫽

i i [sin ⫺ sin(3)] ⫽ [2 sin3 ⫺ sin ], 2r r

i i [3 sin ⫹ sin(3)] ⫽ [3 sin ⫺ 2 sin3 ]. 2r r

70

EIGENSTRAINS

APPENDIX 3.B

The following integrals are given in Mura (1987, pp. 17):

冉冊

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

2ei(1x1⫹2x2) x d1 d2 ⫽ 2 tan⫺1 2 , 2 2 1( 1 ⫹ 2) x1

冕 冕 ⬁

⬁

⫺⬁

⫺⬁

冕 冕 冕 冕 ⬁

⬁

⫺⬁

⫺⬁

⬁

⬁

⫺⬁

⫺⬁

(3.B.1)

21ei(1x1⫹2x2) ⫺ x x d1 d2 ⫽ 2 1 22, 2 2 2 ( 1 ⫹ 2) x1 ⫹ x2

(3.B.2)

ei(1x1⫹2x2) d1 d2 ⫽ ⫺ log(x 21 ⫹ x 22), 21 ⫹ 22

(3.B.3)

22ei(1x1⫹2x2) x 22 2 2 d d ⫽ ⫺ log(x ⫹ x ) ⫺ . 1 2 1 2 ( 12 ⫹ 22)2 2 x 12 ⫹ x 22

(3.B.4)

REFERENCES Burgers, J. M. (1939). ‘‘Some considerations on the ﬁelds of stress connected with dislocations in a regular crystal lattice, I, II,’’ Proc. Kon. Nederl. Akad. Wetensch., Vo. 42, pp. 293–324 and pp. 378–399. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston, MA, Chapter 1.

SUGGESTED READING Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York.

4 INCLUSIONS AND INHOMOGENEITIES In this chapter, we ﬁrst introduce the concepts of inclusions and inhomogeneities. We will then derive the stress and displacement ﬁelds due to the presence of inclusions and inhomogeneities. Finally, we will derive explicitly solutions to ellipsoidal inclusions and inhomogeneities.

4.1 DEFINITIONS OF INCLUSIONS AND INHOMOGENEITIES

Although the terms inclusion and inhomogeneity are used interchangeably in the literature, we will use them differently throughout this book. The readers are advised that the distinction between these two terms made in this book is mainly for the convenience of discussion. An inclusion is deﬁned as a subdomain ⍀ in a domain D, where eigenstrain *(x) is given in ⍀ and is zero in D ⫺ ⍀. The material ij properties in ⍀ and in D ⫺ ⍀ are the same. The domain outside ⍀, that is, D ⫺ ⍀, is called the matrix; see Figure 4.1. For linear elastic material, this can be stated as ⍀ is an inclusion ⇔ *(x) ⫽0 ij

for x 僆 ⍀ 僆 D

ij*(x) ⫽ 0

for x 僆 D ⫺ ⍀

Lijkl is uniform throughout D Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

71

72

INCLUSIONS AND INHOMOGENEITIES

ε ij* (x) = 0 ε ij* (x) ≠ 0 Ω

L(0) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.1 Inclusion.

An inhomogeneity is deﬁned as a subdomain ⍀ in domain D, where the material properties in ⍀ and in D ⫺ ⍀ are different. The domain outside ⍀, that is, D ⫺ ⍀, is called the matrix; see Figure 4.2. For linear elastic material, this can be stated as ⍀ is an inhomogeneity ⇔ Lijkl (x) ⫽

再

L(1) in ⍀ 僆 D ijkl (0) Lijkl in D ⫺ ⍀ no eigenstrain throughout D

From the above deﬁnition, we see that inclusion is nothing but a distribution of eigenstrains in an otherwise homogeneous material. The presence of eigenstrain may cause stresses in the material. On the other hand, inhomogeneity is a foreign material embedded in an otherwise homogeneous matrix material. If the inhomogeneity ﬁts into the sur-

ε ij* (x) = 0 ε ij* (x) = 0 Ω

L(1) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.2 Inhomogeneity.

4.2

INTERFACE CONDITIONS

73

rounding matrix perfectly, there will not be stress produced either in the matrix or in the inhomogeneity.

4.2 INTERFACE CONDITIONS

Consider an inclusion ⍀ in an elastic domain D of elastic stiffness tensor Lijkl. The interface between ⍀ and its surrounding material will be denoted by S. We wish to investigate the continuity of ﬁeld quantities (displacements, strain, stress) across this interface. If the material across the interface S is continuous (e.g., no gap and slip), we call it a perfect interface. For perfect interface, the displacement and the interfacial traction across the interface must be continuous, that is, ⌬ui ⬅ ui(S⫹) ⫺ ui(S⫺) ⫽ 0,

(4.2.1)

⌬ijnj ⬅ [ij(S⫹) ⫺ ij(S⫺)]nj ⫽ 0.

(4.2.2)

where nj is the outward unit normal to the interface S, and ui(S⫹) and ij(S⫹) are the values of ui(x) and ij(x) evaluated at the positive side of S, while ui(S⫺) and ij(S⫺) are the values of ui(x) and ij(x) evaluated at the negative side of S. The positive side of S is the side to which nj points; see Figure 4.3. It then follows from (4.2.1) that the displacement gradient may have a jump across the interface given by ⌬ui, j ⬅ ui, j(S⫹) ⫺ ui, j(S⫺) ⫽ inj,

(4.2.3)

where i is the magnitude of the jump that will be determined shortly. Note that the right-hand side of (4.2.3) is orthogonal to the tangent vector of S. Thus, Eq. (4.2.3) simply says that, due to the constraint of (4.2.1), the tangential derivatives of the displacements along S must be continuous.

S

S−

n S+

Figure 4.3 Interface with positive and negative sides.

74

INCLUSIONS AND INHOMOGENEITIES

Next, making use of Hooke’s law (3.1.5) in (4.2.2) and the fact that the stiffness tensor is the same inside and outside the inclusion yields Lijkl (⌬uk,l ⫺ ⌬*)n kl j ⫽ 0,

(4.2.4)

⌬* *(S⫹) ⫺ kl*(S⫺) ⫽ ⫺kl*(S⫺). kl ⬅ kl

(4.2.5)

⫹ *(S ) ⫽ 0, kl

(4.2.6)

where

Since

substitution of (4.2.3) into (4.2.4) gives ⫺ Lijkl nl njk ⫽ ⫺Lijkl*(S )nj. kl

(4.2.7)

This is a system of algebraic equations for k. Comparing it with (2.6.13), one can easily write out the solution ⫺ i ⫽ ⫺Ljkmn* mn(S )nk Nij(n)/D(n),

(4.2.8)

Nij(n) ⫽ –21 ikljmnKkm(n)Kln(n),

(4.2.9)

D(n) ⫽ mnlKm1(n)Kn2(n)Kl3(n),

(4.2.10)

Kik(n) ⫽ Lijkl ninj,

(4.2.11)

where

ijk ⫽ permutation tensor.

Notice that Nij is the cofactor of Kij and D is the determinant of Kij. Therefore, Nij /D is the inverse of Kij. Expressions of Nij and D for isotropic, cubic, and transversely isotropic materials are given in Appendix 4.A. Substituting (4.2.8) into (4.2.3) we arrived at ⫺ ⌬ui, j ⫽ ⫺Llkmn* mn(S )nknj Nil (n)/D(n).

It thus follows that

(4.2.12)

4.2

INTERFACE CONDITIONS

⫺ ⌬ij ⫽ ⫺–12 Llkmn* mn(S )nk{nj Nil (n) ⫹ ni Njl (n)}/D(n),

75

(4.2.13)

⌬ij ⬅ ij(S⫹) ⫺ ij(S⫺) ⫽ Lijkl (⌬uk,l ⫺ ⌬kl *) ⫺ ⫺1 ⫽ Lijkl{⫺Llkmn* )}. mn(S )nknj Nil (n)/D(n) ⫹ *(S kl

(4.2.14)

Note that for a given inclusion the right-hand sides of (4.2.13) and (4.2.14) involve only known quantities. Therefore, if the strain and stress are known within the inclusion, the corresponding strain and stress just outside the inclusion can be computed from these equations. This proves the following uniqueness theorem. Uniqueness Theorem for Inclusion–Matrix Interface If the stress or strain tensor is known locally at one side of the interface between an inclusion and the surrounding matrix, then their jumps and consequent values at the other side of the interface are explicitly determinable in terms of the matrix moduli, the eigenstrain in the inclusion, and the interface normal. Let us now consider the continuity conditions at the interface between an inhomogeneity and its surrounding matrix. Let the stiffness tensor of inhomogeneity be L(1) ijkl and that of the matrix be Lijkl. Further, we assume that the interface is a perfect one, that is, the continuity conditions (4.2.1) and (4.2.2) are satisﬁed. Consequently, Eq. (4.2.3) also holds. Making use of Hooke’s law, we have ij(S⫹) ⫽ Lijkluk,l (S⫹),

⫺ ij(S⫺) ⫽ L(1) ijkluk,l (S ).

(4.2.15)

Substituting the above into (4.2.2) yields ⫺ Lijkluk,l (S⫹)nj ⫽ L(1) ijkluk,l (S )nj.

(4.2.16)

Eliminating uk,l(S⫹) in the above equation by using (4.2.3), we arrive at the following equation for i: Lijklknl nj ⫽ ⌬Lijkluk,l (S⫺)nj, where

(4.2.17)

76

INCLUSIONS AND INHOMOGENEITIES

⌬Lijkl ⫽ L(1) ijkl ⫺ Lijkl.

(4.2.18)

Similar to (4.2.7), Eq. (4.2.17) can be solved to yield i ⫽ ⌬Ljkmnum,n(S⫺)nk Nij(n)/D(n) ⫽ ⌬Ljkmnmn(S⫺)nk Nij(n)/D(n).

(4.2.19) Making use of the above in (4.2.3) yields ⌬ui, j ⫽ ⌬Llkmnmn(S⫺)nl nj Nik(n)/D(n).

(4.2.20)

Thus, we have ⌬ij ⫽ –12 ⌬Llkmnmn(S⫺1)nl{nj Nik(n) ⫹ ni Njk(n)}/D(n).

(4.2.21)

Further, combination of (4.2.20) and the ﬁrst of (4.2.15) gives ij(S⫹) ⫽ Lijkl{kl (S⫺) ⫹ ⌬Lpqmnmn(S⫺)nl nqNkp(n)/D(n)}

or ⌬ij ⫽ ⌬Lpqmnmn(S⫺)[Lijkl nl nqNkp(n)/D(n) ⫺ ␦pq].

(4.2.22)

Again, we notice from (4.2.21) and (4.2.22) that for a given inhomogeneity, if the strain or the stress ﬁeld on one inside the interface is known, the corresponding strain and stress immediately on the other side of interface can be computed. Therefore, similar to the inclusion case, we can state a uniqueness theorem for the inhomogeneity. Uniqueness Theorem for Inhomogeneity–Matrix Interface If the stress or strain tensor is known locally at one side of the interface between an inhomogeneity and its surrounding matrix, then their jumps and consequent values at the other side of the interface are explicitly determinable in terms of the moduli of the inhomogeneity and the matrix and the interface normal.

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

77

4.3 ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

Consider an inﬁnite domain D containing an ellipsoidal inclusion ⍀ with uniform eigenstrain *. ij Let the stiffness tensor of the material be Lijkl, and the ellipsoidal inclusion (Figure 4.4) be described by ⍀ ⫽ {x1, x2, x3; (x1 /a1)2 ⫹ (x2 /a2)2 ⫹ (x3 /a3)2 ⱕ 1},

(4.3.1)

where a1, a2, and a3 are the semiaxes of the ellipsoid. Since ij*(x) ⫽

再

* ij

for x 傺 ⍀ for x 傺 ⍀,

0

(4.3.2)

it then follows from Green’s function formulation of the general solution to eigenstrain problems (3.3.14), (3.3.15), and (3.3.16) that ui(x) ⫽ Lmjklkl*

冕 ⭸G (x⭸y ⫺ y) dV(y), ⬁ mi

⍀

(4.3.3)

j

⍀ ij(x) ⫽ Lklmn* mnPijkl (x),

(4.3.4)

⍀ ij(x) ⫽ Lijkl (Lpqmnmn * Pklpq (x) ⫺ kl*),

(4.3.5)

where ⌫⬁ijkl (x, y) ⫽

冋

册

1 ⭸2Gki⬁ (x, y) ⭸2G⬁kj(x, y) ⭸2Gli⬁(x, y) ⭸2Glj⬁(x, y) ⫹ ⫹ ⫹ 4 ⭸xj ⭸yl ⭸xi ⭸yl ⭸xj ⭸yk ⭸xi ⭸yk

(4.3.6) was introduced by (3.3.17), and x3 x2

ε ij* Ω

x1

Figure 4.4 Ellipsoidal inclusion ⍀.

78

INCLUSIONS AND INHOMOGENEITIES

P⍀ijkl (x) ⫽

冕⌫ ⍀

⬁ ijkl

(x, y) dV(y).

(4.3.7)

For convenience, we introduce ⍀ Sijkl (x) ⫽ LmnklPijmn (x).

(4.3.8)

Then (4.3.4) and (4.3.5) can be rewritten as ij(x) ⫽ Sijkl (x)*, kl

ij(x) ⫽ Lijkl{Sklmn(x)* mn ⫺ *} kl ⫽ Lijkl{Sklmn(x) ⫺ Iklmn}* mn,

(4.3.9) (4.3.10)

where Iijkl is the fourth-order identity tensor given by Iijkl ⬅ –12 (␦ik␦jl ⫹ ␦il␦jk).

(4.3.11)

It is noted that (4.3.3)–(4.3.10) are valid for both x inside and outside the inclusion ⍀. We now show that P⍀ijkl (x) is a constant fourth-order tensor for x inside ⍀, that is, P⍀ijkl (x) ⫽ Pijkl ⫽

a1a2a3 4

冕H Sˆ

ijkl

ˆ ), x 傺 ⍀ ()a⫺3D⫺1() dS(

(4.3.12)

where Pijkl is referred to as the Hill polarization tensor, and Hijkl () ⫽ Nik()jl ⫹ Njk()il ⫹ Nil ()jk ⫹ Njl ()ik, a ⫽ 兹(a1ˆ 1)2 ⫹ (a2ˆ 2)2 ⫹ (a3ˆ 3)2.

(4.3.13) (4.3.14)

In (4.3.12), the integration is over the surface of the unit sphere Sˆ as shown in Figure 4.5. To this end, let us consider the integral ξ3 1

ξ1

ξ2 Sˆ

ˆ Figure 4.5 Unit sphere S.

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

Gijkl (x) ⫽

冕 ⭸ G⭸x (x,⭸ ) d ⫽ ⫺⭸x⭸ ⭸x 冕 G (x, ) d. ⬁ ki

2

⍀

79

2

j

l

j

l

(4.3.15)

ik

⍀

Replacing Green’s function in the above integral by its expression (2.6.37), we have 1 ⭸2 Gijkl (x) ⫽ ⫺ 2 8 ⭸xj ⭸xl

冕 再冕 ␦[ˆ 䡠 (x ⫺ )]N (ˆ )D ⍀

⫺1

ik

Sˆ

冎

ˆ ˆ ) d. (ˆ ) dS(

(4.3.16) Exchanging the order of integration, 1 ⭸2 Gijkl (x) ⫽ ⫺ 2 8 ⭸xj ⭸xl

冕 再冕 ␦[ˆ 䡠 (x ⫺ )] d冎 N (ˆ )D

ˆ ˆ ). (ˆ ) dS(

⫺1

ik

⍀

Sˆ

(4.3.17) Making use of the result in Appendix 4.A, we have aaa ⭸2 Gijkl (x) ⫽ ⫺ 1 2 3 8 ⭸xj ⭸xl ⫽

a1a2a3 4

冕 ˆ ˆ a Sˆ

j l

冕 a1 [a ⫺ (ˆ 䡠 x) ]N (ˆ )D 2

Sˆ

2

ik

3

ˆ ˆ ) (ˆ ) dS(

⫺1

ˆ ˆ ). Nik(ˆ )D⫺1(ˆ ) dS(

⫺3

(4.3.18)

Substituting (4.3.18) into (4.3.7) yields (4.3.12). Consequently, it follows from (4.3.8) that for x inside the inclusion ⍀, Sijkl ⫽ LmnklPijmn ⫽ lmnkl

a1a2a3 4

冕H Sˆ

ijmn

ˆ ). ()a⫺3D⫺1() dS(

(4.3.19)

This proves (4.3.12). Consequently, it follows from (4.3.9) that the total strain (and the stress as well) is uniform inside the ellipsoidal inclusion when the eigenstrain is uniform, that is, ij(x) ⫽ Sijkl* kl

for x 傺 ⍀

(4.3.20)

where the fourth-order tensor Sijkl is commonly referred to as the Eshelby inclusion tensor, and (4.3.20) is called the Eshelby ellipsoidal inclusion solution. It can be seen from (4.3.12) that

80

INCLUSIONS AND INHOMOGENEITIES

Sijkl ⫽ Sjikl ⫽ Sijlk.

(4.3.21)

However, the Eshelby tensor does not possess the diagonal symmetry, that is, in general, Sijkl ⫽ Sklij. Having obtained the total strain within the inclusion, the stress ﬁeld within the inclusion can be computed from Hooke’s law (3.1.5): ij ⫽ Lijkl (kl ⫺ *) *, kl ⫽ Lijklkl ⫹ ij

(4.3.22)

* ij ⫽ ⫺Lijkl* kl

(4.3.23)

where

is called the stress polarization. It is the stress in the inclusion caused by the eigenstrain *ij when the inclusion is not allowed to deform at all (i.e., the total strain is zero, kl ⫽ 0). This can be easily understood if we recalled the example in Chapter 3, where an aluminum ball is heated while the ball is constrained so the total strain is zero. The corresponding stress generated in the ball, according to (3.2.6), is ij ⫽ ij* ⫽ ⫺␣ALnnij ⌬T

because the eigenstrain in this case is ␣A ⌬T. It then follows from (4.3.19) that the Eshelby solution (4.3.20) can be written as ij ⫽ Sijkl* kl ⫽ PijmnLmnkl* kl ⫽ ⫺Pijmn * mn,

(4.3.24)

where Pijmn ⫽ Sijkl Mklmn is called the stress polarization. Note that this is not the stress on the inclusion. The stress on the inclusion (4.3.22) is given by ij ⫽ Lijkl (Sklmn* mn ⫺ *) kl ⫽ ⫺Qijkl*, kl

where the fourth-order tensor Qijkl ⫽ Lijmn(Imnkl ⫺ Smnkl)

(4.3.25)

can be viewed as the dual of the stress polarization tensor Pijkl.

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

81

One can also show that L(I ⫺ S) ⫽ (I ⫺ ST)L

(4.3.26)

is positive deﬁnite. To this end, consider the total strain energy of the ellipsoidal inclusion problem:

冕 ( ⫺ *) dv ⫽ 21 冕 u dv ⫺ 21 冕 * dv 1 1 ⫽ 冕 [( u ) ⫺ u ] dv ⫺ 冕 L ( ⫺ *)* dv 2 2 1 1 1 ⫽ 冕 u n ds ⫺ 冕 u dv ⫺ 冕 L ( ⫺ *)* dv, 2 2 2

U⫽

1 2

ij

D

ij

ij

D

ij i , j

D

ij, j i

ij i j

S⬁

ij i, j

D

⍀

ij, j i

ij ij

⍀

ijkl

kl

⍀

kl

ijkl

kl

ij

kl

ij

(4.3.27) where S⬁ is the boundary of D. Since D is an inﬁnite domain and the stress vanishes at inﬁnity, the surface integral must be zero. By virtue of the equilibrium equation, the second term on the right-hand side of (4.3.27) is also zero. Therefore, we have

冕 (* ⫺ )L* dv ⫽ 21 冕 (* ⫺ S*)L* dv 1 1 ⫽ 冕 *(I ⫺ S )L* dv ⫽ 冕 *L(I ⫺ S)* dv. 2 2

U⫽

1 2

⍀

⍀

T

⍀

⍀

(4.3.28)

Since the strain energy must be positive and becomes zero only if the eigenstrain is zero, we must have

冕 *(I ⫺ S )L* dv ⫽ 冕 *L(I ⫺ S)* dv ⱖ 0. T

⍀

⍀

(4.3.29)

Note that S is independent of the size of ⍀ and (4.3.29) should hold for any size of ⍀, we can conclude from (4.3.29) that *(I ⫺ ST)L* ⫽ *L(I ⫺ S)* ⱖ 0,

(4.3.30)

and the equal sign is realized only when * ⫽ 0. This proves that L(I ⫺ S) ⫽ (I ⫺ ST)L is positive deﬁnite. Two corollaries of (4.3.30) are

82

INCLUSIONS AND INHOMOGENEITIES

LS ⫽ STL,

(4.3.31)

and (I ⫺ S) is nonsingular. Next, we show that S is also nonsingular. We begin by computing the strain energy stored in the region outside the inclusion:

冕 1 ⫽ 冕 2

Um ⫽

1 2

D⫺⍀

D⫺⍀

ijij dv ⫽

1 2

冕

D⫺⍀

ijui, j dv

[(ijui), j ⫺ ij, jui] dv.

(4.3.32)

Again, the second term on the right hand of (4.3.32) vanishes because of equilibrium. The ﬁrst term can be converted to a surface integral by using the divergence theorem: Um ⫽

1 2

冕

S⬁

ijuinj ds ⫺

1 2

冕 u n ds, S

(4.3.33)

ij i j

where the negative sign of the second term comes about because nj is the outward normal vector of ⍀. The ﬁrst term vanishes because the stresses go to zero at inﬁnity. Thus, we have 1 Um ⫽ ⫺ 2

冕 u n ds ⫽ ⫺12 冕 u S

ij i j

⍀

ij i, j

1 dv ⫽ ⫺ 2

冕 ⍀

ij ij

dv.

(4.3.34)

If S is singular, there must exist an eigenstrain ﬁeld ˆ * kl ⫽ 0

(4.3.35)

such that ij ⫽ Sijklˆ * kl ⫽ 0

on ⍀.

(4.3.36)

In what follows, we will show that (4.3.36) contradicts (4.3.35), that is, if (4.3.36) is satisﬁed, then (4.3.35) cannot be true, thus proving that S cannot be singular. To this end, ﬁrst compute the corresponding stress on ⍀ when (4.3.36) holds:

4.3

ELLIPSOIDAL INCLUSION WITH UNIFORM EIGENSTRAINS (ESHELBY SOLUTION)

ij ⫽ Lijkl (kl ⫺ ˆ *) ˆ *. kl ⫽ ⫺Lijkl kl

83

(4.3.37)

Substitution of (4.3.36) into (4.3.34) leads to Um ⫽ 0. It then follows from (4.3.32) that ij ⫽ ij ⫽ 0 in the region outside the inclusion, or ij(S⫹) ⫽ 0. On the other hand, the traction continuity condition on the inclusion/ matrix interface yields 0 ⫽ ij(S⫹)nj ⫽ ij(S⫺)nj ⫽ ⫺Lijklˆ *n kl j,

(4.3.38)

where (4.3.37) has been used in deriving the last equation of (4.3.38). Note that Lijkl ˆ * kl is a constant second-order tensor while nj varies along the boundary. For (4.3.38) to hold for the entire boundary, we must have Lijklˆ * ˆ kl* ⫽ 0. kl ⫽ 0. Since Lijkl is nonsingular, we end up with This contradicts (4.3.35). Therefore, S cannot be singular. We also note that Sijkl is independent of the eigenstrain. But, it does depend on the matrix material. For general anisotropic materials, numerical methods are typically required to carry out the integral in Sijkl. For isotropic materials, the integral can be written in terms of elliptical integrals and explicit expression in terms of elemental functions can be obtained for certain special cases. For example, the Eshelby tensor Sijkl for a spherical inclusion in an isotropic material is a fourth-order isotropic tensor: Sijkl ⫽ ␥␦ij␦kl ⫹ ␦(␦ik␦jl ⫹ il␦jk ⫺ –23 ␦ij␦kl),

(4.3.39)

where ␥⫽

K 3K ⫹ 4

⫽

1⫹v , 9(1 ⫺ v)

␦⫽

3(K ⫹ 2) 4 ⫺ 5v ⫽ . 5(3K ⫹ 4) 15(1 ⫺ v) (4.3.40)

Using the symbolic notation introduced in (1.3.3), we can simply write S ⫽ (3␥, 2␦).

(4.3.41)

The expressions of Sijkl for inclusions of special shapes are given in Appendix 4.B. Before closing this section, we mention that (4.3.20) is no longer valid for a material point outside the inclusion ⍀. To obtain the strain

84

INCLUSIONS AND INHOMOGENEITIES

and stress ﬁelds outside the inclusion, one needs to evaluate the integral in (4.3.7) for x outside the ellipsoid. An alternative approach is to use the continuity conditions at the interface between an inclusion and its surrounding matrix. Since the stresses and strains are known inside the inclusion, the stresses and strains, based on the uniqueness theorem, can be obtained just outside the inclusion. This allows us to compute the strain and stress ﬁeld anywhere outside the inclusion. The stresses and strains outside the inclusion will not be needed in this book. So, we will not present them. However, we do note that for x outside of ⍀r, Sr(x) decades as 㛳x㛳⫺3 as 㛳x㛳 → ⬁. Readers are referred to the Suggested Readings at end of this chapter for further details.

4.4 ELLIPSOIDAL INHOMOGENEITIES

Consider an elastic body D with elastic modulus L0 containing an ellipsoidal inhomogeneity ⍀ with elastic modulus tensor L1. Let D be subjected to surface traction p0 ⫽ 0 䡠 n on the boundary of D, as shown in Figure 4.6. We are to ﬁnd the stress ﬁelds in D. Obviously, when L1 ⫽ L0, the material is homogeneous. Consequently, the total stress ﬁeld becomes uniform throughout D (see Figure 4.7), and is given by t ⫽ 0

(4.4.1)

It is therefore conceivable that, through the principle of linear superposition, when L1 is different from L0, the total stress ﬁeld in D can be written as

ε ij* (x) = 0 ε ij* (x) = 0 Ω

L(1) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.6 Ellipsoidal inhomogeneity.

4.4

ELLIPSOIDAL INHOMOGENEITIES

85

ε ij* (x) = 0 ε ij* (x) = 0

(0) L(1) ijkl ( x ) = Lijkl ( x )

Ω L(0) ijkl ( x)

D

Figure 4.7 Uniform stress ﬁeld in homogeneous body.

t ⫽ 0 ⫹ ,

(4.4.2)

where is the stress perturbation due to the presence of the inhomogeneity ⍀. Obviously, the perturbed stress ﬁeld should satisfy the equilibrium equations and the homogeneous boundary condition 䡠n⫽0

on S.

(4.4.3)

If 0 is used to denote the strain ﬁeld corresponding to 0, that is, 0 ⫽ L00,

(4.4.4)

then the total strain on the inclusion can be written as t ⫽ 0 ⫹ ,

(4.4.5)

where is the perturbed strain ﬁeld due to the presence of the inhomogeneity. Application of Hooke’s law in D and D ⫺ ⍀ yields, respectively, t ⫽ 0 ⫹ ⫽ L1(0 ⫹ ) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

(4.4.6)

in D ⫺ ⍀,

(4.4.7)

Our task is to solve for and by the so-called equivalent inclusion method. To this end, let us consider a homogeneous body D with elastic modulus tensor L0 everywhere, containing an inclusion ⍀ with eigen-

86

INCLUSIONS AND INHOMOGENEITIES

strain * (the value of which is to be determined); see Figure 4.8. The eigenstrain * is introduced here to simulate the inhomogeneity. In other words, we are trying to create an inclusion problem which, by properly adjusting the value of *, has the same stress ﬁeld as that of the inhomogeneity problem. For the inclusion problem shown in Figure 4.8, Hooke’s law gives t ⫽ 0 ⫹ ⫽ L0(0 ⫹ ⫺ *) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

(4.4.8)

in D ⫺ ⍀,

(4.4.9)

where 0 and 0 are the ﬁelds in D due to the applied traction p0 ⫽ 0 䡠 n when the inclusion is absent, and and are the ﬁelds due to eigenstrain * in the inclusion ⍀. From the Eshelby solution (4.3.20), ⫽ S*,

(4.4.10)

we can rewrite (4.4.8) as t ⫽ 0 ⫹ ⫽ L0(0 ⫹ S* ⫺ *)

in ⍀.

(4.4.11)

Now, recall that we created this inclusion problem to simulate the inhomogeneity problem. We want to adjust the eigenstrain * so that the stress ﬁeld in the inclusion ⍀ given by (4.4.11) is the same as the stress ﬁeld in the inhomogeneity ⍀ given by (4.4.6), namely,

ε ij* (x) = 0 ε ij* (x) ≠ 0 Ω

L(0) ijkl ( x) L(0) ijkl ( x)

D

Figure 4.8 Ellipsoidal inclusion.

4.4

ELLIPSOIDAL INHOMOGENEITIES

L0(0 ⫹ S* ⫺ *) ⫽ L1(0 ⫹ )

in ⍀.

87

(4.4.12)

Making use of the Eshelby solution (4.3.20) again yields L0(0 ⫹ S* ⫺ *) ⫽ L1(0 ⫹ S*)

in ⍀.

(4.4.13)

This is called the equivalent inclusion equation. From this equation, the eigenstrain needed to simulate the inhomogeneity can be solved: * ⫽ ⫺[(L1 ⫺ L0)S ⫹ L0]⫺1(L1 ⫺ L0)0 ⫽ ⫺((L1 ⫺ L0)⫺1[(L1 ⫺ L0)S ⫹ L0])⫺10 ⫽ ⫺[S ⫹ (L1 ⫺ L0)⫺1L0)]⫺10.

(4.4.14)

The total strain on the inclusion thus follows from (4.4.5): t ⫽ 0 ⫹ ⫽ 0 ⫹ S* ⫽ T0,

(4.4.15)

where T ⫽ I ⫺ S[S ⫹ (L1 ⫺ L0)⫺1L0]⫺1 ⫽ [S ⫹ (L1 ⫺ L0)⫺1L0) ⫺ S][S ⫹ (L1 ⫺ L0)⫺1L0]⫺1 ⫽ (L1 ⫺ L0)⫺1L0[S ⫹ (L1 ⫺ L0)⫺1L0]⫺1 ⫽ ([S ⫹ (L1 ⫺ L0)⫺1L0]L0⫺1(L1 ⫺ L0))⫺1 ⫺1 ⫽ [SL⫺1 0 (L1 ⫺ L0) ⫹ I]

(4.4.16)

or ⫺1 T ⫽ [I ⫹ SL⫺1 0 (L1 ⫺ L0)] .

(4.4.17)

Since the stresses in the inclusion are the same as those in the inhomogeneity, the total stress in the inhomogeneity is, therefore, given by t ⫽ 0 ⫹ ⫽ L0(0 ⫹ S* ⫺ *),

(4.4.18)

where * is given by (4.4.14). This completes the solution of the inhomogeneity problem.

88

INCLUSIONS AND INHOMOGENEITIES

To close this section, we need to mention that when the eigenstrain is given by (4.4.14), the stresses for the inclusion problem and the inhomogeneity problem are identical not only inside ⍀ but also in D ⫺ ⍀. This can be shown by using the uniqueness theorem for inclusions and inhomogeneities.

4.5 INHOMOGENEOUS INHOMOGENEITIES

Sometimes an inhomogeneity may possesses its own eigenstrains. Such inhomogeneities are called inhomogeneous inhomogeneities. In other words, a subdomain occupied by foreign material may involve a distribution of eigenstrains as well. Examples of such inhomogeneous inhomogeneities include the formation of martensite blades in quenched carbon steels and precipitations in alloys. To solve for the inhomogeneous inhomogeneity problem, let us consider the inhomogeneity shown in Figure 4.1. Let D be subjected to surface traction p0 ⫽ 0 䡠 n on the boundary. Furthermore, we assume that a uniform eigenstrain p is prescribed on the inhomogeneities ⍀. We are to ﬁnd the stress ﬁeld in D. If 0 is used to denote the strain ﬁeld corresponding to 0, that is, 0 ⫽ L00,

(4.5.1)

then application of Hooke’s law in D and D ⫺ ⍀ yields, respectively, t ⫽ 0 ⫹ ⫽ L1(0 ⫹ ⫺ p) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

(4.5.2)

in D ⫺ ⍀,

(4.5.3)

where and are the perturbed stress and strain ﬁelds, respectively, caused by the sum of two factors, the inhomogeneity and the eigenstrain p in the inhomogeneity. Our task is to solve for and . Imagine that the inhomogeneous inhomogeneity is being simulated by an inclusion in a homogeneous matrix with elastic stiffness tensor L, where the total eigenstrain on the inclusion is p ⫹ *. Then, (4.5.2) and (4.5.3) can be rewritten as

4.5

INHOMOGENEOUS INHOMOGENEITIES

t ⫽ 0 ⫹ ⫽ L0(0 ⫹ ⫺ p ⫺ *) t ⫽ 0 ⫹ ⫽ L0(0 ⫹ )

in ⍀,

in D ⫺ ⍀.

89

(4.5.4) (4.5.5)

Consequently, the equivalent inclusion equation becomes L0(0 ⫹ ⫺ p ⫺ *) ⫽ L1(0 ⫹ ⫺ p)

in ⍀.

(4.5.6)

The Eshelby solution (4.3.20) in this case takes the form of ⫽ S** ⫽ S(p ⫹ *),

(4.5.7)

** ⫽ p ⫹ *.

(4.5.8)

where

Introducing (4.5.7) into (4.5.6) yields L0(0 ⫹ S** ⫺ **) ⫽ L1(0 ⫹ S** ⫺ p)

in ⍀.

(4.5.9)

This can be solved to obtain ** ⫽ [L0(S ⫺ I) ⫺ L1S]⫺1(⌬L M00 ⫺ L1p),

(4.5.10)

⌬L ⫽ L1 ⫺ L0.

(4.5.11)

where

Note that S[L0(S ⫺ I) ⫺ L1S]⫺1 ⫽ S[L0(S ⫺ I) ⫺ L1S]⫺1 ⫽ ⫺(L0S⫺1 ⫺ L0 ⫹ L1)⫺1 ⫽ ⫺(H ⫹ L1)⫺1,

(4.5.12) where

90

INCLUSIONS AND INHOMOGENEITIES

H ⫽ L0S⫺1 ⫺ L0 ⫽ L0(S⫺1 ⫺ I) ⫽ P⫺1 ⫺ L0

(4.5.13)

is known as Hill’s constraint tensor. Therefore, (4.5.10) can be written alternatively, ** ⫽ ⫺S⫺1(H ⫹ L1)⫺1(⌬L M00 ⫺ L1p).

(4.5.14)

Once the eigenstrain ** is known, the total strain on the inhomogeneous inhomogeneity can be computed as t ⫽ 0 ⫹ ⫽ 0 ⫹ S**.

(4.5.15)

Therefore, substituting (4.5.14) into (4.5.15), we can write the total strain in the inhomogeneous inhomogeneity as t ⫽ 0 ⫹ ⫽ 0 ⫺ (H ⫹ L1)⫺1(⌬L M00 ⫹ p),

(4.5.16)

where the stress polarization is deﬁned by p ⫽ ⫺L1p.

(4.5.17)

Similarly, the total stress on the inhomogeneous inhomogeneity is given by (4.5.4) t ⫽ L0(0 ⫹ S** ⫺ **) ⫽ 0 ⫺ L0(I ⫺ S⫺1)(H ⫹ L1)⫺1(⌬L M00 ⫹ p)

in ⍀

⫽ 0 ⫹ H(H ⫹ L1)⫺1(⌬L M00 ⫹ p).

(4.5.18)

Making use of (4.5.16) in (4.5.18) gives an alternative form: t ⫽ 0 ⫺ H(t ⫺ 0)

in ⍀.

(4.5.19)

In the absence of the applied loading, (4.5.16) and (4.5.18) become, respectively, t ⫽ ⫺(H ⫹ L1)⫺1 p, t ⫽ H(H ⫹ L1)⫺1 p ⫽ ⫺Ht

(4.5.20) in ⍀.

(4.5.21)

PROBLEMS

91

PROBLEMS

4.1 A spherical cavity of radius a is present in an otherwise uniform, isotropic, linearly elastic solid of inﬁnite extent with Poisson’s ratio . A uniaxial tension 0ij ⫽ 0␦i3␦j3 is applied at inﬁnity. (See Fig. 4.9.) 1. Use the equivalent inclusion method to ﬁnd the stress components ij(x1, x2, x3) at points (0, 0, a) and (0, a, 0). 2. Deﬁne the stress concentration factors by t ⫽

33(0, a, 0) , 0

c ⫽

11(0, 0, a) 0

and plot the stress concentration factors versus the Poisson’s ratio . 4.2 Prove that the stress polarization tensor Pijkl symmetric and positive-deﬁnite. Further, *M ij ijkl * kl ⱖ *P ij ijkl * kl ⱖ 0

for any arbitrary second-order tensor *. ij 4.3 Prove the identity ⫺(L1 ⫺ L0)⫺1L0 ⫽ M1(M1 ⫺ M0)⫺1.

σ0 x3 x2 x1

σ0

Figure 4.9

92

INCLUSIONS AND INHOMOGENEITIES

APPENDIX 4A

Consider the integral I⫽

冕 ␦[ˆ 䡠 (x ⫺ )] d,

(4.A.1)

⍀

where the integration doman ⍀ is an ellipsoid deﬁned by (4.3.1). To carry out this integral, we introduce the following substitutions: ⫽

冤 冥

冤 冥

1 /a1 2 /a2 , 3 /a3

x1 /a1 x ⫽ x2 /a2 , x3 /a3

a ˆ 1 1ˆ1 ⫽ a , a 2ˆ2 a33

冤 冥

(4.A.2)

where a ⫽ 兹(a1ˆ 1)2 ⫹ (a2ˆ 2)2 ⫹ (a3ˆ 3)2.

(4.A.3)

Then, the volume integral over the ellipsoid can be converted to a volume integral overa unit sphere: I⫽

冕 ␦[ˆ 䡠 (x ⫺ )] d ⫽ 冕 ⍀

iiⱕ1

␦[a( 䡠 x ⫺ 䡠 )]a1a2a3 d.

(4.A.4) In the case 䡠 x ⬍ 1, the above integral can be written as

冕 再冕 冋冕 ␦( 䡠 x ⫺ z) dr册 dz冎 d aaa ⫽ 冕 再冕 (1 ⫺ z )␦( 䡠 x ⫺ z) dz冎 d 2a aaa ⫽ 冕 [1 ⫺ ( 䡠 x) ] d 2a

I⫽

a1a2a3 a 1 2 3

1 2 3

2

1

兹1⫺z2

0

⫺1

0

2

1

0

⫺1

2

2

2

0

⫽

a1a2a3 [1 ⫺ ( 䡠 x)2]. a

See Figure 4.10. Returning to the original variables, we have

(4.A.5)

APPENDIX 4B

ESHELBY TENSOR FOR ISOTROPIC MATERIALS

93

η

r x

ϕ

z

ξ

Figure 4.10 Domain of integration.

I⫽

a1a2a3 a a a [1 ⫺ ( 䡠 x)2] ⫽ 1 32 3 [a2 ⫺ (ˆ 䡠 x)2]. a a

(4.A.6)

For a point x inside the ellipsoid, the corresponding x is inside a unit sphere, that is, 㛳x㛳 ⬍ 1. Since is a unit vector, we have 䡠 x ⬍ 1 for any point x inside the ellipsoid ⍀. Therefore, the above result is valid for any point x inside the ellipsoid ⍀. APPENDIX 4B ESHELBY TENSOR FOR ISOTROPIC MATERIALS WITH POISSON’S RATIO Ellipsoid (a1 ⬎ a2 ⬎ a3)

S1111 ⫽

3 1 ⫺ 2v a2I ⫹ I, 8 (1 ⫺ v) 1 11 8 (1 ⫺ v) 1

S1122 ⫽

1 1 ⫺ 2v a22I12 ⫺ I, 8 (1 ⫺ v) 8 (1 ⫺ v) 1

S1133 ⫽

1 1 ⫺ 2v a23I13 ⫺ I, 8 (1 ⫺ v) 8 (1 ⫺ v) 1

S1212 ⫽

a21 ⫹ a22 1 ⫺ 2v I12 ⫹ (I ⫹ I2). 16 (1 ⫺ v) 16 (1 ⫺ v) 1

All other nonzero components are obtained by the cyclic permutation of the above equations. The components that cannot be obtained by the cyclic permutation are zero; for instance, S1112 ⫽ S1223 ⫽ S1232 ⫽ 0.

94

INCLUSIONS AND INHOMOGENEITIES

In the above equations, the constants I1, I2, I11, I12, and I13 are given by the following: I1 ⫽ I3 ⫽

4a1a2a3 {F(, k) ⫺ E(, k)}, (a ⫺ a22)(a12 ⫺ a32)1 / 2 2 1

再

冎

4a1a2a3 a2(a21 ⫺ a23)1 / 2 ⫺ E(, k) , (a22 ⫺ a32)(a12 ⫺ a32)1 / 2 a1a3

where the elliptical integrals are deﬁned by F(, k) ⫽ E(, k) ⫽

冕 (1 ⫺ k dwsin w)

2

0

2

,

1/2

冕 (1 ⫺ k sin w)

2

2

1/2

dw,

0

⫽ sin⫺1(1 ⫺ a32 /a12)1 / 2,

k ⫽ {(a12 ⫺ a22)/(a12 ⫺ a32)}1 / 2.

Furthermore I1 ⫹ I2 ⫹ I3 ⫽ 4, 3I11 ⫹ I12 ⫹ I13 ⫽ 4 /a12, 3a21I11 ⫹ a22I12 ⫹ a32I13 ⫽ 3I1, I12 ⫽ (I2 ⫺ I1)/(a21 ⫺ a22). These equations and their cyclic counterparts give sufﬁcient relations to express Ii and Iij in terms of I1 and I3. Sphere (a1 ⫽ a2 ⫽ a3 ⫽ a)

I1 ⫽ I2 ⫽ I3 ⫽ 4 /3, I11 ⫽ I22 ⫽ I33 ⫽ I12 ⫽ I23 ⫽ I31 ⫽ 4 /5a2, S1111 ⫽ S2222 ⫽ S3333 ⫽

7 ⫺ 5v , 15(1 ⫺ v)

APPENDIX 4B

ESHELBY TENSOR FOR ISOTROPIC MATERIALS

S1122 ⫽ S2233 ⫽ S3311 ⫽ S1133 ⫽ S2211 ⫽ S3322 ⫽ S1212 ⫽ S2323 ⫽ S3131 ⫽

95

5v ⫺ 1 , 15(1 ⫺ v)

4 ⫺ 5v . 15(1 ⫺ v)

Elliptic Cylinder (a3 → ⬁)

I1 ⫽ 4a2 /(a1 ⫹ a2),

I2 ⫽ 4a1 /(a1 ⫹ a2), I3 ⫽ 0

I12 ⫽ 4 /(a1 ⫹ a2)2,

3I11 ⫽ 4 /a21 ⫺ I12,

3I22 ⫽ 4 /a22 ⫺ I12,

I13 ⫽ I23 ⫽ I33 ⫽ 0,

a32I13 ⫽ I1, S1111 ⫽ S2222 ⫽

a32I23 ⫽ I2,

a32I33 ⫽ 0.

再

冎

a22 ⫹ 2a1a2 a2 ⫹ (1 ⫺ 2v) , 2 2(1 ⫺ v) (a1 ⫹ a2) a1 ⫹ a2 1

再

冎

a21 ⫹ 2a1a2 a1 ⫹ (1 ⫺ 2v) , 2 2(1 ⫺ v) (a1 ⫹ a2) a1 ⫹ a 2 1

S1122 ⫽

1

再

a22

2(1 ⫺ v) (a1 ⫹ a2)

S2233 ⫽

2

1

2va1 , 2(1 ⫺ v) a1 ⫹ a2 S1133 ⫽

S2211 ⫽

1

再

S2323 ⫽

S1212 ⫽ a1

a2 a1 ⫹ a 2

冎

,

冎

,

S3311 ⫽ 0,

1

2va2 , 2(1 ⫺ v) a1 ⫹ a2 a12

2(1 ⫺ v) (a1 ⫹ a2)

S3322 ⫽ 0,

⫺ (1 ⫺ 2v)

S3333 ⫽ 0,

2

⫺ (1 ⫺ 2v)

a1 a1 ⫹ a 2

再

冎

a12 ⫹ a22 1 ⫺ 2v ⫹ , 2(1 ⫺ v) 2(a1 ⫹ a2)2 2 1

, 2(a1 ⫹ a2)

S3131 ⫽

a2

. 2(a1 ⫹ a2)

96

INCLUSIONS AND INHOMOGENEITIES

Penny Shape (a1 ⫽ a2 ⬎⬎ a3)

I1 ⫽ I2 ⫽ 2a3 /a1,

I3 ⫽ 4 ⫺ 2 2a3 /a1,

I12 ⫽ I21 ⫽ 3 2a3 /4a31, I13 ⫽ I23 ⫽ I31 ⫽ I32 ⫽ 3(–34 ⫺ 2a3 /a1)/a12, I11 ⫽ I22 ⫽ 3 2a3 /4a31, S1111 ⫽ S2222 ⫽

13 ⫺ 8v a 3, 32(1 ⫺ v) a1

S1122 ⫽ S2211 ⫽

7 ⫺ 8v a 3, 32(1 ⫺ v) a1

Skk11 ⫽ Skk22 ⫽

S3333 ⫽ 1 ⫺

8v ⫺ 1 a 3, 32(1 ⫺ v) a1

S3311 ⫽ S3322 ⫽ S1212 ⫽

I33 ⫽ –34 /a32;

v 1⫺v

S2233 ⫽

冉

1⫺

2v ⫺ 1 a 3, 8(1 ⫺ v) a1

冊

4v ⫹ 1 a3 , 8v a1

S1313 ⫽ S2323 ⫽

1 ⫺ 2v a3 v ⫹ , 1 ⫺ v 4 a1 1 ⫺ v

1 ⫺ 2v a3 , 1 ⫺ v 4 a1

冉

冊

1 v ⫺ 2 a3 1⫹ , 2 1 ⫺ v 4 a1

Skk33 ⫽ 1 ⫺

1 ⫺ 2v a3 . 1 ⫺ v 2 a1

When a3 ⫽ 0, I1 ⫽ I2 ⫽ 0, I3 ⫽ 4, I12 ⫽ 0,

I23 ⫽ 4 /a22,

I11 ⫽ I22 ⫽ 0,

I31 ⫽ 4 /a12,

a23I33 ⫽ 4 /3,

S2323 ⫽ S3131 ⫽ –12 , S3311 ⫽ S3322 ⫽ v /(1 ⫺ v), S3333 ⫽ 1,

and all other Sijkl ⫽ 0.

APPENDIX 4B

ESHELBY TENSOR FOR ISOTROPIC MATERIALS

97

Flat Ellipsoid (a1 ⬎ a2 ⬎⬎ a3)

I1 ⫽ 4a2a3{F(k) ⫺ E(k)}/(a21 ⫺ a22), I2 ⫽ 4a3E(k)/a2 ⫺ 4a2a3{F(k) ⫺ E(k)}/(a21 ⫺ a22), I3 ⫽ 4 ⫺ 4a3E(k)/a2, I12 ⫽ [4a3E(k)/a2 ⫺ 8a2a3{F(k) ⫺ E(k)}/(a12 ⫺ a22)]/(a12 ⫺ a22), I23 ⫽ [4 ⫺ 8a3E(k)/a2 ⫹ 4a2a3{F(k) ⫺ E(k)}/(a21 ⫺ a22)]/a22, I31 ⫽ [4 ⫺ 4a2a3{F(k) ⫺ E(k)}/(a12 ⫺ a22) ⫺ 4a3E(k)/a2]/a21, I33 ⫽ 4 /3a23, where F(k) and E(k) are the complete elliptic integrals of the ﬁrst and the second kind, respectively, E(k) ⫽

冕

(1 ⫺ k2 sin2 )1/ 2 d,

F(k) ⫽

冕

(1 ⫺ k2 sin2 )⫺1 / 2 d,

/2

0

/2

0

k2 ⫽ (a12 ⫺ a22)/a12. Oblate Spheroid (a1 ⫽ a2 ⬎ a3)

再

冉 冊冎

2a2a a a a2 I1 ⫽ I2 ⫽ 2 1 233 / 2 cos⫺1 3 ⫺ 3 1 ⫺ 23 (a1 ⫺ a3) a1 a1 a1

1/2

,

I3 ⫽ 4 ⫺ 2I1, I11 ⫽ I22 ⫽ I12, I12 ⫽ /a12 ⫺ –41 I13 ⫽ /a21 ⫺ I13 ⫽ I23 ⫽ (I1 ⫺ I3)/(a32 ⫺ a12),

I1 ⫺ I3 , 4(a23 ⫺ a21)

3I33 ⫽ 4 /a32 ⫺ 2I13.

98

INCLUSIONS AND INHOMOGENEITIES

Prolate Spheroid (a1 ⬎ a2 ⫽ a3)

I2 ⫽ I3 ⫽

再 冉 冊

2a1a32 a1 a12 ⫺1 (a12 ⫺ a32)3 / 2 a3 a32

I1 ⫽ 4 ⫺ 2I2,

1/2

⫺ cosh⫺1

冎

a1 , a3

I12 ⫽ (I2 ⫺ I1)/(a21 ⫺ a22),

3I11 ⫽ 4 /a21 ⫺ 2I12, I22 ⫽ I33 ⫽ I23,

3I22 ⫽ 4 /a22 ⫺ I23 ⫺ (I2 ⫺ I1)/(a12 ⫺ a22),

I23 ⫽ /a22 ⫺ (I2 ⫺ I1)/4(a12 ⫺ a22). SUGGESTED READING Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston, Chapters 3–4. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York, Chapter 7.

5 DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS Most engineering materials are heterogeneous in nature. They generally consist of different constituents or phases, which are distinguishable at speciﬁc scales. Each constituent may show different physical properties (e.g., elastic moduli, thermal expansion, yield strength, electrical conductivity, thermal conductivity, etc.) and/or material orientations. However, in many engineering applications, a structure component may contain numerous such constituents such that it is impractical or even impossible to account for each and every one of them for engineering design and analysis. What is really relevant is the overall or effective property of the material from which the component is made. In this chapter, we will lay out the basic deﬁnitions of overall or effective properties of engineering materials that are heterogeneous at the length scale of interest. Generally speaking, heterogeneous materials can be classiﬁed into two categories, periodic and nonperiodic. In this text, we will focus primarily on heterogeneous materials with nonperiodic microstructures. So, unless indicated otherwise, the term heterogeneous material refers to heterogeneous materials with nonperiodic microstructures. Examples of such materials may include most of the ﬁber or particulate reinforced composites and polycrystalline materials. 5.1 HETEROGENEITY AND LENGTH SCALES

Generally speaking, engineering materials are heterogeneous, that is, they have microstructure and they contain heterogeneities. However, Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

99

100

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

what constitutes a heterogeneity depends on the length scales used in the observation. Certain constituents or phases in a given material are identiﬁable only at or below a speciﬁc length scale. At such a length scale, each constituent may be homogeneous, but when observed at a smaller length scale, the constituent itself may become heterogeneous. A polycrystal copper, for example, may seem to be homogeneous with the naked eye (⬃10 m). But, under optical microscope (⬃1 m), the polycrystal copper is composed of many grains—small single copper crystals with different orientations. At this length scale, although each grain can be treated as a homogeneous material, the polycrystal copper as an assembly of grains cannot be treated as a homogeneous material any more because the microstructure attributes, such as grain size, orientation, and grain boundaries, dictate how the material behaves at this length. When we go down further along the length scales, we know that each grain also has its own microstructure. The behavior and properties of materials at each length scale are controlled by the observable microstructure at the corresponding length scale. Therefore, whether a material is heterogeneous or not depends on the length scale used in the observation. In other words, when studying the properties of a real material, which is always heterogeneous, we need to deﬁne the length scale at which the properties of interest are directly relevant. Microstructure features not observable at this length can be neglected. In fact, for practical purposes, it is only certain averaged effects of the microstructure that are of interest. So, in the study of heterogeneous materials, we often speak of overall properties. By that we mean the properties averaged over a certain volume of the heterogeneous material. For such overall properties to be meaningful, the average taken over any arbitrary volume element comparable with the relevant length scale must be the same with the heterogeneous material sample under consideration. Heterogeneous materials that meet this requirement are said to be macroscopically homogeneous. We will give a more quantitative deﬁnition of macroscopic homogeneity later in this chapter. For now, let us consider, for example, a ﬁber-reinforced composite laminate. It is certainly impractical and unnecessary to deal with each individual ﬁber when the overall bending rigidity of the laminate is of primary interest. On the other hand, the bending rigidity of the laminate is very closely related to the lay up of the various layers within the laminate. To derive the overall rigidity of the composite, the laminate must be treated as a stack of plies each being different in composition and/or orientation, albeit each ply can be treated as a homogeneous layer.

5.1

HETEROGENEITY AND LENGTH SCALES

101

In the examples given above, we have implicitly implied that there is a separation of length scales D and d on which the macroscopic properties (e.g., bending rigidity of the composite laminate) and microscopic properties (elasticity of the plies) are deﬁned, respectively. The microscale length d corresponds to the smallest constituent whose physical properties, orientation, and shape are judged to have direct ﬁrst-order effects on the macroscopic overall physical properties of the heterogeneous material at the length scale D. The choice of d is generally adapted to the problem under consideration. An appropriate choice should be guided by systematic ‘‘multiscale’’ experimental observations. Generally speaking, an optimum choice would be the one that includes a good balance between the deﬁnitions of the microscale that have a ﬁrst-order effect on the overall properties, and the simplicity of the resulting model. The macroscale length D should be large enough so that the microscale ﬂuctuations (perturbations) of the stress and strain ﬁelds due to the local variation of microstructure at the scale d inﬂuence the overall effective property only through their averages. In fact, in the framework of micromechanics, the stress and strain ﬁelds are split into contributions corresponding to different length scales. It is assumed that these length scales are sufﬁciently different in terms of their order of magnitude, so that for each pair of them, the ﬂuctuations of stress and strain ﬁelds (micro or local quantities) at the smaller length scale inﬂuence the overall (or macroscopic) behavior at the larger length scale only through their averages, and, conversely, ﬂuctuations of stress and strain ﬁelds as well as the compositional gradients (macro or global quantities) are not signiﬁcant at the smaller length scale. Therefore, at this scale, these macroﬁelds are locally uniform and can be described as uniformly applied stresses and strains. To meet these conditions, the typical dimension of the microscale constituents should be orders of magnitude smaller than the macroscale element so that, d/D ⬍⬍ 1. In the composite laminate example mentioned above, if the thickness of each single ply is on the order of d ⬃ 0.1 mm, the thickness of the laminate should be at least on the order of D ⬃ 1 mm so that the macroscopic effective bending rigidity can be deﬁned meaningfully. Note that the identiﬁcation of d and D is dependent of the length scale of interest. In the above example, since our interest is in the overall bending rigidity of the laminate, we have taken the overall thickness of the laminate to be our macroscopic length parameter and the thickness of each ply to be our microscopic parameter. This way, it implies that each ply is a homogeneous material with no micro-

102

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

structure. However, if we are interested in the behavior of each individual ply, that is, our interest is in the length scale of the ply thickness, we must then identify the ply thickness as our macroscopic length parameter. In this case, the microscopic length parameter d would be the diameter of the individual ﬁbers within the ply. Each ply as a whole can no longer be viewed as a homogeneous material. Instead, it becomes a composite consisting of polymer resin and the ﬁbers. Each constituent can be considered a homogeneous material.

5.2 REPRESENTATIVE VOLUME ELEMENT

In light of the above discussions, we introduce the concept of microhomogeneity. The microstructure of heterogeneous materials is, at any given length scale, very complex, and, to a certain extent, random. To describe the precise topographic features of the microstructure variation is usually impractical and very often impossible. In fact, for practical purposes, it is only certain averaged effects of the microstructure that are of interest. So, in the study of heterogeneous materials, we often speak of overall properties. By that we mean the properties averaged over a certain volume of the heterogeneous material. For such overall properties to be meaningful, the average taken over any arbitrary volume element comparable with the relevant length scale must be the same with the heterogeneous material sample under consideration. Heterogeneous materials that meet this requirement are said to be macroscopically heterogeneous. In light of the discussions in the preceding paragraph, if in a heterogeneous material the microscopic length parameter d and the macroscopic length parameter D can be identiﬁed for a length scale of interest such that d/D ⬍⬍ 1, then the heterogeneous material is microscopically homogeneous at the length scale D. A volume element with characteristic dimension of D is called a representative volume element (RVE) because the overall properties on any RVE would be the same. In other words, the overall properties of each RVE represent the overall properties of the heterogeneous material.

5.3 RANDOM MEDIA

The foregoing discussions assumed that the microstructure of the heterogeneous material is known. In reality, the microstructures of engi-

5.3

RANDOM MEDIA

103

neering materials are very complex and very often random in nature. It is impractical and even impossible to have knowledge on every detail of the microstructure conﬁguration at any given length scale, except in cases such as those displaying periodicity. Typically, only certain ‘‘average’’ features of the microstructure will be known, and such information is likely to be statistical in character. In this section, we will discuss how such statistical information can be incorporated in the deﬁnition of RVE. Consider a batch of particulate-reinforced composite blocks made under the same processing conditions. Let R denote the batch and N be the total number of blocks in R. Assume that all the blocks are the same size D, which is much larger than the particle diameter d, and the particle content (e.g., volume fraction) c is the same for all blocks. However, due to manufacture variability, the distribution of the particles in each block is inevitably different one from the other. Consequently, if we choose a small volume at the same location x on each block, the particle content c(x, ␣) in this small volume may not be the same among all the blocks, and thus, the average 具c(x)典 ⫽

1 N

冘 c(x, ␣), N

␣⫽1

(5.3.1)

may depend on N. However, it is conceivable that if N is very large, the average value computed from (5.3.1) would become relatively independent of N. In the limit of N → ⬁, the summation can be replaced by an integral over the sample space R, and the average becomes independent of N: 具c(x)典 ⫽ lim N→⬁

1 N

冘 c(x, ␣) ⫽ 冕 c(x, ␣) d␣. N

␣⫽1

(5.3.2)

R

Such an averaging scheme is called the ensemble average. Now, let us consider a different average by picking out a block randomly from the batch; call it the ␣th block. First we divide this block into M subdomains of volume Vi, where 兺M i⫽1 Vi ⫽ V with V being the total volume of the block. Then, we calculate the particle volume fraction c(x, ␣) on each of the subdomains, where xi is the coordinate of a representative point, for example, the centroid of Vi. Again, due to manufacture variability, the particle volume fraction on each of the subdomains may not be the same among all the subdomains, and, thus, the average

104

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

c(␣) ⫽

1 V

冘 c(x )V M

i

(5.3.3)

i

i⫽1

may depend on M. However, it is conceivable that if M is very large, the average value computed from (5.3.3) would become relatively independent of M. In the limit of M → ⬁, the summation can be replaced by an integral over the entire volume V and the average becomes independent of M: c(␣) ⫽ lim M→⬁

1 V

冘 c(x )V ⫽ V1 冕 c(x) dv. M

i

i

i⫽1

(5.3.4)

V

We will call this average scheme the volume (or spatial) average. Note that the ensemble average is carried out over a group of blocks made under the same process, while the volume average is performed over an individual block out of the group. The nature of manufacture variability is such that the local particle volume fraction c(x, ␣) at x can be viewed as a random function of the sample ␣, as well as a random function of the position x; each represents a different random process. The ensemble average gives the mean value among all the samples in the sample space, while the volume average tells us the mean value over a particular sample. Imagine that the particle distribution in each and every block were exactly the same; it is plausible that the two average schemes should give the same value, that is, 具c(x)典 ⫽ c(␣),

(5.3.5)

冕 c(x, ␣) d␣ ⫽ V1 冕 c(x, ␣) dV(x).

(5.3.6)

or

R

V

This statement, that is, ensemble average equals volume average, is known as the ergodic hypothesis, a concept used frequently in stochastic analysis, where time average is used in lieu of the volume average deﬁned in (5.3.4). Let us now generalize the ergodic hypothesis to the description of microstructure features in heterogeneous materials. Consider, generally, a group of heterogeneous materials. Let us name the group R and each member of the group will be characterized by the label ␣. The value of ␣ is taken as deﬁning the member (one of the materials in the group)

5.3

RANDOM MEDIA

105

completely. Further, assume that, associated with ␣, there is a probability distribution function p(␣) deﬁned over R, which satisﬁes

冕 p(␣) d␣ ⫽ 1.

(5.3.7)

R

Next, assume that each member of the group has a total volume V and consists of N different types of inhomogeneities or phases. The r th phase in sample ␣ is assumed to occupy the volume Vr(␣), r ⫽1, 2, 3, . . . , N. To describe the material’s microstructure or the spatial distribution of inhomogeneities, it is convenient to introduce the characteristic function that takes the value of 1 if x lies within the volume Vr(␣) and zero otherwise, that is, ƒr(x, ␣) ⫽

再

1 0

x 僆 Vr(␣) . x ⰻ Vr(␣)

(5.3.8)

Clearly, the characteristic function ƒr(x, ␣) satisﬁes the following consistency condition:

冘 ƒ (x, ␣) ⫽ 1. N

(5.3.9)

r

r⫽1

Thus, the ensemble average of ƒr(x, ␣) deﬁnes the probability Pr(x) of ﬁnding phase r at location x: Pr(x) ⫽ 具ƒr(x, ␣)典 ⬅

冕 ƒ (x, ␣)p(␣) d␣. r

(5.3.10)

R

The function Pr(x) is also referred to as the one-point correlation function for the characteristic function ƒr(x, ␣). Likewise, the probability Prs(x, x⬘) of ﬁnding simultaneously phase r at x and phase s at x⬘ is Prs(x, x⬘) ⫽ 具ƒr(x, ␣)ƒs(x⬘, ␣)典 ⬅

冕 ƒ (x, ␣)ƒ (x⬘, ␣)p(␣) d␣. V

r

s

(5.3.11)

The function Prs(x, x⬘) is also referred to as the two-point correlation function for the characteristic function ƒr(x, ␣). Following this approach, probabilities involving, for example, k points, or k-point correlation function, can be deﬁned similarly.

106

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

Let us now develop an understanding of the geometrical interpretations of the correlation functions. Consider an epoxy matrix containing spherical silica particles, a two-phase composite used commonly in the electronics industry. If we take a large group of the material samples, each has the same particle content and a volume V large enough to contain many particles, we can, in principle, compute the one-point correlations Pr(x) (r ⫽ 1, 2) by knowing the distribution density p(␣) and the characteristic function ƒr(x, ␣). Let r ⫽ 1 be the matrix phase and r ⫽ 2 be the particle phase. If we found that P2(x) is a constant (i.e., independent of x), then we can say that the particles are uniformly distributed through each sample. This is because P2(x) ⫽ const. means that the chance of ﬁnding a particle is the same everywhere in V. Note that this does not necessarily mean that the particles are everywhere in V. It just gives us a sense of how ‘‘uniformly’’ the particles are distributed. Next, we take x to be the center of a particle and x⬘ to be the center of another particle, and compute P22(x, x⬘). Let us assume that it satisﬁes P22(x, x⬘) ⫽ P22(x ⫺ x⬘), that is, the two-point correlation function P22(x, x⬘) depends only on the distance between the two points, regardless where these two points are located. What that means is that if one takes a measuring stick shorter than the smallest dimension of V, and places the stick inside V, the chance that there is a particle at each end of the stick is the same regardless of where the stick is placed. The other two-point correlation functions P11(x, x⬘), P12(x, x⬘), and P21(x, x⬘) can be interpreted similarly. Clearly the twopoint correlation functions give us another measure of the ‘‘uniformity’’ of the heterogeneous materials. Said differently, if a material is statistically uniform, then its correlation functions Pr(x), Prs(x, x⬘), and so forth are insensitive to translation, that is, Pr(x) reduces to a constant, Prs(x, x⬘) becomes a function of (x ⫺ x⬘) only, and so on. More generally, in micromechanics, a heterogeneous medium is called statistically homogeneous (or uniform) of grade k if the correlation functions up to the k point are all translation invariant. Since it is very unlikely that enough information is available to computer the k-point correlation function for k greater than 2, in this book we will typically call a statistically homogenous of grade 2 simply statistically homogeneous. In what follows, we show that if the characteristic function of a heterogeneous material satisﬁes the ergodic hypothesis, the material is statistically homogeneous. To this end, consider the volume average of the characteristic function ƒr(x, ␣) for sample ␣:

5.3

ƒr(x, ␣) ⫽

1 V

RANDOM MEDIA

冕 ƒ (x, ␣) dV(x) ⫽ VV ⬅ c , r

V

r

r

107

(5.3.12)

where cr is the volume fraction of the rth phase in the heterogeneous material. The ergodic hypothesis thus means Pr(x) ⫽ 具ƒr(x, ␣)典 ⬅ ƒr(x, ␣) ⫽ cr .

(5.3.13)

Next, consider the volume average of the two-point correlation: ƒr(x, ␣)ƒs(x⬘, ␣) ⫽

1 V

冕 ƒ (x, ␣)ƒ (x⬘, ␣) dV(x). r

V

s

(5.3.14)

Let xⴖ ⫽ x ⫺ x⬘.

(5.3.15)

Then, we have 1 V

冕 ƒ (x, ␣)ƒ (x⬘, ␣) dV(x) ⫽ V1 冕 V

r

s

Vr

ƒs(x ⫺ xⴖ, ␣) dV(x) ⫽ grs(xⴖ), (5.3.16)

or ƒr(x, ␣)ƒs(x⬘, ␣) ⫽ grs(xⴖ) ⫽ grs(x ⫺ x⬘).

(5.3.17)

Therefore, according to the ergodic hypothesis, Prs(x, x⬘) ⫽ 具ƒr(x, ␣)ƒs(x⬘, ␣)典 ⫽ ƒr(x, ␣)ƒs(x⬘, ␣) ⫽ grs(x ⫺ x⬘). This completes the proof. We can summarize the foregoing discussions as follows: 1. The microstructure or the distribution of heterogeneities in a heterogeneous material can be characterized quantitatively by the correlation functions Pr(x), Prs(x, x⬘), and so forth, which are the ensemble average of the characteristic function ƒr(x, ␣).

108

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

2. The heterogeneous material is considered statistically homogeneous if the correlation functions are translation invariant, that is, Pr(x) ⫽ cr, Prs(x, x⬘) ⫽ grs(x ⫺ x⬘), and so forth. 3. If the correlation functions are ergodic, that is, the ensemble average equals the volume average, then they are translation invariant. Therefore, if the correlation functions of a heterogeneous material are ergodic, the material is considered statistically homogeneous. Having considered the random media and introduced the concepts of ergodicity and statistical homogeneity, we can now give the representative volume element (RVE) a more precise deﬁnition. To deﬁne the length scale corresponding to the properties of interest, we need to select an RVE of the heterogeneous material in question. The size of the RVE must be such that it includes a very large number of inhomogeneities and in the meanwhile be statistically homogeneous and representative of the local continuum properties, so that appropriate averaging schemes over these domains give rise to the same mechanical properties, corresponding to the overall or effective mechanical properties. Finally, to close this section, we mention that in the rest of this book, we will be mainly concerned with the statistically homogeneous media. Therefore, it will be assumed implicitly, unless indicted otherwise, that the ensemble average and the volume average are the same, that is, 具h(x)典 ⫽

冕 h(x, ␣) d␣ ⫽ V1 冕 h(x, ␣) dV(x) ⫽ h(␣),

(5.3.18)

V

R

where h(x, ␣) can be either a scalar or a tensor function. 5.4 MACROSCOPIC AVERAGES

In this section, attention is focused on developing averaging theorems devoted to heterogeneous materials with arbitrary constituents independent of their thermomechanical behavior. The average stresses over a domain D is deﬁned as ij ⫽

1 D

冕 D

ij

dV,

or ⫽

1 D

冕 dV. D

Similarly, the average strain over in a domain D is deﬁned as

(5.4.1)

5.4

ij ⫽

1 D

冕 D

ij

dV,

109

MACROSCOPIC AVERAGES

or ⫽

冕 dV.

1 D

(5.4.2)

D

In these deﬁnitions, the domain D does not need to be homogeneous, nor does it need to be a single domain. Note that, as mentioned earlier, the volume average and ensemble average are the same for statistically homogeneous materials. Average-Stress Theorem Let 0ij be a given constant stress tensor and S be the entire boundary of a domain D with outward normal nj. If ij nj兩S ⫽ pj0 ⫽ ij0 nj

(5.4.3)

is prescribed on S, then the average stress on D is given by ij ⫽ ij0 .

(5.4.4)

To prove this theorem, consider the deﬁnition of average stress: ij ⫽

冕

1 D

ij

D

dV ⫽

1 D

冕 ␦

dV.

ik jk

D

(5.4.5)

Note that xj,k ⫽ ␦jk, so ij ⫽

1 D

冕x

dV ⫽

ik j,k

D

1 D

冕 [( x )

ik j ,k

D

⫺ ik,k] dV.

(5.4.6)

When there is no body force as assumed here, the second term in the above integral vanishes. Making use of the divergence theorem and then the traction boundary condition (5.4.3), we have ij ⫽

1 D

冕 x n dS ⫽ D1 冕 x n dS. S

ik j

k

0 ik

S

j

k

(5.4.7)

Making use of the divergence theorem again leads to ij ⫽ ik0

1 D

冕x D

j,k

dV ⫽ ik0

1 D

冕␦ D

jk

dV ⫽ ij0.

This completes the proof of the average stress theorem.

(5.4.8)

110

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

What the average stress theorem tells us is that when a body is subjected to the traction boundary condition (5.4.3) with 0ij being a constant stress tensor, the stress averaged over the entire body is the same as 0ij, regardless the complexity of the stress ﬁeld within the domain. Therefore, in the rest of this book, traction boundary conditions will be written as ij nj兩S ⫽ ij nj,

(5.4.9)

with the understanding that ij is the average stress tensor in the body enclosed by S when (5.4.9) is applied. Average-Strain Theorem Let 0ij be a given constant strain tensor and S be the entire boundary of a domain D with outward normal nj. If ui兩S ⫽ ij0 xj

(5.4.10)

is given on S, then the average strain on D is given by ij ⫽ ij0 .

(5.4.11)

To prove this theorem, consider the deﬁnition of average strain:

冕 dV ⫽ 2D1 冕 (u ⫹ u ) dV 1 ⫽ 冕 u dV ⫹ 2D1 冕 u dV. 2D

ij ⫽

1 D

ij

D

D

i, j

D

i, j

D

j,i

j,i

(5.4.12)

Making use of the divergence theorem yields ij ⫽

1 2D

冕 u n dS ⫹ 2D1 冕 u n dS. S

i j

S

j

i

(5.4.13)

Substitute the boundary condition (5.4.10) into the above integrals:

5.5

ij ⫽

1 2D

111

HILL’S LEMMA

冕 x n dS ⫹ 2D1 冕 x n dS. S

0 ik k j

S

0 jk k i

Making use of the divergence theorem again, ij ⫽

1 2D

冕x D

0 ik k, j

dV ⫹

1 2D

冕x

0 jk k,i

D

dV ⫽

1 0 ( ⫹ ji0) ⫽ ij0. 2 ij (5.4.14)

This completes the proof of the average strain theorem. According to average strain theorem, if the displacements along the entire boundary of a given body is prescribed by (5.4.10) with 0ij being a constant strain tensor, then the strain ﬁeld averaged over the entire body is 0ij, regardless the complexity of strain ﬁeld within the body. Thus, in the rest of this book, displacement boundary conditions will be written as ui兩S ⫽ ij xj,

(5.4.15)

with the understanding that ij is the average strain tensor in the body enclosed by S when (5.4.15) is applied. 5.5

HILL’S LEMMA

Again, consider an RVE with volume V and boundary S. For any stress and strain ﬁelds ij and ij at a given point in the RVE under prescribed boundary traction or boundary displacement condition, one has the following result: ijij ⫺ ijij ⫽

1 D

冕 (u ⫺ x )( n ⫺ n ) dS, S

i

j ij

ik k

ik k

(5.5.1)

where the overbar stands for the volume average; for example, ijij ⫽

1 V

冕 V

ij ij

dv.

(5.5.2)

To prove Hill’s lemma, let us ﬁrst expand the integrand of the surface integral on the right-hand side of (5.5.1):

112

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

冕 (u ⫺ x )( n ⫺ n ) dS ⫽ 冕 (u n ⫺ u n ⫺ n x i

S

j ij

i

S

ik k

ik k

ik k

i k

ik

ik k j ij

⫹ xj nkijik) dS.

(5.5.3)

The following surface integrals can be easily evaluated:

冕 u n dS ⫽ 冕 u S

i

ik k

V

冕 un i k

S

ik

i, j

ij

冕

dV ⫽

dS ⫽ ik

V

冕u

i,k

V

ik k j

ik ik

V

冕 x n dS ⫽ 冕 ␦ S

j

k

V

jk

ij

dV ⫽ Dijij,

dV ⫽ Dikik,

冕 n x dS ⫽ 冕 ␦ S

ij

dV ⫽ Dij,

dV ⫽ D␦jk.

Substituting the above into (5.5.3) yields 1 D

冕 (u ⫺ x )( n ⫺ n ) dS ⫽ S

i

j ij

ik k

ik k

ij ij

⫺ ikik ⫺ ijij ⫹ ikik

⫽ ijij ⫺ ijij.

(5.5.4)

This proves Hill’s lemma (5.5.1). A corollary of Hill’s lemma can be stated as follows: ijij ⫽ ijij,

(5.5.5)

if ijnj兩S ⫽ ij nj, or ui兩S ⫽ ij xj. In other words, for statically admissible stress ﬁelds (ijnj兩S ⫽ ij nj), or kinematically admissible displacement ﬁelds (ui兩S ⫽ ij xj), the volume average of the product ijij is the same as the product of the volume averages ij and ij. Equation (5.5.5) is also known as Hill’s macrohomogeneity condition or Mandel–Hill condition. Note that ijij is twice the value of strain energy density, (5.5.5) implies that the volume-averaged strain energy density of a heterogeneous material can be obtained from the volume averages of the stresses and strains. Accordingly, homogenization can be interpreted as ﬁnding a homogeneous comparison material that is energetically equiv-

5.6

DEFINITIONS OF EFFECTIVE MODULUS OF HETEROGENEOUS MEDIA

113

alent to a given microstructured material. This idea will be used to deﬁne the effective properties of heterogeneous media next. 5.6 DEFINITIONS OF EFFECTIVE MODULUS OF HETEROGENEOUS MEDIA

In this section, we introduce the concept of effective modulus of a statistically homogeneous heterogeneous medium. It is assumed that such a medium can be represented by an RVE consisting of N distinct phases dispersed throughout the RVE as inhomogeneities (or heterogeneities) of dimension much less than the size of the RVE. For the moment, perfect bonding will be assumed across the interfaces between the different phases. Nonperfect interfaces will be considered in Chapter 10. Some common engineering materials are special cases of the heterogeneous material described in the preceding paragraph. For example, a polycrystalline material can be viewed as a heterogeneous material with inﬁnite (N ⫽ ⬁) number of distinct phases. Fiber- (particulate-) reinforced composites contain two distinct phases (N ⫽ 2), namely ﬁbers (particles) and the matrix. Heterogeneous materials with a distinct matrix phase are called composite materials. For convenience, body force is not considered in the remaining part of the book unless indicated otherwise. Consider a heterogeneous material D bounded by surface S. Assume that the heterogeneous material consists of randomly oriented and shaped inhomogeneities embedded in a matrix with stiffness tensor L0. Let the stiffness tenors of the inhomogeneities be L1, L2, L3, . . . , LN, as shown in Figure 5.1.

L( N ) L(2) L( r ) L(1)

L(0) Figure 5.1 Multiphase heterogeneous material.

114

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

A straightforward deﬁnition of the effective modulus (stiffness) tensor of the heterogeneous material is given by the following relationship: ⫽ L,

(5.6.1)

where and are, respectively, the average stress and strain tensors, and the fourth tensor L deﬁned by (5.6.1) is call the effective modulus or effective stiffness tensor of the heterogeneous material. Similarly, the effective compliance tensor of the heterogeneous material is deﬁned by ⫽ M,

(5.6.2)

where the fourth-order tensor M is called the effective compliance tensor of the heterogeneous material. Obviously, it follows from the definitions that LM ⫽ ML ⫽ I,

or L⫺1 ⫽ M.

(5.6.3)

Although such deﬁnitions stated above are straightforward, they are not very convenient to use. An alternative deﬁnition of the effective modulus tensor can be given based on the strain energy concept. To this end, let us consider two materials of the same geometry. One is a heterogeneous material, the other is a homogeneous one with stiffness tensor L, as shown in Figure 5.2. First, assume displacements are prescribed on the boundary of both materials, namely

L( N ) L(2) L

L( r )

L(1) L(0) (a)

(b)

Figure 5.2 (a) Heterogeneous material and (b) its comparison material.

5.6

DEFINITIONS OF EFFECTIVE MODULUS OF HETEROGENEOUS MEDIA

ui兩S ⫽ ij xj,

115

(5.6.4)

where ij, as discussed in the previous section, would be the average strain in both materials. The stiffness tensor L of the homogeneous material is said to be the effective stiffness tensor of the heterogeneous material shown in Figure 5.2(a) if and only if Uc ⫽ Uh,

(5.6.5)

where Uc and Uh are the strain energy stored in the heterogeneous material and in the homogeneous material, respectively. It can be easily shown that the two deﬁnitions of the stiffness tenor given above are equivalent. To this end, we calculate ﬁrst the strain energy stored in the composite: Uc ⫽

1 2

冕 D

ij ij

dv ⫽ Dijij.

(5.6.6)

Making use of (5.6.4) in conjunction with Hill’s lemma (5.5.5), we arrive at Uc ⫽

D . 2 ij ij

(5.6.7)

Uc ⫽

D . 2

(5.6.8)

In matrix notation, we have

For the homogeneous material, it is obvious the strain and stress ﬁelds are uniform when (5.6.4) is applied. They are ij ⫽ ij and ij ⫽ Lijklkl. So, the total strain energy of the homogeneous material is given by Uh ⫽ or in matrix notation

D D ⫽ ij Lijklkl, 2 ij ij 2

(5.6.9)

116

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

Uh ⫽

D L. 2

(5.6.10)

Comparing (5.6.8) with (5.6.10), we conclude that Uc ⫽ Uh for any arbitrary , if and only if ⫽ L. Consequently, we have proved that the two foregoing deﬁnitions of stiffness tenors for heterogeneous materials are equivalent. An alternative deﬁnition of the effective compliance tensor also can be given based on the strain energy concept. For example, consider the two materials shown in Figure 5.2. Assume that the homogeneous material has a compliance tensor M. This time let the traction ijnj兩S ⫽ ij nj be prescribed on the entire boundary of both materials. Then, the compliance tensor M is said to be the effective compliance tensor of the composite shown in Figure 5.2(a) if and only if Uc ⫽ Uh,

(5.6.11)

where again Uc and Uh are the strain energy stored in the composite and in the homogeneous material, respectively. Proof of the equivalency between this deﬁnition and the one given by (5.6.2) is straightforward; see Problem 5.1. Although the deﬁnition based on strain energy does not seem as straightforwards as the direct deﬁnition, it is nevertheless convenient for the determination of the effective properties, as will be seen in later chapters.

5.7 CONCENTRATION TENSORS AND EFFECTIVE PROPERTIES

Consider the composite material shown in Figure 5.2(a). Let the displacement boundary condition be given by ui兩S ⫽ ij xj.

(5.7.1)

Then, it follows from (5.4.11) that

冘 c , N

⫽

r r

r⫽0

(5.7.2)

5.7

CONCENTRATION TENSORS AND EFFECTIVE PROPERTIES

117

where r is the average strain on the rth inhomogeneity and cr is the volume fraction of the rth inhomogeneity. The case of r ⫽ 0 is for the matrix. Note that is the average strain of the entire composite material and r is the average strain of the rth inhomogeneity. Thus, a ‘‘strain concentration tensor’’ Ar (r ⬎ 0) can be deﬁned for the rth inhomogeneity through r ⫽ Ar.

(5.7.3)

Clearly, the ‘‘magnitude’’ of Ar represents the strain concentration on the inhomogeneity. Substituting (5.7.3) into (5.7.2) yields

冘 N

c00 ⫽ ⫺

冘 c A . N

crr ⫽ ⫺

r

r

(5.7.4)

r⫽1

r⫽1

Next, consider the average stress in the composite

冘 c ⫽ c L ⫹ 冘 c L , N

⫽

N

r

r

0

0 0

r

r

r

(5.7.5)

r⫽1

r⫽0

where r is the average stress tensor in the rth inhomogeneity, and Hooke’s law r ⫽ Lrr for each inhomogeneity has been used. Making use of (5.7.4) in (5.7.5) gives the following: ⫽

冤

L0 ⫹

冘 c (L ⫺ L )A 册. N

r

r

0

r

(5.7.6)

r⫽1

Comparing (5.7.6) with (5.6.1) leads to

冘 c (L ⫺ L )A . N

L ⫽ L0 ⫹

r

r

0

r

(5.7.7)

r⫽1

In other words, the effective stiffness tensor of a composite material can be expressed in terms of the stiffness tensors of the constituent materials, their corresponding volume fraction and the strain concentration tensors. Among these, the strain concentration tensor is the only unknown in typical engineering applications. Much of the effort in micromechanics has been devoted to ﬁnd ways to compute the con-

118

DEFINITIONS OF EFFECTIVE MODULI OF HETEROGENEOUS MATERIALS

centration tensor. Several of the most commonly used methods to approximate the concentration tensors are discussed in Chapters 7 and 8. Along a parallel path, it can be shown (Problem 5.2) that under the traction boundary condition ijnj兩S ⫽ ij nj, the effective compliance tensor of a composite is given by

冘 c (M ⫺ M )B , N

M ⫽ M0 ⫹

r

r

0

(5.7.8)

r

r⫽1

where Br is the stress concentration tensor for the rth inhomogeneity, that is, r ⫽ Br,

(5.7.9)

where r is the average stress in the rth inhomogeneity and is the average stress over the entire composite. The concentration tensors introduced above represent the stress– strain concentration of the rth inhomogeneity with respect to the average strain over the entire sample. It can be regarded as the global concentration tensors. Since the composite has a distinctive matrix phase in which all the other inhomogeneities are embedded, one can also introduce the local concentration tensors through r ⫽ Gr0

and r ⫽ Hr0

(5.7.10)

where 0 and 0 are, respectively, the average strain and average stress tensor in the matrix phase. Clearly, Gr and Hr are, respectively, the strain and stress concentration tensors of the rth inhomogeneity with respect to the average strain and stress in the matrix immediately surrounding itself. To ﬁnd the relationship between the local and global concentration tensors, consider the average strain:

冘 c ⫽ c ⫹ 冘 c ⫽ c ⫹ 冘 cG ⫽ 冋c I ⫹ 冘 c G 册 . N

N

⫽

r r

0 0

N

r r

r⫽1

r⫽0

0 0

r

r 0

r⫽1

N

0

r

r⫽1

This yields

r

0

(5.7.11)

SUGGESTED READING

0 ⫽

冋

册

冘

⫺1

N

c0I ⫹

119

.

cnGn

n⫽1

(5.7.12)

Substitution of the above equation into (5.7.10) results in

冋

冘cG册

⫺1

N

r ⫽ Gr c0I ⫹

n

.

n

(5.7.13)

n⫽1

Comparing this to the deﬁnition of global concentration tensor (5.7.3) leads to

冋

r⫽1

冋

冘cH册

Ar ⫽ Gr c0I ⫹

冘 cG册

⫺1

N

r

.

r

(5.7.14)

Similarly, one can show that Br ⫽ Hr c0I ⫹

⫺1

N

n

n

.

(5.7.15)

n⫽1

Because of these relationships, the knowledge of the local concentration tensors is sufﬁcient to determine the effective stiffness (compliant) tensor of the composite. PROBLEMS

5.1 Prove the equivalency between the two deﬁnitions of the effective compliance tensor. 5.2 Assume that a composite is subjected to the traction boundary condition ijnj兩S ⫽ ijnj. Show Eq. (5.7.8). 5.3 Derive (5.7.15). SUGGESTED READING Krajinovic, D. (1996). Damage Mechanics, Elsevier, New York, Chapter 1. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston. Nemat-Nasser, S. and Hori, M. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York, Chapter 1. Torquato, S. (2001). Random Heterogeneous Materials: Microstructure and Macroscopic Properties, Springer, New York.

6 BOUNDS FOR EFFECTIVE MODULI Obtaining the effective modulus tensor of a heterogeneous material is often a very difﬁcult task. In most cases, only approximate solutions can be found. Several of these approximate estimates will be discussed in Chapters 7–9. Although exact solutions to the effective moduli may not be found easily, for all practical purposes, knowing the bounds for these moduli is enough. In this chapter, some of these bounds are derived based on variation principles.

6.1 CLASSICAL VARIATIONAL THEOREMS IN LINEAR ELASTICITY

To prepare for the study of bounds of the effective properties of composite materials, we state here, without proof, two of the classical variational theorems in linear elasticity. Minimum Potential Energy Theorem Among all the kinematically admissible displacement ﬁelds, the true solution makes the following potential energy minimum: ⌸[ui] ⫽

1 2

冕L D

u u d ⫺

ijkl k,l i, j

冕

S

p0i ui ds,

(6.1.1)

where D is the total volume, and S is the portion of the boundary of D where traction p0i is prescribed. 120

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

6.1

CLASSICAL VARIATIONAL THEOREMS IN LINEAR ELASTICITY

121

Minimum Complementary Energy Theorem Among all the statically admissible stress ﬁelds, the true solution makes the following complementary energy minimum: ⌸c[ij] ⫽

1 2

冕M D

冕

klij d ⫺

ijkl

Su

ui0ij nj ds,

(6.1.2)

where D is the total volume, and Su is the portion of the boundary of D where displacement u0i is prescribed. It should be mentioned that the stiffness tensor L, and the compliance tensor M in the above theorems need not be uniform throughout D, meaning that both theorems are applicable to heterogeneous materials. In what follows, we will derive, based on the above theorems, some variational principles that are convenient to use for obtaining the bounds of effective properties. To begin, consider the heterogeneous material considered in Section 5.6. Let the displacement be prescribed on the boundary S: ui兩S ⫽ ij xj,

(6.1.3)

where ij is a constant strain tensor, which, according to the average strain theorem (5.4.11), is also the average in the composite under such boundary condition: ij ⫽

1 D

冕 D

ij

d.

(6.1.4)

Therefore, the overbar on the strain tensor causes no confusion between the given strain tensor on the boundary and the average strain tensor in D since they are the same. Under the displacement boundary condition (6.1.3), the potential energy of the composite, following (6.1.1), can be written as ⌸[ui] ⫽

1 2

冕L D

u u d ⫽

ijkl k,l i, j

1 2

冕L D

d,

ijkl kl ij

(6.1.5)

since no traction is prescribed. To facilitate the following discussions, we will denote the actual displacement ﬁeld by ui and any kinematically admissible displacement ﬁeld by uˆ i. Clearly, under the displacement

122

BOUNDS FOR EFFECTIVE MODULI

boundary condition, all kinematically admissible displacement (the actual displacement included) ﬁelds must satisfy (6.1.3). Let U be the average strain energy density in the heterogeneous material when it is subjected to (6.1.3): U⫽

1 2D

冕L

d ⫽

ijkl kl ij

D

1 L , 2 ij ijkl kl

(6.1.6)

where Lijkl is the effective stiffness tensor of the heterogeneous material and the last equality follows from (5.6.6). Then, according to the minimum potential energy theorem, the following inequality holds for any kinematically admissible displacement ﬁeld uˆ i: Uⱕ

冕L

1 2D

uˆ uˆ d.

(6.1.7)

ijkl k,l i, j

D

Now, consider the complimentary energy. Again, under the displacement boundary condition (6.1.3), the complimentary energy becomes ⌸c[ij] ⫽

1 2

冕M

klij d ⫺

ijkl

D

冕 x n ds. S

ik k

ij

j

(6.1.8)

Upon the use of the divergence theorem on the second term, ⌸c[ij] ⫽

1 2

冕M

klij d ⫺

ijkl

D

冕 ( x ) ds. D

ik k

ij j

(6.1.9)

For any statically admissible stress ﬁeld, that is, ij, j ⫽ 0, the above reduces to ⌸c[ij] ⫽

1 2

冕M D

klij d ⫺ ij

ijkl

冕 D

ij

d,

(6.1.10)

where ij is the average stress in D, ij ⫽

1 D

冕 D

ij

d.

(6.1.11)

Let ij be the actual stress ﬁeld and ˆ ij be any kinematically admissible stress ﬁeld. Then, by making use of Hooke’s law, ij ⫽ Mijklkl, we can show, following the steps described in (5.6.6) and (5.6.7), that

6.2

⌸c[ij] ⫽

1 2

VOIGT UPPER BOUND AND REUSS LOWER BOUND

冕M D

klij d ⫺ ij

ijkl

冕

d ⫽ ⫺DU,

ij

D

123

(6.1.12)

where U is the average strain energy density as introduced in (6.1.7). Thus, according to the minimum complimentary energy theorem, the following inequality holds for any statically admissible stress ˆ ij: U ⱖ ij

1 D

冕 ˆ D

ij

d ⫺

1 2D

冕M D

ˆ klˆ ij d.

ijkl

(6.1.13)

Combining (6.1.7) and (6.1.13), we arrive at the following inequalities, in matrix notations:

冕 ˆ d ⫺ 冕 ˆ Mˆ d ⱕ 2DU ⱕ 冕 ˆ Lˆ d, D

D

(6.1.14)

D

where ˆ ij can be any stress ﬁeld that satisﬁes ˆ ij, j ⫽ 0

in D,

(6.1.15)

and ˆ ij ⫽ (ˆui, j ⫹ uˆ j,i) /2 with uˆ i being any displacement ﬁeld that satisﬁes uˆ i ⫽ ij xj on S.

(6.1.16)

6.2 VOIGT UPPER BOUND AND REUSS LOWER BOUND

Again, consider the heterogeneous material discussed in Section 5.6. Let the heterogeneous material be subjected to the displacement boundary condition, ui ⫽ ij xj on S,

(6.2.1)

where ij is a given constant strain tensor. According to the average strain theorem stated in Section 5.4, the average strain in D is also ij. Next, we deﬁne uˆ i ⫽ ij xj everywhere in D.

(6.2.2)

Obviously, the uˆ i so deﬁned is a kinematically admissible displacement ﬁeld, that is,

124

BOUNDS FOR EFFECTIVE MODULI

uˆ i ⫽ ij xj on S.

(6.2.3)

The kinematical admissible strain ﬁeld corresponding to uˆ i is simply ij. Further, for the boundary condition (6.2.1), any constant stress tensor ˆ ij would be a statically admissible stress ﬁeld. Thus, by substituting (6.2.2) and a constant tensor ˆ ij into (6.1.14) yields 2 ˆ ⫺ ˆ MR ˆ ⱕ 2U ⱕ L⬘,

(6.2.4)

where LV ⫽

1 D

冕 L d,

MR ⫽

D

1 D

冕 M d.

(6.2.5)

D

Since ˆ can be any constant stress tensor, we should try to select one that maximizes the far left-hand side of (6.2.4) to obtain the optimal lower bound. It turns out that ˆ ⫽ LR ⫽ (MR)⫺1

(6.2.6)

would be the choice. Substituting (6.2.6) and (6.1.6) into (6.2.4), we obtain the following: LR ⱕ L ⱕ LV ,

(6.2.7)

where R ⫺1

L ⫽ (M ) R

冋

1 ⫽ D

冕 M d册

⫺1

;

(6.2.8)

D

These inequalities must hold true for any constant strain tensor . Therefore, we conclude LR ⱕ L ⱕ LV,

(6.2.9)

where LV deﬁned by the ﬁrst of (6.2.5) is called the Voigt upper bound, and LR deﬁned by (6.2.8) is called the Reuss lower bound. If the stiffness tensor of the rth phase of volume ⍀r is uniform and given by Lr , where r ⫽ 0, 1, . . . , N (r ⫽ 0 corresponds to the matrix), then the ﬁrst of (6.2.5) can be simpliﬁed to

6.2

VOIGT UPPER BOUND AND REUSS LOWER BOUND

冘cL,

125

N

LV ⫽

r

(6.2.10)

r ⫽ 1, 2, . . . , N

(6.2.11)

r

r⫽0

where cr ⫽

⍀r

D

,

are the volume fraction of the inhomogeneities with stiffness tensor Lr. Obviously, we have the relationship

冘 c ⫽ 1. N

(6.2.12)

r

r⫽0

Equation (6.2.10) gives the Voigt upper bound for the effective stiffness tensor of a composite with N distinct phases. Similarly, (6.2.8) can be written as

冋冘 册

⫺1

N

L ⫽ R

cr Mr

,

(6.2.13)

r⫽0

where Mr is the compliance tensor for the rth phase. It is noted that the bounds are derived in terms of the volume faction of each phase only. Therefore, they are independent of the geometry of the phases and their distribution. Example 6.1 Consider an isotropic matrix of stiffness tensor L0 ⫽ (3K0, 20) reinforced by particles of stiffness tensor L1 ⫽ (3K1, 21). We are to ﬁnd the bounds of the effective elastic constants. To solve this problem, let us ﬁrst consider the compliance tensors. Following the rules discussed in Section 1.4: M0 ⫽ Thus,

冉

冊

1 1 , , 3K0 20

M1 ⫽

冉

冊

1 1 , . 3K1 21

(6.2.14)

126

BOUNDS FOR EFFECTIVE MODULI

⫺1

[c0M0 ⫹ c1M1]

冉 冉

c0 c c c ⫽ ⫹ 1, 0 ⫹ 1 3K0 3K1 20 21 ⫽

冊

⫺1

冊

3K0K1 201 , . c0K1 ⫹ c1K0 c01 ⫹ c10

(6.2.15)

According to (6.2.9), the effective stiffness tensor of the composite satisﬁes the inequality [c0M0 ⫹ c1M1]⫺1 ⱕ L ⫽ (3K, 2) ⱕ c0L0 ⫹ c1L1,

(6.2.16)

where K and are the effective bulk and shear moduli of the composite, respectively, and c1 is the volume fraction of the particles. Making use of (6.2.15) in (6.2.16), we have K0K1 ⱕ K ⱕ K0 ⫹ c1(K1 ⫺ K0), K1 ⫺ c1(K1 ⫺ K0)

(6.2.17)

01 ⱕ ( ⱕ 0 ⫹ c1(1 ⫺ 0). 1 ⫺ c1(1 ⫺ 0)

(6.2.18)

These give the upper and lower bounds for the effective bulk and shear moduli of the composite.

6.3 EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

It is noted that the Voigt upper and the Reuss lower bounds were obtained by specifying a kinematically admissible displacement ﬁeld in the potential energy and by specifying a statically admissible stress ﬁeld in the complimentary energy. In other words, the key to ﬁnd bounds is to ﬁnd suitable admissible ﬁelds. In fact, this approach is rather general. Tighter bounds can be derived by specifying kinematically and statically admissible ﬁelds that make some explicit allowance for the microstructure of the composite. To this end, let us ﬁrst try to develop an alternative form of the classical variational principles that are better suited for developing bounds of the effective properties of heterogeneous materials. For the heterogeneous material considered in Section 5.6, we assume that the following displacement boundary condition is prescribed:

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

ui ⫽ ij xj on S.

127

(6.3.1)

Our objective is to ﬁnd a kinematically admissible displacement ﬁeld (rather than a constant tensor as in the Voigt upper bound) and a statically admissible stress tensor (rather than a constant tensor as in the Reuss lower bound) for this heterogeneous material under the boundary condition (6.3.1). To this end, let us write the elastic stiffness tensor of the heterogeneous material in the following form: L(x) ⫽ Lh ⫹ L p(x),

(6.3.2)

where it is understood that L(x) is a function of position vector x, Lh is a constant fourth-order tensor representing a homogeneous material, and L p(x), being the difference between L(x) and Lh, is also a function of position vector x, representing the perturbation from the homogeneous material. The constant stiffness tensor Lh is introduced to represent a homogeneous ‘‘comparison’’ material. The corresponding actual stress ﬁeld in the heterogeneous material is then given by (x) ⫽ Lh(x) ⫹ (x),

(6.3.3)

where ij (x) ⫽

冉

冊

1 ⭸ui(x) ⭸uj(x) ⫹ 2 ⭸xj ⭸xi

(6.3.4)

is the actual strain tensor in D and (x) ⫽ L p(x)(x)

(6.3.5)

is called the stress polarization in some of the literature. Clearly, (x) is symmetric, that is, ij(x) ⫽ ji(x), because of the symmetry of L p(x). In light of (6.3.3), the equations of equilibrium in terms of the displacement can be written as Lhijkluk,lj (x) ⫹ ij, j (x) ⫽ 0

in D.

(6.3.6)

If we treat the second term on the left-hand side as a body force, the solution to the boundary value problem (6.3.1) and (6.3.6) can be attained in terms of Green’s function; see (2.6.51):

128

BOUNDS FOR EFFECTIVE MODULI

冕L

ui(x) ⫽

h pjkl

S

⭸Gki(x, y) pq yq nj dS(y) ⫹ ⭸xl

冕 G (x, y) ⭸⭸y(y) dV(y), mn

mi

D

n

(6.3.7) where Gmi(x, y) is Green’s function in the homogeneous comparison material satisfying h Lijkl

⭸2Gkm,lj (x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl ⭸xj

in V,

Gij (x, y)兩x僆S ⫽ 0.

(6.3.8) (6.3.9)

By using the divergence theorem and (6.3.8), the surface integral in (6.3.7) can be simpliﬁed to

冕L S

⭸Gki(x, y) pq yq nj dS(y) ⭸xi

h pjkl

冕L

⫽⫺ ⫽

h pjkl

D

⭸2Gki(x, y) y dV(y) ⫹ ⭸xl ⫹ ⭸yj pq q

冕 ␦ ␦(x, y) D

pi

y dV(y) ⫹

pq q

冕L

冕L

h pjkl

D

⭸Gki(x, y) pj dV(y) ⭸xl

Gki(x, y)pj nj dS(y)

h pjkl

S

⫽ iq xq.

(6.3.10)

Substituting (6.3.10) into (6.3.7) and applying the divergence theorem to the volume integral in conjunction with (6.3.9), we have

冕 G (x, y) ⭸⭸y(y) dV(y) ⭸G (x, y) ⫽ x ⫺冕 (y) dV(y). y

ui(x) ⫽ iq xq ⫹

mn

D

mi

n

mi

iq q

mn

D

(6.3.11)

n

The displacement gradient is thus given by ui, j (x) ⫽ ij ⫺

冕 ⭸ G⭸x(x⭸y⫺ y) 2

mi

D

(y) dV(y).

mn

j

n

The strain tensor follows (6.3.12) readily,

(6.3.12)

6.3

ij (x) ⫽ ij ⫺

1 2

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

冕 冉⭸ G⭸x(x⭸y⫺ y) ⫹ ⭸ G⭸x(x⭸y⫺ y)冊 2

2

mj

mi

D

129

j

n

i

mn

(y) dV(y),

n

(6.3.13) Using the symmetry properties of mn(y), we can rewrite the above into (x) ⫽ ⫺

冕 ⌫(x, y)(y) dV(y),

(6.3.14)

D

where ⌫ijkl(x, y) 1 ⭸2Gki(x ⫺ y) ⭸2Gkj (x ⫺ y) ⭸2Gli(x ⫺ y) ⭸2Glj (x ⫺ y) ⫽ ⫹ ⫹ ⫹ . 4 ⭸xj ⭸yl ⭸xi ⭸yl ⭸xj ⭸yk ⭸xi ⭸yk

冋

册

(6.3.15) Since the integral operator in (6.3.14) will be used many times, we will, for convenience, use the following symbolic notation to indicate the integration operation:

冕 ⌫(x, y)(y) dV(y) ⬅ ⌫(x, y) * (y).

(6.3.16)

D

Using this notation, (6.3.14) can be awritten as (x) ⫽ ⫺ ⌫(x, y) * (y).

(6.3.17)

Before proceeding forward, we note that the integral operator is selfadjoint, that is, (x) * [⌫(x, y) * (y)] ⫽ (x) * [⌫(x, y) * (y)].

(6.3.18)

This can be readily proven by noting that ⌫(x, y) ⫽ ⌫(y, x).

Further, we have

(6.3.19)

130

BOUNDS FOR EFFECTIVE MODULI

冕 ⌫(x, y) dV(y) ⫽ 0,

⌫(z, x) * Lh⌫(x, y) ⫽ ⌫(z, y).

D

(6.3.20)

The ﬁrst of (6.3.20) can be veriﬁed by noting, for example,

冕 ⭸ G⭸x (x,⭸y y) dV(y) ⫽ ⭸⭸x 冕 ⭸G ⭸(x,y y) dV(y) ⭸ ⫽ 冕 G (x, y)n dS(y) ⫽ 0. ⭸x 2

ki

D

ki

j

l

j

D

j

S

l

ki

l

(6.3.21)

The second of (6.3.20) can be veriﬁed by noting, for example,

冕 ⭸ G⭸x (z,⭸z x) L ⭸ G⭸x (x,⭸y y) dV(x) ⭸G (x, y) ⭸ ⭸G (z, x) ⫽ 冕 L dV(x) ⭸z ⭸y ⭸x ⭸x ⭸G (x, y) ⭸ ⭸ ⫽ 冕 G (z, x)L 再 冋 册 ⭸z ⭸y ⭸x ⭸x 2

2

ki

D

pm

h klmn

l

j

n

q

2

ki

j

q

D

pm

h klmn

l

n

2

j

D

q

l

⫺ Gki(z, x)Lhklmn ⭸2 ⫽⫺ ⭸zj ⭸yq ⫽

⭸2 ⭸zj ⭸yq

h klmn

ki

冕 G (z, x)L

h klmn

ki

D

冎

⭸Gpm(x, y) ⭸xn ⭸xl

pm

n

dV(x)

⭸Gpm(x, y) dV(x) ⭸xn ⭸xl

冕 G (z, x)␦ ␦(x ⫺ y) dV(x) ki

D

kp

⭸2Gpi(z, y) ⫽ . ⭸zj ⭸yq

(6.3.22)

Let us now consider (6.3.11). Because of (6.3.9), we have ui(x)兩x僆S ⫽ iq xq兩x僆S ⫹

冕 G (x, y)兩 D

mi

x僆S

⭸mn(y) dV(y) ⫽ iq xq兩x僆S, ⭸yn

regardless of the choice of (y). In other words, for any given ˆ (y), the displacement derived from (6.3.11), therefore, the corresponding strain derived from (6.3.17),

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

ˆ (x) ⫽ ⫺ ⌫(x, y) * ˆ (y)

131

(6.3.23)

are kinematically admissible displacement and strain ﬁelds, respectively. Therefore, the minimum potential energy theorem (6.1.7) leads us to the following inequality: 2DU ⱕ

冕 ˆ Lˆ d ⫽ 冕 ˆ L ˆ d ⫹ 冕 ˆ L ˆ d. h

D

p

D

(6.3.24)

D

Substitute (6.3.23) into (6.3.24) and make use of properties of the integral operator ⌫(x, y), and (6.3.19) and (6.3.20), we arrive at the following inequality: 2D(U ⫺ Uh) ⱕ

冕 ˆ ⌫(x, y) * ˆ(y) d ⫹ 冕 L d ⫺ 2 冕 L ⌫(x, y) * ˆ (y) d ⫹ 冕 ⌫(x, y) * ˆ (y)L ⌫(x, y) * ˆ (y) d, p

D

D

p

D

p

D

(6.3.25)

where Uh ⫽

1 2D

冕 L d. h

(6.3.26)

D

Through a straightforward simpliﬁcation, one can show that the last term in (6.3.25) can be rewritten as

冕 ⌫(x, y) * ˆ(y)L ⌫(x, y) * ˆ(y) d ⫽ 冕 [ˆ]L [ˆ] d ⫺ 冕 ˆ (L ) ˆ d ⫺ 2 冕 ˆ ⌫(x, y) * ˆ (y) d ⫺ 冕 L d ⫹ 2 冕 {ˆ ⫹ L ⌫(x, y) * ˆ (y)} d, p

D

p ⫺1

p

D

D

p

D

D

p

D

(6.3.27)

where [ˆ] ⫽ (L p)⫺1ˆ ⫹ ⌫(x, y) * ˆ (y) ⫺ .

(6.3.28)

132

BOUNDS FOR EFFECTIVE MODULI

Substituting (6.3.27) into (6.3.25), we obtain, for any stress tensor ˆ , the desired inequality, 2D(U ⫺ Uh) ⱕ ⫺H[ˆ] ⫹

冕 [ˆ]L [ˆ] d, p

(6.3.29)

D

where H[ˆ] ⫽

冕 ˆ [ˆ] d ⫺ 冕 ˆ d. D

(6.3.30)

D

Next, we want to know what happens if the ˆ in (6.3.29) is indeed the actual stress polarization tensor of the problem, that is, ˆ ⫽ . In this case, we have, from (6.3.5) and (6.3.17), that [] ⫽ (L p)⫺1 ⫹ ⌫(x, y) * (y) ⫺ ⫽ 0,

(6.3.31)

therefore, the second term on the right-hand side of (6.3.29) would vanish. Further

冕 d ⫽ ⫺冕 (L ⫺ L ) d ⫽ ⫺2D(U ⫺ U ).

H[] ⫽ ⫺

h

D

D

h

(6.3.32)

In other words, the right-hand side of (6.3.29) is minimized if ˆ ⫽ is used, and the minimum value is equal to the left-hand side, 2D(U ⫺ Uh). We can now summarize the above derivations. First, once Lh is selected, the perturbed part of the stiffness tensor L p and Green’s function ⌫(x, y) can be computed from (6.3.2) and (6.3.8) and (6.3.9). Second, displacement ui generated from (6.3.11) is a kinematically admissible displacement ﬁeld, which leads the minimum potential energy theorem to the inequality (6.3.29). Third, the inequality is valid for any stress tensor ˆ . Finally, the equal sign is realized when ˆ is replaced by the actual solution to the stress polarization tensor of the problem. Therefore, we have just proved the following theorem. Theorem 6.1 Among all the symmetric second-order tensors, the true solution to the stress polarization tensor ˆ renders the following functional minimum:

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

I[ˆ] ⫽ Uh ⫺

1 1 H[ˆ] ⫹ 2D 2D

冕 [ˆ]L [ˆ] d, p

133

(6.3.33)

D

and the minimum value of I[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{I[ˆ]} ⫽ –12 L.

(6.3.34)

The inequality (6.3.29) can be further simpliﬁed if one assumes that L is negative semideﬁnite, that is, for any , p

冕 [ˆ]L [ˆ] d ⱕ 0. p

(6.3.35)

D

In this case, (6.3.29) reduces to 2D(U ⫺ Uh) ⱕ ⫺H[ˆ].

(6.3.36)

Therefore, we have the following theorem. Theorem 6.1a (Hashin–Shtrikman Variational Principle) When L p is negative semideﬁnite, among all the symmetric second-order tensors, the true solution to the stress polarization tensor ˆ renders the following functional minimum: Ih[ˆ] ⫽ Uh ⫺

1 H[ˆ], 2D

(6.3.37)

and the minimum value of Ih[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Ih[ˆ]} ⫽ –21 L.

(6.3.38)

Let us now turn to the complimentary energy principle. Introducing (6.3.17) to (6.3.3) yields

134

BOUNDS FOR EFFECTIVE MODULI

(x) ⫽ Lh ⫺ Lh

冕 ⌫(x, y)(y) dV(y) ⫹ (x).

(6.3.39)

D

Thus, it follows from, for example,

冕 冉⭸⭸x L ⭸ G⭸x (x,⭸y y)冊 (y) dV(y) ⭸ ⭸ G (x, y) ⫽冕 L (y)冊 dV(y) 冉 ⭸y ⭸x ⭸x ⭸ G (x, y) ⫺冕 L (y) dV(y) ⭸x ⭸x ⭸ G (x, y) ⭸ G (x, y) ⫽冕 L n dS(y) ⫺ 冕 L (y) dV(y) ⭸x ⭸x ⭸x ⭸x ⭸ G (x, y) ⫽ ⫺冕 ␦ ␦(x ⫺ y)n dS(y) ⫺ 冕 L (y) dV(y) ⭸x ⭸x ⭸ G (x, y) ⫽ ⫺冕 L (y) dV(y) ⭸x ⭸x 2

D

km

h ijmn

kl

j

n

l

2

km

h ijmn

D

kl

l

n

j

2

km

h ijmn

D

kl,l

n

j

2

h ijmn

S

2

km

l

n

D

j

km

h ijmn

kl,l

n

j

2

S

ik

l

D

h ijmn

km

kl,l

n

j

2

D

h ijmn

km

kl,l

n

j

that div((x)) ⫽ Lh

冕 ⌫(x, y)div((y)) dV(y) ⫹ div((x)).

(6.3.40)

D

One may then conclude that for any statically admissible stress tensor ˆ (x), that is, div((x)) ⫽ 0, the stress tensor ˆ (x) generated from (6.3.3) ˆ (x) ⫽ Lh(x) ⫹ ˆ (x),

(6.3.41)

is also a statically admissible stress ﬁeld, that is, div( ˆ (x)) ⫽ div(Lh(x) ⫹ ˆ (x)) ⫽ div(Lh(x)) ⫽ 0.

(6.3.42)

Having established that ˆ (x) is statically admissible, whenever ˆ (x) is, we can now consider (6.1.13) for a statically admissible ˆ (x),

6.3

EXTENSIONS OF CLASSICAL VARIATIONAL PRINCIPLES

冕 ˆ d ⫺ 冕 ˆ Mˆ d ⫽冕 ˆ d ⫺ 冕 ˆ (M ⫹ M ) ˆ d,

2DU ⱖ

D

D

D

D

h

p

135

(6.3.43)

where, analogous to (6.3.2), the compliance tensor is written as M(x) ⫽ Mh ⫹ Mp(x),

(6.3.44)

and the superscripts on the compliance tensors carry the same meaning as those for the stiffness tensors. Substituting (6.3.41) into (6.3.43), following similar steps in deriving (6.3.29) and making use of the identity, LhMp ⫹ L p(Mh ⫹ Mp) ⫽ 0,

(6.3.45)

we conclude that 2D(U ⫺ Uh) ⱖ ⫺H[ˆ] ⫺

冕 L [ˆ]M L [ˆ] d, h

p

h

(6.3.46)

D

for any statically admissible stress tensor ˆ (x). As shown earlier, if ˆ (x) happens to be the true stress polarization to the deformation problem considered here, the equal sign in (6.3.46) holds. We have just proved the following variational theorem. Theorem 6.2 Among all the statically admissible stress ﬁelds, the true solution renders the following functional maximum, Ic[ˆ] ⫽ Uh ⫺

1 1 H[ˆ] ⫺ 2D 2D

冕 L [ˆ]M L [ˆ] d, h

p

h

(6.3.47)

D

and the maximum value of Ic[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Ic[ˆ]} ⫽ –12 L.

(6.3.48)

If Mp is negative semideﬁnite (or, equivalently, L p is positive semideﬁnite), that is,

136

BOUNDS FOR EFFECTIVE MODULI

冕 L [ˆ]M L [ˆ] d ⱕ 0, h

p

h

D

then (6.3.46) implies 2D(U ⫺ Uh) ⱖ ⫺H[ˆ].

(6.3.49)

This leads to another form of the Hashin–Shtrikman variational principle. Theorem 6.2a (Hashin–Shtrikman Variational Principle) Among all the statically admissible stress ﬁelds, the true solution renders the following functional maximum: Ich[ˆ] ⫽ 2DUh ⫺ H[ˆ],

(6.3.50)

and the maximum value of Ich[ˆ] is the strain energy density of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Ich[ˆ]} ⫽ –12 L.

(6.3.51)

6.4 HASHIN–SHTRIKMAN BOUNDS

As can be seen from (6.3.36) and (6.3.49), the key to developing the bounds is to ﬁnd an appropriate statically admissible stress tensor ˆ . This is what we will do next. Remembering that the Reuss and Voigt bounds were obtained by assuming uniform admissible ﬁelds throughout the composite, let us try a piecewise uniform ﬁeld for ˆ , ˆ (x)兩x僆⍀r ⫽ ˆ r ,

r ⫽ 0, 1, 2, . . . , N.

(6.4.1)

In other words, we assume that the stress polarization tensor is a constant tensor on each inhomogeneity including the matrix. Introducing (6.4.1) into (6.3.28) yields

6.4

冘 ⍀c 冕

137

HASHIN–SHTRIKMAN BOUNDS

N

[ˆ] ⫽ (L p)⫺1ˆ ⫹ D

r

s⫽0

s

⍀s

⌫(x, y) dV(y)s ⫺ .

(6.4.2)

It thus follows from (6.3.30) that

冘 冕 冋(L ) ⫹ D 冘 ⍀c 冕 ⌫(x, y) dV(y) ⫺ 册 d ⫺ 冘 冕 d ⫽ D 冘 c (L ) ⫹ D 冘 冘 c c P ⫺ 2D 冘 c , N

N

H[ˆ] ⫽

r

⍀r

r⫽0

p ⫺1

r

s⫽0

s

N

N

s

⍀s

N

r⫽0

⍀r

r

N

r r

p ⫺1 r r

N

2

r s r

rs s

r⫽0 s⫽0

r⫽0

r r

r⫽0

(6.4.3) where cr is the volume fraction of the rth inhomogeneity and (L pr )⫺1 ⫽ Prs ⫽

1 ⍀r⍀s

1 ⍀r

冕冕 ⍀r

⍀s

冕

⍀r

(L p)⫺1 d,

⌫(x, y) dV(y) dV(x).

(6.4.4)

(6.4.5)

The validity of (6.4.4) is based on the fact that the stiffness tensor is uniform on each inhomogeneity. Clearly, H[ˆ] is now a quadratic function of the constant tensor r. The speciﬁc r that gives the extreme value of H[ˆ] can be determined from ⭸H[ˆ] / ⭸r ⫽ 0,

冘 c P ⫽ , N

p ⫺1 r r

(L ) ⫹ D

s

rs s

r ⫽ 0, 1, . . . , N.

(6.4.6)

s⫽0

This is a system of linear algebraic equations for r . The solution can be written formally as r ⫽ Rr.

This leads to the following extreme value of H[ˆ]:

(6.4.7)

138

BOUNDS FOR EFFECTIVE MODULI

冘 c R ⫽ D(L ⫺ L)˜ , N

H[ˆ]兩r⫽Rr ⫽ ⫺D

h

r

r

(6.4.8)

r⫽0

where

冘 c R. N

L˜ ⫽ Lh ⫹

r

(6.4.9)

r

r⫽0

For L p being negative semideﬁnite, substituting (6.4.8) into (6.3.36) yields 2U ⫽ L ⱕ L˜ ,

(6.4.10)

or

冘cR, N

L ⱕ L˜ ⫽ Lh ⫹

r

r

(6.4.11)

r⫽0

with L˜ being given by (6.4.9). Dually, for L p being positive semideﬁnite, substituting (6.4.8) into (6.3.49) yields

冘 c R. N

L ⱖ L˜ ⫽ Lh ⫹

r

r

(6.4.12)

r⫽0

The inequalities (6.4.11) and (6.4.12) are the Hashin–Shtrikman bounds for the effective stiffness tensor of a heterogeneous material containing N-phase inhomogeneities. In general, the Hashin–Shtrikman bounds are more restrictive than Voigt and Reuss bounds. It is noted that, in order to evaluate the Hashin–Shtrikman bounds, the double integral in (6.4.5) needs to be evaluated. Although, theoretically speaking, the integral can be carried out for a given heterogeneous material, the large number of inhomogeneities and the statistical nature of their distributions in a heterogeneous material render the integration impractical. We need to ﬁnd a practical way to evaluate it, albeit, approximately. Recall from (6.3.15) that the integrand consists of the second derivatives of Green’s function Gij(x, y) in the domain D, which satisﬁes zero displacement boundary condition; see (6.3.8) and (6.3.9). One of the proposals of simplifying (6.4.5) (see Willis, 1982) is to replace

6.4

HASHIN–SHTRIKMAN BOUNDS

139

Green’s function Gij(x, y) in the ﬁnite domain D by its counterpart in the inﬁnite domain, Prs ⬇

1 ⍀r⍀s

冕冕 ⍀r

⌫⬁(x, y) dV(y) dV(x),

⍀s

(6.4.13)

where ⌫⬁(x, y) is given by (3.3.18), which is related to Green’s function in an unbounded domain, G⬁ij (x, y) derived in Section 2.6: G⬁ij (x, y) ⫽

1 (2)3

冕

⬁

⫺⬁

Nij ()D⫺1()ei䡠(x⫺y) d.

(6.4.14)

For statistically homogeneous and isotropic distribution of inhomogeneities, the integral in (6.4.13) can be evaluated; see Appendix 6.A: Prs ⬇

冕冕 ⍀⍀ 1

r

s

⍀r

⍀s

⌫⬁(x, y) dV(y) dV(x) ⫽

1 ⍀s

(␦rs ⫺ cs)P,

(6.4.15)

where P(x) ⫽

冕

⌫⬁(x, y) dV(y)

Sˆ 2

for x 僆 Sˆ 2,

(6.4.16)

and the integral is over a unit sphere Sˆ 2. It follows from (4.3.19) that the tensor P is related to the Eshelby tensor S through P ⫽ S(Lh)⫺1.

(6.4.17)

Substituting (6.4.15) into (6.4.6) yields

冘 c ⫽ , N

(L pr )⫺1r ⫹ Pr ⫺ P

s s

r ⫽ 0, 1, . . . , N,

(6.4.18)

s⫽0

which can be rewritten as

冉

r ⫽ [(L pr )⫺1 ⫹ P]⫺1 ⫹ P

Further,

冘 c 冊, N

s s

s⫽0

r ⫽ 0, 1, . . . , N. (6.4.19)

140

BOUNDS FOR EFFECTIVE MODULI

冘

冉

冘 ⫽ 冘 c [(L )

N

N

r⫽0

r⫽0

s s

s⫽0

N

r

冘 c冊 N

cr [(L pr )⫺1 ⫹ P]⫺1 ⫹ P

crr ⫽

冘 [(L ) N

p ⫺1 r

⫹ P]⫺1 ⫹

⫹ P]⫺1 P

r⫽0

r⫽0

冘 c. N

p ⫺1 r

s s

s⫽0

(6.4.20) Finally, making use of (6.4.7), we have

冘 c R ⫽ 再I ⫺ 冘 c [(L ) ⫽ 冋 冘 c (I ⫹ L P) N

冎

⫺1

N

s

s

r

p ⫺1 r

r⫽0

s⫽0

N

p r

r

r⫽0

⫹ P]⫺1P

册

⫺1

⫺1

冘 c [(L ) N

p ⫺1 r

r

⫹ P]⫺1

r⫽0

冘 c (I ⫹ L P) N

p r

r

⫺1

L pr .

(6.4.21)

r⫽0

Thus, it follows from (6.4.9) that

冋冘 c (I ⫹ L P) N

L˜ ⫽ Lh ⫹

r

p r

r⫽0

册

⫺1

⫺1

冘 c (I ⫹ L P) N

r

p r

⫺1

L pr .

(6.4.22)

r⫽0

Example 6.2 Let a composite material be made of a matrix with elastic stiffness tensor L0 containing uniformly distributed identical spherical inhomogeneities with elastic stiffness tensor L1. Assume that both L0 and L1 are isotropic and given by L0 ⫽ (3K0, 20),

L1 ⫽ (3K1, 21),

(6.4.23)

where K1 ⬎ K0, 1 ⬎ 0. If the volume fraction of the inhomogeneities is c1, ﬁnd the bounds of its effective stiffness tensor. To ﬁnd the bounds for the effective stiffness tensor of the composites, we need to know the tensor L˜ as given by (6.4.22). To this end, let us compute the relevant tensors one at a time. First, we choose (it will be seen later that the choice is arbitrary) Lh ⫽ L0. Consequently,

(6.4.24)

6.4

L p(x) ⫽

HASHIN–SHTRIKMAN BOUNDS

再

L1 ⫺ L0 x 僆 ⍀1 . 0 x 僆 ⍀0

141

(6.4.25)

So, L p0 ⫽

冕 ⍀ 1

0

⍀0

L p d ⫽ 0,

L 1p ⫽

1 ⍀1

冕

⍀1

L p d ⫽ L1 ⫺ L0. (6.4.26)

Introducing the above to (6.4.22) leads to

冋冘

冋冘

cr(I ⫹ L rpP)⫺1

r⫽0

册

⫺1

1

⫽

⫺1

cr(I ⫹ L P) p r

r⫽0

册

⫺1

1

L˜ ⫽ L0 ⫹

冘 c (I ⫹ L P) 1

p r

r

⫺1

(Lr ⫺ L0)

r⫽0

冘 c (I ⫹ L P) 1

p r

r

⫺1

Lr

r⫽0

⫽ {c0I ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1}⫺1 ⫻ {c0L0 ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1L1}.

(6.4.27)

For spherical inhomogeneities, the Eshelby tensor is given by (see Appendix 4.B) S ⫽ (3␥0, 2␦0),

(6.4.28)

where ␥0 ⫽

K0 3K0 ⫹ 40

⫽

1 ⫹ 0 , 9(1 ⫺ 0)

␦0 ⫽

3(K0 ⫹ 20) 4 ⫺ 5 0 ⫽ . 5(3K0 ⫹ 40) 15(1 ⫺ 0) (6.4.29)

Therefore, making use of (6.4.17), we have I ⫹ (L1 ⫺ L0)P

冉 冊

⫽ (1,1) ⫹ (3K1 ⫺ 3K0, 21 ⫺ 20)(3␥0, 2␦0) ⫽

冉

Thus,

K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␥0(1 ⫺ 0) , . K0 0

冊

1 1 , 3K0 20

(6.4.30)

142

BOUNDS FOR EFFECTIVE MODULI

[I ⫹ (L1 ⫺ L0)P]⫺1 ⫽

冉

冊

K0 0 , . K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␥0(1 ⫺ 0) (6.4.31)

This leads to L˜ ⫽ {c0I ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1}⫺1{c0L0 ⫹ c1[I ⫹ (L1 ⫺ L0)P]⫺1L1} ˘ 2 ⫽ (3K, ˘ ),

where ˘ ⫽ K

˘ ⫽

K0{(1 ⫺ c1)[K0 ⫹ 3␥0(K1 ⫺ K0)] ⫹ c1K1} , K0 ⫹ 3␥0(1 ⫺ c1)(K1 ⫺ K0)

(6.4.32)

0{(1 ⫺ c1)[0 ⫹ 2␦0(1 ⫺ 0)] ⫹ c11} . 0 ⫹ 2␦0(1 ⫺ c1)(1 ⫺ 0)

Introducing (6.4.29) into the above expressions, ˘ ⫽ K

K0(3K1 ⫹ 40) ⫹ 4c10(K1 ⫺ K0) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

˘ ⫽

601(K0 ⫹ 20) ⫹ 0(9K0 ⫹ 80)[c11 ⫹ (1 ⫺ c1)0] . 0(9K0 ⫹ 80) ⫹ 6(K0 ⫹ 20)[c10 ⫹ (1 ⫺ c1)1] (6.4.33)

Since K1 ⬎ K0, 1 ⬎ 0, one can see that the tensor L p(x) deﬁned by (6.4.25) is positive semideﬁnite. It thus follows from (6.4.12) that ˘ 2 L ⫽ (3K, 2) ⱖ L˜ ⫽ (3K, ˘ ),

or equivalently, Kⱖ ⱖ

K0(3K1 ⫹ 40) ⫹ 4c10(K1 ⫺ K0) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(6.4.34)

601(K0 ⫹ 20) ⫹ 0(9K0 ⫹ 80)[c11 ⫹ (1 ⫺ c1)0] . 0(9K0 ⫹ 80) ⫹ 6(K0 ⫹ 20)[c10 ⫹ (1 ⫺ c1)1] (6.4.35)

6.4

HASHIN–SHTRIKMAN BOUNDS

143

These are the Hashin–Shtrikman lower bounds. To ﬁnd the Hashin–Shtrikman upper bounds, we choose Lh ⫽ L1. Consequently, L p(x) ⫽

(6.4.36)

再

L0 ⫺ L1 x 僆 ⍀0 . 0 x 僆 ⍀1

(6.4.37)

So, L p0 ⫽

1 ⍀0

冕

⍀0

L p d ⫽ L0 ⫺ L1,

1

L 1p ⫽

⍀1

冕

L p d ⫽ 0.

⍀1

(6.4.38) Thus, we have

冋冘 c (I ⫹ L P) 1

L˜ ⫽ L1 ⫹

冋冘

p r

r

r⫽0

册

⫺1

1

⫽

⫺1

cr(I ⫹ L P) p r

r⫽0

册

⫺1

⫺1

冘 c (I ⫹ L P) 1

p r

r

⫺1

(Lr ⫺ L1)

r⫽0

冘 c (I ⫹ L P) 1

r

p r

⫺1

Lr

r⫽0

⫽ {c0[I ⫹ (L0 ⫺ L1)P]⫺1 ⫹ c1I}⫺1 ⫻ {c0[I ⫹ (L0 ⫺ L1)P]⫺1L0 ⫹ c1L1}.

(6.4.39)

Since I ⫹ (L0 ⫺ L1)P

冉 冊

⫽ (1,1) ⫹ (3K0 ⫺ 3K1, 20 ⫺ 21)(3␥0, 2␦0) ⫽

冉

K0 ⫹ 3␥0(K0 ⫺ K1) 0 ⫹ 2␥0(0 ⫺ 1) , . K0 0

冊

1 1 , 3K0 20

(6.4.40)

Thus, [I ⫹ (L0 ⫺ L1)P]⫺1 ⫽

冉

冊

0 K0 , . K0 ⫹ 3␥0(K0 ⫺ K1) 0 ⫹ 2␥0(0 ⫺ 1)

(6.4.41)

144

BOUNDS FOR EFFECTIVE MODULI

This leads to L˜ ⫽ {c0[I ⫹ (L0 ⫺ L1)P]⫺1 ⫹ c1I}⫺1 ៣ ៣ ⫻ {c0[I ⫹ (L0 ⫺ L1)P]⫺1L0 ⫹ c1L1} ⫽ (3K, 2),

(6.4.42)

where ៣

K⫽

K20 ⫺ c1(K1 ⫺ K0)(3␥0K1 ⫺ K0) , K0 ⫺ 3␥0c1(K1 ⫺ K0)

2 ⫺ c1(1 ⫺ 0)(2␦01 ⫺ 0) ៣ ⫽ 0 . 0 ⫺ 2␦0c1(1 ⫺ 0)

(6.4.43)

Introducing (6.4.29) into the above expressions, ៣

K⫽

K0(3K0 ⫹ 40) ⫹ c1(K1 ⫺ K0)[40 ⫺ 3(K1 ⫺ K0)] , 3K0 ⫹ 40 ⫺ 3c1(K1 ⫺ K0)

520(3K0 ⫹ 40) ⫹ c1(1 ⫺ 0)[50(3K0 ⫹ 40) ⫺ 61(K0 ⫹ 20)] ៣ ⫽ . 50(3K0 ⫹ 40) ⫺ 6c1(K0 ⫹ 20)(1 ⫺ 0) (6.4.44) Since K1 ⬎ K0, 1 ⬎ 0, one can see that the tensor L p(x) deﬁned by (6.4.37) is negative semideﬁnite. It thus follows from (6.4.11) that ៣

៣

L ⫽ (3K, 2) ⱕ L˜ ⫽ (3K, 2), or equivalently, Kⱕ

K0(3K0 ⫹ 40) ⫹ c1(K1 ⫺ K0)[40 ⫺ 3(K1 ⫺ K0)] , 3K0 ⫹ 40 ⫺ 3c1(K1 ⫺ K0) 520(3K0 ⫹ 40) ⫹ c1(1 ⫺ 0) [50(3K0 ⫹ 40) ⫺ 61(K0 ⫹ 20)] ⱕ . 50(3K0 ⫹ 40) ⫺ 6c1(K0 ⫹ 20)(1 ⫺ 0)

These are the Hashin–Shtrikman upper bounds.

(6.4.45)

(6.4.46)

PROBLEMS

145

PROBLEMS

6.1 Show that 2 ˆ ⫺ ˆ MR ˆ ⱕ (MR)⫺1 for any constant tensor ˆ ij. 6.2 Show that the integral operator

冕 ⌫(x, y)(y) dV(y) ⬅ ⌫(x, y) * (y) D

is self-adjoint, that is, (x) * (⌫(x, y) * (y)) ⫽ (x) * (⌫(x, y) * (y)).

6.3 Show the identity LhMp ⫹ L p(Mh ⫹ Mp) ⫽ 0. 6.4 Show that, for a composite comprising isotropic matrix and Nphase isotropic, spherical inhomogeneities, the Hashin–Shtrikman bounds are given by

冉冘 K ⫹c K*冊

⫺1

N

r⫽0

冉冘 N

r⫽0

r

冊

r ⫹ S*

⫺1

r

r⫽0

S

cr

冉冘 K ⫹c K*冊 N

⫺ K* S ⱕ K ⱕ

r

⫺1

冉冘 N

⫺ S* ⱕ ⱕ

r⫽0

r

⫺ K*, L

L

cr

冊

r ⫹ * L

⫺1

⫺ L*,

where K* L ⫽

4L , 3

L* ⫽

3 , 2[1/ L ⫹ 10/(9KL ⫹ 8L)]

K* S ⫽

4S , 3

* S ⫽

3 , 2[1/ S ⫹ 10/(9KS ⫹ 8S)]

L ⫽ max{0, 1, . . . , N},

S ⫽ min{0, 1, . . . , N},

KL ⫽ max{K0, K1, . . . , KN},

KS ⫽ min{K0, K1, . . . , KN}.

146

BOUNDS FOR EFFECTIVE MODULI

6.5 Assume that the traction boundary condition n兩x僆S ⫽ n is prescribed on the entire boundary, where is a constant stress tensor (the average stress). Use the minimum potential energy theorem to prove that for any continuously differentiable displacement ﬁeld uˆ i,

冕 ˆ Lˆ d ⫹ 2 冕 ˆ d,

2DU ⱖ ⫺

D

D

where U⫽

1 2D

冕 L d ⫽ 12 L, D

ˆ ij ⫽ –12 (ˆui,j ⫹ uˆ j,i).

(Hint: Since there is no displacement boundary, any continuously differentiable displacement ﬁeld would be kinematically admissible.) 6.6 Show that under the traction boundary condition n兩x僆S ⫽ n,

冕L

⫺

D

uˆ uˆ d ⫹ 2ij

ijkl i, j k,l

冕 uˆ D

i, j

d ⱕ 2DU ⱕ

冕 ˆ M D

ij

ˆ kl d,

ijkl

where uˆ i is any continuously differentiable displacement ﬁeld and ˆ ij is any statically admissible stress ﬁelds, that is, ˆ ij,i ⫽ 0 in D and ijnj兩x僆S ⫽ ij nj on S. 6.7 Following the notations introduced in Appendix 6.A, please show that the following inequality holds for any eigenstrain ˆ : ˜ ) ⫺ 2D(U ⫺ Uhc ) ⱖ ⫺H(ˆ

冕 ␥(x)L (x)␥(x) dV(x). p

D

6.8 Prove Theorems 6.4 and 6.4a in Appendix 6A. 6.9 Prove Lpqij 兰S

˜ mi(x, y) ⭸G msns dS(y) ⫽ pq. ⭸xj

APPENDIX 6.A

147

APPENDIX 6.A

In Sections 6.3 and 6.4, the variational theorems have been established for heterogeneous material under the displacement boundary conditions. Let us now consider the traction boundary condition, (x)n兩x僆S ⫽ n,

(6.A.1)

where is a constant stress tensor. Analogous to (6.3.5), we introduce a strain polarization * (or eigenstrain) through ⫽ Mh ⫹ *

or ⫽ (Mh)⫺1( ⫺ *),

(6.A.2)

where Mh is deﬁned in (6.3.44), and is the actual total strain in the heterogeneous material D, which is related to the displacements through (6.3.4). Using Hooke’s law ⫽ M in the ﬁrst of (6.A.2) gives * ⫽ Mp.

(6.A.3)

Substituting the second of (6.A.2) into the equations of equilibrium, Lhijkluk,lj (x) ⫺ Lhijkl*kl, j (x) ⫽ 0

in D,

(6.A.4)

where Lhijkl is to denote the inverse of Mhijkl. To solve (6.A.4) under the traction boundary condition (6.A.1), let us consider the following Green’s function: h Lijkl

˜ km(x, y) ⭸2G ⫹ ␦im␦(x ⫺ y) ⫽ 0 ⭸xl ⭸xj h Lijkl

in V,

˜ km(x, y) ⭸G nj兩x僆S ⫽ 0. ⭸xl

(6.A.5)

(6.A.6)

It then follows from (2.6.51) that ui(x) ⫽

冕 G˜ (x, y) S

mi

msns dS(y) ⫺

冕 G˜ (x, y) ⭸L ⭸y*(y) dV(y). h mnkl kl

V

mi

n

(6.A.7) The corresponding displacement gradient tensor follows immediately:

148

BOUNDS FOR EFFECTIVE MODULI

ui, j (x) ⫽

冕 ⭸G˜ ⭸(x,x y)

ms ns dS(y) ⫺

mi

S

j

冕 ⭸G˜ x(x, y) ⭸L ⭸y*(y) dV(y). h mnkl kl

mi

V

j

n

(6.A.8) The use of Hooke’s law leads us to the corresponding stress tensor:

冕 ⭸G˜ ⭸(x,x y) n dS(y) ˜ (x, y) ⭸L *(y) ⭸G ⫺L 冕 dV(y). ⭸x ⭸y

pq(x) ⫽ Lpqij

mi

ms s

S

j

h mnkl kl

mi

pqij

D

j

(6.A.9)

n

It is easy to show that Lpqij

冕 ⭸G˜ ⭸(x,x y)

n dS(y) ⫽ pq.

mi

ms s

S

(6.A.10)

j

Thus, the stress tensor is simpliﬁed to pq(x) ⫽ pq ⫺ Lpqij

冕 ⭸G˜ ⭸(x,x y) ⭸L ⭸y*(y) dV(y). h mnkl kl

mi

D

j

(6.A.11)

n

Note that pq is a constant stress tensor (the average stress in the composite). Therefore, by making use of the properties of Green’s function, one can show that

冕 ⭸G˜⭸x (x,⭸x y) ⭸L ⭸y*(y) dV(y)

pq,q(x) ⫽ ⫺Lpqij ⫽ ⫽

and

冕␦ D

h mnkl kl

mi

D

j

␦(x ⫺ y)

mp

q

n

h ⭸Lmnkl kl *(y) dV(y) ⭸yn

h ⭸Lpnkl kl *(x) ⫽ Lhpnklkl,n * (x) ⭸xn

(6.A.12)

149

APPENDIX 6.A

pq(x)nq兩x僆S ⫽ ⫺Lpqij ⫽ ⫺Lpqij

冕 ⭸G˜ ⭸(x,x y) n ⭸L ⭸y*(y) dV(y) ⫹ 冕 ⭸G˜ ⭸(x,x y) n ⭸L ⭸y*(y) dV(y) ⫹ h mnkl kl

mi

q

D

j

nq

pq

nq

h mnkl kl

mi

q

D

pq

n

j

n

⫽ pq nq.

(6.A.13)

In other words, regardless of the choice of *(y), the stress tensor kl generated from (6.A.11) is always a statically admissible stress ﬁeld, that is, it satisﬁes (6.A.4) and (6.A.1). For convenience, we deﬁne the following operator to represent the volume integral in (6.A.11): Lpqij

冕 ⭸G˜ ⭸(x,x y) ⭸L ⭸y*(y) dV(y) ⬅ 冕 ⌫˜ h mjkl kl

mi

D

j

j

D

(x, y)kl*(y) dV(y).

pqkl

(6.A.14) Analogues to (6.3.16), the operator can also be written symbolically,

冕 ⌫˜ (x, y)*(y) dV(y) ⬅ ⌫˜ (x, y) * *(y).

(6.A.15)

D

Thus, the stress tensor can be written formally as ˜ (x, y) * *(y). (x) ⫽ ⫺ ⌫

(6.A.16)

It then follows from (6.A.3) that (Mp)⫺1*(x) ⫹ ⌫˜ (x, y) * * ⫽ .

(6.A.17)

Let ˆ (y) be any strain polarization, and ˆ (x) ⫽ ⫺ ⌫˜ (x, y) * *(y)

(6.A.18)

the corresponding statically admissible stress ﬁeld. The minimum complementary energy theorem takes the following form:

150

BOUNDS FOR EFFECTIVE MODULI

2DUc ⱕ

冕 ˆ (x)M(x)ˆ (x) dV(x),

(6.A.19)

D

where 1 2D

Uc ⫽

冕M

klij d ⫽

ijkl

D

1 M. 2

(6.A.20)

Substituting (6.A.18) into (6.A.19), after some simpliﬁcations, yields ˜ ) ⫹ 2D(U ⫺ Uhc ) ⱕ ⫺H(ˆ

冕 ␥(x)M (x)␥(x) dV(x). p

(6.A.21)

D

where the compliance tensor has been decomposed as in (6.3.44) and Uh ⫽ –12 Mh,

(6.A.22)

Lh␥(x) ⫽ ⌫˜ (x, y) * ˆ (y) ⫹ (Mh)⫺1ˆ (x) ⫺ ,

冕 ˆ (x)L ␥(x) dV(x) ⫹ 冕 ˆ (x) d.

˜ ) ⫽ ⫺ H(ˆ

h

D

(6.A.23)

D

If ˆ happens to be the actual strain polarization * for the problem at hand, then the use of (6.A.17) leads to ␥(x) ⫽ 0, ˜ *) ⫽ H(

冕 *(x) d ⫽ 冕 (M(x) ⫺ M ) d ⫽ 2D(U ⫺ U ). h

D

D

c

h c

In other words, the equal sign in (6.A.21) is attained when the actual strain polarization * for the problem at hand is used. Therefore, we can state the following variational principle. Theorem 6.3 Among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional minimum:

APPENDIX 6.A

Jc[ˆ] ⫽

1 1 ˜ 1 Mh ⫺ H(ˆ) ⫹ 2 2D 2D

151

冕 ␥(x)M (x)␥(x) dV(x), p

D

(6.A.24) and the minimum value of Jc[ˆ] is the strain energy of the heterogeneous material under the displacement boundary condition (6.3.1), that is, min{Jc[ˆ]} ⫽ –12 M.

(6.A.25)

The inequality (6.A.21) can be further simpliﬁed if one assumes that Mp(x) is negative semideﬁnite, that is, for any ˆ ,

冕 ␥(x)M (x)␥(x) d ⱕ 0. p

(6.A.26)

D

In this case, (6.A.21) reduces to 2D(U ⫺ Uh) ⱕ ⫺H[ˆ].

(6.A.27)

Therefore, we have the following theorem. Theorem 6.3a When Mp(x) is negative semideﬁnite, among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional minimum: Jch[ˆ] ⫽

1 1 ˜ Mh ⫺ H(ˆ), 2 2D

(6.A.28)

and the minimum value of Jch[ˆ] is the strain energy of the composite under the displacement boundary condition (6.3.1), that is, min{Jch[ˆ]} ⫽

1 M. 2D

(6.A.29)

This is another form of the Hashin–Shtrikman variational principle. The duals of the above theorems can be easily proven by using the minimum potential energy theorem; see Problem 6.7.

152

BOUNDS FOR EFFECTIVE MODULI

Theorem 6.4 Among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional maximum: J[ˆ] ⫽

1 1 ˜ 1 Mh ⫺ H(ˆ) ⫺ 2 2D 2D

冕 ␥(x)L (x)␥(x) dV(x), p

(6.A.30)

D

and the maximum value of J[ˆ] is the strain energy of the composite under the displacement boundary condition (6.3.1), that is, min{J[ˆ]} ⫽ –12 M.

(6.A.31)

The inequality (6.A.21) can be further simpliﬁed if one assumes that Mp(x) is negative semideﬁnite, that is, for any ˆ ,

冕 ␥(x)L (x)␥(x) d ⱕ 0. p

(6.A.32)

D

In this case, we have the following theorem. Theorem 6.4a When Mp(x) is negative semideﬁnite, among all the symmetric second-order tensors, the true solution to the strain polarization tensor * renders the following functional maximum: Jh[ˆ] ⫽

1 1 ˜ Mh ⫺ H(ˆ), 2 2D

(6.A.33)

and the maximum value of Jh[ˆ] is the strain energy of the composite under the displacement boundary condition (6.3.1), that is, min{Jh[ˆ]} ⫽ –12 M.

(6.A.34)

This is another form of the Hashin–Shtrikman variational principle.

REFERENCE Willis, J. R. (1982). Elasticity Theory of Composites, in Mechanics of Solids—The Rodney Hill 60th Anniversary Volume, H. G. Hopkins and M. J. Sewell, eds., Pergamon Press, Oxford. pp. 635–686.

SUGGESTED READING

153

SUGGESTED READING Hashin, Z. and S. Shtrikman. (1961). Note on a Variational Approach to the Theory of Composite Elastic Materials, J. Franklin Inst., Vol. 271, pp. 336– 341. Hashin, Z. and S. Shtrikman. (1963). A Variational Approach to the Theory of the Elastic Behavior of Multiphase Materials, J. Mech. Phys. Solids, Vol. 11, pp. 127–140. Mura, T. and T. Koya. (1992). Variational Methods in Mechanics, Oxford University Press, New York, Chapter 21. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York, Chapter 3, Section 9. Willis, J. R. (1977). Bounds and Self-Consistent Estimates for the Overall Properties of Anisotropic Composites, J. Mech. Phys. Solids, Vol. 25, pp. 185–202. Willis, J. R. (1981). Variational and Related Methods for the Overall Properties of Composites, Adv. Appl. Mech., Vol. 21, pp. 1–78.

7 DETERMINATION OF EFFECTIVE MODULI In this chapter, we develop several methods to evaluate approximately the effective properties of heterogeneous materials. All the approaches presented are based on the Eshelby single-inclusion solution. In the next chapter, we will present other methods of evaluating the effective properties that are based on multiple-inclusion approaches.

7.1 BASIC IDEAS OF MICROMECHANICS FOR EFFECTIVE PROPERTIES

Consider a heterogeneous material D consisting of a matrix phase ⍀0 and ellipsoidal inhomogeneities, ⍀1, ⍀2, . . . , ⍀N, as shown in Figure 7.1. The volume fraction of ⍀r is cr ⫽ ⍀r / ⍀. Clearly, one has

冘 c ⫽ 1. N

r

r⫽0

Let the stiffness tenor of ⍀r be Lr (r ⫽ 0, 1, . . . , N). Our objective is to determine the effective elastic modulus of the composite materials in terms of the stiffness tensors of the matrix and the inhomogeneities and their respective volume fractions. We learned from Section 5.7 that the effective elastic stiffness tensor can be easily computed once the local or the global concentration tensors are known. However, the exact expressions of the concentration tensors are rather difﬁcult to obtain. So, the various methods discussed in this chapter are aimed at obtaining approximate solutions to these concentration tensors. The multiphase composite shown in Figure 7.1 is a very general case. Most engineering composites are two-phase materials, namely, 154

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

7.1

BASIC IDEAS OF MICROMECHANICS FOR EFFECTIVE PROPERTIES

155

Ω3

Ω2 Ωr ΩN

Ω1 Ω0

Figure 7.1 Multiphase composite.

matrix phase and the reinforcement phase. The most common types of reinforcement phases are either particles (particulate-reinforced composites) or ﬁbers (ﬁber-reinforced composites). The results derived below for the multiphase composite can be easily speciﬁed to the case of two-phase composite by assuming that all the inhomogeneities are the same. The basic idea of micromechanics is to develop solutions of either the global or local concentration tensors. Once such concentration tensors are known, the effective properties can be easily obtained per the discussions in Section 5.7. One common approach of developing the concentration tensors is to use the Eshelby solution in conjunction with the equivalent inclusion method. To this end, we assume that the composite is subjected to either the displacement boundary condition u兩S ⫽ 0x

(7.1.1)

or the traction boundary condition • n兩S ⫽ 0n,

(7.1.2)

where 0 and 0 are constant second-order tensors and are related by 0 ⫽ L00.

If all the inhomogeneities are absent and the entire volume D is ﬁlled with the matrix material L0, or equivalently, L0 ⫽ L1 ⫽ L2 ⫽ ⫽

156

DETERMINATION OF EFFECTIVE MODULI

LN, it is obvious that the strain and stress ﬁeld would be 0 and 0, respectively, throughout the volume D; see Figure 7.2. In the actual composite, the inhomogeneities have distinctive properties from the matrix material. The strain and stress in the matrix will no longer be 0 and 0. For example, consider a typical inhomogeneity called the rth inhomogeneity; see Figure 7.3a. It is surrounded by the matrix material with elastic stiffness tensor L0. The strain in the matrix around the rth inhomogeneity is conceivably different from 0 for two reasons. First, the rth inhomogeneity itself perturbs the uniform distribution of strains in the matrix. Second, the other inhomogeneities, especially those near by, also contribute to the strain perturbation. Thus, as far as the rth inhomogeneity is concerned, it might be viewed as an isolated inhomogeneity placed in a uniform matrix that possessed certain strain before the inhomogeneity is embedded. For convenience, we will denote this strain by ˆ 0. Furthermore, it is also plausible that the inﬂuence of other inhomogeneities can be accounted for by assuming that the rth inhomogeneity is embedded in a matrix material that is somewhat different from the actual matrix. We will use Lˆ0 to denote the stiffness tensor of this ﬁctitious matrix material; see Figure 7.3b. Now the companion problem can be restated as follows. An ellipsoidal inhomogeneity ⍀r with stiffness tensor Lr is placed within a uniform matrix of stiffness tensor Lˆ0, which had been subjected to the uniform strain ˆ 0 before the inhomogeneity was embedded; see Figure 7.3b. Our objective is to ﬁnd proper values for ˆ 0 and Lˆ0 so that the stress (and strain) on ⍀r is the same as that occurring on the rth inhomogeneity the actual composite. To ﬁnd such ˆ 0 and Lˆ0, let us pretend at the moment that they are known. We will ﬁrst establish how the stresses and strains of the companion problem are related to ˆ 0 and Lˆ0. This can be done by solving the Eshelby inclusion problem. The stress and strain on the inhomogeneity can be obtained by the equivalent inclusion method discussed in Section 4.4. The equivalent inclusion equation in this case is

L0 0

0

Figure 7.2 Homogeneous material.

7.1

157

BASIC IDEAS OF MICROMECHANICS FOR EFFECTIVE PROPERTIES

V3

V2 Vr

Vr VN

= ˆ0

V1

Lˆ 0

V0

(a)

(b)

Figure 7.3 (a) The rth inhomogeneity in the composite; (b) The rth inhomogeneity in a uniform matrix of stiffness Lˆ 0, which had been subjected to the uniform strain ˆ 0 before the inhomogeneity was embedded.

ˆ 0 ⫹ pt Lr (ˆ0 ⫹ pt r ) ⫽ L0 (ˆ r ⫺ *), r

(7.1.3)

where, according to the Eshelby solution given in Section 4.3, ˆ pt r ⫽ Srr*,

(7.1.4)

where Sˆr is the Eshelby tensor computed using the elastic constants of Lˆ0 and the geometry of the rth inhomogeneity ⍀r. Substitution of the Eshelby solution into the equivalent inclusion equation yields the eigenstrain ˆ ˆ ˆ ⫺1 * 0. r ⫽ [(Lr ⫺ L0)Sr ⫹ L0] (Lr ⫺ L0)ˆ

(7.1.5)

The total strain in the rth inhomogeneity can then be written as r ⫽ ˆ 0 ⫹ pt ˆ 0 ⫹ Sˆ r* ⫽ Tˆ rˆ 0, r ⫽

(7.1.6)

Tˆ r ⫽ [I ⫹ Sˆ rLˆ 0⫺1(Lr ⫺ Lˆ 0)]⫺1.

(7.1.7)

where

The derivation of the last equality in (7.1.6) is similar to that of (4.4.15). The corresponding stress on the rth inhomogeneity is

158

DETERMINATION OF EFFECTIVE MODULI

ˆ rˆ 0. r ⫽ Lrr ⫽ LrT

(7.1.8)

We now have related the strain and stress ﬁelds in the rth inhomogeneity to an unknown strain ﬁeld ˆ 0 and a ﬁctitious matrix material with L ˆ 0. It will be seen later that the micromechanics schemes discussed below use various approximations to identify and compute ˆ 0 and Lˆ0. Once ˆ 0 and Lˆ0 are known, the concentration tensors can be obtained and so can the effective properties of the composite.

7.2 ESHELBY METHOD

If the inhomogeneities in the composite shown in Figure 7.1 are far apart from each other, their interactions may be neglected. In other words, each inhomogeneity can be treated as if it exists in a homogeneous matrix without the interference by other inhomogeneities. Therefore, a typical inhomogeneity, for example, the rth inhomogeneity, can be treated as an ellipsoidal inhomogeneity in an otherwise uniform matrix of stiffness L0, which was subjected to a uniform strain 0 before the inhomogeneity was imbedded. Therefore, we choose in (7.1.3), Lˆ 0 ⫽ L0 and ˆ 0 ⫽ 0

(7.2.1)

and consequently,

V3

V2 Vr

Vr

VN

=

V1 V0

(a)

0

L0

(b)

Figure 7.4 (a) The rth inhomogeneity in the composite. (b) The rth inhomogeneity in the original matrix of stiffness L0, which had been subjected to the uniform strain 0 before the inhomogeneity was embedded.

7.2

ESHELBY METHOD

Sˆ r ⫽ Sr,

159

(7.2.2)

where Sr is the Eshelby tensor computed using the matrix material property L0 and the geometry of the rth inhomogeneity ⍀r. These equations simply imply that other inhomogeneities have no inﬂuence on the rth inhomogeneity at all. So, the interactions between inhomogeneities are completely ignored. In this case, the strain in the rth inhomogeneity follows directly from (7.1.6): r ⫽ 0 ⫹ rpt ⫽ 0 ⫹ Sr* ⫽ Tr0,

(7.2.3)

Tr ⫽ [I ⫹ Sr L0⫺1(Lr ⫺ L0)]⫺1.

(7.2.4)

where

For future reference, we want to mention that although Tr is deﬁned for r ⬎ 0, it is nevertheless true that T0 ⫽ I as seen from (7.2.4). We now assume that the composite is subjected to the displacement boundary condition u兩S ⫽ 0 • x.

(7.2.5)

It follows from the average strain theorem discussed in Section 5.4 that the average strain tensor of the composite is equal to 0, that is, ⫽

1 V

冕 dV ⫽ . 0

(7.2.6)

V

Therefore, Eq. (7.2.3) can be rewritten as r ⫽ Tr.

(7.2.7)

By comparing (5.7.3) and (7.2.7), it is clear that the global strain concentration tensor for the rth inhomogeneity is Ar ⫽ Tr.

(7.2.8)

Thus, it follows from (5.7.7) that the effective stiffness tensor of the composite is given by

160

DETERMINATION OF EFFECTIVE MODULI

冘c (L ⫺ L )T ⫽ L ⫹ 冘 c (L ⫺ L )[I ⫹ S (M L ⫺ I)] N

L ⫽ L0 ⫹

r

r

0

r

r⫽1 N

0

r

r

0

r

0

r

⫺1

.

(7.2.9)

r⫽1

This is the Eshelby estimate of the effective stiffness tensor. Recall that this effective stiffness tensor was derived based on the assumption made earlier that the inhomogeneities in the composite are so far apart that they do not interfere with each other. Thus, the Eshelby estimate is valid only for very low volume fraction of inhomogeneities, or the dilute case. Instead of the displacement boundary conditions, a traction boundary condition • n兩S ⫽ 0n

(7.2.10)

can be prescribed. In this case, the average strain of the composite is no longer equal to 0, that is, ⫽

1 V

冕 dV ⫽ , 0

(7.2.11)

V

where 0 ⫽ M00.

(7.2.12)

Instead, we have, according to the average stress theorem discussed in Section 5.4, ⫽

1 V

冕 dV ⫽ . 0

(7.2.13)

V

Substituting (7.2.12) and (7.2.13) into (7.2.3) and making use of r ⫽ Lrr yield r ⫽ LrTr M0.

(7.2.14)

The global stress concentration tensor is thus given by Br ⫽ LrTr M0 ⫽ [Mr ⫺ Sr (Mr ⫺ M0)]⫺1 M0.

(7.2.15)

7.2

161

ESHELBY METHOD

It then follows from (5.7.8) that the effective compliant tensor of the composite is given by

冘 c (M ⫺ M )B ⫽ M ⫹ 冘 c (M ⫺ M )L T M . N

M ⫽ M0 ⫹

N

r

r

0

r

0

r

r

0

r

r

0

r⫽1

r⫽1

(7.2.16) It can be further simpliﬁed to

冘c [(L ⫺ L )S ⫹ L ] N

M ⫽ M0 ⫺

r

r

0

r

0

⫺1

(Lr ⫺ L0)M0.

(7.2.17)

r⫽1

This is the Eshelby estimate of the effective compliance of the composite in consideration. Finally, let us check the consistency of the Eshelby estimates by considering

冋

冘 册冋 冘c (L ⫺ L )T 册 ⫽ I ⫺ 冋 冘 c (I ⫺ M L )T 册冋 冘 c (I ⫺ M L )T 册 N

ML ⫽ M0 ⫹

N

cr (Mr ⫺ M0)LrTr M0

L0 ⫹

r

r

0

r

r⫽1

r⫽1

N

N

r

r⫽1

⫽ I ⫹ O(c2r ).

0

r

r

r

0

r

r

r⫽1

(7.2.18)

It is seen that ML ⫽ I only when the terms with order of c2r are neglected. In other words, the Eshelby estimates are consistent only up to the ﬁrst order of the volume fraction of the inhomogeneities. To close this section, we note that both the volume fraction and the geometry of the inhomogeneities are taken into consideration in the Eshelby estimate. However, the distribution of the inhomogeneities is neglected. More importantly, the interaction between the inhomogeneities is not taken into consideration because the eigenstrain in each inclusion is calculated by assuming that the other inclusions are not present. Therefore, this method is limited to low (dilute) concentration of inhomogeneities. The method is also called by some authors the dilute concentration method. Example 7.1 Consider a particulate-reinforced composite material. Assume that all particles are spherical and randomly dispersed throughout the matrix. Further, assume that both the particle and the matrix

162

DETERMINATION OF EFFECTIVE MODULI

are made of isotropic elastic materials. Their elastic stiffness tensors are L0 ⫽ (3K0, 20)

for the matrix,

(7.2.19)

for the particles,

(7.2.20)

and L1 ⫽ (3K1, 21)

where the matrix symbolic notation for the fourth-order tensors introduced in Section 1.4 has been used for the stiffness tensors. The isotropic elastic constants Kr and r are the bulk and shear moduli, respectively, for the matrix (r ⫽ 0) and the particles (r ⫽ 1). Finally, we assume that the volume fraction of the particles in the composite is c1. To ﬁnd the effective stiffness tensor of the composites, we can use (7.2.9) directly by specifying N ⫽ 1. To this end, let us compute the relevant tensors one at a time. First, the Eshelby tensor for an isotropic material with L0 ⫽ (3K0, 20) can be written as (see Appendix 4.B) S1 ⫽ (3␥0, 2␦0),

(7.2.21)

where ␥0 ⫽

K0 3K0 ⫹ 40

⫽

1 ⫹ v0 , 9(1 ⫺ v0)

␦0 ⫽

3(K0 ⫹ 20) 4 ⫺ 5v0 ⫽ . 5(3K0 ⫹ 40) 15(1 ⫺ v0) (7.2.22)

Next, let us compute the fourth-order tensor T1: ⫺1 T1 ⫽ [I ⫹ S1L⫺1 0 (L1 ⫺ L0)]

⫽ {(1,1) ⫹ (3␥0, 2␦0)[(3K0, 20)⫺1(3K1, 21) ⫺ (1,1)]}⫺1 ⫽

冋 冋 冋

冉

(1, 1) ⫹ (3␥0, 2␦0)

K1 ⫺ K0 1 ⫺ 0 , K0 0

冊册 册 册

K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␦0(1 ⫺ 0) ⫽ , K0 0 ⫽

⫺1

⫺1

K0 0 , . K0 ⫹ 3␥0(K1 ⫺ K0) 0 ⫹ 2␦0(1 ⫺ 0)

(7.2.23)

7.3

163

MORI–TANAKA METHOD

Finally, L ⫽ L0 ⫹ c1 (L1 ⫺ L0)T1 ⫽ (3K0, 20) ⫹

冋

册

3c1K0 (K1 ⫺ K0) 2c10(1 ⫺ 0) , . K0 ⫹ 3␥0 (K1 ⫺ K0) 0 ⫹ 2␦0(1 ⫺ 0) (7.2.24)

Thus, we have K ⫽ K0 ⫹

c1K0 (K1 ⫺ K0) , K0 ⫹ 3␥0 (K1 ⫺ K0)

⫽ 0 ⫹

c10 (1 ⫺ 0) . 0 ⫹ 2␦0(1 ⫺ 0)

(7.2.25)

Making use of (7.2.22) in (7.2.25) yields alternative expressions c (K ⫺ K0)(3K0 ⫹ 40) K ⫽ K0 ⫹ 1 1 , 3K1 ⫹ 40 ⫽ 0 ⫹

(7.2.26)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 3K0(30 ⫹ 21) ⫹ 40 (20 ⫹ 31)

(7.2.27)

This completes the solution. Note that in the above derivations, we have used the symbolic notations of fourth-order isotropic tensors and followed the rules of operation on using such symbolic notations, as introduced in Section 1.4. The advantages of such operation are clearly seen.

7.3 MORI–TANAKA METHOD

Before presenting the Mori–Tanaka method, let us recall the average strain and average stress of a composite as deﬁned in Section 5.4: ⫽

where

1 D

冕 dV ⫽ 冘 , N

D

r

r⫽0

⫽

1 D

冕 dV ⫽ 冘 , N

D

r

r⫽0

(7.3.1)

164

DETERMINATION OF EFFECTIVE MODULI

r ⫽

冕 ⍀ 1

r

⍀r

dV

and r ⫽

1 ⍀r

冕

⍀r

dV

(7.3.2)

are the strain and stress tensors, respectively, averaged over the rth inhomogeneity. For example, 1 is the average strain in the inhomogeneity with stiffness tensor L1, and 0 is the average strain in the matrix phase, see Fig. 7.5. Furthermore, r ⫽ Lrr.

Now consider the composite material shown in Figure 7.1. For a typical inhomogeneity Lr (r ⬎ 0) in the composite, the effects (or the existence) of other inhomogeneities are communicated to it through the strain and stress ﬁelds in its surrounding matrix material. Although the strain and stress ﬁelds are different from one location to another in the matrix, the averages (0 and 0) represent good approximations of the actual ﬁelds in the matrix surrounding each inhomogeneity, when a large number of inhomogeneities exit and are randomly distributed in the matrix (which is the case for most engineering composites). Also, it would be reasonable to assume that taking only one inhomogeneity out will not affect the overall elastic behavior of the composite. In other words, when the rth inhomogeneity is removed and replaced by the matrix material (or equivalently, let Lr ⫽ L0), the averages (0 and 0) will remain the same. Therefore, as far as the rth inhomogeneity is concerned, it can be viewed as an ellipsoidal inhomogeneity with stiffness tensor Lr placed within a uniform matrix of stiffness tensor

0

V0

Figure 7.5 Average strain in matrix.

7.3

165

MORI–TANAKA METHOD

L0, which had been subjected to the uniform strain 0 before the inhomogeneity was embedded, see Fig. 7.6. Thus, we choose in (7.1.3), Lˆ 0 ⫽ L0 and ˆ 0 ⫽ 0

(7.3.3)

Sˆ r ⫽ Sr.

(7.3.4)

and consequently

Comparing these with (7.2.1) and (7.2.2), it is seen that the only difference between the Eshelby and the Mori–Tanaka methods is the use of ˆ 0. Note that ˆ 0 represents how the effects of other inhomogeneities are accounted for. Because the Eshelby method assumes no interaction between the inhomogeneities, it takes ˆ 0 ⫽ 0, which is the strain in the matrix when none of the inhomogeneities is present. The Mori–Tanaka method also assumes the absence of all inhomogeneities, but it includes certain effects of the inhomogeneity by taking ˆ 0 ⫽ 0, because 0 is the average strain in the matrix phase when all inhomogeneities are present. For this reason, the Mori–Tanaka method provides better estimate of the effective modulus than the Eshelby method does for composite with nondilute reinforcement phases.

Vr

Vr

=

0

0

V0

(a)

L0

(b)

Figure 7.6 (a) The rth inhomogeneity in the composite. (b) The rth inhomogeneity in the original matrix of stiffness L0, which had been subjected to the uniform strain 0 before the inhomogeneity was embedded.

166

DETERMINATION OF EFFECTIVE MODULI

The use of (7.3.3) and (7.3.4) in (7.1.6) yields the strain in the rth inhomogeneity r ⫽ 0 ⫹ rpt ⫽ 0 ⫹ Sr* r ⫽ Tr0,

(7.3.5)

where Tr is the same as that of (7.2.4). Although (7.2.7) and (7.3.5) have similar appearance, they are very different equations in that (7.2.7) relates the total strain on the inhomogeneity to the average strain over the entire composite, while (7.3.5) relates the total strain on the inhomogeneity to the average strain on the matrix surrounding the inhomogeneity. Therefore, the tensor Tr in (7.2.7) represents the global strain concentration, while the tensor Tr in (7.3.5) represents local strain concentration tensor introduced in (5.7.9), that is, Gr ⫽ Tr.

(7.3.6)

Thus, it follows from (5.7.14) that the global strain concentration tensor is

冋

冘cG册

Ar ⫽ Gr c0I ⫹

冋冘 册

⫺1

N

n

⫺1

N

⫽ Tr

n

cnTn

,

(7.3.7)

n⫽0

n⫽1

where the fact that T0 ⫽ I has been used. Consequently, the effective stiffness tensor of the composite follows directly from (5.7.7):

冘 c (L ⫺ L )A ⫽ L ⫹ 冘 c (L ⫺ L )T 冋 冘 c T 册 ⫽ L ⫹ 冘 c L T 冋冘 c T 册 ⫺ L 冘 c T 冋冘 c T 册 ⫽ 冘 c L T 冋冘 c T 册 (7.3.8) N

L ⫽ L0 ⫹

r

r

0

r

r⫽1 N

0

r

r

0

r

n

N

r

r

r

n

N

n

N

r

r⫽0

r

n

n

n⫽0

⫺1

N

r

⫺1

N

0

n⫽0

r⫽0

r

⫺1

N

0

r

n

n⫽0

r⫽0

r⫽0

⫺1

N

n

n

n⫽0

or

冘 c L T 冋冘 c T 册 N

L⫽

r

r⫽0

⫺1

N

r

r

n

n

.

(7.3.9)

n⫽0

This is the Mori–Tanaka estimate of the effective stiffness tensor.

7.3

MORI–TANAKA METHOD

167

To obtain the Mori–Tanaka estimate of the effective complaint tensor, we substitute 0 ⫽ M00,

r ⫽ Lrr

(7.3.10)

into (7.3.5), which yields r ⫽ LrTr M00.

(7.3.11)

The local stress concentration tensor is thus given by Hr ⫽ LrTr M0.

(7.3.12)

It then follows from (5.7.15) that the global stress concentration tensor is given by

冋

冘cH册

⫺1

N

Br ⫽ Hr c0I ⫹

n

n

n⫽1

冋冘 c L T M 册

⫺1

N

⫽ LrTr M0

n

n

n

,

0

(7.3.13)

n⫽0

where the fact that H0 ⫽ L0T0M0 ⫽ I has been used. The Mori–Tanaka effective compliant tensor thus follows from (5.7.8):

冘 c (M ⫺ M )B ⫽ M ⫹ 冘 c (M ⫺ M )L T M 冋 冘 c L T M 册 ⫽ M ⫹ 冘 c T M 冋冘 c L T M 册 ⫺ M 冘 c L T M 冋冘 c L T M 册 ⫽ 冘 c T M 冋冘 c L T M 册 ⫽ 冘 c T 冋冘 c L T 册 N

M ⫽ M0 ⫹

r

r

0

r

r⫽1 N

0

r

r

0

r

r

0

n

N

r

r

0

n

N

n

n

0

⫺1

N

0

r

r

r

0

n

n

n

0

n⫽0

r⫽0

N

⫺1

N

0

n

n

n

0

n⫽0

r⫽0 N

⫺1

N

r

or

0

n⫽0

r⫽0

r⫽0

n

⫺1

N

0

r

n

n⫽0

r⫽0

r

⫺1

N

r

n

n⫽0

n

n

(7.3.14)

168

DETERMINATION OF EFFECTIVE MODULI

冘 N

M⫽

r⫽0

冋冘

册

⫺1

N

crTr

cnLnTn

n⫽0

.

(7.3.15)

This is the Mori–Tanaka estimate of the effective compliance tensor of the composite in consideration. It is easy to see from (7.3.9) and (7.3.15) that, unlike in the Eshelby method, the Mori–Tanaka method yields ML ⫽ LM ⫽ I for any cr. Example 7.2 Let us use the Mori–Tanaka method to estimate the effective elastic tensor and the effective compliant tensor for the composite considered in Example 7.1. First, consider (7.3.9) for r ⫽ 1, L ⫽ (c0L0T0 ⫹ c1L1T1)(c0T0 ⫹ c1T1)⫺1 ⫽ (c0L0 ⫹ c1L1T1)(c0I ⫹ c1T1)⫺1,

(7.3.16)

T1 ⫽ [I ⫹ S1 (M0L1 ⫺ I)]⫺1.

(7.3.17)

where

By substituting (7.3.17) into (7.3.16) and making use of (7.2.19)– (7.2.22), we obtain using the symbolic notation, L ⫽ (3K, 2),

(7.3.18)

where K ⫽ K0 ⫹

c1K0(K1 ⫺ K0) , K0 ⫹ 3␥0(1 ⫺ c1)(K1 ⫺ K0)

(7.3.19)

⫽ 0 ⫹

c10(1 ⫺ 0) . 0 ⫹ 2␦0(1 ⫺ c1)(1 ⫺ 0)

(7.3.20)

Eliminating ␥0 and ␦0 by using (7.2.22), we can rewrite (7.3.20) as K ⫽ K0 ⫹ ⫽ 0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(7.3.21)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 50(3K0 ⫹ 40) ⫹ 6(1 ⫺ c1)(1 ⫺ 0)(K0 ⫹ 20) (7.3.22)

7.4

SELF-CONSISTENT METHODS FOR COMPOSITE MATERIALS

169

These are the Mori–Tanaka estimates of the effective elastic constants for a composite with spherical particles.

7.4 SELF-CONSISTENT METHODS FOR COMPOSITE MATERIALS

Again, consider the composite material stated in Section 7.1. Let us pretend at this point that we already knew the effective stiffness tensor L and its inverse M. Since there are numerous inhomogeneities in the composite, we know that the effective properties (L and M) will not be affected if one inhomogeneity is removed from the composite. Now, focus our attention to a typical inhomogeneity, for example, the rth inhomogeneity. When the composite is subjected to either the displacement boundary condition or the traction boundary condition, one may envision that the effects of the applied loads (through the boundary condition) and the interaction with other inhomogeneity can be accounted for by assuming that the rth inhomogeneity is placed within a homogeneous matrix of stiffness L that had been subjected to the strain tensor before the inhomogeneity is embedded; see Figure 7.7. With this understanding, we can choose in (7.1.3),

V3

V2 Vr

Vr

VN

=

V1

L

V0

(a)

(b)

Figure 7.7 (a) The rth inhomogeneity in the actual composite. (b) The rth inhomogeneity in a homogeneous matrix with (as-yet-unknown) effective stiffness L that has been subjected to the uniform strain before the inhomogeneity was embedded.

170

DETERMINATION OF EFFECTIVE MODULI

Lˆ 0 ⫽ L and ˆ 0 ⫽ ,

(7.4.1)

Sˆ r ⫽ Sr,

(7.4.2)

and consequently,

where the overbar on the Eshelby tensor indicates that its elements should be computed based on the effective elastic constants of the composite. Substituting (7.4.1) and (7.4.2) into (7.1.6) yields the total strain in the rth inhomogeneity: r ⫽ ⫹ pt r ⫽ ⫹ S* r ⫽ Tr,

(7.4.3)

Tr ⫽ [I ⫽ SrL⫺1(Lr ⫺ L)]⫺1.

(7.4.4)

where

The corresponding stress on the rth inhomogeneity is r ⫽ Lrr ⫽ LrTr ⫽ LrTr M.

(7.4.5)

It is seen that the global strain and stress concentration tensors for the rth inhomogeneity are, respectively, Ar ⫽ Tr and Br ⫽ LrTr M.

(7.4.6)

Thus, it follows from (5.7.7) and (5.7.8) that the effective stiffness and compliant tensors of the composite are given, respectively, by

冘 c (L ⫺ L )T ,

(7.4.7)

冘 c (M ⫺ M )L T M,

(7.4.8)

N

L ⫽ L0 ⫹

r

r

0

r

r⫽1 N

M ⫽ M0 ⫹

r

r

0

r

r

r⫽1

where Tr is given in (7.4.4). These are the self-consistent estimates of the effective stiffness and compliant tensors of the composite. Unlike the Eshelby and Mori–Tanaka methods, the self-consistent method

7.4

SELF-CONSISTENT METHODS FOR COMPOSITE MATERIALS

171

yields implicit equations for the effective properties. Solutions to these implicit equations typically require numerical iterations using computers. To prove the consistency of the self-consistent estimates, let us consider (7.4.7). Premultiplying by M0 and postmultiplying by L⫺1, we arrive at

冘 c M (L ⫺ L )T L ⫹ 冘 c (M ⫺ M )L T L N

M0 ⫽ L⫺1 ⫹

r

0

r

0

r

⫺1

r⫽1 N

⫺1

⫽L

r

0

r

r

r

⫺1

.

(7.4.9)

r⫽1

By rearranging the terms, we obtain

冘 c (M ⫺ M )L T L N

⫺1

L

⫽ M0 ⫹

r

r

0

r

r

⫺1

.

(7.4.10)

r⫽1

Comparing (7.4.10) with (7.4.8), we observe that M ⫽ L⫺1.

(7.4.11)

L ⫽ M⫺1.

(7.4.12)

Similarly, one can show that

Thus, we have ML ⫽ LM ⫽ I, that is, the self-consistent estimates are indeed consistent. Example 7.3 Consider again the composite described in Example 7.1. To ﬁnd the effective stiffness tensor of the composites using the selfconsistent method, we can use (7.4.7) directly by specifying N ⫽ 1. To this end, let us compute the relevant tensors one at a time. First, the Eshelby tensor for an isotropic material with L ⫽ (3K,2) can be written as (see Appendix 4.B) S ⫽ (3␥, 2␦), where

(7.4.13)

172

␥⫽

DETERMINATION OF EFFECTIVE MODULI

K 3K ⫹ 4

⫽

1⫹ 3K ⫹ 6 4 ⫺ 5 , ␦⫽ ⫽ . 9(1 ⫺ ) 15K ⫹ 20 15(1 ⫺ )

(7.4.14)

Next, let us compute the fourth-order tensor T1, T1 ⫽ [I ⫹ S(L⫺1L1 ⫺ I)]⫺1 ⫽ {(1,1) ⫹ (3␥, 2␦)[(3K, 2)⫺1(3K1, 21) ⫺ (1,1)]}⫺1

冋 冋 冋

冉

冊册 册 册

⫺1

K ⫺ K 1 ⫺ ⫽ (1,1) ⫹ (3␥, 2␦) 1 , K

K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ ) ⫽ , K ⫽

⫺1

K , . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ )

(7.4.15)

Finally L ⫽ L0 ⫹ c1 (L1 ⫺ L0)T1 ⫽ (3K0, 20) ⫹ c1 ⫽

冋

3K0 ⫹

冋

册

3K(K1 ⫺ K0) 2(1 ⫺ 0) , K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ )

册

3c1K(K1 ⫺ K0) 2c1(1 ⫺ 0) , 20 ⫹ . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ ) (7.4.16)

Thus, we have K ⫽ K0 ⫹

c1K(K1 ⫺ K0) c (1 ⫺ 0) , ⫽ 0 ⫹ 1 . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺ )

(7.4.17)

This is a pair of nonlinear algebraic equations. The roots of these equations are the effective elastic constants of the composite. Because of the uniqueness of the problem, selections must be made judiciously based on physical ground if there are multiple roots. A common method to ﬁnd the roots is iteration. Making use of (7.4.14) in (7.4.17) yields a pair of alternative expressions:

7.5

SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

c1(K1 ⫺ K0)(3K ⫹ 4) , 3K1 ⫹ 4

(7.4.18)

5c1(1 ⫺ 0)(3K ⫹ 4) . 3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)

(7.4.19)

K ⫽ K0 ⫹ ⫽ 0 ⫹

173

7.5 SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

The derivations used to develop the methods of determining the effective properties described in previous sections including the selfconsistent method rely on the fact that the composite has a distinct matrix in which other inhomogeneities are embedded. For certain heterogeneous materials, such as polycrystalline materials, there is no distinct matrix phase. In a polycrystal, each grain can be viewed as an inhomogeneity embedded in the remaining grains, and, hence, all grains have the same signiﬁcance. Clearly, there is a complete symmetry in treating each grain as an inhomogeneity. The concept of a matrix with embedded inhomogeneities is thus no longer meaningful. In this section, we will describe other self-consistent methods that treat all inhomogeneities (one may consider the matrix as one of the inhomogeneities) on an equal footing. To begin, let us consider a polycrystalline material comprising N randomly distributed grains. The different grains can be either different materials (in the case of alloys) or grains with different crystallographic orientations (in the case of single-element polycrystals). We assume that the rth grain has volume fraction of cr, r ⫽ 1, 2, 3, . . . , N. It then follows from (5.4.1) that the average strain and average stress in the polycrystal is given by

冘 c, N

⫽

r r

r⫽1

冘 c, N

⫽

r

r

(7.5.1)

r⫽1

where r and r are the average strain and stress tensors, respectively, on the rth grain. Note that is the average strain of the entire polycrystal and r is the average strain of the rth grain. The global strain concentration tensor Ar is deﬁned for the rth grain through (5.7.3):

174

DETERMINATION OF EFFECTIVE MODULI

r ⫽ Ar.

(7.5.2)

Similarly, the global stress concentration tensor is deﬁned for the rth grain through (5.7.9): r ⫽ Br.

(7.5.3)

It then follows from (7.5.2) and (7.5.3) and the use of Hooke’s law that

冘

冘 c L A ,

(7.5.4)

冘 c ⫽ 冘 c M ⫽ 冘 c M B .

(7.5.5)

N

⫽

N

cr Lrr ⫽

r⫽1

r⫽1

N

⫽

冘 N

crr ⫽

N

r r

r

r

N

r

r

r

r⫽1

r⫽1

r

r⫽1

r

r

r

r⫽1

These lead to

冘 N

L⫽

r⫽1

冘 c MB. N

cr LrAr,

M⫽

r

r

r

(7.5.6)

r⫽1

Clearly, once the strain concentration tensor Ar is known as a function of the effective stiffness tensor L for the polycrystal, the ﬁrst of (7.5.6) can be used to obtain the effective stiffness tensor L. Similarly, if the stress concentration tensor Br is known as a function of the effective compliance tensor M, the second of (7.5.6) can be used to obtain the effective compliance tensor M. Generally speaking, the effective compliance and stiffness tensor obtained from these two equations may not be consistent, unless the exact expressions of Ar and Br are used. One way to obtain an approximate solution to Ar is to view each grain as an ellipsoidal inhomogeneity embedded in a homogeneous matrix (consisting of all the other grains) of elastic stiffness tensor L. Under this assumption, when the polycrystal is subjected to displacement boundary condition u兩x僆S ⫽ x, the strain concentration tensor Ar is given by (7.2.4) and (7.2.7) with M0 and L0 replaced by M and L, respectively, because in this case the rth inhomogeneity is embedded in a homogeneous matrix with L, instead of L0, Ar ⫽ [I ⫹ Sr M(Lr ⫺ L]⫺1,

(7.5.7)

7.5

SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

175

where Sr is the Eshelby tensor computed based on L. Substituting (7.5.7) into the ﬁrst of (7.5.6) results in a self-consistent scheme for L:

冘 c L [I ⫹ S L N

L⫽

r

r

⫺1

r

(Lr ⫺ L)]⫺1.

(7.5.8)

r⫽1

To obtain an approximate solution to Br, let us consider the traction boundary condition (7.2.10). In this case, it follows from (7.2.15) that Br ⫽ [Mr ⫺ Sr(Mr ⫺ M)]⫺1 M.

(7.5.9)

Substituting (7.5.9) into the second of (7.5.6) yields a self-consistent scheme for M,

冘 c M [M ⫺ S (M ⫺ M)] N

I⫽

r

r

r

r

r

⫺1

.

(7.5.10)

r⫽1

It can be shown (see Problem 7.8) that the concentration tensors can be written in alternative forms: Ar ⫽ (Lr ⫹ Hr)⫺1(L ⫹ Hr),

⫺1 ⫺1 Br ⫽ (Mr ⫹ H⫺1 r ) (M ⫹ Hr ),

(7.5.11) where Hr ⫽ L(S⫺1 ⫺ I) r

(7.5.12)

is the Hill’s constraint tensor (4.5.13). Thus, the self-consistent schemes can be recast into more symmetric forms:

冘 c L (L ⫹ H ) N

L⫽

r

r

r

r

⫺1

(L ⫹ Hr),

(7.5.13)

r⫽1

冘 c M (M ⫹ H N

M⫽

r

r⫽1

r

r

⫺1 ⫺1 r

) (M ⫹ Hr⫺1).

(7.5.14)

176

DETERMINATION OF EFFECTIVE MODULI

These are implicit algebraic equations for the effective stiffness tensor L. Solutions to these algebraic equations are the effective properties of the polycrystal. Making use of the relationships (see Problem 7.9) LrAr ⫽ BrL,

MrBr ⫽ Ar M,

one can easily show that the stiffness and compliance tensors predicted from (7.5.13) and (7.5.14), respectively, are indeed consistent, that is, LM ⫽ ML ⫽ I. Let us now consider a single-phase polycrystalline material. Singlephase polycrystal is an assembly of grains, all of which are comprised of the same material. Although all the grains are of the same material, their physical orientations are different. By physical orientation we mean rotations of the grain with respect to a ﬁxed reference frame, or equivalently, the rotation of the stiffness tensor with respect to a ﬁxed coordinate system. For example, let L be the elastic stiffness tensor of a single crystal in a ﬁxed coordinate system (x1, x2, x3). Then, the stiffness tensor of the same crystal in a different orientation can be represented by a rotation of L, that is, L(r) ijkl ⫽ ␣ip␣jq␣kr␣lsLpqrs,

(7.5.15)

where the rotation matrix can be expressed, for example, in terms of the Euler angles , , and : ␣11 ⫽ cos cos cos ⫺ sin sin , ␣12 ⫽ ⫺cos cos sin ⫺ sin cos , ␣13 ⫽ sin cos , ␣21 ⫽ cos sin cos ⫹ cos sin , ␣22 ⫽ ⫺cos sin sin ⫹ cos cos , ␣13 ⫽ sin sin , ␣31 ⫽ ⫺sin cos , ␣32 ⫽ sin sin , ␣32 ⫽ cos ,

where

(7.5.16)

7.5

SELF-CONSISTENT METHODS FOR POLYCRYSTALLINE MATERIALS

0 ⱕ ⱕ 2,

0 ⱕ ⱕ ,

0 ⱕ ⱕ 2.

177

(7.5.17)

Since all the grains are comprised of the same material, only with different orientations, we can write, symbolically, that, ˜ Lr ⫽ L(L, , , ),

˜ Mr ⫽ M(M, , , ).

(7.5.18)

To characterize the physical orientation of the grains in a given single-phase polycrystal, we use a distribution function ƒ(, , ), that is, 1 8 2

冕

2

0

d

冕

0

sin d

冕

2

0

ƒ(, , ) d ⫽ 1.

(7.5.19)

The value ƒ(0, 0, 0) represents the percent of grains that are all oriented in the direction (0, 0, 0). Clearly, ƒ(, , ) ⫽ ␦( ⫺ 0)␦( ⫺ 0)␦( ⫺ 0) would mean all the grains are orientated in the (0, 0, 0) direction. In addition to physical orientation, each grain (ellipsoidal inhomogeneity) in the polycrystal has its own size, shape, and orientation, all of which may not be the same for all grains. Since these geometric attributes come into the self-consistent equations through only the Eshelby tensor, which is independent of the size of the inhomogeneity, one may conclude that the effective stiffness tensor predicted by the selfconsistent methods (7.5.13) and (7.5.14) is invariant to the grain size. Because of the large number of grains involved, distribution functions are typically used to characterize the geometric shapes and orientations of grains. For example, we can use the Euler angles to indicate the geometric orientation of a grain, so that S(r) ijkl ⫽ ␣ip␣jq␣kr␣lsSpqrs,

(7.5.20)

where Spqrs is the Eshelby tensor for an ellipsoidal inclusion written in the same ﬁxed coordinate system (x1, x2, x3). For convenience, one may choose the ellipsoidal inclusion in such a way that its major axes coincide with the axes of the rectangular coordinate system. Therefore, if all grains have similar shape, the Eshelby tensor for each grain can be written as

178

DETERMINATION OF EFFECTIVE MODULI

˜ Sr ⫽ S(L, , , ),

(7.5.21)

where (, , ) follows a distribution function g(, , ). Replacing the summation by integration and the volume fraction by the distribution function, we can change the self-consistent equations (7.5.13) and (7.5.14) to their integral counterparts that are more suited for polycrystalline materials: ˜ ⫺1 ˜ ˜ ⫹ SL 具g具ƒL[I (L ⫺ L)]⫺1典典 ⫽ L,

(7.5.22)

˜ ˜ ˜ ˜ ⫺ S(M ⫺ M)]⫺1典典 ⫽ I, 具g具ƒM[M

(7.5.23)

where the symbol 具 典 ⫽ is deﬁned as 具典⬅

冕

2

0

d

冕

0

sin d

冕

2

0

d.

(7.5.24)

Let us, for brevity, use only (7.5.22) to consider some special cases: 1. Both geometric and physical orientations are random. In this case, ƒ(, , ) ⫽ g(, , ) ⫽ 1. Thus, (7.5.22) reduces to ˜ ⫺1 ˜ ˜ [I ⫹ SL 具具L (L ⫺ L)]⫺1典典 ⫽ L.

(7.5.25)

2. Both geometric and physical orientations are aligned. In this case, ƒ(, , ) ⫽ g(, , ) ⫽ ␦()␦()␦(). Thus, (7.5.22) reduces to ˜ L(L, 0, 0, 0)[I ˜ ˜ ⫹ S(L, 0, 0, 0)M(L(L, 0, 0, 0) ⫺ L)]⫺1 ⫽ L. (7.5.26)

It can be easily seen from (7.5.20) and (7.5.15) that ˜ S(L, 0, 0, 0) ⫽ S,

˜ L(L, 0, 0, 0) ⫽ L.

(7.5.27)

Thus, we have L[I ⫹ SM(L ⫺ L)]⫺1 ⫽ L. Equivalently, this leads to

(7.5.28)

7.6

L ⫽ L,

DIFFERENTIAL SCHEMES

179

(7.5.29)

that is, the effective stiffness tensor is the stiffness tensor of the single crystal. This is certainly expected since all the grains are aligned both geometrically and physically. In other words, the polycrystal in this case is actually a single crystal!

7.6 DIFFERENTIAL SCHEMES

The differential scheme in determining the effective modulus of a composite takes a somewhat different approach from the methods introduced in previous sections. The differential approach was motivated by the fact that the effective properties of a dilute composite can be calculated with relatively high accuracy. Therefore, one may imagine that a composite with a ﬁnite concentration of inhomogeneities can be constructed through the following process. First, start with the homogeneous matrix material with elastic stiffness tensor L0. Then, add a small amount (volume fraction ⌬c) inhomogeneities with elastic stiffness tensor L1. We now have a composite with dilute concentration. The effective elastic stiffness tensor L(1)(⌬c, L0) can be obtained accurately, where the fact that the effective stiffness tensor depends on the volume fraction of the inhomogeneities and the matrix material is explicitly indicated. In the next step, we will start with a homogenous matrix of elastic stiffness tensor L(1)(⌬c, L0). Then add a small amount (volume fraction ⌬c) of inhomogeneities of stiffness tensor L1. Again, we have created a new composite. As far as this composite is concerned, it still has a dilute concentration of L1. Therefore, the effective stiffness tensor of this new composite can be obtained accurately using the same method used for the previous step. The only difference here is that the matrix material in the current step is L(1)(⌬c, L0). Therefore, one can symbolically write the effective stiffness tensor at the current step as L(2)(⌬c, L(1)). This process can continue. Each time, the newly obtained composite will be viewed as a homogeneous matrix, and a small amount of inhomogeneities of L1 is added to obtain the next composite, until the desired volume fraction is achieved. Such a repetitive process leads to differential equations for the effective properties as functions of the concentrations (or volume fractions of the inhomogeneities). This is the basic idea of all the differential schemes. To illustrate how such thought process can be translated into differential equations, let us consider a two-phase composite (N ⫽ 1). Ac-

180

DETERMINATION OF EFFECTIVE MODULI

cording to (5.7.7), the effective stiffness tensor of a two-phase composite can be written as L(c1) ⫽ L0 ⫹ c1 (L1 ⫺ L0)⬊A1(L0),

(7.6.1)

where the dependence of L on the volume fraction c1 and A1 on L0 is explicitly indicated, and the strain concentration tensor A1 is deﬁned by 1 ⫽ A1 (L0)⬊.

(7.6.2)

In the above, the symbol ⬊ has been used to indicate the tensor product. This is to make it clear that A1 (L0) means A1 is a function of L0. Let us assume that the effective stiffness tensor L(c1) is known at a volume fraction c1 ⫽

⍀1 , ⍀0 ⫹ ⍀1

(7.6.3)

where ⍀0 and ⍀1 are, respectively, the volumes of the matrix and inhomogeneities. If the composite with stiffness tensor L(c1) is viewed as a homogeneous ‘‘matrix,’’ a new composite can be made by adding ⌬⍀1 amount of new inhomogeneities to the ‘‘matrix.’’ The volume fraction of the newly added inhomogeneities is ⌬⍀1 . ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1

(7.6.4)

For such small-volume fractions, the effective elastic stiffness tensor can be obtained from (7.6.1) by replacing L0 by the new matrix property L(c1), that is, L(c1 ⫹ ⌬c1) ⫽ L(c1) ⫹

⌬⍀1 (L ⫺ L(c1))⬊A1(L(c1)), ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1 1

(7.6.5) where ⌬c is the increment of the volume fraction of L1 in the composite due to the addition of ⌬⍀1 amount of L1. Clearly, the total volume fraction of L1 in this newly constructed composite is

7.6

c1 ⫹ ⌬c1 ⫽

181

DIFFERENTIAL SCHEMES

⍀1 ⫹ ⌬⍀1 . ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1

(7.6.6)

Subtracting (7.6.3) from (7.6.6) yields ⌬c1 ⫽

⍀0⌬⍀1 (⍀0 ⫹ ⍀1)(⍀0 ⫹ ⍀1 ⫹ ⌬⍀1)

⫽

(⍀0 ⫹ ⍀1 ⫺ ⍀1)⌬⍀1 (⍀0 ⫹ ⍀1)(⍀0 ⫹ ⍀1 ⫹ ⌬⍀1)

⫽

(1 ⫺ c1)⌬⍀1 ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1

(7.6.7)

or ⌬⍀1 ⌬c1 ⫽ . ⍀0 ⫹ ⍀1 ⫹ ⌬⍀1 (1 ⫺ c1)

(7.6.8)

Substitution of (7.6.8) into (7.6.5) yield L(c1 ⫹ ⌬c1) ⫺ L(c1) 1 ⫽ (L ⫺ L(c1))⬊A1(L(c1)). ⌬c1 1 ⫺ c1 1

(7.6.9)

In the limit of ⌬c1 → 0, a ﬁrst-order differential equation is derived: dL(c1) 1 ⫽ (L ⫺ L(c1))⬊A1(L(c1)). dc1 (1 ⫺ c1) 1

(7.6.10)

The initial condition to compliment the differential equation is obviously L(c1)兩c1⫽0 ⫽ L0.

(7.6.11)

It is straightforward to derive the dual of (7.6.10) and (7.6.11), dM(c1) 1 ⫽ (M1 ⫺ M(c1))⬊B1(M(c1)), dc1 (1 ⫺ c1)

(7.6.12)

M(c1)兩c1⫽0 ⫽ M0,

(7.6.13)

182

DETERMINATION OF EFFECTIVE MODULI

where B1 is the stress concentration tensor deﬁned by (5.7.8). These initial value problems are the starting point for the various differential schemes, depending on how the strain concentration tensors A1 and B1 are computed. Let us consider ﬁrst the Eshelby approach discussed in Section 7.2. It follows from (7.2.8) and (7.2.4) that A1(L(c1)) ⫽ T1兩L0⫽L(c1) ⫽ [I ⫹ S1(L⫺1L1 ⫺ I)]⫺1,

(7.6.14)

where L⫺1 ⫽ S1 ⫽ (3␥, 2␦) ⫽

冉

冉

冊

1 1 , , 3K 2

(7.6.15)

冊

3(K ⫹ 2) , . 3K ⫹ 4 5(3K ⫹ 4) K

(7.6.16)

Note that it goes without saying that all the quantities with an overbar are functions of the volume fraction c. Substituting the above into (7.6.10) and (7.6.11) yields dL 1 ⫽ (L ⫺ L)[I ⫹ S1(L⫺1L1 ⫺ I)]⫺1, dc1 1 ⫺ c1 1

(7.6.17)

L(0) ⫽ L0.

(7.6.18)

For the composite described in Example 7.2, we have T1兩L0⫽L(c) ⫽ [I ⫹ S1(L⫺1L1 ⫺ I)]⫺1 K ⫽ , . K ⫹ 3␥(K1 ⫺ K) ⫹ 2␦(1 ⫺

冉

冊

(7.6.19)

Making use of the above in (7.6.17), we have dK (K ⫺ K1)(3K ⫹ 4) ⫹ ⫽ 0, dc (1 ⫺ c)(3K1 ⫹ 4) d 5( ⫺ 1)(3K ⫹ 4) ⫹ ⫽ 0. dc (1 ⫺ c)[3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)] The solution must satisfy the initial conditions

(7.6.20)

(7.6.21)

7.7

COMPARISON OF DIFFERENT METHODS

K(0) ⫽ K0 and (0) ⫽ 0.

183

(7.6.22)

Clearly, this is a set of highly nonlinear ordinary differential equations. Numerical procedures are typically required to obtain the solution. Another version of the differential scheme is attained by following the Mori–Tanaka approach in obtaining the strain concentration tensor. It follows from (7.3.7) that A1(L(c1)) ⫽ T1[(1 ⫺ c1)I ⫹ c1T1]⫺1兩L0⫽L(c1). The differential equation now becomes dL 1 ⫽ (L ⫺ L)T1[(1 ⫺ c1)I ⫹ c1T1]⫺1兩L0⫽L(c1). dc1 1 ⫺ c1 1

(7.6.23)

7.7 COMPARISON OF DIFFERENT METHODS

In the previous sections, we have introduced several methods of estimating the effective stiffness (compliance) tensors for a given composite, namely, the Eshelby method (or the dilute concentration method), the Mori–Tanaka method, the self-consistent method, and the differential method. In this section, we will use these methods to obtain the effective moduli of several idealized composite materials where explicit analytical solutions can be obtained. We will compare the results to assess the validity and accuracy of these methods. We ﬁrst state that, based on the assumptions made in deriving them, all these methods ignore the spatial distribution of the inhomogeneities, that is, they all assume uniform distribution. However, the shapes and orientations of the ellipsoidal inhomogeneities are taken into account through the Eshelby tensor Sr. Note that the Eshelby tensor is shape dependent but not size dependent. Thus, the effective modulus tensor predicted by these methods will not depend on the size of the inhomogeneities. Interactions among the inhomogeneities are taken into consideration differently by different methods. In general, the Eshelby method works only for very dilute concentration, and the other methods are applicable to somewhat higher concentration. We will see some numerical examples later in this section. Now consider the composite material described in Example 7.1. For convenience, we list below the equations for the effective moduli of this composite obtained by all these methods and consider a few special cases.

184

DETERMINATION OF EFFECTIVE MODULI

The Eshelby method: c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K1 ⫹ 40

(7.7.1)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 3K0(30 ⫹ 21) ⫹ 4 0(20 ⫹ 31)

(7.7.2)

K ⫽ K0 ⫹

⫽ 0 ⫹

The Mori–Tanaka method: K ⫽ K0 ⫹

⫽ 0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(7.7.3)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 50(3K0 ⫹ 40) ⫹ 6(1 ⫺ c1)(1 ⫺ 0)(K0 ⫹ 20) (7.7.4)

The self-consistent method: c1(K1 ⫺ K0)(3K ⫹ 4) , 3K1 ⫹ 4

(7.7.5)

5c1(1 ⫺ 0)(3K ⫹ 4) . 3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)

(7.7.6)

K ⫽ K0 ⫹

⫽ 0 ⫹

The differential method: dK (K ⫺ K1)(3K ⫹ 4) ⫹ ⫽ 0, dc1 (1 ⫺ c1)(3K1 ⫹ 4) d 5( ⫺ 1)(3K ⫹ 4) ⫹ ⫽ 0, dc1 (1 ⫺ c1)[3K(3 ⫹ 21) ⫹ 4(2 ⫹ 31)] K兩c1⫽0 ⫽ K0 and 兩c1⫽0 ⫽ 0.

(7.7.7)

(7.7.8) (7.7.9)

7.7

COMPARISON OF DIFFERENT METHODS

185

Dilute Concentration

For dilute concentration of inhomogeneities, we can assume c1 ⬍⬍ 1. Therefore, by expanding (7.7.3) and (7.7.4) into power series of c1 and neglecting high-order terms, we have c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K1 ⫹ 40

(7.7.10)

5c10(1 ⫺ 0)(3K0 ⫹ 40) . 3K0(30 ⫹ 21) ⫹ 40(20 ⫹ 31)

(7.7.11)

K ⫽ K0 ⫹

⫽ 0 ⫹

Comparing the above with the Eshelby estimate, it is seen that at the dilute concentration, the Mori–Tanaka estimate reduces to the Eshelby results. As for the self-consistent estimate, we can ﬁrst expand K and into power series of c1, that is, K ⫽ K0 ⫹ c1K0(1) ⫹ c12K0(1) . . . ,

(7.7.12)

⫽ 0 ⫹ c10(1) ⫹ c120(1) . . . .

(7.7.13)

Substituting these expansions into (7.7.5) and (7.7.6) yields immediately that the self-consistent estimate, in the dilute case, also reduces to the Eshelby estimate. Following similar steps, one can show that the differential method predicts the same results as well (as expected, since the differential method was based on the solution to the dilute case). In other words, all four methods yield the same results when the volume fraction of the inhomogeneity is very low. In the limit of c1 → 0, the effective modulus of the composite as predicted by all these methods reduce to the modulus of the matrix, as it should. High-Concentration Asymptotes

For this case, we are interested in the limit c1 → 1, meaning the entire ‘‘composite’’ consists of particles only. Certainly, this would require multiple size particles; see Problem 7.6. Since the composite contains particles only, it is expected that the effective modulus of the composite

186

DETERMINATION OF EFFECTIVE MODULI

should be the modulus of the particles. Taking the limit c1 → 1 in (7.7.1)–(7.7.6), we ﬁnd that the Eshelby method predicts K0(2K1 ⫺ K0) ⫹ 40K1 , 3K1 ⫹ 40

(7.7.14)

0[3K0(71 ⫺ 20) ⫹ 40(81 ⫺ 30)] . 3K0(30 ⫹ 21) ⫹ 40(20 ⫹ 31)

(7.7.15)

K⫽

⫽

It is not surprising that the Eshelby method does not predict the correct values because the Eshelby method is valid only for dilute concentrations. It is very easy to see by setting c1 ⫽ 1 in (7.7.3) and (7.7.4) that the Mori–Tanaka method does predict the proper limiting values for the effective moduli: K ⫽ K1,

⫽ 1.

(7.7.16)

It can also be easily veriﬁed that (7.7.16) represent a set of solutions to the self-consistent equations (7.7.5) and (7.7.6). In other words, the self-consistent method also predicts the property high-concentration limit. Rigid Particles

To mimic rigid particles, one may consider the limiting case of 0 → 0, 1

K0 → 0. K1

(7.7.17)

Also, on physical grounds, we assume that → 0, 1

K →0 K1

for any 0 ⱕ c1 ⬍ 1. Making use of the above in (7.7.1)–(7.7.4), we obtain

(7.7.18)

7.7

K ⫽ K0 ⫹

COMPARISON OF DIFFERENT METHODS

c1(3K0 ⫹ 40) , 3

⫽ 0 ⫹

187

5c10(3K0 ⫹ 40) , 6(K0 ⫹ 20) (7.7.19)

from the Eshelby method, and K ⫽ K0 ⫹

c1(3K0 ⫹ 40) , 3(1 ⫺ c1)

⫽ 0 ⫹

5c10(3K0 ⫹ 40) 6(K0 ⫹ 20)(1 ⫺ c1) (7.7.20)

from the Mori–Tanaka method. Again, it is seen that both methods predict correctly that K ⫽ K0 and ⫽ 0 at the low-concentration limit c1 → 0. At the high-concentration limit, c1 → 1, the Mori–Tanaka method predicts that the effective modulus increases without bound (as it should because the composite is full of rigid particles), while the Eshelby method yields a ﬁnite value. This is expected, for we know that the Eshelby method is applicable only for the dilute case. Making use of (7.7.17) and (7.7.18) in the self-consistent estimate, we obtain K ⫽ K0 ⫹

c1(3K ⫹ ) , 3

⫽ 0 ⫹

5c1(3K ⫹ 4) . 6(K ⫹ 2)

(7.7.21)

The effective bulk modulus K can be solved from (7.7.21) to yield K⫽

3K0 ⫹ 4c1 . 3(1 ⫺ c1)

(7.7.22)

Substituting (7.7.22) into the second of (7.7.21) yields

冉冊 冋

12(1 ⫺ 2c1)

0

2

⫹

3(2 ⫺ 5c1)

册

K0 6K0 ⫺ 4(3 ⫺ c1) ⫺ ⫽ 0. 0 0 0 (7.7.23)

When c1 ⫽ 0.5, the above equation reduces to

188

DETERMINATION OF EFFECTIVE MODULI

12K00 ⫽⫺ ⬍ 0. 3K0 ⫹ 200

(7.7.24)

This is not a physically possible solution because the effective shear modulus should be positive. For c1 ⫽ 0.5, the quadratic equation (7.7.23) yields two roots. Numerical analysis shows that both roots are real. One of them is always negative and other is given by  ⫽␣⫹ ⫹ 0 1 ⫺ 2c1

冪冉

␣⫹

冊

 1 ⫺ 2c1

2

⫹

1 ⫹ 0 , 3(1 ⫺ 20)(1 ⫺ 2c1) (7.7.25)

where 0 is the Poisson ratio of the matrix material, and 3(1 ⫹ 30) ␣⫽⫺ , 24(1 ⫺ 20)

⫽

11 ⫺ 190 . 24(1 ⫺ 20)

(7.7.26)

In deriving (7.7.25), we have used the relationship 0 3(1 ⫺ 20) ⫽ . K0 2(1 ⫹ 0)

(7.7.27)

Since 0 ⱕ 0 ⱕ 0.5, it can be shown that the right hand of (7.7.25) is positive only for 0 ⱕ c1 ⬍ 0.5. In other words, for spherical rigid particles dispersed in a matrix material, the self-consistent method yields a physically meaningful solution to the effective shear modulus only if the particle volume fraction is less than 50%. Now, consider the differential method. Making use of (7.7.18) in (7.7.7) and (7.7.8) yields dK (3K ⫹ 4) ⫺ ⫽ 0, dc1 3(1 ⫺ c1)

(7.7.28)

d 5(3K ⫹ 4) ⫺ ⫽ 0. dc1 6(1 ⫺ c1)(K ⫹ 2)

(7.7.29)

Solutions to this system of nonlinear differential equations are still fairly complicated. To exam the high-concentration asymptotic behavior of the differential scheme predictions, let us expand the solution near c1 ⫽ 1:

7.7

K⫽

冘 (1 ⫺Ac ) ⬁

n

n⫽0

, m–n

COMPARISON OF DIFFERENT METHODS

⫽

冘 (1 ⫺Bc ) ⬁

n

n⫽0

1

189

,

m–n

(7.7.30)

1

where the asymptotic behavior is dictated by the constant m, which is to be determined from the solution procedure. Substituting (7.7.30) into (7.7.28) and (7.7.29) and keeping the leading order terms only, we obtain the following eigenvalue problem:

冋

3(m ⫺ 1) 3(2m ⫺ 5)

册冋 册 冋 册

⫺4 4(2m ⫺ 5)

A0 0 ⫽ . B0 0

(7.7.31)

The corresponding eigenvalues are m ⫽ 0 and m ⫽ 2. The eigenvalue m ⫽ 2 should be chosen on physical ground. Therefore, the asymptotic behavior of the differential scheme for c1 → 1 is K⬇

A0 , (1 ⫺ c1)2

⬇

B0 . (1 ⫺ c1)2

(7.7.32)

In summary, for the case of rigid particles, the Eshelby method yields ﬁnite values of the effective moduli in the high-concentration limit c1 → 1, while the self-consistent method yields no solution for c1 ⬎ 1 in this case. Both the Mori–Tanaka and the differential methods predict unbounded effective moduli, but their asymptotic behavior is different. The Mori–Tanaka solution behaves as 1/(1 ⫺ c1) while the differential solution behaves as 1/(1 ⫺ c1)2. Other interesting features of the differential scheme can also be explored. For example, in the case of the incompressible matrix, that is, /K → 0, (7.7.28) and (7.7.29) reduce to dK K ⫺ ⫽ 0, dc 1 ⫺ c1

(7.7.33)

d 5 ⫺ ⫽ 0. dc 2(1 ⫺ c1)

(7.7.34)

The solutions that satisfy the initial conditions (7.7.9) are K⫽

K0

, 1⫺c

⫽

0 . (1 ⫺ c1)5 / 2

We see that the differential scheme does predict correctly

(7.7.35)

190

DETERMINATION OF EFFECTIVE MODULI

K ⫽ K0,

⫽ 0

(7.7.36)

in the low-concentration limit c → 0. It also predicts that in the highconcentration limit c → 1, shear modulus approaches to inﬁnity with the order of 1/(1 ⫺ c1)5 / 2. Note that the solutions (7.7.32) and (7.7.35) are different in that the former is valid c1 ⫽ 1, while the later is for the incompressible matrix, and is valid for all ranges of c1 between 0 and 1. Voids

Consider a matrix containing spherical voids. When the void content is zero (c1 ⫽ 0), we should expect that the effective modulus is the same as that of the matrix. For high concentration of voids (c1 → 1), we should expect the effective modulus approaches to zero. Let us see how the various methods predict these limiting cases. For voids, we can consider the limiting case of 1 → 0, 0

K1 → 0. 0

(7.7.37)

The Eshelby estimate reduces to K ⫽ K0 ⫺

c1K0(3K0 ⫹ 40) , 40

(7.7.38)

⫽ 0 ⫺

5c10(3K0 ⫹ 40) . 9K0 ⫹ 80

(7.7.39)

They correctly predict the low-concentration limiting value for c1 → 0. For c1 → 1, the Eshelby method yields 3K 3 K ⫽ ⫺ 0, 40

6 (K ⫹ 20) ⫽⫺ 0 0 . 9K0 ⫹ 80

(7.7.40)

These obviously are not physically admissible solutions. The Mori–Tanaka method gives K ⫽ K0 ⫺

c1K0(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫺ 3(1 ⫺ c1)K0

(7.7.41)

7.7

⫽ 0 ⫺

COMPARISON OF DIFFERENT METHODS

5c10(3K0 ⫹ 40) . 5(3K0 ⫹ 40) ⫺ 6(1 ⫺ c1)(K0 ⫹ 20)

191

(7.7.42)

For low concentration, c1K0(3K0 ⫹ 40) , 40

K ⬇ K0 ⫺

⬇ 0 ⫺

5c10(3K0 ⫹ 40) . 9K0 ⫹ 80 (7.7.43)

For high concentration K⬇

40K0 (1 ⫺ c1), 3K0 ⫹ 40

⬇

0(9K0 ⫹ 80) (1 ⫺ c1). 5(3K0 ⫹ 40)

(7.7.44) We see that the Mori–Tanaka method predicts both low- and highconcentration limits correctly, while the Eshelby method is only good for low concentration. Similarly, the self-consistent estimate reduces K ⫽ K0 ⫺

c1K0(3K ⫹ 4) , 4

⫽ 0 ⫺

5c10(3K ⫹ 4) . 9K ⫹ 8

(7.7.45)

Solving the ﬁrst of (7.7.45) for K yields K⫽

4(1 ⫺ c1)K0 . 3c1K0 ⫹ 4

(7.7.46)

Making use of this in the second of (7.7.45) gives us the following quadratic equation for the effective shear modulus:

冉冊 冋

8 0

2

⫹

3(3 ⫺ c1)

册

K0 K ⫺ 4(2 ⫺ 5c1) ⫺ 9(1 ⫺ 2c1) 0 ⫽ 0. 0 0 0 (7.7.47)

When c1 ⫽ 0.5, the two roots of this quadratic equation are, respectively, zero and

192

DETERMINATION OF EFFECTIVE MODULI

冉

⫽⫺

冊

15K0 0 ⫹ ⬍ 0. 16 4

Neither of them is physically meaningful. For c1 ⫽ 0.5, the two roots are all real. Numerical analysis shows that one of these roots is always negative and the other root is given by ⫽ ␣(1 ⫺ 2c1) ⫺  ⫹ 0

冪[␣(1 ⫺ 2c ) ⫺ ] ⫹ 3(1 ⫹4(1 ⫺)(12⫺) 2c ), 0

2

1

1

0

(7.7.48) where 3(3 ⫺ 70) , 16(1 ⫺ 20)

␣⫽

⫽

7 ⫹ 0 . 16(1 ⫺ 20)

(7.7.49)

Since 0 ⱕ 0 ⱕ 0.5, it can be shown that the right hand of (7.7.48) is positive only for 0 ⱕ c1 ⬍ 0.5. In other words, for spherical voids dispersed in an elastic matrix material, the self-consistent method yields a physically meaningful solution to the effective shear modulus only if the void volume fraction is less than 50%. It is seen from the above cases that the self-consistent method has trouble when the particles are rigid or voids. In fact, it is generally true that the self-consistent method does not work well when the contrast between the inhomogeneities and matrix is too large. Now, consider the differential scheme. Use of (7.7.37) leads to dK K(3K ⫹ 4) ⫹ ⫽ 0, dc1 4(1 ⫺ c1)

(7.7.50)

d 5(3K ⫹ 4) ⫹ ⫽ 0. dc1 (1 ⫺ c1)[9K ⫹ 8]

(7.7.51)

Again, we ﬁrst consider the asymptotic behavior near c1 ⫽ 1: K⫽

冘 A (1 ⫺ c ) ⬁

m⫹n

n

n⫽0

1

,

⫽

冘 B (1 ⫺ c ) ⬁

m⫹n

n

1

.

(7.7.52)

n⫽0

By substituting (7.7.52) into (7.7.50) and (7.7.51) and keeping the leading order terms only, we obtain the following eigenvalue problem:

PROBLEMS

冋

3 3(3m ⫺ 5)

册冋 册 冋 册

4(1 ⫺ m) 4(2m ⫺ 5)

A0 0 ⫽ . B0 0

193

(7.7.53)

The corresponding eigenvalues are m ⫽ 0 and m ⫽ 2. The eigenvalue m ⫽ 2 should be chosen on physical ground. Therefore, the asymptotic behavior of the differential scheme for c1 → 1 is ⬇ B0(1 ⫺ c1)2.

K ⬇ A0(1 ⫺ c1)2,

(7.7.54)

Next, let us further assume that the matrix is incompressible, that is, /K → 0. In this case, Eq. (7.7.51) reduces to d 5 ⫹ ⫽ 0. dc1 3(1 ⫺ c1)

(7.7.55)

The solution that satisﬁes the initial condition (7.7.9) is ⫽ 0(1 ⫺ c1)3 / 5.

In summary, for the case of voids, the Eshelby method yields ﬁnite values of the effective moduli in the high-concentration limit c1 → 1, while the self-consistent method yields no physical solution for c1 ⬎ 0.5 in this case. Both the Mori–Tanaka and the differential physical solution for methods yield vanishing effective moduli, but their asymptotic behavior is different. The Mori–Tanaka solution behaves as 1 ⫺ c1, while the differential solution behaves as (1 ⫺ c1)2. PROBLEMS

7.1 Derive (7.2.17) from (7.2.16). 7.2 Show that the Eshelby estimate of the elastic constants for an isotropic spherical particulate-reinforced composite can also be written as

再 冘 ⫹c (2␦ (⫺ ⫺) )冎 c (K ⫺ K ) K ⫽ K 再1 ⫺ 冘 K ⫹ 3␥ (K ⫺ K )冎

⫺1

N

⫽ 0 1 ⫺

r

r⫽1

0

r

0

0

r

⫺1

N

r

r

0

0

r⫽1

where

,

0

0

0

r

0

,

194

DETERMINATION OF EFFECTIVE MODULI

␥0 ⫽ ␦0 ⫽

K0 3K0 ⫹ 40

⫽

1 ⫹ v0 , 9(1 ⫺ v0)

3K0 ⫹ 60 4 ⫺ 5v0 ⫽ . 15K0 ⫹ 200 15(1 ⫺ v0)

7.3 Show, when all the inclusions are similar in shape, that alternative forms of the Mori–Tanaka effective stiffness and compliance tensors are, respectively, given by

再冘 c (L* ⫹ L ) 冎 ⫺ L*, M ⫽ 再 冘 c (M ⫹ M*) 冎 ⫺ M*, ⫺1

N

L⫽

r

0

r

⫺1

0

r⫽0

⫺1

N

r

r

0

⫺1

0

r⫽0

where ⫺1 L* 0 ⫽ L0(S0 ⫺ I),

⫺1 M* ⫺ I]M(0). 0 ⫽ [(I ⫺ S0)

7.4 Prove (7.4.12). 7.5 Show that all three (Eshelby, Mori–Tanake, and self-consistent) estimates are the same for very low volume fractions of inhomogeneities (dilute concentration). 7.6 Assume spherical particles of equal size are dispersed in a matrix material. What is the highest possible volume fraction of the particles? 7.7 Assume circular cross-section ﬁbers of equal radius are placed in a matrix. If all the ﬁbers are aligned in the same direction, what is the highest possible ﬁber volume fraction? 7.8 Show that [I ⫹ Sr M(Lr ⫺ L)]⫺1 ⫽ (Lr ⫹ Hr)⫺1(L ⫹ Hr), ⫺1 ⫺1 [Mr ⫺ Sr(Mr ⫺ M)]⫺1 M ⫽ (Mr ⫹ H⫺1 r ) (M ⫹ Hr ),

where Hr ⫽ L(Sr⫺1 ⫺ I) is the Hill constraint tensor (4.5.14). 7.9 Prove

SUGGESTED READINGS

195

Lr[I ⫹ Sr M(Lr ⫺ L)]⫺1 ⫽ [Mr ⫺ Sr(Mr ⫺ M)]⫺1, Mr[Mr ⫺ Sr(Mr ⫺ M)]⫺1 ⫽ [I ⫹ Sr M(Lr ⫺ L)]⫺1.

SUGGESTED READINGS Benveniste, Y. (1987). A New Approach to the Application of Mori–Tanaka’s Theory in Composite Materials, Mech. Mat., Vol. 6, pp. 147–157. Christensen, R. M. (1990). A Critical Evaluation for a Class of Micromechanics Models, J. Mech. Phys. Solids, Vol. 38, pp. 379–404. Christensen, R. M. (1991). Mechanics of Composite Materials, Krieger, Malabar, FL. Hashin, Z. (1988). The Differential Scheme and Its Applications to Cracked Materials, J. Mech. Phys. Solids, Vol. 36, pp. 719–734. Hill, R. (1963). Elastic Properties of Reinforced Solids: Some Theatrical Principles, J. Mech. Phys. of Solids, Vol. 11, pp. 357–372. Hill, R. (1965). A Self-Consistent Mechanics of Composite Materials. J. Mech. Phys. Solids, Vol. 13, pp. 213–222. McLaughlin, R. (1977). A Study of the Differential Scheme for Composite Materials, Int. J. Engng. Sci., Vol. 15, pp. 237–244. Mori, T. and K. Tanaka. (1973). Average Stress in Matrix and Average Elastic Energy of Materials with Misﬁtting Inclusions, Acta Metall., Vol. 21, pp. 571–574. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston, Chapter 7, Section 45. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York. Norris, A. N. (1985). A Differential Scheme for the Effective Modulus of Composites, Mech. Mat., Vol. 4, pp. 1–16. Walpole, L. J. (1969). On the Overall Elastic Moduli of Composite Materials, J. Mech. Phys. Solids, Vol. 17, pp. 235–251. Walpole, L. J. (1981). Elastic Behavior of Composite Materials: Theoretical Foundations, Advances in Applied Mechanics, Vol. 21, pp. 169–242.

8 DETERMINATION OF EFFECTIVE MODULI— MULTIINCLUSION APPROACHES The methods discussed in the previous chapter are all based on a singleinclusion idea. In this chapter, we will introduce methods of determining the effective properties based on multiple inclusions. This includes coated inclusions.

8.1 COMPOSITE-SPHERE MODEL

The composite-sphere model was ﬁrst introduced by Hashin (1962). It mainly applies to particulate-reinforced composites. This model postulates that a composite is made of an assembly of composite spheres of various sizes. Each composite sphere has a core of radius a comprised of the particle material with stiffness tensor L1 and a shell of thickness b ⫺ a comprised of the matrix material with stiffness tensor L0. Regardless the size of the composite sphere, the ratio of a/b for all spheres in composite is such that the volume fraction of the particle in each composite sphere is that of the particle volume fraction c1 of the entire composite, that is, c1 ⫽ (a/b)3. The size distribution of the composite spheres must be such that the entire space of the composite is fully occupied by the composite spheres. This requires the presence of composite spheres of inﬁnitely small sizes; see Figure 8.1. Clearly, such a model may not be appropriate for a composite with uniform size particles. However, the microstructure so constructed enables us to ﬁnd an exact solution for the effective bulk modulus.

196

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

8.1

COMPOSITE-SPHERE MODEL

197

a b

a

a

b

b Homoteneous Sphere

Composite Sphere

Figure 8.1 Composite-sphere model.

Let us consider ﬁrst the effective bulk modulus of a typical sphere, for example, the rth composite sphere. This can be easily obtained by solving a spherically symmetric deformation problem; see Problem 8.1: Kr ⫽ K0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) , 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(8.1.1)

where c1 ⫽ (a/b)3 is the volume fraction of the particle material. It is interesting to note that this happens to be the Mori–Tanaka estimate of the effective bulk modulus of a particulate-reinforced composite; see Example 7.2. Although (8.1.1) is for the rth composite sphere, it also applies to the entire representative volume element of the composite. To prove this, let the entire representative volume element be subjected to a hydrostatic pressure p, that is, the stress everywhere in the representative volume element of the composite is given by ij ⫽ p␦ij.

(8.1.2)

The corresponding complimentary energy density can then be written as ⌸c[ij] ⫽

1 p p2 ijij ⫽ ii ⫽ . 2 2 2K

where K effective bulk modulus of the composite.

(8.1.3)

198

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

On the other hand, we also know that (8.1.2) is also a statically admissible stress ﬁeld. Therefore, it follows from the minimum complimentary energy theorem (see Section 6.1) that p2 p2 ⫽ ⌸c[ij] ⱕ ⌸c[ˆ ij] ⫽ , 2K 2Kr

(8.1.4)

1 1 ⱕ . K Kr

(8.1.5)

that is,

Similarly, if we assume that the representative volume element of the composite is subjected to displacement boundary conditions so that the strain everywhere in the representative volume element is given by ij ⫽ 0␦ij, then the use of the minimum potential energy theorem leads to K ⱕ Kr.

(8.1.6)

Combining (8.1.5) and (8.1.6) yields the desired relationship: K ⫽ Kr ⫽ K0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) . 3K0 ⫹ 40 ⫹ (1 ⫺ c1)(K1 ⫺ K0)

(8.1.7)

This equality can also be understood as follows. If the composite sphere is in a state of pure radial compression (dilatation), it can be substituted with a sphere of equivalent homogeneous material without perturbing the state of stress in its surroundings. Since the substitution can be performed on all composite spheres in the composite, and each sphere has the same c1 ⫽ (a/b)3, the effective bulk modulus of the entire composite should also be given by that of each individual composite sphere. Unlike the effective bulk modulus, the effective shear modulus is rather difﬁcult to estimate for the composite sphere model. This is due to the fact that a composite sphere subjected to shear deformation does not behave as a homogeneous sphere. Hence, the substitution scheme is not valid. The composite sphere model was extended by Hashin and Rosen (1964) to the case of inﬁnitely long cylinders imbedded in an isotropic matrix. Later, Hill (1964) and Hashin (1966) used the composite-sphere model to determine the effective modulus of ﬁber-reinforced composite

8.1

199

COMPOSITE-SPHERE MODEL

materials; see Figure 8.2. They were able to ﬁnd the exact solutions to four of the ﬁve elastic moduli (Christensen and Lo, 1979): Longitudinal Young’s modulus EL: EL ⫽ cƒEƒ ⫹ cmEm ⫹

4cƒcm(vƒ ⫺ vm)2 m , (8.1.8) 1 ⫹ 3cƒ m /(3Km ⫹ m) ⫹ 3cm m /(3Kƒ ⫹ ƒ)

Transverse bulk modulus KT: KT ⫽ Km ⫹ ⫹

m 3

cƒ , 3/(3Kƒ ⫹ ƒ ⫺ 3Km ⫺ m) ⫹ 3cƒ /(3Km ⫹ 4m) (8.1.9)

Longitudinal shear modulus L: L ⫽

(cƒƒ ⫹ cmm ⫹ ƒ)m , cmƒ ⫹ cƒm ⫹ m

(8.1.10)

Longitudinal Poisson’s ratio vLT: vLT ⫽ cƒvƒ ⫹ cmvm ⫹

3cƒcm(vƒ ⫺ vm)m[cƒ m /(3Km ⫹ m) ⫹ cmm /(3Kƒ ⫹ ƒ)] , 1 ⫹ 3cƒ m /(3Km ⫹ m) ⫹ 3cm m /(3Kƒ ⫹ƒ) (8.1.11)

Figure 8.2 Two-phase composite-cylinder model.

200

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

where Kƒ, ƒ, and Km, m are the bulk and shear moduli of the ﬁber and the matrix, respectively. The remaining modulus, the transverse shear modulus, cannot be obtained exactly using the two-phase composite-sphere model. It will be obtained in the next section using the three-phase model.

8.2 THREE-PHASE MODEL

The three-phase model or generalized self-consistent model (Christensen and Lo, 1979) is an extension of the composite-sphere model. As in the composite-sphere model, the three-phase model assumes that each particle of radius a is surrounded by a shell of matrix material with thickness b ⫺ a, so that the particle volume fraction is given by c1 ⫽ (a/b)3. Next, instead of using such composite spheres to ﬁll in the entire representative volume element of the composite as in the composite-sphere model, the three-phase model assumes that the composite sphere is imbedded in an effective medium whose properties are yet to be determined; see Figure 8.3. This is very similar to the selfconsistent method discussed in Sections 7.4 and 7.5; thus the name generalized self-consistent method. The reason it is called generalized is that in the three-phase model, each particle is in contact with or surrounded by the actual matrix material, while in the conventional self-consistent methods discussed in Sections 7.4 and 7.5, the particles are in indirect contact with the effective medium instead of the actual matrix.

Effective Medium

a b Matrix Particle

Figure 8.3 Three-phase model.

8.2

201

THREE-PHASE MODEL

It turns out that the effective bulk modulus of a three-phase composite sphere is also given by (8.1.1); see Problem 8.2. Following the similar argument used to arrive at (8.1.7), one can also show that the effective bulk modulus of the representative volume element of a composite coincides with the effective bulk modulus of the three-phase composite sphere, that is, K ⫽ Kr ⫽ K0 ⫹

c1(K1 ⫺ K0)(3K0 ⫹ 40) . 3K0 ⫹ 40 ⫹ 3(1 ⫺ c1)(K1 ⫺ K0)

(8.2.1)

Figure 8.4 shows the comparison of effective bulk modulus obtained experimentally, and predicted by the three-phase model and the selfconsistent model, for a polymer matrix with voids. The data are normalized by the matrix bulk modulus. The Poisson ratio of the matrix is 0.193. The experimental data are from Walsh et al. (1965). It is seen that the conventional self-consistent method underestimates the experimental results. As discussed in Section 7.7, the self-consistent method yields no physically admissible solution for void volume fraction above 0.5. The three-phase model, on the other hand, provides solutions for the entire range of void volume fraction and the results are in fairly good agreement with the experimental data, even when the volume fraction of voids is large. Unlike the effective bulk modulus, obtaining the effective shear modulus is rather complicated. It involves solving the shear deformation of

1.0 Experimental Data: Walsh et al. (1965) Christensen and Lo (1979)

0.8

Self-Consistent Scheme 0.6

K K0

0.4 0.2 0.0 0.0

0.2

0.6 0.4 Volume Fraction

0.8

1.0

Figure 8.4 Normalized effective bulk modulus (void / glass) with vM ⫽ 0.193.

202

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

a three-phase composite sphere. Detailed description of the solution procedure is given in Appendix 8.A. The solution can be written formally as ⫺B Ⳳ 兹B2 ⫺ AC ⫽ , 0 A

(8.2.2)

where the constants A, B, and C are given in Appendix 8.A. Presented in Figure 8.5 are the effective modulus estimated by the three-phase model and the Hashin–Shtrikman bounds (Hashin and Shtrikman, 1963, Hashin, 1966; Walpole, 1966). The material parameters used in this comparison are 1 / 0 ⫽ 135.14, v1 ⫽ 0.20, and v0 ⫽ 0.35. It is seen from Figure 8.5 that the effective shear modulus from the three-phase model is bounded by the Hashin–Shtrikman lower and upper bounds. The three-phase model has also been applied to ﬁber-reinforced composite materials (Christensen and Lo, 1979) for obtaining the effective transverse shear modulus. Again, the solution procedure is rather complicated. The solution can be written formally as ⫺B Ⳳ 兹B2 ⫺ AC T ⫽ , m A

(8.2.3)

where the constants A, B, and C are given in Appendix 8.B. 21

Upper Bound: Hashin (1962) Christensen and Lo (1979)

µ µ0

Lower Bound: Hashin–Strikman (1963) and Walpole (1966)

16

11

6.0

0.0 0.0

0.2

0.6 0.4 Volume Fraction

0.8

1.0

Figure 8.5 Normalized effective shear modulus for spherical model with 1 / 0 ⫽ 135.14, v1 ⫽ 0.20, and v0 ⫽ 0.35 (boron / epoxy composite).

8.3

FOUR-PHASE MODEL

203

8.3 FOUR-PHASE MODEL

The four-phase model was developed in order to take into account more complex heterogeneities found in advanced composite materials. In the four-phase model, an interphase is introduced between the inhomogeneity and the surrounding matrix. This enables the modeling of composites with coated ﬁbers or particles. This model is very commonly used in civil engineering applications (e.g., Li et al., 1999; Hashin and Monteiro 2003; Heukamp et al., 2004). Bardella et al. (2002) have also used the four-phase model to estimate the effective behavior of synthetic foam, which are materials composed of a polymer matrix reinforced with hollow glass inclusions and isolated porosities. The four-phase model can be applied in different ways. Some treat the four phases in a single formulation, while others split them into a threephase model and a composite-sphere model. This later approach was taken by Li et al. (1999) to evaluate the effective elastic properties of an isotropic elastic medium. Their model was divided into two parts; one part corresponds to the three-phase model of Christensen and Lo (1979); the other part corresponds to the two-phase composite-sphere model of Hashin (1962); see Figure 8.6. Note that the problem shown in Figure 8.6(b) is equivalent to the three-phase model. Therefore, the corresponding effective bulk modulus is given by (8.2.1): K ⫽ K0 ⫹

(Ke ⫺ K0)(3K0 ⫹ 40)(b3 /c3) , 3K0 ⫹ 40 ⫹ 3(Ke ⫺ K0)(1 ⫺ b3 /c3)

Effective Medium

Particle Coating Matrix (a)

(8.3.1)

Effective Medium

Homogenized Particle and Coating (b)

Matrix

Particle

Coating (c)

Figure 8.6 Decomposition of four-phase model: (a) four, (b) three, and (c) two phases.

204

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

where K0 and 0 are, respectively, the bulk and shear moduli of the matrix, and Ke is the effective bulk modulus of the coated inhomogeneity, which can be obtained by solving the problem depicted in Figure 8.6(a): Ke ⫽ Kc ⫹

(K1 ⫺ Kc)(3Kc ⫹ 4c)(a3 /b3) , 3Kc ⫹ 4c ⫹ 3(K1 ⫺ Kc)(1 ⫺ a3 /b3)

(8.3.2)

where Kc and c are the bulk and shear moduli of the coating layer, respectively, and K1 is the bulk modulus of the inhomogeneity. Substitution of (8.3.2) into (8.3.1) yields the effective bulk modulus of the representative volume element of the composite. It is interesting to note that the effective bulk modulus depends not only on the elastic properties of the inhomogeneity and the matrix but also on the dimensions of the inhomogeneity and its coating material.

8.4 MULTICOATED INCLUSION PROBLEM

The ideas of the two-phase and three-phase models can be extended to develop the multiphase model. In the multiphase model, it is assumed that a spherical inhomogeneity comprised of isotropic material is coated with N layers of different isotropic materials. The interfaces between the inhomogeneity and the coating and between the coatings are all assumed perfect. To obtain the effective bulk modulus, we subject the multicoated composite to pure dilatational deformation. It follows from the derivation in the previous sections that the effective modulus can be written as Herve and Zaoui (1993):

Rn

K1

K2

Kn

R1 R2

Figure 8.7 Multicoated inclusion schematic.

8.4

Kn ⫽ Kn ⫹

MULTICOATED INCLUSION PROBLEM

(R3n⫺1 /R3n)(Kn⫺1 ⫺ Kn)(3Kn ⫹ 4n) , 3Kn ⫹ 4n ⫹ 3(1 ⫺ R3n⫺1 /R3n)(Kn⫺1 ⫺ Kn)

205

n ⱖ 2, (8.4.1)

where Rn and Rn⫺1 are, respectively, the radii of phase n and (n ⫺ 1), Kn and n are, respectively, the bulk and shear moduli of phase n, and Kn⫺1 is the effective bulk modulus of the (n ⫺ 1)-coated inclusion. If we deﬁne K1 ⫽ K1 and KN ⫽ K, (8.4.1) provides a recursive relationship to compute the effective bulk modulus. For n ⫽ 2, the effective bulk modulus reduces to that of the twophase composite sphere model: K ⫽ K2 ⫹

c2(K1 ⫺ K2)(3K2 ⫹ 42) , 3K2 ⫹ 42 ⫹ 3(1 ⫺ c2)(K1 ⫺ K2)

(8.4.2)

where c ⫽ R31 / R32 gives the volume fraction of the inhomogeneity, and the subscripts 1 and 2 refer to the inhomogeneity and the coating, respectively. For n ⫽ 3, the effective bulk modulus can be expressed as K ⫽ K3 ⫹

(R32 /R33)(K2 ⫺ K3)(3K3 ⫹ 43) , 3K3 ⫹ 43 ⫹ 3(1 ⫺ R32 /R33)(K2 ⫺ K3)

(8.4.3)

K2 ⫽ K2 ⫹

(R31 /R32)(K1 ⫺ K2)(3K2 ⫹ 42) . 3K2 ⫹ 42 ⫹ 3(1 ⫺ R31 /R32)(K1 ⫺ K2)

(8.4.4)

where

Shown in Figure 8.8 are the prediction of the effective bulk modulus by the multicoated inclusion method. The data are normalized by the matrix’s bulk modulus, K3. The parameter  ⫽ K2 /K3 is the ratio of the bulk moduli of the coating and the matrix. The Poisson ratios of the particle, matrix, and coating are all set to be 0.3 (v1 ⫽ v2 ⫽ v3 ⫽ 0.3). The ratio of the bulk modulus of particle and of matrix is set to 6 (K1 /K3 ⫽ 6), and the volume fraction of the particle with coating is c1 ⫹ c2 ⫽ 0.2. It is seen that when  ⬎ 1 the interface is more rigid than the matrix. The case  ⫽ 6 corresponds to a simply coated inclusion (Christensen and Lo, 1979). The same remark stands for all values of  when the volume fraction of coating is in the neighborhood 0.2.

206

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

1.0

β = 1000

K K3

β = 10

β = 100

0.8

β =6

0.6

β =1

0.4

β = 0.1 β = 0.01

0.2 0.0 0.0

0.05

0.1

0.15

0.2

Volume Fraction of Coating

Figure 8.8 Normalized effective bulk modulus K / KN⫺1 (Herve´ and Zaoui, 1993) of a composite material, made of coated particle (phase 2), for different values  ⫽ 1 / M (1 denotes the inclusion) with v1 ⫽ v2 ⫽ v3 ⫽ 0.3, 1 / M ⫽ 6, c1 ⫹ c2 ⫽ 0.2.

The effective shear modulus predicted by the multiphase model is given by ⫺B Ⳳ 兹B2 ⫺ 4AC ⫽ , N 2A

(8.4.5)

where the constants A, B, and C are given in Appendix 8.C. PROBLEMS

8.1 Consider a composite-sphere consists of a core of radius a and a shell of thickness b ⫺ a surrounding the core; see Figure 8.9. Let both the core and shell be made of isotropic elastic material with

b a K1, µ1 K0, µ0

Figure 8.9

207

APPENDIX 8.A

moduli K0, 0 and K1, 1, respectively. Please ﬁnd the effective bulk modulus of the composite sphere. 8.2 Consider a three-phase concentric sphere as shown in Figure 8.10. Please ﬁnd the effective bulk modulus of the composite sphere.

APPENDIX 8.A

To derive (8.2.2), the elasticity problem depicted in Figure 8.3 needs to be solved under simple shear deformation. This can be carried out by writing the displacement ﬁelds in a spherical coordinate system in each of the three regions: the inhomogeneity (r ⱕ a), the matrix (a ⱕ r ⱕ b), and the effective medium (b ⱕ r). The following equation can then be derived after making use of the equilibrium equations and the continuity conditions at the interfaces between the different regions:

冉冊

A 0

2

冉冊

⫹ 2B

⫹ C ⫽ 0, 0

(8.A.1)

where

冉

A⫽8

冊

冋冉 冊 冉 冊

册

1 ⫺ 1 (4 ⫺ 5v0)1c10 / 3 ⫺ 2 63 1 ⫺ 1 2 ⫹ 213 c7 / 3 0 0

⫹ 252

冉

冊

1 ⫺ 1 2c5 / 3 ⫺ 50 1 ⫺ 1 (7 ⫺ 12v0 ⫹ 8v02)2c 0 0

⫹ 4(7 ⫺ 10v0)23,

b a K1, µ0 K0, µ0

K, µ

Figure 8.10

208

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

冉 冊 冋冉 冊 冉 冊 冉 冊 冉 冊

B ⫽ ⫺2

1 ⫺ 1 (4 ⫺ 5v0)1c10 / 3 0

⫹ 2 63 ⫹ 75

C⫽4

册

冉

冊

1 ⫺ 1 2 ⫹ 213 c7 / 3 ⫺ 252 1 ⫺ 1 2c5 / 3 0 0

1 ⫺ 1 (3 ⫺ v0)v02c ⫹ 3(15v0 ⫺ 7)23, 0

冋冉 冊 冉 冊

册

1 ⫺ 1 (5v0 ⫺ 7)1c10 / 3 ⫺ 2 63 1 ⫺ 1 2 ⫹ 213 c7 / 3 0 0

⫹ 252

1 ⫺ 1 2c5 / 3 ⫹ 25 1 ⫺ 1 (v02 ⫺ 7)2c 0 0

⫺ (7 ⫹ 5v0)23,

with 1 ⫽

冉

冊

冉冊 冊 冉

1 ⫺ 1 (49 ⫺ 50v1v0) ⫹ 35 1 (v1 ⫺ 2v0) ⫹ 35(2v1 ⫺ v0), 0 0

冉 冉冊

2 ⫽ 5v1

3 ⫽

冊

1 ⫺8 ⫹7 1⫹4 , 0 0

1 (8 ⫺ 10v0) ⫹ (7 ⫺ 5v0), 0

where c is the volume fraction of the particles, that is, c ⫽ (a/b)3.

APPENDIX 8.B

Detailed derivation of the three-phase composite cylinder model can be found in Christensen and Lo (1979). The results are list below for the effective transverse shear modulus.

APPENDIX 8.B

冉冊

冉冊

2

A T m

⫹ 2B

T ⫹ C ⫽ 0, m

209

(8.B.1)

where A ⫽ 3c(1 ⫺ c)2 ⫹ ⫻

冋 冋 冉 冉

冋

冊冉 冊 冉 冊册 冊 冉 冊册 冊冉 冊 冉 冊册 冊 冉 冊册 冊冋 冉 冊册

ƒ ⫺1 m

ƒ ⫹ ƒ m

ƒ ƒ m ⫹ ƒm ⫺ ⫺ ƒ c3 m m m

cm

ƒ ƒ ⫺1 ⫺ ⫹1 m m m

ƒ ⫺1 m

B ⫽ ⫺3c(1 ⫺ c)2 ⫹

冉

,

(8.B.2)

ƒ ⫹ ƒ m

ƒ 1 ƒ m ⫹ 1 ⫹ ⫺1 c 2 m m

⫻

冋

冉 冉

⫹

ƒ c (m ⫺ 1) ⫺1 2 m

(m ⫺ 1)

ƒ ƒ ⫹ ƒ ⫺ 2 ⫺ ƒ c3 m m m

ƒ ƒ m ⫹ ƒ ⫹ ⫺ 1 c3 , m m

(8.B.3)

冉

C ⫽ 3c(1 ⫺ c)2 ⫹ ⫻

and

冋 冋

ƒ ⫺1 m

冉

冊冉

冊 冊册 冊册

ƒ ⫹ ƒ m

ƒ ƒ ⫹ ƒ ⫺ ⫺ ƒ c3 m m m

冉

ƒ ƒ m ⫹ 1 ⫹ ⫺1 c , m m

(8.B.4)

210

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

冉冊

3

a c⫽ , b

m ⫽ 3 ⫺ 4vm,

ƒ ⫽ 3 ⫺ 4vƒ.

(8.B.5)

APPENDIX 8.C

The constants in (8.4.5) are given by 7 2 A ⫽ 4R10 n (1 ⫺ 2vn)(7 ⫺ 10vn)Z12 ⫹ 20Rn(7 ⫺ 12vn ⫹ 8vn)Z42 ⫹ 12Rn5(1 ⫺ 2vn)(Z14 ⫺ 7Z23) ⫹ 20Rn3(1 ⫺ 2vn)2Z13 ⫹ 16(4 ⫺ 5vn)(1 ⫺ 2vn)Z43,

B ⫽ 4Rn10(1 ⫺ 2vn)(15vn ⫺ 7)Z12 ⫹ 60Rn7(vn ⫺ 3)vnZ42 ⫺ 24R5n(1 ⫺ 2vn)(Z14 ⫺ 7Z23) ⫺ 40R3n(1 ⫺ 2vn)2Z13 ⫺ 8(1 ⫺ 5vn)(1 ⫺ 2vn)Z43, 7 2 C ⫽ ⫺R10 n (1 ⫺ 2vn)(7 ⫹ 5vn)Z12 ⫹ 10Rn(7 ⫺ vn)Z42 ⫹ 12Rn5(1 ⫺ 2vn)(Z14 ⫺ 7Z23) ⫹ 20Rn3(1 ⫺ 2vn)2Z13 ⫺ 8(1 ⫺ 5vn)(1 ⫺ 2vn)Z43,

where Z␣ ⫽ P␣(n⫺1) P(n⫺1) ⫺ P(n⫺1) P(n⫺1) 1 2 1 ␣2 P(n) ⫽

with ␣ 僆 [1,4] and  僆 [1,4],

写M n

( j)

.

j⫽1

ck 3 M

(k)

⫽

0

1

R5k ␣k 2

5(1 ⫺ vk⫹1) ⫺5

6

(1 ⫺ 2vk⫹1)␣kRk3

Rk2(3bk ⫺ 7ck) 5(1 ⫺ 2vk) (1 ⫺ 2vk⫹1)bk 7(1 ⫺ 2vk) 7 ⫺Rk (2␣k ⫺ 147␣k) 70(1 ⫺ 2vk) 7(1 ⫺ 2vk⫹1)␣kRk5 2(1 ⫺ 2vk)

REFERENCES

⫺12␣k 5 k

R

⫺20(1 ⫺ 2vk⫹1)␣k

7R7k dk 7

211

4(ƒk ⫺ 27␣k) 15(1 ⫺ 2vk)Rk3 ⫺12␣k(1 ⫺ 2vk⫹1) 7(1 ⫺ 2v)R ... , 2 Rk (105(1 ⫺ vk⫹1) ⫹ 12␣k(7 ⫺ 10vk) ⫺ 7ek) 35(1 ⫺ 2vk) ek(1 ⫺ 2vk) 3(1 ⫺ 2vk)

with ␣k ⫽

冉 冊

k (7 ⫹ 5vk)(7 ⫺ 10vk⫹1) ⫺ (7 ⫺ 10vk)(7 ⫹ 5vk⫹1), k⫹1

冉 冉 冉 冉 冉

冊 冊 冊 冊 冊

bk ⫽ 4(7 ⫺ 10vk) ⫹

k (7 ⫹ 5vk), k⫹1

ck ⫽ (7 ⫺ 5vk⫹1) ⫹ 2

k (4 ⫺ 5vk⫹1), k⫹1

dk ⫽ (7 ⫹ 5vk⫹1) ⫹ 4

k (7 ⫺ 10vk⫹1), k⫹1

ek ⫽ 2(4 ⫺ 5vk) ⫹ ƒk ⫽ (4 ⫺ 5vk)(7 ⫺ 5vk⫹1) ⫺ ␣k ⫽

k (7 ⫺ 5vk), k⫹1

k (4 ⫺ 5vk⫹1)(7 ⫺ 5vk), k⫹1

k ⫺ 1. k⫹1

REFERENCES Christensen, R. M. and K. H. Lo. (1979). Solutions for Effective Shear Properties in Three Phase Sphere and Cylinder Models, J. Mech. Phys. Solids, Vol. 27, pp. 315–330.

212

DETERMINATION OF EFFECTIVE MODULI—MULTIINCLUSION APPROACHES

Hashin, Z. (1962). The Elastic Moduli of Heterogeneous Materials, J. Appl. Mech., Vol. 29, pp. 143–150. Hashin, Z. (1966). Viscoelastic Fiber Reinforced Materials, AIAA J., Vol. 4, pp. 1411–1417. Hashin, Z. and B. W. Rosen. (1964). The Elastic Moduli of ReinforcedReinforced Materials, J. Appl. Mech., Vol. 31, pp. 223–228. Hashin, Z. and S. Shtrikman. (1963). A Variational Approach to the Theory of the Elastic Behavior of Multiphase Materials, J. Mech. Phys. Solids, Vol. 11, pp. 127–140. Herve´, E. and A. Zaoui. (1993). N-Layered Inclusion-Based Micromechanical Modeling, Int. J. Eng. Sci., Vol. 31, pp. 1–10. Hill, R. (1964). Theory of Mechanical Properties of Fibre-Strengthened Materials—I: Elastic Behavior,’’ J. Mech. Phys. Solids, Vol. 12, pp. 199–212. Li, G., Y. Zhao, and S. S. Pang. (1999). Four-Phase Sphere Modeling of Effective Bulk Modulus of Concrete, Cement and Concrete Research, Vol. 29, pp. 839–845. Walpole, L. J. (1966). On the Bounds for Overall Elastic Moduli of Inhomogeneous Systems—I, J. Mech. Phys. Solids, Vol. 14, pp. 151–162. Walpole, L. J. (1969). On the Overall Elastic Moduli of Composite Materials, J. Mech. Phys. Solids, Vol. 17, pp. 235–251. Walsh, J. B., W. F. Brace, and A. W. England. (1965). The Effect of Porosity on Compressibility of Glass, J. Am. Ceram. Soc., Vol. 48, pp. 605–608.

SUGGESTED READINGS Bardella, L. and F. Genna. (2001). On the Elastic Behavior of Syntactic Foams, Int. J. Solids Structures, Vol. 38, pp. 7235–7260. Benveniste, Y. (1987). A New Approach to the Application of Mori–Tanaka’s Theory in Composite Materials, Mech. Mater., Vol. 6, pp. 147–157. Benveniste, Y., G. J. Dvorak, and T. Chen. (1989). Stress Field in Composite with Coated Inclusions, Mech. Mater., Vol. 7, pp. 305–317. Budiansky, B. and T. Wu. (1962). Theoretical Prediction of Plastic Strains in Polycrystals, In Proc. 4th U.S. Nat. Cong. Theo. Appl. Mech., pp. 1175– 1183. Cherkaoui, M., H. Sabar, and M. Berveiller. (1994). Micromechanical Approach of the Coated Inclusion Problem and Applications to Composite Materials, J. Eng. Mater. Tech., Vol. 116, pp. 274–278. Cherkaoui, M., H. Sabar, and M. Berveiller. (1995). Elastic Composites with Coated Reinforcements: A Micromechanical Approach for Nonhomothetic Topology, Int. J. Eng. Sci., Vol. 33, pp. 829–843. Christensen, R. M. (1991). Mechanics of Composite Materials, Krieger, Malabar, FL.

SUGGESTED READINGS

213

El Mouden, M., M. Cherkaoui, A. Molinari, and M. Berveiller. (1998). The Overall Elastic Response of Materials Containing Coated Inclusions in a Periodic Array, Int. J. Engng. Sci., Vol. 36, pp. 813–829. Hashin, Z. and P. J. M. Monteiro. (2003). An Inverse Method to Determine the Elastic Properties of the Interphase between the Aggregate and the Cement Paste, Cem. Conc. Res., Vol. 32, pp. 1291–1300. Heukamp, F. H., E. Lemarchand, and F. J. Ulm. (2005). The Effect of Interfacial Properties on the Cohesion of Highly Filled Composite Materials, Int. J, Solids Structures, Vol. 42, 287–305. Hill, R. (1963). Elastic Properties of Reinforced Solids: Some Theoretical Principles, J. Mech. Phys. of Solids, Vol. 11, pp. 357–372. Hill, R. (1995). A Self-Consistent Mechanics of Composite Materials, J. Mech. Phys. Solids, Vol. 13, pp. 213–222. Hori, M. and S. Nemat-Nasser. (1993). Double-Inclusion Model and Overall Moduli of Multi-Phase Composites, Mech. Mater., Vol. 14, pp. 189–206. Jasiuk, I. and M. W. Kouider. (1993). The Effect of an Inhomogeneous Interphase on the Elastic Constants of Transversely Isotropic Composites, Mech. Mater., Vol. 15, pp. 53–63. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston. Nemat-Nasser, S. and M. Hori. (1993). Micromechanics: Overall Properties of Heterogeneous Materials, North-Holland, New York. Norris, A. N. (1985). A Differential Scheme for the Effective Modulus of Composites, Mech. Mater., Vol. 4, pp. 1–16. Qiu, Y. P. and G. J. Weng. (1991). Elastic Moduli of Thickly Coated Particle and Fiber-Reinforced Composites, J. Appl. Mech., Vol. 58, pp. 388–398.

9 EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES A ﬁber-reinforced composite laminate is a special kind of heterogeneous material. It typically consists of multiple layers of plies, each ply is thin sheet of matrix material reinforced by unidirectional ﬁbers. Glass ﬁber- and graphite ﬁber-reinforced epoxy matrix composites are the most commonly used composite laminates. In this chapter, we will apply some of the theories developed in previous chapters to determine the effective properties for ﬁber-reinforced composite laminates.

9.1 UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

Consider a matrix material reinforced by circular cross-section ﬁbers all aligned in the x1 direction, as schematically shown in Figure 9.1. Let the volume fraction of the ﬁber be cƒ and volume fraction of the matrix be cm. Obviously, we have cm ⫹ cƒ ⫽ 1.

(9.1.1)

We further assume that both the ﬁber and the matrix are isotropic, and their elastic properties are deﬁned by the Young’s modulus Eƒ, Em and Poisson’s ratio ƒ, m, respectively. Because of the cylindrical nature of the composite, the effective elastic properties are transversely isotropic. In the Voigt notation, this can be written as 214

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

215

x3 x2

x1

Figure 9.1 Unidirectional ﬁber-reinforced composite.

冤冥冤 11 22 33 23 13 12

⫽

C11

C12

C12

0

0

0

C12

C22

C23

0

0

0

C12

C23

C22

0

0

0

0

0

0

0

0

0

0

0

0

C22 ⫺ C23 0 2 0 C66 0

0

0 0 C66

冥冤 冥 11 22 33 223 213 212

(9.1.2)

where Cij are the effective Voigt elastic constants of the unidirectional ﬁber-reinforced composite. For convenience and without causing any confusion, we have omitted the overbar for the effective Voigt elastic constants, which are related to the effective elasticity tensor Lijkl through the relationship described by Table 2.1. Equation (9.1.2) is written in a coordinate system where the x1 axis is in the direction of the ﬁbers. In the coordinate system xˆ i shown in Figure 9.2, where the xˆ 1 axis forms an angle from the ﬁber direction, the expressions for the components Cˆ ij of the Voigt elastic matrix are different. They are related to Cij through a coordinate rotation; see (2.4.13): x1 xˆ2

xˆ1 θ

x1

Figure 9.2 Fibers not aligned with coordinate axis.

216

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

Cˆ 11 ⫽ Q11m4 ⫹ 2(C12 ⫹ 2C66)m2n2 ⫹ C22n4, Cˆ 22 ⫽ C11n4 ⫹ 2(C12 ⫹ 2C66)m2n2 ⫹ C22m4, Cˆ 33 ⫽ C33, Cˆ 12 ⫽ (C11 ⫹ C22 ⫺ 4C66)m2n2 ⫹ C12(m4 ⫹ n4), Cˆ 13 ⫽ C13m3 ⫹ C23n2, Cˆ 23 ⫽ C13n3 ⫹ C23m2, Cˆ 36 ⫽ (C23 ⫺ C13)mn,

(9.1.3)

Cˆ 44 ⫽ C44m3 ⫹ C55n2, Cˆ 55 ⫽ C55m3 ⫹ C44n2, Cˆ 66 ⫽ (C11 ⫹ C22 ⫺ 2C12)m2n2 ⫹ 2C22mn(m2 ⫺ n2) ⫹ C66(m2 ⫺ n2)2, Cˆ 45 ⫽ (C44 ⫺ C55)mn, Cˆ 16 ⫽ (C22 ⫺ C12 ⫺ 2C66)mn3 ⫺ (C11 ⫺ C12 ⫺ 2C66)m3n, Cˆ 26 ⫽ (C22 ⫺ C12 ⫺ 2C66)m3n ⫺ (C11 ⫺ C12 ⫺ 2C66)mn3, in which m ⫽ cos , n ⫽ sin . Therefore, in a coordinate system not aligned with the ﬁber, the Voigt elasticity matrix has the following form:

冤

Cˆ 11 Cˆ 12 ˆ ˆ ⫽ C13 C 0 0 ˆ C16

Cˆ 12 Cˆ 22 Cˆ 23 0 0 ˆ C26

Cˆ 13 Cˆ 23 Cˆ 33 0 0 ˆ C36

0 0 0 Cˆ 44 Cˆ 45 0

0 0 0 Cˆ 45 Cˆ 55 0

冥

Cˆ 16 Cˆ 26 Cˆ 36 . 0 0 ˆ C66

(9.1.4)

Now, let us go back to (9.1.2). Taking the inverse of the elasticity tensor yields

冤冥冤 11 22 33 223 213 212

S11 S12 S12 ⫽ 0 0 0

S12 S22 S23 0 0 0

S12 S23 S22 0 0 0

0 0 0 0 0 0 0 0 0 S44 0 0 0 S66 0 0 0 S66

冥冤 冥

11 22 33 , 23 13 12

(9.1.5)

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

217

where S11 ⫽

⫺2C

C22 ⫹ C23 , ⫹ C11(C22 ⫹ C23)

(9.1.6)

C12 , 2C 212 ⫺ C11(C22 ⫹ C23)

(9.1.7)

2 C 12 ⫺ C11C22 , 2 (C22 ⫺ C23)[2C 12 ⫺ C11(C22 ⫹ C23)]

(9.1.8)

C 212 ⫺ C11C23 , 2 (C22 ⫺ C23)[⫺2C 12 ⫹ C11(C22 ⫹ C23)]

(9.1.9)

S12 ⫽

S22 ⫽

S23 ⫽

2 12

S44 ⫽ 2(S22 ⫺ S23) ⫽

2 C22 ⫺ C23

,

S66 ⫽

1 C66

(9.1.10)

are the ﬁve elastic compliance constants. They can be related to the engineering constants easily as follows. Under a uniaxial loading in the x1 direction, we have 11 ⫽ S1111,

22 ⫽ 33 ⫽ S1211.

(9.1.11)

The ﬁrst of (9.1.11) deﬁnes the longitudinal Young modulus in the ﬁber direction: EL ⫽

11 1 2C 212 ⫽ ⫽ C11 ⫺ . 11 S11 C22 ⫹ C23

(9.1.12)

The contraction in the transverse direction that accompanies the uniaxial stress in the ﬁber direction deﬁnes the corresponding Poisson ratio through S C12 LT ⫽ ⫺ 22 ⫽ ⫺ 33 ⫽ ⫺ 12 ⫽ . 11 11 S11 C22 ⫹ C23

(9.1.13)

Similarly, when the uniaxial stress is in the x2 direction (transverse to the ﬁber), we have

218

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

11 ⫽ S1222,

22 ⫽ S2222,

33 ⫽ S2322.

(9.1.14)

The second of (9.1.14) deﬁnes the Young modulus in the transverse direction: ET ⫽

2 22 1 C 2 (C ⫺ 2C23) ⫹ C11C 23 ⫽ ⫽ C22 ⫺ 12 22 . 22 S22 C11C22 ⫺ C 212

(9.1.15)

In this case, the contraction in the ﬁber direction that accompanies the uniaxial stress in the transverse direction deﬁnes the corresponding Poisson ratio through S C (C ⫺ C23) TL ⫽ ⫺ 11 ⫽ ⫺ 12 ⫽ 12 22 . 2 22 S22 C11C22 ⫺ C 12

(9.1.16)

Analogously, the contraction in the other transverse direction that accompanies the uniaxial stress in one transverse direction deﬁnes another Poisson ratio, S C C ⫺ C 212 TT ⫽ ⫺ 33 ⫽ ⫺ 23 ⫽ 11 23 . 22 S22 C11C22 ⫺ C 212

(9.1.17)

As a convention in labeling the Poisson ratios in this text, the ﬁrst subscript indicates the direction of the uniaxial stress, and the second subscript indicates the direction normal to the loading direction in which the contraction takes place. It is clear from the above or simply from the material asymmetry that TL ⫽ LT. However, it can be easily veriﬁed by direction substitution of their deﬁnitions that LT TL ⫽ . EL ET

(9.1.18)

If a simple shear 12 ⫽ 21 is applied, we will have 212 ⫽ S6612. Thus the longitudinal shear modulus is deﬁned as L ⫽

12 1 ⫽ ⫽ C66. 212 S66

(9.1.19)

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

219

Similarly, when the material is subjected to the simple shear 23, the corresponding shear strain is 223 ⫽ S4423. Thus, the corresponding shear modulus is deﬁned by T ⫽

23 1 1 ⫽ ⫽ (C22 ⫺ C23). 223 S44 2

(9.1.20)

It is clear from the above deﬁnitions that L is the shear modulus when the ﬁbers are shifted relative to each other in the longitudinal direction, while T is the shear modulus when the ﬁbers are shifted relative to each other in the transverse directions. Finally, a plane strain bulk modulus can be introduced by applying biaxial stresses 22 ⫽ 33 ⫽ . Since the elastic properties are isotropic in the x2x3 plane, the corresponding strain ﬁeld is given by 22 ⫽ 33 ⫽ . We thus have ⫽ 2KT ,

(9.1.21)

where KT is the plane strain bulk modulus within the isotropic plane given by KT ⫽ –21 (C22 ⫹ C23).

(9.1.22)

So far, we have introduced two Young moduli, two shear moduli, one bulk modulus, and three Poisson ratios. Not all the eight engineering constants are independent. Since they are deﬁned based on the ﬁve stiffness constants Cij as shown in (9.1.2), it can be easily concluded that there are only ﬁve independent engineering constants. In addition to (9.1.18), the following relationships among these engineering constants can also be veriﬁed by direct substitution: ET ⫽

4TKT , 2 KT ⫹ T ⫹ 4 LT TKT /EL

(9.1.23)

TT ⫽

KT ⫺ T ⫺ 4 2LTTKT /EL , 2 KT ⫹ T ⫹ 4 LT TKT /EL

(9.1.24)

冉

2LT ⫽ ⫺TT ⫺

冊

1 ET 1 ET EL ⫹ . 4 KT 4 T ET

(9.1.25)

220

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

Making use of the deﬁnitions of the engineering elastic constants, the Voigt elasticity matrix for transversely isotropic solids with the x1 direction being the axis of symmetry can be rewritten as

冤

冥

2 EL ⫹ 4 LT KT 2LTKT 2LTKT 0 0 0 2LTKT KT ⫹ T KT ⫺ T 0 0 0 2LTKT KT ⫹ T KT ⫹ T 0 0 0 C⫽ . T 0 0 0 0 0 0 0 0 0 L 0 0 0 0 0 0 L

(9.1.26)

It is interesting to investigate the bounds on the various Poisson ratios. For example, If a material has a very large transverse shear modulus, that is, T → ⬁, then it follows from (9.1.24) that TT → ⫺1. On the other hand, if a material has very large plane strain bulk modulus and very large longitudinal Young’s modulus, that is, KT → ⬁ and EL → ⬁, then it follows from (9.1.24) that TT → 1. Therefore, we can conclude that ⫺1 ⬍ TT ⬍ 1.

(9.1.27)

Next, consider (9.1.23). Solving for 2LT gives 2LT ⫽

冉

冊

EL EL 1 2 ⫺ ⫹ . ET 4 KT T

(9.1.28)

Since the second term on the right-hand side of (9.1.28) is positive, we arrive at 兩LT兩 ⱕ

冪EE .

(9.1.29)

冪EE .

(9.1.30)

L T

Making use of (9.1.18) also yields 兩TL兩 ⱕ

T L

Let us now consider how the effective properties Cij are related to the elastic properties of the ﬁber and the matrix. Several methods can be used for this purpose. We ﬁrst consider a very simple approach.

9.1

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

221

Recall that in Chapter 6, we discussed the Reuss lower and Voigt upper bounds for the effective modulus of heterogeneous materials. In what follows, we will apply these bounds to unidirectional ﬁberreinforced composite materials. Assume that both the ﬁbers and the matrix are isotropic and linearly elastic materials. It then follows from (6.2.10) that the Voigt upper bound of the elasticity tensor is given by LV ⫽ cmLm ⫹ cƒLƒ,

(9.1.31)

where Lƒ and Lm are the elasticity tensors of the ﬁber and the matrix, respectively. In terms of the Voigt notation, (9.1.31) implies that the nonzero components of the elasticity tensor can be written as C V11 ⫽ C V22 ⫽ C V33 ⫽

cƒEƒ(1 ⫺ ƒ) cmEm(1 ⫺ m) ⫹ , (1 ⫹ ƒ)(1 ⫺ 2ƒ) (1 ⫹ m)(1 ⫺ 2m) (9.1.32)

V V V V V V C 12 ⫽ C 21 ⫽ C 13 ⫽ C 31 ⫽ C 23 ⫽ C 32 ⫽

⫹

cƒEƒƒ (1 ⫹ ƒ)(1 ⫺ 2ƒ)

cmEmm , (1 ⫹ m)(1 ⫺ 2m) C V44 ⫽ C V55 ⫽ C V66 ⫽

(9.1.33) cƒEƒ cmEm ⫹ , 2(1 ⫹ ƒ) 2(1 ⫹m)

(9.1.34)

where Eƒ, ƒ and Em, m are the Young moldulus and the Poisson ratio of the ﬁber and matrix, respectively. The corresponding upper bound for the effective Young’s modulus is thus given by 2C V12C V12 ⫽ cƒEƒ ⫹ cmEm V V C 22 ⫹ C 12 2cƒcmEƒEm(ƒ ⫺ m)2 ⫹ . cƒEƒ(1 ⫹ m)(1 ⫺ 2m) ⫹ cmEm(1 ⫹ ƒ)(1 ⫺ 2ƒ)

E V ⫽ C V11 ⫺

(9.1.35) The corresponding upper bound for the effective Poisson’s ratio is

222

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

V ⫽ ⫽

V V C V12(C 11 ⫺ C 12 ) V V V V C 11C 11 ⫺ C 12C 12

cƒƒEƒ(1 ⫹ m)(1 ⫺ 2m) ⫹ cmmEm(1 ⫹ ƒ)(1 ⫺ 2ƒ) . cƒEƒ(1 ⫹ m)(1 ⫺ 2m) ⫹ cmEm(1 ⫹ ƒ)(1 ⫺ 2ƒ)

(9.1.36)

If the Poisson ratios of the ﬁber and the matrix are the same, that is, ƒ ⫽ m ⫽ , we have E V ⫽ cƒEƒ ⫹ cmEm,

V ⫽ .

(9.1.37)

On the other hand, the Reuss lower bound (6.2.13) gives L R ⫽ [cƒMƒ ⫹ cmMm]⫺1.

(9.1.38)

In terms the Voigt notation, this means R R C 11 ⫽ C R22 ⫽ C 33 ⫽

EƒEm[(cƒEm(1 ⫺ ƒ) ⫹ cmEƒ(1 ⫺ m)] , D

R R R R C R12 ⫽ C R21 ⫽ C 13 ⫽ C 31 ⫽ C 23 ⫽ C 32 ⫽

(9.1.39)

EƒEm[(cƒEmƒ ⫹ cmEƒm) , D (9.1.40)

C R44 ⫽ C R55 ⫽ C R66 ⫽

EƒEm[(cƒEm(1 ⫺ 2ƒ) ⫹ cmEƒ(1 ⫺ 2m)] , (9.1.41) 2D

where D ⫽ [(cƒEm(1 ⫺ ƒ) ⫹ cmEƒ(1 ⫹ m)] ⫻ [(cƒEm(1 ⫺ 2ƒ) ⫹ cmEƒ(1 ⫺ 2m)].

(9.1.42)

Following the procedures similar to (9.1.35) and (9.1.36), we obtain the lower bounds for the effective Young modulus and the effective Poisson ratio corresponding to (9.1.38),

9.1

ER ⫽

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

EƒEm , cƒEm ⫹ cmEƒ

R ⫽

cƒƒEm ⫹ cmmEƒ . cmEƒ ⫹ cƒEm

223

(9.1.43)

Again, if the Poisson ratios of the ﬁber and the matrix are the same, that is, ƒ ⫽ m ⫽ , we have ER ⫽

EƒEm , cƒEm ⫹ cmEƒ

R ⫽ .

(9.1.44)

It can be shown (see Problem 9.1) that the Voigt upper bound gives a better approximation in the ﬁber direction, while the Reuss lower bound gives a better approximation in the direction perpendicular (transverse) to the ﬁber. Therefore, by neglecting the difference in Poisson’s ratio, one may take the Young modulus in the ﬁber direction to be EL ⫽ E V ⫽ cƒEƒ ⫹ cmEm,

(9.1.45)

and the Young modulus in the transverse direction to be ET ⫽

EƒEm . cƒEm ⫹ cmEƒ

(9.1.46)

Equations (9.1.45) and (9.1.46) are the well-known rule of mixture formulas used commonly in engineering practice. Based on the derivations above, it is clear that these are actually the upper and lower bounds when the Poisson ratios are the same for the matrix and the ﬁbers. More accurate estimate of the unidirectional ﬁber-reinforced composite can be obtained by using the techniques developed in Chapters 7 and 8. To this end, we ﬁrst evaluate the Eshelby tensor for an inﬁnitely long cylindrical inclusion of circular cross section. It follows from Appendix 4.B that in the limit of a2 ⫽ a3 ⫽ a and a1 → ⬁, we obtain the nonzero components of the Eshelby tensor: S2222 ⫽ S3333 ⫽

5 ⫺ 4 , 8(1 ⫺ )

S2233 ⫽ S3322 ⫽

S2211 ⫽ S3311 ⫽

, 2(1 ⫺ )

4 ⫺ 1 , 8(1 ⫺ )

(9.1.47)

(9.1.48)

224

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

S2323 ⫽ S3223 ⫽ S2332 ⫽ S3232 ⫽

3 ⫺ 4 , 8(1 ⫺ )

(9.1.49)

S3131 ⫽ S1331 ⫽ S3113 ⫽ S1313 ⫽ S1212 ⫽ S2112 ⫽ S1221 ⫽ S2121 ⫽ –41 . (9.1.50) Making use of the Eshelby tensor in, for example, the Mori–Tanaka estimate (7.3.8), we have the effective elasticity tensor of the unidirectional ﬁber-reinforced composite given by L ⫽ (cmLm ⫹ cƒLƒTƒ)[cmI ⫹ cƒTƒ]⫺1,

(9.1.51)

Tƒ ⫽ [I ⫹ S(MmLƒ ⫺ I)]⫺1

(9.1.52)

where

is the strain concentration tensor (7.2.4). In conjunction with the deﬁnitions of the engineering constants, (9.1.51) leads to EL ⫽ [c ⫹ (1 ⫺ c)]Em ⫹

2c(1 ⫺ c)(ƒ ⫺ m)2Em , (1 ⫺ c)(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)[1 ⫹ c(1 ⫺ 2m)] (9.1.53)

KT ⫽

{(1 ⫺ c)(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)[1 ⫹ c(1 ⫺ 2m)]}Em , 2(1 ⫹m)[(1 ⫹ ƒ)(1 ⫺ 2ƒ)(c ⫹ 1 ⫺ 2m) ⫹ (1 ⫺ c)(1 ⫹ m)(1 ⫺ 2m)] (9.1.54)

T ⫽

[(1 ⫺ c)(1 ⫹ ƒ) ⫹ (1 ⫹ m)[c ⫹ (3 ⫺ 4m)]Em , 2(1 ⫹ m){(1 ⫺ c)(1 ⫹ m)(3 ⫺ 4m) ⫹ (1 ⫹ ƒ)[1 ⫹ c(3 ⫺ 4m)]} (9.1.55)

L ⫽

[(1 ⫹ c)(1 ⫹ m) ⫹ (1 ⫺ c)(1 ⫹ ƒ)]Em , 2(1 ⫹ m)[(1 ⫺ c)(1 ⫹ m) ⫹ (1 ⫹ c)(1 ⫹ ƒ)]

(9.1.56)

9.1

LT ⫽

UNIDIRECTIONAL FIBER-REINFORCED COMPOSITES

225

2c(1 ⫺ 2m)ƒ ⫹ (1 ⫺ c)[(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)]m , 2c(1 ⫺ m2 ) ⫹ (1 ⫺ c)[(1 ⫹ ƒ)(1 ⫺ 2ƒ) ⫹ (1 ⫹ m)] (9.1.57)

where c ⫽ cƒ is the ﬁber volume fraction, and ⫽

Eƒ . Em

The other engineering constants can be obtained through their relationships discussed earlier. For example, the transverse Young modulus ET can be obtained from (9.1.23) based on the above equations. Unfortunately, the expression for ET is extremely complex. We will not reproduce it here. By neglecting the difference in Poisson’s ratio between the ﬁber and the matrix, that is, m ⫽ ƒ ⫽ , we have EL ⫽ [c ⫹ (1 ⫺ c)]Em, KT ⫽

(9.1.58)

[1 ⫹ ⫺ 2 ⫺ c(1 ⫺ 2)(1 ⫺ )]Em , 2(1 ⫹ )(1 ⫺ 2)[1 ⫺ c( ⫺ 1) ⫹ ⫺ 2]

(9.1.59)

[1 ⫺ c(1 ⫺ ) ⫹ (3 ⫺ 4)]Em , 2(1 ⫹ )[1 ⫹ (3 ⫺ 4)(c ⫹ (1 ⫺ c))]

(9.1.60)

Em[(1 ⫺ c) ⫹ (1 ⫹ c)] , 2(1 ⫹ )[(1 ⫹ c) ⫹ (1 ⫺ c)]

(9.1.61)

T ⫽

L ⫽

LT ⫽ .

(9.1.62)

Even in this case, the expression for ET is still too long to be recorded here. However, the following expression seems to give a pretty good approximation for most of the materials of practical interest: ET ⬇

2(1 ⫺ c) ⫹ (1 ⫹ 2c) E . (1 ⫺ c) ⫹ (2 ⫹ c) m

(9.1.63)

For the dilute case (c ⬍⬍ 1), the following expression for ET can be derived:

226

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

ET ⫽

Em c ⫹ (1 ⫺ c) c(1 ⫺ )2[1 ⫺ 2 ⫹ 2 2(3 ⫺ 4) ⫹ 2(1 ⫺ 3 ⫹ 5 2 ⫺ 23]Em ⫹ , (1 ⫹ ⫺ 2)(1 ⫹ 3 ⫺ 4)

(9.1.64)

Generally speaking, the solutions from upper and lower bounds, as well as the ones from the Mori–Tanaka methods are approximate. Using the composite cylinder model, see Section 8.1, the exact relationships between the effective engineering constants and the moduli of the ﬁbers and the matrix can be obtained (Christensen, 1979); see (8.1.8)–(8.1.11). Note that the composite cylinder model does not yield the exact solution for the transverse shear modulus T . In the event that m ⫽ ƒ ⫽ , (8.1.8)–(8.1.11) reduce to (9.1.58)– (9.1.62). In other words, the Mori–Tanaka estimate gives the exact solution when m ⫽ ƒ ⫽ .

9.2 EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

In this section, we consider a ﬁber-reinforced composite material consisting of multiple layers. Each layer is assumed to be a unidirectional ﬁber-reinforced composite. The bonding between the layers is assumed perfect, that is, the displacement and tractions across the interfaces are continuous. We further assume that the thickness of the layers is much greater than the ﬁber diameter. As discussed in Chapter 5, the effective properties of the layered composite can be obtained through a hierarchical approach. First, the effective properties of each layer are evaluated based on the method discussed in the previous section. Once this is done, the effective properties of the layered composite will be estimated by assuming that each layer is a homogeneous, transversely isotropic solid. In other words, the individual ﬁbers are not explicitly accounted for in the second level of homogenization. Instead, only the collective effect of all the ﬁbers in each layer is explicitly included in the effective properties of the laminate. Therefore, when we consider the effective properties of a multilayered composite, we may assume that each later is homogeneous. To facilitate the discussions below, let us ﬁrst deﬁne the following:

9.2

n ⫽

冤 冥

33 23 , 13

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

t ⫽

冤 冥

11 22 , 12

n ⫽

冤 冥 33

223 , 213

t ⫽

227

冤 冥

11 22 . 212

(9.2.1) For the rest of this section, the summation convention is temporarily suspended. Sums will be explicitly indicated by the summation sign. This way, we can rewrite Hooke’s law using the Voigt notation as n ⫽ Cnnn ⫹ Cntt,

t ⫽ Ctnn ⫹ Cttt,

(9.2.2)

where

冤

C34 C44 C45

C35 C45 , C55

冥

C13 Cnt ⫽ C14 C15

冤

C14 C24 C46

C15 C25 , C56

冥

C11 Ctt ⫽ C12 C16

C33 Cnn ⫽ C34 C35 C13 Ctn ⫽ C23 C36

冤

C23 C24 C25

C36 C46 , C56

冥

(9.2.3)

冤

C12 C22 C26

C16 C26 . C66

冥

(9.2.4)

Obviously, Cnn ⫽ (Cnn)T,

Ctt ⫽ (Ctt)T, Ctn ⫽ (Cnt)T.

(9.2.5)

Also, because of the positive deﬁniteness of the Voigt elasticity matrix, we know that Cnn and Ctt are positive deﬁnite matrices. Now, consider a multilayer composite consisting of N layers of homogeneous materials as shown in Figure 9.3. We assume that each layer is homogeneous with its Voigt elastic matrix given by C(k), k ⫽ 1, 2, . . . , N. Therefore, for the kth layer, it follows from (9.2.2) that (k) (k) (k) (k) (k) n ⫽ C nn n ⫹ C nt t ,

(k) (k) (k) (k) ⫽ C (k) t tn n ⫹ C tt t ,

(9.2.6)

where the superscript (k) indicates that the base letter is associated with the kth layer. It is assumed that the representative volume element being considered is under a uniform state of deformation, even though the actual composite may be subjected to arbitrary loading. We further assume that the layers are perfectly bonded together, meaning that the

228

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

x3 hN hk

x1

h

h1

Figure 9.3 Multilayer composite.

traction and displacements are continuous across the layer interfaces. This immediately leads to (k) n ⫽ n,

t(k) ⫽ t,

for k ⫽ 1, 2, . . . , N

(9.2.7)

Making use of (9.2.7) in the ﬁrst of (9.2.6) yields (k) ⫺1 (k) (k) n ⫽ (C nn ) (n ⫺ C nt t).

(9.2.8)

Taking the average of (k) n over the representative volume element leads to

冘 c ⫽ 冘 c (C N

n ⫽

N

(k) k n

k⫽1

k

冘 c (C N

(k) ⫺1 nn

)

n ⫺

k⫽1

k

(k) ⫺1 nn

(k) ) C nt t,

(9.2.9)

k⫽1

where ck ⫽ hk /h is the volume fraction of the kth layer. By rearranging the terms in (9.2.9), we have n ⫽ Cnnn ⫹ Cntt,

(9.2.10)

where

冋冘

Cnn ⫽

k⫽1

册

⫺1

N

(k) ⫺1 nn

ck(C )

,

(9.2.11)

9.2

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

冋冘

册

N

⫺1 (k) ck(C (k) . nn ) C n

Cnt ⫽ Cnn

k⫽1

229

(9.2.12)

We next substitute (9.2.8) into the second of (9.2.6). This gives us (k) (k) ⫺1 (k) (k) ⫽ C tn (C nn ) (n ⫺ C (k) t nt t) ⫹ C tt t (k) (k) ⫺1 (k) ⫺1 (k) ⫽ C tn (C nn ) n ⫹ [C tt(k) ⫺ C (k) tn (C nn ) C2 nt ]t.

(9.2.13)

Taking the average of (k) t over the representative volume element leads to

冘 c ⫽ 冘 c C (C ) ⫹ 冘 c [C ⫺ C (C ) C ] . N

t ⫽

N

k

(k) t

(k) ⫺1 nn

(k) tn

k

n

k⫽1

k⫽1

N

(k) tt

k

(k) tn

(k) ⫺1 nn

(k) nt

t

(9.2.14)

k⫽1

Substitution of (9.2.10) into the above yields t ⫽ Ctnn ⫹ Cttt,

(9.2.15)

where

冋冘 c C

册

N

Ctn ⫽

k

(k) ⫺1 (C nn ) Cnn,

(k) tn

k⫽1

冘 N

Ctt ⫽

冘 cC

(9.2.16)

N

ckC tt(k) ⫹

k⫽1

k

(k) ⫺1 (k) (C nn ) (Cnt ⫺ C nt ).

(k) tn

(9.2.17)

k⫽1

Clearly, Cnn, Cnt, Ctn, and Ctt provide the complete effective Voigt elastic matrix of the layered composite. Taking advantage of the symmetry properties (9.2.5), it can be shown that Cnn ⫽ (Cnn)T,

Ctt ⫽ (Ctt)T,

Ctn ⫽ (Cnt)T.

Next, we assume that each layer is a monoclinic material with its plane of symmetry in the x1x2 plane. In this case, the Voigt elastic matrix has the following form:

230

C

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

(k) nn

冤

冥

C (k) 0 0 33 (k) ⫽ 0 C 44 C (k) 45 , (k) 0 C (k) C 45 55

C

(k) tn

C

⫽ (C ) , (k) T nt

C

冤

冥

(k) (k) (k) C 13 C 23 C 36 ⫽ 0 0 0 , 0 0 0

(k) nt

冤

冥

C (k) C (k) C (k) 11 12 16 (k) (k) (k) ⫽ C 12 C 22 C 26 . (k) (k) (k) C 16 C 26 C 66

(k) tt

(9.2.18)

(9.2.19)

Substituting these into (9.2.11) and (9.2.12) yields

冘 Cc

冤 冉 冤

k (k) 33

k⫽1

Cnn ⫽

⫽

0

0

⫺

(k)

k

k⫽1 N

(k) k 45 (k)

k⫽1

冘 Cc 冊

冘 c⌬C 冘 c⌬C N

(k) ckC 55

k⫽1 N

0

0

冘⌬ cC ⫺冘 ⌬ N

k

k⫽1

(k) 45 (k)

(k) 44 (k)

N

k (k) 33

k⫽1

冥

⫺1

N

0 1 D 1 D

0 0

0

冘⌬ 冘 c⌬C N

(k) ckC 44 (k)

k⫽1 N

k

k⫽1

1 D 1 D

(k) 45 (k)

冘 c⌬C 冘 c⌬C N

冥

k

(k) 45 (k)

k

(k) 55 (k)

k⫽1 N k⫽1

,

(9.2.20)

where

冘 N

D⫽

ckC (k) 55 ⌬(k)

k⫽1

冘 N

k⫽1

(k) ckC 44

⌬(k)

冋冘 册 N

⫺

k⫽1

(k) ckC 45

⌬(k)

2

,

(k) (k) (k) 2 ⌬(k) ⫽ C 44 C 55 ⫺ (C 45 ) ⬎ 0.

(9.2.21) (9.2.22)

Next, making use of (9.2.20) in (9.2.16) yields

冉冘 冊 N

Ctn ⫽

k⫽1

Finally, (9.2.17) leads to

ck C (k) 33

⫺1

冘 N

k⫽1

冤

(k) 0 13 ck C (k) C 0 23 (k) C 33 (k) C 36 0

冥

0 0 . 0

(9.2.23)

9.2

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

冤

冘

k⫽1

冘 N

⫺

k⫽1

冤

冥

(k) (k) (k) (k) (k) (k) C 23 C 13 C 36 C 13 13 C 13 ck C (k) (k) (k) (k) (k) (k) C C C C C 13 23 23 23 36 C 23 C (k) (k) (k) (k) (k) (k) 33 C (k) C C C C 13 36 23 36 36 C 36

冉冘 冊 N

⫹

冥

(k) (k) (k) C 11 C 12 C 16 (k) (k) (k) ck C 12 C 22 C 26 (k) (k) (k) C 16 C 26 C 66

N

Ctt ⫽

231

r⫽1

cr (r) C 33

⫺1

冘 冘 C c cC N

N

m k (m) (k) 33 33

k⫽1 m⫽1

冤

冥

(k) (k) (k) C (m) C (m) C (m) 13 C 13 23 C 13 36 C 13 (m) (k) (m) (k) (m) (k) ⫻ C 13 C 23 C 23 C 23 C 36 C 23 . (k) (k) (k) C (m) C (m) C (m) 13 C 36 23 C 36 36 C 36

(9.2.24)

If we let Cij be the elements of the 6 ⫻ 6 Voigt effective elastic matrix C, results from (9.2.20), (9.2.23), and (9.2.24) can be summarized as follows:

冘 c 冋C N

Cij ⫽

k

(k) ij

⫺

k⫽1

(k) C (k) C (k) i3 C j3 i3 ⫹ (k) C (k) C 33 33

冉冘 Cc 冊 冋 冘 cCC ⫺1

N

r⫽1

N

m

r (r) 33

m⫽1

册册

(m) 3j (m) 33

(9.2.25) for i, j ⫽ 1, 2, 3, 6: Cij ⫽

1 D

⫽0

冘 c⌬C N

k

k⫽1

(k) ij (k)

for i, j ⫽ 4, 5,

for i ⫽ 1, 2, 3, 6;

(9.2.26)

j ⫽ 4, 5.

(9.2.27)

Similarly, the compliance matrix can be partitioned as

冤

冥

S13 S23 S36 Snt ⫽ S14 S24 S46 , S15 S25 S56

冤

冥

S11 S12 S16 Stt ⫽ S12 S22 S26 , S16 S26 S66

S33 S34 S35 Snn ⫽ S34 S44 S45 , S35 S45 S55 S13 S14 S15 Stn ⫽ S23 S24 S25 , S36 S46 S56

冤

冥

(9.2.28)

冤

冥

(9.2.29)

232

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

Following the same procedure, elements of the effective compliance matrix are given by (see Appendix 9.A)

冥 冋冘

冤

S11 S12 S16 Stt ⫽ S12 S22 S26 ⫽ S16 S26 S66

⫺1 ck(S (k) tt )

k⫽1

冥 冋冘 冥 冋冘

冤

S13 S14 S15 Stn ⫽ S23 S24 S25 ⫽ Stt S36 S46 S56

冤

S13 S23 S36 Snt ⫽ S14 S24 S46 ⫽ S15 S25 S56

冤

冥

S33 S34 S35 Snn ⫽ S34 S44 S45 ⫽ S35 S45 S55

冘

册

⫺1

N

,

(9.2.30)

册

N

⫺1 (k) ck(S (k) tt ) S tn ,

k⫽1

册

N

(k) ck S nt (S tt(k))⫺1 Stt,

k⫽1

N

冘cS

(9.2.31)

(9.2.32)

N

(k) ck S nn ⫹

k⫽1

k

(k) (S tt(k))⫺1(Stn ⫺ S tn ).

(k) nt

k⫽1

(9.2.33) Example 9.1 Consider a layered material consisting of two alternating layers. The layers are identical, except that the ﬁber directions are perpendicular to each other between adjacent layers. We are to ﬁnd the effective elastic constants for this layered composite. To this end, let us denote the Voigt elasticity matrix for the layer whose ﬁber direction is in the x1 direction by

C (1) ⫽

冤

C11

C12 C12

0

0

0

C12

C22

C23

0

0

0

C12

C23

C22

0

0

0

0

0

0

0

0

0

0

0

0

C22 ⫺ C23 0 2 0 C66 0

0

冥

.

0 0

(9.2.34)

C66

A 90⬚ rotation about the x3 axis yields the Voigt elasticity matrix for the adjacent layer:

9.2

C (2) ⫽

冤

233

EFFECTIVE PROPERTIES OF MULTILAYER COMPOSITES

C22

C12

C23

0

0

0

C12

C11

C12

0

0

0

C23

C23

C22

0

0

0

0

0

0

C66

0

0

0

0

0

0

0

0

0

0

冥

.

C22 ⫺ C23 2 0

0

(9.2.35)

C66

Making use of these in (9.2.25)–(9.2.27) with N ⫽ 2, c1 ⫽ c2 ⫽ –12 , we arrive at (k) (k) ⌬(k) ⫽ C 44 C 55 ⫽

(C22 ⫺ C23)C66 , 2

D⫽

冉

冊

2

1 2 1 ⫹ . 4 C22 ⫺ C23 C66 (9.2.36)

Thus, the nonzero components of the effective Voigt elasticity matrix of the layered composite are C11 ⫽ C22 ⫽

C33 ⫽ C22, C13 ⫽ C23 ⫽

C44 ⫽ C55 ⫽

冋

册

1 (C ⫺ C23)2 C11 ⫹ C22 ⫺ 12 , 2 2C22 C12 ⫽ C12 ⫺

(9.2.37)

(C12 ⫺ C23)2 , 4C22

C12 ⫹ C23 , 2

(9.2.38)

2C66(C22 ⫺ C23) , 2C66 ⫹ (C22 ⫺ C23)

C66 ⫽ C66.

(9.2.39)

Making use of (9.2.30), the in-plane Young modulus and shear modulus can be written in terms of the engineering constants of the individual layer: E0 ⫽

(EL ⫹ ET)2 ⫺ 4E 2L 2TL , 2(EL ⫹ ET)(1 ⫺ LTTL)

0 ⫽

2EL . EL ⫹ ET TL

(9.2.40)

234

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

9.3 EFFECTIVE PROPERTIES OF A LAMINA

In the composite material literature, a lamina is a thin layer of unidirectional ﬁber-reinforced composite material; see Figure 9.4. Because the thickness is much smaller relative to the in-plane dimensions, the deformation of a lamina can be approximated by a state of plane stress. This means 13 ⬇ 23 ⬇ 33 ⬇ 0.

(9.3.1)

It thus follows from Hooke’s law that L13klkl ⫽ L23klkl ⫽ L33klkl ⫽ 0.

(9.3.2)

For a lamina, the effective elasticity tensor is transversely isotropic with the axis of symmetry being the x1 axis, as shown in Figure 9.3, the above equation yields 13 ⫽ 23 ⫽ 0

L l and 33 ⫽ ⫺ 1311 11 ⫺ 1322 22. L3333 L3333

(9.3.3)

Substituting the above into Hooke’s law again, we arrive at

冉 冉

冊 冉 冊 冉

冊 冊

11 ⫽ L1111 ⫺

L1311 L 11 ⫹ L1122 ⫺ 1322 22, L3333 L3333

(9.3.4)

22 ⫽ L2211 ⫺

L1311 L 11 ⫹ L2222 ⫺ 1322 22. L3333 L3333

(9.3.5)

Therefore, in the reduced form of the Voigt notation, the stress–strain relationship for a thin lamina can be written as x3 x2 x1

Figure 9.4 Thin lamina.

9.3

EFFECTIVE PROPERTIES OF A LAMINA

冤冥 冤 1 2 6

冥冤 冥

Q11 Q12 0 Q12 Q22 0 0 0 Q66

⫽

1 2 , 6

235

(9.3.6)

where

冤冥 冤 冥 冤冥 冤 冥 1 2 6

⫽

11 22 , 12

1 2 6

11 22 , 212

(9.3.7)

i, j ⫽ 1, 2, 6

(9.3.8)

⫽

and Qij ⫽ Cij ⫺

Ci3Cj3 , C33

with Cij being the Voigt elastic constants of the lamina. Note that Cij is transversely isotropic so that C63 ⫽ 0. Thus, Q66 ⫽ C66. The matrix Q in (9.3.6) is called the reduced stiffness matrix of the lamina. The reduced compliance matrix S (not to be confused with the Eshelby tensor) for the lamina is obtained by inverting (9.3.6),

冤冥 冤 1 2 6

⫽

S11 S12 0 S12 S22 0 0 0 S66

冥冤 冥

1 2 , 6

(9.3.9)

where S11 ⫽

Q22 , 2 Q11Q22 ⫺ Q12

S22 ⫽

Q12 S12 ⫽ ⫺ , 2 Q11Q22 ⫺ Q12

Q11 , 2 Q11Q22 ⫺ Q12 S66 ⫽

1 . Q66

(9.3.10)

(9.3.11)

The Young moduli in the ﬁber and transverse to the ﬁber directions can thus be deﬁned, respectively, as EL ⫽

2 1 Q Q ⫺ Q12 ⫽ 11 22 , S11 Q22

ET ⫽

1 Q Q ⫺ Q212 ⫽ 11 22 . S22 Q11

The shear modulus in the plane of the lamina is

(9.3.12)

236

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

L ⫽ Q66.

(9.3.13)

The corresponding Poisson ratios are S Q LT ⫽ ⫺ 12 ⫽ 12, S11 Q22

S Q TL ⫽ ⫺ 12 ⫽ 12. S22 Q11

(9.3.14)

Note that LT represents the contraction in the transverse direction when the lamina is stretched in the ﬁber direction, while TL represents the contraction in the ﬁber direction when the lamina is stretched in the transverse direction. These are exactly the same engineering elastic constants as introduced in Section 9.1. As discussed in Section 9.1, only four of these engineering elastic constants are independent because 2 Q12(Q11Q22 ⫺ Q12 ) ⫽ TLEL. Q11Q22

LT ET ⫽

(9.3.15)

Therefore, (9.3.12)–(9.3.14) can be inverted to obtain Q11 ⫽

EL , 1 ⫺ LTTL

Q22 ⫽

Q12 ⫽

ET , 1 ⫺ LTTL

Q66 ⫽ L,

LTET TLEL ⫽ . 1 ⫺ LTTL 1 ⫺ LTTL

(9.3.16)

(9.3.17)

The corresponding components of the reduced compliance tensor are S11 ⫽

1 , EL

S22 ⫽

1 , ET

S66 ⫽

S12 ⫽ ⫺ LT ⫽ ⫺ TL. EL ET

1 , L

(9.3.18)

(9.3.19)

Equations (9.3.6) and (9.3.9) are written in a coordinate system where the x1 axis is in the direction of the ﬁbers. In the coordinate system xˆ i shown in Figure 9.2, where the xˆ 1 axis forms an angle from the ﬁber direction, the stress–strain relationship becomes

9.3

冤冥 冤 x y xy

ˆ 11 Q ˆ 12 ⫽ Q ˆ 13 Q

EFFECTIVE PROPERTIES OF A LAMINA

ˆ 12 Q ˆ 22 Q ˆ 23 Q

ˆ 13 Q ˆ 23 Q ˆ 66 Q

冥冤 冥

x y , ␥xy

237

(9.3.20)

where ˆ 11 ⫽ Q11m4 ⫹ 2(Q12 ⫹ 2Q66)m2n2 ⫹ Q22n4, Q

(9.3.21)

ˆ 22 ⫽ Q11n4 ⫹ 2(Q12 ⫹ 2Q66)m2n2 ⫹ Q22m4, Q

(9.3.22)

ˆ 12 ⫽ (Q11 ⫹ Q22 ⫺ 4Q66)m2n2 ⫹ Q12(m4 ⫹ n4), Q

(9.2.23)

ˆ 16 ⫽ (Q11 ⫺ Q12 ⫺ 2Q66)m3n ⫹ (Q12 ⫺ Q22 ⫹ 2Q66)mn3, Q

(9.3.24)

ˆ 26 ⫽ (Q11 ⫺ Q12 ⫺ 2Q66)mn3 ⫹ (Q12 ⫺ Q22 ⫹ 2Q66)m3n, Q

(9.3.25)

ˆ 66 ⫽ (Q11 ⫹ Q22 ⫺ 2Q12 ⫺ 2Q66)m2n2 ⫹ Q66(m4 ⫹ n4), Q

(9.3.26)

in which m ⫽ cos , n ⫽ sin . Since the lamina is very thin, its deformation can be represented by the deformation of its midplane using the Kirchhoff assumption, that is, a cross-section plane perpendicular to the midplane prior to the deformation remains perpendicular to the midplane after deformation. Mathematically, this means x ⫽

⭸u0 ⭸2w0 ⫺z , ⭸x ⭸x 2

␥xy ⫽ 2xy ⫽

y ⫽

⭸0 ⭸2w0 ⫺z , ⭸y ⭸y 2

⭸u0 ⭸ ⭸2w0 ⫹ 0 ⫺ 2z , ⭸y ⭸x ⭸x⭸y

(9.3.27)

(9.3.28)

where u0 and 0 are the in-plane displacement of the midplane and w0 is the out-of-plane displacement (deﬂection) of the midplane of the lamina. The coordinate z indicates the location relative to the middle plane. Substitution of (9.3.27) and (9.3.28) into (9.3.20) yields

238

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

冤冥 冤 x y xy

ˆ 11 Q ˆ 12 ⫽ Q ˆ 13 Q

冥冤 冥 冤

ˆ 12 Q ˆ 22 Q ˆ 23 Q

ˆ 13 Q ˆ 23 Q ˆ 66 Q

x0 y0 0 ␥ xy

ˆ 11 Q ˆ 12 Q ˆ 12 Q ˆ 22 ⫹z Q ˆ 13 Q ˆ 23 Q

冥冤 冥

ˆ 13 Q ˆ 23 Q ˆ 66 Q

kx ky , kxy (9.3.29)

where

0x y0 ␥ 0xy

冤 冥

冤 冥

(9.3.30)

冤冥

(9.3.31)

⭸u0 ⭸x

⫽

⭸0 ⭸y

⭸u0 ⭸ ⫹ 0 ⭸y ⭸x

is the midplane strain and

冤冥

kx ky ⫽ ⫺ kxy

⭸2w0 ⭸y 2 ⭸2w0 ⭸y 2

2

⭸2w0 ⭸x⭸y

is the midplane curvature.

9.4 EFFECTIVE PROPERTIES OF A LAMINATED COMPOSITE PLATE

Composite laminates in engineering applications typically consist of multiple unidirectional ﬁber-reinforced laminas (or plies) stacked up together. The stacking sequence of a laminate can be designated by a standard notation. For example, [02 /902 / ⫺453 /453]s is used to designate a laminate that starting from the bottom, that is, at z ⫽ ⫺h/2 (h is the total thickness of the laminate), there are two plies at 0⬚ orientation ( ⫽ 0⬚), two plies at 90⬚ orientation, followed by three plies at ⫺45⬚, and last three plies at ⫹45⬚ orientation. The subscript s indicates that the laminate is symmetrical with respect to the midplane (z ⫽ 0), that is, the top half of the laminate is a mirror image of the bottom

9.4

239

EFFECTIVE PROPERTIES OF A LAMINATED COMPOSITE PLATE

half. For nonsymmetrical laminates, the total stacking sequence needs to be explicitly indicated. In this case, a subscript T will be used. For most engineering laminates of practical interest, the thickness of each ply is in the order of millimeters. The diameter of the ﬁber is typically in the order of micrometers. To bridge these two length scales, we will take a hierarchical approach in order to estimate the effective properties of the laminate. First, the effective properties of the unidirectional ply are evaluated based on the method discussed in the previous chapter. Once this is done, the effective properties of the laminate will be estimated by assuming each ply as a homogeneous, transversely isotropic layer. Now consider a generic laminate shown in Figure 9.3. We assume that the bonding between the plies is perfect, that is, displacements and tractions are continuous across the ply interfaces. Since the stresses in a laminate vary from layer to layer, it is convenient to introduce the resultant forces and moments:

冤 冥

Nx Ny ⫽ Nxy

冕

h/2

⫺h / 2

冤冥 x y xy

冤 冥

Mx My ⫽ Mxy

dz,

冕

h/2

⫺h / 2

冤冥

x y z dz. xy

(9.4.1)

In terms of the resultants, (9.3.29) can be rewritten as

冤 冥 冤

Nx A11 Ny ⫽ A12 Nxy A13

A12 A22 A23

A13 A23 A66

冥冤 冥 冤 x0 0y 0 ␥ xy

B11 B12 B13 B22 B23 B13 B23 B66

⫹ z B12

冥冤 冥

kx ky , kxy (9.4.2)

冤 冥 冤

Mx B11 My ⫽ B12 Mxy B13

B12 B22 B23

冥冤 冥 冤 x0 0y 0 ␥ xy

B13 B23 B66

D11 ⫹ z D12 D13

D12 D22 D23

D13 D23 D66

冥冤 冥

kx ky , kxy (9.4.3)

where

冘 (Qˆ ) (h ⫺ h n

Aij ⫽

ij k

k

),

(9.4.4)

2 k⫺1

(9.4.5)

k⫺1

k⫽1

1 Bij ⫽ 2

冘 (Qˆ ) (h ⫺ h n

ij k

k⫽1

2 k

),

240

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

x3 x2 x1

Figure 9.5

Dij ⫽

1 3

冘 (Qˆ ) (h ⫺ h n

ij k

3 k

3 k⫺1

)

(9.4.6)

k⫽1

are called the extensional stiffness matrix, coupling stiffness matrix, and bending stiffness matrix of the laminate, respectively. PROBLEMS

9.1 Consider a unidirectional ﬁber-reinforced composite plate as shown in Figure 9.5 (ﬁbers are in the x1 direction). Find the lower and upper bounds for the effective Young modulus E11 and E22 by using the minimum potential and minimum complementary energy theorems, respectively. Compare your results with the rule of mixture predictions. (Hint: Use 0ij ⫽ 0␦i1␦j1 and 0ij ⫽ 0␦i1␦j1 for E11. Use ij0 ⫽ 0␦i2␦j2 and 0ij ⫽ 0␦i2␦j2 for E22.) 9.2 Derive the extensional stiffness matrix, the coupling stiffness matrix, and the bending stiffness matrix of a generic laminate. 9.3 Prove (9.2.29)–(9.2.32). 9.4 Consider a ﬁber-reinforced cross-ply laminate as shown in Figure 9.4. Further, assume that all the layers have the same thickness and their elastic constants are given by EL, ET, L, LT, and TL. They are related to the elastic properties of the ﬁber, the matrix, and the ﬁber volume fraction through the micromechanics schemes discussed in Section 9.1. Find the matrices A, B, and D as deﬁned in (9.4.6)–(9.4.8).

APPENDIX 9.A

To facilitate the discussions below, let us ﬁrst deﬁne the following:

APPENDIX 9.A

n ⫽

冤 冥

33 23 , 13

t ⫽

冤 冥

11 22 , 12

n ⫽

冤 冥 33

223 , 213

t ⫽

241

冤 冥

11 22 . 212

(9.A.1) Thus, we have n ⫽ Sntt ⫹ Snnn,

t ⫽ Sttt ⫹ Stnn,

(9.A.2)

where

冤

冥

S13 S23 S36 Snt ⫽ S14 S24 S46 , S15 S25 S56

冤

冥

S11 S12 S16 Stt ⫽ S12 S22 S26 . S16 S26 S66

S33 S34 S35 Snn ⫽ S34 S44 S45 , S35 S45 S55 S13 S14 S15 Stn ⫽ S23 S24 S25 , S36 S46 S56

冤

冥

(9.A.3)

冤

冥

(9.A.4)

Obviously, Snn ⫽ (Snn)T,

Stt ⫽ (Stt)T, Stn ⫽ (Snt)T.

(9.A.5)

Also, because of the positive deﬁniteness of the Voigt compliance matrix, we know that Snn and Stt are positive deﬁnite matrices. Now, consider a multilayered composite consisting of N layers of homogeneous materials as shown in Figure 9.3. We assume that each layer is homogeneous with its Voigt elastic matrix given by S(k), k ⫽ 1, 2, . . . , N. Therefore, for the kth layer, it follows from (9.A.2) that (k) (k) (k) (k) (k) n ⫽ S nn n ⫹ S nt t ,

(k) (k) t(k) ⫽ S tn n ⫹ S tt(k) t(k),

(9.A.6)

where the superscript (k) indicates the quantity associated with the kth layer. It is assumed that the representative element being considered is under a uniform state of deformation, even though the actual composite may be subjected to arbitrary loading. We further assume that the layers are perfectly bonded together, meaning that the traction and displacements are continuous across the layer interfaces. This immediately leads to

242

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

(k) n ⫽ n,

t(k) ⫽ t,

for k ⫽ 1, 2, . . . , N.

(9.A.7)

Making use of the above in the second of (9.A.6) yields ⫺1 (k) (k) ⫽ (S (k) t tt ) (n ⫺ S tn n).

(9.A.8)

Taking the average of (k) t over the representative volume element leads to

冘 c N

n ⫽

k

冘 c (S N

(k) t

⫽

k

)

t ⫺

k⫽1

k⫽1

冘 c (S N

(k) ⫺1 tt

k

(k) ⫺1 tt

(k) ) S tn n,

(9.A.9)

k⫽1

where ck ⫽ hk /h is the volume fraction of the kth layer. By rearranging the terms in (9.A.9), we have t ⫽ Sttt ⫹ Stnn,

(9.A.10)

where

冤

冥

S11 S12 S16 Stt ⫽ S12 S22 S26 ⫽ S16 S26 S66

冋冘 c (S k

冥 冋冘

冤

(k) ⫺1 tt

)

k⫽1

S13 S14 S15 Stn ⫽ S23 S24 S25 ⫽ Stt S36 S46 S56

册

⫺1

N

,

(9.A.11)

册

N

⫺1 (k) ck(S (k) tt ) S tn .

k⫽1

(9.A.12)

We next substitute (9.A.8) into the ﬁrst of (9.A.6). This gives us (k) (k) (k) ⫺1 (k) (k) (k) ⫺1 (k) n ⫽ [S nn ⫺ S nt (S tt ) S tn ]n ⫹ S nt (S tt ) t.

(9.A.13)

Taking the average of (k) t over the representative volume element leads to

冘 c ⫽ 冘 c [S N

n ⫽

N

(k) k n

k⫽1

k

冘cS N

(k) nn

(k) ⫺1 tt

⫺ S (S ) S ]n ⫹ (k) nt

(k) tn

k⫽1

Substitution of (9.A.10) into the above yields

k

k⫽1

⫺1 (S (k) tt ) t.

(k) nt

REFERENCE

n ⫽ Snnn ⫹ Sntt,

243

(9.A.14)

where

冥 冋冘

冤

S13 S23 S36 Snt ⫽ S14 S24 S46 ⫽ S15 S25 S56

冤

冥

S33 S34 S35 Snn ⫽ S34 S44 S45 ⫽ S35 S45 S55

冘cS

(k) ck S nt (S tt(k))⫺1 Stt,

k⫽1

N

k

册

N

冘cS

(9.A.15)

N

(k) nn

⫹

k⫽1

k

(k) (S tt(k))⫺1(Stn ⫺ S tn ).

(k) nt

k⫽1

(9.A.16) Clearly, Snn, Snt, Stn, and Stt provide the complete effective Voigt compliant matrix of the layered composite. Taking advantage of the symmetry properties (9.A.5), it can be shown that Snn ⫽ (Snn)T,

Stt ⫽ (Stt)T,

Stn ⫽ (Snt)T.

Next, we assume that each layer is a monoclinic material with its plane of symmetry in the x1x2 plane. In this case, the Voigt elastic matrix has the following forms:

(k) S nn

冤

冥

S (k) 0 0 33 (k) (k) ⫽ 0 S 44 S 45 , (k) (k) 0 S 45 S 55

S

(k) tn

⫽ (S ) , (k) T nt

(k) S nt

S

(k) tt

冤

冥

(k) (k) (k) S 13 S 23 S 36 ⫽ 0 0 0 , 0 0 0

(9.A.17)

冤

(9.A.18)

冥

(k) (k) (k) S 11 S 12 S 16 (k) (k) (k) ⫽ S 12 S 22 S 26 . (k) (k) (k) S 16 S 26 S 66

REFERENCE Christensen, R. M. (1979). Mechanics of Composite Materials, Krieger, Malabar, FL.

244

EFFECTIVE PROPERTIES OF FIBER-REINFORCED COMPOSITE LAMINATES

SUGGESTED READINGS Agarwal, B. D. and L. J. Broutman. (1990). Analysis and Performance of Fiber Composites, Wiley, New York. Chawla, K. K. (1987). Composite Materials—Science and Engineering, Springer, New York. Hyer, M. W. (1998). Stress Analysis of Fiber-Reinforced Composite Materials, McGraw-Hill, Boston.

10 BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES Micromechanics has been used extensively in the study of damage and failure of engineering materials. There is a large body of literature in this area. It is certainly not possible, nor the intent of this chapter, to provide an extensive summary of existing results. The objective here is to take a few examples that are illustrative of how the micromechanics methods and techniques are being used to understand and model certain commonly seen damage and failure modes in engineering composite materials. We will discuss one example in each of the three areas; interfaces, ﬁber, and matrix.

10.1 IMPERFECT INTERFACES

Let the interface between two media be denoted by S. As discussed in Section 4.2, we call an interface S a perfect interface if the two media are mechanically coherent, that is, the displacement and traction ﬁelds are continuous across this interface. The continuity of displacement and traction across a perfect interface can be written as ⌬ui ⬅ ui(S⫹) ⫺ ui(S⫺) ⫽ 0,

(10.1.1)

⌬ij nj ⬅ [ij(S⫹) ⫺ ij(S⫺)]nj ⫽ 0,

(10.1.2)

where nj is the unit normal vector of the interface S, and ui(S⫹) and ij(S⫹) are the values of ui(x) and ij(x) evaluated at the positive side Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

245

246

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

of S, while ui(S⫺) and ij(S⫺) are the values of ui(x) and ij(x) evaluated at the negative side of S. It is assumed that nj points to the positive side of S; see Figure 4.3. In many engineering applications, the interfaces in a composite material may not be perfect. In this section, we will discuss one of the simplest models used to model the imperfect interfaces. For quasi-static problems, the imperfection of interfaces is reﬂected mainly by the discontinuity of displacement ﬁeld across the interface. The interfacial spring model therefore postulates that the traction is continuous across the interface ⌬ij nj ⬅ [ij(S⫹) ⫺ ij(S⫺)]nj ⫽ 0,

(10.1.3)

but the displacement ﬁeld is discontinuous. The jump in the displacement ﬁeld across the interface is proportional to the traction vector on the interface, that is, ⌬ui ⬅ ui(S⫹) ⫺ ui(S⫺) ⫽ ijik nk,

(10.1.4)

where the second-order tensor ij represents the compliance of the interface. For simplicity, we assume that ij is symmetric and positive deﬁnite. It is clear from (10.1.4) that ij ⫽ 0 corresponds to a perfect interface, while ij → ⬁ represents complete debond (ik nk ⫽ 0). From this point of view, a slight deviation from the perfect interface case can be modeled by the limit of ij → 0. A special form of ij that has some physical signiﬁcance is given by ij ⫽ ␣␦ij ⫹ ( ⫺ ␣)ninj.

(10.1.5)

It can be easily shown that ␣ and  represent the compliance in the tangential and normal directions of the interfaces, respectively, that is, ⌬ui(␦ik ⫺ ni nk) ⫽ ␣ij nj(␦ik ⫺ ni nk),

(10.1.6)

⌬ui ni ⫽ ij nj ni.

(10.1.7)

When  ⫽ 0, such constitutive characterization of the interfaces allows for relative sliding between the two surfaces, but not separation. Furthermore, the free-sliding case studied by Mura (1987) can be achieved by setting ␣ → ⬁ with  ⫽ 0. Therefore, solutions to the case of small ␣ with  ⫽ 0 provide the approximations in contrast to the sliding interface. It also should be mentioned that material interpenetration

10.1

IMPERFECT INTERFACES

247

may take place when  ⫽ 0, which is a violation of the compatibility requirement. Further discussions on this may be found in Achenbach and Zhu (1989). For the remainder of this section, we focus on the effective elastic properties of composite materials with imperfect interfaces. First, we will solve the Eshelby inclusion problem with imperfect interface. Then, we will use the Mori–Tanaka approach to estimate the effective elastic properties. Finally, the bounds of the effective properties for such composite will be developed based on the classical variational principles. Consider an elastic solid of inﬁnite extent containing an ellipsoidal inclusion ⍀ with eigenstrain distribution ij*. Assume that the interface between the inclusion and the surrounding medium is imperfect and the displacement jump across the interface is governed by (10.1.6) and (10.1.7). We will call this eigenstrain problem the modiﬁed Eshelby inclusion problem. In what follows, we would like to develop a solution to this modiﬁed Eshelby inclusion problem. It follows from (3.3.5) that the displacement ﬁeld should satisfy the following equations of equilibrium: Lijkl uk,lj(x) ⫺ Lijkl *kl, j(x) ⫽ 0 ui(x) → 0

in ⍀.

as 兩x兩 → ⬁.

(10.1.8) (10.1.9)

Furthermore, it follows from (2.6.23) and (2.6.24) that the Green function G⬁ij (x, y) satisﬁes Lijkl

⭸2G⬁km(x, y) ⫹ ␦im␦(x ⫺ y) ⫽ 0, ⭸xl ⭸xj

(10.1.10)

G⬁ij (x, y) → 0

(10.1.11)

as 兩x兩 → ⬁,

where ␦(x) is the three-dimensional Dirac delta function. Now, let us multiply (10.1.10) by ui(x) and integrate the resulting equation over a volume V. This leads to

冕 u (x)L V

i

ijkl

⭸2G⬁km(x, y) dV(x) ⫽ ⭸xl ⭸xj

再

⫺um(y)

0

y僆V . yⰻV

(10.1.12)

By using the divergence theorem, we can rewrite the volume integral in (10.1.12) as

248

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冕 u (x)L ⭸ G⭸x (x,⭸x y) dV(x) ⭸G (x, y) ⫽ 冕 u (x)L n dS(x) ⫺ 冕 u (x)L ⭸x 2

km

i

V

ijkl

l

j

km

i

S

ijkl

j

V

l

i, j

ijkl

⭸Gkm(x, y) dV(x), ⭸xl

(10.1.13) where S is the surface of V, and ni is the unit outward normal of S. Next, multiplying (10.1.8) by Gim(x, y) and integrating the result over the volume V lead to

冕 G (x, y)L V

⬁ im

ijkl

uk,lj(x) dV(x) ⫺

冕 G (x, y)L V

⬁ im

* (x) dV(x) ⫽ 0.

ijkl kl, j

(10.1.14) Following the procedures that led to (10.1.13), the ﬁrst volume integral in the above equation can be written as

冕 G (x, y)L u (x) dV(x) ⭸G (x, y) ⫽ 冕 G (x, y)L u (x)n dS(x) ⫺ 冕 L ⭸x ⬁ im

V

ijkl

⬁ im

⬁ im

S

k,lj

ijkl

k,l

j

ijkl

V

uk,l(x) dV(x).

j

(10.1.15) Note that the last volume integral on the right-hand side of (10.1.13) is the same as that of (10.1.15). Therefore, by subtracting (10.1.12) from (10.1.14), we arrive at

冕L S

冋

⬁ Gim (x, y)uk,l(x) ⫺ ui(x)

ijkl

⫺

冕 G (x, y)L V

⬁ im

* (x) dV(x) ⫽

ijkl kl, j

册

⭸G⬁im(x, y) nj dS(x) ⭸xl

再

um(y) 0

y僆V . yⰻV

(10.1.16)

Finally, making use of the divergence theorem on the volume integral, we arrive at

10.1

再

冕L

⬁ Gim (x, y)[uk,l(x) ⫺ *(x)] ⫺ ui(x) kl

ijkl

S

⫹

冕 ⭸G ⭸(x,x y) L ⬁ im

*(x) dV(x) ⫽

ijkl kl

V

l

再

IMPERFECT INTERFACES

冎

⭸G⬁im(x, y) ⭸xl

nj dS(x)

y僆V . yⰻV

um(y) 0

249

(10.1.17)

Now, taking the region V to be the inclusion ⍀, and letting y 僆 ⍀ where the eigenstrain is given, the above integral representation yields um(y) ⫽

冕

S⫺

⫹

再

⬁ Lijkl Gim (x, y)[uk,l(x) ⫺ *(x)] ⫺ ui(x) kl

冕 ⭸G ⭸(x,x y) L ⬁ im

冎

⭸G⬁im(x, y) ⭸xl

*(x) dV(x).

(10.1.18)

ijkl kl

V

nj dS(x)

l

Note that for y 僆 S⫺, Hooke’s law (3.3.2) yields Lijkl[uk,l(x) ⫺ *(x)] ⫽ ij(x). kl

(10.1.19)

Therefore, (10.1.18) can be rewritten as um(y) ⫽

冕

S⫺

⫹

冋

G⬁im(x, y)kl(x) ⫺ ui(x)Lijkl

冕 ⭸G ⭸(x,x y) L ⬁ im

V

册

⭸G⬁im(x, y) ⭸xl

nj dS(x)

*(x) dV(x).

(10.1.20)

ijkl kl

l

Next, take V to be the region exterior to ⍀. Then, for y inside ⍀, or equivalently, for y outside V where the eigenstrain is zero, (10.1.17) yields

冕

S⫹

冋

⬁ Lijkl Gim (x, y)uk,l(x) ⫺ ui(x)

or, make use of Hooke’s law,

册

⭸G⬁im(x, y) ⭸xl

nj dS(x) ⫽ 0,

(10.1.21)

250

冕

S⫹

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冋

G⬁im(x, y)kl(x) ⫺ ui(x)Lijkl

册

⭸G⬁im(x, y) ⭸xl

nj dS(x) ⫽ 0.

(10.1.22)

Note that both (10.1.20) and (10.1.22) are valid for y inside ⍀. Thus, it follows from subtracting (10.1.21) from (10.1.18) that

冕 ⭸G ⭸(x,y y) L *(y) dV(y) ⭸G (x, y) ⫹ 冕 ⌬u (y)L n dS(y), ⭸y ⬁ im

um(x) ⫽

ijkl kl

V

l

⬁ im

i

S

ijkl

j

(10.1.23)

l

where we have used the traction continuity condition (10.1.3). For convenience, we have also switched the variables x and y and made use of the symmetry properties of the inﬁnite domain Green’s function (2.6.26). The above equation is an integral representation of the displacement ﬁeld within the inclusion. An integral equation can be derived by letting the point x approach the boundary S. Solving such integral equations typically requires numerical methods. In what follows, we will discuss some special cases of (10.1.23) and develop approximate and asymptotic solutions. First, we assume that the eigenstrain is uniform on ⍀. Then, (10.1.23) leads to um,n(x) ⫽

冕 ⭸G⭸y (x,⭸x y) L * dV(y) ⭸G (x, y) ⫹ 冕 ⌬u (y)L n dS(y), ⭸y ⭸x ⬁ im

ijkl kl

V

l

n

⬁ im

i

S

ijkl

j

l

(10.1.24)

n

or ij(x) ⫽ Lklmn* kl ⫹

冕L

冕⌫

klmn

S

⬁ ijmn

⍀

(y, x) dV(y)

⌬uk(y)⌫⬁ijmn(y, x)nl dS(y),

(10.1.25)

where ⌫⬁ijmn(y, x) is deﬁned by (4.3.6). It then follows from (4.3.8) that ij(x) ⫽ *S kl ijkl ⫹

冕L S

klmn

⌬uk(y)⌫⬁ijmn(y, x) nl dS(y),

(10.1.26)

10.1

IMPERFECT INTERFACES

251

where Sijkl is the Eshelby inclusion tensor. Making use of (10.1.4) in (10.1.26) gives ij(x) ⫽ Sijkl* kl ⫹

冕L S

⬁ kppq(y)⌫ijmn (y, x)nqnl dS(y).

klmn

(10.1.27)

Clearly, the ﬁrst term in (10.1.27) is identical to the original Eshelby solution. The effect of imperfect interface comes through the surface integral involving the displacement jump at the interface. Since perfect interface corresponds to ij ⫽ 0, a weakly imperfect interface may be modeled by a very small ij. Thus, (10.1.27) provides a convenient basis for constructing asymptotic solutions for the imperfect interface problem. To this end, we make use of Hooke’s law (3.3.2) in (10.1.27) to obtain ij(x) ⫽ *S kl ijkl ⫺ ⫹

冕L S

冕L S

L

⬁ kpst*⌫ijmn (y, x)nqni dS(y)

L

klmn pqst

klmn pqst

⬁ kpst(y)⌫ijmn (y, x)nqnl dS(y).

(10.1.28)

An iteration procedure can now be formulated, (n) ij (x) ⫽ *S kl ijkl ⫺ ⫹

冕L S

冕L S

L

⬁ kpst*⌫ijmn (y, x)nqnl dS(y)

klmn pqst

⬁ kpst(n⫺1)(y)⌫ijmn (y, x)nqnl dS(y)

L

klmn pqst

for n ⫽ 1, 2, . . . . The initial value can be set to (0) *. ij ⫽ Sijklij

(10.1.29)

The leading order solution for small ij can now be obtained as ij(x) ⬇ (1) ij (x) ⫽ Sijkl* kl ⫹ Zijst(x)(Istkl ⫺ Sstkl)*, kl

(10.1.30)

冕⌫

(10.1.31)

where Zijst(x) ⫽ LklmnLstpq

S

⬁ kp ijmn

(y, x)nqnl dS(y).

252

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

Alternatively, (10.1.30) can also be written as ij(x) ⫽ S M ijkl(x)*, kl

(10.1.32)

SM ijkl(x) ⫽ Sijkl ⫹ Zijst(x)(Istkl ⫺ Sstkl)

(10.1.33)

where

can be viewed as the modiﬁed Eshelby inclusion tensor for an ellipsoidal inclusion with weakly imperfect interface. One signiﬁcant difference of the modiﬁed Eshelby inclusion problem is that the strain within the ellipsoidal inclusion is no longer uniform even though the eigenstrain is. A quantity that will be needed later is the average of the modiﬁed Eshelby tensor SM ijkl(x) ⫽

1 ⍀

冕S ⍀

M ijkl

(x) dV.

(10.1.34)

To carry out the integral, consider

冕Z ⍀

(x) dV ⫽ LklmnLstpq

ijst

⫽ LklmnLstpq ⫽ SijmnLstpq

冕 冋冕 ⌫ (y, x) dV(x)]n n dS(y) 冕 P n n dS(y) 冕 n n dS(y), (10.1.35) S

S

S

kp

kp

⍀

⬁ ijmn

q l

⬁ ijmn q l

mp q n

where (4.3.7) has been used. Making use of the above, the integral in (10.1.34) can be carried out to yield SM ijkl ⫽ Sijkl ⫹ SijmnRmnpqLpqst(Istkl ⫺ Sstkl),

(10.1.36)

where Rmnpq ⫽

1 4⍀

冕 ( S

n n ⫹ mqnpnn ⫹ npnqnm ⫹ nqnpnm) dS(y).

mp q n

(10.1.37) Clearly, we have Rmnpq ⫽ Rnmpq ⫽ Rnmqp ⫽ Rmnqp. Note that Rmnpq depends on the interface properties through ij and the geometry of the

10.1

IMPERFECT INTERFACES

253

inclusion. Expressions of Rmnpq for ellipsoids, cylinders, and spheres are given in Appendix 10.A. Now, we are ready to consider a composite material consisting of randomly oriented and shaped inhomogeneities embedded in a matrix with stiffness tensor L0. Let the stiffness tenors of the inhomogeneities be L1, L2, L3, . . . , LN, as shown in Figure 7.1. We further assume that interfaces between the inhomogeneities and the matrix are not perfect. The interfacial jump condition is given by (10.1.4). We ﬁrst consider the average stress and average strain ﬁelds in the composite. It follows from (5.4.1) and (5.4.2) that the average stress over the entire representative volume element of the composite is ⫽

1 D

冕 dV ⫽ 冘 c , N

r

D

r

(10.1.38)

r⫽0

where r ⫽

1 ⍀r

冕

⍀r

dV

is the average stress on the rth inhomogeneity, while the average strain over the entire representative volume element of the composite is given by ⫽

1 D

冕 dV ⫽ 冘 c ⫹ 2D1 冘 冕 N

N

r r

D

r⫽0

r⫽1

Sr

(⌬u 嘸 n ⫹ n 嘸 ⌬u) dS, (10.1.39)

where Sr is the surface of ⍀r, r is the average stain in the rth inhomogeneity r ⫽

1 ⍀r

冕

⍀r

dV,

(10.1.40)

and the symbol 嘸 indicates a dyad, see Section 1.4. By using the displacement jump condition (10.1.4), the surface integral in (10.1.39) can be written as

冕

Sr

(⌬u 嘸 n ⫹ n 嘸 ⌬u) dS ⫽

冕

Sr

[( 䡠 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 䡠 n)] dS.

(10.1.41)

254

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

The integral is rather difﬁcult to evaluate. So, we will make an ad hoc approximation (Qu, 1993a),

冕

Sr

[( 䡠 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 䡠 n)] dS ⬇

冕

Sr

[( 䡠 r 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 r 䡠 n)] dS,

(10.1.42)

that is, replacing the stress distribution along Sr by the average stress on ⍀r. Clearly, (10.1.42) would be exact if the stress is uniform on ⍀r. The right-hand side of (10.1.42) can be further written as

冕

Sr

[( 䡠 r 䡠 n) 嘸 n ⫹ n 嘸 ( 䡠 r 䡠 n)] dS ⫽ 2⍀r Rrr,

(10.1.43)

where the fourth-order tensor Rr is deﬁned by (10.1.37). Finally, we can write the average strain on the composite as

冘 c ⫹ 冘 cR. N

⫽

N

r r

r

r

r

(10.1.44)

r⫽1

r⫽0

Let us now consider the effective elastic properties of the composite. To this end, let the representative volume element of the composite be subjected to the following traction boundary condition: 䡠 n兩S ⫽ 䡠 n,

(10.1.45)

where is the average stress over the representative volume element of the composite, according to the average stress theorem introduced in Section 5.4 (It can be easily shown that the average stress theorem is still valid in this case). The Mori–Tanaka method assumes that the average strain in the rth inhomogeneity can be written as [see (7.3.5)] r ⫽ 0 ⫹ pt r ,

r ⫽ 1, 2, . . . , N,

(10.1.46)

pt where pt r is the average r perturbance of the strain ﬁeld in the rth inhomogeneity. The corresponding average stress is

r ⫽ Lrr ⫽ Lr(0 ⫹ pt r ),

r ⫽ 1, 2, . . . , N.

(10.1.47)

10.1

IMPERFECT INTERFACES

255

The Mori–Tanaka method further assumes that each inhomogeneity ⍀r (r ⬎ 0) is embedded, in the absence of other inhomogeneities, in a uniform material of stiffness L0, which was prestressed by 0. When the inhomogeneity is simulated by an inclusion with eigenstrain *, r the equivalent inclusion equation becomes (see Section 4.4) r ⫽ Lr(0 ⫹ rpt) ⫽ L0(0 ⫹ rpt ⫺ r*).

(10.1.48)

It is further assumed that M pt r ⫽ S r *, r

(10.1.49)

where S M r is the modiﬁed Eshelby tensor averaged over ⍀r as given by (10.1.36). Substituting (10.1.49) into (10.1.48) yields an equation for r*, which can be solved to obtain M ⫺1 * r ⫽ [(Lr ⫺ L0)S r ⫹ L0] (Lr ⫺ L0)0.

(10.1.50)

The total strain in the rth inhomogeneity can then be written as r ⫽ 0 ⫹ rpt ⫽ 0 ⫹ S rMr* ⫽ TrM 0,

(10.1.51)

M ⫺1 ⫺1 TM r ⫽ [I ⫹ S r L0 (Lr ⫺ L0)] .

(10.1.52)

where

The above derivation is very similar to the steps leading to (7.1.6). The average stress on the rth inhomogeneity then follows from substituting (10.1.51) into (10.1.47), r ⫽ LrTrM 0 ⫽ HrM 0,

(10.1.53)

where M HM r ⫽ LrTr M0

is the local stress concentration tensor; see (7.3.11). Note that, although (10.1.53) was derived for r ⬎ 0, it can be easily see that it is also valid for r ⫽ 0. Making use of (10.1.53) in the average stress leads to

256

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冘 c ⫽ 冘 cH . N

⫽

N

r

r

M r

r

(10.1.54)

0

r⫽0

r⫽0

Consequently,

冉冘 冊

⫺1

N

0 ⫽

.

crHM r

(10.1.55)

r⫽0

Introducing (10.1.55) back to (10.1.53) yields r ⫽ BM r ,

(10.1.56)

where

冉冘 冊

⫺1

N

B ⫽H M r

M r

M r

crH

(10.1.57)

r⫽0

is the global stress concentration tensor; see (7.3.12). It then follows from (10.1.56) that the average strain in the rth inhomogeneity is r ⫽ Mr BrM .

(10.1.58)

Making use of (10.1.56) and (10.1.58) in (10.1.44) yields

冘 c M B ⫹ 冘 c R B . N

⫽

N

r

M r

r

r

M r

r

r⫽1

r⫽0

This immediately leads to

冘 cM B ⫹ 冘 cR B ⫽ c M B ⫹ 冘 c (M ⫹ R )B ⫽ 冋c M ⫹ 冘 c (M ⫹ R )L T M 册冉 冘 c L T M 冊 ⫽ 冋c I ⫹ 冘 c (M ⫹ R )L T 册冉 冘 c L T 冊 . N

N

M⫽

r

M r

r

r

r

M r

r⫽1

r⫽0

N

0

M 0

0

r

r

M r

r

r⫽1

N

0

0

r

r

r

r

0

r

N

0

⫺1

N

r

r⫽1

r

M r

r⫽0

r⫽1

0

⫺1

N

M r

r

r

r

M r

r

r⫽0

r

M r

(10.1.59)

10.1

IMPERFECT INTERFACES

257

This gives the Mori–Tanaka estimate of the effective compliance of the composite material with imperfect interfaces:

冋

冘

册冉冘

N

M ⫽ c0I ⫹

crLrTM r

r⫽0

r⫽1

冊

⫺1

N

cr(Mr ⫹ Rr)LrTM r

.

(10.1.60)

By specifying displacement boundary conditions, one can obtain the effective stiffness tensor; see Problem 10.1:

冉冘 N

L⫽

冊冋

crLrTrM

r⫽0

c0I ⫹

冘

册

⫺1

N

cr(Mr ⫹ Rr)LrTrM

r⫽1

.

(10.1.61)

Obviously, we have LM ⫽ ML ⫽ I.

(10.1.62)

Furthermore, it can be easily veriﬁed that when → 0, we have Rr → 0 and T M r → Tr. Therefore, the effective elastic properties (10.1.59) and (10.1.61) reduce to those of the perfect interface cases (7.3.14) and (7.3.8), respectively. Example 10.1 Consider a composite consisting of an isotropic matrix with L0 and isotropic, spherical particles of L1. The interface between the particles and the matrix is described by the displacement jump condition (10.1.4) where ij ⫽ ␣(␦ij ⫺ ni nj).

(10.1.63)

We are to ﬁnd the effective elastic properties of the composite. Since the materials are isotropic, we may represent them as L0 ⫽ (3K0, 20),

L1 ⫽ (3K1, 21).

(10.1.64)

The composite should also be isotropic, that is, L ⫽ (3K, 2). It follows from Appendix 10.A that R1 ⫽

2␣ (0, 3), 5d

(10.1.65)

where d is the diameter of the particles. The modiﬁed Eshelby tensor is thus given by

258

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

M M SM 1 ⫽ S1 ⫹ S1R1L0(I ⫺ S1) ⫽ (3␥ 0 , 2␦ 0 ),

(10.1.66)

where

冉

冊

(10.1.67)

冊

(10.1.68)

L ⫽ (c0L0 ⫹ c1L1T1M)(c0I ⫹ c1(M1 ⫹ R1)L1T1M)⫺1.

(10.1.69)

M (3␥ M 3␥0, 2␦0 ⫹ 0 , 2␦ 0 ) ⫽

24␣0␦0 (1 ⫺ 2␦0) . 5d

Thus, M ⫺1 ⫺1 TM 1 ⫽ [I ⫹ S 1 L0 (L1 ⫺ L0)]

⫽

冉

K0 0 , . M K0 ⫹ 3␥ M (K ⫺ K ) ⫹ 2 ␦ 0 1 0 0 0 (1 ⫺ 0)

The effective stiffness tensor is obtained from

Carrying out the matrix algebra, we ﬁnally arrive at K ⫽ K0 ⫹ ⫽ 0 ⫹

c1K0(K1 ⫺ K0) , K0 ⫹ 3␥0(1 ⫺ c1)(K1 ⫺ K0)

c10[5d(1 ⫺ 0) ⫺ 12␣01] . 5d0 ⫹ 10d␦ 0M(1 ⫺ c1)(1 ⫺ 0) ⫹ 12c1␣01

(10.1.70)

(10.1.71)

It is seen that the effective bulk modulus is the same as that of the perfect interface case. Only the effective shear modulus is affected by the imperfect interface. It is also noticed that the effective shear modulus depends not only on the volume fraction of the particles but also on the particle size. This is very different from the perfect interface case where only the volume fraction of the particles matters. To close this section, we state two variation principles for composites with imperfect interfaces (Qu, 1993b). The proof of them is straightforward; see Problem 10.2. Principle of Minimum Potential Energy Among all kinematically admissible displacement ﬁelds, the true one makes the following functional minimum:

10.2

⌸(u) ⫽

1 2

冕 :L: dV ⫺ 冕 D

S

u 䡠 䡠 n dS ⫹

1 2

FIBER BRIDGING

冕 ⌬u 䡠

⫺1

⌫

259

䡠 ⌬u dS,

(10.1.72) where S is the portion of the external boundary where traction is prescribed, and ⌫ is the union of all internal interfaces. Principle of Minimum Complimentary Energy Among all statically admissible stress ﬁelds, the true one makes the following functional minimum: ⌸c() ⫽

冕 :M: dV ⫺ 冕 u 䡠 䡠 n dS 1 ⫹ 冕 n 䡠 䡠 䡠 䡠 n dS, 2 1 2

D

Su

⌫

(10.1.73)

where Su is the portion of the external boundary where displacement is prescribed, and ⌫ is the union of all internal interfaces.

10.2

FIBER BRIDGING

Fibers in engineering composites typically have higher elastic modulus than the matrix. Because of this, the effective elastic modulus of the composite is higher than that of the matrix material. In addition to the enhancement of elastic stiffness, ﬁbers can also enhance the fracture toughness of the matrix material. In this section, we will consider a very simple example to illustrate how the ﬁbers in a composite affect the composite’s fracture behavior. Let us consider a unidirectional ﬁber-reinforced composite material. Assume that the matrix has a crack perpendicular to the ﬁber direction, as shown in Figure 10.1. When the composite is subjected to a uniform tensile load ⬁ in the ﬁber direction at inﬁnity, a mode I stress intensity is created at the crack tips, which is characterized by the stress intensity factor KI. According to linear elastic fracture mechanics, the crack may start growing leading to the fracture of the material if the stress intensity factor KI becomes greater than the fracture toughness of the matrix material KIc, that is,

260

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

σ∞

2a

σ∞ Figure 10.1 Unidirectional ﬁber-reinforced composite with Grifﬁth crack.

KI ⱖ KIc.

(10.2.1)

If, under the same given load, KI can be reduced, it effectively improves the fracture toughness of the material. We will see from the following analysis that ﬁbers that bridge the crack surfaces can effectively reduce KI, thus improving the fracture strength of the composite. For simplicity, we will limit ourselves to plane strain deformation, so the crack can be considered as a two-dimensional slit, which is referred to as the Grifﬁth crack in fracture mechanics literature. We further assume that the size of the existing crack in the composite is much greater than the ﬁber diameter. This assumption is valid for most engineering applications where the ﬁber diameter is in the order of micrometers, while the ﬂaw size is typically several hundred micrometers, or millimeters. Under this assumption, the unidirectional ﬁberreinforced composite can be viewed as a homogeneous, transversely isotropic solid as discussed in Section 9.1. To proceed, we ﬁrst transfer the externally applied load ⬁ to the crack surface. A simple linear superposition argument would show that loading on the crack surfaces is equivalent to loading at inﬁnity in that they produce the same stress intensity factors. So, in what follows, we will consider ⬁ being applied on the cracks surface instead of at inﬁnity. If there were no ﬁbers bridging the crack faces, the stress intensity factor of a Grifﬁth crack of length 2a in a homogeneous, transversely

10.2

FIBER BRIDGING

261

isotropic elastic solid subject to normal loading ⬁ on the crack surfaces is given by (see Tada et al., 1985; Qu and Bassani, 1993) dx 冕 冪 兹a ⫺ x .

KI ⫽ 2

a

a

⬁ 2

0

2

(10.2.2)

However, the bridging ﬁbers limit the opening of the crack faces, so the actual (or effective) stress intensity factor at the crack tip is rather different from (10.2.2). In other words, not all the applied stress ⬁ is working to open the crack surfaces. Instead, a portion of the applied stress ⬁ has to stretch the bridging ﬁbers. Or, one may view this in a different way. The bridging ﬁbers exert a stress p(x) on the crack surfaces, which works against the applied stress ⬁ by trying to close the crack. Thus, effectively, the problem at hand is equivalent to a crack without bridging ﬁbers, but the externally applied load is ⬁ ⫺ p(x). Therefore, the actual stress intensity factor should be, following (10.2.2), KI ⫽ 2

dx . 冪 冕 [兹⫺a p(x)] ⫺x a

a

0

⬁

2

2

(10.2.3)

What we need to do next is to ﬁnd p(x). Since the total load is shared between the ﬁbers and the matrix, we have ⬁ ⫽ cƒƒ⬁ ⫹ cm⬁m,

(10.2.4)

where, as deﬁned before, cƒ and cm are the volume fractions of the ﬁber and the matrix, respectively. Away from the crack, the axial stresses in the ﬁber and in the matrix are denoted by ⬁ƒ and m⬁ , respectively. Since the axial strain is the same for both ﬁber and matrix (no gross ﬁber pull-out), one must have ⬁ƒ ⬁ ⫽ m ⫽ ⬁, Eƒ Em EL

(10.2.5)

where, again, Eƒ and Em are the Young moduli of the ﬁber and matrix, respectively, while EL is the effective Young modulus of the unidirectional ﬁber-reinforced composite in the ﬁber direction. Combining (10.2.4) and (10.2.5) yields the stress in the ﬁber

262

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

⬁ƒ ⫽

⬁Eƒ , cmEm(1 ⫹ )

(10.2.6)

Eƒcƒ . Emcm

(10.2.7)

where ⫽

This is the axial stress in the ﬁber far away from the crack (or when the crack is absent). We now consider the axial stress in the ﬁber near the crack faces. Shown in Figure 10.2 is a representative element near the crack faces containing one ﬁber. The center of the ﬁber is x distance away from the center of the crack. Due to geometric singularities, the stresses near the intersection of the ﬁber and crack surfaces are very high. It is perceivable that certain portions of the ﬁber–matrix interface had failed and sliding between the ﬁber and matrix had occurred. We assume that the length of the sliding region is l and the shear stress on the interface due to friction is denoted by (assume it is a constant). Outside the sliding area, the axial stress in the ﬁber is given by (10.2.6). Within the sliding area, the axial stress in the ﬁber can be obtained by balancing the axial stress in the ﬁber and the shear stress on the ﬁber surface due to friction, ƒ(z) ⫽ ƒ⬁ ⫹

2b 2 z ⫽ ƒ⬁ ⫹ z, 2 b b

(10.2.8)

where b is the ﬁber radius. According to Hooke’s law, the strain in the ﬁber follows from (10.2.8),

l(x)

z

x

2v(x)

Fiber

2b

Matrix

Figure 10.2 Representative element of crack surfaces r distance from crack center.

10.2

ƒ(z) ⫽

FIBER BRIDGING

⬁ƒ 2 ⫹ z. Eƒ bEƒ

263

(10.2.9)

Integration of (10.2.9) with respect to z leads to the total elongation of the ﬁber within the sliding area

冕

冉

l(x)

2⌬ƒ(x) ⫽ 2

0

ƒ(z) dz ⫽ 2

冊

⬁ƒ l(x) ⫹ l(x). Eƒ bEƒ

(10.2.10)

The factor 2 in the above equation comes from the fact that the sliding area is symmetric with respect to the crack plane. We now consider the matrix surrounding the ﬁber. Analogous to (10.2.8), we assume that the stress in the matrix within the sliding area is also a linear function of z. Further, the axial stress in the matrix must be zero on the crack surfaces. Thus, we write

冋

m(z) ⫽ 1 ⫺

册

z ⬁ . l(x) m

(10.2.11)

The corresponding strain thus follows:

冋

册

⬁m z 1⫺ . Em l(x)

m(z) ⫽

(10.2.12)

Consequently, integration of (10.2.12) gives the axial elongation of the matrix within the sliding area

冕

l(x)

2⌬m(x) ⫽ 2

m(z) dz ⫽

0

⬁ml(x) . Em

(10.2.13)

Comparing (10.2.10) and (10.2.13), we have the total crack opening displacement

冋

2v(x) ⫽ 2⌬ƒ(x) ⫺ 2⌬m(x) ⫽ 2

册

⬁ƒ l(x) ⬁ l(x) ⫹ l(x) ⫺ m . Eƒ bEƒ Em

(10.2.14)

Substituting (10.2.6) into (10.2.14) yields the following crack opening displacement:

264

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

v(x) ⫽

冋

册

l(x) ⬁ ⫹ l(x). bEƒ 2(Eƒcƒ ⫹ Emcm)

(10.2.15)

This can also be solved to obtain the length of the sliding zone, l(x) ⫽

⬁b 4(1 ⫹ )cƒ

冋冪

1⫹

册

16(1 ⫹ )2Eƒc2ƒv(x) ⫺1 . 2 ⬁2 b

(10.2.16)

Clearly, for the ﬁber at the crack tip, the crack opening displacement is zero, that is, v(a) ⫽ 0. It thus follows from (10.2.16) that l(a) ⫽ 0. That means that the ﬁbers outside the cracked area do no show any pull-out, which is consistent with our intuition. If we now substitute (10.2.16) back to (10.2.8), we can calculate the stress exerted on the crack surface by the bridging ﬁbers: p(x) ⫽ cƒƒ(l) ⫽

⬁ 2(1 ⫹ )

冋冪

1⫹

册

16(1 ⫹ )2Eƒc2ƒv(x) ⫹1 . 2 ⬁2 b (10.2.17)

Note that p(x) is positive. It represents the stress carried by the bridging ﬁbers over the cracked area. One may also view p(x) as the stress acting on the crack surface trying to close the crack opening by working against the externally applied load ⬁. Equation (10.2.17) is a relationship between p(x) and v(x). For convenience, let us recast (10.2.17) into a nondimensional form: p(x) ⫽ ⬁ 2(1 ⫹ )

冋冪

1⫹

册

4(1 ⫹ )(x) ⫹1 , 20

(10.2.18)

where 0 ⫽

2⬁b . 4(1 ⫹ )Eƒc2ƒ

(10.2.19)

Since p(x) ⱕ ⬁, it can be easily shown from (10.2.18) that (x) ⱕ 0. Shown in Figure 10.3 is the relationship between the bridging force p(x) and the parameter ⫽ Eƒcƒ /Emcm for various crack opening displacement values. It is seen that as increases (either higher ﬁber

10.2

265

FIBER BRIDGING

1.0 0.8

p( x) 0.6 σ∞

v( x) v0 = 0.2 v( x) v0 = 0.4 v( x) v0 = 0.6

0.4 0.2 0.0 0.0

0.5

1.0

1.5

η

2.0

2.5

3.0

Figure 10.3 Relationship between bridging force and ⫽ Eƒcƒ / Emcm.

modulus, or more ﬁbers, or both), the bridge forces increase as well. Higher crack opening displacement also causes higher bridging forces. For a given crack, the crack opening displacement is typically highest near the center of the crack. Therefore, that is where the bridging force is the highest. Higher bridging means higher stress in the bridging ﬁber. So, conceivably, some of the ﬁbers near the center of the crack may break. Such a situation has been studied by a number of investigators (e.g., Cui, 1992; Xia et al., 1994; Budiansky and Cui, 1995). As discussed earlier, the problem at hand is equivalent to a crack in a homogeneous, transversely isotropic solid subject to normal pressure ⬁ ⫺ p(x). The crack opening displacement in this case is given by (see, e.g., Qu and Bassani, 1993)

(r) ⫽

2D

冕 [

冏

a

0

⬁

⫺ p(t)]log

2D ⫽ 2D⬁兹a ⫺ x ⫺ 2

2

兹a2 ⫺ x2 ⫹ 兹a2 ⫺ t2 兹a2 ⫺ x2 ⫺ 兹a2 ⫺ t2

冏

dt

冕 p(t)log冏兹a ⫺ x ⫺ 兹a ⫺ t 冏 dt, a

0

兹a2 ⫺ x2 ⫹ 兹a2 ⫺ t2 2

2

2

2

(10.2.20) where

266

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

D⫽

冪冉A 2A 冊冉2A 2A 11

22

12

⫹ A66

⫹

11

A11 ⫽

1 ⫺ 2 , ET

22

(10.2.21)

11

A22 ⫽

(1 ⫹ ) A12 ⫽ ⫺ TT , EL

冪AA 冊,

EL ⫺ 2ET , E 2L

A66 ⫽

1 . L

(10.2.22)

In deriving the above expressions, it has been assumed that ƒ ⫽ m ⫽ . The other engineering constants EL, ET, and L, and TT are deﬁned in Section 9.1. They are related to the elastic properties of the ﬁber and matrix through the formulas discussed in the same section. Substituting (10.2.17) into (10.2.20) yields an integral equation for the crack opening displacement. Numerical methods are needed to obtain the solution to the integral equation. Once the crack opening displacement (x) is solved, the pressure p(x) can be evaluated from (10.2.17). Once p(x) is known, linear elastic fracture mechanics dictates that fracture may occur when KI ⫽ 2

dx ⫽K . 冪 冕 [兹⫺a p(x)] ⫺x a

a

0

⬁

2

2

Ic

(10.2.23)

Since p(x) is positive, the stress intensity factor calculated from (10.2.23) is lower than the case without ﬁber bridging. Therefore, the bridge ﬁber effectively increases the fracture toughness of the composite.

10.3

TRANSVERSE MATRIX CRACKS

Transverse matrix cracking is one of the most common damage mode in cross-ply laminates. It has been observed in both ceramic matrix and polymer matrix composites that the evolution of transverse matrix cracking shows two distinct stages. When tensile stress is applied in the ﬁber direction of the 0⬚ ply, cracks are formed in the 90⬚ ply at a load level much lower than the ultimate strength of the laminate. These transverse matrix cracks are tunneling cracks in that they almost instantaneously run through the entire specimen width and the thickness

10.3

TRANSVERSE MATRIX CRACKS

267

of the 90⬚ ply but arrest at the 0⬚ /90⬚ ply interfaces. As the load further increases, more transverse cracks are initiated. At some critical load, the number of cracks ceases to increase; instead, the existing cracks may penetrate into the adjacent 0⬚ layers and eventually fracture the 0⬚ ﬁbers (for ceramic matrix composite CMCs), or divert into the 0⬚ /90⬚ ply interfaces (for polymer matrix composite PMCs). Catastrophic failure becomes imminent when the 0⬚ ﬁbers are broken. In what follows, we will develop a micromechanics model for the onset and subsequent multiplication of transverse cracks in the 90⬚ layers at the ﬁrst stage of damage evolution based on the Grifﬁth fracture criterion. The cross section of a typical ﬁber-reinforced cross-ply laminate is schematically shown in Figure 10.4. For convenience, the following convention is adopted here. The layers with vertical ﬁbers in the y direction are called 0⬚ layers (or plies) and the layers with ﬁbers perpendicular to the page (in the z direction) are called 90⬚ layers (or plies). It is assumed that the cross-ply laminates have equal distribution of 0⬚ and 90⬚ plies. The effective modulus of the ﬁber-reinforced cross-ply laminate shown in Figure 10.4 has been studied in Section 9.2. What we will need here is the plane-strain Young modulus in the y direction of the uncracked cross-ply laminate; see (9.2.40): E0 ⫽

(EL ⫹ ET)2 ⫺ 4E 2L 2TL , 2(EL ⫹ ET)(1 ⫺ LTTL)

0 ⫽

2EL , EL ⫹ ET TL

y

x 2

1

z

Figure 10.4 Cross section of cross-ply laminate.

(10.3.1)

268

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

where TL LT, EL, and ET are the effective engineering elastic constants of the unidirectional ﬁber-reinforced composite. These engineering elastic constants can be related to the Young moduli of the ﬁber and the matrix materials as discussed in Chapter 9. If we assume further that the Poisson ratios for the ﬁber and the matrix are the same, that is, m ⫽ ƒ ⫽ , the above equations reduce to E0 ⫽

(EL /ET ⫹ 1)2 ⫺ 4 2(EL /ET)2 ET, 2(EL /ET ⫹ 1)(1 ⫺ 2)

0 ⫽ .

(10.3.2)

It is obvious from (9.1.58) to (9.1.64) that the ratio EL /ET depends only on the ﬁber volume fraction c and the ratio ⫽ Eƒ /Em. Therefore, one can conclude that, besides a common factor Em, for a cross-ply laminate with equal number of 0⬚ and 90⬚ plies of equal thickness, the effective elastic properties depend only on , , and c. As the matrix cracks multiply, the effective stiffness of the composite decreases. We will use a differential scheme to estimate the effective modulus as a function of the crack density. The idea is based on the notion of incremental construction of the strain energy by introducing one crack at a time in the 90⬚ layer. Suppose that at a given crack density ƒ in the 90⬚ layer, the composite is homogenized with effective Young’s modulus Ec(ƒ), where the dependence of Ec on the crack density is explicitly indicated. The fundamental assumption of the differential method is that when an additional crack is introduced in the 90⬚ layer, the change of strain energy due to this addition is the energy released from the formation of the new crack. To this end, consider a pair of 0⬚ and 90⬚ layers in the cross-ply laminate as shown in Figure 10.5. Assume that there are N cracks in the 90⬚ layer (material 1) within the height L. Let the representative element be subjected to an applied strain in the y direction. Then, at this given crack density, the total strain energy in this pair of layers can be written as U(ƒ) ⫽ –12 Ec(ƒ) 2(4t)L,

(10.3.3)

where h⫽

L . 2N

(10.3.4)

When an additional crack is introduced, the crack density becomes

10.3

2t

2t

2

1

TRANSVERSE MATRIX CRACKS

269

σ

2h

L

σ

Figure 10.5 Transverse matrix cracks in cross-ply laminate under uniaxial loading.

ƒ1 ⫽

t , h1

h1 ⫽

L

. 2(N ⫹ 1)

(10.3.5)

The total strain energy at this crack density becomes U(ƒ1) ⫽ –12 Ec(ƒ1) 2(4t)L.

(10.3.6)

Based on the differential scheme, the difference between (10.3.3) and (10.3.6) is the energy released due to one transverse crack given by

再冕

1 U(ƒ1) ⫺ U(ƒ) ⫽ ⫺ 2 2

t

⫺t

冎

(x)␦(x) dx ,

(10.3.7)

where ␦(x) is the crack opening displacement deﬁned by ⌬(x) ⫽ uy(x, 0⫹) ⫺ uy(x, 0⫺)

for ⫺t ⱕ x ⱕ t.

(10.3.8)

Note that the right-hand side of (10.3.7) is the energy released when a crack is formed in the laminate with effective Young’s modulus Ec(ƒ). Therefore, the stress (x) in the 90⬚ layer (prior to the formation of this crack) should be uniform and given by

270

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

冋

(x) ⫽ 2Ec(ƒ) ⫺

册

EL , 1 ⫺ 2ET /EL

(10.3.9)

where EL is the longitudinal (ﬁber direction) modulus of the individual layers. Substituting (10.3.9) into the right-hand side of (10.3.7) yields

冋

U(ƒ1) ⫺ U(ƒ) ⫽ ⫺ 2Ec(ƒ) ⫺

册

EL 2t⌬, 1 ⫺ 2ET /EL

(10.3.10)

where ⌬ is the average crack opening displacement deﬁned by ⌬⫽

1 2t

冕

t

⫺t

⌬0(x) dx,

(10.3.11)

and ⌬0(x) is the crack opening displacement due to a unit applied strain ﬁeld, that is, ⌬0(x) ⫽

⌬(x) .

(10.3.12)

Since ⌬(x) can be calculated by the ﬁnite-element method for given , ⌬0(x) can then be obtained through linear superposition from (10.3.12). Next, consider the left-hand side of (10.3.10). It follows from (10.3.3) and (10.3.6) that U(ƒ1) ⫺ U(ƒ) ⫽ 2 2 Lt[Ec(ƒ1) ⫺ Ec(ƒ)].

(10.3.13)

On the other hand, making use of (10.3.4) and (10.3.5) yields L⫽

2t

. ƒ1 ⫺ ƒ

(10.3.14)

Substitution of (10.3.14) into (10.3.13) gives U(ƒ1) ⫺ U(ƒ) ⫽ 4 2t2

[Ec(ƒ1) ⫺ Ec(ƒ)] . ƒ1 ⫺ ƒ

(10.3.15)

Obviously, in the limiting of ƒ1 → ƒ, (10.3.15) can be written as a differential equation:

10.3

TRANSVERSE MATRIX CRACKS

U(ƒ1) ⫺ U(ƒ) ⫽ 4 2t2

dEc(ƒ) . dƒ

271

(10.3.16)

Combining (10.3.10)–(10.3.16) yields

冋

册

dEc ⌬ EL ⫽⫺ 2Ec(ƒ) ⫺ . dƒ 4t 1 ⫺ 2ET /EL

(10.3.17)

In addition to (10.3.17), Ec(ƒ) should also satisfy the initial condition that when there is no crack (ƒ ⫽ 0), Ec(0) ⫽ E0.

(10.3.18)

Equations (10.3.17) and (10.3.18) form an initial value problem for the effective Young modulus of the composite. The solution to the initial value problem (10.3.17) and (10.3.18) is given by (Qu and Hoiseth, 1998)

再 冉 冊

冋

冉 冊册冎

ƒ⌬ EL ƒ⌬ Ec(ƒ) ⫽ E0 exp ⫺ ⫹ 1 ⫺ exp ⫺ 2t EL ⫹ ET 2t

.

(10.3.19)

It is seen that this solution approaches the theoretical limit Ec(ƒ) EL → , E0 ET ⫹ EL

(10.3.20)

as ƒ → ⬁ in which only the 0⬚ layers carry the load. It is seen from (10.3.19) that once ⌬, the crack opening displacement of a single crack in an inﬁnitely long (h/t → ⬁) specimen, is known, the effective elastic modulus of the laminate with any crack density can be predicted. Shown in Figure 10.6 is the predicted Young modulus Ec as a function of crack density ƒ for c ⫽ 0.55 and various values of . The solid lines are the analytical solution from (10.3.19), and the symbols are the exact solutions from the ﬁnite-element method (Qu and Hoiseth, 1998). It is found that for the wide range of materials considered, the maximum difference between the ﬁnite element and the analytical solutions is less than 5 percent. The effective Young modulus given by (10.3.19) can only give the stiffness as a function of crack density. To predict the effective (overall) stress–strain behavior, damage (cracking) evolution must be modeled.

272

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

1.0

0.9 Ef /Em = 30 0.8

Ec /E0

Ef /Em = 20 0.7 Ef /Em = 10 0.6

ν = 0.3, c = 0.55

0.0 0.0

Ef /Em = 5

0.5 1.0 1.5 2.0 Transverse Crack Density, f

2.5

Figure 10.6 Effective Young’s modulus. Lines are from the analytical solution and symbols are from the ﬁnite-element solutions.

To this end, a fracture criterion is required. Once a fracture criterion is established, solutions of crack density can be obtained as a function of the applied strain . As the cross-ply laminate is loaded in the y direction, transverse cracks develop in the 90⬚ layers. Assume the transverse cracks initiate as tunneling cracks, namely, they span the entire 90⬚ ply and propagate in the width direction of the laminate (the z direction). Then, based on linear elastic fracture mechanics, the energy released due to the formation of a new tunneling crack can be written as (Hutchinson and Suo, 1991), Gss(ƒ) ⫽

1 4t

冕

t

⫺t

(x)⌬(x) dx,

(10.3.21)

where ⌬(x) is the crack opening displacement given in (10.3.11) and (x) ⫽ y(x, 0), that is, the normal stress on the crack line prior to cracking. Note that both ⌬(x) and (x) depend on the crack density ƒ. Therefore, Gss is a function of ƒ. Through simple dimensional analysis, the energy release rate can be written as

10.3

TRANSVERSE MATRIX CRACKS

Gss(ƒ) ⫽ 2tE0g(, , c, ƒ),

273

(10.3.22)

where is the applied strain, E0 is the overall plane strain Young modulus for the uncracked composite deﬁned in (10.3.2), and g(, , c, ƒ) is the nondimensional energy release rate. The energy release rate Gss(ƒ) can also be related to the effective stiffness through the principle of conservation of energy. To develop such a relationship, consider a specimen containing N cracks in the 90⬚ layer. It follows from the conservation of strain energy that (Qu and Hoiseth, 1998) 1 1 Nt Ec(ƒ) 2(2hNt) ⫽ E0 2(2hNt) ⫺ G (ƒ), 2 2 2 ss

(10.3.23)

where 2hN is the height of the specimen (thickness is unit). Substituting (10.3.22) into (10.3.23) yields

冋

g(, , c, ƒ) ⫽ 1 ⫺

册

Ec(ƒ) 2 , E0 ƒ

(10.3.24)

where Ec is the effective Young modulus determined in the previous section. Making use of (10.3.24) gives the steady-state energy release rate for tunneling cracks

冋

冉 冊册

Gss(ƒ) 2ET ␦ƒ ⫽ g(, , c, ƒ) ⫽ 1 ⫺ exp ⫺ 2 tE0 (EL ⫹ ET)ƒ 2t

.

(10.3.25)

An interesting limit of (10.3.25) as ƒ → 0 is Gss(0) ⫽

ET 2␦ E0. ET ⫹ EL

(10.3.26)

This can also be obtained directly from (10.3.21) by using (10.3.9) and (10.3.11). Next, consider a 90⬚ layer with an existing set of transverse matrix cracks of density ƒ. Assume that a new set of cracks bisecting the existing set is in the process of tunneling across the layer; see Figure 10.7. The energy released by the cracks in the process of tunneling is (Hutchinson and Suo, 1991)

274

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

2h

New Cracks 2t

Figure 10.7 Multiplication of transverse matrix cracking in cross-ply laminate.

2Gss(2ƒ) ⫺ Gss(ƒ).

(10.3.27)

Then, based on the Grifﬁth energy criterion in linear elastic fracture mechanics, a new set of cracks will be initiated if the following equation is satisﬁed: G (2) c ⫽ 2Gss(2ƒ) ⫺ Gss(ƒ),

(10.3.28)

where G (2) is the plane strain mode I toughness of the 90⬚ layer c (material 2). Substituting (10.3.26) into (10.3.28) yields G c(2) ⫽

冋 冉 冊

冉 冊册

2 2tE0ET ␦ƒ ␦ƒ exp ⫺ ⫺ exp ⫺ (EL ⫹ ET)ƒ 2t t

.

(10.3.29)

Equation (10.3.29) is the desired evolution equation for the crack density ƒ as a function of the applied strain . For ⫽ 0.3, c ⫽ 0.55, the crack density ƒ as a function of 兹tE0 /G (2) c is plotted in Figure 10.8 for ⫽ 1, 5, 10, 20, 30. Figure 10.9 presents a comparison between the theoretical predictions and the experimental data for crack density versus applied load. The experimental data is from Varna and Berglund (1991). The tested material is an AS/3501-06 carbon ﬁber–epoxy [02 /902]s laminate. In the numerical calculations, no adjustment parameters are used. All material constants are taken directly from Varna and Berglund (1991). It is seen that the predicted crack density versus load curve (dotted line) has the same trend as the experimental one but is slightly shifted to the right. This may be attributed to many factors. Chief among them

10.3

TRANSVERSE MATRIX CRACKS

275

1.0

Transverse Crack Density, f

0.8

0.6

0.4

Ef /Em = 1 Ef /Em = 5 Ef /Em = 10 Ef /Em = 20 Ef /Em = 30

0.2

0.0 0

1

2

3

4

5

ε E0t Gc( 2 )

Figure 10.8 Crack density vs. applied strain.

AS/3501-60 [02/902]s 2.0 (2)

2

Theoretical Prediction (Gc = 104 J/m ) (2) 2 Theoretical Prediction (Gc = 130 J/m ) Experimental Data

Crack Density f

1.5

1.0

0.5

0.0 0.0

0.5

1.0

1.5

2.0

Applied Stress s 0 (GPa)

Figure 10.9 Comparison between experimental and analytical results for crack density vs. applied load.

276

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

is the fact that the model is based on the assumption that the laminate contains an inﬁnite number of layers, while the experimental data were obtained for a [02 /902]s laminate. Since the model predicts the trend correctly, a simple parameter adjustment can be done in practical applications to correlate the prediction with the measurement. For example, in the case considered here, by reducing the toughness of the 2 90⬚ layer in the direction of the ﬁber from G(2) c ⫽ 130 J/m as reported (2) 2 in Varna and Berglund (1991) to Gc ⫽ 104 J/m , the model predicts excellent agreement with the experiments as shown by the solid line in Figure 10.10. Note that, in the limit of ƒ → 0, Eq. (10.3.29) becomes G (2) c ⫽

2␦ E0ET . ET ⫹ EL

(10.3.30)

Thus, the threshold strain at which transverse matrix cracking starts to occur is th ⫽

冪

G (2) c (ET ⫹ EL) . ␦ E0ET

(10.3.31)

4

E f /E m = 1 E f /E m = 5

3

E f /E m = 1 0

σ

E f /E m = 2 0

E 0 G c( 2 ) t

E f /E m = 3 0 2

1

0 0

1

2

ε E 0t G

3 (2) c

Figure 10.10 Effective stress–strain curves.

4

277

APPENDIX 10.A

Now, consider the effect of matrix cracking on the overall stress–strain behavior. To begin the calculation, the threshold strain th is obtained from (10.3.31) for the given composite system. Then, the strain is increased gradually. For each value of ⬎ th, the corresponding crack density ƒ is computed from (10.3.29). Substituting this value of ƒ into (10.3.19) yields the corresponding effective Young modulus at this given strain. Finally, the stress (ƒ) corresponding to this strain is evaluated from (ƒ) ⫽ Ec(ƒ)(ƒ).

(10.3.32)

For ⫽ 0.3, c ⫽ 0.55, the overall stress–strain curves for various values of are presented in Figure 10.10. Note that these curves are invariant to G(2) c because of the normalization. PROBLEMS

10.1 Consider a composite material consisting of randomly oriented and shaped inhomogeneities embedded in a matrix with stiffness tensor L0. Let the stiffness tenors of the inhomogeneities be L1, L2, L3, . . . , LN, as shown in Figure 7.1. We further assume that interfaces between the inhomogeneities and the matrix are not perfect. The interfacial jump condition is given by (10.1.4). Find the effective stiffness tensor of this composite. 10.2 Prove the two variational principles stated in Section 10.1. APPENDIX 10.A

By substituting (10.1.5) into (10.1.36), we obtain the following: Rijkl ⫽ ␣Pijkl ⫹ ( ⫺ ␣)Qijkl

(10.A.1)

with Pijkl ⫽

冕 冋冕

册

2 3 d (␦iknˆ j nˆ l ⫹ ␦jknˆ i nˆ l ⫹ ␦ilnˆ j nˆ k ⫹ ␦jlnˆ i nˆ k) 0 16 0 n ⫻ sin d, (10.A.2)

Qijkl ⫽

3 4

冕 冋冕

2

0

0

册

nˆ i nˆ j nˆ k nˆ l d sin d, n

(10.A.3)

278

BRITTLE DAMAGE AND FAILURE OF ENGINEERING COMPOSITES

where n ⫽ 兹nˆ i nˆ i, nˆ ⫽

冉

(10.A.4)

冊

sin cos sin sin cos , , . a1 a2 a3

(10.A.5)

For spheres (a1 ⫽ a2 ⫽ a3 ⫽ a), we have n ⫽ 1/a. Thus, Pijkl ⫽

1 I , a ijkl

Qijkl ⫽

1 (2I ⫹ ␦ij␦kl). 5a ijkl

(10.A.6)

For cylinders (a1 ⫽ a2 ⫽ a, a3 → ⬁), the non-zero components are P1111 ⫽ P2222 ⫽ 4P2323 ⫽ 4P1313 ⫽ 2P1212 ⫽

3 , 8a

(10.A.7)

Q1111 ⫽ Q2222 ⫽ 3Q2323 ⫽ 3Q1313 ⫽ 3Q1212 ⫽

9 . 32a

(10.A.8)

REFERENCES Achenbach, J. D. and H. Zhu. (1989). Effects of Interfacial Zone on Mechanical Behavior and Failure of Fiber-Reinforced Composites, J. Mech. Phys. Solids, Vol. 37, pp. 381–393. Budiansky, B. and Y. Cui. (1995). Toughening of Ceramics by Short Aligned Fibers, Mech. Mater., Vol. 21, pp. 139–146. Cui, Y. (1992). Interaction of Fiber and Transformation Toughening, J. Mech. Phys. Solids, Vol. 40, pp. 1837–1850. Hutchinson, J. W. and Z. Suo. (1991). Mixed Mode Cracking in Layered Materials, Adv. Appl. Mech., Vol. 29, pp. 62–191. Mura, T. (1987). Micromechanics of Defects in Solids, Martinus Nijhoff, Boston. Qu, J. (1993a). Eshelby Tensor for an Elastic Inclusion with Slightly Weakened Interface, J. Appl. Mech., Vol. 60, pp. 1048–1050. Qu, J. (1993b). Effects of Slightly Weakened Interfaces on the Overall Elastic Properties of Composite Materials, Mech. Mater., Vol. 14, p. 269–281. Qu, J. and J. L. Bassani. (1993). Interfacial Fracture Mechanics for Anisotropic Bimaterials, J. Appl. Mech., Vol. 60, pp. 422–431.

SUGGESTED READINGS

279

Qu, J. and K. Hoiseth. (1998). Evolution of Transverse Matrix Cracking in Cross-Ply Laminates, Int. J. Fatigue Fracture Eng. Mater. Structures, Vol. 21, pp. 451–464. Tada, H., P. Paris, and G. R. Irwin. (1985). The Stress Analysis of Cracks Handbook, Del Research, St. Louis. Varna, J., and L. A. Berglund. (1991). Multiple Transverse Cracking and Stiffness Reduction in Cross-Play Laminates, J. Composites Tech. Res., JCTRER, Vol. 27, pp. 99–106. Xia, Z. C., J. W. Hutchinson, A. G. Evans, and B. Budiansky. (1994). On Large Scale Sliding in Fiber-Reinforced Composite, J. Mech. Phys. Solids, Vol. 42, pp. 1139–1158.

SUGGESTED READINGS Budiansky, B. and J. W. Hutchinson. (1986). Matrix Fracture in FiberReinforced Ceramics, J. Mech. Phys. Solids, Vol. 34, pp. 167–189. Christensen, R. M. (1979). Mechanics of Composite Materials, Wiley, New York. Hashin, Z. (1985). Analysis of Cracked Laminates: A Variational Approach, Mech. Mater., Vol. 4, pp. 121–136. Hoiseth, K. and J. Qu. (2003). Cracking Paths at the Ply Interface in a CrossPly Laminate, Composites Part B: Engr., Vol. 34, pp. 437–445. Laws, N. and D. J. Dvorak. (1988). Progressive Transverse Cracking in Composite Laminates, J. Composite Mater., Vol. 22, pp. 900–916. Xia, Z. C., R. R. Carr, and J. W. Hutchinson. (1993). Transverse Cracking in Fiber-Reinforced Brittle Matrix, Cross-Ply Laminates, Acta Metall., Vol. 41, pp. 2365–2376.

11 MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR In previous chapters, we have assumed that all the inhomogeneities in the heterogeneous material behave linear elastically. Therefore, the overall behavior of the heterogeneous material is also linear elastic. For linear elastic behavior, the effective stiffness tensor is usually sufﬁcient to fully characterize the stress–strain relationship, or the material’s response under load. If one or more of the inhomogeneities in a heterogeneous medium behave nonlinearly (nonlinear elastic, viscoelastic, elastoplastic, elastoviscoplastic, etc.), the overall behavior, or the effective properties of the heterogeneous medium, will not be linear elastic. Unlike the effective stiffness and compliance for linear materials, the effective properties of nonlinear heterogeneous materials are much more complex to model and characterize. The main difﬁculty is the typical strong intraphase ﬂuctuations of the stress and strain ﬁelds in nonlinear heterogeneous materials and in the hereditary nature of most inelastic behaviors. At a given length scale, the responses of the inhomogeneities can vary markedly at different load levels. For example, a two-phase elastoplastic composite material effectively behaves as a multiphase material, and phase averages have less predictive capabilities than in the linear elastic case. In this chapter, we will develop a general framework based on the mean ﬁeld theories to describe the nonlinear behavior of heterogeneous media. Historically, the mean ﬁeld theory for inelastic behavior was developed mainly for crystalline materials initially. The early knowledge acquired through physical metallurgical studies of the plastic behavior 280

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

281

of single crystals leads naturally to a certain interest in their extension to polycrystals, where the main challenge is to relate the mechanical response of an aggregate of crystals (known as a polycrystal) to the fundamental mechanisms of single-crystal deformation. Speciﬁcally, the problem of predicting the yield stress of a polycrystal as a function of the yield strength of the constituent single crystals was considered by Sachs (1928) and studied more extensively later by Taylor (1938), whereas Schmid and Boas (1935) originated their fundamental law regarding the crystallographic slip within single crystals. Note that these earlier theoretical frameworks are speciﬁc to crystal plasticity and are formulated within a context closer to physical metallurgy than to mechanics of materials. More rigorous mechanistic analysis was carries out by Bishop and Hill (1951), who generalized the Taylor model to describe the different loading paths and to show their extreme features for the yield stress of polycrystalline materials. Subsequently, the development of metal forming processing and related plastic anisotropy problems resulting from texture evolutions provided the driving force in extending the Taylor model to more accurate approaches. In 1957, Eshelby introduced the concept of eigenstrains. The plastic deformation in each single crystal can be simulated by an eigenstrain distribution. Thus, the same homogenization techniques for linear elasticity can be followed to describe the nonlinear behavior of polycrystalline materials. This way of thinking was ﬁrst adopted by Budiansky and Mangasarian (1960) and developed later by Kro¨ner (1961). Their work constitutes the fundamental basis of the self-consistent mean ﬁeld theories for nonlinear behavior of heterogeneous materials. Unlike the Sachs and Taylor models, the self-consistent framework ensures both the compatibility and equilibrium conditions across the grains interface in polycrystalline aggregate. However, as discussed later, Kro¨ner’s model is limited to spherical inhomogeneities and isotropic matrix with incompressible plasticity. The next breakthrough was made by Hill (1965), who adopted the same concept as Kro¨ner (in the sense of Eshelby) by introducing an original idea of describing the plastic ﬂow by a sequence of linearizations leading to an incremental procedure of homogenization. In Hill’s approach, the overall behavior of the polycrystal, as well as the behavior of each grain, is approximated by a ‘‘pseudo’’-elastic behavior at each loading increment. Therefore, plastic unloading is accounted for. However, the nonlinear material behavior, compounded by the nonuniformity of stress and strain ﬁelds, renders the linearized properties nonuniform in each phase. This constitutes the major difﬁculty in using the Hill model without appropriate approximations.

282

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

The treatment of this difﬁculty was the center of different investigations leading to the emergence of mean ﬁeld theories with different varieties of linearization sequences of the nonlinear behavior. Within these procedures, one can distinguish between the secant, the tangent, and afﬁne approaches. The classical secant formulation was developed by Berveiller and Zaoui (1979) for crystalline materials and adapted later by Tandon and Weng (1988) to the case of two-phase elastoplastic composite materials. The secant formulation, which can be viewed as an intermediate method between the Kro¨ner approach and the incremental method of Hill, reduces signiﬁcantly the complexity of the Hill model by assuming isotropic homogeneous plastic ﬂow in each phase. The ﬁrst tangent mean ﬁeld method was introduced by Hutchinson (1976) to describe steady-state creep behavior of crystalline materials. It turns out that Hutchinson’s use of the power law creep also leads to another variant of the secant method (see below). More recently, Molinari et al. (1987) derived a tangent formulation for viscoplastic power law by adopting a sequence of linearization similar to linear thermoelasticity. All of these self-consistent methods rely on the assumption of piecewise uniform properties so that the Eshelby inclusion solution could be combined with the linearization procedure to obtain the overall nonlinear properties. However, for most nonlinear behavior such as plastic ﬂow, the ﬁelds ﬂuctuate in each phase and their heterogeneity increases (e.g., with the plastic ﬂow) at each loading increment. This makes it difﬁcult to assess the predictive capabilities of these self-consistent methods and to select the accurate one. Such limitation was the main motivation behind the development of the variational principles for nonlinear behaviors in the mid-1990s. Variational approaches for elastic and viscoelastic composites (Willis, 1983; Talbot and Willis, 1985; Castan˜eda, 1991; Suquet, 1993) combined with a linearization procedure enable us to compare some nonlinear mean ﬁeld theories to rigorous bounds of the Hashin– Shtrikman type. It turned out (Gilormini, 1997) that both tangent and secant approaches lead to estimates that are too stiff and can even violate the bounds in some cases. Different ways of thinking have emerged recently to overcome this deﬁciency of the mean ﬁeld theories. Improvements can be made by modifying the secant approach to take into account a better description of stress and strain ﬂuctuations at the microscale level. A ﬁrst attempt in this direction was made for particulate-reinforced composite by Qiu and Weng (1992). It uses the average strain energy in the matrix to

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

283

deﬁne its effective stress. Under this theory, the results are valid only for incompressible materials. A more general theory valid for arbitrary microstructure and compressible matrix has been developed by Suquet (1995). It was based on the second-order moments in each individual phase of the linear comparison solid. The use of second order moments has also been adopted independently by Hu (1996) and Buryachenko (1996). Another variety of the second-order estimates has been proposed by Castan˜eda (1996). It was based on Taylor’s second-order developments of stress, strain, and resulting potentials. An alternative in extending mean ﬁeld theories to secant formulation plasticity has been introduced by Dvorak (1992) using the transformation ﬁeld theory. The methodology models the plastic ﬂow of multiphase materials by a uniform piecewise distribution of eigenstrains. Such approaches are in principle suitable for use as micromechanically based constitutive laws in ﬁnite element codes. They are also very attractive in terms of computational requirements but tend to strongly overestimate the nonlinear overall response of heterogeneous materials because they essentially use elastic accommodation of microstress and strains throughout the loading history. In this chapter, several varieties of self-consistent mean ﬁeld theories will be discussed in details. Illustrative results for face-center-cubic (FCC) elastoplastic polycrystalline materials using an incremental selfconsistent scheme at small strains will be presented.

11.1

¨ NER’S MODEL ESHELBY’S SOLUTION AND KRO

As discussion above, the ﬁrst attempts made in modeling the elastoplastic behavior of polycrystalline materials through a homogenization scheme had their principal inspiration from the Eshelby inclusion solution in linear elasticity. The idea of liking these two problems came from two considerations. First of all, it is possible to describe the plastic strain of each individual grain by a distribution of eigenstrains (or stress-free strain) as introduced by Eshelby. Second, the interactions between a typical grain and its surrounding grains can be simulated by an inclusion problem of a single inhomogeneity undergoing a stressfree plastic strain while being surrounded by an equivalent homogeneous elastoplastic medium with appropriate boundary conditions. To introduce Kro¨ner’s model, let us consider a representative volume element of a polycrystalline material of total volume D comprised of N single crystals. It is assumed that D is much larger than the volume

284

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

of each crystal in the representative volume element of the polycrystal aggregate so that N ⬎⬎ 1. The representative volume element may be subjected to either the traction boundary condition • n兩S ⫽ • n

(11.1.1)

or the rate form of displacement boundary condition u˙ 兩S ⫽ ˙ • x,

(11.1.2)

where S is the surface of D and n is the outward unit normal of S. The overdot indicates the rate, or increment. Note that the rate here is typically not the change with respect to time. Instead, it is the change (or increment) with respect to the load. According to the average stress and average strain theorems introduced in Section 5.4, the volume averages of stress and strain tensors are ⫽

1 D

冕 dV, D

˙ ⫽

1 D

冕 ˙ dV.

(11.1.3)

D

For the sake of simplicity, we will consider in this chapter smallstrain deformation only. Therefore, it is possible to decompose the total strain and total strain rate into elastic and plastic parts, that is, ⫽ e ⫹ p,

˙ ⫽ ˙ e ⫹ ˙ p,

(11.1.4)

where e and p are the elastic and plastic parts of the strain tensor, respectively. The volume averages of strain and strain rate tensors can be decomposed similarly: ⫽ e ⫹ p,

˙ ⫽ ˙ e ⫹ ˙ p.

(11.1.5)

Note that, as discussed in Section 3.1, neither the elastic strain e nor the plastic strain p is compatible by itself, although the sum of these two ﬁelds is compatible. In other words, there is no, for example, such displacement ﬁeld uei such that eij ⫽ (ui,e j ⫹ uej,i)/2.

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

11.1

285

As discussed in Section 3.1, the elastic strain is related to the total stress through Hooke’s law, ⫽ Le ⫽ L( ⫺ p).

(11.1.6)

Single-phase polycrystals can be viewed as an assembly of essentially the same single crystals of different orientations and sizes. Therefore, an ensemble average of a ﬁeld quantity can be deﬁned as the average over all single crystals; see Section 5.3. For example, the ensemble averages of the stress and strain tensors are

冘 c ,

冘 c ,

N

具典 ⫽

r

r

N

具典 ⫽

r r

(11.1.7)

r⫽1

r⫽1

where cr is the volume fraction of the rth crystal in the polycrystal assembly D. As discussed in Section 5.3, we consider only statistically homogeneous media in this book. Therefore, the volume average and ensemble average of a ﬁeld quantity should be the same, for example, ⬅

⬅

1 D

冕 dV ⫽ 具典 ⬅ 冘 c ,

(11.1.8)

1 D

冕 dV ⫽ 具典 ⬅ 冘 c .

(11.1.9)

N

r

D

r

r⫽1 N

D

r r

r⫽1

Similarly, ˙ ⫽ 具典 ˙ ,

˙ ⫽ 具˙ 典.

(11.1.10)

However, due to the interphase incompatibilities of the elastoplastic strain ﬁelds, the elastic and plastic strain tensors by themselves may not be ergodic, that is, e ⫽ 具e典,

p ⫽ 具p典,

˙ e ⫽ 具˙ e典,

˙ p ⫽ 具˙ p典.

(11.1.11)

To illustrate these, let us assume that the representative volume element D is subjected to the traction boundary condition (11.1.1). In the absence of body forces (so assumed for the rest of this chapter), the total stress ﬁeld must satisfy

286

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

ⵜ⫽0

in D

(11.1.12)

n兩S ⫽ n.

(11.1.13)

and

Next, let e be the stress ﬁeld in D induced by the traction boundary condition (11.1.1) when all the single crystals in the polycrystal assembly D are linear elastic, that is, ⵜ e ⫽ 0

in D

(11.1.14)

e n兩S ⫽ n.

(11.1.15)

and

Clearly, the above equations imply that e is a statically admissible stress ﬁeld for the polycrystal assembly D subjected to the traction boundary condition (11.1.1), even when plastic deformation occurs. Further, since (11.1.14) and (11.1.15) describe a pure linear elastic problem, it then follows from (11.1.9) that e ⫽ ⫽ 具典 ⫽ 具 e典.

The strain ﬁeld corresponding to e can be written as ij ⫽ –12 (uei, j ⫹ uei, j) ⫽ Mijklekl,

(11.1.16) (11.1.17) (11.1.18)

where uei is the displacement ﬁeld when all the single crystals in the polycrystal assembly D behave linear elastically. Note that this ij is typically not the elastic part of the total strain ﬁeld eij introduced in (11.1.4), that is, ij ⫽ eij. Conceivably, e and are different because of plastic deformation that occurred in D. So, we introduce the plastic residual stress ﬁeld by p ⫽ ⫺ e

or ⫽ e ⫹ p.

(11.1.19)

It is so named because p represents the stress ﬁeld remained in the plastically deformed polycrystal assembly D after elastic unloading ( e ⫽ 0). Further, it follows from (11.1.16) that

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

p ⫽ 具 p典 ⫽ 0.

287

(11.1.20)

Equations (11.1.12)–(11.1.15) also imply that ⵜ p ⫽ 0

in D

(11.1.21)

and p n兩S ⫽ 0.

(11.1.22)

We call such stress ﬁeld self-equilibrium stress ﬁeld. Note that generally e ⫽ Le,

(11.1.23)

⫽ e ⫽ Le.

(11.1.24)

although

These can be seen from (11.1.6) and (11.1.19). Now, consider again the linear elastic problem. The stress ﬁeld in the rth single-crystal ⍀r can be written as er ⫽ Br

in ⍀r

(11.1.25)

where Br is the local elastic stress concentration tensor introduced in (5.7.9), which can be determined approximately by the homogenization schemes developed in Chapter 7. Note that

冘 c ⫽ 冘 c B ⫽ 冘 c B 具典 ⫽ 冘 c B 具 典. N

具 典 ⫽ e

N

r

r⫽1

e r

N

N

e

r

r

r⫽1

r

r

r

r⫽1

r

r⫽1

(11.1.26)

Thus,

冘 c B ⫽ I. N

具Br典 ⫽

r

r

r⫽1

Substituting (11.1.25) into the second of (11.1.19) yields

(11.1.27)

288

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

r ⫽ Br ⫹ rp

in ⍀r .

(11.1.28)

It then follows from the decomposition (11.1.4) that 具BT典 ⫽ 具BTe典 ⫹ 具BTp典,

(11.1.29)

具BT典 ⫽ 具MB典 ⫹ 具BTp典.

(11.1.30)

or

In deriving (11.1.30), we have substituted the elastic strain by using Hooke’s law in terms of elastic compliance M. The diagonal symmetry of M allows us to replace BT with B. In (11.1.30), we can show easily that the ﬁeld MB is kinematically admissible. Thus, application of the Hill lemma to 具MB典 yields 具MB典 ⫽ 具典具MB典 ⫽ M ⫽ e,

(11.1.31)

where M ⫽ 具MB典 is the effective elastic compliance of the polycrystalline material. On the other hand, since BT is statically admissible, one can write 具BT典 ⫽ 具BT典 ⫽ 具典 ⫽ ,

(11.1.32)

where (11.1.27) has been used. By combining (11.1.29), (11.1.31), and (11.1.32), one can conclude that e ⫽ 具BTe典 ⫽ 具e典,

p ⫽ 具BTp典 ⫽ 具p典.

(11.1.33)

The same statement can be made for the rates, ˙ e ⫽ 具BTe典 ⫽ 具˙ e典,

˙ p ⫽ 具BT˙ p典 ⫽ 具˙ p典.

(11.1.34)

Based on the foregoing discussions, one can derive some interesting and well-known features of crystalline materials.

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

289

Stored Elastic Strain Energy

The total elastic strain energy stored in D is given by U⫽

1 2

冕 dV. e

(11.1.35)

D

Making use of (11.1.6) and (11.1.19), we can rewrite this as

冕 M dV ⫽ 12 冕 ( ⫹ )M( ⫹ ) dV 1 1 ⫽ 冕 M dV ⫹ 冕 M dV ⫹ 冕 M dV. 2 2

U⫽

1 2

e

D

p

e

p

D

e

e

p

D

e

p

D

p

D

(11.1.36) Note that the ﬁrst term on the right-hand side is the strain energy in an elastic body. Thus, it follows from the discussions in Section 5.6 that

冕 M e

D

e

dV ⫽ DeMe ⫽ DM.

(11.1.37)

The second integral is

冕 M p

D

e

dV ⫽

冕 D

p ij

ij dV ⫽

冕 u

p e ij i, j

D

dV ⫽

冕 u n dV ⫽ 0, S

p e ij i j

(11.1.38) where we have used (11.1.18), (11.1.21), and (11.1.22). Thus, the strain energy stored in D when subjected to the traction boundary condition (11.1.13) is given by U⫽

D 1 M ⫹ 2 2

冕 M p

p

dV.

(11.1.39)

D

We see that the stored elastic strain energy contains, in addition to the macroscopic strain energy resulting from the applied load, a contribution from the plastic residual stresses.

290

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

Dissipated Energy

The dissipated energy due to plasticity, or the stress power from plasticity, is deﬁned as [see (2.3.5)] W⫽

1 2

冕 ˙ dV. p

D

Making use of the strain decomposition, this can be rewritten as W⫽

1 2

冕 ˙ dV ⫺ 12 冕 ˙ dV. e

D

(11.1.40)

D

It follows from the Hill lemma (5.5.5) that the ﬁrst term on the righthand side of (11.1.40) can be written as

冕 ˙ dV ⫽ D˙ ⫽ D D

e

⫹ D p .

(11.1.41)

Following the same arguments used in deriving the strain energy, the second term on the right-hand side of (11.1.40) can be written as

冕 ˙ dV ⫽ 冕 M˙ dV ⫽ D˙ ⫹ 冕 M˙ e

D

e

D

p

p

dV.

(11.1.42)

D

Hence D 1 ˙ p ⫽ W ⫹ 2 2

冕 M˙ p

D

p

dV ⫽

1 2

冕 ˙ dV ⫹ 21 冕 M˙ p

D

p

p

dV.

D

(11.1.43) This clearly shows that the macroscopic plastic stress power D˙ p is not completely dissipative. The ﬁrst term on the right-hand side of (11.1.43) is dissipative, while the second term resulting from the plastic residual stress is stored in the material. This contribution may explain the ‘‘interphase’’ work hardening observed in polycrystalline materials (see below).

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

291

Interphase Work Hardening

Following the same procedure used in calculating the dissipation energy, one can easily obtain the following: D 1 ˙ ˙ p ⫽ 2 2

冕 ˙ ˙ dV ⫹ 12冕 ˙ M˙ p

p

D

p

dV.

(11.1.44)

D

If all the single crystals in the polycrystal assembly behave as elastic perfectly plastic materials (without work hardening), then the plastic ﬂow of each crystal can be described using the normality rule as ˙ ˙ p ⫽ ˙ ƒ˙ ⫽ 0

in D,

where ƒ() is the yield surface and ˙ is the well-known plastic parameter. Therefore, we have D 1 ˙ ˙ p ⫽ 2 2

冕 ˙ M˙ p

D

p

dV ⱖ 0

(11.1.45)

because M is positive deﬁnite. Clearly, one can conclude from the inequality (11.1.45) that the macroscopic or homogenized behavior of polycrystal assembly display work hardening during its plastic ﬂow even though all of its single crystals are perfectly plastic. In other words, the inhomogeneity of the material is one of the sources of its work hardening. Such prediction has been conﬁrmed experimentally for polycrystalline materials. For example, for most single crystals, there is very little work hardening during the early stage (easy glide region) of deformation. However, during this stage, the polycrystal experiences a signiﬁcant work hardening due to the intergranular interactions among the single crystals. In general, a nonlinear heterogeneous material can be considered as a standard generalized material (in the sense of thermodynamics) by deﬁning appropriate internal variables, state variables, and associated thermodynamic forces. Such formulation requires an inﬁnite number of internal variables (e.g., the plastic strain ﬁeld), which renders such a procedure not feasible for practical situations. This is why nonlinear heterogeneous materials require suitable approximations to model their overall behavior. The modeling of nonlinear behavior in inhomoge-

292

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

neous materials is still a challenging issue and has not been solved completely yet.

Kro¨ner’s Approach

The modeling of elastoplastic behavior of polycrystalline materials by the concept of Eshelby’s elastic solutions was initiated by Budiansky and Mangasarian (1960). Their original idea was to model the ﬁrst stage of the plastic deformation so that Eshelby’s elastic inclusion solution is applicable without any major modiﬁcations. They argued that the favorably oriented grains that ﬁrst experience a plastic deformation can be simulated by an ellipsoidal inclusion subjected to stress-free plastic strain (eigenstrain) in interaction within an elastic inﬁnite medium representing the other grains that are still at the elastic regime. This approximation is also supported by the fact that the number of grains undergoing plastic deformation is low at the earlier stage of the plastic ﬂow, and hence the homogenization procedure can be performed by the dilute approximation. In other words, the interactions between the plastically deformed grains can be neglected. Subsequently, Kro¨ner, who initiated the self-consistent scheme in elasticity, proposed a similar formulation that enables us to describe the elastoplastic behavior beyond the earlier stages of the plastic ﬂow. Unlike Budiansky’s approach, Kro¨ner considered the inﬁnite medium in the Eshelby scheme as the ‘‘unknown’’ homogeneous medium subjected to an average p at a certain stage of the plastic ﬂow. To solve the interaction or localization problem for a given set of grains subjected to uniform plastic strain p, whereas the polycrystals as a whole is plastically deformed by p, Kro¨ner’s approximation adopts the Eshelby solution by describing the set of grains by an ellipsoidal inclusion subjected to an eigenstrain p and surrounded by an inﬁnite medium, which in turn is subjected to a uniform deformation p. One of the limitations of Kro¨ner’s model is that the framework was developed based on isotropic and spherical grains, and incompressible plasticity. Let us ﬁrst consider a homogeneous elastic matrix of stiffness L and volume D, subjected to a uniform strain . Let ⍀r be an ellipsoidal inclusion embedded within the matrix. It goes without saying that ⍀r ⬍⬍ D. To simulate the plasticity, let pr be an eigenstrain ﬁeld distributed in ⍀r . According to the Eshelby inclusion solution, the total strain on the inclusion is given by

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

r ⫽ ⫹ Srrp

in ⍀r ,

293

(11.1.46)

where Sr is the Eshelby inclusion tensor for ⍀r . This gives pr ⫽ Sr⫺1(r ⫺ )

in ⍀r .

(11.1.47)

The total stress ﬁeld in the inclusion is thus given by [see (4.3.22)] r ⫽ L(r ⫺ pr )

in ⍀r .

(11.1.48)

Substituting (11.1.46) into (11.1.48) gives r ⫽ L ⫹ L(Sr ⫺ I)rp ⫽ ⫹ L(Sr ⫺ I)rp,

(11.1.49)

where ⫽ L is the stress tensor averaged over the entire polycrystal assembly D. Recall that Eshelby’s tensor Sr depends on the elastic stiffness tensor L and the shape and orientation of the inclusion. Therefore, in its general form, (11.1.49) is capable of capturing the plastic anisotropy resulting from morphological aspects related to the irregular shape of grains. As mentioned above, Kro¨ner initially considered the case of spherical inclusions in isotropic matrix. Under such conditions, one has [see (2.4.23)] L ⫽ 3KIh ⫹ 2Id,

Sr ⫽ 3␥Ih ⫹ 2␦Id,

(11.1.50)

where ␥⫽

K 3K ⫹ 4

⫽

1⫹ , 9(1 ⫺ )

␦⫽

3(K ⫹ 2) 4 ⫺ 5 ⫽ , 5(3K ⫹ 4) 15(1 ⫺ ) (11.1.51)

K and are, respectively, the bulk and shear moduli, and is the Poisson ratio of the isotropic matrix material. The symbolic notation introduced in Section 1.4 has been used for isotropic fourth-order tensors. Thus, we have

294

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

L(Sr ⫺ I) ⫽ 3K(3␥ ⫺ 1)Ih ⫹ 2(2␦ ⫺1)Id.

(11.1.52)

The incompressibility of the plastic deformation means Ihpr ⫽ 0.

(11.1.53)

Thus, substituting (11.1.52) into (11.1.49) yields r ⫽ ⫹ 2(2␦ ⫺ 1)Idpr .

(11.1.54)

To describe the plastic ﬂow, (11.1.54) should be written in a rate or incremental form, that is, ˙r ⫽ ˙ ⫹ 2(2␦ ⫺1)Id˙ rp.

(11.1.55)

Substituting the second of (11.1.47) into (11.1.55), we arrive at ˙r ⫽ ˙ ⫹

(2␦ ⫺ 1) d I (˙r ⫺ ˙ ). 2␦

(11.1.56)

Equation (11.1.56) relates local quantities ˙ r and ˙ r to the macroscopic quantities ˙ and ˙ . It constitutes the ﬁrst step for a homogenization scheme crucial for an accurate prediction of the macroscopic behavior. It is clearly seen from (11.1.56) that the interaction between the different quantities is purely elastic. This results from the description of the plastic strain as an eigenstrain leading to a purely heterogeneous elastic problem. In reality, however, during the plastic ﬂow, constraints exerted by the aggregate on a single grain become softer than in the elastic regime and change with the plastic deformation. Since the Kro¨ner model is based on elastic constraints that remain elastic during the plastic ﬂow, it will result in stiffer predictions of the overall behavior. Let us now introduce the instantaneous or tangent modulus of the polycrystal Lt and the tangent modulus of the single-crystal Lt through ˙ ⫽ Lt˙ ,

˙ r ⫽ Lrt ˙ r .

(11.1.57)

Substituting (11.1.57) into (11.1.56) leads to

冋

Ltr ⫺

or

册 冋

册

(2␦ ⫺ 1) d (2␦ ⫺ 1) d I ˙ r ⫽ Lt ⫺ I ˙ 2␦ 2␦

(11.1.58)

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

11.1

˙ r ⫽ Ar˙ ,

295

(11.1.59)

where

冋

Ar ⫽ Lrt ⫺

册 冋

(2␦ ⫺ 1) d I 2␦

⫺1

Lt ⫺

册

(2␦ ⫺ 1) d I 2␦

(11.1.60)

deﬁnes the strain rate concentration tensor. Substitution of (11.1.60) into the second of (11.1.57) leads to

冘 c ˙ ⫽ 冘 L A ˙ . N

˙ ⫽

N

r

t r

r

(11.1.61)

r

r⫽1

r⫽1

One can then conclude that

冘LA N

L ⫽ t

t r

(11.1.62)

r

r⫽1

or

冘L 冋 N

L ⫽ t

t r

r⫽1

册 冋 ⫺1

(2␦ ⫺ 1) d L ⫺ I 2␦ t r

Lt ⫺

册

(2␦ ⫺ 1) d I . 2␦

(11.1.63)

Equation (11.1.63) inherits the implicit character of the selfconsistent scheme as is the case in linear elasticity. Clearly the nonlinearity is captured in (11.1.63) since the local tangent modulus depends on the plastic strain p. If we further assume that the instantaneous tangent modulus tensor is also isotropic, that is, Ltr ⫽ 3KtrIh ⫹ 2trId,

Lt ⫽ 3KtIh ⫹ 2tId,

(11.1.64)

then t r

L

冋

册 冋

(2␦ ⫺ 1) d L ⫺ I 2␦ t r

⫽ 3KtrIh ⫹

⫺1

Lt ⫺

2tr[4␦t ⫺ (2␦ ⫺ 1)] d I. 4␦tr ⫺ (2␦ ⫺ 1)

Making use of this in (11.1.63) gives us

册

(2␦ ⫺ 1) d I 2␦

(11.1.65)

296

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

[4␦ ⫺ (2␦ ⫺ 1)] . 冘 c 4␦ ⫺ (2␦ ⫺ 1) N

t ⫽

r

t r

t

t r

r⫽1

(11.1.66)

To see some insight of the Kro¨ner model prediction, we consider the case tr ⬍⬍ ,

t ⬍⬍ .

(11.1.67)

This is approximately true for later stages of plastic deformation. Under this assumption, (11.1.66) reduces to

冘 c. N

t ⬇

r

t r

(11.1.68)

r⫽1

This last equation is the Taylor–Lin bound, which is equivalent to the Voigt model in linear elasticity. In fact, the Taylor–Lin model (Taylor, 1938; Payne et al. 1958) assumes homogeneous strain in the polycrystalline aggregate so that ⫽ . Therefore, the effective tangent modulus predicted by the Taylor–Lin model simply leads to (11.1.68). Treating the interactions between grains as elastic instead of elastoplastic is one of the major limitations of the Kro¨ner model. Additionally, the consistency attributed to the Kro¨ner approach is not really true since in his procedure the equivalent homogeneous medium is taken to be elastic even though with assigned plastic deformation. These shortcomings are taken into consideration in the Hill selfconsistent model to be discussed next. In closing this section, we mention that although the Kro¨ner model presented here is in terms of a summation over all the single crystals, the results can be easily recast into integral forms (ensemble average), as discussed in Section 7.5. Hill’s Self-Consistent Model

To solve the nonlinear elastoplastic deformation, Hill proposed solving successive linear problems at each loading increment. To accomplish this, Hill introduced the following local and global constitutive laws: ˙ r ⫽ Lrt ˙ r ,

˙ ⫽ Lt˙ ,

(11.1.69)

where Ltr is the tangent modulus of the rth grain, Lt is the effective tangent modulus of the polycrystal assembly, and ˙ r and ˙ r are, re-

11.1

ESHELBY’S SOLUTION AND KRO¨NER’S MODEL

297

spectively, the stress and strain rates averaged over the rth grain, while ˙ and ˙ are, respectively, the stress and strain rates averaged over the entire polycrystal assembly. The inverse of these equations are ˙ r ⫽ Mrt ˙ r,

˙ ⫽ Mt ˙,

(11.1.70)

where Mtr is the tangent compliance of the rth grain and Mt is the effective tangent compliance tensor of the polycrystal assembly. To solve for Lt, we assume that the rth grain in the polycrystal assembly is simulated by an ellipsoidal inclusion ⍀r embedded in a homogeneous matrix with effective modulus tensor Lt, which is yet to be determined. As in the linear elastic case, such self-consistent approach accounts for, at least partially, the interactions between the grains. Making use of the rate form of (4.5.19), we have ˙r ⫽ ˙ ⫹ Hr(˙ ⫺ ˙ r),

(11.1.71)

where the concentration tensor Hr is given by [see (4.5.13)] Hr ⫽ Lt(S⫺1 ⫺ I). r

(11.1.72)

In the above, Sr is the Eshelby inclusion tensor computed for the inclusion ⍀r embedded in a matrix with elastic stiffness tensor Lt. It depends on the shape of ⍀r and on the overall property Lt. Note that, although (11.1.71) and (11.1.72) are similar to the linear elastic case, the effective property to be determined here is the effective tangent modulus of the heterogeneous material, not the effective elastic modulus. Substituting (11.1.69) into (11.1.71), one obtains (Ltr ⫹ Hr)˙r ⫽ (Lt ⫹ Hr)˙.

(11.1.73)

From this equation, the average strain rate on the rth grain is expressed in terms of the macroscopic strain rate as ˙ r ⫽ Ar˙ ,

(11.1.74)

Ar ⫽ (Lrt ⫹ Hr)⫺1 (Lt ⫹ Hr),

(11.1.75)

where

298

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

is the strain rate concentration tensor in elastoplastic deformation, which depends on the effective tangent modulus and geometrical aspects of the grain in consideration ⍀r . Similarly, making use of (11.1.70) in (11.1.71) gives the average stress rate on the rth grain in terms of the global stress rate, ˙ r ⫽ Br ˙,

(11.1.76)

Br ⫽ (H⫺1 ⫹ Mtr)⫺1 (H⫺1 ⫹ Mt). r r

(11.1.77)

where

It then follows from (11.1.74)–(11.1.76) and (11.1.69) and (11.1.70) that

冘 c ˙ ⫽ 冘 c L ˙ ⫽ 冘 c L A ˙ ,

(11.1.78)

冘 c ˙ ⫽ 冘 c M ˙ ⫽ 冘 c M B ˙ .

(11.1.79)

N

˙ ⫽

N

r

r

r

r⫽1

r⫽1

N

˙ ⫽

N

t r r

N

r r

t r

r

N

r

t r

r

r⫽1

r⫽1

r

r⫽1

r

t r

r

r⫽1

These lead to

冘cLA, N

Lt ⫽

r

r⫽1

t r

r

冘 c MB . N

Mt ⫽

r

t r

r

(11.1.80)

r⫽1

The last two equations are the Hill self-consistent scheme to evaluate the effective tangent modulus and effective tangent compliance tenors of a polycrystal assembly. Note that the second of (11.1.80) requires that the tangent compliance tensor Mt for each grain to exist. When this is the case, one can show that (see Problem 11.6) LtAr ⫽ BrLt and MtBr ⫽ ArMt.

(11.1.81)

This leads to ML ⫽ LM ⫽ I; see Problem 11.6. Therefore, it is sufﬁcient to solve either the ﬁrst or the second of (11.1.80). In practice, the ﬁrst of (11.1.80) is more widely used because Mt is not always well deﬁned for all single crystals for a given polycrystal assembly.

11.2

APPLICATIONS

299

As discussed in Section 7.5, (11.1.80) can be cast into an integral form. We will not repeat the discussion here. Readers are encouraged to formulate (11.1.80) into an integral form on their own. Note that (11.1.80) reduces to the self-consistent estimates (7.5.13) and (7.5.14) if the tangent modulus and tangent compliance tensors are replaced by their corresponding elastic stiffness and compliance tensors. This implies that the linear elastic behavior is a special case of the Hill model for elastoplastic behavior. Generally, (11.1.80) gives more accurate results in comparison with Kro¨ner’s model because Hill’s model captures at least partially the ﬂuctuations of strains between each grain. However, the Hill model is still an approximation because of the use of piecewise uniform mechanical properties on each grain. Therefore, any intraphase ﬂuctuation arising naturally from the elastoplastic behavior is disregarded in this approach. It should also be noted that obtaining Lt from (11.1.80) is not an easy task. This is due to the implicit nature of the equation and the anisotropy of the linearized constitutive laws (11.1.69), which makes the calculation of the Hill constraint tensors a complicated task. In general, the determination of Lt through (11.1.80) requires an iterative procedure. First, for a given state of deformation, an initial guess of Lt is used on the right hand of (11.1.80) to calculate an improved value for Lt. Then, this improved Lt is substituted back into the right-hand side of the equation again to obtain the next improvement. This procedure is repeated sufﬁciently until a convergent value is obtained for Lt. Another major difﬁculty behind the Hill self-consistent model is related to how the effective tangent modulus Lt depends on the prescribed values of strain rate ˙ . Unlike in the single-crystal case where only a ﬁnite number of branches exist, for polycrystals Lt varies continuously as the direction of prescribed strain rate varies in the strain rate space. In other words, Lt is a homogeneous function of degree zero of ˙ (Hutchinson, 1970). In practice, additional assumptions are usually made regarding the anisotropy of the tangent modulus in order to simplify the calculations. Examples of this will be discussed in the next section.

11.2

APPLICATIONS

The main purpose of this section is to explore the feasibility using the Hill self-consistent method to predict stress–strain behavior of poly-

300

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

crystalline materials from the elastoplastic properties of single-crystal constituents. We will focus on FCC metallic materials by presenting brieﬂy the main features of plastic deformation at the continuum level of single crystals under conventional loading conditions of strain rates and temperature. Our attention is not to describe exhaustively the various mechanisms of plastic deformation from a physical metallurgy point of view, for such a purpose the readers are referred to more specialized textbooks and technical papers that are recommended at the end of this chapter. Instead, we will follow a mechanistic procedure to bridge the scales between the single-crystal level and the polycrystalline level. Plastic Deformation of Single Crystals

The physical understanding of single-crystal plasticity was established during the earlier years of the last century, in 1900 to 1938, with the contribution of Ewing and Rosenhain (1900), Bragg and Bragg (1933), Taylor and co-workers (1923, 1925, 1934, 1938), Polanyi (1922), Schmid and Boas (1935), among others. Their experimental measurements established that at room temperature the major source of plastic deformation is the dislocation movements through the crystal lattices. These motions occur on certain crystal planes in certain crystallographic directions, and the crystal structure of metals is not altered by the plastic ﬂow. Mathematical descriptions of these physical phenomena of plastic deformation in single crystals were presented by Taylor (1938), when he investigated the plastic deformation of polycrystalline materials in terms of single-crystal deformation. More rigorous and rational formulations were given by Hill (1965), Hill and Rice (1972), Asaro and Rice (1977), and by Hill and Havner (1982). A comprehensive review of this subject can be found in Azaro (1983). The kinematics of single-crystal deformation and the resulting elastoplastic constitutive laws are based on an idealization of dislocation motion as a collective movement of the atoms leading to slips in certain directions on speciﬁc crystallographic planes. This process occurs when the resolved shear stress on one or more of these slip systems reaches a critical value. As plastic deformation proceeds, the critical yield stresses associated with the slip systems increases. This contributes to the strain hardening of the polycrystalline aggregate. Consider a single crystal with N possible slip systems. Each system g is characterized by the unit normal ng to the slip plane on which the collective movement of dislocations occurs, and by the direction mg of

11.2

APPLICATIONS

301

dislocation gliding, which is colinear with the Burger vector bg of gliding dislocations on the system g, so that bg ⫽ bmg, where b is the magnitude of the Burger vector. The mathematical tool treating the collective movement of dislocations considers each dislocation line as the boundary of a cutting surface Sg with a unit normal ng, across which the discontinuities of the displacement vector are uniform and characterized by the Burger vector bg so that bgi ngi ⫽ 0. This transformation can be described at each material point by a second-order tensor p(r) as pij(r) ⫽ bgi ngj ␦(Sg),

(11.2.1)

where ␦(Sg) is the surface Dirac function given by ␦(Sg) ⫽

冕

Sg

␦(r ⫺ r) dS⬘.

(11.2.2)

If many dislocations with the same Burger vector bg and the same cutting surfaces are present in the single-crystal volume V, one can deﬁne an average transformation p by pij ⫽ bmgi ngj

1 V

冕 ␦(S ) dV. g

(11.2.3)

V

Introducing the average plastic shear ␥ g by ␥g ⫽ b

1 V

冕 ␦(S ) dV g

(11.2.4)

pij ⫽ ␥ gmgi ngj .

(11.2.5)

V

leads to

If we account for all dislocations present at the slip systems, (11.2.5) can be extended to pij ⫽

冘␥mn. g

g g i j

g

The shear rate ␥˙ g is calculated from (11.2.4) as

(11.2.6)

302

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

␥˙ g ⫽ b

⭸ ⭸t

再

1 V

冕 ␦(S ) dV冎. g

(11.2.7)

V

Equation (11.2.7) describing the creation and movement of dislocations at the continuum level corresponds to the Orowan relation. The rate of plastic distortion ˙ p is the sum of the contributions of the shear rates ␥˙ g from all the active slip systems. That is ˙ pij ⫽

冘 ␥˙ m n . g

g g i j

(11.2.8)

g

The symmetric part of the plastic distortion gives the plastic strain rate ˙ pij ⫽

1 ˙p ( ⫹ ˙ pji) ⫽ 2 ij

冘 ␥˙ R , g

g ij

(11.2.9)

g

where Rgij ⫽ –12 (mgi ngj ⫹ mgj ngi ).

(11.2.10)

The antisymmetric part of the plastic distortion deﬁnes the plastic spin, w ˙ pij ⫽

1 ˙p ( ⫺ ˙ jip) ⫽ 2 ij

冘 ␥˙ R˜ , g

g ij

(11.2.11)

g

where R˜ gij ⫽ –12 (mgi ngj ⫺ mgj ngi ).

(11.2.12)

˜ g are also called the orientation The second-order tensors Rg and R tensors because they depend only on the orientation of the single crystal in consideration. Let denote the stress in the single crystal. The so-called resolved shear stress on a slip system g is given by

g ⫽ ij Rgij.

(11.2.13)

Within the framework of time-independent plasticity (any viscous effect is neglected), a slip system g is considered to be active if the resolved shear stress g reaches a critical value gc , which depends on

11.2

APPLICATIONS

303

the previous deformation history of the single crystal, leading to a strain hardening state. It is generally assumed that the deformation history of a given slip system g depends on only the amplitude of shear strain associated with N active systems, so that one can write gc ⫽ F˜ g (␥1, ␥2, . . . , ␥ N).

(11.2.14)

When the amount of shear is small enough, we can use a linear approximation of (11.2.14), gc ⬇ F˜ g (0, 0, . . . , 0) ⫹

冘 ⭸⭸␥F˜ (0, 0, . . . , 0)␥ , g

h

h

h

(11.2.15)

where F˜ g (0, 0, . . . , 0) can be viewed as the initial critical shear stress of the slip system g. It is generally assumed the same for all slip systems. Therefore, (11.2.15) can be expressed as gc ⫽ 0 ⫹

冘H ␥ gh

h

(11.2.16)

h

where 0 ⫽ F˜ g (0, 0, . . . , 0), and Hgh ⫽ ⭸F˜ g / ⭸␥ h (0, 0, . . . , 0) is the strain hardening matrix, which describes the hardening interactions between the different slip systems. Note that the diagonal components of the matrix Hgh deﬁne the self-hardening due to the plastic shear in the same system, while the nondiagonal components correspond to the latent hardening due to shear slip on the other systems. The matrix coefﬁcients can be evaluated by experimental characterization performed on single crystals. At any stage of the deformation process, the rate of changes of critical shear stress is deduced from (11.2.16) as ˙ gc ⫽

冘 H ␥˙ . gh

h

(11.2.17)

h

It follows from the above deﬁnitions that a slip system is potentially active if g ⫽ gc and loading or unloading, respectively, depending on whether ˙ g ⫽ ˙ gc

or

with ␥˙ g ⱖ 0

(11.2.18)

304

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

˙ g ⬍ ˙ gc

with ␥˙ g ⫽ 0.

(11.2.19)

A system is inactive if g ⬍ cg and ␥˙ g ⫽ 0. Relation (11.2.17) is known as the consistency condition whose resolution for each active system g determines the shear rate ␥˙ g on this system. Taking into account (11.2.13) and (11.2.18), the consistency condition writes ˙ ijRijg ⫽

冘 H ␥˙ . gh

h

(11.2.20)

h

From the deﬁnition (11.2.9) of the plastic strain rate, the total strain rate is the sum of the elastic and plastic parts, that is, ˙ ⫽ ˙ e ⫹ ˙ p ⫽ L⫺1 ˙ ⫹

冘 ␥˙ R g

g

(11.2.21)

g

or

冉

˙ ⫽ L ˙ ⫺

冘 ␥˙ R 冊. g

g

(11.2.22)

g

Note that for a given state of stress , ˙ is uniquely related to ˙ if the hardening matrix Hgh, governing the shear rates in different slip systems, is positive semideﬁnite (Hill, 1966), while only for certain hardening laws are the shear rates ␥˙ g always unique. At least one set of shear rates exists that satisﬁes the constitutive relations (11.2.9) and (11.2.17) through (11.2.21) for a prescribed strain rate ˙ (or prescribed stress ˙ ). If there are N nonzero ␥˙ g, they would satisfy N equations resulting from the combination of the consistency condition ˙ g ⫽ ˙ gc and the constitutive relations (11.2.22). In fact, substituting (11.2.22) into (11.2.20) yields the following set of equations:

冘 Q ␥˙ gh

h

⫽ RgL˙,

(11.2.23)

h

where Qgh ⫽ Hgh ⫹ RgLRh.

(11.2.24)

These equations are associated with the loading system together with the constraints ␥˙ h ⱖ 0.

11.2

APPLICATIONS

305

Only for certain hardening laws will the N ⫻ N matrix Qgh be necessarily nonsingular. For perfect plasticity (Hgh ⫽ 0), for example, it is always possible to choose at least one set of linearly independent slip systems among the potentially active ones such that this matrix is nonsingular and the auxiliary equations (11.2.20) are satisﬁed. Thus, for perfect plasticity the dimension of Qgh is never greater than 5 ⫻ 5. If ˜ gh, the N nonzero shear rates for this choice its inverse is denoted by Q of active slip systems are expressed by ៣ ␥˙ g ⫽ ˙ g˙

with

៣g ˙ ⫽

冘Q˜ LR . gh

h

(11.2.25)

h

Recall that the tangent modulus and compliance tensors of a single crystal are given, respectively, by (11.1.69), that is, ˙ ⫽ Lt˙ ,

˙ ⫽ Mt ˙.

(11.2.26)

From the foregoing kinematics of single-crystal plastic deformation, the main feature of the tangent modulus and compliance is that they depend on the set of active slip systems, which in turn depends on the prescribed strain rate ˙ (or stress ˙ ). It is well known in crystal plasticity that the deﬁnitions of tangent modulus and tangent compliance lead to a multibranch description. It also should be noted that, regarding (11.2.26), the inverse of tangent modulus does not exist in all situations. In other words Lt may possess some singularities. Perfect plastic behavior is one of such cases, where the problem of homogenization is typically carried out by using directly the tangent modulus rather than its inverse, since there is no restriction on the strain rate, whereas the stress rate is subjected to certain conditions regarding the regions in stress rate space. Substituting (11.2.25) into (11.2.22) and in comparison to (11.2.26), one obtains the following expression for single-crystal tangent modulus:

冉

Ltijmn ⫽ Lijkl Iklmn ⫺

冘 R ៣˙ g kl

g

冊

g mn

.

(11.2.27)

Using (11.2.25) and (11.2.24), (11.2.27) can be explicitly rewritten as

冉

Ltijkl ⫽ Lijmn Imnkl ⫺

冘 (H

gh

g,h

冊

⫹ RgLRh)⫺1 RgmnLklpqRhpg .

(11.2.28)

306

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

It can be readily shown that the tangent modulus Lt as given by (11.2.28) satisﬁes the symmetries Ltijkl ⫽ Ltklij if Hgh ⫽ Hhg.

(11.2.29)

If the single crystal is assumed to be elastically isotropic, then we have [see (1.4.5)] L ⫽ 3KIh ⫹ 2Id,

(11.2.30)

where Ihijkl ⫽ –13 ␦ij␦kl,

d Iijkl ⫽ –12 (␦ik␦jl ⫹ ␦il␦jk ⫺ –32 ␦ij␦kl).

The tangent modulus thus becomes Ltijkl ⫽ 3KIhijkl ⫹ 2Idijkl ⫺ 42

冘R

g ij

(Hgh ⫹ 2RgpqRhpq)⫺1 Rhkl,

g,h

(11.2.31) where the plastic incompressibility is used. In summary, the single-crystal tangent modulus described by (11.2.28) and (11.2.31) is unique for a given strain rate ˙ even if the strain rates ␥˙ g are not. Referring to (11.2.31), one can remark that even though the elasticity is approximated as isotropic, the tangent moduli are anisotropic in nature. This results from the typical process of the plastic ﬂow activated on discrete slip systems and their interactions governing the strain hardening behavior. Plastic Deformation of Polycrystalline Materials

In the previous section, we presented a possible way to determine the tangent modulus of a single crystal from the theory of homogeneous and continuum slip on well-deﬁned slip systems. Let us now consider a polycrystalline material where the current conﬁguration has undergone certain plastic deformation, and the potentially active slip systems as well as the stress distribution in each grain are known. In this stage the polycrystal is subjected to a loading increment characterized, for example, by a strain rate ˙ . To determine the effective tangent modulus Lt using the Hill self-consistent model, we need to evaluate the instantaneous stress and strain rates, ˙ and ˙ , as well as the tangent moduli t L , for a given prescribed macroscopic stress rate ˙ or strain rate ˙ .

11.2

APPLICATIONS

307

To this end, an iterative procedure is needed. First, a tentative guess is made for Lt so that the Hill constraint tensor given by (11.1.72) can be determined. Then, for each active set of slip systems, necessarily a subset of potentially active systems, the tangent modulus for the grain considered is calculated from (11.2.28) or (11.2.31) in the case of isotropic elasticity. Next, the strain concentration tensor A is computed for this grain using (11.1.75). To ensure that the assumed set of active slip systems do constitute the correct branch of Lt for the prescribed ˙ (or ˙ ), the auxiliary conditions (11.2.20) should be checked by taking into account Eqs. (11.1.75) and (11.2.26). If condition (11.2.20) is fulﬁlled, then Lt is correct for this iteration; if not, a new set of potentially active systems should be chosen until the correct Lt and A are found. This procedure is carried out for each grain orientation. The ﬁnal step in the ﬁrst iteration is to calculate an improved estimate (in comparison to the initial guess) of Lt from (11.1.80). The entire procedure is then repeated until a convergent Lt is reached. In the next two sections, the method is illustrated by simulating a monotonically increasing uniaxial load. In this case, the tangent modulus tensor is transversely isotropic. The corresponding Eshelby inclusion tensor and the Hill constraint tensors are obtained for computing the strain or stress concentration tensors. Hutchinson’s Calculations

Hutchinson (1970) implemented the Hill self-consistent model to study the behavior of a polycrystal consisting of randomly oriented FCC single crystals. In his computational procedure, the grains are considered spherical in shape and their orientations are assumed equally represented so that the average procedure required for the homogenization steps can be performed over all orientations. The elasticity of each single crystal is described by three independent Voigt elastic constants C11, C12, and C44 in the classical way of cubic symmetries. The random distribution of single crystals leads to isotropic overall elastic constant of the polycrystalline aggregate characterized by its bulk modulus K and shear modulus . Using the linear elastic self-consistent method for randomly distributed cubic crystal, the elastic moduli of the polycrystal can be obtained (Problem 11.4): K ⫽ –13 (C11 ⫹ 2C12), 83 ⫹ (5C11 ⫹ 4C12) 2 ⫺ C44 (7C11 ⫺ 4C12) ⫺ C44 (C11 ⫺ C12)(C11 ⫹ 2C12) ⫽ 0.

(11.2.32)

(11.2.33)

308

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

An FCC single crystal has crystallographically similar systems whose unit normals are the four [1,1,1]-type directions, relative to the crystal axes, and whose slip directions are the [1,1,0] types. As for elastic deformation, the self-consistent method can be used to express the initial critical macroscopic stress 0c (the yield stress) in terms of the initial shear stress 0c of a slip system introduced by (11.2.16). That is (see Problem 11.5) 0c ⫽ 0c

冪冉

3

2 ⫹ 32 2 2

冊

,

(11.2.34)

where 2 ⫽

C11 ⫺ C12 , 2(1 ⫺ 2␦) ⫹ 2␦(C11 ⫺ C12)

3 ⫽

C44 , (1 ⫺ 2␦) ⫹ 2␦C44 (11.2.35)

and ␦ is given by (4.3.38). For the case of isotropic elasticity where 2C44 ⫽ C11 ⫺ C12, it can be readily shown that 2 ⫽ 3 ⫽ 1. Hence 0c ⫽ 0c . Note that expression (11.2.33) is equivalent to assuming a Tresca criterion for the overall yield stress. This is only valid if no residual stresses are present in the polycrystalline materials. During a monotonic uniaxial tensile test in the x3 direction, the tangent moduli L display transverse isotropy with respect to the macroscopic coordinate system, so that Hooke’s law can be written in terms of the Voigt elastic constants:

冢冣冢 ˙ 11 ˙ 22 ˙ 33 ˙ 13 ˙ 23 ˙ 12

⫽

Ct11 Ct12 Ct13 Ct11 Ct11 Ct13 Ct11 Ct11 Ct33 0 0 0 0 0 0 0 0 0

0 0 0 0 0 0 t C44 0 t 0 C44 0 0

冣冢 冣

0 0 0 0 0 Ct66

˙ 11 ˙ 22 ˙ 33 2˙13 2˙23 2˙12

,

(11.2.36)

where t t Ct66 ⫽ –21 (C11 ⫺ C12 ).

(11.2.37)

11.2

APPLICATIONS

309

Copper is selected for this simulation because its single crystal shows strong elastic anisotropy. The elastic moduli for single-crystal copper used in our calculations are C12 /C11 ⫽ 0.722 and C44 /C11 ⫽ 0.447. The self-consistent predictions using Eqs. (11.2.32)–(11.2.34) give, respectively, the polycrystalline elastic moduli and initial critical shear stress: K ⫽ 0.815C11,

⫽ 0.285C11,

0c ⫽ 1.129 0c

(11.2.38)

or ⫽ 0.343,

E ⫽ 0.722C11,

(11.2.39)

where E is Young’s modulus and Poisson’s ratio. Furthermore, we pay particular attention to the single-crystal strain hardening and its effect on the polycrystalline hardening, by considering both perfect plasticity for each grain, as well as different forms of the hardening matrix Hgh. As shown by Kneer (1965), the transverse isotropy of the overall tangent modulus leads to analytical expressions of the Eshelby tensor. It follows from the Kneer calculations that the Eshelby tensor can be expressed as Sijkl ⫽ TijmnLmnkl, where

冘 K T˜ , 1 z ⫽ 冕 dz, 8 a ⫹az ⫹az ⫹az 3

Tijmn ⫽

(m) (m) ijmn

m⫽0

1

K(m)

0

2m

2

0

1

4

2

6

(m ⫽ 0, 3).

3

The coefﬁcients am and T˜ (m) ijmn are a polynomial functions of the components Cij of the transverse isotropic tangent modulus. Details of this calculation can be found in (Kneer, 1965). We ﬁrst consider the case without strain hardening in single crystals. The results are presented in Figure 11.1 for isotropic elasticity and anisotropic elasticity with the moduli of copper listed in (11.2.38). Clearly, the results show that the elastic anisotropy increases the initial

310

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

2.0 Anisotropic, Nonhardening Single Crystals C12 C11 = 0.722 C44 C11 = 0.447

1.6

σ 2τ c0 1.2 Isotropic, Nonhardening Single Crystals ν = 13 0.8

1

2

Eε 2τ c0

3

4

Figure 11.1 Tensile stress–strain curves for FCC polycrystals with randomly oriented and perfectly plastic single crystals.

yield stress of the polycrystal. This is not expected because the inhomogeneous elasticity arising from single-crystal anisotropy should decrease, rather than increase, the yield strength of the polycrystal yields. This might be explained by the fact that stresses in each grain are estimated by treating them as spherical inclusions. This is one of the limitations of the self-consistent model. As discussed previously, the polycrystalline aggregate displays a strain hardening behavior even if every single crystal in the aggregate behaves as a perfect plastic material. This arises from the intergranular interactions. To show the effect of single-crystal strain hardening, the interaction matrix Hgh should be estimated. In general, this procedure requires an experimental analysis performed on single crystals. Different forms of strain hardening matrix have been proposed in the literature. Taylor’s (1938) isotropic hardening law is the simplest and the most widely used one. This law states that the yield stresses of all slip systems remain equal and increase in proportion to the total shear. So that Hgh ⫽ h for all g and h, we have ˙ gc ⫽ h兺h ␥˙ h. Taylor’s simple hardening law is not able to reproduce the principal features of a single-crystal hardening, nor can it capture the polycrystalline hardening behavior, especially, at later stages of plastic deformation where multiple activations of slip systems render the interactions highly anisotropic. Nevertheless, the Taylor’s hardening law is used in the calculations presented in Figure 11.2 to show at least at the earlier stage of the

11.2

1.6

1.4

h = 0.04 µ

311

h = 0.02 µ

σ 2τ c0

h = 0.0 µ

1.2

1.0

APPLICATIONS

1

3

2

4

Eε p 2τ c0 Figure 11.2 Effect of single-crystal hardening.

plastic ﬂow the effect of single crystals hardening. The computations are performed for different hardening parameters h. Finally, under the same conditions without single-crystal hardening, the stress–strain relationship for polycrystal copper is estimated using the upper bound of the Taylor–Lin model and the Kro¨ner’s selfconsistent model. The comparison is shown in Figure 11.3. As discussed throughout this chapter, the stress–strain curve obtained from Kro¨ner’s model lies above the one obtained by the Hill method. This is expected because in the Kro¨ner inclusion problem, the matrix exerts

Kröner’s model

1.4

σ 2τ c0

Hill’s model 1.2 Lin’s model

1.0

1

2

Eε p

3

4

2τ c0 Figure 11.3 Upper and lower bounds on stress–strain curves.

312

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

an elastic constraint, whereas in the Hill model the matrix provides a much softer constraint because of plastic deformation.

11.3 TIME-DEPENDENT BEHAVIOR OF POLYCRYSTALLINE MATERIALS: SECANT APPROACH

Time-dependent behavior of polycrystalline materials was ﬁrst modeled by Hutchinson (1976) by assuming a power law describing the shear rate on slip systems for a given single crystal. The analysis was performed under small-strain condition leading to an elastoviscoplastic type behavior. Hutchinson (1976) assumed a steady-state creep behavior for single crystals for which the shear rate induced in a slip system g by a given resolved shear stress g is described by a rate-sensitive criterion, which is equivalent to assuming a nonlinear viscous behavior:

冉冊

n

␥˙ ⫽ ␥˙ g

0

g , gc

(11.3.1)

where ␥˙ 0 is a reference rate and n is the inverse of rate sensitivity. When n ⬎⬎ 1, the shear rate increase is negligible unless g is very close to gc . This statement is equivalent to conditions (11.2.19) and (11.2.20) for slip systems activation in time-independent plasticity. The critical shear stress gc , often called reference stress in time-dependent plasticity, is strongly dependent on temperature. The exponent n depends also on temperature, although somewhat less strongly, and usually falls between 3 and 8 for metals. A survey on the temperature ranges where the steady-state creep of polycrystal and single crystal can be approximated by a power law was given by Ashby and Frost (1975). If N is the total number of slip systems, the total strain rate is the sum of the contributions from all these systems:

冘 ␥˙ N

˙ ij ⫽

g⫽1

where

g

s Rijg ⫽ Mijpq pq,

(11.3.2)

11.3

TIME-DEPENDENT BEHAVIOR OF POLYCRYSTALLINE MATERIALS

冘冉 N

s ijpq

M

⫽

g⫽1

␥˙ 0 gc

冊冉 冊 g gc

313

n⫺1

RgijRgpq

(11.3.3)

with Ms being the so-called secant viscoplastic compliance of the single crystal. As reported by Hutchinson (1976), the compliance tensor is homogeneous of degree n ⫺ 1 in stress so that Ms () ⫽ n⫺1Ms ().

(11.3.4)

Let us now deﬁne the stress potential () and strain rate potential (˙ ) such that ˙ ⫽

⭸ ⭸

and ⫽

⭸ . ⭸˙

(11.3.5)

The viscoplastic constitutive law (11.3.2) leads to the following typical relationships between the dissipation ˙ , (), and (˙ ): ˙ ⫽ (n ⫹ 1)() ⫽

n⫹1 (˙) ⫽ n

冘 ␥˙ . n

g

g

(11.3.6)

g⫽1

Substituting (11.3.5) into (11.3.6) and by differentiating (11.3.6) with respect to the stresses, one obtains ⭸ ⭸ ⭸ ⭸2 (kl˙ kl) ⫽ (n ⫹ 1) ⫽ ⫹ kl . ⭸ij ⭸ij ⭸ij ⭸ij ⭸kl

(11.3.7)

This last equation leads to n

⭸ ⭸2 ⫽ kl . ⭸ij ⭸ij ⭸kl

(11.3.8)

Combining (11.3.8) with (11.3.2), we can readily show that Msijkl ⫽ where

1 ⭸2 , n ⭸ij ⭸kl

(11.3.9)

314

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

⭸2 ⭸˙ ⫽ ij ⫽ Mtijkl. ⭸ij ⭸kl ⭸ij

(11.3.10)

In Eq. (11.3.10), Mt is the tangent compliance tensor. On the other hand, a Taylor expansion of (11.3.2) at the vicinity of a point ˜ ⫺ ˙ can be written as ˙ ij ⫽

冏

⭸˙ ij ⭸kl

kl ⫹ ˜˙ ij ⫽ Mtijkl ( ˙ ) kl ⫹ ˜˙ ij,

(11.3.11)

⫽ ˜

where ˜˙ ij is called the back-extrapolated strain rate. From (11.3.9) and (11.3.10), the relation between the grain’s secant and tangent compliances are Mt ⫽ nMs.

(11.3.12)

At the polycrystal level, the macroscopic constitutive law is assumed to be similar to that of single crystals, so that one can write s ˙ ij ⫽ Mijpq pq,

(11.3.13)

where Ms is the macroscopic secant compliance tensor. In the same way as in the single-crystal case, Taylor expansion of (11.3.13) at the vicinity of the macroscopic stress leads to the deﬁnition of a macroscopic tangent modulus Mt as t ˙ ij ⫽ Mijpq () pq ⫹ ˙ ij0,

(11.3.14)

where Mtijkl () ⫽ ⭸˙ ij / ⭸kl兩⫽ and ˙ 0ij is a macroscopic extrapolated strain rate. Hutchinson (1976) has shown that the macroscopic tangent and secant compliance tensors are linked by a relation similar to the one for single crystals, that is, Mt ⫽ nMs. This is derived by deﬁning the macroscopic dissipation ˙ , macroscopic strain rate potential ⌽(˙ ), and stress potential ⌿() such that ˙ ⫽

⭸⌿ ⭸

and ⫽

⭸⌽ . ⭸˙

Note that Eqs. (11.3.11) and (11.3.14) are exact only when they describe the strain rate associated with the stress used as a reference

11.3

TIME-DEPENDENT BEHAVIOR OF POLYCRYSTALLINE MATERIALS

315

for the expansion. Otherwise they are only approximate. This will not present a limitation for the treatment of the grains since the stress and the strain rates are assumed to be uniform within the framework of the self-consistent scheme. As a result, the actual value of stress in the grain considered can be selected to perform the expansion. Starting from the linearized equation (11.3.14), the macroscopic tangent compliance tensor Mt can be estimated by adopting a Hill-type self-consistent method. In other words, one can consider each grain with tangent compliance Mt and prescribed reference strain rate ˜˙ embedded in a homogenized effective medium having the properties of Mt and prescribed reference strain rate ˙ 0. Following the same procedure as for Eqs. (11.1.71) and (11.1.72), the Eshelby solution extended to a tangent formulation gives the interaction relation linking the local to the macroscopic quantities [see (4.5.19)], ˜ ⫺ ), ˙ ⫽ ˙ ⫹ H(

(11.3.15)

˜ is the inverse of the Hill constant tensor, where H ˜ ⫽ (S⫺1 ⫺ I)⫺1 Mt. H

(11.3.16)

Note that Eshelby’s tensor in (11.3.16) depends on the tangent compliance tensor together with the shape of the grain in consideration. As reported by Lebensohn and Tome´ (1993), the relation Mt ⫽ nMs enables us to express the equations in terms of the secant compliance tensor as ˜ ⫽ n(S⫺1 ⫺ I)⫺1 Ms. H

(11.3.17)

Substituting (11.3.2) and (11.3.12) into (11.3.15) yields ⫽ B,

(11.3.18)

where ˜ ⫺1 (Ms ⫹ H). ˜ B ⫽ (Ms ⫹ H)

Finally, the homogenization procedure using ⫽ 具典 and Ms ⫽ 具MsB典 leads to ˜ ⫺1 (Ms ⫹ H) ˜ 典. Ms ⫽ 具Ms ⬊(Ms ⫹ H)

(11.3.19)

316

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

In summary, we have introduced in this section the viscoplastic selfconsistent model initially developed by Hutchinson (1976) for modeling steady-state creep of polycrystalline materials, and have shown how to relate a secant formulation to a tangent formulation. We have also shown how the Eshelby solution required for the self-consistent scheme can be used to combine both the secant and tangent moduli for solving interaction problems. Since Hutchinson’s work (1976), the viscoplastic self-consistent model has been adopted by many authors as an alternative strategy to tackle the problem of large plastic deformations by simply neglecting the elastic deformation. This way of thinking was successively adopted by Molinari et al. (1987) to describe the texture development in cubic polycrystals. For more information regarding the numerical implementation and limitations of the method, the readers are referred to the work of Lebensohn and Tome´ (1993). PROBLEMS

11.1 Prove Eq. (11.1.30). 11.2 Check the consistency L ⫽ (M)⫺1 of the prediction from (11.1.80). 11.3 Show that, for perfect plasticity, the dimension of Qgh is never greater than 5 ⫻ 5. 11.4 For cubic symmetries, if we assume that all single crystals are randomly oriented, show that a self-consistent estimation of the elastic constant of the polycrystal gives isotropic moduli expressed by Eqs. (11.2.32) and (11.2.33). 11.5 For cubic symmetries, if we assume that all single crystals are randomly oriented, show that the overall critical shear stress is given by (11.2.38). 11.6 Show the following relationships: LtAr ⫽ BrL and MtBr ⫽ ArM.

REFERENCES Asaro, R. J. (1983). Crystal Plasticity, J. Appl. Mech., Vol. 50, pp. 921–934. Asaro, R. J. and J. R. Rice (1977). Strain Localization in Ductile Single Crystals, J. Mech. Physics Solids, Vol. 25, pp. 309–338.

REFERENCES

317

Ashby, M. F. and Frost, H. J. (1975). The Kinematics of Inelastic Deformation Above 0 K, in Constitutive Equations in Plasticity, A. S. Argon, ed., MIT Press, Cambridge. pp. 117. Berveiller, M. and A. Zaoui (1979). An Extension of the Self-Consistent Scheme to Plastically-Flowing Polycrystals, J. Mech. Phys. Solids, Vol. 26, pp. 325–344. Bishop, J. F. W. and R. Hill (1951). A Theoretical Derivation of the Plastic Properties of a Polycrystalline Facecentered Metal, Phil. Mag. Vol. 42, pp. 1298–1307. Bragg, W. H. and W. L. Bragg (1933). The Crystalline State, Bell, London. Budiansky, B. and O. L. Mangasarian (1960). Plastic Stress Concentration at Circular Hole in Inﬁnite Sheet Subjected to Equal Biaxial Tension, J. Appl. Mech., Vol. 27, pp. 59–64. Buryachenko, V. (1996). The Overall Elastoplastic Behavior of Multiphase Materials with Isotropic Components, Acta Mech., Vol. 119, pp. 93–117. Castan˜eda, P. (1991). The Effective Mechanical Properties of Nonlinear Isotropic Composites, J. Mech. Phys. Solids, Vol. 39, pp. 45–71. Castan˜eda, P. (1996). Exact Second-Order Estimates for the Effective Mechanical Properties of Nonlinear Composite Materials, J. Mech. Phys. Solids, Vol. 44, pp. 827–862. Dvorak, G. J. (1992). Transformation-Field Analysis of Inelastic Composite Materials, Proc. R. Soc. London, Ser. A, Vol. 431, pp. 89–110. Ewing, J. A. and W. Rosenhain (1900). Experiments In Micro-Metallurgy: Effects of Strain. Preliminary Notice, Philos. Trans. R. Soc. Lond., Vol. A199, pp. 85–90. Eshelby, J. D. (1957). The Determination of the Elastic Field of an Ellipsoidal Inclusion and Related Problems, Proc. Roy. Soc. Lond. Vol. A241, pp. 376– 396. Gilormini, P. (1997). Shortcomings of Several Extensions of the Self Consistent Model for Heterogeneous, Nonlinear Solids, Revue de Metallurgie, Vol. 94, pp. 1081–1087. Hill, R. (1965). Continuum Micro-mechanics of Elastoplastic Polycrystals, J. Mech. Phys. Solids, Vol. 13, pp. 89–101. Hill, R. (1966). Generalized Constitutive Relations for Incremental Deformation of Metals by Multislip, J. Mech. Phys. Solid, Vol. 14, p. 99. Hill, R. and K. S. Havner (1982). Perspectives in the Mechanics of Elastoplastic Crystals, J. Mech. Phys. Solids, Vol. 30, pp. 5–22. Hill, R. and J. R. Rice (1972). Constitutive Analysis of Elasto-Plastic Crystals at Arbitrary Strains, J. Mech. Phys. Solids, Vol. 20, pp. 401–413. Hu, G. (1996). A Method of Plasticity for General Aligned Spheroidal Void of Fiber-Reinforced Composites, Int. J. Plasticity, Vol. 12, pp. 439–449. Hutchinson, J. W. (1970). Elastic-Plastic Behaviour of Polycrystalline Metals and Composites, Proc. R. Soc. Lond., Vol. A319, pp. 247–272.

318

MEAN FIELD THEORY FOR NONLINEAR BEHAVIOR

Hutchinson, J. W. (1976). Bounds of Self-Consistent Estimates for Creep of Polycrystalline Materials, Proc. R. Soc. Lond., Vol. A348, pp. 101–127. Kro¨ner, E. (1961). Zur plastischen Verformung des Vielkristalls, Acta Metall., Vol. 9, pp. 155–161. Lebensohn, R. and C. N. Tome´ (1993). A Self-Consistent Anisotropic Approach for the Simulation of Plastic Deformation and Texture Development of Polycrystals Applications to Zirconium Alloys, Acta Metall. Mater., Vol. 41, pp. 2611–2624. Masson, R. and A. Zaoui (1999). Self-Consistent Estimates for the RateDependent Elastoplastic Behaviour of Polycrystalline Materials, J. Mech. Phys. Solids, Vol. 47, pp. 1543–1568. Molinari, A., G. R. Canova, and S. Ahzi (1987). A Self-Consistent Approach of the Large Deformation Polycrystal Viscoplasticity, Acta Metall., Vol. 35, pp. 2983–2994. Kneer, G. (1965). Uber die Berechnung der Elastizitatsmoduln vielkristalliner Aggregate mit Textur, Phys. Stat. Sol., Vol. 9, pp. 825–838. Polanyi, von M. (1922). Rontgenographische Bestimmung von Ksistallanordnunge, Naturwissenschaften, Vol. 10, p. 411. Qui, Y. P. and G. J. Weng (1992). A Theory of Plasticity for Porous Materials and Particle-Reinforced Composites, J. Appl. Mech., Vol. 59, pp. 261–268. Schmid, E. and W. Boas (1935). Kristallplastizita¨t, Springer, Berlin, p. 64. Sachs, G. (1928). Zur ableilung einer ﬂeissbedingung (stresses causing ﬂow), VDI Z., Vol. 72, pp. 734–736. Suquet, P. (1993). Overall Potentials and Extremal Surfaces of Power Law or Ideally Plastic Materials, J. Mech. Phys. Solids, Vol. 41, pp. 981–1002. Suquet, P. (1995). Overall Properties of Nonlinear Composites: A Modiﬁed Secant Moduli Theory and Its Link with Ponte Castan˜eda’s Nonlinear Variational Procedure, C.R. Acad. Sci. Paris, Vol. 320 (Se´rie IIb), pp. 563– 571. Talbot, D. and J. Willis (1985). Variational Principles for Inhomogeneous Nonlinear Media,’’ IMA J. Appl. Math., Vol. 35, pp. 39–54. Tandon, G. P. and G. J. Weng (1988). A Theory of Particle-Reinforced Plasticity, J. Appl. Mech., Vol. 55, pp. 126–135. Taylor, G. I. (1934). Plastic Deformation of Crystals, Proc. Roy. Soc., Vol. A145, pp. 362–404. Taylor, G. I. (1938). Plastic Strain in Metals, J. Inst. Metals, Vol. 62, p. 307. Taylor, G. I. and C. F. Elam (1923). The Distortion of an Aluminum Crystal During a Tensile Test, Proc. Roy. Soc., Vol. A102, p. 647. Taylor, G. I. and C. F. Elam (1925). The Plastic Extension and Fracture of Aluminum Crystals, Proc. Roy. Soc., Vol. A108, pp. 28–51. Willis, J. R. (1983). The Overall Response of Composite Materials, J. Appl. Mech., Vol. 50, pp. 1202–1209.

12 NONLINEAR PROPERTIES OF COMPOSITES MATERIALS: THERMODYNAMIC APPROACHES Thermodynamic approaches in micromechanics consist of solving the ﬁeld equations by minimizing a free energy, where the minimum found corresponds to the desired macroscopic potential W(), which represents the mechanical energy stored in the domain V of the representative volume element (RVE) subjected to a macroscopic strain . As mentioned in the linear case through the introduction of variational principles, which leads to different bounds, an exact solution to these ﬁeld equations is rather difﬁcult to obtain and becomes impossible to derive in the nonlinear case. This is mainly due to highly ﬂuctuating ﬁelds resulting from the nonlinear behavior of the constituents. It has been shown that approximated solutions for the local problem can be obtained in the linear case, leading to pertinent estimations of the macroscopic behavior, which are capable of accounting for the inﬂuence of morphological parameters and phase spatial distribution on the global behavior. Unfortunately, due to the nonapplicability of the superposition principle, on which most developments are based in linear cases (e.g., use of elementary solutions such as Eshelby’s one), the philosophy behind these approaches cannot be transported directly to nonlinear behaviors. To take advantage of the knowledge acquired in linear cases, linearization of the local constitutive laws could be one of the interesting approaches. The procedure consists of replacing the nonlinear ﬁeld equations in the RVE by linear equations in the same RVE, whose solution can be evaluated exactly or approximately via the use of the tools developed for linear materials. The linearization is completed with Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

319

320

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

a set of complimentary equations, which characterizes the parameters deﬁning the linear problem (e.g., elasticity moduli). Typically, these equations are nonlinear so that the character of the initial problem is conserved. However, in this case, we will not deal with ﬁeld equations but with equations involving a ﬁnite set of variables which can be solved with the appropriate numerical tools. In most cases, simple algorithms lead to a solution. The methodology presented in the above is referred to as the ‘‘nonlinear extension’’ of a linear model. The local linear problem resulting from the linearization procedure is identical to the homogenization problem for linear composites, referred to as linear comparison composite (LCC). This virtual LCC results solely from the linearization step and has no physical existence. Further, its moduli are distinct from the initial elasticity moduli of the real nonlinear composite. Although it is often the case, the LCC does not necessarily have the same spatial distribution of phases, or the same number of constituents, as the real nonlinear composite. One of the difﬁculties of this method lies in the use of the linear model to obtain the nonlinear macroscopic behavior. Typically, linear models do not provide detailed description of the local ﬁelds in the LCC but only averaged strains or stresses in the phases. This information is sufﬁcient in the case of linear problems since the macroscopic stress can be obtained from averaged strains in the phases via the following equation: ⫽

冘 c ⫽ 冘 c L. r

r

r

r

r r

r

Due to the nonlinear behavior of the constituents, this property does not hold for nonlinear composites where the macroscopic stress is given by ⫽

冘 c ⫽ 冘 c 冓⭸⭸()冔 ⫽ 冘 c ⭸⭸( ) r

r

r

r

r

r

Vr

r

r

r

where () is the local free energy, cr the volume fraction of each phase, and Lr their stiffness. The above general principles will be addressed in this chapter, in the particular case where the LCC is obtained from the secant moduli of the nonlinear constituents. Two approaches, the ‘‘classical’’ approach and the ‘‘modiﬁed’’ approach, will be presented and compared. These

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

321

two approaches are both relatively simple to use and differ only from the set of complimentary equations characterizing the LCC. In the ﬁrst part, the nature of the constitutive laws will be presented and illustrated with examples. Both tangent and secant linearization methods for the constitutive laws will be deﬁned. The variational formulation that deﬁnes the homogenized behavior of heterogeneous materials will be presented in the second part. The general method of ‘‘nonlinear extension’’ of linear models is presented at the end and applied to the case of the classical secant linearization, which shows inconsistencies related to the lack of information regarding the intraphase ﬂuctuations of local ﬁelds. An attempt to estimate these heterogeneities is made through the modiﬁed-secant formulation based on the second-order deformation moments within the phases, correcting the deﬁciencies of the classical extension. The two approaches will be illustrated and compared through the different problems given at the end of this chapter. Recent methodologies to describe the overall behavior of nonlinear composites adopt variational procedures. These approaches are not addressed here. The reader may refer to the Suggested Readings at the end of the chapter.

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

Thermodynamic Potentials

The behavior of the constituents treated in this chapter can be described by two thermodynamic potentials: the free energy and the dissipation potential , which are both expressed as a function of strain and of the appropriate internal variables ␣ (scalar or tensorial): Constitutive laws:

rev ⫽

⭸(, ␣) , ⭸

Complimentary laws: irr ⫽ with

⭸(˙, ␣ ˙) , ⭸˙

⫽ rev ⫹ irr.

⭸(, ␣) , ⭸␣

a⫽⫺

⭸(˙, ␣ ˙) , ⭸␣ ˙

a⫽⫺

(12.1.1)

(12.1.2) (12.1.3)

The convexity of and its nullity at ˙ ⫽ 0 impose a positive dissipation and, consequently, the second law is satisﬁed. The convexity of is associated with the stability of the material. Although many

322

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

approximate formulations have been proposed, there is no homogenization theory giving rigorous solutions to the homogenized behavior of phase mixtures described by (12.1.1)–(12.1.3). However, theories based on rigorous bounds have recently been developed in the simple case where the behavior of the phases can be described with only one potential, the free energy or the dissipation potential, the remaining potential being equal to zero. Behaviors Described by a Single Potential

We assume the behavior of each phase is described with a single convex potential, () or (˙), the remaining potential is equal to zero, such that the stress–strain or stress–strain rate relation can be written as follows: ⫽ rev ⫽

⭸() , ⭸

⫽ 0.

(12.1.4)

⫽ irr ⫽

⭸(˙) , ⭸˙

⫽ 0.

(12.1.5)

Or

Equation (12.1.4) describes a nonlinear elastic behavior under smallstrain deformation, while (12.1.5) corresponds to a purely viscous behavior where deformation can be ﬁnite (the problem is purely Eulerian). For the sake of simplicity of the notations, only the ﬁrst expression will be used (nonlinear elasticity). The results will be directly transferable to the second case by considering as a strain rate. Equation (12.1.4) can be inverted to obtain ⫽

⭸ ˜ () , ⭸

(12.1.6)

where ˜ () is the complimentary energy of the material. Mathematically, the relation between ˜ () and () is obtained via the Legendre transformation: ˜ () ⫽ sup{ : ⫺ ()}.

Let us now consider a few examples.

(12.1.7)

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

323

Isotropic Materials

Most isotropic materials are linear under hydrostatic load and nonlinear under shear; their behavior can be written with the following expressions: m ⫽ 3km,

s ⫽ 2 sec(eq)e,

sec(eq) ⫽

eq , 3eq

(12.1.8)

where m ⫽

kk , 3

m ⫽

kk

3

eq ⫽ (–32 s:s)1 / 2,

,

sij ⫽ ij ⫺ m␦ij, (12.1.9)

eij ⫽ ij ⫺ m␦ij.

eq ⫽ (–23 :)1 / 2,

(12.1.10)

Therefore, the bulk modulus K is constant while the shear modulus sec depends on strain (hence the nonlinearity of the deformation). This behavior is derived from the following free energy: () ⫽ –92 k 2m ⫹ eq(eq),

eq(eq) ⫽

冕

eq

0

eq deq,

(12.1.11)

where eq is the area under the curve in the eq(eq) diagram. The associated complimentary energy ˜ () is written as follows: ˜ () ⫽

1 2 ⫹ ˜ eq(eq). 2K m

(12.1.12)

Here ˜ eq is the dual potential of eq. Hencky’s Model in Plasticity

The elastoplastic behavior is rigorously described with incremental relations that enable us to distinguish plastic and elastic loads. In the case of isotropic hardening (where the hardening variable is ) with the Von Mises criterion, these relations are written as follows:

324

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

e ⫽

⫽ e ⫹ p,

冉 冊

3 s:˙s d y ˙ ⫽ 2 eq d

m 1 I⫹ s, 3K 2

˙ p ⫽

3 ˙ s , 2 eq

⫺1

if eq ⫽ y(),

˙ ⫽ 0

if eq ⬍ y(). (12.1.13)

Hencky’s model, also referred to as the deformation theory of plasticity, neglects the incremental nature of plasticity and replaces the equation describing the evolution of the plastic deformation (12.1.13) by ⫽ e ⫹ p,

e ⫽

m 1 I⫹ s, 3K 2

p ⫽

3 s , 2 eq

⫽ ( y)⫺1(eq).

(12.1.14)

For example, the model proposed by Ramberg and Osgood describes a power law hardening y() ⫽ 0( / 0)1 / n. This model can be written in the three-dimensional case: ⫽ e ⫹ p,

e ⫽

m 1 I⫹ s, 3K 2

p ⫽

冉 冊

30 eq s , 2 0 eq (12.1.15)

which is derived from the following potential:

冉 冊

eq 1 2 1 ˜ () ⫽ m ⫹ (eq)2 ⫹ 0 0 2K 6 n ⫹ 1 0

n⫹1

,

(12.1.16)

where , n ⱖ 1, 0, and 0 are the elastic shear modulus, the hardening exponent, and reference material constants, respectively. In the case of monotonic loading, Hencky’s model is a useful approximation. Unfortunately, it is inapplicable in the case of complex loadings. It can be shown that the incremental method and the deformation theory give the same response under monotonic and radial (the principle stress directions are time independent) loading. The adoption of the deformation theory in the case of heterogeneous materials supposes the stress state to be monotonic and radial at any point of the RVE. This hypothesis is more than likely not satisﬁed. However, in simple cases (e.g., elastoplastic matrix reinforced with simply shaped elastic inclusions), it can be observed that under a monotonic and radial

12.1

NONLINEAR BEHAVIOR OF CONSTITUENTS

325

macroscopic load, deviations from this hypothesis are small. Therefore, the approximation of the incremental theory by a deformation theory is fairly good. For a more detailed discussion on the relationship between the incremental plasticity and the deformation theory, one can refer to Hutchinson (1976). Creep Behavior

The high-temperature creep of metals can often be treated by neglecting elastic deformation. It is typically expressed by a power law relation between strain rate and Cauchy’s stress: ⫽ mI ⫹ s,

eq ˙ eq ⫽ , 0 ˙ 0

s 2 e˙ ⫽ , eq 3 ˙ eq

˙ m ⫽ 0.

(12.1.17)

The potentials and ˜ describing the dissipation are written as follows:

冉冊

˙ eq ˙ (˙) ⫽ 0 0 m ⫹ 1 ˙ 0

冉 冊

eq ˙ ˜ () ⫽ 0 0 n ⫹ 1 0

m⫹1

,

n⫹1

.

(12.1.18)

Here m ⫽ 1/n, and ˙ 0 and 0 are the strain rate sensitivity exponent and the reference strain rate and stress, respectively. Continuum Description of Single Crystals

The general framework of thermodynamic potentials can also be applied to crystalline materials. The total strain rate, ˙ , in a single crystal is given by a superposition of the elementary shear rates in each slip system

冘 ␥˙ R , N

˙ ⫽

g

g

(12.1.19)

g⫽1

where the shear rate ␥˙ g in the slip system g depends only on the critical shear stress g in this system, such that ␥˙ g ⫽

⭸˜ g g ( ), ⭸ g

(12.1.20)

where the potential ˜ g is convex and typically given by a power law as follows:

326

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

冉 冊

g␥˙ 兩 g兩 ˜ ( ) ⫽ g 0 0 n ⫹ 1 0g g

g

n g⫹1

.

(12.1.21)

In the above, ng ⱖ 1 is the creep exponent, g0 is the critical shear stress for the considered system, and ␥˙ 0 is a reference shear rate. The constitutive law described by Eqs. (12.1.19) and (12.1.20) are derived from a convex potential for the single crystal: ⭸˜ () ˙ ⫽ , ⭸

冘 ˜ ( ) ⫽ 冘 ˜ (R :). N

˜ () ⫽

N

g

g

g⫽1

g

g

(12.1.22)

g⫽1

Secant Moduli Description of the Behavior

In what follows, only one notation of the behavior will be used, based on the elastic potentials, and ˜ . The constitutive law (12.1.8) can be written in a more compact form as follows: ⫽ Lsec():,

(12.1.23)

where Lsec is the secant modulus tensor. In the case of isotropic materials, it is a function of the projection tensors I h and I d: Lsec() ⫽ 3KIh ⫹ 2 sec(eq)Id.

(12.1.24)

Note that Lsec is not uniquely deﬁned. For example, one can add an anisotropic component to the secant tensor without changing the constitutive law: sec d 2 L˜ sec ˜ ije˜ kl), ijkl ⫽ Lijkl ⫹ ␣(I ijkl ⫺ – 3e

e˜ ij ⫽

eij eq

(12.1.25)

such that Lsec(): ⫽ L˜ sec(): for all ␣. And L˜ sec is a secant tensor in the sense described by (12.1.23), but Lsec given by (12.1.24) is the only isotropic tensor verifying this relation. Incremental Formulation and Tangent Moduli

We now discuss homogenization methods based on tangent moduli. It results from an incremental form of the constitutive law given by (12.1.4), obtained with a differentiation with respect to time:

12.1

˙ ⫽ Ltg():˙,

327

NONLINEAR BEHAVIOR OF CONSTITUENTS

Ltg ijkl() ⫽

⭸ij() ⭸2() ⫽ , ⭸ij⭸kl ⭸kl

(12.1.26)

where Ltg() is the tangent modulus tensor, which is typically anisotropic, even when the material is isotropic. Accordingly, in the case of an isotropic material described by Eqs. (12.1.23) and (12.1.24), the tangent tensor is given by h sec d Ltg (eq)I ijkl ⫹ ijkl() ⫽ 3KIijkl ⫹ 2

4 d sec ( ) e˜ e˜ . 3 deq eq eq ij kl

(12.1.27)

For convenience, Ltg can be expressed as h sec Ltg (eq)E 1ijkl ⫹ 2 tg(eq)E 2ijkl, ijkl() ⫽ 3KI ijkl ⫹ 2

(12.1.28)

where E 2ijkl ⫽ –23 e˜ ije˜ kl,

E1 ⫽ I d ⫺ E 2,

tg ⫽ sec ⫹

d sec(eq) 1 deq(eq) eq ⫽ eq. deq 3 deq

(12.1.29)

The tensors E1 and E2 have the following properties: E 2:E 2 ⫽ E 2,

E1:E1 ⫽ E1,

E 2:I h ⫽ 0,

E 2:E1 ⫽ 0,

E1:I h ⫽ 0.

(12.1.30)

The shear modulus tg gives the slope of the curve eq(eq). In the case of isotropic incompressible materials described by a power law, the secant tensor Lsec (12.1.24) and the tangent tensor Ltg (12.1.28) are given by L () ⫽ ⫹⬁I ⫹ 2 (eq)I , sec

h

sec

d

冉冊

1 0 eq (eq) ⫽ 3 0 0 sec

m⫺1

,

(12.1.31) and Ltg() ⫽ ⫹⬁I h ⫹ 2 sec(eq)(E1 ⫹ mE 2),

tg(eq) ⫽ m sec(eq).

(12.1.32)

328

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

To illustrate the nonuniqueness of the secant moduli, it can be easily veriﬁed that the anisotropic tensor (1/m)Ltg is also the secant tensor for isotropic materials described by a power law see Problem 12.1. The tangent modulus tensor is uniquely deﬁned with equation (12.1.26). However, in some cases, it is approximated, to simplify the algebra, by an isotropic tensor, Ltg() ⫽ ⫹⬁I h ⫹ 2 tg(eq)I d.

iso

(12.1.33)

Another isotropic tangent tensor is expressed by Ltg() ⫽ ⫹⬁I h ⫹

iso

1 tg d d 4 ⫹ m sec (L ⬋I )I ⫽ ⫹⬁I h ⫹ 2 (eq)I d. 5 5 (12.1.34)

It should be noted that the above approximation may lead to severe discrepancies in the homogenization schemes adopting a tangent linearization of local constitutive laws.

12.2

EFFECTIVE POTENTIALS

Let us now consider a RVE with volume V and boundary S representing a nonlinear heterogeneous material. The boundary conditions on S are given in terms of combined loading: traction boundary condition p0 on S and displacement boundary condition u0 on Su with S ⫽ S ⫹ Su. We are to ﬁnd the ﬁelds u, , and so that u and fulﬁll the conditions of kinematics:

冦

⫽ –12 (ⵜu ⫹ (ⵜu)T)

u u ⫽ u0

within V is continuous in V. on Su

(12.2.1)

Under the conditions (12.2.1), u and are called kinematically admissible:

再

div ⫹ f ⫽ 0 n ⫽ p0

inside V . on Su

(12.2.2)

Under the conditions (12.2.2), is called statically admissible.

12.2

EFFECTIVE POTENTIALS

329

By introducing the thermodynamics potentials, and are related at each material point r of V by the constitutive laws: (r) ⫽

⭸((r), r) , ⭸

(r) ⫽

⭸ ˜ ( (r), r) . ⭸

(12.2.3)

The solution to the nonlinear problem requires solving one of the following problems: Under displacement boundary conditions related to an applied macroscopic strain , the problem consists of solving the following problem for statistically admissible stress: ∀r僆V

(r) ⫽

⭸((r), r) , ⭸

(12.2.4)

具(r)典V ⫽ .

Under traction boundary conditions related to an applied macroscopic stress , the problem consists of solving the following problem for kinematically admissible strain: ∀r僆V

(r) ⫽

⭸((r), r) , ⭸

(12.2.5)

具 (r)典V ⫽ .

Solutions to (12.1.1) or (12.1.2) lead to the deﬁnition of local stress and strain ﬁelds fulﬁlling the following variational properties, which result from the convexity of the local potentials and ˜ . This can be stated as: The solution of strain ﬁeld for the ﬁrst problem minimizes the free energy , so that 具()典 ⫽ inf具(˜)典,

(12.2.6)

where ˜ is a kinematically admissible strain with 具˜ 典 ⫽ . The solution of stress ﬁeld for the second problem minimizes the complementary free energy ˜ , so that 具 ˜ ()典 ⫽ inf具˜ ( ˜ )典,

˜ is a trial statically admissible stress with 具典 ˜ ⫽ . where

(12.2.7)

330

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

Deﬁnition (12.2.6) corresponds to the macroscopic or effective free energy of the representative volume element, denoted by W (), so that the macroscopic constitutive relation writes ⫽

⭸W() , ⭸

(12.2.8)

with W() ⫽ inf具(˜)典.

(12.2.9)

Equation (12.2.8) can be shown from (12.2.4) and (12.2.6) by using the Hill lemma. Similarly, one can deﬁne a macroscopic complementary energy as ⫽

˜ ) ⭸W( ⭸

˜ ) ⫽ inf具 with W( ˜ ( ˜ )典.

(12.2.10)

˜ are dual convex functions, such that Note that the potentials W and W with the help of the Hill lemma, one has ˜ ) ⫽ 具()典 ⫹ 具 W() ⫹ W( ˜ ()典 ⫽ 具 :典 ⫽ :.

(12.2.11)

The principles of minimum energy (12.2.6) and (12.2.7) may be used ˜ For example, by to set bounds for the effective potentials W and W. choosing the solution of problem (12.1.1) or (12.1.2) corresponding to a uniform stress ⫽ and uniform strain ﬁeld ⫽ , respectively, one obtains the equivalent Voigt and Reuss bounds for the effective potentials. By setting ⫽ in (12.2.9), one has

冘 c ().

(12.2.12)

冘 c ˜ ().

(12.2.13)

n

W() ⱕ 具()典 ⫽

r

r

r⫽1

Similarly n

˜ ) ⱕ 具 W( ˜ ()典 ⫽

r

r

r⫽1

As an application for incompressible power law materials deﬁned by (12.1.18), the Voigt and Reuss bounds read (see Problem 12.2)

12.3

冉冊

0Reuss0 eq m ⫹ 1 0

m⫹1

ⱕ W() ⱕ

THE SECANT APPROACH

冉冊

0Voigt0 eq m ⫹ 1 0

331

m⫹1

,

(12.2.14)

where ⫺m Reuss ⫽ 具⫺n , 0 0 典

12.3

0Voigt ⫽ 具0典.

(12.2.15)

THE SECANT APPROACH

For general purposes, the secant method solves the following ﬁeld equations: ⫽ –12 (ⵜu ⫹ (ⵜu)T),

div ⫽ 0, 具典 ⫽ , (r) ⫽ Lsec(r, (r)):(r),

(12.3.1)

where Lsec is the local secant modulus tensor, which depends on the phase considered. It typically ﬂuctuates within a phase due to the ﬂuctuation of the local strain (r). Therefore, the secant modulus tensor is highly heterogeneous. Its ﬂuctuation results from the nonlinearity of the problem associated with its dependency on the local strain. Indeed, the heterogeneity of secant modulus tensor depends on which type of nonlinear behavior is displayed by the constituents and also on the amount of applied strain. To set up a direct homogenization procedure of such highly heterogeneous materials is very difﬁcult unless systematic approximations are used, which, in general, relies on a linearization procedure with appropriate complementary laws. As a ﬁrst attempt and within a general procedure, the problem could be seen at a given strain state as a linear problem with the following local constitutive law: (r) ⫽ Llin(r):(r),

(12.3.2)

Llin(r) ⫽ Lsec(r, (r)).

(12.3.3)

with

332

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

Deﬁnition (12.3.2) is the linear model required for the linearization procedure of the local behavior, whereas deﬁnition (12.3.3) corresponds to additional or complementary relationships, so that the nonlinear behavior can be captured. When these two steps are accomplished, the problem becomes a classical one. Then an appropriate ‘‘classical’’ linear homogenization scheme can be chosen to obtain the nonlinear macroscopic behavior. However, (12.3.2) and (12.3.3) are still not suitable for analytical calculations due to the inﬁnite number of complementary equations required for deﬁnition (12.3.3). Therefore, approximations are needed, which, clearly, need to render a ﬁnite number of complementary equations with a certain accuracy in describing the heterogeneous nature of the nonlinear behavior. For such a purpose, approximations are introduced both in the step of linearization and complementary equations. The linear model in Eq. (12.3.2) may be assumed piecewise uniform for the stiffness tensor Llin(r), so that, for a given phase r(r ⫽ 1, . . . , n) one has Llin(r) ⫽ Lr. In addition, the complementary equations are reduced to a ﬁnite number corresponding to the identiﬁed number of constituents or phases, which lead to a deﬁnition of stiffness tensors Lr at some effective piecewise uniform strains ˜ r, representing the strain distribution in each phase, and therefore requiring an accurate model to be determined. The n complementary equations read Lr ⫽ Lrsec(˜r),

(12.3.4)

where the nonlinearity of the problem lies in the dependency of each individual effective strain ˜ r on the stiffness Lr of the different phases, so that n nonlinear problems have to be solved, requiring in general simple iterative procedures. Once the tensors Lr are determined, the problem becomes a classical one by taking advantage of the homogenization approaches developed in linear elasticity. The choice of the appropriate linear homogenization scheme to describe the microstructure of the real nonlinear composite material deﬁnes the so-called linear comparison composite, for which the overall effective stiffness L is expressed formally as L ⫽ L(cr, Lr, . . .) ⬅ L(),

(12.3.5)

which depends on the stiffness of each constituent and some morphological aspects related to the microstructure. The overall constitutive law is then nonlinear and formally given by

12.3

THE SECANT APPROACH

⫽ L():.

333

(12.3.6)

In the following, two methods to deﬁne the effective strains ˜ r are discussed and compared. The ﬁrst approach is known as the classical secant method. It simply deﬁnes the effective strains as the average strain in each phase. The second method, called the ‘‘modiﬁed’’ secant method, could be seen as a reﬁnement of the ﬁrst method by introducing the second-order moment of the strain ﬁeld. Classical Method

The classical method has been extensively used to deal with the nonlinear behavior of composite materials. It consists of deﬁning the effective strain ˜ r as the mean value of the local strain ﬁeld over the considered phase. That is ˜ r ⫽ 具(r)典Vr.

(12.3.7)

The main advantage behind assumption (12.3.7) lies in the expression of effective strains ˜ r as a function of the applied strain by means of the global strain concentration Ar: ˜ r ⫽ Ar:, r(r ⫽ 1, . . . , n),

(12.3.8)

which are determined by appropriate explicit or implicit linear mean ﬁeld theories (see Chapter 7), which give the n concentration tensors in terms of the stiffness tensors Lr of each phase for explicit schemes and the overall stiffness L for implicit schemes. That is Ar ⫽ Ar(L, Lr, s ⫽ 1, . . . , n).

(12.3.9)

Finally, since Lr depends on the corresponding effective strain ˜ r through Eq. (12.3.4), Eq. (12.3.8) together with expression (12.3.9) provide n nonlinear equations, whose solutions determine the overall nonlinear property L by means of the constitutive equation (12.3.6). As noticed before, such a scheme requires in general iterative procedure and suitable convergence criteria. Note that through the deﬁnition of a linear comparison composite, upper and lower bounds of the effective properties L can be found using the linear variational principles presented in Chapter 6.

334

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

The classical secant method can be illustrated in case of two-phase materials. In fact, combination of 具(r)典V ⫽ , ˜ 1 ⫽ A1:,

(12.3.10) ˜ 2 ⫽ A2:

leads to c1A1 ⫹ c2 A2 ⫽ I.

(12.3.11)

In addition, from the constitutive law of each constituent, we have 1 ⫽ L1:˜1,

2 ⫽ L2:˜2,

(12.3.12)

and ⫽ c11 ⫹ c22.

(12.3.13)

L ⫽ c1L1:A1 ⫹ c2L2:A2.

(12.3.14)

Equation (12.3.10) gives

Then substituting (12.3.11) in (12.3.14) yields A1 ⫽ A2 ⫽

1 (L ⫺ L2)⫺1(L ⫺ L2), c1 1

(12.3.15)

1 (L ⫺ L1)⫺1(L ⫺ L1). c2 2

Therefore, when the linear homogenization model is identiﬁed to obtain the effective stiffness as L ⫽ L(c1, L1, L2),

(12.3.16)

the solution to the nonlinear problem is given by the following set of equations:

12.3

THE SECANT APPROACH

˜ 1 ⫽

1 (L ⫺ L2)⫺1(L ⫺ L2):, c1 1

˜ 2 ⫽

1 (L ⫺ L1)⫺1(L ⫺ L1):, c2 2

L1 ⫽ L1sec(˜1),

335

(12.3.17)

L2 ⫽ L2sec(˜2)

When the two phases are isotropic, (1) d (2) d L1(˜1) ⫽ 3K1Ih ⫹ 21sec(˜eq )I and L2(2) ⫽ 3K2Ih ⫹ 22sec(˜eq )I ,

(12.3.18) and the linear comparison composite displays an overall isotropy such that L() ⫽ 3KIh ⫹ 2(eq)Id,

(12.3.19)

where the linear homogenization scheme gives K ⫽ K(K1, K2, 1, 2, c1),

⫽ (K1, K2, 1, 2, c1).

(12.3.20)

The set of nonlinear equations (12.3.17) is reduced to (1) ˜ (1) m ⫽ Am m,

(2) (2) ˜ m ⫽ Am m,

(1) (1) ˜ eq ⫽ Aeq eq,

(2) (2) ˜ eq ⫽ Aeq eq,

Am(1) ⫽

1 K ⫺ K2 , c1 K1 ⫺ K2

(1) Aeq ⫽

1 ⫺ 2 , c1 1 ⫺ 2

Am(2) ⫽

1 K ⫺ K1 , c2 K2 ⫺ K1

(2) Aeq ⫽

1 ⫺ 1 , c2 2 ⫺ 1

1 ⫽ sec (1) 1 (˜ eq ),

(12.3.21)

2 ⫽ sec (2) 2 (˜ eq ).

Further, if the materials are incompressible, the linear homogenization model gives ⫽ (1, 2, c1),

and the nonlinear set of equations become

(12.3.22)

336

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

(1) ˜ (1) eq ⫽ Aeq eq,

A(1) eq ⫽

1 ⫺ 2 , c1 1 ⫺ 2

(1) 1 ⫽ 1sec(˜eq ),

(2) (2) ˜ eq ⫽ Aeq eq, (2) Aeq ⫽

1 ⫺ 1 , c2 2 ⫺ 1

(12.3.23)

2 ⫽ sec (2) 2 (˜ eq ).

As discussed above, when the appropriate linear homogenization scheme is chosen, the classical method becomes relatively easy to implement through an iterative algorithm. A few examples are treated as problems at the end of this chapter. Modiﬁed Secant Method

The classical secant method for describing the nonlinear behavior of composite materials assumes basically homogeneous strain ﬁeld within each phase and therefore neglects any intraphase ﬂuctuations of local ﬁelds. This results in few discrepancies and limitations, which was behind the principal motivations in developing the modiﬁed secant approach. Let us ﬁrst recall the basis of the classical secant method, which leads to a certain number of inconsistencies. As shown above, the classical method derives the average stress r over a phase r (r ⫽ 1, . . . , n) as r ⫽ Lr:r ⫽ Lrsec(r):r,

(12.3.24)

which implies the existence of a phase strain energy potential (r)( (r)) determined with respect to the average strain r, such that r ⫽

⭸r(r) . ⭸r

(12.3.25)

In the case of incompressible materials, (12.1.24) reads

(r) eq

where

(r) ⭸(r) eq ( eq ) ⫽ , (r) ⭸ eq

(12.3.26)

(r) eq ⫽

冋

冕

1 Vr

Vr

册

(r) dV

(r) eq ⫽

,

eq

12.3

THE SECANT APPROACH

冋

冕 (r) dV册 .

1 Vr

V

337

(12.3.27)

eq

One can also deﬁne the following equivalent average strain as (r) eq ⫽

1 Vr

冕

Vr

eq(r) dV.

(12.3.28)

The ﬁrst discrepancy of the classical method results from the equalities (12.3.25) and (12.3.26), which are satisﬁed only if the strain ﬁeld is homogeneous in each phase. Or, in general, the nonlinear behavior leads to highly intraphase ﬂuctuations, and as a result one can show that r ⫽

1 Vr

冕

Vr

(r) dV ⫽

1 Vr

冕

Vr

⭸r() ⭸ ( ) dV ⫽ r r , ⭸ ⭸r

(12.3.29)

or in the case of incompressible materials (r) eq ⫽

(r) ⭸(r) eq ( eq ) . ⭸ (r) eq

(12.3.30)

The result (12.3.30) is shown in the following. In fact, one has

冕 (r) dV册 ⫽ 冋V1 冕 ⭸ ( ) ⭸ () 1 ⫽ 冕 dV册 V ⭸ ⭸

(r) eq ⫽

冋

1 Vr

Vr

eq

(r) eq

r

Vr

eq

r

Vr

册

⭸r() dV ⭸

eq

eq

(12.3.31)

eq

eq

which leads to (r) eq ⫽

冋

1 Vr

冕

Vr

册

⭸(r) eq (eq) 2e() dV ⭸eq 3eq

.

(12.3.32)

eq

On the other hand, the convexity of the function e:e leads to the following inequality:

338

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

(r) eq ⫽

冋

1 Vr

冕

Vr

册

⭸(r) eq (eq) 2e() dV ⭸eq 3eq

ⱕ

eq

1 Vr

冕

Vr

⭸(r) eq (eq) dV. ⭸eq

(12.3.33)

Since for most nonlinear composite the function [⭸ (r) eq (eq) / ⭸eq] is concave, one can easily show that 1 Vr

冕

Vr

(r) (r) ⭸(r) ⭸eq ( (r) ⭸eq ( (r) eq (eq) eq ) eq ) dV ⬍ ⫽ , ⭸eq ⭸eq ⭸eq

(12.3.34)

(r) where we further assume that (r) eq ⫽ eq . With (12.3.34), statement (12.3.30) is proved. Another limitation of the classical method results from the fact that the deﬁnition of the macroscopic properties does not necessarily rely on the deﬁnition of a macroscopic W (), so that

⫽

⭸W() . ⭸

(12.3.35)

In fact, it turned out that in some cases of nonlinear composite materials, the following property of the macroscopic potential of isotropic materials ⭸2W(eq, m) ⭸2W(eq, m) ⭸eq ⭸ ⫽ m⫽ ⫽ , ⭸eq ⭸m ⭸eq ⭸m ⭸eq ⭸m

(12.3.36)

is not fulﬁlled by the classical secant approach, see Problem 12.4. The modiﬁed secant method took its inspiration from the above statement. It was developed in accordance to the following. The ﬁrst step is the deﬁnition of the macroscopic potential from the Hill lemma: W() ⫽

1 V

冕 :L(r): dV ⫽ :L:,

(12.3.37)

V

and its derivative with respect to the stiffness Lr of the r phase in the linear comparison composite: ⭸W() ⭸L 1 ⫽ : (r) : ⫽ ⭸L(r) ⭸ L V ijkl ijkl

2 ⭸ 冕 :⭸⭸L(r) : dV ⫹ 冕 :L(r): L V ⭸L V

(r) ijkl

V

(r) ijkl

dV,

(12.3.38) where the local stiffness Lr(r) is assumed to be piecewise uniform:

12.3

THE SECANT APPROACH

冘 L ƒ (r),

339

n

Lr(r) ⫽

(12.3.39)

r r

r⫽1

where ƒr is the characteristic function deﬁned in (5.3.8). With (12.3.39), the ﬁrst term on the right-hand side of (12.3.38) yields 1 V

1 冕 :⭸⭸L(r) : dV ⫽ c 冕 L V V

r

(r) ijkl

r

Vr

ijkl dV ⫽ cr具ijkl典Vr,

(12.3.40)

while the second term writes 1 V

冕 :L(r):⭸⭸L V

(r) ijkl

dV ⫽

再

1 V

冕 (r) dV冎再: V1 冕 ⭸⭸L V

V

(r) ijkl

冎

dV ⫽ 0. (12.3.41)

To establish (12.3.41) we used the Hill lemma in accordance to the fact that the strain ﬁeld ⭸ / ⭸L(r) ijkl is kinematically admissible, so that

冕 ⭸⭸L V

(r) ijkl

dV ⫽ 0.

According to (12.3.40) and (12.3.41), (12.3.38) is reduced to 具ijkl典Vr ⫽

1 ⭸L : (r) :. cr ⭸Lijkl

(12.3.42)

The fourth-order tensor 具ijkl典Vr corresponds to the second-order moment of the strain ﬁeld over the r phase in the linear comparison composite material. It is calculated by (12.3.42) and therefore requires the deﬁnition of the linear homogenization scheme to express the macroscopic properties in terms of the local ones. The diagonal term 具:典Vr of the second-order moment can be adopted in the modiﬁed second method as an alternative way to measure the intraphase ﬂuctuation of the strain ﬁeld better than the classical method. This comes from the convexity of the function :: 具:典Vr ⱖ 具典Vr:具典Vr,

(12.3.43)

where the equal sign holds only if the strain ﬁeld is homogeneous.

340

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

In the case of isotropic materials, the second-order moment uses the equivalent strain such that ⭸L(r) 1 ⭸L 1 ⭸L ijkl d 2 : : ⫽ : (r) : ⫽ 2具ijkl典Vr I ijkl ⫽ 3( (r) eq ) , cr ⭸r cr ⭸Lijkl ⭸r

(12.3.44)

where (r) eq is given by (12.3.28). Finally, by adopting the second-order moment of strain, the modiﬁed secant method involves the following steps: • The identiﬁcation of the appropriate linear homogenization

scheme, which give the overall stiffness L as function of the phase stiffness L(r) ijkl in the linear comparison composite. Then the derivatives in (12.3.44) can be accomplished. • The resolution of the following n nonlinear set of equations (r) (r) L(r) ijkl ⫽ Lijkl( eq ),

(r) eq ⫽

冉

冊

1 ⭸L : : 3cr ⭸r

1/2

,

(12.3.45)

(r) which gives the n unknown secant tensors L(r) ijkl( eq ). As in the case of the classical method, the modiﬁed method requires simple iterative algorithm to derive the overall properties of the nonlinear composite. If the linear comparison composite has overall isotropy, one can easily show from (12.3.45) that

(r) eq

冋冉

1 1 ⭸K 2 ⭸ 2 ⫽ m ⫹ cr 3 ⭸r ⭸r eq

冊册

1/2

,

(12.3.46)

where K and are computed by a linear homogenization approach. Let us illustrate the method in the case of a two-phase isotropic composite material, where phase (1) is softer and dispersed in phase (2). Suppose that Hashin–Shtrikman lower bounds are appropriate to derive the overall properties of the linear composite. One has (see Example 6.2)

12.3

c1

K ⫽ K2 ⫹

1 K1 ⫺ K2

⫽ 2 ⫹

⫹

341

THE SECANT APPROACH

,

c2 K2 ⫹ –43 2

(12.3.47)

c1 , 1 6c2(K2 ⫹ 22)2 ⫹ 1 ⫺ 2 5(3K2 ⫹ 42)

from which one can derive explicit expressions for the second-order moment of strain required to compute the tensor of secant moduli in each phase. The results are (1) eq ⫽

1 ⫺ 2 , c1 1 ⫺ 2 eq

(2) 2 2 1/2 eq ⫽ (N m ⫹ M eq ) ,

(12.3.48)

with

冋

冉

冊

1 1 K ⫺ K2 N⫽ K ⫺ c1K1 3c22 c1 K1 ⫺ K2

2

冉

冊册

1 K ⫺ K1 ⫺ c2K2 c2 K2 ⫺ K1

2

,

(12.3.49) M⫽

冋

冉

冊

2

1 1 ⫺ 2 ⫺ c1 (1) c22 c1 1 ⫺ 2 2 12 1 ⫺ 2 1 ⫺ 2 ⫺ c1c2k2 5 c1 1 ⫺ 2 3K2 ⫹ 42

冉

冊冉

冊册 2

.

(12.3.50)

Concluding Remarks

In the classical and modiﬁed secant nonlinear extensions presented in the above, the phase distribution is the same in the LCC and in the nonlinear composite. As explained in previous sections, this results from the choice of a particular linearization scheme. This option is pertinent and does not lead to any ambiguity in the choice of the linear homogenization model used to describe the morphology of the LCC. However, another richer strategy can be used in which the homogeneous domain for the secant moduli tensors does not correspond to the domain occupied by the constitutive phases. For example, one could deﬁne LCCs with more phases than the nonlinear composite. One can

342

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

easily anticipate that this richer description of the local heterogeneity of the secant moduli will be closer to the real distribution of the moduli in the nonlinear composite. Hence, the prediction will be more suited. However, the evaluation of a large number of internal variables, the critical choice of a linear model, and the difﬁculty related to the larger number of considered phases complicate the use of this approach. There is a conﬁguration where this description can be naturally called upon, at least theoretically; when the phase distribution of the nonlinear composite can be appropriately described with morphological patterns. Let us consider the simple case of Hashin’s composite spheres assembly. In this case, the linear isotropic behavior of the microstructure can be well described with a three-phase self-consistent scheme based on the analytical solution of the problem of a composite inclusion embedded in an inﬁnite medium. PROBLEMS

12.1 Show that (1/m)Ltg is a secant modulus for power law materials deﬁned by constitutive equations (12.1.18), where Ltg is the tensor of tangent moduli given by (12.1.26). 12.2 Show equation (12.2.15). 12.3 Consider a two-phase composite material made of two power law isotropic materials. The two phases obey constitutive relations (12.1.8). They have the same components n and m, the same reference strain 0, but differ by their ﬂow stress denoted by (2) (1) 0 for phase (1) and 0 for phase (2). By combining the nonlinear problem (12.3.23) with a lower bound Hashin–Shtrikman type of estimation of the effective shear modulus , the average strain distribution in each phase does not depend on the volume fractions of the constituents, so that (1) eq ⫽ (2) eq

1 , 2 1 1⫹ ⫺1 5 2

冉

冊

with

冉 冊

(1) 1 0(1) eq ⫽ (2) (2) 2 0 eq

m⫺1

When phase (1) is rigid show from the average condition (2) c1 (1) eq ⫹ c2 eq ⫽ eq

the following results:

.

343

PROBLEMS

(1) lim eq ⫽ 0,

(2) lim eq ⫽

(1) 0→⫹⬁

0(1) →⫹⬁

eq

c2

,

(1) m 5 (2) (2) m lim (1) 0 ( eq ) ⫽ – 2 0 ( eq ) .

(1) 0→⫹⬁

From the deﬁnition of the overall stress deviator s s ⫽ c1s1 ⫹ c2s2 and the constitutive equations of each phase

冉 冊

2 (1) (1) eq s1 ⫽ lim 0 (1) 0 0→⫹⬁ 3

m

e1

冉 冊

(2) 2 (2) eq s2 ⫽ lim 0 0 0(1) →⫹⬁ 3

,

(1) eq

m

e2 (2) eq

show that the overall constitutive equation reads s⫽

冉冊

2 0 eq 3 0 0

m⫺1

e,

with 0 ⫽ 0(2)

(1 ⫹ –23 c1) . (c2)m

12.4 Consider the above problem when the inclusions [phase (1)] are voids. Show that the effective properties of the linear comparison composite are given by K⫽

4 c2 , 3 c1 2

⫽ 2

冉

冊

c2 1 ⫹ –32 c1

and the solution of the nonlinear problem is reduced to (2) eq ⫽

eq . 1 ⫹ –23 c1

Express the overall constitutive laws for the spherical and deviatoric parts and show that the following condition ⭸2W(eq, m) ⭸2W(eq, m) ⭸eq ⭸ ⫽ m⫽ ⫽ ⭸eq ⭸m ⭸eq ⭸m ⭸eq ⭸m

is not satisﬁed.

344

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

12.5 Consider Problem 12.4 when both phases are rigid plastic (m ⫽ 0) and show that the nonlinear problem is reduced to the following relations: (1) 5 eq ⫽ (2) eq 3

冉

(1) eq ⫽0 (2) eq

冊

1⫺

2 (1) 0 5 0(2)

if

(1) 5 0 ⱕ . (2) 0 2

if

0(1) 5 ⱕ , 0(2) 2

If we denote by 0 the ﬂow stress of the rigid plastic composite, show that (2) 0 ⫽ c1 (1) 0 ⫹ c2 0

3 0 ⫽ (2) 0 (1 ⫹ – 2 c1)

if if

(1) 5 0 ⱕ , (2) 0 2 0(1) 5 ⬎ . 0(2) 2

12.6 Consider Problem 12.3 and apply the modiﬁed secant method for what follows. Show Eqs. (12.3.48)–(12.3.50). Show that the linear problem deﬁned by Eq. (12.3.45) is reduced to

(1) eq (2) eq

⫽

⭸ c2 ⭸1 c1 ⭸ ⭸2

冢 冣

1/2

,

with

冉 冊

(1) eq 1 (1) ⫽ 0(2) (2) 2 0 eq

m⫺1

with a lower bound Hashin–Shtrikman estimation of , show that (1) eq ⫽ (2) eq

再冋 冉

2 1 1⫹ ⫺1 5 2

冊册

2

冉

6 ⫹ c1 1 ⫺ 1 25 2

冊冎 2

1/2

.

Show that the ﬂow stress of the composite with rigid inclusions is expressed by 0 ⫽ (2) 0

(1 ⫹ –32 c1)m⫹1 / 2 . (c2)m

SUGGESTED READINGS

345

12.7 Consider Problem 12.4 and show that the nonlinear problem using the modiﬁed method writes

(2) eq

冋

4 2 1 ⫽ m ⫹ ( )2 9c1 1 ⫹ –23 c1 eq

册

1/2

.

Rewrite the overall constitutive laws for the spherical and deviatoric parts and check the following equality: ⭸2W(eq, m) ⭸2W(eq, m) ⭸eq ⭸ ⫽ m⫽ ⫽ ⭸eq ⭸m ⭸eq ⭸m ⭸eq ⭸m

SUGGESTED READINGS Castan˜eda, P. (1991). The Effective Mechanical Properties of Nonlinear Isotropic Composites Materials, J. Mech. Phys. Solids, Vol. 39, pp. 45–71. Castan˜eda, P. (1992). New Variational Principles in Plasticity and Their Applications to Composite Materials, J. Mech. Phys. Solids, Vol. 40, pp. 1757–1788. Castan˜eda, P. (1996). Exact Second-Order Estimates for the Effective Mechanical Properties of Nonlinear Isotropic Composite Materials, J. Mech. Phys. Solids, Vol. 44, pp. 827–862. Castan˜eda, P. and P. Suquet. (1995). On the Effective Mechanical Behavior of Weakly Inhomogenous Nonlinear Materials, Eur. J. Mech. A/Solids, Vol. 14, pp. 205–236. Castan˜eda, P. and J. R. Willis. (1988). On the Overall Properties of Nonlinearly Viscous Composites, Proc. R. Soc. Lond. A, Vol. 416, pp. 217– 244. Castan˜eda, P. and M. Zaidman. (1994). Constitutive Models for Porous Materials with Evolving Microstructure, J. Mech. Phys. Solids, Vol. 42, pp. 1459–1497. Gilormini, P. (1995). A Shortcoming of the Classical Nonlinear Extension of the Self Consistent Model, C. R. Acad. Sci. Paris, Se´rie IIb, Vol. 320, pp. 115–122. Hutchinson, J. W. (1976). Bounds and Self-Consistent Estimates for Creep of Polycrystalline Materials, Proc. R. Soc. Lond., Vol. A 348, pp. 101–127. Michel, J. C. and P. Suquet. (1992). The Constitutive Law of Nonlinear Viscous and Porous Material, J. Mech. Phys. Solids, Vol. 40, pp. 783–812.

346

NONLINEAR PROPERTIES OF COMPOSITES MATERIALS

Suquet, P. (1993). Overall Potentials and Extremal Surfaces of Power Law or Ideally Plastic Composites, J. Mech. Phys. Solids Struct., Vol. 41, pp. 981– 1002. Suquet, P. and P. Castan˜eda. (1993). Small-Contrast Perturbation Expansions for the Effective Properties of Nonlinear Composites, C.R. Accad. Sci. Paris, Se´rie II, Vol. 317, pp. 1515–1522. Qiu, Y. P. and G. G. Weng. (1992). A Theory of Plasticity for Porous Materials and Particle-Reinforced Composites, J. Appl. Mech., Vol. 59, pp. 261–268.

13 MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS Martensitic transformation in solids has received considerable attention in recent years because of its broad potential applications. Such phase change can be induced by the application of stress as well as by temperature change. The original interest in martensitic phase transformation came from the special mechanical properties of the transformation product, namely the strength of martensite and the corresponding thermomechanical treatments to produce adequate behavior for engineering applications. Various strain mechanisms enter the behavior of such materials. Most of them are ductile materials, and, therefore, in addition to the plastic ﬂow, a microstructure evolution accompanying the phase change leads to complex strain mechanisms ensuring basically the coexistence of the two phases. These strain mechanisms result from an accommodation process, which enhances ductility at a particular strength level by means of ‘‘transformation induced plasticity,’’ known as the TRIP effect. The classical deﬁnition given to this phenomenon corresponds to the irreversible strain observed even if the specimen is loaded by a stress state less than the yield stress of the softer phase. In such materials, the overall behavior depends strongly on the temperature since the martensitic phase transformation kinetics is related with temperature through the so-called chemical energy. Furthermore, since martensitic phase transformation occurs without diffusion through a cooperative shear movement of atoms, it is recognized that the applied as well as the internal stresses assist the transformation. The role of plastic strain on the progress of martensitic transformation is much Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

347

348

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

Stress

more complicated. Martensitic phase transformation occurs on cooling without applied stress at Ms temperature. Above Ms, the critical stress to undergo martensitic phase transformation increases linearly with temperature up to the Ms temperature deﬁned as the maximum temperature at which martensitic transformation occurs by elastic stress. In this temperature range, martensitic transformation is deﬁned as the stress-assisted transformation. At temperatures above Ms , signiﬁcant plastic ﬂow precedes the transformation, and an additional contribution to transformation arises from the production of new nucleation sites by plastic deformation. In this temperature regime where the transformation critical stress decreases signiﬁcantly, the phase change is deﬁned as the plastic-strain-induced transformation. The temperature dependence of the critical stress for causing martensitic transformation is schematically represented in Figure 13.1 where the Md temperature is introduced to reﬂect the stability of austenitic phase. From a micromechanics point of view, materials with phase transformation can be considered as two-phase composite materials where the ‘‘reinforcement’’ phase evolves. In addition to the usual thermoelastic properties, which may be assumed homogenous for most of these materials, the inelastic behavior of austenite–martensite twophase material appears strongly heterogeneous. According to the diversity of active mechanisms and the evolving microstructure, various coupling have to be described. From a kinematical point of view, a volume element experiences a plastic strain in its austenitic state, followed by the instantaneous transformation strain according to discrete

Strain-Induced Transformation

Stress-Assisted Transformation Ms

M σs

Temperature

Yield Stress of Austenite

Md

Figure 13.1 Schematic representation of critical stress for martensitic transformation as function of temperature.

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

349

values of the possible set of transformation strains and plastic ﬂow in the martensitic state. This phenomenon is also known as dynamic softening. Beside the chemical part of the free energy, the elastic part is due to applied stresses, as well as due to internal stresses generated by the incompatibilities of the total inelastic strain ﬁeld (plastic ⫹ transformation). These couplings render possible a good combination between ductility and strength in materials with phase transformation. In fact any tendency to increase ductility in conventional materials will decrease the strength. For example, a good combination between strength and ductility is a required property to design lightweight structures in automotive bodies and also to improve body safety. To reproduce the various features of materials exhibiting martensitic phase transformation is not a simple task. Since the problem has to be considered from a multiscale point of view taking into account the microstructure evolution accompanying martensitic transformation, only partial solutions have been developed during the last decades. Basically, modeling the behavior of such materials raises, naturally, the following problems: 1. To deﬁne adequate variables describing the microstructure evolution during the phase transformation. For example, the volume fraction ƒ of martensite or a set of volume fractions ƒI (I ⫽ 1, 2, . . .) may constitute an appropriate internal variable. If it is the case, the evolution law of this variable should be speciﬁed. It may be formally written as ƒ˙ ⫽ ( )˙ ⫹ ( )T˙ in terms of control variables, stress and temperature, for example. It should be noticed that any attempt to perform a systematic solution to this problem has to be accomplished through a thermodynamic study to derive energetic criteria for phase transformation. 2. To deﬁne the appropriate scale to describe the transformation strain or TRIP strain, accompanying the phase transformation. As this inelastic strain results from complex accommodation processes, which occur at the microscale, morphological considerations of the transformation product have to be taken into account. At this scale, the deﬁnition of the TRIP strain may leads to a set of transformation strains trI (I ⫽ 1, 2, . . .), which depends on the possible crystallographic orientations of martensite related to the concept of martensitic variants.

350

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

It may be possible to adopt a more macroscopic description by introducing a kind of metallurgical variable tr (,T) to deal with the TRIP strain. However, such a description may lead to a model with limited predictive capabilities. 3. To adopt an appropriate nonlinear homogenization scheme for a well-deﬁned representative volume element (RVE). The choice of an appropriate RVE is also conditioned per the choice of internal and metallurgical variables describing the microstructure evolution and the morphological aspects of the transformation. If the problem is described by the macroscopic variables ƒ and tr (,T), the RVE simply represents a two-phase austenite–martensite composite material. For such a case, simple isotropic secant approach (see Chapter 12) may be sufﬁcient to describe the overall behavior. However, a multivariant description of the transformation product may require the deﬁnition of various RVE. For example, an RVE representing a single crystal with a certain number of martensitic variants (different orientations), surrounded by an austenitic matrix, is required to approximate the stress and strain distribution in each phase. Another RVE can also be deﬁned to account for the polycrystalline structure of these materials. Complete descriptions of the above interrelated problems are still under investigation both experimentally and theoretically. In particular, reﬁned microstructural analyses are needed to understand various mechanisms at different scales. As the problem of multiscale modeling is still challenging for these materials, the reader will ﬁnd in this chapter an introduction to the different microscale mechanisms with certain guidance in terms of micromechanical modeling. We pay particular attention to the problem of coexistence of two phases and resulting discontinuities in terms of stress, strain, and mechanical properties. For such a purpose we describe in details the concept of energy momentum, originally introduced by Eshelby. We show how this framework can be adapted to derive energetic criteria for phase transformation at different scales.

13.1 PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

The elementary mechanism accompanying martensitic transformation lies in a nondiffusion process at the atomic level, which transforms the parent crystallographic lattice (austenite) into a new crystallographic lattice of the transformation product (martensite); see Figure 13.2. This

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

Z⬘

Z

冢

兹2a␣⬘

B ⫽ Y

a␥ 0 0

0 兹2a␣⬘ a␥ 0

351

0 0

冣

c␣⬘ a␥

a␥ ⫽ lattice parameter of austentite a␣⬘, c␣⬘ ⫽ lattice parameters of martensite X⬘

X

Y⬘

Figure 13.2 Bain strain resulting from lattice change during phase transformation.

solid–solid phase transformation results from purely geometrical features in a local lattice distortion called the Bain strain. The Bain strain B describing the geometrical transformation from austenite to martensite is incompatible in nature and therefore requires an accommodation procedure that, in general, affects the transformed regions. This accommodation step depends on the mechanical properties of the parent and product phases and leads to a typical length, shape, and spatial distribution of the product of phase transformation. The concept of the incompatibility accompanying the Bain strain means that the lattice change will generate elastic strain both in parent and product phases and, as a result, internal stresses. These stresses may be sufﬁcient to initiate relaxation mechanisms with certain diversity depending on the mechanical properties of the considered material, which are controlled by the chemical composition, thermomechanical processes, and other parameters. The relaxation mechanisms may be activated as follows: • Inelastic deformations by plastic shear or twinning in parent and

product phases • A typical resulting morphology of the transformed domains, which consists, in general, in a plate and lath shapes • Formation of autoaccommodating groups of martensite Indeed, a complete determination of such an accommodating step relies on a ﬁne description of the typical microstructure of the transformation product. Therefore, it could only be accomplished through

352

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

approximate ways leading to the crystallographic theories of martensitic transformation. One of the well-known theories is the method of Wechsler, Liebermann, and Read (1953), which describes the accommodation step by an inelastic strain preserving the parent phase lattice and leading to the concept of habit plane or interface between austenite and martensite. This theory is based on the concept of inelastic compatibility of a local transformation strain tr (r) assumed to be uniform within an elementary transformed volume VI. In other words, the methodology assumes a given morphology of the transformed region and deals with the compatibility conditions through two different ways: one is based on a concept of energy minimization using the elementary Eshelby’s inclusion, the other deals with the problem of stress and strain discontinuities across the interface SI of the considered domain, where the compatibility conditions rely on the coherency of this interface. Eshelby’s Inclusion Method

Through the basic concept of Eshelby’s inclusion problem, the transformed domain VI is assumed to be ellipsoidal in shape and experiences an eigenstrain corresponding to the lattice distortion described by the Bain strain B. If we denote by L the elastic stiffness tensor of the inﬁnite medium and by V its volume, the free energy density reads W⫽

1 VI B ⬊L⬊(I ⫺ SI)⬊B, 2 V

(13.1.1)

where SI is the Eshelby tensor. If the lattice change do not generate any elastic deformation and therefore any increase of the elastic free energy, the compatibility conditions should fulﬁll the following eigenvalue problem: (I ⫺ SI)⬊B ⫽ 0.

(13.1.2)

In general, with the purely geometric lattice change described by B, Eq. (13.1.2) has no solution. Therefore, an additional inelastic mechanism is required to satisfy the eigenvalue problem raised by (13.1.2). One of the accommodation mechanisms corresponds to a plastic shear or twinning within the transformed domain by preserving its crystallographic lattice; see Figure 13.3. The resulting strain is called ‘‘lattice

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

B

P

353

R

Habit Plane

Figure 13.3 Schematic representation of the accommodation process by twinning or slip in martensite by lattice invariant strain (B, Bain strain; P, plastic deformation or twinning; R, rotation).

invariant strain’’ and denoted here by inv. From this analysis, the transformation strain tr ⫽ B ⫹ inv is compatible so that the conditions (I ⫺ SI)⬊tr ⫽ 0

(13.1.3)

det(tr) ⫽ 0 (determinant).

(13.1.4)

is satisﬁed if

Therefore, a complete determination of tr from (13.1.4) can be performed following the next steps: 1. Plastic shear or twinning is assumed to occur along a slip system of the transformed region with a magnitude ␥ so that the lattice invariant strain reads inv ⫽ ␥R,

(13.1.5)

where R deﬁnes the orientation tensor of the slip or twin system deﬁned by its unit normal n˜ and shear direction m ˜ as Rij ⫽ –12 (m ˜ in˜ j ⫹ m ˜ jn˜ i).

(13.1.6)

2. The second step deﬁnes an interface called the habit plane between the two phases, so that the transformation strain is considered to be predominately shear along this plane. That is trij ⫽ –21 g(minj ⫹ mj ni),

(13.1.7)

354

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

where m is the shear direction and n the unit normal to the habit plane; g is the magnitude of the shear. As stated above, the accommodation process occurs mainly by shear, however, when phase transformation is accompanied by substantial plastic ﬂow, a volumic component is measured, which ranges from 1 to 4%. In other words, the two vectors m and n are not necessarily perpendicular (Fig. 13.4). From Eq. (13.1.7) and for a given B and R, the compatibility equations (13.1.3) and (13.1.4) determine g and the vectors m and n. This ends the second step; see Problem 13.1. Method Using Jump Conditions

For this analysis, the compatibility conditions lie in the deﬁnition of a coherent interface or habit plane SI between the parent and product phases with n being the unit normal of the surface. This hypothesis corresponds to the continuity of displacement ([u] ⫽ 0) and/or velocity ([v] ⫽ 0) ﬁelds as well as the stress vector ([] n ⫽ 0), where [x] ⫽ x⫹ ⫺ x⫺ denotes the jump of x across the interface. In the present case, the ‘‘positive’’ side belongs to the parent phase (austenite), whereas the ‘‘negative’’ one corresponds to the transformed regions (martensite). It is interesting to note that, in the case of shape memory alloys where the transformation occurs mainly without a plastic deformation and under speciﬁc conditions, the analysis can also be adapted to martensite–martensite interfaces. The ﬁeld equations expressed at the interface can be reduced to the following compatibility conditions; see Problem 13.2:

→

gm

Martensite

→

n

→

m Austenite Habit Plane

Figure 13.4 Schematic representation of Eq. (13.1.7).

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

⫺ 1 [ij] ⫽ ⫹ ij ⫺ ij ⫽ – 2 (inj ⫹ j ni),

355

(13.1.8)

where the total strain at each side of the interface ⫹,⫺ ⫽ e⫹,e⫺ ⫹ tr⫹,tr⫺ consists of an elastic part e and a transformation contribution tr resulting from the accommodation process accompanying the phase change; is a vector to be determined. For simplicity, the behavior from each side of the interface is described by linear elastic constitutive law, such that ⫹,⫺ ⫽ L⫹,⫺⬊(⫹,⫺ ⫺ tr⫹,tr⫺).

(13.1.9)

If we further introduce a reference homogeneous elastic medium L such that L⫹,⫺ ⫽ L ⫹ (L⫹,⫺ ⫺ L) ⫽ L ⫹ ⌬ L⫹,⫺, Eq. (13.1.9) is equivalent to [] ⫽ L⬊[] ⫺ L⬊[tr] ⫹ [⌬ L⬊e],

(13.1.10)

or by taking into account the condition [] n ⫽ 0, it results that L⬊[]⬊n ⫽ L⬊[tr]⬊n ⫺ [⌬ L ⬊ e]⬊n.

(13.1.11)

Substituting (13.1.8) into (13.1.11) leads to the following equations whose resolution gives the components of the vector . That is ᑣikk ⫽ ℵi,

(13.1.12)

where ᑣik ⫽ Lijklnj nl and ℵi ⫽ Lijkl [trkl]nj ⫺ [⌬ Lijklkle ]nj. Clearly, Eq. (13.1.11) shows that a compatible phase transformation (e.g., e⫹,e⫺ ⫽ 0) requires heterogeneous transformation strain, for example, [tr] ⫽ 0. Therefore, it results from (13.1.11) that a compatible expression of the transformation strain reads [trij ] ⫽ [ij] ⫽ –21 (inj ⫹ j ni).

(13.1.13)

Direct applications of compatibility conditions (13.1.13) can be generated as follows:

356

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

1. The Bain strain described in Figure 13.2 from purely geometrical considerations does not fulﬁll (13.1.13). In fact, if from the austenitic side we state that tr⫹ ⫽ 0 and from the martensitic side tr⫺ ⫽ B, Eq. (13.1.13) gives [trij ] ⫽ ijB ⫽ –21 (inj ⫹ j ni).

(13.1.14)

2. The accommodation process described in the previous section, which relies on a slip or twinning in the transformed regions [see (13.1.5)], fulﬁlls the compatibility conditions (13.1.13), such that if one assumes that tr⫹ ⫽ 0 and tr ⫽ B ⫹inv, the compatibility conditions writes [trij ] ⫽ ⫺(ijB ⫹ ijinv) ⫽ –21 (inj ⫹ j ni),

(13.1.15)

which is equivalent to Eq. (13.1.7). More recently, mathematical-based approaches have been proposed to predict other compatible morphologies during phase transformation. For details, the reader could refer to the Suggested Readings at the end of this chapter.

Notion of Martensitic Variants

As discussed in previous sections, the accommodation process accompanying the lattice change during phase transformation leads to a typical morphology of the transformation product, which implicitly results in a heterogeneous transformation strain tr (r). In the previous analysis, we adopt an accommodation process through a shear or twinning by deﬁning a habit plane between austenite and martensite leading to expressions (13.1.7) and (13.1.15) of the transformation strain tr. From purely crystallographic considerations and due to high symmetries of the parent phase, 24 couples of n and m are possible to deﬁne a habit plane leading to the notion of martensitic variant. From this concept, each possible martensitic variant is described by its crystallographic orientation, morphology, and transformation strain, which are implicitly interrelated by the accommodation process of the lattice change.

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

357

Kinematics at Single-Crystal Level

The purpose of this section is to discuss the different strain mechanisms during phase transformation at the single-crystal level. This step is required to build micromechanical tools for the ﬁrst scale transition linking the appropriate features of transformed regions to constitutive equations of single crystals. At this level, the concept of martensitic variants is taken into account by assuming that the transformation strain is piecewise uniform within elementary transformed regions corresponding to the different martensitic variants, so that one can write

冘 N

(r) ⫽ tr

trI

I (r),

(13.1.16)

I⫽1

where I (r) are the Heaviside step functions for the different transformed domains or variants I and N their number. The transformation strain trI associated with a martensitic variant I is described by (13.1.7) as trij I ⫽ –12 g (miInjI ⫹ mjI niI) ⫽ gRijI ,

(13.1.17)

where RI is the orientation tensor of the variant I. For a single crystal (taken as an RVE) with volume V subjected at its external boundary ⭸V to a displacement ui ⫽ ij xj, and undergoing an inelastic strain ﬁeld tr (r) ⫹ p (r) within V, the total macroscopic strain is ⫽

1 V

冕 ( (r) ⫹ e

V

tr

(r) ⫹ p (r)] dV ⫽ 具e (r) ⫹ tr (r) ⫹ p (r)典. (13.1.18)

Note that the elastic strain ﬁeld e (r) arises from and the incompatibilities of the ﬁelds tr (r) and p (r), where p (r) denote the plastic strain ﬁeld. In general, it is difﬁcult to distinguish experimentally between the plastic contribution and the transformation one at the macroscopic level. However, in terms of modeling, we will be able to make this distinction if we adopt a crystallographic description of phase transformation.

358

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

For homogeneous elasticity with its elastic stiffness L, one obtains directly the elastic part e of as follows: ⫽ L⫺1⬊ ⫹ tp,

(13.1.19)

where ⫽ 具 (r)典, and tp ⫽ 具tr (r) ⫹ p (r)典 corresponds to the macroscopic inelastic strain arising from the phase transformation and the plastic ﬂow. At this stage, one can distinguish between two cases where the physical aspects of martensitic transformation change signiﬁcantly: 1. In the case of shape memory alloys, the plastic contribution is neglected and the transformation strain becomes

冕

1 tr (r) dV. (13.1.20) V V Due to typical properties of the strain ﬁeld tr (r), one can differenciate between two simpliﬁed forms for tr: • The microstructure of variants as well as the fact that tr (r) is piecewise uniform, this leads to tr ⫽

tr ⫽

1 V

冘冕

VI

I

trI dV ⫽

冘

trI

ƒI,

(13.1.21)

I

where trI are material constants, and ƒI are the internal variables subjected to the following constraints: 0ⱕ

冘 ƒ ⱕ 1,

0 ⱕ ƒI ⱕ 1.

I

(13.1.22)

I

• Since the transformation strain vanishes within the austenitic

phase, thus (13.1.21) can be written as tr ⫽

1 V

冕

VM

tr (r) dV ⫽

再

VM 1 V VM

冕

VM

冎

tr (r) dV

⫽ ƒ˜tr,

(13.1.23) where ƒ ⫽ 兺IƒI is the total volume fraction of martensite, and ˜ tr being the average transformation strain over the total volume VM of martensite, which is an unknown to be determined from solving the deformation problem.

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

359

2. The case of iron base alloys where the phase transformation is accompanied by substantial plastic ﬂow in the parent phase. In this case, it is more critical to distinguish at the macroscopic level between a macroscopic transformation strain [in the sense of Eq. (13.1.23)] and a macroscopic plastic strain. This basically results from the fact that the transformation part contains a plastic contribution resulting from the accommodation process discussed above. An incremental formulation with a multivariant description is more appropriate for this class of materials (see below).

Incremental Formulation: Concept of Moving Boundaries

In most heterogeneous materials, the mechanical properties may be assumed piecewise uniform at appropriate scales. These materials are made up of different phases and/or grains separated by interfaces called grain or phase boundaries. The interfaces are in general stationary with respect to particles and often considered as perfect, at least at low temperatures. This hypothesis corresponds to the continuity of displacement ([u] ⫽ 0) and/or velocity ([v] ⫽ 0) ﬁelds as well as the stress vector ([] n ⫽ 0). The continuity assumptions extended to equivalent forms for the volume lead to the usual localization and homogenization relations, from which the classical scale transition methods are developed. The overall behavior of the RVE is then deduced from the microstructure and the local behavior (basically the purpose of previous chapters). In various situations where inelastic strains result from discrete physical mechanisms such as twinning, martensitic transformation, or recrystallization, the previous hypotheses are no longer valid because of evolving microstructures or moving boundaries whose velocities are different from those of the particles. Consequently, the strain ﬁeld and/ or mechanical properties exhibit discontinuities across moving boundaries and therefore: • Additional terms in localization and homogenization relations have

to be introduced in the framework of local thermodynamics and micromechanics to account for the moving boundaries. • Driving forces, germination, and growing laws describing the evolving microstructure need to be determined. These are discussed next.

360

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

Kinematics of Evolving Microstructure

In materials undergoing martensitic phase transformation, the parent and product phases coexist with the same chemical composition but differ in their lattices, volumes, and shapes. As a result, a complex accommodation process (discussed in the previous section) occurs leading to a typical morphology of the transformation product with multiple interfaces S or boundaries within the transformed region itself, and with the parent phase. During a loading increment (stress or temperature), two scenarios are possible: • The material experiences phase transformation with a complex

movement of interfaces between parent and product phases. • Under particular conditions, reorganization of preexisting trans-

formed regions is possible by a typical movement of interfaces within these regions. For example, it is interesting to link, from kinematics purpose, the macroscopic strain increment ˙ acting on the boundary of an RVE to the velocity ﬁeld. The velocity v of particles belonging to the external boundary of the RVE is assumed as d ij i ⫽ ˙ ij xj ⫽ x. dt j

(13.1.24)

From the deﬁnition of macroscopic strain ij ⫽

1 V

冕 V

ij

(r) dV.

The strain increment is given by ˙ ij ⫽

冉 冊冕

d 1 dt V

V

ij (r) dV ⫹

1 ⭸ V ⭸t

冋冕

V

册

ij (r) dV .

(13.1.25)

By neglecting the change in volume V of the RVE, (13.1.25) is reduced to

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

˙ ij ⫽

1 ⭸ V ⭸t

冋冕

册

ij (r) dV .

V

361

(13.1.26)

The strain ﬁeld is discontinuous along the different moving interfaces, the time derivative in (13.1.26) reads ˙ ij ⫽

1 V

冕 ⭸⭸t(r) dV ⫺ V1 冕 [

˙ ij ⫽

1 V

冕 冋⭸⭸t(r) ⫺ [

ij

V

ij

S

(r)]w␣ n␣ dS,

(13.1.27)

or ij

ij

V

册

(r)] w␣ n␣␦(S) dV,

(13.1.28)

where ␦(S) ⫽ 兰S ␦(r ⫺ r⬘) dS⬘ is the Dirac delta function. [] ⫽ ⫹ ⫺ ⫺ is the jump of the local strain ﬁeld; w is the velocity of the interface at a material point, where the outward unit normal to the interface is denoted by n; and w␣n␣ is a scalar describing the normal velocity of the interface. Applications

For example, the time derivative of (13.1.20) shows different mechanisms associated with martensitic transformation in shape memory alloys, which are not revealed through a simple ‘‘static’’ comparison between the actual conﬁguration and the reference one (austenite). By taking into account the discontinuities [tr (r)] ⫽ tr⫹ ⫺ tr⫺ of the strain ﬁeld tr (r) along the moving boundaries, one has ˙ tr ⫽

1 V

冕 ˙

tr

V

1 V

(r) dV ⫺

冕 [

tr

S

(r)]w␣ n␣ dS,

(13.1.29)

and since the concept of stress-free or eigenstrain is adopted for the transformation strain, so that ˙ tr (r) ⫽ 0. It then follows that ˙ tr ⫽ ⫺

1 V

冕 [

tr

S

(r)]w␣ n␣ dS,

(13.1.30)

362

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

where S represents all of the moving boundaries (austenite–martensite as well as boundaries between the martensitic variants), and ␣ n␣ is the normal velocity of the interface. The ‘‘crystalline’’ description of the martensitic transformation (analogous to crystal plasticity) comes directly from (13.1.30); see Problem 13.3: ˙ tr ⫽

冘

trI

ƒ˙ I,

(13.1.31)

I

where in (13.1.31) the distinction between transformation and exchange between existing variants is not explicitly shown. The different mechanisms are more explicitly described when one expands the time derivative of (13.1.23): ˙ tr ⫹ ƒ˜˙ tr. ˙ tr ⫽ ƒ˜

(13.1.32)

In fact, the analysis of (13.1.32) allows us to distinguish the following phenomena: • Transformation (ƒ˙ ⫽ 0) without deformation (˜ tr ⫽ 0, ˙˜ tr ⫽ 0). • Transformation (ƒ˙ ⫽ 0) with deformation (˜ tr ⫽ 0) but without

reorientation (˙˜ tr ⫽ 0). • Deformation by reorientation (˜˙ tr ⫽ 0) without transformation (ƒ˙ ⫽ 0). • Transformation, deformation, and reorientation ( ƒ˙ ⫽ 0, ˜ tr ⫽ 0, ˜˙ tr ⫽ 0).

In the case of iron-based alloys, the average inelastic strain of the single crystal is given by tp ⫽

1 V

冕 [

tr

V

(r) ⫹ p (r)] dV,

(13.1.33)

where p(r) describes simultaneously the plastic strain of an elementary volume element at austenitic and martensitic states. When the plastic ﬂow becomes signiﬁcant during phase transformation, the reorientation and inverse transformation mechanisms can be disregarded. The pro-

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

363

gression of the transformation can be described by the instantaneous growth of new plates or laths in the austenitic phase. The time derivative of (13.1.33) leads to ˙ tp ⫽

1 V

冕 ˙

tp

V

1 V

(r) dV ⫺

冕 [

tp

S

(r)]w␣ n␣ dS.

(13.1.34)

The volume integral in (13.1.34) describes the plastic ﬂow in residual austenite and preexisting martensitic variants, it could be written as the following form involving the average plastic strain rate ˙ pA in austenite and the average one over a martensitic variant. That is 1 V

冕 ˙

tp

V

(r) dV ⫽ (1 ⫺ ƒ)˙ pA ⫹

冘 ƒ ˙

I MI

.

(13.1.35)

I

The surface integral is much more complicated. It requires the determination of the inelastic strain jump at each point of the moving interface, which can be expressed as [tp (r)] ⫽ p⫹ ⫺ (p⫺ ⫹ trI) ⬇ ⫺trI.

(13.1.36)

Such a jump may be assumed to result only from the accommodation process leading to the deﬁnition of compatible transformation strain trI. However, as can be seen from (13.1.36), a heterogeneous plastic strain p⫹,⫺ ⫽ 0 may occur during the phase transformation. Its determination is not a simple task and may require complex numerical calculations. Since the transformation strain trI contains a plastic contribution corresponding to lattice invariant strain, the contribution of p⫹,⫺ can be neglected. Therefore, the surface integral reads ⫺

1 V

冕 [

tp

S

(r)]w␣ n␣ dS ⫽

冘

trI

ƒ˙ I.

(13.1.37)

I

Substituting (13.1.35) and (13.1.37) into (13.1.34) yields ˙ tp ⫽ (1 ⫺ ƒ)˙ pA ⫹

冘 ƒ ˙ ⫹ 冘 I

I

MI

trI

ƒ˙ I.

I

In (13.1.38) one can distinguish the following contributions:

(13.1.38)

364

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

• The ﬁrst term describes the average plastic ﬂow in the residual

austenitic phase. • The second term corresponds to the plastic ﬂow in the preexisting martensitic phase. • The last term expresses the formation of new plates or laths. At the single-crystal level, the plastic ﬂow of residual austenite may be described through the crystallographic slip by introducing the slip systems of FCC lattices. The plastic strain increment is then expressed by (see Chapter 11) ˙ pA ⫽

冘 P ␥˙ , g

g

(13.1.39)

g

where Pg is the Schmidt tensor and ␥˙ g the shear rate on slip system g. However, it is more difﬁcult to track the crystallographic slip in martensitic variants. This is due to the large number of variables (24 ⫻ 24 variables, 24 possible variants, for each 24 possible slip system). Due to the typical ﬁne microstructure of the transformation product and their typical crystallographic orientation, the plastic deformation of martensite may have no signiﬁcant contribution to the overall ﬂow of the RVE. This statement is also supported by the fact that martensite is a hard phase. Equation (13.1.38) is then reduced to ˙ tp ⫽ (1 ⫺ ƒ)

冘 P ␥˙ ⫹ 冘 g

g

g

trI

ƒ˙ I.

(13.1.40)

I

Equation (13.1.40) contains a classical crystal plasticity problem with internal variables, namely the volume fraction of each possible martensitic variant. To come out with a constitutive law of the RVE representing the single crystal, evolution laws of these internal variables have to be speciﬁed. In general, this step requires additional approximations and can be accomplished through two different ways: 1. To establish a thermodynamic framework to obtain the driving forces for the activation of the internal variables. This method is more appropriate to derive energetic criteria for the phase transformation. 2. To assume evolution laws based on experimental observations without any link with thermodynamics. This method does not require the determination of driving forces; however, its predictive capacities are limited.

13.1

PHASE TRANSFORMATION MECHANISMS AT DIFFERENT SCALES

365

In next sections we present an example displaying the ﬁrst methodology. This is possible by adopting the original work of Eshelby’s momentum tensor. Eshelby’s Energy Momentum Tensor

Eshelby introduced an important concept to deal with the conﬁguration of a solid. It corresponds to the energy momentum tensor, which is another way to combine the ﬁeld equations with energetic considerations. Let us consider a homogeneous material without any incompatibility in which the elastic energy density (r,) only depends on the elastic distortion . Therefore, we can perform the following: ,i (r,) ⫽

⭸ ⭸ ⭸jk ⫽ , ⭸xi ⭸jk ⭸xi

(13.1.41)

where the stress tensor reads jk ⫽

⭸ , ⭸jk

(13.1.42)

and jk ⫽ uj,k, and u is the displacement vector. From the equilibrium equation ik,k ⫽ 0, one can easily show that ,i (r,) ⫽ [jk (r)uj,i (r)],k.

(13.1.43)

Thus, (13.1.43) is equivalent to [(r,)␦ik ⫺ jk (r)uj,i (r)],k ⫽ 0.

(13.1.44)

Eshelby’s energy momentum tensor denoted here by ⍀ is expressed by ⍀ik ⫽ ␦ik ⫺ kjuj,i.

(13.1.45)

Therefore, the energy momentum tensor satisﬁes the following equation resulting from (13.1.44): ⍀ik,k ⫽ 0

13.1.46)

Let us consider now the case of martensitic transformation where the accommodation process leads to a nonhomogeneous transformation

366

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

strain ﬁeld tr (r) undergoing a jump [tr (r)] across an interface between the parent and product phases. Let us deﬁne the following local quantity Fi ⫽ [⍀ik]nk, which can be expressed from (13.1.45) as Fi ⫽ [␦ik ⫺ jkuj,i]nk ⫽ []ni ⫺ [jkuj,i]nk.

(13.1.47)

From the diagonal symmetries of the elastic constant L and the decomposition of the total distortion  into an elastic part e and a transformation contribution tr, one obtains for the jump of elastic energy (see Problem 13.4) [] ⫽ –12 (ij⫹ ⫹ ij⫺)]ije ].

(13.1.48)

On the other hand, the continuity of the traction vector, [] n ⫽ 0, leads to 1 ⫹ ⫺ [jkuj,i]nk ⫽ –21 (jk⫹ ⫹ ⫺ jk )[uj,i]nk ⫽ – 2 (jk ⫹ jk )[ji]nk.

(13.1.49)

Substituting (13.1.48) and (13.1.49) into (13.1.47), one has Fi ⫽ –21 (jk⫹ ⫹ jk⫺){[jke ]ni ⫺ [ji]nk},

(13.1.50)

and by taking into account the compatibility equation (13.1.8), it results [ji]nk ⫽ [uj,i]nk ⫽ j nink ⫽ j nkni ⫽ [jk]ni.

(13.1.51)

Finally with (13.1.51), it follows that Fi ⫽ [⍀ik]nk ⫽ –21 (jk⫹ ⫹ jk⫺)[jktr ]ni.

(13.1.52)

If one follows a complete thermodynamic study—see Cherkaoui et al. (1998)—one can show that the scalar F ⫽ Fiwi

(13.1.53)

is the mechanical driving force if one considers the normal velocity of the interface w␣n␣ as the internal variable describing the microstructure evolution. This variable is, in general, not appropriate to derive constitutive equations of materials with evolving microstructure. It requires time-consuming and complex computational tools. By means of addi-

13.2.

APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS

367

tional hypotheses taking into account the typical morphology of martensite, an alternative description is possible. It could be considered as another scale of description, which adopts the volume fractions of martensite as internal variables. 13.2 APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS FOR SINGLE CRYSTALS Thermodynamic Driving Forces

Recently, Cherkaoui et al. (1998) extended Eshelby’s (1970) pioneering work on the energy momentum tensor to derive the thermodynamic driving force acting on a moving boundary point between the product and the parent phases. That is F ⫽ ⫺–12 (⫹ ⫹ ⫺)⬊[tp] ⫹ [],

(13.2.1)

where [tp] and [] denote the jumps of the inelastic strain and the chemical energy, respectively; ⫹ and ⫺ correspond to the limiting values of the local stress ﬁeld for each side of the moving interface, which can be linked with the help of interface operators Q(L, n), ⫹ ⫽ ⫺ ⫺ Q(L, n) ⬊ [tp],

(13.2.2)

depending on the unit normal to interface and elastic constant of the material. With (13.2.2), (13.2.1) can be rewritten as F ⫽ [–12 Q(L, n) ⫺ ⫺]⬊[tp] ⫹ [].

(13.2.3)

As noticed above, the introduction of (13.2.3) as a thermodynamic driving force assumes that the interface normal velocity is taken as the internal variable characterizing the phase transition. It is also noticed that equation (13.2.3) requires the determination of the local stress and strain ﬁelds in each point of the moving interface. Therefore, the determination of (13.2.3) for any topology of the interface could be obtained only through strong numerical calculations. To go a step further in the scale transition, an alternative relation of (13.2.3) is obtained by introducing the concept of an ellipsoidal growing. The former hypothesis assumes that the moving interface represents an ellipsoidal growing domain. This is in accord with the microstructure developed during

368

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

martensitic transformation corresponding to the formation of microdomains of a typical morphology of plate or lath. Furthermore, as we discussed in the previous kinematic study, the martensitic transformation progresses by the nucleation and instantaneous growth of new domains. This is related to a high interface velocity between the parent and product phases, leading consequently to the following expression for the local jump [tp] of the inelastic strain [tp]I ⫽ p⫹ ⫺ (p⫺ ⫹ trI) ⫽ ⫺trI.

(13.2.4)

In other words, the instantaneous growth of a martensitic domain allows the continuity of the plastic strain over its boundary. In connection with (13.1.40), it implies that the volume fractions ƒI of each possible martensitic variant are the internal variables characterizing the phase transition at the mesoscale, the integration of (13.2.3) along the ellipsoidal domain interface, and thanks to (13.2.4) one obtains the driving force FI for the ‘‘ﬂow’’ ƒ˙ I of a martensitic variant due to the formation of a new domain. That is, S˙ I FI ⫽ ⫺⬊trI ⫺ B(T ⫺ T 0) ⫹ –21 trI⬊L⬊(I ⫺ SI)⬊trI ⫹ –12 trI ⬊L⬊ ˙ I⬊trI ƒI, ƒ (13.2.5) where I is the identity tensor and SI is Eshelby’s tensor depending on the aspect ratio as well as on the orientation of the martensitic microdomain; S˙I corresponds to the variation of SI due to the ellipsoidal growth. For the sake of simplicity, a homothetic growth is assumed giving S˙I ⫽ 0. The term B(T ⫺ T 0) is a linear approximation of the chemical energy jump []. B is a material constant and T 0 the equilibrium temperature. It should be noticed that the derivation of (13.2.5) requires the hypothesis of a uniform stress ﬁeld ⫺ within the growing ellipsoidal domain. Details on the derivation of (13.2.5) as well as on the notion of ellipsoidal growing can be found in Cherkaoui et al. (1998). Equation (13.2.5) gives the thermodynamic driving force for nucleation and growth of martensitic microdomains belonging to different martensitic variants; it requires the knowledge of the stress ﬁeld inside the growing domains. In addition to the overall applied stress, this stress ﬁeld contains several contributions due to different couplings between plasticity and phase transformation at the microscale. In the

13.2.

APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS

369

following, several ways for the determination of internal stresses are discussed from a micromechanics point of view: 1. The simplest way is to neglect any source of internal stresses. In such conditions, Patel and Cohen (1953) have formulated the energy term resulting only from the interaction of applied stress with transformation strains. This corresponds in (13.2.5) to the term ⬊trI ⫺ B(T ⫺ T 0), where ⫺is assumed equal to the applied stress , and all the other contributions are neglected. 2. It is possible to assume an ellipsoidal growth of a martensitic microdomain inside a homogeneous stress ﬁeld corresponding to the average stress over the austenitic phase. At the current conﬁguration of the RVE, if we denote by pA the average plastic strain in the austenitic phase, the interactions between plasticity and martensitic phase transformation are taken into account through the average stress A in the austenitic phase; see Exercise Problem 13.5:

冘 ƒ L ⬊ (I ⫺ S ) ⬊ ( N

A ⫽ ⫺

I

I

pA

⫺ trI),

(13.2.6)

I⫽1

where N is the number of active martensitic variants at the current conﬁguration of the RVE and ƒI their volume fractions. With the instantaneous growth hypothesis, the stress inside a growing microdomain ⫺ belonging to a martensitic variant I is related to A by the following simple form (see Problem 13.6): ⫺ ⫽ A ⫺ L ⬊ (I ⫺ SI) ⬊ trI.

(13.2.7)

With (13.2.7), (13.2.3) leads to FI ⫽ A ⬊ trI ⫺ B(T ⫺ T 0) ⫺ –21 trI ⬊ L ⬊ (I ⫺ SI) ⬊ trI.

(13.2.8)

In the thermodynamic force (13.2.8), one can distinguish two contributions: • A long-range internal stress effect through the term A : trI ⫺ B(T ⫺ T 0). The stress A contains the effects of plastic strain of both

phases, as well as of transformation strains undergone by the pre-

370

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

existing martensitic variants. Depending on the applied and internal stresses, A plays the role of variant selection. • A self-internal stresses effect through the term –12 trI : L : (I ⫺ SI) : trI depending essentially on the morphology of the growing microdomain. The effect of the internal stress ﬁeld (emerging from the plastic ﬂow) on the martensitic phase transformation is known as the strain-induced martensitic phase transformation phenomenon. Classically, the plastic ﬂow at the grain level is described by a homogeneous plastic strain through the plastic slip on crystallographic glide systems. Intragranular stresses arising from this description correspond to the second-order internal stresses. However, for ductile materials undergoing martensitic phase transformation, the role of plastic strain in phase transition is more complicated. In fact, the martensitic plates nucleate at dislocation pile-ups, dislocation dipole, or intersection of slip bands. In such a situation, the description of the strain-induced martensitic transformation is insufﬁcient through a homogeneous plastic strain. In other words, a third-order stress ﬁeld emerging from the heterogeneity of plastic strain has to be taken into account. This can be performed by the decomposition of the local austenitic plastic strain p (r) into: • A uniform part pA corresponding to its average over the whole

volume of the austenitic grain (this part is described by the crystallographic slip). • A ﬂuctuating part ⌬p (r) taking into account the heterogeneity of the plastic strain due to various conﬁgurations of inelastic defects. To take into account the ﬂuctuations of the plastic strain, (13.2.7) giving the stress inside a growing microdomain belonging to a martensitic variant I is extended to ⫺ ⫽ A ⫺ L ⬊ (I ⫺ SI) ⬊ trI ⫹ p (r),

(13.2.9)

where p (r) is a third-order stress ﬁeld resulting from ⌬p (r) p (r) is evaluated using an inclusion problem, where we assume that the martensitic domain nucleates and grows at a plastic defect with volume V p and undergoing a plastic heterogeneity with strength ⌬p. The initial shape of the martensitic nucleus coincides with one of the plastic defects. In such conditions, the thermodynamic force (13.2.8) is extended to the following form [see Cherkaoui et al. (2000)]:

13.2.

APPLICATION: THERMODYNAMIC FORCES AND CONSTITUTIVE EQUATIONS

371

FI ⫽ A ⬊ trI ⫺ B(T ⫺ T 0) ⫺ –12 trI ⬊ L ⬊ (I ⫺ SI) ⬊ trI ⫹ gHIn␥ n, (13.2.10) where HIn ⫽ RI ⬊ L ⬊ (SI ⫺ Spn) ⬊ PAn,

(13.2.11)

Spn is Eshelby’s tensor depending on the morphology of the plastic ‘‘defect’’ assumed to have the initial shape of the martensitic nucleus; g and RI are given in Eq. (13.1.17); ␥ n is the plastic slip in the residual austenitic phase; PAn is the corresponding Schmidt tensor; and is a model parameter. For the plastic ﬂow in residual austenitic phase, the associated driving forces are the resolved shear stresses on slip systems given by (see Chapter 11) An ⫽ A ⬊ PAn.

(13.2.12)

As shown by equation (13.2.12), the plastic ﬂow is affected by the phase transformation through the average stress A. This constitutes in addition to the transformation strain the mechanisms of ductility enhancement in these materials. Critical Forces and Constitutive Equations of a Single Crystal

From an energetic point of view, the formation of a martensitic domain is allowed, if the associated driving force FI overcomes a transformation barrier Fc. This critical force stems from the energy necessary to rebuild the crystal lattice at the front of the developed domain. Fc can be considered as a material parameter. Concerning the plasticity of the austenitic phase and since the predominant mechanisms are the plastic slips on the crystallographic glide systems, the usual hardening matrix Hgh A is introduced describing the self and the latent hardening in FCC metals; see Chapter 11. In such conditions, the critical force cg A to achieve for plastic slip on a glide system g is expressed as h cAg ⫽ cA0 ⫹ Hgh A ␥ ,

(13.2.13)

where cA0 is the initial critical shear stress and is identical for all the slip systems.

372

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

When the thermodynamic driving forces reach their critical values, the consistency rule leads to the evolution laws for ƒ˙ I and ␥˙ n. From (13.2.10) and (13.2.12), the consistency rule applied to the transformation type of internal variables gives the following expression: ˙ RI ⫹ gƒ˙ JL⬊(I ⫺ SJ)⬊RI ⬊ RJ ⫺ ƒJL⬊(I ⫺ SJ)⬊RI⬊PAn␥˙ n ⬊ ⫹ HIn␥˙ n ⫺

B ˙ T ⫽ 0. g

(13.2.14)

In the same way, one obtains from (13.2.13) and (13.2.12) the following relation for the plastic type of internal variables: ˙ PAg ⫹ gƒ˙ JL⬊(I ⫺ SJ)⬊PAg ⬊ RJ ⬊ ⫺ ƒJL⬊(I ⫺ SJ)⬊PA ⬊ PA ␥˙ n ⫺ HAgn␥˙ n ⫽ 0. g

n

(13.2.15)

which is added to Eq. (13.2.14) to build a nonlinear system whose solution gives the evolution laws of the internal variables Xi characterizing the martensitic phase transformation and the plastic ﬂow of the parent phase. This could be formally written as ˙ X˙ i ⫽ Akli (,T,X)˙ kl ⫹ Bi (,T,X)T.

(13.2.16)

Equation (13.2.16) can be also expressed formally as function of internal variables Xi as follows: k ˙ ˙ tp ij ⫽ Mij (X)Xk.

(13.2.17)

Combining (13.2.16) and (13.2.17), the inelastic response of an austenitic single crystal is expressed as k k k k ˙ ˙ ˙ tp ij ⫽ Mij (X) Amn (,T,X)mn ⫹ Mij (X)B (,T,X)T.

(13.2.18)

˙ , one obtains the constiBy adding the elastic response ˙ e ⫽ L⫺1 ⬊ tutive equation of an austenitic single crystal undergoing martensitic phase transformation coupled with plasticity. That is

13.3.

OVERALL BEHAVIOR OF POLYCRYSTALLINE MATERIALS

373

k k ˙ ˙ ij ⫽ [L⫺1 ijmn ⫹ Mij (X) Amn (,T,X)]mn

˙ ⫹ Mkij (X) Bk (,T,X)T.

(13.2.19)

Equation (13.2.19) can also be formally written as ˙ ˙ ij ⫽ (L)⫺1˙ mn ⫺ mT,

(13.2.20)

where L and m are the average tangent elastoplastic and thermal moduli of a single crystal, respectively. Equation (13.2.20) is similar to a nonhomogeneous thermoelastic problems where both elastic modulus and thermal expansion coefﬁcients ﬂuctuate in a given composite material. In our case, it corresponds to a polycrystalline aggregate of single crystals with given crystallographic orientations with their constitutive laws described by (13.2.20). Here the thermal contribution arises only from the chemical energy related to phase transformation. Under purely mechanical loading conditions (T˙ ⫽ 0), Eq. (13.2.20) is reduced to the incremental formulation adopted by Hill for his selfconsistent model; see Chapter 11. An extension of Hill’s approach to account for the ‘‘thermal’’ ﬂuctuations of local ﬁelds is not straightforward. In the next section, we recall the ﬁeld equations within a thermomechanical framework. The analysis leads to a thermomechanical integral equation. A self-consistent approximation of this equation reduces to Hill’s model when a purely mechanical loading is applied.

13.3 OVERALL BEHAVIOR OF POLYCRYSTALLINE MATERIALS WITH PHASE TRANSFORMATION

In the previous section, the constitutive equation of an austenitic single crystal has been established within micromechanics and thermodynamics frameworks. This accomplishes the ﬁrst transition method, which takes into account different features of martensitic transformation and its couplings with plastic ﬂow. Interactions between crystals have to be undertaken to describe the thermomechanical behavior of a polycrystalline aggregate, where each constituent is described by the constitutive equation (13.2.20). For such a purpose, let us consider a representative volume element of the polycrystalline aggregate with volume V, subjected on its boundary ⭸V to a velocity ﬁeld v(r) such that

374

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

i(r) ⫽ u˙ i(r) ⫽ ˙ ij xj

if r(xi) 僆 ⭸V,

(13.3.1)

where ˙ is the macroscopic applied strain. The ﬁeld equations ˙ ij,j(r) ⫽ 0,

˙ ij(r) ⫽ –12 [˙ui,j(r) ⫹ u˙ j,i(r)],

˙ ij(r) ⫽ Lijkl(r)˙kl(r) ⫺ mij(r)T˙

(13.3.2)

can be combined to solve the problem through the solution of a thermomechanical integral equation; see Problem 13.7: ˙ mn(r) ⫽ ˙ mn ⫹

冕

V⬘

0 ˙ dV⬘. ⌫mnij (r ⫺ r⬘)[⌬ Lijkl(r⬘)˙kl(r⬘) ⫺ ⌬ mij(r⬘)T]

(13.3.3) To derive (13.3.3), a reference homogeneous medium with properties L0 and M0, and with the same boundary conditions (13.3.1), is introduced such that Lijkl(r) ⫽ L0ijkl ⫹ ⌬ Lijkl(r),

mijkl(r) ⫽ M 0ijkl ⫹ ⌬ mijkl(r),

(13.3.4)

where ⌫0mnij (r ⫺ r⬘) is the modiﬁed Green’s function, expressed by 0 ⌫0mnij(r ⫺ r⬘) ⫽ ⫺–12 [G0ki,kl (r ⫺ r⬘) ⫹ Gkj,li (r ⫺ r⬘)]

(13.3.5)

in terms of Green’s functions G0(r ⫺ r⬘) related to the reference homogeneous medium. Originally, the self-consistent mean ﬁeld theory has its great interest in the properties of the modiﬁed Green tensor ⌫0, which can be divided for any homogeneous medium with tangent moduli L0 into a local part ⌫loc and nonlocal part ⌫nloc such as nloc ⌫0ijkl (r) ⫽ ⌫loc ijkl␦(r) ⫹ ⌫ijkl (r).

(13.3.6)

Substituting (13.3.6) into (13.3.3), and using the properties of the Dirac function ␦(r), the integral equation becomes,

13.3.

OVERALL BEHAVIOR OF POLYCRYSTALLINE MATERIALS

375

loc ˙ ˙ mn(r) ⫽ ˙ mn ⫹ ⌫mnij [⌬ Lijkl (r)˙kl (r) ⫺ ⌬ mij (r)T]

冕⬘ ⌫

⫹

V

(r ⫺ r⬘)

nloc mnij

˙ dV⬘, [⌬ Lijkl(r⬘)˙kl(r⬘) ⫺ ⌬ mij(r⬘)T]

(13.3.7) where the integral form in (13.3.7) is generally difﬁcult to estimate due to high and stochastic ﬂuctuations of the ﬁeld ⌬ L(r⬘)⬊˙ (r⬘) ⫺ ⌬ m(r⬘)T˙. To overcome this difﬁculty, the self-consistent mean ﬁeld theory for elastic materials chooses a reference medium (L0, M0) so that the mean value of the ﬁeld ⌬ L(r⬘)⬊˙ (r⬘) ⫺ ⌬ m(r⬘)T˙ vanishes and therefore the integral in (13.3.7) can be neglected. This condition of vanishing mean value of the ﬂuctuating ﬁeld is also known as the self-consistency condition. In fact, this condition writes

冕

V⬘

˙ dV⬘ ⫽ 0. [⌬ L(r⬘)⬊˙ (r⬘) ⫺ ⌬ m(r⬘)T)

(13.3.8)

On the other hand, one can show in a straightforward manner that Eq. (13.3.8) leads to the following macroscopic behavior (see Problem 13.8): ˙ ij ⫽ L0ijkl˙ kl ⫺ M ij0 ˙T.

(13.3.9)

Expression (13.3.9) shows an interesting property that consists in the typical choice of the reference medium (L0, M0) to fulﬁll the consistency condition stated above. Clearly, it follows from (13.3.9) that the properties of the reference medium should be the effective properties of the considered composite, that is, L0 ⫽ L and M0 ⫽ M. Under the self-consistent approximation, Eq. (13.3.7) is reduced to loc ˙ mn(r) ⫽ ˙ mn ⫹ ⌫mnij [(Lijkl(r) ⫺ Lijkl]˙kl(r)

˙ ⫺ [mij(r) ⫺ Mij]T.

(13.3.10)

Here ⌫loc is calculated with respect to the effective properties L of the polycrystalline material. Equation (13.3.10) may be reorganized as follows:

376

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

˙ ˙ ij(r) ⫽ Aijkl(r)˙ kl ⫺ aij(r)T,

(13.3.11)

where the concentration tensors A and a are expressed by loc Amnkl(r) ⫽ {Imnkl ⫺ ⌫mnij [Lijkl(r) ⫺ Lijkl]}⫺1, loc akl(r) ⫽ Aklmn(r)⌫mnij [mij(r) ⫺ Mij].

(13.2.12)

Note that Eq. (13.3.11) solves the concentration or localization problem, which allows us to determine the effective properties as L ⫽ 具L(r)⬊A(r)典V,

(13.3.13)

M ⫽ 具L(r)⬊a(r) ⫹ m(r)典V,

(13.3.14)

where the following properties have been used: ˙ ⫽ 具 ˙ (r)典V,

˙ ⫽ 具˙ (r)典V,

˙ ⫽ L⬊˙ ⫺ MT. ˙

Note that the mean ﬁeld self-consistent model developed by Hill and extensively discussed in Chapter 11 can be described by the localization problem (13.3.11) in the case of purely mechanical load (T˙ ⫽ 0). In fact, Eshelby’s elementary inclusion problem used by Hill to solve the concentration problem is deduced from (13.3.11) by assuming piecewise uniform tangent modulus, so that ˙ rij ⫽ Arijkl˙ kl

loc r with Arijkl ⫽ [Imnkl ⫺ ⌫mnij (Lijkl ⫺ Lijkl)]⫺1.

(13.3.15)

In Eq. (13.3.15), one can readily show the relationship between ⌫loc and the Hill’s tensor H and as a result the equivalency between Eq. (13.3.13) and (11.1.61) given in Chapter 11; see Problem 13.9. Finally, to adopt the above framework for polycrystalline materials, the representative volume element is assumed to be an aggregate of N single crystals with homogeneous properties (Lg, mg) (g ⫽ 1, . . . , N) and volume fractions ƒg. The integral forms (13.3.13) and (13.3.14) are reduced to the following discrete expressions:

PROBLEMS

冘 ƒ L ⬊A ,

377

N

L ⫽ 具L(r)⬊A(r)典V ⫽

g

g

g

(13.3.16)

g⫽1

冘 ƒ (L ⬊a ⫹ m ), N

M ⫽ 具L(r)⬊a(r) ⫹ m(r)典V ⫽

g

g

g

g

(13.3.17)

g⫽1

where Ag ⫽ [I ⫺ ⌫loc(L)⬊(Lg ⫺ L)]⫺1,

(13.3.18)

ag ⫽ Ag ⬊ ⌫loc (L)⬊(mg ⫺ M).

(13.3.19)

As discussed in Chapter 11, the implementation of Eq. (13.3.16) to (13.3.19) required an iterative numerical scheme. Note that the tangent moduli (Lg, mg) (g ⫽ 1, . . . , N) are deduced from Eq. (13.2.19), which requires the resolution of a nonlinear system involving the various internal variables related to phase transformation and plastic ﬂow in each considered single crystal. Indeed, the present problem dealing with the behavior of polycrystalline materials with phase transformation is much more complicated than a purely plastic problem. Numerical implementation of the present framework and applications to real polycrystalline materials can be found in Cherkaoui et al. (2000). PROBLEMS

13.1 Let us assume that the accommodation process accompanying the Bain strain occurs by plastic deformation p on a slip system with unit normal n˜ and shear direction m ˜ . We denote by ␥, the magnitude of shear. (a) If n˜ is of (1,0,1) type and m ˜ parallel to (1,0,⫺1) direction, provide the expression of p. (b) If the Bain strain is expressed by B ⫽

冢

冣

a 0 0 0 a 0 with a ⫽ 0.132, c ⫽ ⫺0.199 0 0 c

(a and b are lattice parameters) express the compatibility condition and determine ␥.

378

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

(c) Determine n and m in Eq. (13.1.7). 13.2 Prove the compatibility conditions (13.1.8). 13.3 Let us consider a RVE with volume V and that consists of a twophase austenite–martensite composite. We denote by ƒ ⫽ VM /V the volume fraction of martensite. Let us assume that the existing martensite is described by an ellipsoidal domain with boundary or interface S. If the phase transformation occurs by the ellipsoidal growth of this domain: (a) Show that the volume fraction change is expressed by (indications: use the half-axes of an ellipsoid) ƒ˙ ⫽

V˙ M 1 ⫽ V V

冕wn S

␣ ␣

dS.

(b) If the transformation strain is assumed to be piecewise uniform, so that

冘 (r), N

tr(r) ⫽

trI I

l⫽1

prove Eq. (13.1.31). 13.4 Prove Eq. (13.1.48). 13.5 Consider a RVE with an austenitic matrix containing N martensitic variants. Each variant I has experienced an eigen strain trI during the phase transformation. Denote by A the average stress in the matrix and by MI the one in a martensitic variant. By using Kroner’s inclusion problem where the inﬁnite medium represents the austenitic matrix: (a) Show that MI ⫽ A ⫹ L⬊(I ⫺ SI )⬊(PA ⫺ trI). (b) Prove Eq. (13.3.20). 13.6 Consider an inﬁnite medium representing an austenitic matrix with prescribed A and pA. Assume that a martensitic ellipsoidal domain growth instantaneously in this matrix. If we denote by ⫺ the stress within this domain: Show that ⫺ ⫽ A ⫺ L⬊(I ⫺ SI) ⬊ trI.

13.7 Using Green’s functions for inﬁnite medium, prove the integral equation (13.3.21).

SUGGESTED READINGS

379

13.8 Prove Eq. (13.3.22). 13.9 Provide the relation between ⌫loc and Hill’s tensor and prove the equivalency between Eq. (13.3.13) and Eq. (11.1.61) given in Chapter 11.

REFERENCES Cherkaoui, M., M. Berveiller, and X. Lemoine (2000) Couplings Between Plasticity and Martensitic Phase Transformation: Overall Behavior of Polycrystalline TRIP Steels, Int. J. Plasticity, Vol. 16, pp. 1215–1241. Cherkaoui, M., M. Berveiller, and H. Sabar (1998). Micromechanical Modeling of Martensitic Transformation Induced Plasticity (TRIP) in Austenitic Single Crystals, Int. J. Plasticity, Vol. 14, pp. 597–626. Eshelby, J. D. (1970). Energy Relations and the Energy-Momentum Tensor in Continuum Mechanics, In Inelastic Behavior of Solids, M. F. Kanninen, W. F. Alder, A. R. Rosenﬁeld, and R. I. Joffee, eds., McGraw-Hill, New York, pp. 77–115. Patel, J. R. and M. Cohen (1953). Criterion for the Action of Applied Stress in the Martensitic Transformation, Acta Metall., Vol. 1, pp. 531–538. Wechsler, M. S., D. S. Lieberman, and T. A. Read (1953). On the Theory of the Formation of Martensite, AIME Trans. J. Metals, Vol. 197, pp. 1503– 1515.

SUGGESTED READINGS Diani, J. M., and D. M. Parks (1998). Effects of Strain State on the Kinetics of Strain Induced Martensite in Steels, J. Mech. Phys. Solids, Vol. 46, pp. 1613–1635. Fischer, F. D. and S. M. Schlo¨gl (1995). The Inﬂuence of Material Anisotropy on Transformation Induced Plasticity in Steel Subject to Martensitic Transformation, Mech. Mater., Vol. 21, pp. 1–23. Franciosi, P., M. Berveiller, and A. Zaoui (1980). Latent Hardening in Copper and Aluminium Single Crystal, Acta Met., Vol. 28, pp. 273. Gautier, E. and A. Simon (1988). In Phase Transformation, Vol. 87, G. W. Lorimer, ed., Institute of Metals, London, pp. 285–287. Greenwood, G. W. and R. H. Johnson (1965). The Deformation of Metals under Small Stresses During Phase Transformation, Proc. Roy. Soc., Vol. A283, pp. 403.

380

MICROMECHANICS OF MARTENSITIC TRANSFORMATION IN SOLIDS

Leblond, J. B., J. Devaux, and J. C. Devaux (1989) Mathematical Modelling of Transformation Plasticity in Steels, I: Case of Ideal-Plastic Phases, Int. J. Plasticity, Vol. 5, pp. 551–572. Magee, C. L. (1966). Transformation Kinetics, Microplasticity and Aging of Martensite in Fe-31 Ni, Ph.D. Thesis, Carnegie Institute of Technology, Pittsburgh. Olson, G. B. and M. Cohen (1975). Kinetics of Strain-Induced Martensitic Nucleation, Metall. Trans. A, Vol. 6A, pp. 791. Stringfellow, R. G., D. M. Parks, and G. B. Olson (1992). A Constitutive Model for Transformation Plasticity Accompanying Strain-Induced Martensitic Transformation in Metastable Austenitic Steels, Acta Metall. Mater., Vol. 40, pp. 1703–1716.

INDEX

A adiabatic deformation, 21 austenitic phase, 348, 358, 363– 364, 369, 371 auto-accommodating groups, 351 average strain theorem, 110 average stress theorem, 109 axial stress, 261–263 B Bain strain, 351–352, 354–356, 377 body force, 15, 17, 35, 37, 53–54, 109, 113, 127, 285 bound Hashin-Shtrikman lower, 143, 340 Hashin-Shtrikman upper, 143, 144 Poisson’s ratio, 220 Reuss lower, 123, 138, 330 Voigt upper, 123, 138, 330 boundary value problem, 35–36, 41–43, 54–55, 127 bridging ﬁbers, 261, 264 Burgers vector, 57, 58, 62 C Cauchy formula, 15–17 strain, 14 stress, 15–16, 18, 20, 22, 24, 33 characteristic function, 105–107 coefﬁcient of thermal expansion, 28–29, 52–53 cofactor, 37, 74

compatibility condition, 50, 352, 354–356, 377–378 composite sphere model, 196, 198, 200, 203, 205 concave surface, 32 concentration tensors, 118–119, 154–155, 158, 175, 333 conjugate pair, 20 conservation of energy, 20, 273 consistency condition, 105, 304, 375 constitutive law, 22 continuity of displacement, 245, 354, 359 coordinate rotation, 215 correlation function, 105–108 crack density, 268–269, 271–272, 274, 276, 277 crack opening displacement, 263– 266, 269–272 crack tip, 2, 259, 261, 264 creep behavior, 325 creep function, 29–31 critical shear stress, 303, 309, 312, 316, 325–326, 371 crystal polycrystal, 100, 173–174, 176– 177, 179, 281, 284–286, 291– 294, 296–299, 306–307, 310– 312, 314, 316–318, 373 single, 176, 179, 281, 283, 285– 287, 291, 294, 296, 298–303, 305–314, 316, 325–326, 350, 357, 362, 364, 372–373, 376– 377, 379

Fundamentals of Micromechanics of Solids. Jianmin Qu and Mohammed Cherkaoui © 2006 John Wiley & Sons, Inc. ISBN: 978-0-471-46451-8

381

382

INDEX

D debond, 246 deformation tensor, 14, 20, 22–33 deformed conﬁguration, 12–13, 15–17, 20, 50 deformed surface, 17 determinant, 37, 74, 353 Differential Scheme, 179, 195, 213 dilute case, 160, 185, 187, 225 dilute concentration, 185 dislocation dipole, 370 edge, 58 general, 62 loop, 62–64, 66 pile-ups, 370 screw, 56 displacement boundary condition, 111, 116, 121–123, 126, 133, 135–136, 138, 147, 151–152, 155, 159–160, 169, 174, 198, 257, 284, 328–329 distribution function, 177–178 distribution of the inhomogeneities, 161, 183 divergence theorem, 18–19, 41, 55, 82, 109–122, 128, 247, 248 dot product, 6 double dot product, 6 dyad, 6 E effective compliance, 114, 116, 118–119, 161, 168, 174, 232, 257 effective modulus, see also effective stiffness, 113–114, 120, 165, 179, 183, 185, 187, 190, 198, 202, 204, 221, 267– 268, 297 effective stiffness, see also effective modulus, 114–115, 117, 119, 122, 125, 126, 138, 140, 159, 160, 162, 166, 169– 171, 174, 176, 177, 179, 180,

183, 194, 257, 258, 268, 273, 277, 280, 332, 334 elastic distortion, 64, 365 elastic polarization strain, 49 elasticity, 22, 34, 35, 47, 120, 153 elastic-plastic material, 32, 34 elastoviscoplasticity, 312 ellipsoidal inclusion, 71, 77, 79, 81, 86, 177, 247, 252, 292, 297, 317 ellipsoidal inhomogeneity, 84, 156, 158, 164, 174, 177 energy dissipated, 290 elastic, 289 Gibbs free, 21 Helmholtz free, 21 momentum tensor, 365, 367 release rate, 272–273 engineering constants, 217, 219, 224–226, 233, 266 ensemble average, 103–105, 107, 108–109, 285, 296 enthalpy, 21 equivalent inclusion equation, 87, 89, 156, 157, 255 equivalent inclusion method, 85, 91, 155–156 ergodic hypothesis, 104, 106, 107 Eshelby energy momentum tensor, 365, 367 estimate, 160–161, 185, 190, 193 method, 158, 184 modiﬁed, 247, 252 modiﬁed tensor, 252 solution, 40, 80, 86–89, 155, 157, 251, 315, 316 tensor, 79, 80, 83, 139, 141, 157, 159, 162, 170–171, 175, 177, 183, 223–235, 251–252, 255, 257, 293, 297, 307, 309, 352 Euler

INDEX

angles, 176–177 conﬁguration, 12, 17 coordinate, 12 strain, see also Cauchy strain, 14 evolving microstructure, 360 extensional stiffness matrix, 240 external heat ﬂux, 20 F Fiber, 113, 212–214, 217, 243, 244, 259, 278, 279, 317 ﬁber bridging, 259 ﬁber-reinforced composite, 100, 155, 214–215, 221, 223–224, 226, 234, 240, 259–261 ﬂow rule, 32–33 ﬂuctuating ﬁeld, 319, 375 fracture criterion, 2, 267, 272 fracture toughness, 259, 260, 266 G geometric singularity, 262 global strain concentration, 159, 166, 173, 333 grain, 100, 173–174, 176–177, 179, 281, 283, 292–294, 296, 297–299, 306–307, 309–310, 315, 359, 370 Green function, 38, 40–43, 55, 63, 64, 77, 79, 127–128, 132, 138, 139, 147–148 strain, 14 theorem, 18 H habit plane, 352–354, 356 Hashin-Shtrikman variational principle, 133, 136 hereditary nature, 280 hierarchical approach, 226, 239 high concentration, 185 Hill

383

constraint tensor, 90, 175, 194, 299 lemma, 111, 115, 290, 330, 338–339 polarization tensor, 78 homogeneous polynomial, 39 homogenization scheme, 283, 287, 294, 328, 332, 335–336, 339–340, 350 Hooke’s law, 24, 30, 35, 50–53, 58, 62, 74, 75, 80, 85–86, 88, 117, 122, 147–148, 174, 227, 234, 285, 288, 308 Hutchinson’s calculation, 307 hyperelastic material, 22 I incompressibility, 34, 294, 306 incompressible material, 283, 327, 336–337 incremental formulation, 326, 359 indicial notation, 5 inelastic behavior, 280, 348 initial conﬁguration, 12, 13, 17 interface imperfect, 246, 247, 257, 258 inclusion-matrix, 75 inhomogeneity-matrix, 76 perfect, 73, 245–246, 251, 257– 258 sliding, 246 spring model, 246 velocity, 368 internal energy, 19, 20, 21 internal heat source, 20 internal variable, 291, 321, 342, 358, 364, 367–368, 372, 377 interphase incompatibility, 285 intra-phase ﬂuctuation, 280 isentropic deformation, 21, 22 isothermal deformation, 21–23 J jump condition, 354

384

INDEX

K kinematic tensor, 14 kinematically admissible displacement, 112, 120–123, 126–127, 131–132, 258 kinematically admissible strain, 329 kinetic energy, 19 Kirchhoff assumption, 237 Kronecker delta, 9, 23, 52 Kro¨ner approach, 282, 296 Kro¨ner model, 294, 296 L Lagrange description, 12 strain, see also Green strain, 14 lamina, 234 latent hardening, 371 lattice, 70, 350–354, 356, 363, 371, 377 left stretch tensors, 13 linear comparison composite, 320, 332–333, 335, 338–340, 343 M Mandel-Hill condition, 112 martensite-martensite interfaces, 354 martensitic microdomains, 368, 369 martensitic variant, 349–350, 356– 357, 362–364, 368–370, 378 mass density, 17, 19 material asymmetry, 218 coordinates, 16 cubic, 45, 46 isotropic, 25–26, 37, 40, 58, 61– 62, 69, 74, 83, 204, 323, 326, 328, 338, 340, 342 orthotropic, 44 transversely isotropic, 45–46 matrix cracks, 266, 268

minimum complementary energy theorem, 121 minimum potential energy theorem, 120 mocrohomogeneity, 102 modulus bulk, 187, 196–198, 201, 203– 207, 213, 219–220, 258, 307, 323 effective, 261, 268, 269, 271– 273, 277 longitudinal shear, 199 longitudinal Young’s, 199 shear, 26, 126, 162, 188, 190– 192, 198, 200–202, 204–206, 208, 218–220, 226, 233, 235, 258, 293, 307, 323–324, 327, 342 transverse bulk, 199 Young, 51, 214, 221–223, 225, 233, 240 monoclinic material, 229, 243 Mori-Tanaka Method, 163, 184 moving boundary, 359 multicoated inclusion, 204 multilayer composites, 226 Mura formula, 65 N nonlinear behavior, 280–282, 291, 319–320, 331–333, 336–337 non-perfect interface, see also imperfect interface, 113 O one-point correlation, 105–106 orientation tensors, 302 P perfect interface, 73, 245–246, 251, 257–258 perfect plasticity, 305, 309, 316 permutation tensor, 9, 37, 74

INDEX

phase transformation, 49, 53, 347– 351, 354–360, 362–364, 368– 373, 377–379 physical entity, 5, 19 plane strain, 219–220, 238, 260, 273–274 plastic behavior, 280, 305 plastic distortion, 302 plasticity, 31, 316–317, 323, 347, 379 Poisson’s ratio, 199 polar decomposition, 13 potential convex, 322, 326 dissipation, 321, 322 effective, 328 macroscopic, 319, 338 thermodynamics, 18, 20, 21, 321, 325 probability distribution function, 105 Q quadratic equation, 188, 191 quasi-static problems, 246 R reciprocal theorem, 39, 41 recrystallization, 359 reduced stiffness matrix, 235 reference conﬁguration, 14, 20, 21, 23 relaxation function, 29, 31 representative volume element, 102, 108, 197, 198, 200–201, 204, 227, 228, 229, 242, 253– 254, 283, 284, 285, 330, 350, 373, 376 resolved shear stress, 300, 302, 312, 371 right stretch tensor, 13 right stretch tensors, 13 rigid particles, 186 rotation matrix, 176

385

rotation tensor, 13, 24 rule of mixture, 223, 240 RVE, see also representative volume element, 102, 103, 108, 111, 113, 319, 324, 328, 350, 357, 359, 360, 364, 369, 378 S scalar function, 8, 18, 19 secant approach, 312, 331 compliance tensor, 314–315 moduli, 326 viscoplastic compliance, 313 second order elastic constant, 23 self-adjoint operator, 129, 145 self-consistent method, 169, 173, 184 self-equilibrium stress ﬁeld, 287 size distribution, 196 size-dependent propertiy, 183 slip plane, 62, 66, 300 slip system, 300–308, 310, 312, 325, 353, 364, 371, 377 spatial coordinates, 16 spin tensor, 14 statically admissible stress, 112, 121–124, 126–127, 134–136, 146, 149, 198, 259, 286 statistically homogeneous medium, 106, 108, 109, 113, 139, 285 steady-state creep, 282, 312 step function, 357 Stokes’ theorem, 19, 64 strain concentration tensor, 117, 166, 174, 180, 182–183, 224, 307 strain energy, 19, 23, 81–82, 112, 114–116, 122–123, 133, 135– 136, 151–152, 268–269, 273, 282, 289, 290, 336 strain hardening, 300, 303, 306, 309

386

INDEX

strain rate, 284, 295, 297–300, 302, 304–306, 312–315, 322, 325, 363, 374 stress Cauchy, 15–16, 18, 20, 22, 24, 33 deviatoric, 31, 33 ﬁrst Piola-Kirchhoff, 16 power, 20–21, 290 second Piola-Kirchhoff, 16, 23 stress concentration tensor, 118, 160, 167, 170, 174, 182, 255– 256, 287, 307 stress intensity factor, 259–261, 266 stress polarization, 80, 90–91, 127, 132–133, 135–136, 149 stress-free transformation strain, 49 stress-strain relationship, 28, 29, 31–33, 50, 234, 236, 280, 311 summary convention, 5 symbolic notation, 7, 26, 83, 129, 162–163, 168, 293 T tangent compliance tensor, 297– 299, 314–315 tangent modulus, 294–299, 305– 307, 309, 314, 327–328, 376 Taylor expansion, 23, 27, 314 Taylor-Lin model, 296, 311 tensor transformation, 24 texture, 281, 316 thermoelasticity, 26 third order elastic constant, 23 threshold strain, 276, 277 traction boundary condition, 109, 110, 118–119, 146–147, 155, 160, 169, 175, 254, 284–286, 289, 328–329 traction vector, 16, 17, 18, 246, 366 transform Fourier, 36, 37, 54, 57, 58

Laplace, 30–31 Legendre, 322 transverse matrix crack, 266, 269, 273 Tresca yield function, 33 TRIP, 347, 349–350, 379 twinning, 351–354, 356, 359 two-point correlation function, 105–106 U unit outward normal, 16, 248 unit sphere, 39, 78, 92, 93, 139 V variant, 282, 357–358, 362–364, 368, 370, 378 velocity of the interface, 361–362, 366 viscoelasticity, 29, 48 Voids, 190 Voigt elastic constant, 25, 44, 216, 220, 227, 232, 233 Volterra formula, 63 volume average, 104, 106–109, 111, 112, 284, 285 volume fraction, 103–104, 107, 117, 125–126, 137, 140, 154, 160–162, 173, 178–180, 182, 185, 188, 192, 194, 196, 197, 200–201, 205, 208, 214, 225, 228, 240, 242, 258, 261, 268, 285, 320, 342, 349, 358, 364, 367–369, 376, 378 Von Mises criterion, 323 von Mises yield function, 33 W work-hardening, 34 Y yield function, 32–33 yield surface, 32–33, 291

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close